Magnetic Techniques for the Treatment of Materials
Magnetic Techniques for the Treatment of Materials by
Jan Svoboda ...

Author:
Jan Svoboda

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Magnetic Techniques for the Treatment of Materials

Magnetic Techniques for the Treatment of Materials by

Jan Svoboda Formerly Research Programme manager and Principal Technology leader, De Beers Diamond Research Laboratory, De Beers Consolidated Mines (Pty.) Ltd., Johannesburg, South Africa

KLUWER ACADEMIC PUBLISHERS NEW YORK, BOSTON, DORDRECHT, LONDON, MOSCOW

eBook ISBN: Print ISBN:

1-4020-2107-0 1-4020-2038-4

©2004 Springer Science + Business Media, Inc.

Print ©2004 Kluwer Academic Publishers Dordrecht All rights reserved

No part of this eBook may be reproduced or transmitted in any form or by any means, electronic, mechanical, recording, or otherwise, without written consent from the Publisher

Created in the United States of America

Visit Springer's eBookstore at: and the Springer Global Website Online at:

http://www.ebooks.kluweronline.com http://www.springeronline.com

Contents Contents

v

Preface

xi

1 Principles of Magnetic Treatment 1.1 Magnetic separation and innovation . . . . . . . . . . . . . . . . 1.2 Principles of magnetic separation . . . . . . . . . . . . . . . . . . 1.2.1 Magnetic force on a magnetizable particle . . . . . . . . 1.2.2 Competing forces in a magnetic separator . . . . . . . . . 1.3 Fundamental quantities of magnetism . . . . . . . . . . . . . . . 1.3.1 Magnetic ﬁeld and magnetization . . . . . . . . . . . . . . 1.3.2 Magnetic susceptibility and permeability . . . . . . . . . 1.3.3 Magnetic units . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Magnetic properties of materials . . . . . . . . . . . . . . . . . . 1.4.1 Diamagnetism . . . . . . . . . . . . . . . . . . . . . . . . 1.4.2 Paramagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.3 Ferromagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.4 Antiferromagnetism . . . . . . . . . . . . . . . . . . . . . 1.4.5 Ferrimagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.6 Demagnetization . . . . . . . . . . . . . . . . . . . . . . . 1.4.7 Mixtures containing ferromagnetic (s.l.) materials . . . . 1.5 Magnetic properties of minerals . . . . . . . . . . . . . . . . . . . 1.5.1 The classiﬁcation of minerals according to their magnetic properties . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.2 Magnetite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.3 Titanomagnetites . . . . . . . . . . . . . . . . . . . . . . . 1.5.4 Ilmenohematites . . . . . . . . . . . . . . . . . . . . . . . 1.5.5 Maghemite . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.6 Hematite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.7 Goethite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.8 Siderite . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.9 Iron sulphides . . . . . . . . . . . . . . . . . . . . . . . . 1.5.10 Chromites . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 Measurement of magnetic properties . . . . . . . . . . . . . . . .

1 1 3 5 6 9 9 10 10 11 13 14 15 21 21 21 24 25

v

25 26 27 29 31 31 32 33 33 34 34

CONTENTS

vi

1.7

1.6.1 Measurement of the magnetic ﬁeld strength 1.6.2 Measurement of magnetic susceptibility and Sources of magnetic ﬁeld . . . . . . . . . . . . . . . 1.7.1 Permanent magnets . . . . . . . . . . . . . 1.7.2 Iron-core electromagnets . . . . . . . . . . . 1.7.3 Solenoid electromagnets . . . . . . . . . . . 1.7.4 Superconducting magnets . . . . . . . . . . 1.7.5 Generation of the magnetic ﬁeld gradient .

. . . . . . . . magnetization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 Review of Magnetic Separators 2.1 Dry low-intensity magnetic separators . . . . . . . . . . . . 2.1.1 Magnetic pulleys . . . . . . . . . . . . . . . . . . . . 2.1.2 Plate magnets . . . . . . . . . . . . . . . . . . . . . 2.1.3 Grate magnets . . . . . . . . . . . . . . . . . . . . . 2.1.4 Suspended magnets . . . . . . . . . . . . . . . . . . 2.1.5 Drum magnetic separators . . . . . . . . . . . . . . . 2.2 Wet low-intensity drum magnetic separators . . . . . . . . . 2.2.1 Concurrent tank . . . . . . . . . . . . . . . . . . . . 2.2.2 Counter-rotation tank . . . . . . . . . . . . . . . . . 2.2.3 Counter-current tank . . . . . . . . . . . . . . . . . . 2.2.4 Design of the drum . . . . . . . . . . . . . . . . . . . 2.3 Dry high-intensity magnetic separators . . . . . . . . . . . . 2.3.1 Cross-belt magnetic separator . . . . . . . . . . . . . 2.3.2 Induced magnetic roll separator . . . . . . . . . . . . 2.3.3 Permanent magnetic roll separator . . . . . . . . . . 2.3.4 High-intensity drum separators . . . . . . . . . . . . 2.4 Wet high-intensity magnetic separators . . . . . . . . . . . . 2.4.1 Dry separation versus wet separation . . . . . . . . . 2.4.2 Iron core-based wet high-intensity separators . . . . 2.4.3 Solenoid-based magnetic separators . . . . . . . . . . 2.5 Superconducting magnetic separators . . . . . . . . . . . . . 2.5.1 Cyclic superconducting HGMS . . . . . . . . . . . . 2.5.2 Reciprocating superconducting HGMS . . . . . . . . 2.5.3 Open-gradient superconducting magnetic separators 2.6 Laboratory magnetic separators . . . . . . . . . . . . . . . . 2.6.1 Davis Tube . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Frantz isodynamic separator . . . . . . . . . . . . . 2.6.3 Separators with a rotating magnetic ﬁeld . . . . . . 2.7 Eddy-current separators . . . . . . . . . . . . . . . . . . . . 2.8 Separators with magnetic ﬂuids . . . . . . . . . . . . . . . . 2.8.1 Basic concept . . . . . . . . . . . . . . . . . . . . . . 2.8.2 Ferrohydrostatic separators . . . . . . . . . . . . . . 2.8.3 Magstream separator . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

35 39 45 47 53 56 57 59 67 69 70 72 72 73 78 81 82 82 84 84 86 86 88 89 94 96 96 97 112 128 131 132 136 138 139 141 146 147 153 153 156 159

CONTENTS

vii

3 Theory of Magnetic Separation 3.1 The forces and the equations of particle motion . . . . . . . . . . 3.2 Particle motion in drum and roll separators . . . . . . . . . . . . 3.2.1 Motion of a particle on the drum or roll surface . . . . . . 3.2.2 Motion of the particle after it leaves the roll . . . . . . . . 3.3 Separation of particles by a suspended magnet . . . . . . . . . . 3.3.1 Magnetic force in a suspended magnet . . . . . . . . . . . 3.3.2 Torque on a magnetizable body . . . . . . . . . . . . . . . 3.3.3 Demagnetization factors . . . . . . . . . . . . . . . . . . . 3.3.4 The eect of the burden . . . . . . . . . . . . . . . . . . . 3.4 High-gradient magnetic separation . . . . . . . . . . . . . . . . . 3.4.1 Theory of particle capture by a single-collector . . . . . . 3.4.2 Capture of particles in multi-collector matrices . . . . . . 3.5 Linear open-gradient magnetic separation . . . . . . . . . . . . . 3.6 Magnetic ﬂocculation . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 Magnetic ﬂocculation of strongly magnetic materials . . . 3.6.2 Magnetic ﬂocculation of weakly magnetic minerals . . . . 3.7 Magnetic separation by particle rotation . . . . . . . . . . . . . . 3.7.1 RMF rotation separation . . . . . . . . . . . . . . . . . . 3.7.2 Magnetic torque on a particle and condition for separation by rotation . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.3 Rotation of particles in a liquid . . . . . . . . . . . . . . . 3.8 Separation in magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . 3.8.1 Apparent density of a magnetic ﬂuid . . . . . . . . . . . . 3.8.2 A particle suspended in a magnetic ﬂuid . . . . . . . . . . 3.8.3 The eect of the hydrodynamic drag . . . . . . . . . . . . 3.8.4 The eect of particle magnetic susceptibility . . . . . . . 3.8.5 Motion of particles in a ferroﬂuid . . . . . . . . . . . . . . 3.8.6 Separation in a rotating ferroﬂuid . . . . . . . . . . . . . 3.9 Eddy-current separation . . . . . . . . . . . . . . . . . . . . . . . 3.9.1 Static ramp eddy-current separator. . . . . . . . . . . . . 3.9.2 Rotating drum eddy-current separators . . . . . . . . . . 3.9.3 Eddy-current separation by particle rotation . . . . . . .

163 164 166 169 170 172 173 175 178 179 181 181 198 206 208 208 210 221 222

4 Design of Magnetic Separators 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Design of circuits with permanent magnets . . . . . . . 4.2.1 Basic concepts and ﬁgures of merit . . . . . . . . 4.2.2 The static gap design . . . . . . . . . . . . . . . 4.2.3 Leakage factors . . . . . . . . . . . . . . . . . . . 4.2.4 Determination of permeance and leakage factors 4.2.5 Magnetic ﬁeld around a permanent magnet . . . 4.2.6 Magnetic forces . . . . . . . . . . . . . . . . . . . 4.2.7 Soft iron components of the magnetic circuits . . 4.2.8 Stability of permanent magnets . . . . . . . . . . 4.2.9 Magnetization of permanent magnets . . . . . .

251 251 252 252 255 257 258 259 263 264 266 269

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

224 226 227 227 229 233 234 235 240 243 243 245 249

CONTENTS

viii 4.3

. . . . . . . . . . . . . . . . . . . . . .

270 271 272 274 278 280 280 280 281 282 282 284 289 291 291 293 298 299 301 304 308 311

5 Practical Aspects of Magnetic Methods 5.1 Selection of magnetic separation technique . . . . . . . . . . . . . 5.2 Dry magnetic separation . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Electrostatic phenomena in dry separation . . . . . . . . . 5.2.2 Density and magnetic tracers . . . . . . . . . . . . . . . . 5.2.3 Comparison of dry magnetic separation techniques . . . . 5.3 Wet magnetic separation . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Wet low-intensity drum magnetic separation . . . . . . . 5.3.2 Wet high-intensity magnetic separation . . . . . . . . . . 5.3.3 Magnetic ﬁeld in high-intensity magnetic separators . . . 5.3.4 Matrix in high-gradient magnetic separators . . . . . . . . 5.3.5 Flow velocity of the slurry . . . . . . . . . . . . . . . . . . 5.3.6 Slurry density . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.7 Feed rate . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.8 The eect of particle size . . . . . . . . . . . . . . . . . . 5.3.9 Pre-treatment of slurry . . . . . . . . . . . . . . . . . . . 5.3.10 The selectivity of separation . . . . . . . . . . . . . . . . . 5.3.11 Comparative tests with wet high-intensity magnetic separators . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Magnetic ﬂocculation . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Magnetic ﬂocculation of ferromagnetic materials . . . . . 5.4.2 Magnetic ﬂocculation of weakly magnetic minerals . . . . 5.5 Demagnetization . . . . . . . . . . . . . . . . . . . . . . . . . . .

319 320 321 323 326 328 342 342 354 360 375 396 399 402 403 405 411

4.4

4.5

4.6

4.7 4.8

Design of iron-core electromagnets . . . . . . . . . . 4.3.1 Calculation of the magnetic ﬁeld . . . . . . . 4.3.2 Shape of iron parts of the circuit . . . . . . . 4.3.3 Practical procedure for design of the poles . . Design of solenoid magnets . . . . . . . . . . . . . . 4.4.1 The power requirements . . . . . . . . . . . . 4.4.2 The choice of the conductor . . . . . . . . . . 4.4.3 The cooling of coils . . . . . . . . . . . . . . . 4.4.4 Thickness of the iron cladding . . . . . . . . . Design of drum magnetic separators . . . . . . . . . 4.5.1 The basic magnet arrangements . . . . . . . . 4.5.2 Geometry of the magnet assembly . . . . . . 4.5.3 Electromagnetic modelling of the design . . . Design of a magnetic roll . . . . . . . . . . . . . . . . 4.6.1 Basic concepts of design . . . . . . . . . . . . 4.6.2 Design parameters . . . . . . . . . . . . . . . Design of a suspended magnet . . . . . . . . . . . . . Design of a ferrohydrostatic separator . . . . . . . . 4.8.1 FHS separators with a wedge-shaped working 4.8.2 Separators with hyperbolic pole tips . . . . . 4.8.3 Calculation of proﬁles of pole tips in FHS . . 4.8.4 Scale-up of ferrohydrostatic separators . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . gap . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

417 420 420 422 422

CONTENTS 5.6

5.7

ix

Separation in magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . 425 5.6.1 Magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . . . . . 426 5.6.2 Ferrohydrostatic separation . . . . . . . . . . . . . . . . . 440 5.6.3 Ferroﬂuid recovery and recycling . . . . . . . . . . . . . . 454 5.6.4 Separation in a rotating ferroﬂuid . . . . . . . . . . . . . 458 Magnetism in other areas of material handling . . . . . . . . . . 459 5.7.1 Magnetic cyclone . . . . . . . . . . . . . . . . . . . . . . . 460 5.7.2 Magnetic gravity separation, ﬂotation and vacuum ﬁltration466 5.7.3 Magnetic jigging . . . . . . . . . . . . . . . . . . . . . . . 467

6 Industrial Applications 6.1 Treatment of minerals . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Recovery of grinding ball fragments from SAG and ball mills . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.2 Heavy medium recovery circuits . . . . . . . . . . . . . . 6.1.3 Beneﬁciation of iron ores . . . . . . . . . . . . . . . . . . 6.1.4 Beneﬁciation of manganese ores . . . . . . . . . . . . . . . 6.1.5 Beneﬁciation of ilmenite ores . . . . . . . . . . . . . . . . 6.1.6 Beneﬁciation of ores of non-ferrous metals . . . . . . . . . 6.1.7 Mineral sands . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.8 Industrial minerals . . . . . . . . . . . . . . . . . . . . . . 6.1.9 Magnetic beneﬁciation of coal . . . . . . . . . . . . . . . . 6.2 Nuclear industry . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Removal of solids from fuel dissolver liquor . . . . . . . . 6.2.2 Removal of ferric hydroxide ﬂocs . . . . . . . . . . . . . . 6.2.3 Soil decontamination . . . . . . . . . . . . . . . . . . . . . 6.3 Waste water treatment . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Steel industry . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Thermal power plants . . . . . . . . . . . . . . . . . . . . 6.4 Magnetic carrier techniques . . . . . . . . . . . . . . . . . . . . . 6.4.1 General principles . . . . . . . . . . . . . . . . . . . . . . 6.4.2 E"uent processing and metal ion removal . . . . . . . . . 6.4.3 Biomagnetic extraction of heavy metals . . . . . . . . . . 6.5 Magnetic carriers and separation in biosciences . . . . . . . . . . 6.5.1 Principles of biomagnetic separation techniques . . . . . . 6.5.2 Magnetic separators in biosciences . . . . . . . . . . . . . 6.5.3 The application of magnetic separation . . . . . . . . . . 6.5.4 Separation of red blood cells by HGMS . . . . . . . . . . 6.6 Recovery of metals from wastes . . . . . . . . . . . . . . . . . . . 6.6.1 The separation processes in metal recycling . . . . . . . . 6.6.2 Sorting of heavy non-ferrous metals . . . . . . . . . . . . 6.7 The applications of ferrohydrostatic separation . . . . . . . . . . 6.7.1 Recovery of gold and other platinum-group metals . . . . 6.7.2 Applications in the diamond winning industry . . . . . . 6.7.3 The fractionation analysis of coal . . . . . . . . . . . . . .

469 470 470 472 472 488 489 494 498 504 507 510 510 511 511 514 514 517 519 519 520 524 525 525 528 530 533 534 535 539 542 543 545 546

x

CONTENTS

7 Innovation and future trends 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Science and technological innovation . . . . . . . . . . . . . . . 7.3 Magnetic separation and innovation . . . . . . . . . . . . . . . 7.3.1 Reliance on an empirical approach? . . . . . . . . . . . 7.3.2 A walk through innovation in magnetic separation . . . 7.4 The current status of magnetic separation technology . . . . . . 7.5 What the future holds? . . . . . . . . . . . . . . . . . . . . . . 7.5.1 Mineral processing . . . . . . . . . . . . . . . . . . . . . 7.5.2 Biomedical applications . . . . . . . . . . . . . . . . . . 7.5.3 Recycling and waste processing . . . . . . . . . . . . . . 7.5.4 Prospects for superconductivity in magnetic separation 7.6 Research and development needs . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

551 551 552 555 556 556 567 567 568 569 569 570 573

List of Symbols

577

Bibliography

583

Index

629

Preface In the years following the publication of Magnetic Methods for the Treatment of Minerals by Elsevier in 1987, many changes have taken place in magnetic technology. While fundamental and thorough, the above treatise reﬂected preferences and philosophy of research and the development and application of magnetic methods as they were practiced in the second half of the last century. Although demand for metals and minerals has not diminished, the dominant drivers of the early 21st century dier signiﬁcantly from those of the late 20th. The priorities of nuclear power, defence, and energy-demanding and waste-generating beneﬁciation of mineral resources are being replaced by those associated with technology sustainability, environmental and knowledge management, recycling, and health care. Research priorities and product development of the last century cannot, therefore, satisfactorily meet criteria of the 21st century. Considerable technological progress has been achieved in areas such as automation, computerization, sustainable material science, laboratory and plant practices and separation equipment. New permanent magnetic materials, advances in practical applications of superconductivity and availability of sophisticated modelling tools have changed the technological landscape. As a result, innovation and technology transfer in magnetic technology have been remarkably successful during the last two decades. The title of this monograph reﬂects the fact that the book covers not only the application of magnetic techniques in the minerals industry, but also in recycling, environmental engineering and biomedical sciences. The goal of the book is to reﬂect the current technological trends and to re-position the research, development and practice of magnetic methods of material manipulation, according to current needs and strategic thinking. The book is intended for researchers, students, development workers and consulting metallurgists, as well as plant practitioners and equipment manufacturers who wish to acquire comprehensive knowledge of magnetic separation technology. The book is based on work of numerous scientists and engineers. I am grateful to many of my colleagues and friends at universities, research organizations, and mining and manufacturing companies around the world, for their contribution in advancing magnetic separation technology. Interaction and collaboration with them over the years has been enriching and rewarding and they will be identiﬁed in this monograph by citation of their published work. I am xi

PREFACE

xii

also indebted to many individuals and companies who have given me invaluable help by providing data and photographs for reproduction. Their important contributions have been acknowledged directly in the text. I am grateful to Mr. E. H. Roux and Drs. D. Slatter, G. Hill and N. Allen for their kindness in reading portions of the manuscript and suggesting improvements. I also wish to express my appreciation to my colleagues Drs. V. Murariu and L. Krüger and Mr. A. Sarelis for assistance with various aspects of this book. Jan Svoboda Johannesburg, South Africa February 2004

Chapter 1

Principles of Material Treatment by Magnetic Means 1.1

Magnetism and the innovation milestones in magnetic separation

Magnetic phenomena have been known and exploited for many centuries. The earliest experiences with magnetism involved magnetite, the only material that occurs naturally in a magnetic state. Thales of Miletus stated that the magnetic interaction between lodestone, or magnetite, and iron was known for at least as long ago as 600 B.C. That magnetite can induce iron to acquire attractive powers, or to become magnetic, was mentioned by Socrates. Permanent and induced magnetism, therefore, represents one of man’s earliest scientiﬁc discoveries. Practical signiﬁcance of magnetic attraction as a precursory form of magnetic separation was recognized in 1792, when W. Fullarton obtained an English patent for separating iron ore by magnetic attraction [D1]. Since that time the science and engineering of magnetism and of magnetic separation have advanced rapidly and a large number of patents have been issued. While separation of inherently magnetic constituents was a natural early application of magnetism, Wetherill’s separator, devised in 1895, was an innovation of signiﬁcant proportions. It demonstrated that it was possible to separate two components, both of which were commonly considered to be non-magnetic. In the ensuing time various types of disk, drum and roll dry magnetic separators were developed although the spectrum of minerals treatable by these machines was limited to rather coarse and moderately strongly magnetic materials. Since the end of the nineteenth century there has been a steady expansion of both the equipment available and the range of ores to which magnetic separation is applicable. The development of permanent magnetic materials and improvement in their 1

2

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.1: Development of permanent magnet materials.

magnetic properties have been main drivers of innovation in magnetic separation. Figure 1.1 illustrates the history of improvement of the maximum energy product (EK)max of permanent magnets. Three innovation milestones can be identiﬁed in the graph. At the end of the nineteenth century very feeble steelbased magnets were employed, while in the 1940s permanent magnets that were able to compete with electromagnets, were developed. Probably the most important innovation step was made in the late seventies of the last century when rare-earth magnets became available. These magnets allowed new solutions for challenges that were not possible or feasible with electromagnets. Another signiﬁcant driver of innovation in magnetic separation was the introduction of ferromagnetic bodies (such as balls, grooved plates or mesh) into the magnetic ﬁeld of a separator. In 1937 Frantz developed a magnetic separator consisting of an iron-bound solenoid packed with ferromagnetic steel ribbons [F1] and this proved to be an important milestone in the development of the present high-intensity and high-gradient magnetic separators. This innovation extended the range of applicability of magnetic separation to many weakly magnetic and even to diamagnetic minerals of the micrometer size. Although the signiﬁcance of the discovery of superconductivity has been equated with the invention of the wheel [K1], its importance for magnetic separation does not seem to represent a major breakthrough. The need for magnetic induction greater than 2 T has never been convincingly demonstrated in matrix separators [S1, S2] and the main advantage of superconducting magnets is, therefore, the reduced energy consumption and the possibility of generating a high magnetic force in large volumes, even without using matrices. The concentration of various ferrous and non-ferrous minerals has been an

1.2. PRINCIPLES OF MAGNETIC SEPARATION

3

Feed Magnetic force

Competing forces

Non-mags

Mags Middlings

Figure 1.2: Schematic representation of the process of magnetic separation. important application of magnetic separation, as has the removal of low concentrations of magnetizable impurities from industrial minerals. In recent years, as a result of numerous economic, environmental and social challenges, the recycling of metals from industrial wastes and the concentration or removal of biological objects in medicine and biosciences have become important areas of application of magnetic technology. Recent research and development of eddycurrent separators, magnetic ﬂuids and magnetic carriers illustrate the enormous eort that has been expended over the last twenty years in order to convert a wealth of novel ideas into workable techniques and introduce them into material manipulation operations.

1.2

Principles of magnetic separation

Magnetic separation is used for the concentration of magnetic materials and for the removal of magnetizable particles from ﬂuid streams. The separation is achieved by passing the suspensions or the mixtures of particles through a non-homogeneous magnetic ﬁeld. This process leads to preferential retention or deﬂection of the magnetizable particles. The same objective is often achieved in a very dierent fashion, the common features being a competition between a wide spectrum of forces of various magnitudes and ranges. In magnetic separation the separating (dierentiating) external force is the magnetic force. The separation of one material from another or the removal of magnetizable particles from streams depend upon their motion in response to the magnetic force and to other competing external forces, namely gravitational, inertial, hydrodynamic and centrifugal forces. Interparticle forces of electromagnetic and electrostatic origin contribute to the overall scenario, which is depicted in Fig. 1.2. It is thus clear that a necessary (but not su!cient) condition for a successful

4

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

separation of more strongly magnetic from less strongly magnetic particles in a p magnetic ﬁeld is that the magnetic force Ipdj acting on more magnetic particles lp . Simultaneously, must be greater than the sum of all the competing forces Ifrps q a magnetic force acting on less strongly magnetic particles, Ipdj must be smaller than the sum of the corresponding competing forces. Therefore, the following conditions must be met in a magnetic separator: p Ipdj

X l

lp Ifrps

and

q Ipdj

X

lq Ifrps

(1.1)

l

For dierent objectives eqs. (1.1) will have speciﬁc forms. For instance, in order to achieve high recovery of magnetic particles, the magnetic separating force must be greater than the sum of the competing forces as shown in eqs. (1.1). If, however, the magnetic force is much greater than the competing forces, i.e. Ipdj AA Ifrps (1.2) selectivity of separation will be poor, as no distinction will be made between magnetizable species of dierent values of magnetic susceptibilities. High selectivity of the separation process can thus be obtained when the magnitudes of the magnetic and competing forces are of comparable magnitudes, compatible with conditions given by eqs. (1.1). The selectivity of the process will be, therefore, critically determined by the relative values of the magnetic and competing forces. And these are aected by the correct choice of a separator and its operating conditions. For instance, selective separation of a magnetizable material (1) from magnetizable material (2) will be achieved when the following relationship is met: (1) (2) Ipdj A Ifrps A Ipdj (1.3) If the non-magnetic fraction is the valuable product, the ”brute force” approach to separation, expressed by relationship (1.2), will result in poor yield of the non-magnetic product, as a result of mechanical and magnetic entrainment of the non-magnetic material in the magnetic tailings. In general, a mixture of particles introduced into the magnetic separator will be split into two or more components. However, in any real separation, both magnetic and non-magnetic particles can be found in the magnetic fraction, non-magnetic fraction and the middling fractions. The e!ciency of separation is usually expressed by the recovery of the magnetic component, and by the grade of the magnetic product. However, these criteria are not unique and they must be selected on the basis whether the useful product is the magnetic or non-magnetic fractions. Since all materials are magnetic to some extent, methods of separation that use magnetic force oer a unique approach to material manipulation in a wide array of industries. One of the main advantages of material treatment in a magnetic ﬁeld is that the magnetic force can be applied in a controlled manner, in a wide range of values. Moreover, this force can be superimposed on other physical forces and several physical properties of materials can thus be exploited

1.2. PRINCIPLES OF MAGNETIC SEPARATION

5

simultaneously. In addition, magnetic separation can treat a wide range of types of materials, ranging from colloidal to large sizes and from ”non-magnetic” to strongly magnetic. Magnetic separation is an environmentally friendly technique and it can operate in wet and dry modes, making it a technique of choice for arid or arctic regions.

1.2.1

Magnetic force on a magnetizable particle

The density of the magnetic energy zp in a linear isotropic medium is given by: 1 K ·E (1.4) 2 where K and E are, respectively, the magnitudes of the magnetic ﬁeld and the magnetic ﬂux density (magnetic induction). It transpires from eq. (1.4) that the magnetic energy Xps of a magnetizable particle of volume Ys placed in the magnetic ﬁeld is: zp =

1 Ys K 2 2 s while the magnetic energy of a ﬂuid of the same volume is given by Xps =

Xpi =

1 Ys K 2 2 i

(1.5)

(1.6)

In eqs. (1.5) and (1.6), s and i are magnetic permeabilities of the particle and the ﬂuid, respectively. The energy increment X of the system (particle + ﬂuid) is given, to ﬁrst order, as the dierence between the energies given by eqs. (1.5) and (1.6). For weakly magnetic particles this is a good approximation [G1]. Thus: X=

1 ( s )Ys K 2 2 i

(1.7)

In general, a force can be expressed as I = uX , where u is the operator of the gradient. Taking into account that m = 0 (1 + m ) , where m is the volume magnetic susceptibility of material m and 0 is the magnetic permeability of vacuum, the magnetic force can be written (in SI units): 1 Ip = 0 (s i )Ys uK 2 2

(1.8)

In practical situations the magnetic ﬂux density E is frequently used, rather than the magnetic ﬁeld strength K, and eq. (1.8) can then be expressed as: 1 (s i )Ys EuE Ip = 0

(1.9)

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

6

For su!ciently strongly magnetic particles (s AA i ) it is advantageous to re-write eq. (1.8) as: Ip = 0 Ys P uK

(1.10)

where P is the magnetization of the particle. Researchers as well as practitioners of magnetic separation sometimes use old cgs system of units, in which eq. (1.9) can be written Ip = (s i )Ys EuE

(1.11)

In practice it is easier to measure speciﬁc (mass) magnetic susceptibility " rather than volume susceptibility and eq. (1.9) can be re-written, assuming that "i ?? "s : 1 (" "i )ps EuE Ip = 0 s

(1.12)

where ps is the mass of the particle. It can be seen from eqs. (1.8) to (1.12) that the magnitude of the magnetic force is proportional to the product of the magnetic ﬂux density and its gradient. This force is in the direction of the ﬁeld gradient, not of the magnetic ﬁeld. It is also clear that in a homogeneous magnetic ﬁeld, i.e. when uE = 0, the force on a particle is zero. It can also be seen from the above equations that Ip e3

(1.13)

where e the particle radius.

1.2.2

Competing forces in a magnetic separator

As has been mentioned above, magnetic force in a magnetic separator competes with various external forces such as forces of gravity and inertia, centrifugal force and hydrodynamic drag. The importance of each force is a function of the type of the separator and of the mode in which it operates. For a spherical particle of density s the gravitational force is given by: Ij = (s i )Ysj

(1.14)

where i and j are the density of the ﬂuid medium and the acceleration by gravity, respectively. The centrifugal force can be expressed as: If = (s i )$Ysu

(1.15)

where u is the radial position of the particle and $ is the angular velocity. The hydrodynamic drag force can be obtained from Stokes’s equation:

1.2. PRINCIPLES OF MAGNETIC SEPARATION

7

Figure 1.3: Hydrodynamic drag and force of gravity, as a function of particle diameter, for particles of density 5000 kg/m3 (e.g. hematite), moving in water ( = 103 Pa×s), with relative velocity y..

Ig = 6e(yi ys )

(1.16)

where is the dynamic viscosity of the ﬂuid and yi and ys are velocities of the ﬂuid and the particle, respectively. It can be seen from the last three equations that: Ij e3 > If e3 and Ig e1

(1.17)

Because some of the forces have dierent dependence on particle radius, their relative importance will vary with particle size. The dependence of the force of gravity on the third power of the particle radius means that the force of gravity will be signiﬁcant for large particles, On the other hand, the hydrodynamic drag, which in the Stokes regime depends on the ﬁrst power of particle size, will be important for small particles. This situation in depicted in Fig. 1.3 and demonstrates that the force of gravity, for this speciﬁc case, is dominant for particle diameter greater than 500 m, while for particle diameter smaller than 50 m the hydrodynamic drag is the main competing force. The magnetic force depends on the cube of particle radius and its relative importance in the process of magnetic separation is determined by the magnetic properties of the particles and by technical parameters of the magnetic separator (i.e. magnetic ﬁeld strength and its gradient). Figure 1.4 illustrates the dependence of the magnetic force on a hematite particle of magnetic susceptibility = 9.4×103 (SI) (" = 188×108 m3 /kg), as a function of particle size,

8

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.4: Magnetic force on a hematite particle in several types of magnetic separators, as a function of particle size. Table 1.1: Typical values of BuB for selected magnetic separators.

Suspended magnet 0.05

EuE[T2 /m] Nd drum Nd roll magmagnetic netic separaseparator tor 80 300

HGMS with steel wool matrix 5×104

for various types of magnetic separators. The values of the product EuE used in construction of the graph are summarized in Table 1.1. It is clear from eq. (1.9) and from Fig. 1.4 that the particle size is a more important discriminating factor in magnetic separation than the magnetic susceptibility. Since Ip e3 , even a large dierence in magnetic susceptibilities of components of a poorly classiﬁed mixture to be separated will not necessarily result in selective separation. As can be seen in Table 1.2, a particle characterized by magnetic susceptibility of 1 a.u. (arbitrary unit) and size 10 a.u. will be acted upon by the same magnetic force as a particle with susceptibility of 1000 a.u. and size 1 a.u. Selectivity of separation will be determined by the balance of the magnetic and competing forces acting on these two components. It is evident from the above discussion that the subject of magnetic separation cannot be treated without ﬁrst deﬁning the physical quantities usually encountered in magnetism, and the units in which these quantities are measured. The next sections will be devoted to these issues.

1.3. FUNDAMENTAL QUANTITIES OF MAGNETISM

9

Table 1.2: Magnetic force vs particle size. Particle size [a.u.] 10 1

1.3 1.3.1

Magnetic susceptibility [a.u.] 1 1000

Magnetic force [a.u.] 1000 1000

Fundamental quantities of magnetism and their units Magnetic ﬁeld and magnetization

When we describe a magnetic ﬁeld, we employ two dierent quantities, namely magnetic ﬁeld strength K and magnetic ﬂux density (or magnetic induction) E. K and E are both vector quantities having direction as well as magnitude. In vacuum E and K are not independent and are related by the equation = 0 K E

(1.18)

where the magnetic permeability of vacuum 0 is numerically equal to 4 ×107 H/m. In a magnetic material of magnetization P , the total magnetic induction becomes, in Sommerfeld convention, adopted by IUPAP: = 0 (K +P ) E

(1.19)

In the cgs system, since 0 = 1, eq. (1.19) becomes =K + 4 P E

(1.20)

Magnetization is deﬁned as the total magnetic moment P of dipoles per unit volume Y , i.e. P = P @Y . The factor 4 arises from the fact that a unit pole produces a unit ﬁeld everywhere on the surface of a sphere of unit radius (1 cm) enclosing the pole, and the surface of this sphere is 4 cm2 = In the Kennelly system, which is traditionally favoured by electrical engineers, E is given in SI by:

= 0 K + M E where M is the magnetic polarization. M and P are related by equation: M = 0 P

(1.21)

The magnetic induction thus includes contributions from the magnetization P , which is deﬁned as the magnetic dipole moment of a body per unit volume, or polarization M deﬁned by eq. (1.21).

10

1.3.2

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Magnetic susceptibility and permeability

The magnetization of a material, in general, depends on the magnetic ﬁeld acting on it. For many materials, P is proportional to K (at least when K is not too large) and we may write: = K P

(1.22)

where , the volume magnetic susceptibility, is a property of the material. Since P and K have the same dimensions, is dimensionless. We can combine eq. (1.22) with eq. (1.19) to get = 0 (1 + )K = 0 u K = K E

(1.23)

u = 1 + and

(1.24)

where = 0 (1 + )

The quantity u is called relative magnetic permeability and is dimensionless, while is called magnetic permeability and has a unit of H/m. While eq. (1.19) is general, eqs. (1.23) and (1.24) are based on assumption that the material is both isotropic and linear. In other words, that P is proportional to H and in the same direction. This assumption is never completely true for ferromagnetic materials. Either u or may be used to characterize a material. Volume magnetic susceptibility ranges from values close to 0, both positive and negative, to positive values greater than 1, for dierent materials. For materials that have very small susceptibilities, it is much more convenient to use than u . For instance for = 106 , u = 1.000001, and for = - 106 , u = 0.999999. Magnetic susceptibility can also be expressed with respect to the unit mass of material of density , and then "=

(1.25)

where " is the mass, or speciﬁc, magnetic susceptibility. Since a sample mass p is usually better known than its volume, mass magnetic susceptibility is very commonly employed. For the same reason the mass magnetization rather than magnetization P is often used to characterize materials. The mass magnetization is deﬁned as =

1.3.3

P thus P = p

(1.26)

Magnetic units

The units and symbols used in this book are those of the Système International d’Unités, designated SI. This system, which is based on the meter, kilogram, second, ampere, kelvin and candela, is essentially the same as the Giorgi, or MKSA, system in the ﬁeld of electromagnetism.

1.4.

MAGNETIC PROPERTIES OF MATERIALS

11

Essentially all students today are taught in SI units and most scientiﬁc journals require their contributors to use SI units. Nevertheless, many papers on magnetism - and magnetic separation is no exception - are still published in cgs units. Occasionally, the cgs system is polluted with the emu ”unit”, which is not really a unit to which dimensional analysis can be applied [S3]. Therefore, even today the ﬁeld of magnetism is not blessed with a lucid system of quantities and units and numerous panel discussions and articles on the subject illustrate the reigning chaos [C1, S4, G2]. Those authors who follow the current trend and convert cgs units to SI units ﬁnd that the task of conversion is gigantic and that errors almost always creep in. Table 1.3 lists the SI units in use for most important quantities, together with their conversion factors to electromagnetic cgs units. Conversion of magnetic induction in the cgs unit of Gauss into the SI unit of Tesla should present no di!culty, with the values in Gauss divided by 104 . When the magnetic ﬁeld strength is used, Oersted multiplied by 103 @4 (approximately 79.58) will give the value in the SI unit of A/m. Magnetic susceptibility is a more complicated quantity. It is the volume magnetic susceptibility that enters most equations used in magnetic separation. Although dimensionless in both systems of units, volume magnetic susceptibility diers by a factor of 4 in the systems of units, as can be seen in Table 1.3. Experimentally, it is easier to determine the mass magnetic susceptibility and therefore most values of magnetic susceptibility that can be found in the literature are those of mass susceptibility, often in cgs units. Various names are used for this unit, e.g. emu/cm, emu/g×Oe and cgs, but all of them usually represent the same unit, namely cm 3 /g. Thus in SI the unit is m 3 /kg and conversion factor from cgs to SI is 4×103 . The following equations summarize relationships between volume and mass magnetic susceptibilities, in both SI and cgs systems of units (density is expressed in g/cm3 ).

1.4

(VL) = 4(fjv)

(1.27)

(fjv) = "(fjv) and (VL) = 103 "(VL)

(1.28)

(VL) = 4"(fjv)

(1.29)

"(VL) =

4 "(fjv) 103

(1.30)

"(fjv) =

103 "(VL) 4

(1.31)

Magnetic properties of materials

It has been stated at the outset that all materials display certain magnetic properties, regardless of their composition and state. According to their magnetic

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

12

Table 1.3: Units of important magnetic quantities. The quantity is cgs units is obtained by multiplying the quantity in SI by the conversion factor. For instance, 1 G = 10e-4 T. Quantity Magnetic ﬁeld strength Magnetic induction (ﬂux density) Magnetization Mass magnetization Magnetic ﬂux

Symbol

SI unit

cgs unit

H

A/m

Oersted (Oe)

B

Tesla (T)

Gauss (G)

104

M

A/m

103

Am2 /kg

Oe, erg/Gcm3 emu/g

Wb (Weber)

Mx (Maxwell) G erg/G

108

Polarization Magnetic moment Volume magnetic susceptibility Mass (speciﬁc) magnetic susceptibility Demagnetization factor Energy product Permeability of vacuum Bohr magneton

J P

Nuclear magneton Anisotropy constant

Q

Tesla (T) Am2

dimensionless dimensionless, emu/cm3 Oe

"

m3 /kg

N

dimensionless dimensionless

BH 0

J/m3 H/m

E

9.274×1024 Am2 5.051×1027 Am2 J/m3

K

cm3 /g

GOe 1 (dimensionless)

erg/cm3

Conversion factor 103 @4

1

104 103 4 4 · 103

1/4 1/40 4 · 107

101

1.4.

MAGNETIC PROPERTIES OF MATERIALS

Paramagnetic

Ferromagnetic

Antiferromagnetic

Ferrimagnetic

13

Figure 1.5: Schematic diagram of the alignment of magnetic moments. properties, materials can be divided into ﬁve basic groups: diamagnetic, paramagnetic, ferromagnetic, antiferromagnetic and ferrimagnetic. The last three groups have generally higher magnetic susceptibilities than the other groups and are frequently termed ”ferromagnetic” sensu lato (s.l.). This broad deﬁnition must be distinguished from one of its subdivisions, ferromagnetic sensu stricto (s.s.) [T1] as discussed below. The alignment of magnetic moments in each type of material is shown in Fig. 1.5. The classiﬁcation of magnetism in terms of magnetic permeability is given in Table 1.4.

1.4.1

Diamagnetism

Diamagnetism has its origin in the modiﬁcation of the electron orbit magnetic moment by an external magnetic ﬁeld. The currents thus induced give rise to an extra magnetic moment. However, according to Lenz’s law, the resulting magnetic moment is in the opposite direction to the ﬁeld that has induced the current. Therefore, approaching a source of the magnetic ﬁeld, a diamagnetic material is repelled from it. This eect is present in all materials, independently of temperature. Diamagnets have a very small and negative volume magnetic susceptibility, of the order of - 105 (SI). While many inorganic and almost all organic molecules are diamagnetic, in many materials their diamagnetism is hidden by a much stronger paramagnetic/ferromagnetic (s.l.) eect. This is, for instance, the case of metals that are normally associated with small negative susceptibility, often overwhelmed by positive paramagnetic or ferromagnetic contribution. The values of selected diamagnetic metals and non-metallic compounds are given in Table 1.5. Table

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

14

Table 1.4: Magnetic susceptibility in various types of magnetism. Parameter

Diamagnetism

Susceptibility Relative permeability

?0 ?1

Paramagnetism Ferromagnetism Antiferromag- Ferrimagnetism netism 0 AA 0 1 AA 1

Table 1.5: Magnetic susceptibilities of diamagnetic materials. [SI] × 105 -1.0 -1.4 -3.6 -1.56 -2.0 -0.9 -0.73

Material Copper Zinc Gold Lead Diamond Water Ethylalcohol

"[m3 @kg] × 109 -1.1 -1.96 -1.86 -1.38 -5.6 -9.0 -9.3

1.6 summarizes the magnetic susceptibilities of various diamagnetic minerals.

1.4.2

Paramagnetism

In paramagnetic materials the magnetic atoms or ions have permanent intrinsic magnetic moments and occur in low concentrations. Susceptibility arises from the competition between the aligning eect of the applied magnetic ﬁeld and the randomizing eect of thermal vibrations. In zero applied magnetic ﬁeld, the moments point in random directions. When a ﬁeld is applied, a small magnetization develops, but the magnetic susceptibility is very small and is inversely proportional to the absolute temperature. In the presence of the external magnetic ﬁeld, and under standard practical conditions (i.e. when P [email protected] ?? 1, where P is the magnetic moment, n is the Boltzmann constant and T is the absolute temperature) the magnetization of a paramagnetic material is f q2 K P (1.32) = 0 P nW where f is a constant and q is the number of magnetic dipoles. The susceptibility of paramagnetic materials is then given by =

F f0 q2P = nW W

(1.33)

1.4.

MAGNETIC PROPERTIES OF MATERIALS

15

Table 1.6: Mass magnetic susceptibilities of assorted diamagnetic minerals. Mineral

Quartz Calcite Sphalerite Galena Baddeleyite Barite Magnesite Apatite Fluorite Halite Kaolinite

Chemical formula

SiO2 CaCO3 ZnS PbS ZrO2 BaSO4 MgCO3 Ca5 [PO4 ]3 (F,Cl) CaF2 NaCl Al4 Si4 O10 (OH)8

Mass magnetic susceptibility [m3 /kg]×109 - 6.0 - 4.8 - 3.2 - 4.4 - 1.4 - 3.8 - 6.4 - 3.3 - 7.9 - 9.0 - 20.0

where F is the Curie constant. Equation (1.33) is called the Curie law, which states that magnetic susceptibility of the paramagnetic substance is inversely proportional to the temperature. The paramagnetic susceptibility is always small ( 105 to 103 (SI)), although paramagnetism can be several orders of magnitude larger than diamagnetism. As follows from eq. (1.32), the dependence of the magnetization of a paramagnetic material on the ﬁeld strength is expressed by a straight line. In most cases, in standard conditions such as W = 300 K and E = 1 T, the above formulae apply. In extreme conditions, such as at cryogenic temperatures and very high magnetic ﬁeld, a saturation eect appears. Taking into account eq. (1.23), it transpires from eq. (1.32) that for paramagnetic materials the magnetic susceptibility is independent of the magnetic ﬁeld. Table 1.7 summarizes the values of magnetic susceptibility for selected paramagnetic metals and compounds, while Table 1.8 lists susceptibilities of assorted paramagnetic minerals. Compilations of susceptibility of minerals are numerous [A1, S1, K2, D2] and large variations can be observed. Conﬂicting data can be explained by the inherent variability in mineral composition and the presence of inclusions and contaminants. Dierent measuring techniques tend to give diering values of susceptibility [M1] and the usage of dierent systems of units also contributes to frequent inconsistency of the values of magnetic susceptibility found in the literature.

1.4.3

Ferromagnetism

In ferromagnetic materials (s.s.) interaction between neighbouring atoms is strong so that the magnetic moments of all atoms are aligned parallel to each other against the randomizing force of thermal motion. The strong internal

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

16

Table 1.7: Magnetic susceptiblities of paramagnetic materials. Material

Aluminium Chromium Titanium Vanadium Platinum Zirconium CuSO4 ·5H2 O NiSO4 ·7H2 O MnO

Mass magnetic susceptibility [m3 /kg]×109 7.67 42.0 42.2 73.0 12.3 16.7 76.7 201 860

Volume magnetic susceptibility [SI]×105 2.1 30.2 19.0 44.5 26.4 10.8 17.5 39.8 445.5

Table 1.8: Magnetic susceptibilities of paramagnetic minerals. Mineral

Chemical composition

Hematite Siderite Goethite Ilmenite Rutile Wolframite Pyrite Limonite Manganite Pyroxene Dolomite

Fe2 O3 FeCO3 FeOOH FeTiO3 TiO2 (Mn,Fe)WO4 FeS2 Fe2 O3 ·nH2 O MnO2 ·Mn(OH)2 (Mg,Fe)2 Si2 O6 CaMg(CO3 )2

Mass magnetic susceptibility [m3 /kg]×109 250 - 3800 350 - 1500 250 - 400 200 - 1500 10 - 50 350 - 1200 3 - 200 100 - 400 100 - 500 40 - 1000 5 - 20

ﬁelds, which align the spins, are called molecular or Weiss ﬁelds. These ﬁelds are the result of a quantum mechanical process called exchange interaction. Weiss assumed that the molecular ﬁeld is very large, its magnitude independent of external magnetic ﬁeld, and its direction not ﬁxed, but always parallel to the magnetization. The Weiss hypothesis predicts that a material can be spontaneously magnetized even in the absence of an applied magnetic ﬁeld at temperatures below the Curie temperature, at which the thermal agitation overcomes the molecular ﬁeld. This tendency aids the external ﬁeld in producing saturation, i.e. complete alignment. There is an apparent contradiction between theory, which explains that magnetic materials are fully magnetized even in the absence of an external ﬁeld, and practice, which generally shows that such materials exhibit no magnetization or magnetization much smaller than saturation. In fact, theory is correct at a mi-

1.4.

MAGNETIC PROPERTIES OF MATERIALS

17

Figure 1.6: Temperature behaviour of various classes of magnetic materials. croscopic level, but at a macroscopic scale the ferromagnetic body is subdivided into Weiss domains, each of which is spontaneously magnetized to saturation, but not in the same direction, by virtue of a strong exchange magnetic ﬁeld. Inside a domain the magnetization is at a maximum (saturation), but as all domains compensate each other, on macroscale the mean magnetization is nil. The value of the saturation magnetization varies with temperature, decreasing from a maximum value at W = 0 K, becoming zero at the Curie temperature Wf . Above Wf , the behaviour is similar to that of a paramagnetic material, with the magnetization being proportional to the ﬁeld and the susceptibility decreasing with increasing temperature. However, the susceptibility does not follow the Curie law, eq. (1.33), but varies as =

F W Wf

(1.34)

Equation (1.34) is called the Curie-Weiss law. The temperature behaviour of various types of magnetism is shown in Fig. 1.6. In contrast to diamagnetic and paramagnetic materials, magnetization of ferromagnetic materials (v=o=) depends not only on the ﬁeld strength, but also on the shape and the magnetic history of the sample. For instance, a ferromagnetic material can remain magnetized after removal of the external ﬁeld. The ferromagnetics (s.l.) are thus characterized by hysteresis as is illustrated in Fig. 1.7.

18

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.7: Hysteresis loop of a ferromagnetic (s.l.) material.

It can be seen in Fig. 1.7 that two kinds of the magnetic curve (or hysteresis loop) can be determined. The induction curve is E = E(K)> while the magnetization (or intrinsic) curve illustrates the P = P (K) dependence. Since E = 0 (P + K), and since P is much greater than K in most parts of the initial magnetization curve (curves OP and OQ, respectively, in Fig. 1.7), both curves are comparable. The dierence occurs mainly in the saturation region where P (K) is asymptotic to Pv , while E(K) approaches 0 (Pv + K). It can be seen in Fig. 1.7 that after the initial (or virgin) magnetization reaches its saturation value Ev or Pv , (points P and Q, respectively), irreversibility, resulting from imperfections in the material, prevents the magnetization (or the induction) from returning to zero when the external ﬁeld is removed. Magnetization and induction at K = 0 are called remanent magnetization, or remanent induction, respectively. By reversing the direction of the external ﬁeld K, the residual induction and magnetization decrease to zero for particular ﬁelds Kf and Kfl called coercive force and intrinsic coercive force, respectively. As can be seen in Fig. 1.7, Kf is not the same for P (K) and E(K) curves. For low-Kf materials (soft magnetic materials) the dierence is generally negligible, while for hard material or permanent magnets (high Kf ) the dierence becomes signiﬁcant. Magnetic permeability, deﬁned as = [email protected], can vary widely at various points on the magnetizing and demagnetizing portions of the hysteresis loop. The initial permeability l and the maximum permeability max are important

1.4.

MAGNETIC PROPERTIES OF MATERIALS

19

Figure 1.8: The initial magnetization curve and permeabilities of a ferromagnetic material.

parameters that can be determined as the slopes of the magnetization curve as shown in Fig. 1.8. The initial permeability illustrates the behaviour of the permeability when the external magnetic ﬁeld approaches zero. With increasing magnetic ﬁeld the permeability of the ferromagnetics (s.l.) increases and reaches its maximum. With further increase of the magnetic ﬁeld permeability decreases and the relative permeability asymptotically approaches unity. This trend is shown in Fig. 1.9 which illustrates the dependence of the relative permeability on the external magnetic ﬁeld for decarburized steel used for magnetic yokes [B1]. In a similar way we can deﬁne magnetic susceptibility of a ferromagnetic material, taking account relationship (1.24). Magnetic susceptibility has a similar trend as permeability, and at a high magnetic ﬁeld it asymptotically approaches zero. Ferromagnetism occurs in nine elements: three transition metals, iron, cobalt and nickel, and six rare earth metals, gadolinium, terbium, dysprosium, holmium, erbium and thulium. Most alloys consisting of the three transition metals are ferromagnetic, and so are many of their alloys with non-magnetic elements. Many alloys of manganese with non-magnetic elements are also ferromagnetic, although manganese is not ferromagnetic in the pure state. On the other hand, there is no mineral that would possess ferromagnetic properties. The values of magnetization and of the Curie temperature for three ferromagnetic elements (v=v) and other ferromagnetic materials are given in Table 1.9.

20

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.9: Permeability of decarburized steel used for manufacture of magnet yokes [B1].

Table 1.9: Magnetization and Curie temperatures of ferromagnetic materials. Material Iron Nickel Cobalt Armco Si-Fe Permalloy 45 Permendur Mumetal

Magnetization 0 Pv [T] at 0 K 2.18 0.64 1.81 2.11 1.97 1.6 2.45 0.8

Curie temperature Tf [0 C] 770 358 1120

1.4.

MAGNETIC PROPERTIES OF MATERIALS

1.4.4

21

Antiferromagnetism

Antiferromagnetic materials were originally thought of as a class of anomalous paramagnets, since they have small positive susceptibilities of similar magnitude to many materials of the latter class. However, their magnetic susceptibility does not increase steadily as the temperature decreases all the way to absolute zero. At high temperatures they follow the relationship =

F W + WQ

(1.35)

where WQ is the so-called Néel temperature. At this critical temperature the susceptibility ceases to obey eq. (1.35) and below WQ the susceptibility generally decreases with decreasing temperature. The situation is depicted in Fig. 1.6. In the original Néel’s theory, an antiferromagnetic substance was envisaged as composed of two sublattices, one of whose spins tend to be antiparallel to those of the other. Néel assumed the magnetic moments of the two sublattices to be equal, so that the net moment of the material was zero, as is schematically shown in Fig. 1.5. Since Néel’s original hypothesis the term antiferromagnetism has been extended to include materials with more than two sublattices and those with triangular, spiral and canted spin arrangements. Antiferromagnetism occurs mostly in transition metal oxides, such as MnO, CoO and NiO, as well as in other similar compounds such as sulphides and selenides. Antiferromagnets have small (1010 to 108 m3 /kg) positive susceptibilities and hematite is one of the minerals that possess antiferromagnetic properties.

1.4.5

Ferrimagnetism

In a ferrimagnetic material magnetic moments are ordered regularly in an antiparallel sense, but the sum of the moments pointing in one direction exceeds those pointing in the opposite direction. This situation is illustrated in Fig. 1.5. The magnetic properties of ferromagnets and ferrimagnets are generally similar: both exhibit saturation and their magnetization is much greater than that of other magnetic classes. Ferrimagnetism occurs mainly in ferrites, mixed oxides of iron and of other elements, and also in two of the oxides of iron, namely magnetite Fe3 O4 and maghemite Fe2 O3 . The shapes of magnetization curves of various classes of materials are shown in Fig. 1.10 and a summary of magnetic properties of materials is given in Table. 1.10.

1.4.6

Demagnetization

It was previously stated that the magnetic properties of ferromagnetic (v=o=) particles also depend on the shape of the body. The magnetic ﬁeld Kl inside a magnetized body is not equal to the ﬁeld applied to it (K0 ). The magnetization of a ferromagnetic body of a ﬁnite size will produce a magnetic ﬁeld inside the

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

22

Table 1.10: Classiﬁcation of materials according to their magnetic properties. Class Diamagnetic

Critical temperature None

Paramagnetic

None

Ferromagnetic

Curie temperature Wf Néel temperature WQ

Magnitude of [SI] Approximately 106 to 5 - 10 Approximately + 105 to + 103 Large, e.g. A 1 (below Wf ) As paramagnetic

Curie temperature Wf

As ferromagnetic

Antiferromagnetic

Ferrimagnetic

Temperature variation of Constant = [email protected] Above Wf F W Wf

=

Above WQ F = (W ±W with l) Wl 6= WQ below WQ decreases, anisotropic Above Wf F (W ±Wl ) with W 6= Wl

body in a direction opposite to that of the magnetization. The induced ﬁeld is called the demagnetizing ﬁeld Kg because it always tends to oppose the applied ﬁeld K0 . The situation is depicted in Fig. 1.11. The magnitude of Kg is proportional to that of magnetization P : g = Q P K

(1.36)

where Q is the dimensionless constant of proportionality called the demagnetization factor. The value of Q varies from zero to unity, depending upon the shape of the material and the direction of magnetization. The resulting magnetic ﬁeld inside the body is given by l = K 0 + K g = K 0 QP K

(1.37)

In general, the calculation of Q is quite complex and numerical values for various shapes can be found e.g. in [B2, B3, D3]. With increasing aspect ratio, with the major axis parallel to the ﬁeld, the demagnetization factor decreases. For a sphere Q = 1/3, while for the inﬁnitely long cylinder whose axis coincides with the direction of the ﬁeld, Q = 0. For a thin disc, perpendicular to the ﬁeld, the demagnetization factor achieves its maximum value, Q = 1. For a linear soft magnetic material, for which P = K> eq. (1.37) can be re-written l = K

1 0 K 1 + Q

l = 0 and E

1 0 K 1 + Q

(1.38)

1.4.

MAGNETIC PROPERTIES OF MATERIALS

23

Figure 1.10: Shapes of the magnetization curves of various classes of materials (not in scale).

Figure 1.11: The demagnetizing ﬁeld in a short magnetic sample.

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

24

In the studies of mineral magnetism it is important to distinguish extrinsic susceptibility h , which is the susceptibility that is conventionally measured by most instruments, from intrinsic susceptibility lq > which is the true susceptibility after removal of the eects of internal demagnetizing ﬁelds [T1]. These susceptibilities are related by the following equation: h =

1.4.7

lq 1 + Q lq

(1.39)

Mixtures containing ferromagnetic (s.l.) materials

In magnetic separation, many weakly magnetic materials contain ferromagnetic (v=o=) impurities. As a result of a high magnetic permeability of most ferromagnetic (v=o=) materials, the bulk magnetic susceptibility of a weakly magnetic mineral will be determined by the concentration of ferromagnetic impurities. For such a mixture the observed magnetic susceptibility is given by h =

flq (1 + Q lq )

(1.40)

where f is the volume concentration of the ferromagnetic (v=o=) material. Contributions of various ferromagnetic (v=o=) and paramagnetic minerals to the total susceptibility of a mixture is shown in Fig. 1.12 [T1]. Since the magnetic permeability and susceptibility of a ferromagnetic (v=o=) material is a function of the magnetic ﬁeld, the deﬁnition of magnetic susceptibility is determined by measuring techniques used to determine the susceptibility. The most frequently quoted value is the initial susceptibility (or permeability) l as shown in Fig. 1.8. For strongly susceptible materials, such as magnetite, h = [email protected] , and the initial susceptibility can be written: f Q For spherical particles Q = 1/3 and thus l =

(1.41)

l 3f

(1.42)

while for ovoid particles, with the ratio of long and short axes of 10, the susceptibility is [L1, T1]: l 18f

(1.43)

Although the magnetic susceptibility of paramagnetic material is independent of the magnetic ﬁeld, minerals displaying various forms of magnetic order (i.e. ferromagnets (v=o.)), or paramagnetic minerals containing the admixtures of the magnetically ordered materials, exhibit a ﬁeld-dependent magnetic susceptibility. This phenomenon can seriously alter the predictions of the results of magnetic separation based on the ﬁeld-independent magnetic susceptibility. The measured magnetic susceptibility, in a relatively low applied magnetic ﬁeld (E? 0.6 T), can be represented by the Owen-Honda equation [O1, H1]:

1.5. MAGNETIC PROPERTIES OF MINERALS

25

Figure 1.12: Contribution of various minerals to the total susceptibility of a mineral mixture [T1].

Pv Pv = 4 + (1.44) K K where s and g are paramagnetic and diamagnetic susceptibilities, respectively, 4 is the magnetic susceptibility extrapolated to the inﬁnite magnetic ﬁeld, and Pv is the saturation magnetization of the ferromagnetic (v=o=) component of the mixture. It has been experimentally determined ([N2, P2]) that 4 is characteristic of a mineral, and is nearly constant for samples of the same mineral from dierent localities. On the other hand, saturation magnetization Pv , which indicates the degree of weak ferromagnetism, varies widely between samples from diering localities and between size fractions of the same sample. = s + g +

1.5 1.5.1

Magnetic properties of minerals The classiﬁcation of minerals according to their magnetic properties

Although all matter responds to the presence of the external magnetic ﬁeld, the degree of this response varies widely. For practical reasons the technical classiﬁcation of materials, and particularly of minerals, diers from physical

26

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

categorization discussed in previous sections. For the purposes of magnetic separation, materials can be divided into three basic groups: Strongly magnetic materials can be recovered by a magnetic separator with the use of a relatively weak magnetic ﬁeld, up to, for example, 0.15 T, with a modest ﬁeld gradient of the order of 0.5 T/m. The magnetic susceptibility that responds to such a low magnetic ﬁeld is generally greater than 104 m3 /kg and ferromagnetic and ferrimagnetic materials like mild steel, iron, magnetite, maghemite and pyrrhotite fall under this group. Weakly magnetic materials can be recovered by a magnetic separator that generates magnetic induction up to 1.0 T, and the ﬁeld gradient in the range from 50 to 500 T/m. This broad group of materials includes antiferromagnetic, paramagnetic and some ferrimagnetic minerals. The group comprises iron and manganese oxides and carbonates, ilmenite, wolframite and other materials. Magnetic susceptibility of these materials ranges from 107 m3 /kg to 5×106 m3 /kg. ”Non-magnetic" materials are those materials that cannot be easily recovered by conventional magnetic separators. They include very weakly paramagnetic and antiferromagnetic materials with magnetic susceptibility smaller than, for example, 107 m3 /kg. Austenitic stainless steel, aluminium, rutile, pyrite, garnet and red blood cells belong to this group. Diamagnetic materials, with their negative magnetic susceptibility are also included. This classiﬁcation is only conditional as it does not take into account such an important variable as particle size, which, as we have seen in Section 1.2.2, is as important as magnetic susceptibility in determining the e!ciency of magnetic separation. Recent developments and innovation in magnetism extended the range of materials that can be treated by the magnetic means to such a degree that all classes of matter are included, down to the submicrometer or even nanosize range.

1.5.2

Magnetite

Magnetite Fe3 O4 is the most fundamental and important magnetic mineral. It has a cubic crystalline structure in which Fe3+ and Fe2+ cations form two distinct lattices. Each of the lattices is magnetized in opposite directions and magnetite behaves as a ferrimagnetic mineral . The saturation polarization of magnetite at room temperature ranges from 0.55 T to 0.61 T and the Curie temperature is 575 0 C. The density of pure Fe3 O4 is 5200 kg/m3 , calculated from the cell dimensions [N1]. As has been mentioned earlier, magnetic properties of magnetically ordered mineral grains depend, among other things, on the grain size. The most important distinction is between very small particles, each of which is a single domain, and large grains, which are multidomain. For any material there is a maximum size for spherical simple domain, referred to as the critical size. For magnetite this critical size is about 0.05 m [S5], while for hematite, for instance, this value is much higher, of the order of 200 to 300 m [N1].

1.5. MAGNETIC PROPERTIES OF MINERALS

27

Figure 1.13: Magnetic susceptibility and coercive force of ferromagnetic particles, as a function of grain size. The variation of the coercive force Kf with particle diameter g, in granular magnetic materials and over a wide range of grain sizes, is well represented by the relationship Kf gq

(1.45)

The value of q is usually in the range between 0.25 and 1. The eect of transition from single domain to multidomain structure, on magnetic properties of a ferromagnetic grain, is illustrated in Fig. 1.13. This Figure shows that, at the transition between multidomain and single domain arrangement, magnetic susceptibility achieves its minimum, while the coercive force is maximum. A simpliﬁed dependence of the coercive force and mass magnetic susceptibility on particle diameter is shown in Fig. 1.14. Fig. 1.15 illustrates the dependence of the mass magnetic susceptibility of magnetite on the external magnetic ﬁeld, ranging from 0 to 240 kA/m (0 to 3 kOe). The data reported in [P1] were obtained with size fraction - 74 + 53 m.

1.5.3

Titanomagnetites

Titanomagnetites Fe3{ Ti{ O4 are one of the most common magnetic minerals. Magnetic susceptibility, saturation magnetization and Curie temperature vary in a regular manner with the composition parameter { from { = 0 (magnetite)

28

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.14: Dependence of the coercive force and magnetic susceptibility of magnetite on the particle size (after Derkach [D4]).

Figure 1.15: The ﬁeld dependence of the magnetic susceptibility of magnetite (adapted from Derkach [D4]).

1.5. MAGNETIC PROPERTIES OF MINERALS

29

Figure 1.16: Variation of the room temperature magnetic susceptibility with composition, for titanomagnetites (after [O1]).

to { = 1 (ulvöspinel). The variation of the initial magnetic susceptibility with composition, for three size fractions, is shown in Fig. 1.16 [O1]. Fig. 1.17 illustrates the dependence of the initial magnetic susceptibility on particle size, for assorted compositions of titanomagnetites.

1.5.4

Ilmenohematites

Titanium-rich ilmenohematites Fe2| Ti| O3 are signiﬁcant magnetic minerals, as their susceptibilities are more than two to three orders of magnitude greater than those of paramagnetic minerals. Ilmenite FeTiO3 is antiferromagnetic below the Néel temperature of 55 K. Above the Néel temperature ilmenite is paramagnetic [N1] and its magnetic susceptibility (approximately 5×103 (SI) or 10×107 m3 /kg) is somewhat lower than for other members of the series [T1, D2], and was found to be essentially independent of the magnetic ﬁeld strength in the range from 0.1 T to 9 T [D2]. Magnetic susceptibility measured below the Néel temperature (at 4.3 K) was found to be equal to 150×107 m3 /kg at magnetic ﬁelds smaller than 0.6 T. At higher magnetic ﬁelds the value of the susceptibility dropped to about 100×107 m3 /kg [D2]. Figure 1.18 illustrates the variation of the saturation magnetization of ilmenohematite samples of particle size of 9.8 m, at room temperature, with composition [O2]. It can be seen that ilmenite (| = 0) is one of the magnetically weakest members with saturation polarization of approximately 0.012 T.

30

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.17: Variation of the initial magnetic susceptibility, at room temperature, with grain size, for titanomagnetites (after [O1]).

Figure 1.18: Saturation magnetization of ilmenohematites as a function of their composition (after [O2]).

1.5. MAGNETIC PROPERTIES OF MINERALS

31

Figure 1.19: Magnetic susceptibility of hematite as a function of the applied magnetic ﬁeld (after [N2]).

1.5.5

Maghemite

The magnetic properties of maghemite (-Fe2 O3 ) are very similar to those of magnetite (albeit slightly less pronounced). Both minerals have fundamentally the same spinel structure, although the composition of maghemite is essentially that of hematite. Maghemite is metastable and converts to hematite at temperatures in the range from 300 0 C to 350 0 C. The saturation polarization at room temperature ranges from 0.48 T to 0.51 T.

1.5.6

Hematite

Pure hematite -Fe2 O3 has antiferromagnetic structure above the Néel temperature of approximately 680 0 C. Between the Néel temperature and the Morin temperature WP = - 100 0 C hematite is a canted antiferromagnet (”weak ferromagnet”). At room temperature, the magnetic polarization is about 0.5 % that of magnetite, i.e. between 15×104 to 30×104 T. The weak ferromagnetism (v=o=) of hematite is not fully understood because of its complex and contradictory behaviour. The properties vary from sample to sample and depend on their origin. For instance, the ratio of the remanent polarization to saturation polarization MU @MV for ﬁne hematite, ranges from close to zero to about 0.8 [A2]. The coercive force of ﬁne hematite is very high, up to 2.5×105 A/m, in contrast to the low values of the order of 8×102 A/m [S5, D5], observed with crystals, which were a few millimeters in size.

32

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.20: The eect of temperature and magnetic ﬁeld on the magnetic susceptibility of specularite (after [P2]). Hematite is also strongly anisotropic, i.e. crystals can be magnetized by magnetic ﬁelds applied along the basal plane, but are almost unaected by ﬁelds perpendicular to this plane, unless extremely strong ﬁelds are employed [T1]. Hematite also tends to ﬂake parallel to its basal plane and the ﬂakes are often termed specularite. The magnetic susceptibility of pure hematite is a complicated function of particle size, magnetic ﬁeld, and temperature, determined by the interplay between contributions from weak ferromagnetism and antiferromagnetism [D5]. The eects of magnetic ﬁeld strength and temperature on magnetic susceptibility are shown in Figs. 1.19 and 1.20, respectively. A signiﬁcant change in magnetic susceptibility for magnetic ﬁelds smaller than 8×105 A/m (10 kOe) can be seen in Fig. 1.19. The ﬁeld-independent magnetic susceptibility 4 was found to be equal to 1.43×103 (SI) [N2]. Pastrana and Hopstock [P2] investigated the eect of temperature and magnetic ﬁeld on magnetic susceptibility in terms of eq. (1.44). They found that 4 increased only slightly with temperature but the eect of temperature on was dramatic, as illustrated by Fig. 1.20.

1.5.7

Goethite

Goethite (FeOOH) is an antiferromagnetic mineral, which ideally should have perfectly compensated spins, and hence no net spontaneous magnetic moment. It appears, however, that one of the sublattices is usually canted; as a result the mineral behaves ferrimagnetically. It has a magnetization greater

1.5. MAGNETIC PROPERTIES OF MINERALS

33

Table 1.11: Some physical properties of ferromagnetic (s.l.) minerals. Mineral

Magnetite Maghemite Hematite Goethite Pyrrhotite Chromite

Composition

Fe3 O4 Fe2 O3 Fe2 O3

Curie/Néel temperature [r C] 575 350 680

FeOOH

120 - 130

FeS FeCrO4

320 - 84

Saturation polarization [T] 0.59 - 0.61 0.48 - 0.51 10×104 to 30×104 50×107 to 50×104 0.1 1.9×105

Density [kg/m3 ] 5200 4800 5300 4300 4600 5090

than that of hematite but weaker than that of magnetite. Goethite also has a high coercivity, comparable to that of hematite. The mass magnetic susceptibility ranges from 2.5×107 m3 /kg to 6×107 m3 /kg [A1, P2]. The temperature and the magnetic ﬁeld dependence of the magnetic susceptibility of goethite, as reported by Pastrana and Hopstock [P2] is shown in Fig. 1.21. Physical properties of selected ferromagnetic (v=o) minerals, including goethite, are summarized in Table 1.11.

1.5.8

Siderite

Siderite FeCO3 undergoes an antiferromagnetic transition at the Néel temperature of about 14 K. When heated under oxidizing conditions, it decomposes into minerals such as maghemite, magnetite and iron hydroxide. The ﬁnal decomposition product is hematite [B4]. Results of extensive measurements of magnetic susceptibility of samples of siderite (- 150 + 105 m) at room temperature [P3] show that the susceptibility does not vary with the applied magnetic ﬁeld. The susceptibility ranges from 8×107 m3 /kg to 11×107 m3 /kg and similar values were reported in [T1, M2].

1.5.9

Iron sulphides

Iron sulphides exhibit magnetic properties over a narrow range of speciﬁc compositions, but these are strongly aected by impurities, grain size and similar factors. Pyrrhotite (FeS1+{ for 0.10 ? { ? 0.14) is the most common ferromagnetic (v=o=) iron sulphide. Most of these minerals are chemically unstable on heating and the Curie temperature of pyrrhotite, 320 0 C, is almost the same as the temperature at which is decomposes to magnetite [T1]. As in hematite, the spin structure consists of ferromagnetic order, the magnetic moments of adjacent planes being coupled parallel. Unlike hematite, the moments of the planes dier in magnitude and a strong ferrimagnetism results [O2]. Pyrrhotite is generally more strongly magnetic than hematite and the

34

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.21: Magnetic susceptibility of goethite as a function of magnetic ﬁeld strength and temperature (after [P2]). saturation polarization, at room temperature, is about 0.12 T [O2], although smaller values are often found in literature (e.g. [T1]). The magnetic ﬁeld dependence of the mass magnetic susceptibility is shown in Fig. 1.22 [D4].

1.5.10

Chromites

The magnetic properties of natural chromium-bearing spinels or chromites (Fe, Mg)(Cr,Al,Fe)2 O4 are highly variable, the variation being closely related to the variation in their chemical composition. It is frequently assumed that the magnetic susceptibility and the hysteresis behaviour of chromites is controlled by the end-member magnetite [H2, S6]. The magnetic susceptibility is reported to range from 6×107 m3 /kg to 30×107 m3 /kg at 4.3 K [D2] and from 5×107 m3 /kg to 12×107 m3 /kg at elevated temperatures (78 and 136 K) [D2, S6].

1.6

Measurement of magnetic properties

This section brieﬂy describes experimental techniques used for the measurement of magnetic quantities. There are hundreds of dierent techniques and their modiﬁcations, each having distinct merits as well as limitations. There is no single technique which is universally applicable to all types of measurements. There are several comprehensive sources of information [Z1, F2, B5, B6, C2] that provide a good starting point in the pertinent literature. It is interesting

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

35

Figure 1.22: Mass magnetic susceptibility of pyrrhotite as a function of the magnetic induction (after [D4]). to note that while the measurement methods have remained virtually unchanged for a long period, the equipment has been subjected to continuous development. Practitioners as well as researchers who use magnetic techniques as a tool for mineral beneﬁciation, material concentration or removal will be interested primarily in the measurement of the magnetic ﬁeld strength and its gradient and of magnetic susceptibility. There is a wide range of measuring instruments commercially available, some of them easily aordable and suitable for ﬁeld applications.

1.6.1

Measurement of the magnetic ﬁeld strength

There are several ways of measuring the magnetic ﬁeld strength or magnetic induction. The choice of the measurement method depends on several factors. The ﬁeld strength, its non-homogeneity, as well as the required accuracy all need to be considered. Figure 1.23 shows the accuracy of absolute measurements of magnetic ﬁeld strength for a few commonly used methods. The ﬂuxmeter method This method, which is based on Faraday’s induction law, is one of the oldest, and still very accurate, techniques of the ﬁeld measurement. It consists of placing a coil in the magnetic ﬁeld so that part of that ﬁeld is enclosed as a magnetic ﬂux through the coil area. Switching o the ﬁeld or removing the coil from the ﬁeld gives rise to an induction voltage across the coil terminals. The ﬂux is

36

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.23: Measurement of the magnetic ﬁeld strength: accuracies and ranges of various methods [H3]. then measured as the time integral of the voltage produced. Measurements are performed either by using ﬁxed coils in a dynamic magnetic ﬁeld, or by moving the coils in a static ﬁeld. The Hall Eect method E.H. Hall discovered in 1879 that a metal strip immersed in a transverse magnetic ﬁeld and carrying a current developed a voltage mutually at the right angle to the current and the voltage that opposed the Lorentz force on the electrons. The Hall-probe meters, known as gaussmeters, use very simple electronic instrumentation and provide an instant measurement. The small size of the probe sensing area (1 mm2 and less), its static physical characteristics, as no motion of the probe is required, and there are no moving parts, make gaussmeters very useful instruments. The basic premise of the Hall probe is that when a current L is ﬂowing along one axis of a conductor or semiconductor, and when the magnetic ﬁeld E is applied perpendicularly to the plane of the probe (or generator), then the Hall voltage XK given by eq. (1.46) is generated perpendicular to both the current and the magnetic ﬁeld. The situation is depicted in Fig. 1.24. L ·E (1.46) g where g is the thickness of the Hall generator and UK is the Hall constant. The Hall voltage is thus, in the ﬁrst approximation, proportional to the XK = UK

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

37

B FL

UH v

B

d

I +

Figure 1.24: Schematic representation of the Hall-eect probe.

ﬂux density. The Hall constant depends on various material parameters as well as temperature and, to a small extent, on the ﬂux density E. The resulting linearity error is kept as small as possible by applying an appropriate ohmic resistor to the Hall voltage. This allows the construction of measuring devices that are linear to within ±1 % for a ﬂux density of about 1 T. Equally important for accuracy is the eect of the temperature coe!cient of the Hall voltage. The Hall probes, usually made using indium arsenide, are very fragile. The Hall element is generally only a few hundredths of a millimeter thick and needs mechanical support. Aluminium is usually used as a substrate. The Hall probes can be used to measure d.c. ﬁelds, a.c. ﬁelds and pulsed magnetic ﬁelds. The probes are available in various shapes and their use depends on the direction of the magnetic ﬁeld to be measured. The probes are either transverse or axial. With the transverse probe, the ﬂux density is measured perpendicular to the probe rod, while with the axial probe the measured magnetic ﬁeld is in the direction of the probe axis. The overall views of hand-held and bench-scale gaussmeters are shown in Figs. 1.25 and 1.26. In order to generate a high magnetic force on particles to be separated, the magnetic ﬁeld in magnetic separators is generally very non-uniform. The value of the magnetic ﬁeld thus changes considerably, often over a scale of several hundreds of micrometers, particularly in high-gradient type magnetic separators such as HGMS, or permanent magnet roll separators. In view of the ﬁnite size of the Hall sensing element, it is the mean magnetic ﬁeld over the relatively large cross-sectional areas of the sensor, and not the maximum ﬁeld, that is being measured by the Hall probe. With common commercially available Hall probes the measured magnetic ﬁeld is usually much less than the maximum ﬁeld. For instance, magnetic induction usually measured in an NdFeB permanent magnetic roll separator rarely exceeds 1 T, while a special Hall microprobe can

38

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.25: A portable hand-held gaussmeter (courtesy of Walker LDJ Scientiﬁc, Inc.).

Figure 1.26: A precision laboratory gaussmeter (courtesy of Walker LDJ Scientiﬁc, Inc.).

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

39

measure the ﬁeld as high as 1.9 T. Such values agree with the ﬁeld strength obtained in computer modelling. The above discussion indicates that it is rather di!cult to measure accurately the magnetic ﬁeld gradient in a magnetic separator. Although the knowledge of the spatial distribution of the magnetic ﬁeld and its proﬁle is important for serious understanding of the process of magnetic separation and of the design of magnetic separators, commercial Hall probes are usually unsuitable for this exercise. However, commercially available gaussmeters can be used for measurements of the magnetic ﬁeld gradient in a low-gradient class of magnetic separators, such as magnetic pulleys and suspended magnetic separators. Accuracy of the measurement can be enhanced by devising a measuring rig [S7].

1.6.2

Measurement of magnetic susceptibility and magnetization

All techniques for the determination of magnetic susceptibility fall into two principal categories. The ﬁrst is based on the measurement of a force that acts on a sample when it is placed in a non-uniform magnetic ﬁeld. The other method makes use of the electromagnetic force induced in a coil when the magnetic ﬁeld changes, or when there is a relative motion of the sample and the coil. The force methods The most familiar of the force techniques for measurement of magnetic susceptibility is the Gouy method. The sample under investigation is packed into a long cylindrical container, which is positioned so that one end is in a strong uniform magnetic ﬁeld E1 (near the centre of the magnet gap), while the other is in a much weaker ﬁeld E2 , e.g. outside the gap. The magnetic force acting on the sample is equal to Ip =

v p D(E12 E22 ) 20

(1.47)

where v and p are volume magnetic susceptibilities of the sample and of the surrounding medium, respectively, and D is the cross-sectional area of the sample. This force is detected as a weight dierential between the ﬁeld-on and ﬁeld-o conditions. The principal merit of the Guoy method lies in its simplicity - one needs only a balance, a sample container and the magnet [D6]. The Faraday method rests in the measurement of the force exerted on a small sample by a non-homogeneous magnetic ﬁeld. This can be achieved, for instance, by the use of special pole pieces. In this case the force on the sample can be written v p gE Ip = YE (1.48) 0 g} where } is the direction of the magnetic ﬁeld gradient and Y is the volume of the sample.

40

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.27: Magnetic susceptibility meter KLF-4 (courtesy of Agico Instruments). Magnetic induction methods In the simplest application of the induction principle, a sensing coil is wound around a sample. A second winding is used to generate variable magnetic ﬁeld, which produces a magnetization. There are several instruments based on the induction principle available commercially. They are essentially induction bridges that measure magnetic susceptibility of a sample of any shape and form while the mass of the specimens can range from a few grams to several tens of grams. Figure 1.27 illustrates such an automatic computer-controlled inductivity bridge, which is suitable for rapid laboratory measurement of magnetic susceptibility of rocks, soils, minerals and other materials. Sensitivity of the instrument is 1×106 (SI) and the measurement is conducted at the magnetic ﬁeld range from 10 A/m to 300 A/m (0.12 G to 3.8 G). A similar instrument with resolution of 2×106 (SI) is shown in Fig. 1.28. An even more sensitive instrument is the KLY-3 Kappabridge shown in Fig. 1.29. It employs a fully automatic zeroing system with autoranging and automatic compensation of the thermal drift and its sensitivity is speciﬁed as 2×108 (SI). While the above described laboratory susceptibility meters could be of considerable interest and use for practitioners and researchers in magnetic separation, they might not be easily aordable and su!ciently portable in plant operation. For ﬁeld operation there are several types of portable susceptibility meters commercially available. Figure 1.30 shows such an easily aordable pocket-size susceptibility meter. The instrument weighs 0.18 kg and has the measurement sensitivity of 1×107 (SI). The ﬁeld data can be stored in 250 memory registers and recalled later. The advantages of the induction bridge susceptibility meters are their high accuracy, fast measuring rate and automated computer-controlled mode of operation. High sensitivity enables one to measure the magnetic susceptibility of

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

41

Figure 1.28: Magnetic susceptibility meter MS2 (courtesy of Bartington Instruments).

Figure 1.29: Magnetic susceptibility meter Kappabridge KLY-3 (courtesy of Agico Instruments).

42

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.30: Pocket-size magnetic susceptibility meter SM-30 (courtesy of ZH Instruments). Table 1.12: Magnetic susceptibility of pyrrhotite measured by an induction bridge [S8]. Magnetic ﬁeld [G] 0.0256 0.9 5.36

Volume magnetic susceptibility ([SI]x103 ) 186 233 357

materials ranging from diamagnetic to ferromagnetic. The main drawback from the magnetic separation point of view is that these instruments operate at very low magnetic ﬁeld and do not allow measurement of the susceptibility as a function of the magnetic ﬁeld strength. The measurement of susceptibility at a low magnetic ﬁelds is only acceptable for paramagnetic and diamagnetic materials for which the susceptibility is ﬁeld-independent. For materials with ordered structures, such as ferromagnetic (v=o=) materials, magnetic permeability and magnetic susceptibility are strongly dependent on the external magnetic ﬁeld, as has been demonstrated in Figs. 1.9 and 1.15. Table 1.12 illustrates the dependence of the initial magnetic susceptibility on the magnetic ﬁeld strength, as measured by an induction bridge. It can be seen from Figs. 1.9 and 1.15 that the initial permeability or susceptibility is generally smaller than the eective permeability at the magnetic ﬁeld at which magnetic separation takes place, i.e. l ? hi i = If the external magnetic ﬁeld is su!ciently high then $ 1 and $ 0, and the magnetic force on a particle will be determined by the saturation magnetization Pv as follows from eq. 1.44. The value of Pv can be high or low, depending on the

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

43

Figure 1.31: Vibrating sample magnetometer (courtesy of LDJ, Inc.). type of material, irrespective of what the value of the initial permeability (or susceptibility) is. It is thus clear that evaluation of separability of ferromagnetic (v=o=) materials based on the measurement of the initial magnetic susceptibility can lead to erroneous conclusions. Vibrating sample magnetometer A vibrating sample magnetometer (VSM), shown in Fig. 1.31, is one of the most popular techniques in magnetometry [F3]. The sample is vibrated at small amplitude with a known frequency and phase in a uniform applied magnetic ﬁeld. The ﬁeld distortion produced by the sample varies in an a.c. manner and is detected by a pick-up coil. Using a lock-in ampliﬁer to ﬁlter out signals at frequencies other than the sample vibration frequency, VSM is able to make highly sensitive measurements. The magnitude of the signal is dependent on the magnetic properties of the sample. The external magnetic ﬁeld can be produced by superconducting magnets, various types of electromagnets or Helmholtz coils, providing excitation ﬁelds from a fraction of milliTesla to many Tesla. For all magnetizable materials, the VSM test results are displayed as magnetization curves. For ferromagnetic (v=o=) materials the results are in the form of the simple hysteresis loop, with values provided for all of the critical parameters, such as coercive force, remanent and saturation magnetization, applied magnetic ﬁeld and others. VSM can be used to test magnetic properties of metal alloys, minerals, permanent magnets, thin ﬁlms, magnetic ﬂuids etc. A typical hysteresis curve, as obtained by VSM, is shown in Fig. 1.32. For purposes of evaluation of magnetic separability of materials, VSM is a very useful, albeit rather expensive instrument. Since susceptibilities of diamagnetic and paramagnetic materials do not depend on the strength of the

44

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.32: The hysteresis curve for mild steel, as obtained by VSM.

external magnetic ﬁeld, information obtained using inductive bridges is su!cient to access separability of such materials. For ferromagnetic (v=o=) materials, however, the magnetic susceptibility is strongly dependent on the ﬁeld strength and separability of such materials is determined by the magnetic properties at the operating magnetic ﬁeld strength of a given magnetic separator. Vibrating sample magnetometer allows the determination of the magnetic susceptibility at any point on the hysteresis curve (Fig.1.32), as the tangent to the curve. It is thus possible to determine the magnetic susceptibility at any value of the magnetic ﬁeld. This procedure is useful only in the linear part of the magnetization curve. Once the material begins to saturate magnetically, the susceptibility approaches zero and the magnetic force on a particles is determined by the saturation magnetization. A typical ﬁeld dependence of the magnetic susceptibility as determined from the magnetization curve obtained using VSM is shown in Fig. 1.33. As has been stated earlier, in magnetic separation many paramagnetic and diamagnetic materials, and minerals in particular, contain ferromagnetic (v=o=) admixtures. These admixtures can signiﬁcantly inﬂuence the values of magnetic susceptibility as a consequence of its dependence on magnetic ﬁeld, temperature and particle size. A correct evaluation of magnetic susceptibility in terms of eq. (1.44), under given experimental or operational conditions, can only be eected with instruments such as VSM. However, VSM is only rarely accessible to a practitioner or even researcher in magnetic separation and detailed information about magnetic properties of minerals available in literature is limited. An exception is the work of Dahlin and Rule [D2] who investigated the magnetic susceptibility of numerous minerals as a function of the magnetic ﬁeld strength.

1.7. SOURCES OF MAGNETIC FIELD

45

Figure 1.33: Volume magnetic susceptibility of magnetite and ferrosilicon 270D, as a function of magnetic ﬁeld, as measured by VSM [S8]. A vibrating sample magnetometer with a superconducting magnet capable of producing a magnetic ﬁeld of 7.16×106 A/m (90 kOe) was used. The results showed that magnetic susceptibility of most minerals that were investigated was essentially constant in magnetic ﬁelds above those needed to saturate the ferromagnetic constituents, in agreement with eq. (1.44). Figure 1.34 illustrates some of the results. Hysteresisgraphs Hysteresisgraphs are systems for testing and analyzing hysteresis properties (BH loop) of hard and soft magnetic materials. The commercially available units are usually precision personal computer-controlled systems. Designers of permanent magnet-based magnetic separators can use such instruments to test, analyze and quality-control hard magnetic materials such as ferrites, Alnico, samarium-cobalt and neodymium-iron-boron alloys. Figure 1.35 illustrates such a hysteresisgraph.

1.7

Sources of magnetic ﬁeld in magnetic separation equipment

The aim of magnetic separation is to recover or remove particles with sizes ranging from several tens of millimeters down to a fraction of micrometre, with a wide spectrum of magnetic susceptibilities, from ferromagnetic to weakly paramagnetic. Furthermore, it is frequently necessary to separate two or more ma-

46

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.34: Magnetic susceptibilities of various minerals, measured by VSM, as a function of magnetic ﬁeld strength (adapted from [D2]).

Figure 1.35: Hysteresisgraph Permagraph (courtesy of Magnet Physik GmbH) for quality control of permanent magnets.

1.7. SOURCES OF MAGNETIC FIELD

47

terial species, the magnetic susceptibilities of which do not dier very much, of a wide range of particle sizes. The magnetic ﬁeld strength needed to recover such particles, therefore, varies substantially from one application to another and dierent ways of generating the magnetic ﬁeld are employed. As can be seen from eq. (1.8), the magnetic force required to separate a magnetizable particle depends not only on the physical properties of a material, and on the magnetic ﬁeld strength, but also on the value of the gradient of the magnetic ﬁeld. Therefore, to achieve a selective separation of a valuable material from unwanted ones, a carefully selected combination of the magnetic ﬁeld strength and its gradient must be used to warrant a high recovery and simultaneously a high grade of the concentrate. Magnetic separation can be considered successful only if it produces the right quality of the concentrate with the right recovery. In some applications of magnetic separation, for instance in magnetic ﬁltration, the ”brute force” approach is often used to ensure a high degree of removal of magnetizable solids from suspension. Consequently an eort is usually made to maximize the external magnetic ﬁeld or the ﬁeld gradient, or both. This approach is also employed in some applications in mineral processing, for instance in removal of magnetic contaminants from industrial minerals. Such a combination of high magnetic ﬁeld and ﬁeld gradient often results in a high-quality non-magnetic product, at the expense of losses of the non-magnetic component into the magnetic fraction. Undue emphasis on the magnetic ﬁeld strength and/or ﬁeld gradient sometimes results in reduced recovery of the valuable components and reduced selectivity. Excessively high capital and operating costs are additional consequences of such an approach. In the majority of applications, only a moderate magnetic ﬁeld, combined with an optimized ﬁeld gradient, are required to achieve the optimum results. The desired magnetic induction and the ﬁeld gradient are thus a function of the type of application, required metallurgical performance and economic criteria. In the following section the basic methods of the generation of magnetic ﬁelds and their gradients, as used in magnetic separation, will be reviewed.

1.7.1

Permanent magnets

Recent years have seen a strongly increasing industrial demand for permanent magnet materials. Permanent magnets have become essential components in many electric, electronic and electromechanical devices, including magnetic separators. Although the earliest permanent magnet, lodestone, was known in ancient times, the greatest strides in magnet development have occurred only over the past hundred years. Each advance has been connected with the discovery of a new class of materials, characterized by ever more desirable properties. This evolution has been monitored generally by one ﬁgure of merit for a permanent magnet, the maximum energy product (EK)max , which provides a measure of the ﬁeld that can be produced outside a unit volume of magnet material. The so-called theoretical maximum energy product, the largest value realizable in

48

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT Table 1.13: Magnetic properties of Alnico alloys. Material

Alnico Alnico Alnico Alnico Alnico

5 5-7 5DG 8B 9

Bu [T]

Hf [Oe]

Hfl [Oe]

1.27 1.34 1.33 0.9 1.05

640 740 685 1600 1500

645 745 690 1640 1515

(BH)max [MGOe (kJ/m3 )] 5.5 (44.0) 7.5 (60.0) 6.5 (52.0) 6.75 (54.0) 10.5 (84.0)

principle, is an intrinsic quantity deﬁned by (EK)max =

1 Mv 2 ( ) 0 2

(1.49)

where Mv is the saturation polarization (in [T]). This maximum energy product (in [J/m3 ]) can be achieved only if the magnet retains Mv in a reverse ﬁeld at least as large as Mv @2 [H4]. The maximum energy product is thus limited, to perhaps 1.2×106 kJ/m3 (150×106 MGOe), by the maximum saturation polarization of elements and alloys of approximately 2.5 T. At the present time, one third of this maximum has been achieved with NdFeB material. The chronological trend of the maximum energy product achieved in various permanent magnet materials is shown in Fig. 1.1. It can be seen that there are four major families of permanent magnet materials: Alnico, ferrite, rare-earth-cobalt and rare-earth-iron.

Alnico A major advance in permanent magnet technology began in 1932 with the discovery of excellent magnetic properties of an aluminium-nickel-iron alloy, Alnico. Numerous subsequent investigations resulted in many variations in composition and properties. Alnico magnets are expensive when compared to ferrite magnets since they contain 20% to 40 % of cobalt in addition to other components. Alnico alloys have desirably high remanent magnetization, good thermal stability, but comparatively low coercivities. Curie temperature is about 900 0 C and the maximum recommended operating temperature is 500 0 C. Alnico magnets are very resistant to corrosion, nearly as resistant as stainless steel. Only slight discolouration of the surface is encountered when a magnet is heated in air to 450 0 C [P4]. The physical properties of Alnico alloys are rather poor. High coercivity is closely accompanied by extreme hardness and brittleness. Forming is by casting or sintering as close as possible to the desired size and shape. For close tolerance it is necessary to cut or wet-grind the magnet [P4]. Magnetic properties of several grades of Alnico are summarized in Table 1.13.

1.7. SOURCES OF MAGNETIC FIELD

49

Table 1.14: Magnetic properties of the ferrite magnets. Material Ferrite 5 Ferrite 7B Ferrite 8A Ferrite 8D Ferrite 8C

Bu [T] 0.395 0.38 0.39 0.40 0.43

Hf [Oe] 2200 3250 2950 3100 4100

Hfl [Oe] 2230 3800 3000 3000 2200

(BH)max [MGOe (kJ/m3 )] 3.6 (29.0) 3.3 (26.0) 3.5 (28.0) 3.8 (30.0) 4.3 (34.0)

Ferrite magnets A new class of permanent magnetic materials was announced in 1952. The materials were based on the crystal anisotropy of barium oxide. This class of magnets is generally known as ferrite, but is sometimes referred to as oxide or ceramic magnets. Today, ferrite magnets are by far the most widely used magnets. The success of ferrites is due to several reasons. The raw materials are inexpensive and non-strategic. Their high coercive force combined with reasonably high magnetic induction has allowed permanent magnets to be incorporated into many types of devices. Ferrites are mechanically hard and brittle and their magnetic properties are characterized by relatively low remanent magnetization while the coercive force is satisfactory. The Curie temperature is 450 0 C and the recommended maximum operating temperature is 250 0 C. At the same time, surfaces of ferrite magnets are stable and are not subject to oxidation. Ferrites are produced by powder metallurgy. Their chemical formula can be expressed as MO·6(Fe2 O3 ), where P is Ba, Sr or Pb. Strontium ferrite has a higher coercive force than barium ferrite and is produced on a larger scale [P4]. Ferrite magnets are available in isotropic and anisotropic grades. Magnetic properties of various grades of ferrites are shown in Table 1.14. Samarium-cobalt-based rare-earth magnets The family of rare-earth permanent magnets (REPM) has evolved in the last 35 years. The materials quickly surpassed all earlier magnets, with currently best values of energy product and coercivity, both being 5 to 10 times those of Alnico and ferrites. While they are rather costly for universal use, the REPM, together with the hard magnetic ferrites, are rapidly broadening applications of permanent magnets in general [S9]. Two major subgroups are being distinguished: rare-earth Co-based magnets (particularly Sm-Co) and rare-earth Fe-based magnets represented by Nd-Fe-B. The latter third-generation REPM, in rapid development since 1983, use cheaper, more plentiful raw materials than Sm-Co and oer still higher energy density at room temperature. Sm-Co-based rare earth magnets are of two types: the SmCo5 group and Sm2 Co17 group. These two groups constitute the ﬁrst and second generation rare-earth magnets, respectively [H5]. SmCo5 alloys are the most basic materials that make up rare-earth magnets. More advanced Sm2 Co17 alloys were devel-

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

50

Table 1.15: Magnetic properties of Sm-Co magnets [W1]. Material SmCo5 Sm2 O17

Bu [T] 0.90 1.10

Hf [kOe] 9.0 10.0

Hfl [kOe] 29.0 33.0

(BH)max [MGOe (kJ/m3 )] 20.2 (162.0) 37.5 (300.0)

oped following the success of SmCo5 , to obtain higher performance. In order to increase its rather low coercivity, the latter alloy is now based on Sm-Co-Cu composition. The general composition of this new class of Sm-Co magnets is R(Co,M)} , where U stands for at least one rare-earth element, P for a combination of transition metals and/or copper and } is between 6 and 8.5. These multicomponent magnet alloys are generally termed the 2:17 systems. They have the advantage of higher magnetization and use less Sm and Co. As a results of their high Curie temperature of 700 0 C to 800 0 C, Sm-Co-based permanent magnets satisfy the needs for applications with operating temperatures up to about 300 0 C. Further demand for operation at even higher temperatures has led to development of a new class of Sm-based alloys, which can operate at temperatures as high as 550 0 C [W1]. Magnetic properties of Sm-Co magnets are listed in Table 1.15. The samarium-cobalt materials are attractive replacements for electromagnets in many applications, but their use has been constrained by economic disadvantages. Samarium is the least abundant, and hence the most expensive, of the light rare earths, and this unfavourable circumstance is compounded by the fact that the price and availability of cobalt are subject to large, unpredictable excursions. The bulk of cobalt is mined in Congo and regional political instability in Africa resulted in diminished supplies and radically increased prices. This situation led to a continued eort to develop alternative high performance magnets not containing cobalt. Neodymium-iron-boron magnets Iron-based materials having the characteristics of Sm-Co had long been desired and in 1983 two dierent processing routes were announced. The standard powder metallurgy route (Sumitomo route) [S10] and the melt-spinning method (General Motors route) [C3] were proposed for the production of Nd-Fe-B permanent magnets. In the ensuing years production and application of this new type of magnet has been steadily increasing. It has been predicted that the NdFeB permanent magnet market will grow from the 2002 value of $2 billion to $4.8 billion in 2007 [B7]. Presently three common fabrication routes can be used to categorize NdFeB magnets: sintering, polymer bonding and hot deformation. The most successful procedure on the production scale is the powder metallurgical method. The reason is that sintered NdFeB magnets have outstanding magnetic properties, good productivity and superior energy e!ciency and cost performance. On

1.7. SOURCES OF MAGNETIC FIELD

51

Figure 1.36: Progress in development of NdFeB sintered permanent magnets (after [K4]). the other hand, sintered NdFeB magnets have certain disadvantages in terms of thermal and environmental stability. The theoretical value of the maximum energy product of the magnetic Nd2 Fe14 B phase is 512 kJ/m3 (64 MGOe) [S11]. So far, energy products exceeding 400 kJ/m3 have been achieved, with the latest record of 444 kJ/m3 (55.8 MGOe) [K4]. Progress in development of NdFeB sintered magnets is depicted in Fig. 1.36. Bonded magnets have intermediate energy products of 80 to 145 kJ/m3 (10 to 18 MGOe) and can be formed into intricate shapes. Hot deformed magnets possess intermediate to high energy product of 120 to 370 kJ/m3 (15 to 46 MGOe), isotropic and anisotropic properties and the potential to be formed into net shapes. Comparison of magnetic properties of several types of NdFeB permanent magnets is shown in Table 1.16. While NdFeB permanent magnets possess outstanding magnetic properties, they have insu!cient level of thermal and environmental stability. The Curie temperature of the NdFeB alloys is about 310 0 C. This proximity to the room temperature limits the practical range of applications of NdFeB magnets and causes appreciable changes in the ﬂux density as the temperature varies. Operation of a permanent magnet at elevated temperatures can result in structural changes, which in turn lead to irreversible losses of magnetic properties. Table 1.17 compares the loss of remanent magnetization, at 20 0 C, of various magnet materials, after exposure to the indicated temperature. Another study [F4] observed that after 30 minute exposure to the temperature of 220 0 C NdFeB magnets lost up to 80% of their magnetization. The maximum operating temperature of NdFeB magnets is about 150 0 C.

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

52

Table 1.16: Magnetic properties of NdFeB permanent magnets [B7]. Magnet

Sintered VCM Bonded MQ1-B Hot-pressed MQ2-E Die-upset MQ3-F Sintered (Sumitomo) [K4]

Bu [T]

Hfl [kOe]

1.31 0.69 0.825 1.31 1.51

14 9 17.5 16 8.68

(BH)max [MGOe (kJ/m3 )] 42 (336.0) 10 (80.0) 15 (120.0) 42 (336.0) 55.8 (445.0)

Table 1.17: Temperature-induced irreversible losses in permanent magnets [P4]. Magnet Alnico Ferrite SmCo5 NdFeB

-600 C -1.45% -27% 0 0

+1000 C 0.4% 0 0.5% 6.5%

+2000 C 0.8% 0 1.7% 65.0%

+3000 C 1.1% 0

Comparison of the Curie and maximum operating temperatures for various permanent magnets is given in Table 1.18. NdFeB permanent magnets are also sensitive to attack by both climatic and corrosive environments, resulting in a deterioration of the magnetic and physical properties. It appears that the susceptibility to corrosion is a problem that all NdFeB magnets experience, regardless of the fabrication process [H6]. It was found [C4] that the corrosion rate increases more with an increase in the humidity level than it does with an increase in the environmental temperature. It was also observed that nitrogen in the air retards the rate of corrosion. In practice, surface protection by epoxy resins or by Al coating, combined with chromating is applied. Typical coating thickness is from 10 m to 24 m for Al-chromated and about 25 m for electrically deposited epoxy [H6]. The application of two separate coatings, shot-peened and chromated aluminium deposited by ion vapour

Table 1.18: Curie and maximum operating temperatures of various permanent magnets. Magnet Ferrite Alnico RECo5 NdFeB

Curie temperature [0 C] 450 900 700 310

Maximum operating temperature [0 C] 350 500 250 150

1.7. SOURCES OF MAGNETIC FIELD

53

deposition and electropaint deposited cathodically have been shown to resist a variety of climatic and corrosive atmospheres [M3]. Permanent magnets in magnetic separation The early history of magnetic separation is closely associated with permanent magnets, which were used to remove strongly magnetic matter from wastes or to recover strongly magnetic (mostly iron) minerals from ores. With the development of powerful electromagnets the interest in permanent magnets as applied to magnetic separation temporarily diminished. In recent years, however, we have witnessed a remarkable renaissance of interest in permanent magnets, a phenomenon associated with the dramatic development of novel permanent magnets materials, based on rare earths. Although the magnetic induction that can be generated by permanent magnets rarely exceeds 1 T, the value that can be easily produced by electromagnetic coils, in a much larger volume, permanent magnets oer several advantages over electromagnets. In small devices, permanent magnets have major advantages over electromagnetism. Even in large systems, however, permanent magnets are a good solution, as a result of their advantageous volume e!ciency, low operating costs and simple support facilities. And very importantly, permanent magnets do not require a source of energy or a cooling ﬂuid.On the other hand, permanent magnets possess a few disadvantages, among them the fact that the magnetic ﬁeld is di!cult to vary and that it cannot be switched o. As a result of notable development of new permanent magnet materials during the last three decades, permanent magnets are currently used in a wide range devices for magnetic treatment of materials. In most applications, in which a relatively short reach of the magnetic force is required, permanent magnets replaced electromagnets. Permanent magnetic rolls, magnetic pulleys, suspended magnets, high-ﬁeld permanent drum magnetic separators and eddy-current separators are typical examples. Even in those applications of magnetic separation where the magnetic force must be generated in a relatively large volume, permanent magnets are employed. Multiple-ring high-gradient magnetic separators are an example. In the application of magnetic techniques in biosciences permanent magnets are an essential part of biomagnetic separators and devices for drug targeting and hyperthermia.

1.7.2

Iron-core electromagnets

Of the several ways of generating a magnetic ﬁeld in magnetic separation, the choice is dictated mainly by the required ﬁeld magnitude, by the volume in which a given magnetic ﬁeld is to be generated and by methods used to generate the ﬁeld gradient. An eective separation of weakly magnetic particles of a small size often requires an increase of both the magnetic ﬁeld and of its gradient beyond the values available with permanent magnets. Furthermore, as the magnetic ﬁeld falls very rapidly from the surface of a permanent magnet, the eective volume in which a su!ciently high magnetic force can be created is limited.

54

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT U - DIPOLE Coils

Iron Yoke

Figure 1.37: Schematic cross-section of the U-dipole iron-core electromagnet, with two possible positions of the magnetizing coils. Therefore, in order to generate a su!ciently high magnetic ﬁeld in a large volume that would guarantee a large throughput of a magnetic separator, an electromagnet must be used. Of the several ways of generating a magnetic ﬁeld by an electromagnet, the choice is dictated by consideration of the required ﬁeld magnitude, the volume in which the ﬁeld is to be generated and by the duty cycle of the separation process. The relative importance of these considerations usually determines the method with little overlapping of choice. For example, if the separation process requires a magnetic ﬁeld less than 2 T in a relatively small volume, an iron-core electromagnet is a good choice. For the ﬁeld of 2 T or less, in a large volume, a water-cooled iron-clad solenoid should be used, although a superconducting magnet could also be a choice. Magnetic ﬁelds in excess of 2 T will undoubtedly dictate the use of superconducting solenoids. In iron-core electromagnets, the electric current passing through the windings magnetizes a great mass of iron, which in turn produces a ﬁeld in the working volume. Judicious location of the iron and of the windings may increase considerably the e!ciency of the magnet. Although the ﬁeld strength obtained in this way is limited by the saturation magnetization of iron, for most large-scale applications of magnetic separation for the recovery of weakly magnetic materials, the magnetic force generated by such iron-core electromagnets is usually su!cient. Design of iron-core electromagnets is largely a matter of practical experience, and it is generally considered impossible to predict accurately the ﬁeld which a particular magnet will produce [I1]. The situation has improved recently, when modern computer modelling software has been made available to magnet de-

1.7. SOURCES OF MAGNETIC FIELD

55

C DIPOLE Iron yoke Coils

Figure 1.38: Schematic cross-section of the C-dipole iron-core electromagnet.

signers. The fact that the ﬁeld magnitude and conﬁguration is almost always determined by the iron pole pieces has both advantages and disadvantages. On the one hand, the presence of iron permits useful values of the magnetic induction (say, up to 2 T) to be reached with modest investments in magnetomotive force (ampere-turns). Iron also conﬁnes the stray magnetic ﬂux to the immediate vicinity of the gap of the magnet. On the other hand, numerous drawbacks are due to the properties of iron such as nonlinearity, saturation, hysteresis and remanent ﬁeld. Figures 1.37 and 1.38 schematically illustrate cross-sections of the U-dipole and C-dipole electromagnets. These conﬁgurations are frequently used in the design of magnets for magnetic separators. The U-dipole design has been employed in conventional wet high-intensity magnetic separators (WHIMS) such as Jones (Humboldt Wedag), Eriez Magnetics or Boxmag-Rapid. On the other hand, the C-dipole conﬁguration is used, for instance, in induced magnetic roll separators. A detailed description of such units will be given in Chapter 2, while the fundamentals of the design of iron-core magnets will be discussed in Chapter 4. It is clear from Figs. 1.37 and 1.38 that as the working space of the magnet becomes larger, the iron core and the coils also become larger and therefore require increasing amount of power to generate the required magnetizing ﬁeld. There is a deﬁnite crossover point at which a greater magnetic ﬁeld can be generated for the same power in a solenoid of bore equal to the gap of the ironcore magnet [M4]. Iron can still be used in the form of a cladding surrounding the magnet.

56

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT Energising coils

Iron cladding

Working volume

Figure 1.39: Comparison of a solenoid magnet (solid lines) and an iron-core electromagnet (dotted lines).

1.7.3

Solenoid electromagnets

As has been already mentioned, the magnetic induction obtained with iron-core electromagnets is limited by the saturation of the iron. To obtain still stronger ﬁelds, at even larger volume, one has to return to the original technique of the magnetic ﬁeld generation, namely the construction of a solenoid. Instead of making use of the magnetization of iron, the ﬁeld should be obtained directly from the current in the electrical conductor. Hence the magnet must be constructed in such a way that the windings are as close as possible to the ﬁeld space, and the current through them must be as high as possible. Thus we come to a magnet consisting of a short coil, usually clad with a steel return frame which facilitates the passage of the magnetic ﬂux. Comparison of ironcore electromagnet with an iron-clad solenoid both having the same width of the working space is shown in Fig. 1.39. The total magnetic induction in the working volume of a magnet is equal to the sum of the contribution from the coil (Ef ) and of the contribution from the magnetized iron (El ) Ewrw = Ef + El (1.50) Approximately 75% to 90% of El comes from the iron in the proximity of the working volume. Therefore, approximately the same portion of iron of the yoke could have been eliminated without reducing El [M5]. Contribution from the coils to the ﬁeld in the working gap in iron-core conﬁgurations (Figs. 1.37 and 1.38) is thus generally rather small. The coils are used mainly to magnetize

1.7. SOURCES OF MAGNETIC FIELD

57

Figure 1.40: Contribution from iron cladding and from the coil to the total magnetic induction in the iron-clad solenoid. iron and to generate high El . Nevertheless, if the iron-clad solenoid is used, the contribution from the coil to the magnetic induction Ef from the coil is much higher than in the iron-core magnet, while El remains the same. Comparison of the magnetization curves for these two magnetic circuits is shown in Fig. 1.40. It can be seen that El (iron-core magnet) u El (iron-clad solenoid) and Ef (iron-core magnet) ?? Ef (iron-clad solenoid). It is thus clear that the iron-clad solenoid uses much less material and exhibits better parameters. The concept of iron-clad solenoids has been used successfully in the design of magnetic separators. Design of conventional high-gradient magnetic separators that operate in a cyclic mode, such as those used to beneﬁciate kaolin, is based on an iron-clad solenoid. Several designs of continuous HGMS machines, such as Sala-HGMS carousel separator, VMS and SLON separators also use the ironclad solenoid approach.

1.7.4

Superconducting magnets

Superconductivity is a remarkable phenomenon whereby certain metals and other compounds, when cooled to very low temperatures, become perfect conductors of electricity. Unlike the gradual changes in electrical resistance shown by all metals at more familiar temperatures, the superconducting state appears quite abruptly at a critical temperature Wf , which is characteristic of the metal in question. It is accepted that below this temperature the resistance of conventional class II superconductors suitable for magnet manufacture is indeed zero [H7]. Critical temperatures of these superconductors are very low, a few Kelvin (K), and the use of liquid helium as a refrigerant is essential. In recent

58

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Table 1.19: Critical temperatures and magnetic induction of assorted superconductors. Material Nb3 Sn NbTi V3 Ga Nb3 Al Y-Ba-Cu-O Hg-Ba-Ca-Cu-O

Tf [K] 18.0 10.6 15.0 16 - 20 92 135 - 160

Bf [T] at 0 K 28 15 26 35 140 (k)> 29 (B) 1150 (k), 149 (B)

years, however, remarkable progress has been achieved in developing materials that become superconducting at temperatures as high as 160 K [M6, F5, C5]. After the discovery of superconductivity in 1911, it was recognized that large electromagnets, capable of generating high magnetic ﬁelds and consuming no power, could be built. However, these hopes were quickly dashed when it was discovered that superconductors, in addition to their critical temperature, have a critical ﬁeld Ef , above which they revert from the superconducting state to a normal resistive state. Metals that were investigated at those times, i.e. mercury, lead and tin, the so—called class I superconductors, exhibited very low critical ﬁeld, of the order of 0.05 T. The era of superconducting magnets started only in 1960 after the discovery of the high-ﬁeld properties of new class II superconductors, namely Nb3 Sn and NbTi. During the following years, the search for new materials of ever higher performance was actively carried out and a multitude of composites, such as V3 Ga and Nb3 Al, were investigated. Most of these materials proved to be di!cult to prepare in the form of conductors and progressively disappeared [D7]. The only materials available commercially at present are the two very ﬁrst Nb3 Sn and NbTi. The latter is by far the most widely used because of its excellent mechanical properties, while the former one, although di!cult to work with, is the only choice for ﬁelds exceeding 10 T [D7]. Critical temperatures Wf and critical magnetic induction Ef of assorted superconducting materials are summarized in Table 1.19. There are three obvious areas where superconducting magnets will have considerable impact. The ﬁrst area covers all applications which will beneﬁt from a signiﬁcant reduction in the consumption of electrical energy. The second area includes those applications in which the reduction of the mass and size of the magnet is important. The third area is the market for very high ﬁeld magnets where there is no viable alternative, or the magnets that can generate magnetic ﬁeld in a large volume. An example of a superconducting solenoid is shown in Fig. 1.41. As discussed above, conventional magnets make use of iron yoke or cladding to reduce magnetic reluctance, thereby minimizing the number of ampere-turns required. Superconducting magnets do not suer from this constraint because additional ampere-turns are to be had relatively cheaply and do not signiﬁcantly

1.7. SOURCES OF MAGNETIC FIELD

59

Figure 1.41: A superconducting solenoid for high-energy experiments (courtesy of Ansaldo spa.). aect the refrigeration power load. For this reason iron core or cladding are seldom used to augment the working ﬁeld, but they are often used for shielding, to reduce stray magnetic ﬁelds [W2]. All these three areas play a role in the application of superconductivity to magnetic separation. With the use of a superconducting magnet in material separation it should be possible to generate very high magnetic ﬁelds at low input power, in large volumes. On the other hand, the need for these very high magnetic ﬁelds in material separation has not been su!ciently convincingly demonstrated. Although it was envisaged [K1] that magnetic separation will be the ﬁrst industrial application of superconductivity, superconducting magnets have not yet made a signiﬁcant impact in material processing. Superconductivity has found application in cyclically operating solenoidbased high-gradient magnetic separators for beneﬁciation of kaolin. Further development resulted in industrial-scale operation of continuous reciprocatingcanister HGMS. On the other hand, superconducting drum magnetic separators and open-gradient magnetic separators have not been, so far, successfully introduced into the material treatment industry.

1.7.5

Generation of the magnetic ﬁeld gradient

As transpires from eq. (1.8), the magnetic force acting on a magnetizable particle in a magnetic separator is determined not only by the strength of the magnetic ﬁeld but also by its gradient. A suitable combination of these parameters must be determined for each application. It is thus essential to provide

60

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.42: Pattern of the magnetic ﬁeld around a suspended magnet. not only a strong magnetic ﬁeld but also a non-uniform ﬁeld. A large variety of designs have evolved over the years to render the magnetic ﬁeld non-uniform and to produce suitable magnetic gradients. Separators based on these modes of the ﬁeld gradient generation can be classiﬁed into three basic categories: • Open-gradient separators • Closed-gradient separators • Matrix (polygradient) separators In open-gradient separators the ﬁeld gradient is generated in several ways: a. As a result of the natural non-homogeneity of the ﬁeld caused by the dependence of the ﬁeld on the distance from its source. Typical examples are overband, suspended, plate and grate magnets. The pattern of the magnetic ﬁeld around a suspended magnet as shown in Fig. 1.42 illustrates the formation of the ﬁeld gradient in the separation zone below the magnet. b. By special arrangements of permanent magnets or of the windings of electromagnets so that the patterns of alternate polarity are generated. Magnetic rolls, pulleys and drum separators use this type of the ﬁeld gradient. Multipolar windings of conventional or superconducting coils with alternating polarity are employed in open-gradient magnetic separators (OGMS). Fig. 1.43 illustrates the open-gradient magnetic system of a drum magnetic separator while Fig. 1.44 shows the 3D pattern of the ﬁeld around a permanent magnet roll. The magnitude of the gradient and the reach of the magnetic force are determined, among other things, by the dimensions of the permanent magnet elements or

1.7. SOURCES OF MAGNETIC FIELD

61

Figure 1.43: Pattern of the magnetic ﬁeld around a magnetic drum [U1].

electromagnetic winding relative to the dimensions of the spacers (either air or steel) between these magnetic elements. A schematic view of a linear multipole OGMS system is shown in Fig. 1.45. In closed-gradient separators a high ﬁeld gradient is usually achieved by a suitable shaping of the pole pieces of the opposing magnetic poles. Magnetic ﬁeld is thus focused on the working element of the separator and a high ﬁeld gradient is created. Assorted geometrical arrangements of poles and counterpoles is shown in Fig. 1.46. These dierent geometries, such as a hyperbolic pole facing a ﬂat pole (case A), or a grooved pole (case B), triangular pole and multi-tooth arrangement generate various patterns of the magnetic ﬁeld and its gradient [D4, S12]. The gradient of the ﬁeld and the reach of the magnetic force are the function of the curvature of the poles and the counter-poles, by the pitch of the teeth and by the width of the separation gap. Induced magnetic roll and wet high-intensity magnetic roll separators employ this type of closed-gradient arrangement. Ferrohydrostatic separators with magnetic ﬂuids also generate a closed gradient by a suitable shaping of the pole tips [R1]. Multipolar windings or multipolar arrangements of permanent magnets also generate closed gradient of the magnetic ﬁeld. A quadrupole geometry was used to build a magnetic separator for biomedical applications [Z2, H8]. A sextupole arrangement is employed in Magstream separator with magnetic ﬂuids [W9], while quadrupole magnets, either resistive [A3] or superconducting [C6] were also tested in magnetic separation. Figure 1.47 shows a schematic diagram of a pure quadrupole while the coil and pole arrangement in a conventional quadrupole magnet for physical experiments are illustrated in Fig. 1.48.

62

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.44: Pattern of the magnetic ﬁeld on the surface of a permanent magnetic roll.

Figure 1.45: A multipole open-gradient magnetic system.

1.7. SOURCES OF MAGNETIC FIELD

63

B

A

D

C

Figure 1.46: Shapes of poles and counter-poles in magnetic separators with closed gradient.

S pole

N pole F B B

F

F

B B

N pole

F

S pole

Figure 1.47: Magnetic ﬁeld and forces inside a quadrupole magnet. Particles are entering the paper.

64

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.48: A quadrupole resistive magnet for high-energy physics experiments (courtesy of Danfysik A/S).

Figure 1.49: Magnetization curves for bulk steel and steel wool (after [K5]).

1.7. SOURCES OF MAGNETIC FIELD

65

Table 1.20: Typical values of the gradient of the magnetic ﬁeld in magnetic separators. Separator Suspended magnet Nd magnetic roll Nd drum separator Davis tube Frantz isodynamic Belt separator Steel wool (HGMS) Steel balls (WHIMS) Expanded metal Grooved plates Split pair OGMS FHS Magstream

Gradient of the magnetic ﬁeld T/m kG/cm 0.8 0.08 200 20 80 8 10 1 20 2 1 - 10 0.1 - 1 2.5×104 2.5×103 3 1×10 100 4×103 400 2×103 200 40 - 100 4 - 10 2 0.2 30 3

In matrix (polygradient) magnetic separators, the gradient of the magnetic ﬁeld is generated by means of induced magnetic moment in the ferromagnetic bodies (called the matrix) and placed in the external magnetic ﬁeld. Strong magnetic ﬁeld gradient is generated in the close vicinity of these bodies and its magnitude depends on the size and the shape of the matrix elements. Ferromagnetic bodies of various shapes have been used in high-intensity magnetic separators (such as balls, grooved plates, mesh, expanded metal, steel wool, rods etc.) and a proper choice of the matrix is one of the crucial prerequisites for successful separation. Since the ﬁeld gradient is inversely proportional to radius d of the matrix element, i.e. uE [email protected], the magnetic force acting on the magnetizable particles is maximized by using as ﬁne a matrix as possible. On the other hand, the dimensions of the matrix elements must be selected taking into account particle size of the material to avoid straining and to ensure the selectivity of separation. At the same time, the dimensions of the matrix bodies must be chosen in such a way that the magnetic force is su!ciently strong to recover the magnetic fraction. On the other hand, the magnetic force must not be too strong to cause the matrix blockage and retention of the ”non-magnetic” component. In order to magnetize a ﬁne matrix, su!ciently strong external magnetic ﬁeld is required. This is because the ﬁlling factor of the matrix is often low and the matrix does not conduct magnetic ﬂux very well. Typically, the ﬁlling factor ranges from 0.04 (4%) for steel wool matrix to about 0.20 (20%) for expanded metal. The exception is the ball matrix where the ﬁlling factor can be as high 0.50, and grooved plates with the ﬁlling factor up to 0.80. Figure 1.49 illustrates that a background magnetic induction of at least 0.7 T is needed to saturate the steel wool matrix, compared to about 0.2 T that is necessary to

66

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.50: The magnetic ﬁeld lines around a cross-section of a magnetized steel sphere or steel wire. saturate the bulk material. The large background induction needed to saturate steel wool is a result of demagnetization eects. A large proportion of ﬁlaments in the randomly orientated steel wool is arranged along the di!cult axis of magnetization and exhibits thus a large demagnetization factor. The pattern of the magnetic ﬁeld around a magnetized steel wire or steel sphere is shown in Fig. 1.50. Typical values of the gradient of the magnetic ﬁeld for various types of magnetic separators are given in Table 1.20.

Chapter 2

Review of Magnetic Separation Equipment and Techniques In reviewing magnetic separators, it is necessary to examine hundreds of patents and papers and it is not possible to give adequate coverage to all of these. Moreover, there appear to be more models and modiﬁcations of magnetic separators than there are applications. Since each embodiment of a magnetic separation technique possesses distinct merits as well as limitations, no single technique is universally applicable to all types of magnetic separation. Various classiﬁcation schemes exist by which magnetic separator can be subdivided into categories. These schemes are based upon the dominant physical or technological feature. Magnetic separators can thus be grouped as follows: a) Based upon the medium carrying the ore: • dry • wet b) Based upon the requirement of the system: • removal of iron and similar materials for the protection of machinery subjected to damage or wear • extraction of valuable magnetic constituents • removal of deleterious magnetic impurities • separation of materials based on properties other than magnetic (e.g. density, conductivity) • material handling 67

68

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS c) Based upon the way the magnetic ﬁeld is generated: • permanent magnets • electromagnets with iron yoke • resistive solenoids • superconducting magnets d) Based upon the magnitude of the magnetic ﬁeld and its gradient: • low-intensity magnetic separators • high-intensity magnetic separators • high-gradient magnetic separators.

Low-intensity separators are primarily used for the manipulation of ferromagnetic materials or paramagnetic materials of high magnetic susceptibility, and/or of su!ciently large particle size. These separators can operate either in dry or wet modes. High-intensity separators are used for treatment of weakly magnetic materials, coarse or ﬁne, in wet or dry modes. Very ﬁne, feebly magnetic materials can be treated in high-gradient magnetic separators. From the practical point of view, classiﬁcation according to the requirement of the system is the most illustrative. For example, the application of magnetic separation to iron removal is usually dictated by the material handling system involved. The most commonly used magnetic separators include: • Magnetic pulleys, applied in belt conveyor systems as head pulleys • Suspended magnets, applied over belt conveyor chutes or feeders • Magnetic drums • Plate magnets, applied in chutes • Grate magnets, applied in product streams. For concentration or removal of magnetizable particles, a wide spectrum of magnetic separators is used. These include: • Magnetic pulleys • Magnetic low-intensity or high-intensity drums • Induced magnetic rolls • Permanent magnet roll separators (IMR)

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

69

• Cross-belt and disk magnetic separators • Magnetic ﬁlters • Wet high-intensity magnetic separators (WHIMS) • High-gradient magnetic separators (HGMS) For magnetic material handling, the magnetic systems usually applied are: • Magnetic conveyors • Magnetic rolls • Lifting magnets

Magnets are also used in numerous special applications: • Separators with magnetic ﬂuids, in which material is separated mainly on the basis of its density (FHS, MHS) • Eddy-current separators for separation of non-ferrous metals (ECS) • Dense-medium separators, in which a magnet is used to control magnetic heavy medium • Demagnetizing coils • Magnetic ﬂocculators.

2.1

Dry low-intensity magnetic separators

Dry low-intensity magnetic separators are usually used to remove tramp iron, to concentrate coarse strongly magnetic iron ores, and to recover iron values from blast furnace and steel mill slag. Removal of strongly magnetic impurities from a variety of materials is also accomplished with dry low-intensity separators. Tramp iron magnetic separators are used to protect handling and processing equipment such as crushers and pulverizers. These separators are usually used on dry material or on material which contains only surface moisture. Tramp iron comes in many shapes and sizes. By conventional deﬁnition, tramp iron means that a particle has a signiﬁcant size, which is su!cient to cause damage. Iron of abrasion, or particles smaller than 3 mm in diameter, usually do not cause equipment damage although they can discolour or contaminate the product [D7]. As far as the top size is concerned, large pieces as long as 2 m can be successfully removed. The size and shape of the tramp iron, together with the material handling system used must be considered in selecting the protective magnet.

70

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.1: Magnetic pulley (courtesy of Steinert GmbH).

2.1.1

Magnetic pulleys

An easy and simple way to remove tramp iron from material on a conveyor belt is by means of a magnetic head pulley. These are available both in permanent magnet and electromagnetic construction. They are relatively inexpensive and easy to install, and accomplish continuous tramp iron removal. The magnetic pulley, shown in Figure 2.1, usually replaces the head pulley or the tail pulley of a belt conveyor, converting the conveyor into a magnetic separator. Material carried on the conveyor passes over the magnetic pulley which holds the magnetic particles until they leave the region of the magnetic ﬁeld while the non-magnetic material is discharged over the pulley. A typical installation is shown in Fig. 2.2, while Fig. 2.3 illustrates an actual process of separation by the pulley. The permanent magnetic pulleys can be manufactured with axial poles in which the polarity alternates along the circumference, or radial poles, in which the polarity changes across the width the of the belt. For large particles and elongated shapes, the radial pole design is more suitable. For ﬁnely divided material, the uniformity of the ﬁeld across the belt width makes the axial pole design more advantageous. Strontium ferrite magnets are usually used. Electromagnetic pulleys are used where control of the magnetic ﬁeld is required. The magnetic pulleys are manufactured in a range of diameters, from 500 mm to 1250 mm. The width of the magnetic pulley should be selected to match the belt width. The throughput of magnetic pulleys of dierent dimensions is shown in Figure 2.4. Standard belt speeds for which the throughputs were calculated are shown in Table 2.1. Inclined belts provide additional areas of contact with the magnetic ﬁeld of the pulley and can tolerate higher capacities.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

Figure 2.2: Principle of operation of a magnetic pulley.

Figure 2.3: Operation of a magnetic pulley (courtesy of Steinert GmbH).

71

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

72

Table 2.1: Standard belt speed for magnetic pulley operation. Pulley diameter [mm] 500 630 800 1000 1250

Belt speed [m/s] 1.1 1.45 1.7 2.0 2.2

Table 2.2: Recommended diameters of magnetic pulleys. Feed size [mm] 50 - 100 25 - 50 6 - 25

Pulley diameter [mm] 750 - 900 450 - 600 300 - 450

Throughput [t/h/m] 250 - 400 165 - 250 75 -135

Magnetic pulleys of special design are used in the concentration of magnetite and other ferromagnetic minerals. For the best results, the feed should be screened into sized fractions and each fraction treated on a separate pulley. Typical feed sizes would be - 100 mm + 50 mm, - 50 mm + 25 mm and 25 mm + 6 mm. The magnetic pulley is not suited for the treatment of - 6 mm material. Pulley diameters recommended for various feed sizes are given in Table 2.2 [M7].

2.1.2

Plate magnets

Where the amount of tramp iron contained in a product is reasonably small and where automatic removal is not required, plate and grate magnets can be incorporated in chutes and ducts to remove both tramp iron and iron of abrasion. Such a plate magnet is shown in Fig. 2.5. The plate consists of a series of alternating poles, uniform across the chute width and alternating along the chute length. As the material passes over the magnet face, tramp iron is trapped on the magnet face while the remaining nonmagnetic material proceeds down the chute. The plate magnets must be cleaned and inspected daily since they are not eective if the accumulated tramp iron is allowed to remain on the face. The magnetized plates are usually of permanent magnet type, either ferrite or rare earth. The eective depth of the magnetic ﬁeld can be as high as 200 mm, depending on the type of the magnetic material and on the shape of particles to be removed. A chute angle not exceeding 450 is recommended [M7].

2.1.3

Grate magnets

The grate magnet shown in Figs. 2.6 and 2.7, consists of a series of magnetic tubes, which have poles alternating between one another and along their length.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

73

Figure 2.4: Throughput of magnetic pulleys of various diameters, for dierent widths of the conveyor belt. Standard belt speeds were assumed (after [M7]).

These units are used for granular free-ﬂowing materials ﬁner than 12 mm and are typically mounted at the discharge of a hopper. A number of rows of tubes provide several passes of ﬁnely divided material and can remove essentially all the magnetic particles. The permanent magnets used in the grate magnets are either ferrites, which are suitable for temperatures up to 150 0 C, or NdFeB magnets, with operating temperature up to 90 0 C. For higher temperature applications, up to 350 0 C, the Alnico magnetic grates are also manufactured.

2.1.4

Suspended magnets

Suspended magnetic separators have been used over many decades to improve material purity and to protect processing machinery. Particularly when the belt speed is high and/or if large tramp iron objects are to be removed, suspended magnets are recommended. Suspended magnets are available in both circular and rectangular construction. The rectangular magnet is most commonly used and permits installation of self-cleaning construction. Units based on permanent magnets or electromagnets are manufactured, with the permanent magnet design being restricted to lighter burdens. Simple suspended magnets, designed to remove small amounts or occasional pieces of tramp iron, employ the manual cleaning mechanism. They must be periodically turned o in order to remove

74

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Cleaning position S N

Plate magnet

Figure 2.5: Plate magnet.

Figure 2.6: Grate magnet.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

Figure 2.7: Grate magnet.

Figure 2.8: Principle of operation of an in-line suspended magnet.

75

76

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.9: Installation of a cross-belt suspended magnet (courtesy of BoxmagRapid Ltd.).

iron accumulated on the face of the magnet. Where a large amount of tramp iron is expected, or where access to the magnet for cleaning is di!cult, selfcleaning magnets should be used. A belt driven across the magnet face allows continuous automatic removal of tramp iron. Suspended magnets can be installed at many points in a material handling system: at any point along a conveyor belt, at the discharge end of feeders or screens and above chutes or launders. The preferred location for a suspended magnet is at an angle over the conveyor belt as shown in Fig. 2.8. In this orientation the tramp iron is moving into the face of the suspended magnet and the load is breaking open, allowing easier tramp iron removal. Self-cleaning magnets can be operated across the belt, as shown in Fig. 2.9, and as inline units as illustrated in Fig. 2.10. In the cross-belt mode of operation, the magnet belt moves perpendicularly to the conveyor belt. Because the tramp iron must be attracted and turned by 900 from the movement of the conveyor belt, a cross-belt magnet is usually larger and stronger than an in-line magnet. Typical values of the magnetic ﬁeld as a function of suspension distance for oil-cooled suspended electromagnets, for dierent lengths of the magnet, are shown in Fig. 2.11 [M7]. The selection process for suspended magnets will be discussed in Chapter 5.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

77

Figure 2.10: Installation of an in-line suspended magnet (courtesy of Steinert GmbH).

Figure 2.11: Magnetic ﬁeld as a function of the suspension distance for oil-cooled suspended electromagnets of dierent lengths.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

78

Figure 2.12: Pole conﬁgurations in drum magnetic separators [M8].

2.1.5

Drum magnetic separators

Drum magnetic separators are probably the most widely used type of magnetic separation equipment. The design of drum separators is predominantly based upon permanent magnet technology, although electromagnetic drums can also be occasionally found in industrial practice. Drum separators are applied to the treatment of particle sizes, which range from several centimeters down to several micrometers, and operate either in a dry or wet mode. While ferrite magnets are used in conventional low-intensity drum separators, recent progress in availability and aordability of rare-earth permanent magnets has resulted in the construction of powerful high-intensity drum separators. The basic design of all drum magnetic separators is essentially the same. Blocks of permanent magnets are arranged in a stationary position inside a non-magnetic rotating drum, as shown in Fig. 2.12. Drums are made in several conﬁgurations depending on the application. The magnet assembly, consisting of three to nine magnetic blocks of alternating polarity, covers an angle usually ranging from 900 to 1200 . As can be seen in Fig. 2.12, in the radial arrangement of the magnets, the polarity alternates across the width of the drum, and is the same along the drum circumference. Such an arrangement is suitable for the removal of elongated tramp iron or concentration of coarse particles when high recovery is required. In the axial arrangement, the polarity alternates along the circumference of the drum and is uniform across the width of the drum. This arrangement

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

79

Figure 2.13: A pattern of the magnetic ﬂux around a magnetic drum.

provides an agitating action enabling the release of entrained non-magnetic particles. The axial arrangement is used when a high quality magnetic concentrate is required, although sometimes at the cost of reduced recovery. The development of improved permanent magnet materials resulted in increased magnetic induction available on the drum surface and at a suitable operating distance from the drum. Conventional ferrite-based drums generate up to about 0.22 T on the drum surface and 0.10 T at 50 mm. In NdFeB-based drums a magnetic induction as high as 1 T can be reached on the drum surface. A pattern of the magnetic ﬂux around a magnetic drum is shown in Fig. 2.13. Drums are manufactured with dierent diameters and widths. While diameters of ferrite drums range from 600 mm to 1500 mm, rare-earth drum are generally smaller, with diameters from 380 mm to 1000 mm. The most common width of the low-intensity drums is 1500 mm, although units 3000 mm wide are also manufactured. Dry low-intensity drum magnetic separators are used mainly for tramp iron removal where magnetic pulleys and suspended magnets are not feasible. With rare-earth magnets, the drums are also able to separate stainless steel and ironbearing minerals. These separators can operate with top feed and bottom feed, as shown in Figs. 2.14 and 2.15. The material to be separated is fed at the top of the rotating drum surface, as shown in Fig. 2.16; the non-magnetic fraction leaves the drum, while the magnetic fraction is retained by the magnetic force at the drum surface until carried outside the eective magnetic ﬁeld. In bottomfeed drums, the magnetic component of the feed is picked up by the magnet while the non-magnetic fraction leaves the system unaected. Drums with top feed produce the highest magnetic removal and are suitable for materials that contain relatively small amount of magnetic particles. However, the drum with

80

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.14: Dry drum magnetic separator with top feed [M8].

Figure 2.15: Dry drum magnetic separator with bottom feed [M8].

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

81

Figure 2.16: Operation of a dry drum magnetic separator (courtesy of Steinert GmbH). bottom feed produces a clean magnetic concentrate with little non-magnetic carry-over and should be used to treat materials containing a high percentage of magnetic particles.

2.2

Wet low-intensity drum magnetic separators

Wet drum magnetic separators are used to recover ferromagnetic solids from a slurry feed. The major areas for their use are in media recovery in dense medium separation plants and in beneﬁciation of magnetite ore. Figure 2.17 shows the recovery of the magnetic particles by a wet drum magnetic separator. Physical construction of wet drum separators is slightly dierent for the two applications, with the ore concentrator being more rugged in construction and subject to more detailed speciﬁcations than the media recovery units. The drum is partially submerged in a tank of water and carries the material to be treated across the face of the magnetic system and the magnetic concentrate out of the tank. The size of the feed treated in these separators rarely exceeds 6 mm while the bottom size of the feed can be as small as 20 m= The design of the tanks for the drum separator is very important and is determined by the objectives of the separation process. There are three basic tank designs, based on the slurry ﬂow: • concurrent • counter-current

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

82

Figure 2.17: A wet drum magnetic separator. • counter-rotation.

2.2.1

Concurrent tank

The concurrent tank design is shown schematically in Fig. 2.18. The feed is introduced at one end of the separator through the feed box and ﬂows in the direction of drum rotation. Magnetic material is picked up by the magnet and the non-magnetic material is discharged at the bottom through the tailings discharge opening. Magnetic particles continue to adhere to the surface of the drum and pass through an opening between the drum shell and the tank wall. The magnetic fraction is then discharged down the discharge lip. The concurrent design of the tank is used mainly for treating coarser material in the size range 5 mm and below. High throughput and high quality of the magnetic concentrate are characteristic features of this design.

2.2.2

Counter-rotation tank

In the counter-rotation design of the tank (Fig. 2.19), the feed is introduced through a special feed box to the drum, which rotates in the opposite direction to the slurry ﬂow. Magnetic material is picked up by the drum and discharged almost immediately. Since the tailings ﬂow along the entire magnetic arc of the drum before being discharged, losses are minimum. This tank design is used

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

Figure 2.18: The concurrent tank.

Figure 2.19: The counter-rotation tank.

83

84

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.20: The counter-current (Steenson) tank. primarily where surges in throughput are experienced, possibly involving high content of the magnetic material. Very high recoveries can thus be achieved with this design, while the grade of the concentrate is of secondary importance only. The particle size can be up to 4 mm, but is preferably smaller than 0.5 mm.

2.2.3

Counter-current tank

The counter-current tank (Fig. 2.20) is used mostly for ﬁnishing where very thorough cleaning is required. The term ”counter-current” refers to the fact that the tailings must ﬂow counter to the rotation of the drum when leaving the separator. Feed is introduced near the bottom of the drum and agitated through wash-water jets. Tailings ﬂow out from the opposite end of the tank through a tailings discharge overﬂow, which also acts as the slurry level control. This ensures a high recovery of magnetic material and a high quality of the concentrate. These tanks are most suited to ﬁnely ground material of 100 m and less.

2.2.4

Design of the drum

The separating drum consists of two main parts: a stationary magnetic circuit and a shell, usually made of stainless steel and often protected by an anti-wear cover. The shell rotates freely around the magnets that cover an angle up to 1500 . The choice of the permanent magnet material and design of the magnetic circuit are the same as those for dry drum magnetic separators as discussed in Section 2.1.5. The drums are available in 760 mm (30”) to 1200 mm (48”) diameter; 900 mm (36”) drum diameters being the most frequently used. The drum width ranges from 610 mm to 3050 mm, usually in increments of 300 mm.

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

85

Figure 2.21: Throughput of a drum magnetic separator, as a function of the drum diameter (after [K6], [S13]).

With increasing diameter of the drum, the throughput also increases. This is illustrated, for dierent types of tank design, in Fig. 2.21. It appears, however, that the 1200 mm diameter is the optimum size, as a further increase in diameter has not apparently resulted in the corresponding increase in processing capacity [S13]. The increased throughput with increasing drum diameter can be expected as the residence time of particles in the magnetic ﬁeld increases as the length of the magnetic arc increases. This increase in residence time results either in improved recovery of the magnetic particles (possibly with a reduced grade of the concentrate due to increased entrainment of non-magnetic particles) or, at constant recovery, in increased throughput. Large diameter drums usually incorporate a larger pitch of the magnetic poles [S13]. Such a modiﬁcation of the magnetic design then results in a deeper magnetic ﬁeld around the drum and in the ability to treat higher volumes of material. However, a larger pitch of the poles reduces the ﬁeld gradient and thus the magnetic force acting on the magnetizable particles. This could result in a reduced recovery. Figure 2.22 illustrates the operation of wet-intensity drum separators in an iron-ore beneﬁciation plant. A more detailed discussion of practical aspects of operation and selection of wet drum magnetic separators is given in Chapter 5.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

86

Figure 2.22: Wet drum magnetic separators in an iron-ore beneﬁciation plant.

2.3

Dry high-intensity magnetic separators

Weakly magnetic minerals can only be removed from a material stream in magnetic ﬁelds much greater than those available in low-intensity magnetic separators. Dry high-intensity magnetic separation has been used commercially since the beginning of the last century, while wet high-intensity high-gradient magnetic separators were developed only relatively recently. Five types of dry high-intensity magnetic separators are in use: • cross-belt separators • induced magnetic roll separators • permanent magnetic roll separators • magnetic ﬁlters • rare-earth drum magnetic separators.

2.3.1

Cross-belt magnetic separator

The cross-belt magnetic separator is one of the oldest types of separators used to concentrate moderately magnetic ores. The operating principle is shown in Fig. 2.23. Dry material is fed in a monolayer onto a conveyor belt and is carried between the poles of the magnetic system. The belt, with its load, passes

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

87

Figure 2.23: Cross-belt magnetic separator.

between the poles of two or more electromagnets. The lower pole-pieces are ﬂat and immovable, while the corresponding upper pole-pieces are shaped and may be raised or lowered as required for the material undergoing treatment. An endless cross-belt runs around a series of pulleys and across each upper poleface surface at right angles to the conveyor belt. As the material passes, the magnetic particles are attracted to the cross-belt, carried with it towards the discharge side and fall into a bin. The material may be passed successively between several pairs of magnet poles when it is desired to make several products in one pass. Non-magnetic tailings discharge as the conveyor belt passes over its end pulley. Machines with two to eight pairs of poles are available and each pair can be adjusted independently by regulating the position of the upper poles and by altering the current through the coils. The height of the upper pole-pieces above the belt should be set at least 2.5 times the size of the largest particle in the feed. The conveyor belt width ranges from 100 mm to 600 mm and particles ranging from 4 mm to 75 m may be treated, preferably sized into several fractions. Depending on the gap between the poles and on the current setting, the operating magnetic induction ranges from 0.2 T to 2.0 T. The main advantage of the cross-belt separator is that several types of magnetic products can be recovered in one pass. However, low throughput is a major drawback. A ﬁve-pole cross-belt separator is shown in Fig. 2.24.

88

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.24: A cross-belt separator (courtesy of Roche Mining).

2.3.2

Induced magnetic roll separator

The induced magnetic roll (IMR) separator shown in Figs. 2.25 and 2.26 consists of a revolving laminated roll formed of alternate magnetizable and non-magnetic discs. The roll is placed between shaped pole-pieces of an electromagnet. The electromagnet induces a magnetic ﬁeld in the magnetic lamination of the roll and generates regions of high magnetic ﬁeld gradient. Material to be treated is fed in a controlled thin stream by a vibratory feeder to the top of the roll. As the roll revolves, the material passes through a narrow gap between the pole of the magnet and the roll. Non-magnetic particles are discharged from the roll while the magnetic particles are attracted to the roll and report into a separate chute when they enter a region outside the sphere of inﬂuence of the magnet. Ferromagnetic material should be removed with a separate magnetic scalper before feeding to IMR, to prevent plugging the gap. The gap between the feed pole and the roll is adjustable and also the setting of the splitter is of great importance. Depending on the width of the separation gap and the current in the magnetizing coils, the magnetic induction in the gap can approach 2 T. The material to be treated must be dry, free-ﬂowing and for best results it should be in the size range - 2 mm + 100 m. The gap should be set to at least 2.5 times the average grain size. The throughput can range from 1 to 3 t/h per meter length of the roll. IMR separators have been extensively used for the beneﬁciation of beach sands and for the removal of weakly magnetic impurities from glass sand, andalusite, feldspar, wollastonite, magnezite and other industrial minerals. IMRs can also be used for concentration of materials such as chromite, monazite and wolframite. IMRs possess several limitations, namely relatively low throughput, limited particle size range and large mass. In recent years, much simpler and easier to operate permanent magnetic roll separators have replaced IMRs in numerous

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

89

Figure 2.25: Schematic diagram of an induced magnetic roll separator (courtesy of Roche Mining). applications. An induced magnetic roll with bottom feed was developed by Carpco, Inc. It is oered as a laboratory or pilot-scale separator for treatment of particles up to 1 mm in size, in throughputs up to 50 kg/h. The separator, shown in Fig. 2.27, achieves highly selective separation by magnetically lifting weakly magnetic particles against gravity. As no entrapment of unwanted material takes place, the separator is suitable in those applications where the grade of the magnetic concentrate or the recovery of the non-magnetic concentrate are of prime importance.

2.3.3

Permanent magnetic roll separator

Although the idea of a permanent magnetic roll separator, consisting of permanent magnet disks or rings interleaved with mild steel disks, as shown in Fig. 2.28, dates back to 1968 [A4], it was only the advent of rare-earth permanent magnet materials that spurred the rapid development of these machines. A patent by E.L. Bateman Ltd. [Y1] became a starting point for a productive period of competitive development of a wide array of roll separators. Initially Sm-Co permanent magnets were used but they were quickly replaced by NdFeB magnets when they became commercially available. The active part of this separator is a roll consisting of disks or rings of permanent magnets, sandwiched between mild steel rings. The adjacent per-

90

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.26: Reading induced magnetic roll separator (courtesy of Roche Mining).

Figure 2.27: An induced magnetic roll separator with bottom feed (courtesy of Outokumpu Technology, Carpco Division).

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

Permanent magnet ring

91

Steel ring

Figure 2.28: Details of a permanent magnet roll. Table 2.3: Typical values of magnetic induction on the roll surface, as determined from modelling and by measuring using a conventional HallEect probe. Magnet Nd-Fe-B Sm-Co Ferrite

B [T] - modelled 1.9 1.5 0.5

B [T] -measured 1.0 8.0 0.3

manent rings are arranged with the same polarity facing one another. Very high magnetic ﬁelds and ﬁeld gradients are generated on the surface of the roll. As discussed in Section 1.6.1, it is di!cult to measure the real magnitude of the ﬁeld using conventional measuring equipment because the ﬁeld varies over a scale of several hundreds of micrometers. Electromagnetic modelling software, however, allows determination the pattern of the ﬁeld around a roll as shown in Fig. 2.29. Typical values of the magnetic ﬁeld are shown in Table 2.3. The values of the magnetic ﬁeld strength measured using a conventional Hall-Eect probe are also shown. The values of the magnetic ﬁeld strength and its gradient on the roll surface and around the roll are strongly dependent on the conﬁguration of the magnet and steel rings. Thin magnet and steel rings generally produce a very high ﬁeld, the ﬁeld gradient and the magnetic force at the surface of the roll, while a long reach of the magnetic force can be achieved using thicker steel rings. The relative thicknesses of the magnet and steel rings generate a widely diering pattern of the magnetic ﬁelds around the roll. While the most common ratio of the widths of the magnet to the steel is 4:1, the correct choice of the roll

92

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.29: Pattern of the magnetic ﬂux lines around a magnetic roll.

Figure 2.30: Operation of a permanent magnetic roll separator.

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

93

c Figure 2.31: Permanent magnetic roll separator Permroll° (courtesy of E.L. Bateman Ltd.).

conﬁguration is determined mainly by the magnetic properties and particle size distribution of the material to be treated. Operation of permanent magnetic roll separators is schematically shown in Fig. 2.30. For easy removal of magnetic particles, the roll is covered by a belt, which can be as thin as 0.12 mm, to allow the feed material to be as close to the magnet as possible. The belt is supported by an idler roll. Below the conveyor is a hopper which collects the discharging material, while adjustable splitters divert the dierent fractions into collection bins placed beneath the hopper. The most common diameter of the roll used to be 72 mm or 76 mm, while rolls 100 mm and 300 mm in diameter have now become commonly available from several manufacturers. The latter design is based on magnet segments rather than rings. With increasing roll diameter, the residence time of particles in the magnetic ﬁeld, the ﬁeld depth and the e!ciency of separation increase. Alternatively, by increasing the speed of rotation, to maintain the same residence time as with a smaller roll, a higher throughput could be achieved with the roll of a larger diameter. For production-scale applications, the width of the magnetic zone of the roll is either 1000 mm or 1500 mm, although for smaller scale applications 250 mm and 500 mm wide rolls are available. Throughput of roll separators is aected by many factors, which include particle size, particle density, proportion of the magnetic component in the feed and the desired quality of the ﬁnal product. As a guideline, a throughput of 2 to 6 t/h/m can be achieved with material smaller than 2 mm, while larger material can be processed at a throughput up to 15 t/h/m. A modular design enables a number of passes to be arranged into a compact unit.

94

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.32: Installation of multistage Inprosys roll magnetic separators (courtesy of Outokumpu Technology Inc.).

A photograph of a two-stage production-size unit is shown in Fig. 2.31, while Fig. 2.32 illustrates the installation of multistage machines. One of the most important issues that aects operational ﬂexibility, ease of maintenance and cost e!ciency is the belt tracking. Tracking, tensioning and changing the belts can be extremely time-consuming, in addition to a high cost of replacement of damaged belts. Several proprietary tracking and tensioning systems and roll support structure are available and it is claimed that it is possible to replace a belt in less 5 minutes [D8]. The magnetic force generated by the permanent magnetic roll is of the same order of magnitude as that in induced magnetic rolls. A spectrum of minerals that can be successfully treated by either magnetic separator is practically identical. Permanent roll separators, however, possess numerous advantages such as low energy consumption, and smaller mass and ﬂoor space. The absence of an air gap allows treatment of particles as large as 25 mm. A few drawbacks include belt wear and inability to control the magnetic ﬁeld strength. While permanent roll separators are predominantly dry machines, wet units are being used, for instance, for the concentration of diamonds [R2].

2.3.4

High-intensity drum separators

Recent progress in the availability and aordability of rare-earth permanent magnets has resulted in design and construction of powerful high-intensity drum magnetic separators (REDS). Eriez Magnetics were probably the ﬁrst to replace

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

95

Figure 2.33: Operation of a dry NdFeB drum magnetic separator (courtesy of Outokumpu Technology Inc.). standard ferrite magnets with NdFeB permanent magnets and nearly all current suppliers of REDS adhere to this conventional design philosophy [A13]. Figure 2.33 illustrates the operation of a rare-earth dry drum magnetic separator. A somewhat dierent approach [M13, W6, U1] to the design of the highintensity drum separator was based on a plurality of small magnet blocks whose direction of magnetization changed in small increments, as can be seen in Fig. 2.34. This system which was claimed to require less magnetic material in comparison to a conventional system [W6] to achieve the magnetic induction of 0.7 T on the drum surface, was incorporated into the Permos separator of KHD Humboldt Wedag AG. The density of the magnetic force (or the force index) EuE of a rare-earth drum magnetic separator is much smaller than the force index generated by most roll separators, usually not exceeding 20% of EuE for an NdFeB roll (see Table 1.1). The main reason is that the magnetic ﬁeld gradient in REDS is much lower than that in a roll separator, as a result of the geometry of the magnetic system. On the other hand, the reach of the magnetic force can be extended to greater depths, allowing eective treatment of coarse particles. The current consensus is that roll magnetic separators are not only more powerful than drum magnetic separators, but they also seem to oer greater selectivity and ﬂexibility [A13]. Generation of eddy currents in the rotating shell of the drum separator can be a serious problem because of limited temperature tolerance of NdFeB permanent magnets. The level of these currents depends on the magnetic induction, the number of magnetic poles, the speed of rotation, the shell thickness and the

96

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.34: The magnet structure of the Permos separator [U1].

conductivity of the shell material. Heat will develop in proportion to the drive power that is required for the shell to overcome the braking eect of the eddy currents [A13]. The heat generation, sometimes aggravated by high temperature of the feed material represents, therefore, a problem for standard NdFeB materials, for which a maximum operating temperature of 800 is recommended. In such situations, more advanced magnet materials with a higher temperature tolerance must be used.

2.4 2.4.1

Wet high-intensity magnetic separators Dry separation versus wet separation

Although dry high-intensity magnetic separators have been successfully applied to the beneﬁciation of a large spectrum of minerals, several basic disadvantages exist, which prohibit a wider use of a dry process. For dry magnetic separation to be successful, the ore must be completely dry and it almost invariably requires the ore to be sized into several fractions, each of which must be spread in a monolayer over the separators. With dry methods, care must also be taken to ensure control of a possible dust hazard, an expensive precaution both in capital and operating costs. Furthermore, dry separators have considerably lower throughputs than wet machines. While dry separators frequently yield an excellent separation on material coarser than 75 m, on unsized material containing a large portion of ﬁnes, the wet process is the only acceptable one. Considerable advantages must, therefore, be oered by dry separation to justify its use in preference to wet separation. In order to extend the process of magnetic separation to ﬁne weakly magnetic minerals, wet magnetic separators generating su!ciently high magnetic

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

97

Figure 2.35: The principle of operation of a continuous wet high-intensity magnetic separator. force in the working space must be used. A major development was achieved in this direction in 1955 by Jones [J1], who combined a high magnetic ﬁeld strength with Frantz’s idea of a magnetized matrix [F1]. By this approach, the magnetic force acting on magnetizable particles was increased by several orders of magnitude compared to dry magnetic separators. As shown in Table 1.1, a typical value of the product EuE for an Nd-Fe-B roll separator is 300 T2 /m, while with the magnetized steel wool matrix, this value is as high as 5×104 . Jones’s wet high-intensity magnetic separator (WHIMS) became the starting point of a remarkable progress in this ﬁeld and resulted in the development of a wide array of high-intensity high-gradient magnetic separators. This new type of separators extended the application of magnetic separation to classes of materials otherwise considered untreatable by magnetic means. A schematic diagram of operation of a continuous wet high-intensity magnetic separator is shown in Fig. 2.35.

2.4.2

Iron core-based wet high-intensity separators

Jones high-intensity magnetic separator The production-size Jones wet high-intensity separator is shown in Fig. 2.36 The magnetic ﬁeld in the working gap is generated by a conventional ironcore electromagnet and the ﬁeld gradient is enhanced by a matrix consisting of grooved plates of salient pole or of triangular groove plates, placed in the air gap. The plates, shown in Fig. 2.37, are vertically arranged in plate boxes that are placed around the periphery of the rotors.

98

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.36: Perspective view of a Jones continuous wet high-intensity magnetic separator (courtesy of Humboldt Wedag AG).

Figure 2.37: Grooved plates of Jones WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

99

Figure 2.38: Flush device for the magnetic fraction in the Jones WHIMS.

The slurry is gravity-fed onto the matrix where the magnetic particles are captured onto the plates, while the non-magnetic fraction passes through and is collected in a trough below the magnet. The feed points are at the leading edges of the magnetic ﬁeld. Feeding is continuous due to the rotation of the plate boxes in the rotors. Each rotor has two symmetrically disposed feed points. Before a plate box with captured particles leaves the magnetic ﬁeld, any entrained nonmagnetic particles are washed out by low-pressure water and these middlings are collected in a separate launder under the rotor. When the plate boxes reach the demagnetized zone half-way between the two magnetic poles, where the magnetic induction changes its polarity, and the magnetic ﬁeld is essentially zero, the adhering magnetic particles are washed out with high-pressure water sprays. A ﬂush device is shown in Fig. 2.38. The particles in the slurry feed should be smaller than 1 mm and this determines the gap between the grooved plates. As a rule of thumb, the gap width, measured between two grooved plate tips, should be 1.5 to 2 times the maximum particle size [B8]. Particle size distribution also aects selection of the pitch of the grooves. Salient pole plates are used when a high grade of the magnetic concentrate is required, while triangular groove plates are used when high recovery into the magnetic fraction is important. The height of the plates is 190 mm and the ﬁlling factor of the plate box can range from 50% to 80 %, depending on the type of plates and the gap between them. The maximum magnetic induction in the empty separation space does not exceed 1 T, although values up to 2 T are often stated. Such values can be

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

100

Table 2.4: Various models of Jones WHIMS. Type DP 335 DP 317 DP 250 DP 140 DP 90

Capacity [t/h] 180 120 75 25 10

Mass [t] 114 98 70 30 16

Rotor diameter [m] 3.35 3.17 2.50 1.4 0.9

Figure 2.39: Jones WHIMS DP 317 (courtesy of Humboldt Wedag AG).

achieved with the matrix installed in the plate box. The Jones separators are available in several sizes, some of them are summarized in Table 2.4. A photograph of a DP 317 separator is shown in Fig. 2.39. The Jones magnetic separators have been widely used in the mining industry to beneﬁciate a wide spectrum of minerals. Although these separators have been used to upgrade industrial minerals such as glass sand, feldspar and bauxite, the main area of application has been the concentration of weakly magnetic iron ores. The success of Jones separators has been based on sound mechanical design and reasonably e!cient performance. However, the grooved plates have proved to be an obstacle to long-term trouble free operation. As a result of the high ﬁlling factor of the matrix, several problems have been experienced. The frequently blocked matrix has to be removed from the plate boxes and the hard sediment must be laboriously removed. Also the eort to ﬂush the matrix,

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

101

Figure 2.40: Schematic diagram of the three-stage 6-ERM-35/135 magnetic separator [U2]. which represents up to 80 % of the volume of the plate boxes, with high-pressure water, sometimes results in uncontrolled spillage. 6-ERM-35/135 high-intensity magnetic separator The 6-ERM-35/135 WHIMS was developed in the former USSR in order to meet the increasingly demanding requirements for beneﬁciation of complex oxidized iron ores. It was observed [U2] that Jones separators could not ensure the e!cient separation of ores with complicated mineral composition and ﬁne dissemination, such as the deposits of Krivoy Rog and Kursk Magnetic Anomaly. While the design of the ERM separator is based on the Jones concepts, improved design of the matrix and of the feed mode, and incorporation of several stages of separation in one unit resulted in a greater resistance to matrix blockage, higher recovery and better selectivity of separation [U2, U3, T2]. A schematic diagram of the 6-ERM-35/135 separator is shown in Fig. 2.40. The three-rotor separator has two electromagnetic systems 1, each consisting of a magnetic circuit 2, two blocks of coils 3 and an additional upper pole 4. The rotor blocks 5, shown in Fig. 2.41, are positioned between the poles of the magnetic system. The upper rotor operates as a scalping stage to remove magnetite at a magnetic induction of 0.3 T. The lower rotors recover feebly magnetic particles at increasing magnetic induction, the lowest stage operating at a magnetic induction of 1.3 T. The throughput is speciﬁed as 100 t/h [U2]. The ERM separators are manufactured in the Ukraine by Magnis Co., Lugansk.

102

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.41: A rotor of the 6-ERM-35 magnetic separator. Eriez high-intensity magnetic separator Various designs of the magnetic circuits, diering from that of the Jones separators, were employed by other manufacturers of magnetic separators. For example, in the Eriez WHIMS, the carousel containing the matrix rotates between two poles of the electromagnet, as shown in Fig. 2.42. The background magnetic induction of up to 1.2 T in the air gap is generated by oil-cooled coils. Matrix types commonly used include expanded metal and steel balls. Commercial models range in capacity from 1 t/h to 120 t/h while the required input power ranges from 3 kW to 360 kW. A similar design was used by Boxmag-Rapid in their HIW separators. The matrix in these separators was trapezoidal wire bars placed at an angle in the carousel. For treatment of particles smaller than 30 m, the wedge wire was placed horizontally to increase the residence time. Figure 2.43 illustrates a single-head unit, while a photograph of two single rotor Boxmag-Rapid WHIMS operating in an ilmenite recovery plant is shown in Fig. 2.44.. Reading wet high-intensity separators The Reading wet high-intensity magnetic separators are based on yet another concept of the magnetic circuit design. The magnetic poles of the electromagnetic system, shown in Fig. 2.45 are arranged along the circumference of the carousel with polarity illustrated in Fig. 2.46. The iron cores are magnetized by oil-cooled coils. Each two poles with opposite polarity form a unit in which a high magnetic ﬁeld is generated and in which separation is taking place. The

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

103

Figure 2.42: Two-head Eriez CF-600 WHIMS, with capacity up to 60 t/h (courtesy of Eriez Magnetics, Inc.).

Figure 2.43: A single-head Boxmag-Rapid WHIMS (courtesy of Boxmag-Rapid, Ltd.).

104

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.44: Two Boxmag-Rapid WHIMS machines installed in an ilmenite recovery plant.

Figure 2.45: A detailed view of the magnet poles in the separation zones of the Reading WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

105

Figure 2.46: Schematic diagram of operation of the Reading wet high-intensity magnetic separator (courtesy of Roche Mining).

feed points are located close to the regions of the high magnetic ﬁeld. While the non-magnetic fraction passes through the matrix unaected, the magnetic fraction is ﬂushed from the matrix at the zero ﬁeld points that occur between the poles of like polarity. Grooved plates of the salient type are used as the matrix, with an air gap of 2.5 mm. The radial length of the matrix is 68 mm although a wider version with 120 mm radial length is also available. The throughput of these two versions is 2 t/h to 3 t/h per feed point for the narrower version and 4 t/h to 5 t/h per feed point for the wider model. The Reading WHIMS, shown in Fig. 2.47, are manufactured in several models, namely 4 pole (2 feed points), 8 pole (4 feed points) and 16 pole (8 feed points). The Reading wet high-intensity magnetic separators were developed by Reading of Lismore (Pty.) Ltd., Australia. They are well established in beach sand operations. Concentration of ilmenite, chromite and monazite are typical applications. The units are also applied to the beneﬁciation of ﬁne weakly magnetic iron ores and to puriﬁcation of various industrial minerals such as glass sand. Figure 2.48 illustrates the assembly of Reading WHIMS for application in the beach sand industry. The Reading product range was acquired by Roche Mining MT (formerly MD Mineral Technologies) in 2000.

106

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.47: The Reading 16-pole WHIMS (courtesy of Roche Mining).

Figure 2.48: Assembly of banks of Reading WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

107

Figure 2.49: Schematic diagram of the Ferrous Wheel magnetic separator, operating in rougher/cleaner mode (courtesy of Eriez Magnetics, Inc.).

Ferrous Wheel magnetic separator A Ferrous Wheel separator combines the basic concept of a high-gradient magnetic separator with the low-cost permanent magnet circuit. The principles of design and operation can be seen in Fig. 2.49. The vertical separating ring consists of two discs with the matrix situated in pockets between them, as shown in Fig. 2.50. The rings are assembled into a horizontal drum, the length of which is 5.5 m and outer diameter 2.4 m. Rotational speed of the drum is approximately 2 rpm. The length of the matrix, fabricated from screen cloth, is 150 mm. The choice of the mesh size of the screen cloth is determined by the size distribution of the feed ore. The separating ring is open in the middle to allow the removal of the separated products. Barium ferrite permanent magnets are mounted on each side of the separating rings, as is shown in Fig. 2.51. Each of the two magnetic heads covers an arc of 600 and the magnetic induction generated in

108

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.50: The Ferrous Wheel separating ring with 125 mm wide matrix (courtesy of Eriez Magnetics, Inc.). the gap is 0.1 T. The Ferrous Wheel separator allows a two-stage separation. The separator can be conﬁgured as either rougher/scavenger or rougher/cleaner, the latter mode being illustrated in Fig. 2.49. The feed enters the matrix in the magnetic zone located at the top of the ring. The non-magnetic particles pass through the matrix and are channeled out of the separator. This fraction represents the rougher tailings. The magnetic particles, collected onto the matrix, are ﬂushed from the matrix outside the magnetic ﬁeld and then introduced, from inside the separating ring, into the second magnetic head, to remove the entrained gangue material. An assembly of Ferrous Wheel separators is shown in Fig. 2.52. Roll-type wet high-intensity magnetic separator A useful wet alternative to dry induced roll high-intensity magnetic separators was developed in the nineteen sixties in the former USSR [D4, K2]. These separators, suitable for treatment of weakly magnetic, relatively coarse materials (up to 10 mm), consist of proﬁled rolls that rotate against proﬁled stationary poles. The poles and the rolls are magnetized by electromagnetic coils wound around the iron yoke. Various proﬁles of the rolls and of the pole pieces, as shown in Fig. 1.46, have been employed, their selection depending upon the required magnetic force and the application. Triangular teeth facing grooved poles with cuts were found to be the most e!cient proﬁle [D4]. Magnetic induction as high as 1.6 T can be achieved in the working zone of the separator. A schematic

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

109

Figure 2.51: Magnetic system of the Ferrous Wheel magnetic separator. Permanent magnets are located on each side of the vertical separating ring (courtesy of Eriez Magnetics, Inc.).

Figure 2.52: Ferrous Wheel separators under construction at Eriez Magnetics (USA) (courtesy of Eriez Magnetics, Inc.).

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

110

Feed

Magnetics Roll

Non-magnetics

Pole-tip

Coil

Iron yoke

Figure 2.53: Schematic diagram of a four-roll wet high-intensity magnetic separator. Table 2.5: Speciﬁcation of wet high-intensity roll magnetic separators. Parameter Throughput [t/h] Roll diameter [mm] Roll length [mm] Number of rolls Magnetic ﬁeld [T] Mass of separator [t] Water consumption [m3 /h] Input power [kW]

5SVK 2 to 6 300 2000 2 1.2 4.7 8 to 10 6

ERM3 5 300 2000 4 1.6 10.9 8 to 10

2MSM5 3 to 6 270 2000 2 1.2 4.9 10 4

diagram of the four-roll separator is shown in Fig. 2.53 while an isometric view of the four-roll separator ERM-3 is shown in Fig. 2.54. A detailed view of the proﬁled roll can be seen in Fig. 2.55. The lower pole tip contains slots through which the non-magnetic fraction leaves the separator. Magnetic particles from the feed are attracted to the teeth of the roll and are discharged when the roll leaves the sphere of inﬂuence of the magnetic ﬁeld. Typical speciﬁcations of various models of wet high-intensity roll magnetic separators are summarized in Table 2.5. A photograph of a 2-MSM-5 separator is shown in Fig. 2.56. These separators were successfully applied to the beneﬁciation of coarse (- 5 mm) manganese ore, iron ores such as siderite and limonite, and to the removal of serpentine from magnezite. While these separators cannot treat e!ciently

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

111

Figure 2.54: A four-roll wet high-intensity roll magnetic separator ERM-3.

Figure 2.55: A detailed view of the proﬁled roll of a wet high-intensity roll magnetic separator.

112

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.56: 2-MSM-5 wet high-intensity roll magnetic separator (courtesy of ˇ B, Czechoslovakia). Z very feebly magnetic and very ﬁne particles, their main advantage, compared to WHIMS, is the ability to treat coarse particles and the absence of the matrix blockage. The range of applicability is similar to that of the rare-earth drum magnetic separators, although the ﬁeld generated by these separators is somewhat higher than that by the drum separators, with similar magnitude of the ﬁeld gradient. Further advantage of wet induced roll separators is that it is possible to control the magnetic ﬁeld strength. They can be e!ciently applied to materials that fall between low-intensity magnetic separation and high-intensity high-gradient separation.

2.4.3

Solenoid-based magnetic separators

All wet high-intensity magnetic separators already discussed have produced the magnetic ﬁeld by means of an electromagnet with iron yoke. For small working volumes and for moderately large magnetic induction, this constitutes an e!cient and relatively cheap design, although the machines tend to be massive. The input power needed to saturate the iron poles is modest and reasonably high magnetic induction, of the order of 1 T, can be generated in the air gaps, which guarantees su!ciently high throughputs (tens of tonnes per hour) of ﬁne weakly magnetic material. However, it follows from the discussion in Section 1.7.3 that this design suers two serious drawbacks: a. The maximum magnetic induction that is obtainable in the working volume is limited by the saturation polarization of iron (approximately 2 T). Since such an induction can be generated only in a narrow gap, much lower inductions

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

113

Figure 2.57: Frantz Ferroﬁlter magnetic separator. are usually created in units designed for practical large-scale applications. b. Scale-up is very di!cult. In order to increase the throughput, the gap between the poles must be increased. This results either in a dramatic drop in the magnetic induction in the working volume, or in a substantial increase in the number of ampere-turns in order to maintain the same magnetic induction. The machine becomes extremely massive in relation to its capacity, magnetic induction becomes increasingly limited by the width of the gap, and the cooling of coils also becomes a problem. To generate su!ciently large magnetic induction at large volumes, it is necessary to use an iron-clad solenoid, as has been analyzed in Section 1.7.3. Frantz Ferroﬁlter The ﬁrst magnetic separator that used the iron-clad solenoid was the so-called Frantz Ferroﬁlter, introduced by S.G. Frantz in 1937 [F1]. This separator, shown in Fig. 2.57, became the conceptual basis of cyclic high-gradient magnetic separators. It consists of an iron-bound solenoid magnet generating a magnetic ﬁeld of about 0.15 T, while the matrix is formed by screens fashioned from thin sharp ribbons of magnetic stainless steel, as shown in Fig. 2.58. The device operates intermittently; the ﬂow is interrupted, the magnetic ﬁeld is reduced to zero and the magnetic particles are backwashed. Then the ﬁeld is switched on again and the entire cycle is repeated. Because of the low demagnetizing factor of the ribbon elements that are

114

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.58: A ribbon matrix used in a Frantz Ferroﬁlter. oriented parallel with the direction of the magnetic ﬁeld, the magnitude of the background magnetic induction was su!cient for the recovery of ﬁne ferromagnetic particles. However, in order to magnetize the randomly oriented ﬁlamentary matrix with very high aspect ratio, a much higher magnetic ﬁeld is needed. As a means of achieving a high degree of retention of quasicolloidal, feebly magnetic impurities from kaolin, Frantz’s concept was extended so that more powerful iron-clad solenoids were used in conjunction with randomly oriented steel wool. The early developments of cyclic high-gradient magnetic separators are described in detail in references [O3, K5, K7, I2, I3]. Modern cyclic high-gradient magnetic separators The ﬁrst industrial high-gradient magnetic separator, which grew from Frantz’s concept and from investigations into the removal of weakly magnetic discolouring agents from clays was built in 1969 [O4]. Figure 2.59 shows schematically the essential elements of operation of such a separator. The system comprises a canister ﬁlled with a matrix formed of compressed mats of magnetic stainless steel wool, although other types of matrices can be used. The canister is placed in an iron-clad solenoid which generates a magnetic induction up to 2 T. The matrix creates a high degree of non-homogeneity of the magnetic ﬁeld and produces a large magnetic force acting on the magnetizable particles. The slurry is fed to the canister either vertically downwards or upwards through the matrix with the magnetic ﬁeld switched on. The magnetic particles from the slurry are trapped into the surface of the magnetized matrix, while the non-magnetic particles pass through the canister. When the matrix has been loaded with the magnetic particles, the ﬂow is halted, the magnetic ﬁeld

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

Figure 2.59: Schematic diagram of operation of a cyclic HGMS.

Figure 2.60: An automated small capacity cyclic Sala-HGMSW P

115

116

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.61: High-gradient magnetic ﬁlter for e"uent control in the steel industry (courtesy of Metso Minerals, Ltd.). is reduced to zero and the magnetic fraction is ﬂushed from the matrix. Such cyclic devices are useful in applications where a slurry to be processed contains a small fraction of magnetic particles. These machines have found a widespread application in the kaolin industry and in waste water treatment. A range of cyclic high-gradient magnetic separators is manufactured by several companies. The solenoid diameter ranges from 1 m to 3 m, input power from 100 to 500 kVA and throughput as high as 200 t/h is claimed. Figure 2.60 shows a small-scale cyclic HGMS while Fig. 2.61 presents a Metso Minerals cyclic HGMS for waste water ﬁltration. A production-scale Eriez Magnetics HGMS for puriﬁcation of kaolin is shown in Fig. 2.62. Dry Allis-Sala HGMS Dry matrix high-gradient magnetic separation was developed by Allis Sala [J7] in order to extend applicability of dry separation to such a ﬁne particle range that cannot be easily beneﬁciated by roll or drum dry separators. Schematic diagram of the separator is shown in Fig. 2.63. The magnetic ﬁeld is generated by an iron-clad water-cooled solenoid and the matrix is placed in the bore of the coil. Particle transport through the matrix is accomplished by a compressed air-driven vacuum pump. The pump sucks the air through the heater into the separation circuit. The air inlet is positioned at the feed point, where the pre-heated air and particles are mixed before entering the matrix. The economic expansion of high-gradient magnetic separation to numerous mineral processing applications requires the utilization of fully continuous mag-

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

117

Figure 2.62: Eriez Magnetics cyclic HGMS for kaolin beneﬁciation (courtesy of Eriez Magnetic, Inc.).

Air heater

Feed

Air

Filter bed with matrix

Solenoid

Vacuum pump

Figure 2.63: Schematic diagram of dry Sala HGMS.

118

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.64: Continuous Sala high-gradient magnetic separator. netic separation. Cyclic devices are limited in their use to separations in which the magnetic fraction is a small portion of the feed and to the feeds that must be passed through the device at controlled slow feedrates. Continuous solenoid high-gradient magnetic separators have eliminated the limitations of the cyclic machines and several advanced devices have been built. Sala-HGMS carousel separator The Sala-HGMS carousel separator was developed from the cyclic separator to meet the need for a continuous industrial machine capable of processing ores containing a high proportion of magnetics [O5, M9, A5]. As can be seen in Fig. 2.64, a double-saddle iron-clad coil surrounds the carousel ring. Seals mounted on the ring allow independent control of feed and ﬂush velocity to enhance the separation and to increase the ﬂushing e!ciency of the magnetics. The operational sequence is similar to that used in conventional continuous iron-core-type high-intensity separators as is evident in Fig. 2.65. Further advantage of such a magnetic separator is that it can be scaled up to treat high volumes of material. Magnetic ﬁeld is parallel to the slurry ﬂow. When increased throughput is required, the width of the magnet is increased, while its height remains constant. The surface area of the matrix can, therefore, be enlarged without increasing the width of the air gap and thus the number of ampere-turns to generate the required magnetic ﬁeld. The iron return frame reduces the magnetic ﬂux leakage to places outside the magnetic head. In high-intensity magnetic separators with iron yokes, the stray

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

119

Figure 2.65: The operational sequence in a continuous Sala HGMS [A5]. magnetic ﬁeld is so high despite a reversal of polarity of two adjacent magnetic heads that the magnetic induction in the ﬂush station area usually amounts to about 20 mT. This is su!ciently high to hamper the e!cient ﬂushing of the matrix. With iron-clad solenoids, the magnetic induction outside the magnet is as low as 2 mT, depending on the matrix used. Sala HGMS are manufactured under the Metso Minerals label in various models. The number of magnetic heads ranges from one to four and magnetic induction varies from 0.5 T to 2 T. Throughput of 200 t/h per magnet head is speciﬁed for the largest model 480 ABCD. The matrix is, typically, a compartmented stack of expanded metal screens. A photograph of a single-head Sala-HGMS unit, with nominal throughput of 15 t/h is shown in Fig. 2.66. The largest model that is presently being oered by Metso Minerals is the HGMS 350 shown in Fig. 2.67. This unit can be ﬁtted with up to three magnetic heads and can reach a throughput up to 300 t/h. VMS magnetic separator A novel concept for replacement of a horizontal rotor or carousel by a vertical wheel was incorporated in the VMS magnetic separator. The VMS magnetic separator, the isometric view of which is shown in Fig. 2.68, was developed in the Ore Research Institute in Prague, in former Czechoslovakia [H9, H10, C7]. A magnetic ﬁeld is generated by the horizontally oriented solenoid wound with a water-cooled hollow conductor. The coil is enclosed in steel cladding, the upper and lower pole-pieces of which are perforated to allow passage of the slurry. The slurry is fed into the separator via a feed box and it then enters

120

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.66: MK III Sala-HGMS carousel unit.

Figure 2.67: A three-head HGMS 350 carousel machine (courtesy of Metso Minerals, Ltd.).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

121

Figure 2.68: An isometric view of VMS. a rotating drum, which carries separation chambers ﬁlled with matrix. The non-magnetic and the middling fractions are collected in launders underneath the magnet. Magnetizable particles are attracted to the matrix, placed in compartments along the periphery of the vertical wheel. When the matrix leaves the region of the magnetic ﬁeld during the rotation of the wheel, the captured particles are ﬂushed from the matrix. The magnetic product is thus washed o from the matrix at the ﬂush station in a direction opposite to that of the feed and is collected in the trough at the bottom of the separator. The maximum background magnetic induction generated by the magnet is 1.7 T, while stray magnetic induction outside the magnet is less than 5 mT. Mild steel rods of 3 mm and 5 mm in diameter, with spacing of between 1.5 mm and 2.5 mm, are used as a matrix. Woven wire mesh has also been used in some applications. In order to increase the capacity of a magnetic separator, the width of the working space must be increased. The VMS concept allows this very simply by increasing the width of the wheel. Taking into account that the magnetic ﬁeld in the VMS separator is oriented vertically, perpendicularly to the increase of the wheel width, the basic characteristics of the magnetic circuit remain unchanged, i.e. the vertical length of the air gap, which determines the magnetomotive force, or the number of ampere-turns needed to achieve the required magnetic induction, is the same for any width of the wheel. Because of the increase in the length of the conductor, energy consumption increases only linearly with the wheel width. A throughput of up to 150 t/h was speciﬁed for the largest separators VMS 100.

122

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.69: A vertical ring of the VMS HGMS, with matrix compartments ˇ B Spišská Nová Ves, Slovakia). (courtesy of Z

Figure 2.70: VMS high-gradient magnetic separator (courtesy of Ore Research Institute, Czech Republic).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

123

Figure 2.71: VMS-100 separators in a manganese ore beneﬁciation plant in the Ukraine (courtesy of Ore Research Institute, Czech Republic).

By replacing the conventional horizontal rotor by a vertically rotating wheel, Fig. 2.69, the VMS separator also addressed the problem of matrix clogging, an onerous problem for most carousel WHIMS or HGMS machines. The reverse ﬂush and very low stray magnetic ﬁeld in the ﬂush section are additional features of this separator. The VMS magnetic separator, shown in Fig. 2.70, was manufactured in sevˇ B Co. in the former Czechoslovakia. These separaeral models and sizes by Z tors were earmarked for incorporation into the Krivoy Rog and Kursk Magnetic Anomaly iron ore beneﬁciation plants in the Ukraine. The proposed capacity of the plants was 30 Mt/a and it was envisaged that at least forty VMS separators, each with capacity of 100 t/h, would be required. At the same time, several units, Fig. 2.71, were installed in manganese ore beneﬁciation plants in the Ukraine. In many demanding applications, particularly when feebly magnetic admixtures from industrial minerals are to be removed, it is necessary to control the residence time of the slurry in the separating zone and thus the ﬂow velocity through the matrix. To cater for such applications, the VMS separator was modiﬁed in such a way that the magnetic system was situated below the rotation axis of the rotor. This VMKS separator, shown in Figure 2.72 and schematically in Figure 2.73, generates a magnetic induction of 2 T and has a rotor diameter of 3 m, width of 1.4 m and throughput of 10 t/h. It was successfully applied to puriﬁcation of kaolin [Z3].

124

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.72: Continuous magnetic separator VMSK for puriﬁcation of kaolin (courtesy of Ore Research Institute, Czech Republic).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

125

Figure 2.73: Sectional view of the VMKS separator for kaolin puriﬁcation (Ore Research Institute, Czech Republic).

SLON magnetic separator It became obvious in the late eighties, that the use of an iron-clad solenoid and application of the reverse ﬂush of the matrix enhances the e!ciency, scalability and availability of continuous high-gradient magnetic separators. The technical success of VMS separators prompted further innovative eort. The SLON HGMS, developed in 1988 by Ganzhou Non-ferrous Metallurgy Research Institute, Ganzhou, China [X1], and shown in Figure 2.74, is based on the VMKS concept. However, in order to improve the e!ciency of separation even further, the pulsation of the slurry within the matrix was incorporated into the SLON separator. The pulse generator induces vertical pulses in the slurry within the matrix. The particles are thus exposed to the pulsation force, which is much greater than the force of gravity and acts in both directions [Y2]. By the pulsation action, the mechanically entrained non-magnetic particles are removed from the matrix, which results in improvement of the quality of the magnetic concentrate. At the same time, the pulsation allows the magnetic particles in the slurry to be exposed to the entire depth of the matrix, which increases the recovery of the magnetic component. The SLON separators are manufactured in several models, speciﬁcations of three of which are listed in Table 2.6. The separator is used, on a large scale, to beneﬁciate feebly magnetic iron and ilmenite ores and appears to enjoy considerable commercial success in China.

126

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.74: SLON-2000 pulsating high-gradient magnetic separator (courtesy Ganzhou Non-Ferrous Metallurgy Research Institute, China).

Table 2.6: Parameters of SLON magnetic separators. Parameter Ring diameter [mm] Maximum magnetic induction [T] Input power [kW] Pulsating stroke [mm] Feed size [mm] Feed solid density (%) Throughput [t/h] Mass of the machine [t]

SLON-1000 1000 1

SLON-1500 1500 1

SLON-2000 2000 1

26 0 to 30 -1 10 to 45 4 to 7 6

38 0 to 30 -1 10 to 45 20 to 35 20

82 0 to 30 -2 10 to 45 50 to 80 50

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

127

Figure 2.75: SLON-1500 magnetic separators operating in Pang Zhi Hua ilmenite processing plant in China (courtesy of Ganzhou Non-ferrous Metallurgy Research Institute, China). It is set to make inroads into international markets. Figure 2.75 illustrates the operation of a bank of SLON-1500 separators in the Pang Zhi Hua ilmenite processing plant (China). Other innovative designs of solenoid-based magnetic separators Matrix blockage and insu!cient throughput was the main limitation to recovery of uranium and gold from Witwatersrand ores and cyanidation residues by wet high-intensity magnetic separation [C8]. In order to satisfy all the requirements for a cost-eective and reliable machine that would be able to operate for a su!ciently long period in industrial conditions, the Council for Mineral Technology (Mintek), Randburg, South Africa, designed and constructed a prototype separator [S14] shown in Figure 2.76. The design of the Mintek linear magnetic separator was based on a split-coil magnet that consisted of two parallel short race-track coils, internally watercooled, separated by a gap through which the matrix could pass. This pair of coils was enclosed in a steel cladding. The matrix consisted of woven mesh screens held vertically on a ﬂexible belt. The belt moved linearly in a horizontal direction and inverted back on itself by means of pulleys. As the belt moved round the pulleys, the matrix elements ﬂared out, thus facilitating the removal of ferromagnetic material and wood chips. The residual mechanically entrained particles were then removed by a reverse ﬂush on the lower side of the separator.

128

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.76: The Mintek linear high-gradient magnetic separator. Scale-up of the machine could be accomplished by increasing the width of the belt and by the installation of two to four magnetic heads in a single machine along the belt. Although the separator performed well on pilot-plant scale, non-technical issues prevented the industrial application of the machine. An innovative approach to the concept of the VMS separator was employed by Magnetic Technology Consultants (MTC) (South Africa) who designed and built a high-gradient separator (Figure 2.77) designed to treat weakly magnetic materials [A6]. Figure 2.78 illustrates the MTC separator operating in a glass sand plant. The feed material containing 0.08 % Fe2 O3 was upgraded to 0.022% Fe2 O3 in the ﬁrst pass and to 0.011% Fe2 O3 in the second pass. Although the separator was designed primarily for wet applications, it was successfully tested in a dry mode. A vacuum system with vacuum seals was used to propel the pyroxenite ore through the matrix and high velocity of the ore and thus high throughput were achieved.

2.5

Superconducting magnetic separators

Although high-intensity and high-gradient magnetic separators that use resistive magnets meet, in most instances, the technological requirements of the mining and materials industries, their cost-eectiveness is impaired by high energy consumption, the need to cool the windings, limited working volume and considerable mass owing to the massive iron yokes or cladding. These disadvantages can, however, be overcome by using superconducting magnets, which

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

129

Figure 2.77: The MTC continuous HGMS separator (South Africa).

Figure 2.78: MTC HGMS separator at the glass sand plant. The feed into the separator is on the right-hand side while the non-magnetic product in the ﬁrst pass is shown on the left.

130

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

oer a number of advantages: a) Superconducting magnets can produce high magnetic induction in large volumes at low energy consumption. The power is required mainly for cooling rather than to compensate for ohmic losses in the coil of the magnet. Moreover, the cost of cooling is independent of the magnetic ﬁeld generated, unlike resistive magnets where the cost of cooling is proportional to the square of the ﬁeld intensity. The economic e!ciency of the superconducting magnets thus increases with increasing ﬁeld strength. In some applications the increased magnetic ﬁeld allows the ﬂow rate of the slurry to increase and thus the throughput of the separator increases. b) Since iron cladding is generally not needed, the machine can be made physically smaller. c) The superconducting coils can be arranged in such a way that a su!ciently large ﬁeld gradient can be generated without using a matrix, while still maintaining high magnetic force. Two types of magnetic separators that use superconducting coils have been introduced into industrial practice, namely the matrix separators and opengradient magnetic separators (OGMS). The matrix separators fall into two distinct design categories, namely cyclic vertical ﬂow units operating with liquid nitrogen and helium liqueﬁer, and reciprocating HGMS. As a simple extension of the matrix-based high-gradient magnetic separators, the conventional resistive solenoid magnet was replaced by a superconducting coil. These separators operating in the cyclic mode in the switch on/o regime are based on short, large diameter, coils, processing at slow slurry velocities with fairly infrequent ﬂushing. In order to minimize the energy consumption and the running costs of superconducting magnet systems, the magnet should be as passive as possible. The persistent mode option allows the magnet to remain energized with no additional power input. Elimination of the switch on/o regime would also result in a longer duty cycle and thus in higher throughput of the separator. These issues of a passive magnet were addressed by the reciprocating concept [S15, W4, R3]. In this operation, one canister with the matrix processes the slurry while the second canister is cleaned in a region of zero magnetic ﬁeld. This technology, ﬁrst proposed by English China Clays, was not viable until the magnet technology caught up with the operational requirements in the early nineties [R4]. The second type of superconducting magnetic separators, namely OGMS, is based upon deﬂection of magnetizable particles in a non-homogeneous magnetic ﬁeld, according to their magnetic susceptibility and size. Instead of employing a matrix to generate a magnetic ﬁeld gradient, the geometry of the magnet winding is used to create the ﬁeld gradients and magnetic force that deﬂects the magnetizable particles. These open-gradient magnetic separators include a linear multipole separator and a drum magnetic separator.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

131

LHe standpipe Slurry out

Liquifier

LHe Dewar LHe GHe

LHe GHe Slurry in

Superconducting magnet

Figure 2.79: Schematic diagram of a cyclic superconducting HGMS.

2.5.1

Cyclic superconducting HGMS

The cyclic resistive high-gradient magnetic separators were exclusively designed for puriﬁcation of kaolin. A resistive magnet of diameter of 2100 mm (84”) generated the ﬁeld of 1.8 T at a power input of up to 400 kW. Bigger units with a solenoid diameter of 3000 mm and weighing up to 625 tonnes consumed 600 kW. In order to reduce the energy consumption, the Huber Corporation (USA) decided to replace the resistive solenoid by the superconducting coil. A schematic diagram of a cyclic superconducting HGMS is shown in Fig. 2.79. The ﬁrst such unit, designed and built by Eriez Magnetics and shown in Fig. 2.80, was installed at Huber Corp. in May 1986 [S16]. The ﬁlling factor of the steel wool matrix is about 6% and the matrix is 500 mm deep. The clay slurry is pumped from holding tanks into the distributor header; it ﬂows upward through the matrix to the return header. A typical ﬂowrate is between 1 and 2 m3 /min, and typical retention time ranges from 50 to 90 seconds [W5]. After a period of time, the matrix accumulates enough magnetic material so that the e!ciency of separation drops o. At this point the slurry feed is stopped, the magnet is de-energized, and the steel wool is washed in both directions with clean water. The magnet is then re-energized and the feed slurry is re-started. A typical duty cycle is 26 minutes separation, 1 minute of de-energizing, 2 minutes of ﬂushing and rinsing, and 1 minute of re-energizing [W5]. This process means that two dead time periods occur during the ramp up and down of the magnetic ﬁeld, along with a dead time while the ﬂush of the magnetics is carried out. In order to reduce this dead time, fast ramp

132

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.80: A cyclic superconducting Eriez Magnetics HGMS for kaolin beneﬁciation (courtesy of Eriez Magnetics, Inc.). superconducting magnets are used. The coil and power supply are subjected to rapid current cycles in order to apply and remove the magnetic ﬁeld. This results in increased heating of the coil by eddy currents and larger and more expensive cooling power is required. A more robust power supply to drive the current quickly is also required. This results in signiﬁcant cyclic stresses within the magnet itself [R4].

2.5.2

Reciprocating superconducting HGMS

Superconducting magnets can take advantage of a higher magnetic ﬁeld compared to resistive magnets, and can increase the processing velocity. However, as the slurry velocity increases, the duty cycle decreases and the economics of separation is aected. Also, for the optimum operation of a superconducting magnet, taking into account coil stresses, ﬁeld uniformity and power requirements, it is preferable to operate the superconducting HGMS in persistent mode. The issues of long duty cycles of separation and of optimum magnet operation are addressed by a reciprocating technology. In order to achieve economic operation, the captured particles must be ﬂushed from the matrix, with the ﬁeld on, and the capture zone must, therefore, be removed from the magnetic ﬁeld. The train of canisters, as shown in Figure 2.81, is moved by means of a ram that operates on a magnetically balanced canister, which houses a multi-section separation region. As one matrix canister is engaged in separation, the second is undergoing ﬂushing and rinsing. Reciprocation can be accomplished in 10

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

133

REFRIGERATOR

Reciprocating matrix train

Product DUMMY

ACTIVE

DUMMY

ACTIVE

DUMMY Feed

LINEAR ACTUATOR

Iron yoke

Superconducting coil

Figure 2.81: Schematic diagram of a reciprocating canister HGMS.

seconds [S17]. While economic design of resistive solenoids is based on short, large diameter coils, for superconducting coils it is far simpler to provide a coil whose length is greater than the diameter. Such a geometrical arrangement, used in Outokumpu/Carpco separators, allows the use of a radial slurry ﬂow rather than an axial ﬂow. As can be seen in Figure 2.82, the radial ﬂow allows the feed area, and thus the throughput, to be increased. The ﬁrst industrial superconducting magnetic separator was designed by the Institute for Refrigeration Engineering in Prague, Czech Republic [F6, K8]. This 5 T unit, shown in Figure 2.83 was a reciprocating canister machine for the beneﬁciation of kaolin. Although, initially, the performance of the separator was encouraging, subsequent deterioration in e!ciency and drop in throughput as a result of matrix blockage were given as the main reasons for closure of the separator [A7]. It was suspected that insu!cient velocity of ﬂush water and a strong stray magnetic ﬁeld in the ﬂush station were the main sources of the problems. In order for a superconducting magnet to operate, it has to be cooled below its critical temperature. The most common way of cooling such a magnet is to immerse it in a bath of liquid helium at 4.2 K within a vacuum-insulated cryostat. The period between liquid helium additions can be further extended by using thermal insulation and liquid nitrogen. Mechanical coolers, based on the Giord-McMahon refrigeration cycle, can extend the period between helium reﬁlls ever further. In this technique, a small volume of high-purity helium gas recirculates through a closed loop, generating a cooling eect at the point of

134

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.82: Diagram of an active matrix canister in reciprocating superconducting HGMS (Outokumpu Technology, Carpco Division).

Figure 2.83: The Czechoslovak reciprocating-canister superconducting magnetic separation for beneﬁciation of kaolin.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

135

Table 2.7: Cryoﬁlter HGMS models [S18]. Cryoﬁlter Model 5T/200 5T/360 5T/460 5T/1000

Application Pilot Industrial Industrial Industrial

Throughput 400 kg/h up to 15 t/h up to 50 t/h up to 150 t/h

Figure 2.84: Superconducting Cryoﬁlter HGMS (courtesy of Outokumpu Technology, Carpco Division). forced gas expansion. Carpco Cryoﬁlter systems are using this concept of a combination of a liquid helium bath and mechanical cooling, which ensures a reﬁll period of 1 year in normal processing operations [K9]. R ° Further developments in the Oxford Instruments Cryofree technology now allow superconducting magnet systems to be totally cooled by mechanical means, removing the requirement for helium completely [K9, A8]. Outokumpu Technology, Carpco Division, produce a range of the Cryoﬁlter HGMS employed mainly in kaolin puriﬁcation. Figure 2.84 illustrates the Outokumpu/Carpco Cryoﬁlter HGMS, while Table 2.7 lists Cryoﬁlter models. While the Cryoﬁlter supply package depends on the application, the primary items and options include [S18]: • Basic Cryoﬁlter with integral iron sheet, reciprocating canister and standard control package.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

136

Table 2.8: Comparison of resistive and superconducting cyclic magnetic systems for HGMS, with reciprocating superconducting separators [K9]. Magnet type 2100 mm resistive electromagnet 3000 mm resistive electromagnet 2100 mm superconducting magnet 3000 mm superconducting magnet 5T360 Cryoﬁlter 5T/460 Cryoﬁlter 5T/1000 Cryoﬁlter

Magnetic ﬁeld [T] 1.8

Mass [t] 270

Power [kW] 270 to 400

Capacity

1.8

625

300 to 400

2C

2.5

270

25

1.25C

2.5

625

25

2.5C

5 5 5

12 24 120

? 10 ? 10 ?12

0.4C 1.3C 4C

C

• Slurry handling system. • Advanced process control panel and SCADA monitoring system. • Detergent matrix wash system. Table 2.8 compares various types of matrix-based superconducting magnetic separators used for kaolin beneﬁciation [K9].

2.5.3

Open-gradient superconducting magnetic separators

The presence of a ferromagnetic matrix in high-gradient magnetic separators brings about a problem associated with keeping the matrix clean and passable under industrial conditions. One possible approach to eliminate the problems inherent in matrix machines is to employ a system in which magnetic particles are continuously deﬂected in a non-uniform magnetic ﬁeld, according to their magnetic properties and size. These open-gradient magnetic separators, designed for the treatment of ﬁne feebly magnetic materials, must be equipped with superconducting coils in order to provide su!ciently strong magnetic force. The ﬁeld gradients generated by a suitable combination of the conductor ﬁlaments or by coils of varying polarity are much weaker compared to the gradients created by a matrix. Magnetic induction exceeding 2 T is thus required to achieve adequate magnetic force. Figure 2.85 illustrates two dierent modes of operation of an open-gradient magnetic separator.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

137

Figure 2.85: Dierent systems of open-gradient magnetic separators: linear multipole system [(a) and (b)] and drum separator (c). Linear multipole OGMS The design of the linear multipole system, as shown in Figure 2.85 (a) and (b), is based on the concept of the ancient Edison’s deﬂection separator [T3]. It consists of an array of vertically positioned coaxial superconducting coils that are energized in opposite directions [S19]. In its simplest form, Figure 2.85(a), the dry ore is permitted to fall vertically as a curtain around the circumference of the magnet. The magnetic force directed radially inwards diverts the magnetic particles inwards while the non-magnetic particles fall vertically, unaected by the magnetic force. The method failed to meet expectations mainly because the separation was taking place away from the region of the highest magnetic force. As a result of low depth of the magnetic ﬁeld, its gradient and interparticle collisions, the metallurgical results were unsatisfactory even at low feedrates. An improvement was achieved by bringing the feed point close to the magnet and introducing a ramp, as is shown in Figure 2.85(b). The performance of the system was su!ciently encouraging for Cryogenic Consultants Ltd. (CCL) to design and build a production-scale Cryofos OGMS unit for beneﬁciation of the pyroxenite ore in South Africa [G3]. In order to circumvent scale-up problems of magnets of cylindrical geometry used up to that time for OGMS, Good [G3] abandoned the cylindrical geometry in favour of a linear geometry. The split pair was replaced by a linear dipole of rectangular cross section, each side having a separation length of 3 m. The separator could be utilized along almost its entire length on both sides of its axis. Unfortunately, the magnet and the cryogenic system proved to be di!cult to manufacture and the separator never reached operational status [S1].

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

138

Figure 2.86: Superconducting drum magnetic separator Descos (Humboldt Wedag AG). Further development at CCL and at Carpco Inc. addressed the issues of the optimized feeding close to the region of the strongest magnetic force and of the removal of the magnetic particles from the walls of the separator. The concept of a ﬂat-faced magnet inclined at an angle with respect to the feeder R ° evolved into the Cryostream series of OGMS units marketed by Outokumpu Technology, Carpco Division [K9, S17]. In spite of considerable design progress, the concept of Cryostream has not yet enjoyed commercial success. Descos OGMS The drum magnetic separator developed by KHD Humboldt Wedag AG employed a multipole magnet and combined the advantages of a superconducting magnet with those of a conventional drum separator. As can be seen in Fig. 2.86, eight poles of the magnet system were arranged along one third of the circumference of the drum. Four race-track coils were placed in a liquid helium tank and generated 3.2 T on the surface. The drum of the separator was made of carbon-ﬁbre reinforced plastic. The diameter of the drum was 1200 mm and its length 1500 mm. Commercialization of the product proved to be di!cult as a result of its high cost, in spite of its reportedly satisfactory metallurgical performance.

2.6

Laboratory magnetic separators

A rule that applies to magnetic separation as much as to most physical separation techniques, is that the quickest and surest way of ﬁnding out how a material

2.6. LABORATORY MAGNETIC SEPARATORS

139

will behave in a separator is to run it through the machine. Theoretical models of the process, which would help to predict the e!ciency of low-intensity magnetic separation are scarce and mostly too simpliﬁed to be of practical value. A wealth of theoretical descriptions of high-intensity and high-gradient magnetic separation applies mainly to idealized situations, with limited signiﬁcance for practical problems. The information obtained from these models can sometimes even be misleading and this, combined with the fact that magnetic and some physical and chemical properties of the ores and other materials are di!cult to ascertain, indicates that laboratory tests should be carried out before conclusions can be drawn about the e!ciency of material treatment by magnetic means. A wide spectrum of laboratory devices and bench-scale magnetic separators have been built to simulate a particular process in a particular production-scale machine. Generally, the usefulness of these small-scale machines is limited. For instance, in magnetic separators based on permanent magnets, such as magnetic pulleys, overband magnets and drum magnetic separators, the magnetic ﬁeld generated is a function of the volume of the permanent magnets used in the manufacture of the separator. A small-scale separator will thus generate a lower magnetic ﬁeld, often of dierent pattern, compared to a production-scale machine. Moreover, physical dimensions of the separators, such as the diameter of a pulley or a drum, determine the residence time of material in the magnetic ﬁeld and thus the e!ciency of separation. Also, a small width of a magnetic roll or a drum introduces signiﬁcant end eects into the results. In laboratory-scale tests of high-gradient magnetic separation, it is essential to keep the matrix depth and ﬂow velocity of the slurry through the matrix the same as in the industrial conditions. Quite often it is not possible. Overall, tests on laboratory-scale units can thus be misleading and practical experience in evaluating the results of small-scale tests, on small, not necessarily representative samples, is essential. Commercially available laboratory-scale magnetic separators, such as Davis Tube and Frantz isodynamic separator can, however, be used for a reliable analysis of the separability of materials.

2.6.1

Davis Tube

A Davis Tube (DT), shown in Figure 2.87, is a laboratory instrument designed to separate small samples of strongly magnetic ores into strongly magnetic and weakly magnetic fractions. It has become a standard laboratory equipment used for the assessment of the separability of magnetic ores by low-intensity magnetic separators [S20, S1]. It was developed in 1921 and no signiﬁcant changes have been made in its design since then. The separator consists of an inclined tube 25 mm in diameter, placed between pole-tips of an electromagnet. Material to be separated is passed through the tube; the strongly magnetic fraction is held by the magnetic ﬁeld while the weakly magnetic material is washed down the tube.

140

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.87: Davis Tube magnetic separator.

Figure 2.88: The 3D model of the Davis Tube electromagnet [M24, M10].

2.6. LABORATORY MAGNETIC SEPARATORS

141

Figure 2.89: Frantz isodynamic separator.

Schultz [S20] suggested that a magnetic induction of 0.4 T or greater between the magnet poles should be used. However, Steinert and Boehm [S21] claimed that the current practice was to conduct the Davis Tube tests at a magnetic induction equal to that on the surface of the drum of the magnetic separator. Since it is the magnetic force or the force index, and not the magnetic ﬁeld strength, that are decisive in the operation, it is unlikely that this practice would yield correct information. Computer modelling of the pattern of the magnetic force generated by drum magnetic separators and a Davis Tube (shown in Fig. 2.88) was carried out by Murariu and Svoboda [M10]. It was found that in the case of conventional ferrite drum separators, with a standard gap of 25 mm between the drum and the tank, Davis Tube tests should be conducted at the magnetic induction of 0.1 T. On the other hand, correct assessment of performance of a rare-earth drum can be obtained by operating a Davis Tube at about 0.3 T or higher, depending on the design of the magnetic systems of the drum.

2.6.2

Frantz isodynamic separator

The Frantz isodynamic separator is a magnetic device that allows fractionation of materials based on their magnetic properties. This separator, shown in Fig. 2.89 consists of an electromagnet having two long pole pieces with a long narrow air gap between them. The pole design is such that the magnetic ﬁeld proﬁle is isodynamic, so that the magnetic force density across the width of the air gap

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

142 A

Fm Fg

ș

Magnetic fraction

mg

B

Non-magnetic fraction

Splitter

Figure 2.90: Forces acting on a particle in a Frantz isodynamic separator. is constant, i.e. EuE = frqvw=

(2.1)

Material to be separated enters the magnetic ﬁeld at point A, as is illustrated in Fig. 2.90. If the force of gravity Ij and the magnetic force Ip on a particle are balanced in such a way that the particle moves along the central line of the air gap, this particle has a 50 % chance of reporting to a magnetic or non-magnetic fraction. The balance of forces can be expressed as: ps j sin =

Ys EuE 0

(2.2)

where ps and Ys are the mass and the volume of the particle, respectively, j is the gravitational constant and is the transverse slope of the air gap. By re-arrangement we obtain: j " = 0 sin (2.3) EuE It can be seen that, because of the isodynamic pattern of the ﬁeld, the action of the separator on a particle is determined solely by its mass magnetic susceptibility, and is independent of the size and the mass of the particle. The magnitude of the term EuE is determined by the electric current L in the electromagnet so that sin (2.4) "= nL q where q and n are constants [M11]. With an electric current of 1.8 A, the magnetic induction at the narrowest part of the gap is approximately 2 T. In order

2.6. LABORATORY MAGNETIC SEPARATORS

143

Table 2.9: Chemical compounds used for calibration of magnetic susceptibility instruments. Compound Mohr’s salt Nickel sulphate Copper sulphate Cobalt sulphate Ferrous sulphate Manganese chloride Manganese pyrophosphate

Formula Fe(NH4 )2 (SO4 )2 ·6H2 O NiSO4 ·7H2 O CuSO4 ·5H2 O CoSO4 ·7H2 O FeSO4 ·7H2 O MnCl2 Mn2 P2 O7

" [107 ·m3 /kg] 4.1 2.0 0.74 4.6 5.2 15.4 12.9

to determine the exact values of these constants, each Frantz separator must be calibrated with compounds having well deﬁned values of magnetic susceptibilities. Chemical compounds usually used for calibration are listed in Table 2.9, together with their mass magnetic susceptibilities. Mass magnetic susceptibility " can thus be obtained from eqs. (2.3) or (2.4) by plotting the cumulative per cent recovery of the material into the magnetic fraction, versus the current. Typical magnetic proﬁles, or partition curves, are shown in Fig. 2.91. The mean magnetic susceptibility of a sample can be deﬁned as the value of " for which 50 % of the sample reports into the magnetic fraction. While the sample represented by curve 1 in Fig. 2.91 has a narrow distribution of magnetic susceptibility, the sample described by curve 2 contains a wider spectrum of the values of magnetic susceptibility. The Frantz magnetic barrier separator While the Frantz isodynamic magnetic separator employs the isodynamic pattern of the magnetic force density, expressed by eq. (2.1), the operation of the barrier separator is based on the presence of the anadynamic and katadynamic force patterns [F7]. In the katadynamic region, the magnetic force increases with the increasing ﬁeld strength, while in the anadynamic region the force decreases with the increasing magnetic ﬁeld: g g EuE A 0 (katadynamic), EuE ? 0 (anadynamic) gE gE

(2.5)

As can be seen in Fig. 2.92, the magnetic force density between the pole tips of the separator is bell-shaped and creates a barrier in the isodynamic plane, between the katadynamic and anadynamic regions [J2]. Depending upon whether paramagnetic or diamagnetic susceptibility is to be exploited, a mixture of particles is fed into the anadynamic or katadynamic region. As the mixture moves under gravity towards the isodynamic plane, the magnetic force slows the particles of the susceptibility to be exploited and accelerates the particles having susceptibility of the opposite sign. In the vicinity of the barrier, where

144

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.91: Magnetic proﬁles, or magnetic partition curves, of two types of materials, as obtained by Frantz isodynamic separator.

Figure 2.92: Superimposed graphs of the magnetic induction and magnetic force density in the barrier separator, showing katadynamic (k) and anadynamic (a) regions.

2.6. LABORATORY MAGNETIC SEPARATORS

145

Figure 2.93: Rotating disk isodynamic magnetic separator. the magnetic force has the maximum value, particles having susceptibility such that the magnetic force equals or exceeds the opposing force of gravity, are deﬂected in the direction parallel to the isodynamic plane. Particles having susceptibilities lower, or of the opposite sign, pass through the barrier. The barrier separator thus allows selective separation and fractionation of materials based on small dierences in magnetic susceptibility [R5]. Disk isodynamic magnetic separator Frantz isodynamic separator is a selective device that allows separation of mixtures based on dierences in magnetic properties. This is in contrast to most other magnetic separators (such as roll, drum and matrix separators) which use the katadynamic ﬁeld pattern and are thus non-selective from ﬁrst principles. In these machines the separation is based on dierences in magnetic properties as well as on particle size. Frantz separator is a laboratory unit that does not lend itself to scale-up. In order to overcome limitations of the Frantz separator and, at the same time to retain its high selectivity, Gerhold et al. [G29, G30, G31] designed and built a rotating disk isodynamic magnetic separator shown in Fig. 2.93. The separator consists of a horizontally rotating disk and magnetic system with pole-pieces that generate an isodynamic magnetic ﬁeld in the separation gap. The magnetic force created by the magnetic system acts radially inwards while the competing force is the centrifugal force. This force can be adjusted to the values ranging from ﬁve to ten times the force of gravity.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

146

Pole

Pole

Tails

Tails

Pole

Feed

Pole Feed

Mags

Mags

Tails

Tails Rotating disc

Tails collector

Rotating disc

Tails collector

Figure 2.94: Schematic diagrams of operation of a dry rotating disk isodynamic separator, with two dierent proﬁles of the magnetic ﬁeld (adapted from Gerhold [G30]). Particles fed onto the disk assume the rotational velocity of the disk. The weakly magnetic particles are deﬂected outwards and are collected in a nonmagnetic bin. More strongly magnetic particles are deﬂected inwards in a form of a rotating ring and are removed before they each the feed region. The operation of the separator, with two dierent proﬁles of the magnetic ﬁeld, is shown schematically in Fig. 2.94. A pilot-scale separator with a throughput of 2 t/h, maximum magnetic induction of 2 T and ﬁeld gradient of 10 T/m, was built [G29] and selective separation of ferrimagnetic and strongly paramagnetic materials in the size ranging from 3 mm to 50 m was obtained [G30].

2.6.3

Separators with a rotating magnetic ﬁeld

Particle separation in rotating or alternating magnetic ﬁelds was proposed in the early years of development of magnetic separation technology [T3, D1]. It appears that this idea has not made its mark on the mineral processing industry. However, in many magnetic separators, the particle rotation is present as a sideeect rather then a deliberate attempt to rotate the particles. For instance, magnetic clusters in low-intensity magnetic separators are rotated slowly as they are carried past successive magnetic poles of opposing polarity. In doing so, the ﬂocs release mechanically or magnetically entrained ”non-magnetic” particles, improving thus the grade of the magnetic concentrate. In some applications it is possible to use particle rotation alone to achieve separations not possible using conventional attraction-based magnetic separation, as has been shown by Allen [A9, A10, A11]. For instance, particles

2.7. EDDY-CURRENT SEPARATORS

147

Particle rotation

S

N

S Magnet travel

Figure 2.95: Generation of particle rotation. having similar magnetic susceptibilities, but considerably dierent magnetic anisotropies, can be separated from each other by their selective rotation. As a result of magnetic anisotropy the external magnetic ﬁeld exerts a torque on the particle in order to align its axis of easy magnetization with the direction of the external ﬁeld. If the magnetic ﬁeld generated, for example, by permanent magnets with alternating polarity, is moving, then the particles will rotate as is shown in Fig. 2.95. The concept of a rotating magnetic ﬁeld has been employed in rotating magnetic ﬁeld (RMF) laboratory separators developed and manufactured by Ka (Pty.) Ltd., Australia. Figure 2.96 shows an RMF lift separator that can be employed for separation by rotating weakly ferromagnetic or even paramagnetic particles with magnetic anisotropy. Figure 2.97 illustrates an RMF separator for separation of paramagnetic minerals. In these separators, the rotating magnetic ﬁeld is generated by a rotating magnet rotor ﬁtted with magnetic poles of alternating polarity around its circumference. The rotor in Fig. 2.96, rotating in a clockwise direction, produces a ﬁeld that appears (to a particle on the outer drum surface) to be rotating in an anticlockwise direction. Therefore, a magnetically anisotropic particle dropped onto the drum will respond by rotating in an anticlockwise direction. Non-rotating particles will be carried by the drum and its belt in a clockwise direction. RMF rotation separation is basically a separation of ferromagnetic (s.l.) particles from paramagnetic particles because of a large dierence in magnetic anisotropies and thus rotabilities of these two classes of materials.

2.7

Eddy-current separators

Although the ﬁrst patent for an eddy-current separator (ECS) was granted to T.A. Edison as early as 1889, a large-scale application of eddy-current separation started only recently, particularly in connection with the recycling of wastes

148

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.96: RMF lift separator (courtesy of Ka (Pty.), Ltd.).

Figure 2.97: RMF separator for separation of paramagnetic particles (courtesy of Ka (Pty.), Ltd.).

2.7. EDDY-CURRENT SEPARATORS

149

Figure 2.98: Eddy-current separator (courtesy of Steinert GmbH).

containing non-ferrous metals. The ﬁrst industrial ECSs were based on an electromagnetic ﬁeld induced either by single coils or by linear motor technique. As a result of the dramatic development of rare-earth magnets, the currently manufactured ECSs employ exclusively permanent magnets. Figure 2.98 illustrates such an eddy-current separator. The eddy-current technique is based on the fact that if conductive particles are exposed to an alternating magnetic ﬁeld, or move through a steady magnetic ﬁeld, eddy currents are generated within the particles. These eddy currents are generated in such a way that the magnetic ﬁeld they produce opposes the external magnetic ﬁeld, according to Lenz’s law. The opposite ﬁeld then produces a repulsive force (Lorentz force) on the particle. Particles are thus deﬂected from the stream of material, as is shown in Fig. 2.99, depending on their conductivity, size, shape, and the ﬁeld strength and the rate of change of the ﬁeld. The industrial eddy-current separators consist of two drums carrying a belt, the belt usually being driven by the rear steel drum. The front non-metallic drum contains a rapidly rotating magnetic system. The permanent magnets are arranged, with alternating polarity, along the circumference of the magnetic system. The separators usually have 6 to 18 poles which rotate at frequencies up to 3000 rpm. Depending on pole arrangement and the system speed, the frequencies of magnetic ﬁeld change up to 1 kHz are achieved [N3, H11]. Two main designs of eddy-current separators, each with two dierent magnet conﬁgurations, are illustrated in Fig. 2.100, while Table 2.10 reviews the designs used by various manufacturers. Type 2 design, which employs an eccentric magnetic system, is reported to have several advantages [N3, H11]. In concentric systems, strongly magnetic particles tend to accumulate between the belt and the magnetic drum and ulti-

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

150

Figure 2.99: Material separation in eddy-current separator (courtesy of Steinert GmbH).

Type 1

Type 2

Configuration A

N

S

Configuration B

N

S N S

S

N

N S

Figure 2.100: Two designs of drum eddy-current separators (after [N3]).

2.7. EDDY-CURRENT SEPARATORS

151

Table 2.10: Manufacturers of eddy-current separators [N3]. Manufacturer Steinert (D) Lindemann (D) Eriez Magnetics (USA) Huron Valley (USA) Andrin (F) Bakker Magnetics (NL) Raoul Lenoir (F) Newell Industries (USA) Rutherford Light Metals

Type 2 1+2 1 1 1 1 1 1 1

Conﬁguration A A A A or B A A A A B

mately to damage the drum. In eccentric design, the ferromagnetic material is removed automatically from the region of the magnetic ﬁeld generated by the rotating drum. The repulsive force acting by eddy currents on a small particle [S22, Z4] is proportional to: s g 2 (2.6) Iuhs ps E s i where ps and g are the mass and diameter of the particle, respectively, E is the magnetic induction and i the frequency of its change, and s and s are the electrical conductivity and density, respectively, of the particle. It can be seen that the e!ciency of separation is determined, amongst other factors, by the ratio of material conductivity and density. The larger the dierence in the values of this ratio for the materials to be separated, the more selective the separation will be. Table 2.11 lists this ratio for materials of interest in eddycurrent separation. It is evident that aluminium and magnesium can be rather e!ciently separated from semi- and non-conductors, while lead and stainless steel will not respond to eddy currents. Selection of dierent models of eddy-current separators is usually dictated by particle size distribution of the feed material and the required throughput. The width of the belt ranges from 500 mm to 2000 mm and nominal throughput is of the order of 10 m3 /h/m. Magnetic induction on the surface of the shell ranges from 0.25 T to 0.38 T. Particles in the size range - 100 + 5 mm are usually treated in standard ECSs. Separation of ﬁne particles Although separation of particles smaller than 5 mm poses a problem [Z5, R6], several innovative designs have successfully reduced the minimum particle size to 0.1 mm. The Steinert model 6119 [H11] and Raoul Lenoir model Eddybox, are claimed to be able to separate e!ciently particles as small as 1 mm. The Eddybox separator is based on free-fall of metallic particles through a magnetic structure, has no moving parts and is claimed to achieve a throughput as high as 1 t/h.

152

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Table 2.11: The material parameter for eddy-current separation [N3, S22]. Material Aluminium Magnesium Copper Silver Zinc and Zamac Gold Brass Tin Lead Stainless steel Glass Plastics

@ [103 ×s×kg1 ×m2 ] 13.0 12.2 6.3 6.0 2.4 2.1 1.3 to 1.8 1.2 0.45 0.18 0 0

Figure 2.101: Eddy-current separator Fourmi for separation of ﬁne particles (Raoul Lenoir).

2.8. SEPARATORS WITH MAGNETIC FLUIDS

153

Figure 2.102: Schematic diagram of an eddy-current separator based on rotation of ﬁne particles (courtesy of N. Allen). R ° The design of Fourmi eddy-current separator (Raoul Lenoir), shown in Fig. 2.101, is based on a horizontally rotating polar disc with radially mounted NdFeB permanent magnets. An alternating magnetic ﬁeld generates eddy currents in metallic particles that are fed on a stationary separation disc placed above the polar disk. The conductive particles, being acted upon by repulsive forces, become ﬂuidized and are removed by air jets. Particles as small as 0.1 mm are claimed to be e!ciently separated. It will be shown in Section 3.9.3 that with decreasing particle size the torque on a particle becomes an important force. Particles in ECS then respond to the ﬁeld changes by rotation rather than by repulsion. Allen [A21, A22] proposed the use of particle rotation as the separating mechanism of ﬁne metal particles. A schematic diagram of such an ECS based on particle rotation is shown in Fig. 2.102.

2.8 2.8.1

Separators with magnetic ﬂuids Basic concept

Separation in magnetic ﬂuids is a sink-and-ﬂoat technique, which exploits dierences in the densities of materials to be separated. In this technique, a magnetic ﬂuid, placed in a non-homogeneous magnetic ﬁeld, exhibits an apparent density dierent from its natural density [R7, R8]. This density can be controlled through a wide range of values, exceeding densities of all known elements and materials. While the scope of the conventional sink-and-ﬂoat technique is re-

154

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

stricted by a limited range of densities of the separation medium, the upper limit of ferrosilicon medium being approximately 3500 kg/m3 , and that of Clerici solution about 4200 kg/m3 at room temperature, magnetic ﬂuids allow densities as high as 20 000 kg/m3 or even higher to be achieved. The apparent density d of a magnetic ﬂuid placed in a non-homogeneous magnetic ﬁeld can be written (in SI units) as: d = 0 +

i EuE 0 j

(2.7)

where 0 is the physical (true) density and i is the volume magnetic susceptibility of the ﬂuid. The apparent density of a magnetic ﬂuid is thus dependent on the magnetic properties of the ﬂuid, and the magnetic ﬁeld strength and its gradient. A magnetic ﬂuid, placed in a non-homogeneous magnetic ﬁeld, is attracted to the regions of the highest magnetic ﬁeld. This magnetic force produces an opposite force within the ﬂuid that tends to expel an immersed non-magnetic body. This results in additional, magnetically generated, levitation, which causes particles to ﬂoat. In the early days, solutions of paramagnetic salts (such as MnCl2 ) were used as a magnetic ﬂuid [A12, A1]. As a result of their low magnetic susceptibility (of the order of 6×107 m3 /kg) very high magnetic ﬁelds and high gradient were required to achieve densities greater than those obtained using heavy liquids. For instance, in order to achieve an apparent density of the paramagnetic liquid equal to 3500 kg/m3 , the second term on the right-hand side of eq. (2.7) must be equal to 5×104 T2 /m. For a magnetic induction of 2 T, a gradient as high as 2.5×104 T/m is required. These are unrealistically high values, particularly for meaningful production-scale applications of this technique. In the late sixties of the last century methods of preparation of stable suspensions of nano-sized magnetite particles in hydrocarbon carrier ﬂuids were developed [P5, R10]. These ferromagnetic ﬂuids (ferroﬂuids) are considerably more magnetic than the paramagnetic liquid and become magnetically saturated at moderate magnetic ﬁelds. Equation (2.7) can then be re-written as: d = 0 +

Pi uE j

(2.8)

where Pi is the magnetization of the ﬂuid (in [A/m]). If magnetic polarization Mi , (in [T]) is used, then eq. (2.8) is expressed in the form d = 0 +

Mi uE 0 j

(2.9)

In fjv units eq. (2.8) can be re-written as d = 0 + where Pi and E are given in [G].

Pi uE 4j

(2.10)

2.8. SEPARATORS WITH MAGNETIC FLUIDS

155

FEED

MAGNET

PRODUCTS:

N

S

FLOAT SINK

MAGNETIC FLUID

Figure 2.103: Schematic diagram of a separator with magnetic ﬂuids.

Figure 2.104: Laboratory ferrohydrostatic separator FGS-40 (courtesy of GMUO, the Ukraine).

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

156

Table 2.12: FHS separators manufactured by GMUO [G4]. Model FGS-1A FGS-70 FGS-40 FGS-40/3 FGS-200

Feed size [mm] - 50 + 0.2 - 25 + 2.5 - 10 + 0.2 - 5 + 0.2 - 100 + 10

Throughput [kg/h] 60 200 5 2 4000

Density range [kg/m3 ] 1200 - 11 000 6500 - 10 000 4000 - 9000 2500 - 3500 3000 - 6000

It can be seen from eqs. (2.8) to (2.10) that in order to achieve a constant apparent density of separation, in a magnetically saturated ferroﬂuid, the gradient of the magnetic ﬁeld must be constant. This is achieved by suitably shaping the pole tips of the magnetic system. A ferrohydrostatic separator (FHS), which uses a ferroﬂuid as a working medium, thus produces two fractions, namely a ﬂoat and a sinks products. Figure 2.103 illustrates the concept of a separator with magnetic ﬂuids. The e!ciency of ferrohydrostatic separation decreases with decreasing size of particles. In order to overcome this ine!cient separation of ﬁne particles in gravity-based FHS, a rotation-based separation Magstream process was developed [W7].

2.8.2

Ferrohydrostatic separators

AVCO Corporation and NASA (USA) pioneered the FHS technique in 1973 by employing a kerosene-based ferroﬂuid to separate automobile scrap [M12]. Considerable eort to develop this technology was subsequently expended in Japan and the USA. Hitachi [N4], Nittetsu Mining Co. [S51], Tohoku University [S50] and US Bureau of Mines [R9] further conﬁrmed the unique features of the FHS technology. Numerous pilot-plant-scale separators were designed and built, with throughputs up to 500 kg/h. Although extensive tests conﬁrmed viability of this technique, particularly when applied to the recovery of non-ferrous metals from automobile scrap, production-scale application did not take place in the Western World at that time [F8]. Comprehensive review of the history of FHS in Japan and the USA was given by Fujita [F8]. Ferrohydrostatic separation was also researched and used, in approximately the same time period, on a production scale in the former Soviet Union. The Gipromashugleobogashcheniye Institute (GMUO) in Lugansk, the Ukraine, developed a comprehensive range of models of ferrohydrostatic separators for different applications and throughputs. These separators were used in such diverse applications as densimetric analysis of coal, recovery of gold from gravity concentrates, diamond concentration and separation of non-ferrous scrap. Table 2.12 summarizes various models of FHS units manufactured by GMUO [G4]. Figure 2.104 illustrates the versatile FGS-40 separator suitable for laboratoryscale separation of various minerals in the density range from 4000 kg/m3 to

2.8. SEPARATORS WITH MAGNETIC FLUIDS

157

Figure 2.105: Production-scale ferrohydrostatic separator FGS-70 for separation of non-ferrous metals (courtesy of GMUO, the Ukraine).

158

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.106: Ferrohydrostatic separator Shlikh-1 with permanent magnets for recovery of alluvial gold (Too Geos Co.). 9000 kg/m3 . The FHS unit designed to separate non-ferrous metals in the density range between 6500 kg/m3 and 10 000 kg/m3 , with particle size up to 25 mm, is shown in Figure 2.105. As a result of geopolitical changes in the nineties of the last century, most markets for GMUO ferrohydrostatic separators in the former Soviet Union disappeared and the separators have not been innovated to meet the current standard of technology. Ferrohydrostatic separators based on permanent magnets are produced by Too Geos Co. (Russia). These small-scale low-throughput machines have been designed for the recovery of alluvial gold from gravity concentrates. Throughput of the Shlikh-2 model is approximately 50 kg/h, while a laboratory model Shlikh1, shown in Fig. 2.106 can treat about 10 kg/h. All models of the Shlikh FHS separator are supplied together with a vibrating screen and disk and roll magnetic separators, as shown in Fig. 2.107. These units allow the classiﬁcation of the material and the removal of strongly and medium magnetic materials from the feed into the FHS unit. Since FHS is a unique technique for material manipulation in areas such as diamond-processing industry, De Beers Consolidated Mines (Pty.) Ltd. (South Africa) developed a range of selective FHS separators. These fully automated computer-controlled, hands-o units are capable of treating particles in the size

2.8. SEPARATORS WITH MAGNETIC FLUIDS

159

Figure 2.107: Shlikh-1 system comprising a vibrating screen, disk and roll magnetic separators and a ferrohydrostatic separator (Too Geos Co.). range - 25 + 0.3 mm and can distinguish a density dierence of at least 20 kg/m3 (0.02 g/cm3 ). Units with a throughput exceeding 1 t/h, depending on the feed density and size, have been built [S23]. Figure 2.108 shows a twostage automated and secure ferrohydrostatic separator built by De Beers for R ° the recovery of diamonds. The ferrohydrostatic separator Rhomag , shown in Figure 2.109, is used for separating ﬁne fractions of exploration samples.

2.8.3

Magstream separator

The main limitation of ferrohydrostatic separation, in which the important competing force is the force of gravity, is ine!cient separation of ﬁne particles. Efforts were made by Revnetsev [R11] and Andres et al. [A14] to replace the force of gravity by the centrifugal force. This proposal resulted in a rotation-based separation process Magstream [W7] developed by Intermagnetics General Corp. The essential features of the Magstream separation process are shown in Fig. 2.110. Particles to be separated are combined with a ferroﬂuid and passed downward through a long, vertically oriented annular duct where they rotate with the ﬂow guide and duct about the duct axis. The duct is surrounded by a multipole magnet that produces a non-homogeneous magnetic ﬁeld. A radially inward displacement force, which results from the radially outward attraction of the magnetic ﬂuid, is felt by all particles. This force is opposed (or aided) by a radially outward (or inward) magnetic force acting on paramagnetic (or diamagnetic) particles, and by the centrifugal force. At a given speed of rotation, the inward displacement forces are greater on light particles, which then move radially inwards. Heavier particles experiencing

160

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.108: An automated hands-o two-stage ferrohydrostatic separator (courtesy of De Beers Consolidated Mines (Pty.) Ltd.).

R ° Figure 2.109: Ferrohydrostatic separator Rhomag for separation of ﬁne particles (courtesy of De Beers Consolidated Mines (Pty.) Ltd.).

2.8. SEPARATORS WITH MAGNETIC FLUIDS

Flowguide

Feed

Magnetic fluid

Magnet

Splitter

Light fraction

Heavy fraction

Figure 2.110: Schematic diagram of the Magstream separator.

Figure 2.111: Magstream 200 separator.

161

162

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

higher centrifugal and magnetic forces, at the same speed of rotation, overcome displacement forces to move radially outwards. The separation density is then given by: Pi E d = 0 + frqvw 2 (2.11) $ where $ is the angular velocity. It can be seen that the additional degree of freedom, namely the speed of rotation, can be used to control the separating force acting on the particles. The Magstream separators were available in several models, ranging from laboratory-scale portable units for batch separation of samples up to 300 g, to large continuous separators with a throughput up to 250 kg/h. Figure 2.111 shows the 200 Magstream model. Magstream separators can separate particles over a range of densities from 1300 kg/m3 to beyond 21 000 kg/m3 . The accuracy of separation is claimed to be 100 kg/m3 (0.1 g/cm3 ). For the most e!cient separation, the sample should be sized between 60 m and 1 mm. Separation of samples up to 4 mm is possible with special accessories.

Chapter 3

Theory of Processes of Magnetic Separation of Materials In view of the diversity of magnetic separation techniques the theoretical descriptions of the magnetic separation process are of limited general applicability. So many factors may aect the behaviour of a system of particles that many problems appear at ﬁrst sight to be of bewildering complexity. In general, the particle motion in a non-homogeneous magnetic ﬁeld is so involved as to prevent reasonable theoretical approach. On the other hand, however, a particular problem can often be simpliﬁed considerably and a realistic appraisal of the equations describing the motion of the particles is possible. As has been mentioned in Chapter 1, a particle in a magnetic separator is acted upon by a wide array of forces of various magnitudes and ranges. The necessary (but not su!cient) condition for successful separation of more strongly magnetic particles from less strongly magnetic particles is expressed by eq. (1.1). In real situations, however, such a condition is di!cult to evaluate. The general expression for the magnetic force (eq. (1.8)) acquires speciﬁc forms in dierent types of magnetic separators, depending on the pattern of the magnetic ﬁeld and its gradient. Also, the importance of various competing forces acting on particles in a magnetic separator depends on the type of magnetic separator, on the properties of the particles, such as size, shape, magnetic properties, density, and on the type of ﬂuid in which the particles to be separated are suspended. Workable models of material separation must, therefore, be developed separately for individual types of magnetic separators. The situation is complicated by the fact that many branches of magnetic separation, such as separation by suspended magnets, magnetic pulleys or wet low-intensity drum magnetic separators still constitute highly empirical technology. Hesitant steps have been taken to develop theoretical models of dry separation in roll and drum magnetic separators. On the other hand, open-gradient magnetic separation, magnetic 163

164

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

ﬂocculation of weakly magnetic particles and wet high-gradient magnetic separation have received considerable theoretical attention. A notable number of papers dealing with the problem of particle capture in HGMS led to an understanding of the interaction between a particle and a matrix element. However, completely general treatment of the magnetostatic and hydrodynamic behaviour of an assembly of the ore particles in a system of matrix elements, in the presence of a strong magnetic ﬁeld, is a theoretical problem of considerable complexity. A brief survey of the current theoretical descriptions of separation of materials in various types of magnetic separation equipment will be given in the following sections.

3.1

The forces and the equations of particle motion

The equations of particle motion are relations between accelerations, velocities and coordinates of the particles. They are second-order dierential equations for the function u(w)> where u is the radius vector and w is the time. Their integration makes possible, in principle, the determination of this function and so of the path of the particles. The equation of particle motion in a magnetic separator can be written in a vector form as psds = l Il (3.1) where psds is the inertial force, ps is the mass of the particle and ds its acceleration. Il are all the forces that may be present in a magnetic separator, such as the magnetic force, force of gravity, hydrodynamic drag, centrifugal force, the friction force, surface forces, magnetic dipolar forces and electrostatic forces among the particles and others. In order to be able to solve eq. (3.1), it is necessary to evaluate the components of all its terms in suitable coordinates. To obtain the components of the inertial force in polar coordinates that are convenient for most types of magnetic separators, let us consider two mutually perpendicular unit vectors uˆ and ˆ= We shall assume that these vectors have directions of increasing u and and their directions change with time. Since the derivative of a unit vector is perpendicular to the vector, the time rates of uˆ and ˆ can be expressed as [G1] gˆ u g ˆ = gw gw

(3.2)

g gˆ = uˆ gw gw

(3.3)

Now, the position of the particle, in polar coordinates, is given by u = uˆ u. Dierentiating this equation and using eqs. (3.2) and (3.3), the components of

3.1. THE FORCES AND THE EQUATIONS OF PARTICLE MOTION 165 the particle velocity y are found to be yu =

gu gw

(3.4)

g (3.5) gw The subscripts u and indicate the radial and azimuthal components, respectively. By further dierentiation, the components of the particle acceleration ds are obtained and hence the components of the inertial force are [G1] " µ ¶2 # g g2 u (3.6) u ps dsu = s Ys gw2 gw · 2 ¸ gu g g ps ds = s Ys u 2 + 2 (3.7) gw gw gw In Cartesian coordinates these equations can be written as y = u

ps ds{ = s Ys

g2 { gw2

(3.8)

ps ds| = s Ys

g2 | gw2

(3.9)

Complete equations of motion are obtained by combining eq. (3.1) with eqs. (3.6) and (3.7) or (3.8) and (3.9). While it is fairly straightforward to express components of most of the competing forces, such as the force of gravity and the hydrodynamic drag, the magnetic force is more complicated. The general form of the components of the magnetic force, in polar coordinates are given by: Iu =

s CEu CEu Ys (Eu + E ) 0 Cu Cu

(3.10)

s 1 CEu CE Ys (Eu + E ) (3.11) 0 u C C In the Cartesian system the components of the magnetic force can be expressed as: s CE{ CE| Ys (E{ I{ = + E| ) (3.12) 0 C{ C{ s CE{ CE| Ys (E{ + E| ) (3.13) I| = 0 C| C| where s is the volume magnetic susceptibility. It can be seen that in order to use the above equations, we must be able to specify the components of the magnetic induction and its gradient. Each type of a magnetic separator generates its speciﬁc pattern of the magnetic ﬁeld and the problem of particle motion has to be solved separately for each type of a magnetic separator. I =

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

166

Permanent magnets

ș

R

r

ș0

Rotating drum

Figure 3.1: Arrangement of magnetic poles in a drum magnetic separator.

3.2

Particle motion in drum and roll separators

Drum and roll magnetic separators are characterized by periodic arrays of magnetic poles. Laurila [L2] made a fundamental investigation of the periodic magnetic ﬁeld of the cylindrical array of magnets with radial and axial poles used in drum and roll separators. The general expressions for the components of the magnetic force derived in [L2] can then be simpliﬁed in speciﬁc geometrical arrangements of the magnetic poles. Hopstock [H12] derived, based on mathematical and empirical analysis, approximate expressions for the radial and azimuthal components of the magnetic ﬁeld around a magnetic drum with axial arrangement of the magnetic poles, as shown in Fig. 3.1. Magnetic force in a drum separator The approximate expressions for the radial and azimuthal components of the magnetic induction, derived by Hopstock [H12] are : · ¸ (u U) Eu = E0 cos( ) exp (3.14) 0 0 U · ¸ (u U) E = E0 sin( ) exp (3.15) 0 0 U These equations were found to give a good ﬁt to experimental data in a number of dierent magnet conﬁgurations [H12]. The magnetic induction around a drum, shown in Fig. 3.1, is then given by: · ¸ (u U) (3.16) E = E0 exp 0 U

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

167

y

Ff

Fc Fgt

Fgr

ș

Fm

Fg

Figure 3.2: Forces acting on a particle placed on a magnetic drum or roll. where E0 is the magnetic induction on the surface of the drum. It can be seen that in this approximation E is independent of angle . The approximation is most accurate when the following condition is met uU =

0 U

(3.17)

The term on the right-hand side of eq. (3.16) expresses the depth of the ﬁeld, deﬁned as a distance from the surface at which the ﬁeld is reduced to 1/h of its surface value. Equations (3.14) and (3.15) allow calculation of the magnetic ﬁeld gradient and thus the magnitude of the magnetic force. As a ﬁrst approximation, Hopstock found that the radial component of the magnetic force, acting on a magnetite particle in a drum magnetic separator is given by Ipu =

3Ys E02 0 0 U

(3.18)

Under Hopstock’s approximations, the azimuthal component of the magnetic force is equal to zero, which is incorrect. In a more rigorous treatment by Birss et al. [B9], accurate expressions for the components of the magnetic ﬁeld and force were derived in the form of a Fourier series. Whether or not a particle is held on the drum and carried to the magnetic fraction depends on the relative magnitudes of the magnetic force and the gravitational and centrifugal forces. The forces acting on a particle situated on the surface of a drum or a roll are shown in Fig. 3.2. For a given angle of rotation

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

168

r Ȝ

z

R Magnets

Figure 3.3: Arrangement of magnetic poles in a roll magnetic separator. , the radial force acting of a particle can be expressed as: Iu =

s gEu Ys Eu + Ys s j cos Ys s $ 2s U 0 gu

(3.19)

where $ s is the angular velocity of the particle on a roll or drum of radius U. For a speciﬁc case of a high-speed drum, when the force of gravity can be neglected, the centrifugal force equals the magnetic force acting on a magnetite particle when the drum is rotating at the critical angular velocity (in rad/s) given by [H12]: · ¸[email protected] 3E02 (3.20) $f = 0 s 0 U2 Expressions for the components of the magnetic induction for a roll magnetic separator, shown in Fig 3.3, can be written, in cylindrical coordinates, in a more rigorous form [M14]: · ¸ 2 2 Eu = E0 sin( }) exp (u U) (3.21) · ¸ 2 2 E} = E0 cos( }) exp (u U) (3.22) where E0 is the magnetic induction on the surface of the roll, U is the radius of the roll and is the periodicity of the magnetic system. The above equations can be re-written in a more general form as [M14]: Eu = E0 sin(n1 }) exp [n2 (u U)]

(3.23)

E} = E0 cos(n1 }) exp [n2 (u U)]

(3.24)

where n1 and n2 are constants that describe the pattern of the magnetic ﬁeld as a function of u and }. These constants can be determined, for instance, from the electromagnetic modelling of a speciﬁc roll separator.

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

169

Figure 3.4: The forces acting on a particle in a drum magnetic separator (adapted from [C9] and [S24]). Magnetic force acting on a spherical particle of radius e and volume magnetic susceptibility s , on the magnetic roll or drum, can then be written as: Ip = 0 s E02

3.2.1

e2 {exp [2n2 (u e U)] exp [2n2 (u + e U)]} 3

(3.25)

Motion of a particle on the drum or roll surface

The motion of a particle of radius e> situated on the surface of a drum separator of radius U, can be divided into three phases [C9], as shown in Fig. 3.4. In the ﬁrst phase, the particle is accelerating under the inﬂuence of the force of friction Ii and the tangential component of the force of gravity Ijw , given by the following equation: Ii = g (Ip + Iju If )

(3.26)

Ijw = jYs s sin

(3.27)

where g is the coe!cient of dynamic friction and the angle is deﬁned in Fig. 3.2. The end condition of phase 1 was deﬁned by Cakir et al. [C9] as the point when the particle reaches rotor speed $ u , i.e. $ s = $ u . Once the particle acquires the speed of the drum, a static friction coe!cient v , replaces the dynamic friction coe!cient in eq. (3.26). The particle then moves with the constant angular velocity equal to the speed of the drum. When the tangential component Ijw of the force of gravity (Fig. 3.2) becomes greater than the force of friction Ii , or when the particle leaves the drum, the motion of the particle enters the third phase. At the end of the second phase Ii = v (Ip + Iju If ) = Ijw

(3.28)

170

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

In the third phase the particle begins to accelerate as it slips on the drum surface. The radial component of the force of gravity decreases in this region until the centrifugal force exceeds the radial force and the particle leaves the drum: If = Ys s $ 2u (U + e) = Ip + Iju (3.29) Equations of motion of a particle on a magnetic drum in these three phases were developed by Murariu [M14]. The equation of particle motion in the ﬁrst phase can be written · ¸ j Ip j g2 g 2 = + sin + cos ( ) (3.30) g gw2 U+e U+e gw s Ys (U + e) In the second phase the equation of motion is: g g2 = 0 and thus = $u gw2 gw In phase three the equation of motion becomes: · ¸ j Ip j g2 g 2 = sin v cos ( ) + gw2 U+e U+e gw s Ys (U + e)

(3.31)

(3.32)

with initial conditions: = 01

(3.33)

g (3.34) = $u gw where 01 is the angle of the slip point at the end of phase 2. At a certain value of the angle , denoted by 02 , the particle leaves the drum. At that moment [M14]: g s Ys (U + e)( )2 = s Ys j cos + Ip (3.35) gw It should be mentioned that in the case of the roll, the ﬁrst phase is absent since a particle is deposited on the roll at the speed of the roll.

3.2.2

Motion of the particle after it leaves the roll

When the particle leaves the roll or the drum, it is being acted upon by the force of gravity and by the magnetic force. Schematic diagram of this situation is shown in Fig. 3.5. The equations of motion, in Cartesian coordinates, are [M14]: g2 { { Ip (3.36) = 2 2 g w s Ys ({ + | 2 )[email protected] Ip | g2 | = j gw2 s Ys ({2 + | 2 )[email protected]

(3.37)

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

171

y v0 =Ȧ0 (R+b)

Fmx ș

ș02

Fmy Fm

Fg x

Figure 3.5: Forces acting on a particle when it has left the drum. where the magnetic force is given by: ¤ ¾ £ ½ 2 2 [email protected] e2 exp 2n £ 2 (({ 2+ | )2 [email protected]) e U ¤ Ip = 0 s E02 exp 2n2 (({ + | ) ) + e U 3

(3.38)

Dierential equations (3.36) and (3.37) obey the following initial conditions {(w = 0) = (U + e) sin 02

(3.39)

|(w = 0) = (U + e) cos 02 g{ (w = 0) = $ 0 (U + e) cos 02 gw g| (w = 0) = $ 0 (U + e) sin 02 gw In equations (3.39) the term $ 0 (U + e) represents the initial velocity of the particle at the moment when it leaves the drum, while $ 0 is the angular velocity of the particle at that moment. By solving the equations of motion (3.36) and (3.37), trajectories of particles can be obtained as a function of their magnetic susceptibility, size, density and of the coe!cient of friction, magnetic ﬁeld strength on the surface of the roll, the spatial distribution of the magnetic ﬁeld and the angular velocity of the roll. An example of a family of particle trajectories is shown in Fig. 3.6.

172

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.6: Particle trajectories in a roll magnetic separator. Roll diameter: 76 mm, speed of rotation: 200 rpm, particle size: 2 mm and particle mass magnetic susceptibilities (from right to left): 2.5×107 > 2.5×106 and 5×106 m3 /kg.

3.3

Separation of particles by a suspended magnet

Suspended (or overband) magnetic separators have been used over many decades to improve material purity and to protect processing machinery by removing unwanted iron and steel objects from conveyed bulk material. Although the design procedures of such magnetic systems, that use either electromagnets or permanent magnets are well established, the understanding of fundamental principles for extraction of metal is inadequate and standards for selecting suitable separators are inconsistent and often incorrect. The common practice [A15, H13] is to base the evaluation of a magnetic separator on the so-called ”force index”, which is essentially the magnetic force density acting on a ferromagnetic body to be removed from a stream of material. Such an approach requires that, for the extraction to occur, the product of the magnetic induction and its gradient assumes a certain minimum value Although such a concept is valid for certain special shapes of bodies, it does not, in general, describe correctly the behaviour of ferromagnetic particles in a magnetic ﬁeld and can lead to erroneous design of a magnetic circuit.

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

3.3.1

173

Magnetic force in a suspended magnet

A starting point in the evaluation of the e!ciency of a suspended magnet is the requirement that the magnetic force Ip acting on a particle must be greater than the sum of the competing forces, e.g. the force of gravity Ij , the drag of the environment Ig , the force of friction Ii and others. The magnetic force on a ferromagnetic particle can be conveniently written as I

p

0 = (P · u)E

(3.40)

where P is the eective magnetic dipole moment of the particle and E0 is the external magnetic induction. When both the particle and the external medium are homogeneous and isotropic, and the body has an ellipsoidal shape, the eective dipole moment is [L3] s p 0 P = Ys K (3.41) p + Q (s p ) where K0 is the external magnetic ﬁeld strength, s and p are the relative magnetic permeabilities of the particle and the external medium, respectively, Q is the demagnetization factor appropriate for the axis of the ellipsoid along which K0 is directed. Using eqs. (3.40) and (3.41) we get for the magnetic force [S25]: Ip = Ys

s p 0 0 · u)E (K p + Q (s p )

(3.42)

For a ferromagnetic body in a non-magnetic or weakly magnetic medium we = have s AA 1 and p = 1, so that eq. (3.42) becomes: Ip = Ys

s 1 0 0 · u)E ¤ (E £ 0 1 + Q (s 1)

(3.43)

The relative magnetic permeability s of the particle is the function of the magnetic ﬁeld inside the particle, s = s (K), where [L3] = K

0 0 p K E ¤ £ = p + Q (s p ) 0 1 + Q (s 1)

(3.44)

for p = 1= Q is the demagnetization factor appropriate for the axis of the easiest magnetization (i.e. the axis of the smallest Q ), as the particle is assumed to be oriented so that its axis is parallel to the external ﬁeld K0 = The expression (3.43) for the magnetic force is a product of two factors: the ﬁrst factor reﬂects the physical properties of particles to be removed, while the second factor, the magnetic force density 02 ) ip = u(E

(3.45)

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

174

Table 3.1: Static force indices (FI) and their ratios for selected shapes [S25] (l length, d-diameter). Object Rod

Sphere Plate 13×50×50 13×200×200 25×200×200

[email protected] 1.0 4.0 10.0

Force index [106 T2 m1 ] 29 889 9 515 4 037 31 811

Ratio FI/FIurg 7.4 2.4 1.0 7.9

20 300 11 130 15 300

5.0 2.8 3.8

describes the properties of the magnetic system. It is this magnetic force density that many designers call ”force index” and use to evaluate magnetic separators. Let us assume that a particle to be extracted by a suspended magnet rests on a stationary conveyor and that no burden of bulk material is present. In equilibrium Ip = Ij , where Ij = Ys (s p )j

(3.46)

and p is the density of the medium. Assuming that s AA p , and combining eqs. (3.43), (3.45) and (3.46) Svoboda obtained [S25]: ¤ £ 1 + Q (s 1) ip = s (3.47) 0j s 1 Equation (3.47) determines the minimum force density (or force index) required to lift a stationary ferromagnetic body of relative magnetic permeability s , density s and demagnetization factor Q , from its position on a belt, in the absence of a burden of bulk material. It can be seen that this minimum magnetic force density is independent of particle size and depends solely on its shape (through the demagnetization factor), its magnetic properties (through the relative magnetic permeability) and its density. Equation (3.47) also shows that the ratio of force indices for various shapes is in the ratio of their demagnetization factors (provided that Q (s 1) AA 1, which is satisﬁed for all shapes but very long rods or thin plates, for which Q ?? 1). Table 3.1 gives several examples of ratios of force index The minimum static force index (or magnetic force density) as a function of the demagnetization factor, for a given material characterized by s and s , in the absence of the burden has, therefore, general validity for any size of the object to be lifted. Figure 3.7 shows such a dependence for steel (s = 7800 kg/m3 , s = 1000). It can be seen that, for instance, for a steel sphere (Q = 0.33) I L = 0.03 T2 /m (80.8×103 G2 @inch).

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

175

Figure 3.7: Magnetic force density (or force index), for steel, as a function of demagnetization factor (adapted from [S25]). For majority of objects that are encountered in practice, the assumption that the external magnetic ﬁeld is directed along the axis of easy magnetization of the body is invalid. Objects such as plates, rods or bolts usually rest on a conveyor belt with their axes of easy magnetization perpendicular to the direction of the external magnetic ﬁeld. Demagnetization factors appropriate for such orientations are high and large force densities (or force indices) are required to lift the body towards the magnet.

3.3.2

Torque on a magnetizable body

Under the above mentioned circumstances, the role of the magnet should be ﬁrst to re-orient the ferromagnetic body in such way that its long axis (the axis of easy magnetization) is parallel with the direction of the external magnetic ﬁeld. This is accomplished by exerting a torque on the body by the externally applied magnetic ﬁeld. The magnetic torque is given [L3, L4] by: 0 W = P × E

(3.48)

s > where Ps is the magnetization of the particle, eq. (3.48) Since P = Ys P can be rewritten: 0 s ×E (3.49) W = Ys P Assuming a body of spheroidal shape, the torque is perpendicular to the plane passing through the axis of symmetry of the body and the direction of

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

176

Axis of symmetry

Į B

b t

a

Figure 3.8: A ferromagnetic bar in a transverse external magnetic ﬁeld. E0 . The magnitude of the torque is given [L5] (by analogy with the torque on a dielectric spheroid in an electric ﬁeld)[S25]: W =

(s p )2 | 1 3Q | K0 E0 Ys sin 2 ¤£ ¤ 2 (p + Q (s p ) s + p Q (s p ) £

(3.50)

and for p =1 W =

( 1)2 | 1 3Q | E02 Ys sin 2 ¤£ ¤ £ s 20 1 + Q (s 1) 1 + s Q (s 1)

(3.51)

Here is the angle between the direction of E0 and the axis of symmetry of the spheroid. It can be seen that the maximum torque occurs at = 450 . The torque is directed in such a way that it tends to turn the axis of symmetry of a prolate (i.e. Q ? 0.33) or oblate (Q A 0.33) spheroid parallel or perpendicular to E0 , respectively. Therefore, the torque tends to align the axis of easy magnetization of the body along E0 . In equilibrium, the magnetic torque is balanced by the torque exerted by the weight of the particle Js and by the weight of the burden Je . We can thus write for a particle having a shape of a bar: 1 k (3.52) jd(s + e )Ys 2 w where d and w and dimensions of the bar, as shown in Fig. 3.8, k is the height of the burden of the material and e is its bulk density. Combining eqs. (3.51) and (3.52) we obtain, in equilibrium, [S25]: W =

E02 sin 2 = dj(s +

k ) w e 0

(

s + 1 1 + Q )( Q) s 1 s 1 | 1 3Q |

(3.53)

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

177

Figure 3.9: Minimum values of the magnetic induction, required to orient steel rods of selected sizes, as a function of the depth of the burden (adapted from Svoboda [S25]). For s AA 1 we then have: k Q (1 Q ) E02 sin 2 = dj0 (s + e ) w | 1 3Q |

(3.54)

It can be seen that if the magnetic system generates the ﬁeld that is perpendicular to the plane of the rod, the rod will not orient itself since = 900 and thus W = 0. It also transpires from eq. (3.48) that the gradient of the magnetic ﬁeld does not contribute, in the ﬁrst approximation, to the torque. Therefore, only the magnitude of the ﬁeld determines whether the reorientation of the body takes place or not. It is clear that in contrast to the conventional description of separation by a suspended magnet, which requires that the magnetic system is designed in such a way that the force index EuE achieves a certain minimum value, the physical picture based on the magnetic torque approach requires a minimum value of the magnetic ﬁeld only. The physical content of such a description can have important implications for the design of the magnetic system. It follows from the previous analysis that in a suspended magnet the important parameter is the magnetic ﬁeld strength. If the ﬁeld strength is high enough so that it can orientate the body along the axis of easy magnetization, the magnitude of the force index is required to be high enough to lift the particle in the direction of its axis of easy magnetization, only. Therefore, the force index is not the only parameter needed to evaluate a suspended magnet. For instance, the force index EuE may be just large enough to lift an

178

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.10: Minimum values of the magnetic induction needed to orient steel plates of selected sizes, as a function of the depth of the burden (adapted from Svoboda [S25]). object in the direction of its axis of easy magnetization, but the magnitude of the magnetic ﬁeld itself may still be too low for the condition of eq. (3.53) to be met. The object then will not re-orientate itself appropriately and will not be lifted. When designing the magnetic system of a suspended magnet two conditions thus must be met: the magnitude and the direction of the magnetic ﬁeld must satisfy eq. (3.54) and, at the same time, the force index must fulﬁll condition given by eq. (3.47). Typical dependence of the minimum magnetic ﬁeld on the depth of the burden, for selected sizes of steel rods and plates, is shown in Figs. 3.9 and 3.10. Similar diagrams can be constructed for other shapes and sizes using eq. (3.53), provided the demagnetization factors are known. A comparison between theoretical values of the minimum magnetic induction Emin required to orient a body along its axis of easy magnetization, calculated using eq. (3.53), and experimental values is given in Table 3.2. It can be seen that the agreement is satisfactory.

3.3.3

Demagnetization factors

Calculation of the demagnetization factor for objects of shapes dierent from that of an ellipsoid is complex and the values found in literature, e.g. for ellipsoids and inﬁnite cylinders, are often of limited practical use. Brown [B3] gives tables for circular cylinders of ﬁnite length, magnetized longitudinally, and for

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

179

Table 3.2: Comparison of theoretical and experimental values of the minimum magnetic induction required to orient steel objects, as a function of the depth of the burden [S25]. Object Rod 3×30 mm Plate 0.1×22×43 mm

Bmin [T] Burden depth [mm] Exp. 0 0.0124 10 0.016 0 0.0033 10 0.0131

Theor. 0.0113 0.0132 0.0034 0.0114

Table 3.3: Demagnetization factors of ferromagnetic objects [S25]. Cylinders and plates are magnetized longitudinally(l - length, d - diameter). Object Sphere Finite cylinder

Plate

Size ([email protected]) 0 0.4 1.0 4.0 10.0 40.0 100.0 1000.0 13×50×50 mm 13×200×200 25×200×200

N 0.33 1.0 0.528 0.3116 0.098 0.041 0.011 0.004 0.0004 0.19 0.06 0.11

rectangular rods magnetized transversely. These geometries, together with an ellipsoid, should be su!cient for analysis since other shapes usually encountered in the separation practice (plates, hexagons) can be, in the ﬁrst approximation, converted into geometries for which the demagnetization factors are available. Values of demagnetization factors for selected shapes and sizes are given in Table 3.3.

3.3.4

The eect of the burden

It transpires from the above analysis that a ferromagnetic object to be lifted by the suspended magnet must be ﬁrst re-orientated by the action of the magnetic ﬁeld, in such a way that its long axis (i.e. the axis of easy magnetization) is parallel with the direction of the magnetic ﬁeld. Once this is achieved, the magnetic force is needed to overcome the weight of the object. The object will then be lifted provided the force index acting on a particle is greater than the minimum force index given by eq. (3.47).

180

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.11: The static force index as a function of the depth of the burden, for various sizes of a ferromagnetic sphere (s = 1000> s = 7800 kg/m3 , e = 800 kg/m3 ) (adapted from [S25]). In practice, however, a ferromagnetic particle is usually buried in a layer of loosely packed material, e.g. coal. With the body at rest, the minimum magnetic force required to move the object is determined by its weight and by the force of pressure on the upper hemisphere of the body: Is = e Yej

(3.55)

where Ye is the volume of the burden above the body. In equilibrium Ip = Ij + Is

(3.56)

From eq. (3.56), taking into account that s AA e > a modiﬁed version of eq. (3.47) can be written [S25]: ¤ £ 1 + Q (s 1) Ye ip = 0 (3.57) (s + e )j s 1 Ys It can be seen from eq. (3.57) that the static magnetic force density (or force index in the presence of the burden depends not only on the shape of the object, but also, in contrast to the situation when the burden is absent (eq. (3.47)), on the size of the object. A typical dependence of the static force index on the depth of the burden, for various sizes of a ferromagnetic sphere, is shown in Fig. 3.11.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

181

Similar diagrams can be constructed, using eq. (3.57), for other shapes. It can be seen that the static force index increases steeply with increasing depth of the burden for small particles, while for larger objects the dependence is mild.

3.4

High-gradient magnetic separation

During the last three decades, high-gradient magnetic separation (HGMS) has attracted considerable attention, both experimentally and theoretically. It has established itself as a powerful technique for the manipulation of ﬁne weakly magnetic particles. HGMS has also become a beloved subject of theoretical modelling and a notable number of publications dealing with the problem of particle capture led to an understanding of the interaction between a magnetizable particle and a matrix element. The problem of particle capture in a matrix of a high-gradient magnetic separator can be looked upon from both the macroscopic and microscopic points of view. The macroscopic studies are aimed at the phenomenological description of the separation process and the prediction of its dynamic behaviour. The microscopic theories are intended to provide insight into the mechanisms of particle capture by the matrix. The complex problems facing the microscopic theories were considerably simpliﬁed by considering, in the ﬁrst instance, the interaction between a single particle and a single matrix element. The theory of multi-particle and multi-collector magnetic separation was then developed as a direct extension of the single element model. Validity of such an approach has been questioned and theoretical analysis and experimental data conﬁrm only limited applicability of such an extension to real-life multi-element scenario. A detailed description of the theoretical models of high-gradient magnetic separation is given in a book by Gerber and Birss [G1] and other publications [B10, S1]. A brief survey of the theory of HGMS is given in the following section.

3.4.1

Theory of particle capture by a single-collector

The main emphasis in the early models of high-gradient magnetic separation was on the analysis of particle trajectories in the vicinity of a single magnetized matrix collector, usually a wire [W8, W9, L6, C10]. These studies were inspired by the early analysis by Zabel [Z6] who studied the mechanisms of dielectrophoretic capture on ﬁber matrix. Watson [W8] considered a ferromagnetic wire of radius d placed along the } -axis in a diamagnetic ﬂuid, as shown in Fig. 3.12. A uniform magnetic ﬁeld K0 , strong enough to saturate the wire, is applied in the { direction. Spherical paramagnetic particles of radius e are carried by a ﬂuid of viscosity that ﬂows with uniform velocity y0 in the negative {-direction. This orientation is one of the three possible arrangements between the directions of the magnetic ﬁeld and particle ﬂow velocity with respect to the ferromagnetic wire. It is always assumed that the wire is orthogonal to the external magnetic ﬁeld; the ﬂuid ﬂow can be either parallel (longitudinal - L-

182

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Y H0

v0 b

a

X

Z

Figure 3.12: A ferromagnetic wire and a paramagnetic particle in a magnetic ﬁeld.

Figure 3.13: Graphic representation of three geometrical conﬁgurations in HGMS and of the proﬁles of the particle build-up on the ferromagnetic wire.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

183

b y

H0

g

r

v0

ș ȕ Ȗ x

a

Figure 3.14: The conﬁguration of particle capture in a single-wire approximation. orientation) or perpendicular (transverse - T - orientation) to the direction of magnetic ﬁeld. The third conﬁguration, when the initial ﬂuid ﬂow is parallel to the wire, is known as the axial (A) conﬁguration. These three geometrical conﬁgurations are illustrated in Fig. 3.13. In order to describe the motion of a small paramagnetic particle travelling in a ﬂuid stream in the presence of a magnetized wire, one assumes that the particle experiences magnetic, hydrodynamic and gravitational forces. The balance of forces which describes the particle motion is given by eq. (3.1), or in a more explicit form by eq. (3.58): Il = Ip + Ig + Ij

(3.58)

where Il is the inertial force. The general conﬁguration of the particle motion problem in a single-wire approximation is shown in Fig. 3.14. In order to obtain the magnetic force acting on a small paramagnetic particle in the vicinity of a magnetized wire, the magnetic ﬁeld, external to and generated by the magnetized wire must be expressed as a function of the wire radius. The components of the magnetic ﬁeld outside the wire, in polar coordinates, as deﬁned in Figure 3.14, can be written [G1, S1] as: Ku = K0 (1 + N

d2 ) cos u2

K = K0 (1 N

d2 ) sin u2

(3.59) (3.60)

184

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where N=

P 2K0

(3.61)

For K0 ? Kv N = 1 while for K0 A Kv N = Pv @2K0 . Kv and Pv are the saturation magnetic ﬁeld strength and saturation magnetization of the wire material, respectively. The magnetic force By inserting eqs. (3.59) and (3.60) into eq. (1.8), components of the magnetic traction force on a magnetizable particle are obtained: Ipu =

0 Ys Pv d2 Pv d2 ( 2 + K0 cos 2) u3 u

(3.62)

0 d2 Ys Pv K0 sin 2 u3

(3.63)

Ip =

Ip} = 0

(3.64)

If the net volume magnetic susceptibility = s i is positive, then the radial component of the magnetic traction force between the particle and the wire is attractive provided that Pv d2 + K0 cos 2 A 0 u2

(3.65)

The component Ipu becomes repulsive for s A i in two symmetrical regions, the boundaries of which are determined by a critical angle f [B10] d2 u2 ) f = arctan( d2 1N 2 u 1+N

(3.66)

As shown in Fig. 3.15, the angle f determines sections of the wire surface that are attractive or repulsive to paramagnetic or diamagnetic particles. It is apparent from eq. (3.65) that paramagnetic particles will be collected at angles smaller than f and repelled at angles greater than f = On the other hand, diamagnetic particles, with negative susceptibilities, will be attracted to the wire collector at angles A f and repelled in regions where ? f = The situation is summarized in Fig. 3.16, which shows the contours of the magnetic force around a magnetized cylindrical wire. The hyperbolae indicate the lines of zero radial force. It can be seen from eq. (3.66) that the angle f decreases with increasing magnetic ﬁeld strength. Therefore, the area on the matrix collector, available for the capture of paramagnetic particles decreases with increasing ﬁeld strength.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

185

Figure 3.15: Attractive and repulsive regions around a wire collector (rd = [email protected])=

Figure 3.16: Pattern of the magnetic force around a magnetized cylindrical wire.

186

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The ﬂuid ﬂow distribution and the viscous drag The hydrodynamic drag acting on a particle travelling in a ﬂuid stream is evaluated by calculating the ﬂow ﬁeld around a circular cylinder. The simplest approach to this di!cult problem is to assume that the ﬂuid is inviscid and incompressible. Then the ﬂuid velocity can be written as the gradient of the velocity potential and by solving Laplace’s equation it is possible to obtain the ﬂuid velocity in polar coordinates [G1]: d2 ) cos( ) (3.67) u2 d2 (3.68) y = y0 (1 + 2 ) sin( ) u The potential ﬂow gives good description of the ﬂow conditions on the front side of wire for high Reynolds number, i.e. for Re A 1, where Re is given by 2y0 i d Re = (3.69) yu = y0 (1

For high Reynolds numbers the inertial forces exceed the viscous forces everywhere in the ﬂow ﬁeld except within a thin boundary layer at the wire surface and at the rear side of the wire. For low Reynolds numbers, Re?1, the inertial forces are smaller than the viscous forces and the ﬂow has a viscous (or creeping or laminar) character. The velocity distribution can then be obtained by Lamb’s method [B11, G1]: h u d i ln( ) 0=5 1 ( )2 d u yu = y0 cos( ) (3.70) 2=002 ln Re i h u d ln( ) + 0=5 1 ( )2 u sin( ) (3.71) y = y0 d 2=002 ln Re As has been mentioned above, ﬂow velocity at the wire surface becomes zero in the viscous ﬂow model, while in the potential ﬂow model it can reach values up to 2y0 . These dierences between the two models are particularly noticeable in the collection process. It was shown by Cummings et al. [C11] that particles in viscous (laminar) ﬂow begin to move away from the wire much further upstream than those in potential ﬂow. Because the viscous ﬂow ﬁeld ”sees” the wire much further upstream, particle transport to the region of the highest magnetic force is greatly diminished. Viscous drag force is obtained from Stokes’s equation (eq. (1.16)) and the components of this drag force can be written: gu ) (3.72) gw g Ig = 6e(y u ) (3.73) gw The components of the ﬂuid velocity yu and y are given by eqs. (3.67) and (3.68) or eqs. (3.70) and (3.71), depending on the value of the Reynolds number. Igu = 6e(yu

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

187

The gravitational force The gravitational force is given by eq. (1.14) and its components, in polar coordinates, can be written [G1, G5]: Iju = (s i )jYs cos( )

(3.74)

Ij = (s i )jYs sin( )

(3.75)

Equations of particle motion The dynamic behaviour of the particle in a single-wire approximation of highgradient magnetic separation is described by eq. (3.58). The complete equations of motion in polar coordinates were obtained by a number of authors, for instance [W8, G1, G5, C11, L6, L7]. If the analysis is limited to the motion of small particles (e.g. 2e ? 75 m), for which the gravitational force is much smaller than the hydrodynamic force, and the condition 2s e2 ?? 1 9

(3.76)

is satisﬁed, the inertial and gravitational terms in eq. (3.58) can be neglected. The radial and azimuthal components of the equation of motion can be written [B10] as : yp N cos 2 gud y0 1 ) (3.77) = (1 2 ) cos( ) ( 5+ gw d ud d ud ud3 ud

yp sin 2 yd 1 g = (1 + 2 ) sin( ) gw d ud dud3

where ud = [email protected] and yp =

20 (s i )P K0 e2 9d

(3.78)

(3.79)

is the parameter introduced by Watson [W8]. It has the dimension of [m/s] and is termed magnetic velocity. When = 0, eqs. (3.77) and (3.78) describe the motion of a particle in the longitudinal conﬁguration, while when = @2 they describe the motion in transverse conﬁguration. By combining eqs. (3.77) and (3.78) the timeindependent equation is obtained [W8]: 1 gud = ud g

yp N cos 2 1 ) cos( ) ( + ) ud2 y0 ud5 ud3 1 yp sin 2 (1 + 2 ) sin( ) + ud y0 ud3

(1

(3.80)

Particle trajectories can thus be described by an equation of a general form yp P 1 gud > ud > ) = i( > ud g y0 2K0

(3.81)

188

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The path taken by the particle depends, therefore, only on yp @y0 > [email protected] , and the initial position and the initial velocity of the particle. The complete equations of motion (eqs. (3.77) and (3.78)) can be solved only numerically. The solutions (i.e. the particle trajectories) are of two types, depending on whether the particle is captured by the wire or not. The critical trajectory, for which the particle is just captured, is characterized by the capture radius Uf . Approximate analytical solutions of the equations of motions s in the case of the potential ﬂow, under the condition that | ypd @y0d | 2> yield the following expression for the capture radius in the longitudinal and transverse conﬁgurations [G1, G5]: s · ¸ 3 3 ypd [email protected] 2 ypd [email protected] 1 ( (3.82) |) ) (| Ufd ' 4 y0d 3 y0d where the normalized quantities are deﬁned as Ufd = Uf @d> ypd = yp @d and y0d = y0 @d= Thus, for a given | ypd @y0d | ratio, both conﬁgurations have the same capture radius. s When | ypd @y0d |? 2> the critical capture radius in the longitudinal conﬁguration ( = 0) is given by Ufd =

i 1 ypd h (1 N 2 )[email protected] + N( arccos N) 2 y0d

(3.83)

and in the transverse conﬁguration ( = @2) [G1]: Ufd =

i 1 ypd h (1 N 2 )[email protected] + N(2 arccos N 2 y0d

(3.84)

It is apparent from eqs. (3.82), (3.83) and (3.84) that the dependence of Ufd upon the ratio yp @y0 can be divided into two categories: at low values of yp @y0 , the capture radius increases linearly with this ratio Ufd

yp y0

(3.85)

while at large values it increases approximately as Ufd (

yp [email protected] ) y0

(3.86)

Axial conﬁguration The analysis of a particle motion in the axial (A) conﬁguration, where the wire axis and the ﬂuid ﬂow are mutually parallel, and the magnetic ﬁeld is perpendicular to them (Figs. 3.13 and 3.17), does not require, in contrast to other cases, numerical computations. Since the results can be derived in an analytical form, this conﬁguration became a favourite object of the modelling of particle capture. The dynamics of the particles and their build-up on the wire

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

189

y H0

v0

ș

x

z

Figure 3.17: The axial conﬁguration.

in A-conﬁguration have been described in numerous papers, for example [G9, B12, U4, B13]. The equations of particle motion (eqs. (3.77) and (3.78)) are reduced in this conﬁguration to the simpliﬁed forms cos 2 gud yp N ) = ( 5 + gw d ud ud3

(3.87)

g yp sin 2 = gw d ud4

(3.88)

g}d y0 = gw d

(3.89)

The elimination of time from eqs. (3.87), (3.88) and (3.89) produces a set of dierential equations N gud = + ud cot 2 g ud sin 2

(3.90)

g}d y0 ud4 = g yp sin 2

(3.91)

From these equations the particle trajectories can be determined analytically [G1,G9, B12].

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

190

Upstream build-up

y

H0

v0 θc

x

Downstream build-up Figure 3.18: Build-up of paramagnetic particles on a magnetized wire in the longitudinal conﬁguration. Particle build-up Previous analyses of particle trajectories in the vicinity of a magnetized wire considered the capture process in the initial stage, i.e. with no loading of the wire with the captured particles. The determination of the exact process of the particle build-up is a complicated problem. As the suspension ﬂows through the matrix, some of the particles, under the inﬂuence of several forces, are deposited onto the matrix elements or onto already deposited particles. Consequently the geometry, the structure and the surface characteristics of the matrix may be signiﬁcantly modiﬁed. These changes, in turn, aect the ﬂow of the suspension through the matrix and the subsequent capture. Further complications may also arise as a result of dislodgment of the captured particles and their possible re-capture. As a result, the dynamic behaviour of the separation process varies with the time as well as with other variables. The force that is principally responsible for the particle capture is the magnetic force. Particles are attracted towards the wire if the radial component of the magnetic force Ipu ? 0= Thus the condition Ipu = 0 deﬁnes the critical angle f given by eq. (3.66). The stability of a particle on the wire surface is determined by the balance of the tangential components mainly of the magnetic and hydrodynamic forces. Gerber found that the angle s , for which a paramagnetic particle will be retained on the wire, is given as [G1]: · ¸[email protected] y0 2 | s |6 arcsin 1 ( ) yp

(3.92)

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

y

191

v0 θc

H0 x

Figure 3.19: Build-up of paramagnetic particles on a magnetized wire in the transverse conﬁguration. It transpires from eq. (3.92) that retention will occur only if yp @y0 A 1 [W8, W9]. However, the experimental results show that a much less stringent condition can still lead to a reasonably high degree of capture. Examples of the build-up of paramagnetic particles on a magnetized wire in three principal conﬁgurations are shown in Figs. 3.18, 3.19 and 3.20. Diamagnetic particles are retained in the complementary regions as follows from Fig. 3.16. The experimentally determined build-up of paramagnetic kimberlite particles in the transverse conﬁguration is shown in Fig. 3.21. Essentially all theoretical descriptions of particle capture by a magnetized wire assumed the idealized situation in which the collection wire axis was oriented orthogonally to the magnetic ﬁeld direction. This assumption resulted from the belief that only these conﬁgurations would create sizable deposits. Birss et al. [B14, S26] considered the collection process on a cylinder with its axis oriented at an angle with the magnetic ﬁeld direction. They found that the eect of the non-orthogonal wire orientation can be taken into account by replacing the coe!cients yp @y0 and N by more general terms. These terms are the functions of the oset angle , deﬁned in Fig. 3.22. Experimental observation by Svoboda et al. [S27], of particle collection at various oset angles , demonstrated that even at the oset angle as large as 800 there is considerable collection of particles, as shown in Fig. 3.23. The length of the section of the wire where the diamagnetic capture takes place is a function of the oset angle. For the oset angle equal to @2 (the magnetic ﬁeld parallel with the wire axis) the paramagnetic capture takes place only at the end of the wire while the entire length of the wire is repulsive for paramagnetic particles, as shown in Fig. 3.24.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

192

y v0

H0 x

Figure 3.20: Build-up of paramagnetic particles on a magnetized wire in the axial conﬁguration.

Figure 3.21: Build-up of paramagnetic particles of kimberlite (mean size 4.7 m, magnetic susceptibility 1.7×106 m3 /kg) on a magnetized nickel wire in transverse conﬁguration (E0 = 1.7 T, y0 = 0.25 cm/s) [S27].

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

193

Į H0

x

vo z

Figure 3.22: The plane view of the generalized transverse orientation with the magnetic ﬁeld making an angle (@2 ) with the wire axis.

Figure 3.23: Collection of kimberlite particles on a nickel wire (diameter 125 m) in the transverse conﬁguration, with the magnetic ﬁeld making an angle of 100 with the wire axis (oset angle = 800 ), (B0 = 1.7 T, v0 = 0.25 cm/s) [S27].

194

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.24: Collection of paramagnetic kimberlite particles on a nickel wire magnetized along its axis (oset angle = 900 ) [S27]. Nesset and Finch [N2, N5] developed a static model of particle capture in HGMS, in which the ﬂuid drag force included the changing boundary layer thickness over the front portion of the wire. They assumed that for a particle to remain attached to the wire, two conditions would have to be met. First, the net radial force acting on a particle must be attractive, that is Ipu + Iju 6 0

(3.93)

where Ipu and Iju are given by eq. (3.62) and (3.74), respectively. The second condition is that the net tangential force must push particles towards the region of a greater attractive radial force. In the case of the longitudinal paramagnetic build-up, this condition can be expressed as: Ip + Ij + Ig 6 0

(3.94)

where Ig is the ﬂuid drag force, which is proportional to the shear stress 0 in the boundary layer. Thus [N2] Ig =

2 2 e 0 2

(3.95)

By solving equations (3.93) and (3.94), the outline of the build-up proﬁle can be found computationally as intersecting loci of points {u> } satisfying these equations. The two retention criteria are satisﬁed only in the cross-hatched region shown in Fig. 3.25.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

195

Figure 3.25: Loci of zero radial and azimuthal forces around the wire in the longitudinal orientation (adapted from [N5]).

Capture of diamagnetic particles It transpires from eq. (1.8) that if the susceptibility dierence s i is positive, then the magnetic force between the wire and the particle is attractive, provided that the radial component Iu is negative. This is the case of capture of paramagnetic particles, under the condition that eq. (3.65) is satisﬁed. On the other hand, there are two symmetrical curved volumes, the boundaries of which are determined by the critical angle f , given by eq. (3.66), in which the radial force acting on paramagnetic particles is repulsive, while the radial force acting on diamagnetic particles is attractive. These regions, in which collection of diamagnetic particles takes place, are complementary to the regions of collection of paramagnetic particles, as illustrated in Figs. 3.18, 3.19 and 3.20. The value of f depends on both Pv (or Mv ) and K0 (or E0 ) as shown in Fig. 3.26. It can be seen that as the strength of the external magnetic ﬁeld increases, the area of the wire collector available for the capture of diamagnetic particle also increases. The eective area for the capture of paramagnetic particles is, therefore, correspondingly reduced. This phenomenon indicates that an increase in the operating magnetic ﬁeld can negatively aect the loading capacity of the matrix, the selectivity of separation and the overall performance of a magnetic separator. The ﬁrst experimental conﬁrmation of the diamagnetic capture was reported by Friedlaender et al. [F9]. They showed that by dissolving a paramagnetic salt in water, i can be made positive and su!ciently large, so that =| s i | is large and the attractive magnetic force is su!ciently strong to recover particles of aluminium oxide. A theory of diamagnetic capture was developed and published by Birss and Parker [B15], simultaneously with

196

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.26: The critical angle f as a function of the magnetic induction (for Mv = 1.7 T) [S1]. Friedlaender’s experimental paper [F9]. Although the recovery of diamagnetic particles by magnetic separation is feasible in principle, simultaneous capture of paramagnetic particles prevents a magnetic separator from being a selective device for separation of diamagnetic materials. This limitation can be, however, overcome by magnetizing the wire collectors along their long axes (the oset angle = @2). At this orientation, the paramagnetic particles are captured only at the end tip of the wire, as is shown in Fig. 3.24. The entire length of the wire is then attractive for diamagnetic particles. Collection of diamagnetic bismuth particles in this conﬁguration was observed by Svoboda et al. [S27] and is shown in Fig. 3.27. Magnetic separation at moderate Reynolds numbers Experimental investigation by Friedlaender et al. into the particle capture on a single wire in the longitudinal conﬁguration indicated [F10] that for moderate values of Reynolds number for the wire (Re 6 to 40), the material can be captured at the rear of the wire. Theoretical treatment by Watson [W10] showed that at higher velocities of the suspension a pair of stable standing vortices, which appear on the downstream side of a wire, can induce capture of particles on the trailing side of a matrix collector. This situation is illustrated in Fig. 3.28. The shaded areas on the upstream and downstream sides of the wire are attractive for paramagnetic particles. The unshaded portions around the | axis are repulsive, and particles arriving from the front part of the wire towards the wake must, therefore, pass through the repulsive regions. It was shown in subsequent studies that the magnitude of the Reynolds num-

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

197

Figure 3.27: Collection of diamagnetic particles of bismuth (" = - 16.3×109 m3 /kg) on the upstream and downstream sides of the nickel wire magnetized parallel to its axis ( E0 = 1.9 T, v0 = 0.13 cm/s) [S27].

y O VO

x

Figure 3.28: The downstream capture into a stationary wake formed by twin vortices.

198

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

ber is not the only condition for the vortex capture [W11]. The thickness of the boundary layer, the particle size and the ﬁeld strength were found to be the main factors aecting the vortex capture. In particular it was determined that, for vortex capture to occur, it is necessary that yp @yr ? 1. The separation process, taking place under such conditions, for which the downstream particle capture takes place, was termed vortex magnetic separation by Watson [W11]. The applicability of this phenomenon, investigated mainly in single-wire experiments, to real operational situations, has been a subject of controversy [S28, W12]. It was argued by Watson et al. [L8] that if the conditions for the downstream capture are met, the recovery, the grade of the magnetic concentrate and the throughput would be very high. However, it was shown by Svoboda [S28] that such conditions can be possibly met only when very ﬁne (e.g. 125 m) steel wool matrix is used and when the ﬂow rate of the slurry through the matrix is close to the upper limit possible in such a matrix [S29]. Such conditions are usually used to remove ﬁne weakly magnetic impurities from industrial minerals, such as kaolin. In those applications, however, the magnetic fraction is a waste and its grade is of no relevance to the e!ciency of the process. On the other hand, in those applications where the magnetic fraction is the useful product, such as beneﬁciation of ferrous and non-ferrous ores, much coarser matrix (e.g. expanded metal or woven mesh) and much higher slurry velocities must be used in order to maintain meaningful economically viable throughput. Under these circumstances the conditions for the vortex formation are not met since the Reynolds number is at least an order of magnitude greater than the upper value required for downstream capture to take place.

3.4.2

Capture of particles in multi-collector matrices

The matrix of a real magnetic separator consists of a large number of individual collectors. There are essentially two possible ways of developing a theory of multi-collector magnetic ﬁlters: one way is to build the theory from ﬁrst principles and the other is to incorporate the single-collector model into a multicollector phenomenological description. In the ﬁrst approach, the particle trajectories and the capture e!ciencies were investigated for the case of wire collectors arranged in regular arrays. Conﬁgurations of single and double layers of wires were analyzed and reported in numerous publications [H14, T4, E1, S30, G7, R12, R13]. As a result of considerable mathematical complexity of the problem the applicability of the theory to real matrix is limited. Particle capture by ferromagnetic spheres. In spite of high e!ciency of a ball matrix in some industrial applications of magnetic separation [S1], only a limited attention has been paid to the theoretical analysis of particle capture by spherical collectors. The character of the particle capture and of the buildup is inevitably dierent for spheres compared to the wires. The dierence follows from the fact that the cross-sectional capture area of a sphere increases

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

199

Figure 3.29: The e!ciency of magnetic ﬁltration of Fe2 O3 particles (diameter 0.08 m) in a bed of steel spheres, as a function of the applied magnetic ﬁeld (adapted from [A16]). quadratically with the capture radius Ufd , whereas that of a wire increases only linearly. Friedlaender et al. [F11, F12] solved numerically the equation of motion (eq. 3.58) in transverse conﬁguration and found that the capture of paramagnetic particles occurred in conically shaped surfaces deﬁned by the critical angle ; h d i< ? 2 1 + 2Nv ( )3 @ u i h (3.96) | f |= arcsin = 3 1 + N ( d )3 > v u which is equivalent to eq. (3.66) derived for a cylindrical wire. The parameter Nv given by P Nv = (3.97) 3K0 is equivalent to eq. (3.61) for the wire. Capture of diamagnetic particles then takes place on conical surfaces complementary to those for paramagnetic capture. It transpired from theoretical analysis of particle capture in a bed of spheres by Watson and Watson [W13] that the probability of particle capture increased with increasing background magnetic ﬁeld until the ﬁeld was high enough to saturate magnetically the ferromagnetic spheres. However, Moyer et al. [M15, M16] argued that the observed saturation of the capture probability occurred at the magnetic ﬁeld strengths far below those required to saturate magnetically the spheres comprising the matrix bed.

200

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.30: Schematic view of the normalized build-up [email protected] in a ﬁlter, as a function of the ﬁlter length. This theoretical prediction was conﬁrmed experimentally by Arajs et al. [A16]. As Fig. 3.29 illustrates, the ﬁltration e!ciency of submicrometer particles of Fe2 O3 in a bed of steel spheres levelled o at the magnetic induction of about 0.1 T, far below the saturation polarization of 1 T of the sphere material. Such a behaviour was not observed for an isolated collecting sphere [F12]. This is a very signiﬁcant observation, since it indicates that the mechanisms of particle capture on a single collector and on an assembly of collectors in a packed bed are governed by dierent laws. It becomes clear again that it is not permissible to extend single-collector theoretical models (eqs. (3.83) and (3.84)) to multicollector assemblies of matrix collectors. Phenomenological model of HGMS The alternative approach to multi-collector magnetic separation is a phenomenological model [W14, G1], which is less rigorous but at the same time less complicated and closer to practical needs of high-gradient magnetic ﬁltration. It cannot, however, be easily applied to the process of separation of multicomponent mixtures of materials. The fundamental equations describing the particle retention in a ﬁlter and the time-dependent performance of a ﬁlter are the macroscopic conservation equations and the rate equation. Let us consider particles travelling through an absorption ﬁlter of length O, as illustrated in Fig. 3.30. By equating the dierence between the numbers of particles entering and leaving the volume { per unit time, to the time rate of increase of the number of particles, the conservation equation is obtained as CQ ({> ) Cf({> ) = y0 C C{

(3.98)

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

201

1

cout/cin

T

t

Figure 3.31: A breakthrough curve of a ﬁlter with a constant absorption coe!cient . At time W the ﬁlter becomes fully saturated. where Q ({> ) is the number of captured particles in the ﬁlter between { and { + {, at time = f({> ) is the number of suspended particles in a volume of the ﬂuid {, is the porosity of the ﬁlter matrix, y0 the superﬁcial velocity and the displacement time deﬁned as = w {@y0 = The rate equation can be expressed in the form of the Iwasaki relation [R14] (

Cf )w = f C{

(3.99)

where is the ﬁlter coe!cient having the dimension of the reciprocal length. Equation 3.99 shows that the proﬁle of the particulate concentrate in the liquid phase throughout a ﬁlter is logarithmic. The solution of the rate equation can thus be written as f({) = exp({) flq

(3.100)

frxw = exp(O) flq

(3.101)

where flq and frxw are the inﬂuent and e"uent concentrations. Since nothing is known, in the phenomenological approach, about the physical processes taking place inside the ﬁlter, all information about the ﬁlter performance must be derived from its breakthrough curve, i.e. from the output concentration as a function of time, as shown in Fig. 3.31. By incorporating the single-wire magnetic separation model into the above eqs. (3.100) and (3.101) Watson found [W8], the e!ciency of the magnetic ﬁlter to be frxw i OUfd = exp( ) (3.102) flq d

202

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where = 2 for ordered ﬁlters and = 4/3 for random ﬁlters. Ufd is the normalized capture radius given, for example, by eqs. (3.82) to (3.84), while i is the ﬁlling factor of the ﬁlter matrix (i = 1 ). Equation (3.102) clearly illustrates that it is not possible to extend the singlewire capture approach to multi-collector situation, as already demonstrated by Fig. 3.29. According to eq. (3.102), the e!ciency of the ﬁlter depends on the capture radius calculated for the single-collector scenario. In the single-collector situation the particle capture is indeed determined by the capture radius and, therefore, by the magnetic velocity or by the strength of the applied magnetic ﬁeld. In a multi-collector situation, there are several additional mechanisms that lead to particle collisions with the collectors and ultimately to capture. As will be shown in the next section, under suitable conditions, usually present in real operational situations, these mechanisms can be signiﬁcantly more important than the magnetic traction mechanism, the only mechanism of particle capture considered in the single-collector approach. By inclusion of the single-collector capture radius Ufd , eq. (3.102), therefore, underestimates, by a wide margin, the e!ciency of the ﬁlter and, at the same time, overestimates the role of the magnetic ﬁeld in particle capture. Particle capture in a real matrix It transpires from the above discussion that it is not permissible to incorporate the single-collector model into a multiple-collector situation. In a single-collector situation the probability of a particle colliding with the matrix element is very small and the particle thus must be attracted to the collector by the magnetic traction force. On the other hand, in a real situation, where the matrix is essentially a bed of matrix elements, the e!ciency of particle collision with the matrix elements is determined, to a great extent, by mechanical, i.e. ”nonmagnetic” mechanisms of collision, as has been argued by Svoboda [S31, S32]. It can, therefore, be assumed that HGMS is essentially a deep bed ﬁlter with an externally applied magnetic ﬁeld. High-gradient magnetic separation can thus be viewed as a stochastic process in which the chance of a particle reporting into the magnetic fraction is the product of two probability terms: Suhfryhu| = Sfroolvlrq × Suhwhqwlrq

(3.103)

where Suhfryhu| is the probability of recovery of a particle into the magnetic fraction, Sfroolvlrq is the probability of collision between a particle and the matrix and Suhwhqwlrq is the probability of retention of a particle on the matrix. While the ﬁrst term on the right-hand side of eq. (3.103) is controlled by the hydrodynamic and geometrical conditions in the matrix, the second term depends on the magnetic and surface forces between the particle and the matrix element, and on the hydrodynamic regime. Collision of particles with the matrix. Figure 3.32 illustrates typical collision mechanisms in a deep bed ﬁlter. These mechanisms also play a decisive role

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

203

A C

D

B a

Figure 3.32: Collision mechanisms in deep-bed ﬁltration. in multi-collector HGMS. A particle following a streamline may come in contact with the matrix element by virtue of its ﬁnite size (interception or straining, case A), and as a result of inertia (case B), sedimentation (case C) or diusion (case D). The velocity of the liquid can be also greater on one side of the particle than on the other, causing the particle to rotate. As a result, a force that develops laterally to the direction of ﬂow will drive particles across the ﬂow ﬁeld. This hydrodynamic eect also contributes to the collision of particles with collectors. The collision probability can then be written, according to eq. (3.101): ffro = 1 exp(O) flq

(3.104)

where ffro is the concentration of particles which collided with the matrix collectors. The ﬁlter coe!cient can be written in terms of the collision e!ciency of a single collector as [M17] = (

3 [email protected] s ) ln(1 ) 4 d

(3.105)

where s = (1 )[email protected] . The total ﬁlter coe!cient can be obtained from eq. (3.105) by calculating the collision e!ciencies l of individual processes (e.g. [W15, I4, C12, H15]) that lead to collision. It was found [S33] that, for example, for steel wool and ball matrices, with element diameter of 200 m and 6 mm, respectively, the dominant mechanism of collision is sedimentation. The hydrodynamic eect also contributes, particularly for small particles. On the other hand, wedging in the crevices of the matrix becomes signiﬁcant for larger particles. Equation (3.104) then can be used to calculate the ratio ffro @flq , i.e. the ratio of the concentration of particles that collided with the matrix, to the concentration of particles that entered the matrix bed. Figure 3.33 documents that all particles as small as 4 m, moving with superﬁcial velocity of 0.07 m/s

204

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.33: The proportion of particles colliding with steel wool matrix as a function of of the matrix length. y = 0.07 m/s, 2d = 400 m, = 0.95 (adapted from Svoboda [S33]).

Figure 3.34: The proportion of particles colliding with a steel ball matrix, as a function of the matrix depth. y = 0.07 m/s, 2d = 6 mm, = 0.4 (adapted from Svoboda [S33]).

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

205

Figure 3.35: The proportion of particles colliding with steel wool matrix, as a function of superﬁcial velocity. O = 200 mm, 2d = 400 m, = 0.95 (adapted from [S33]). or smaller, will have collided with the steel wool matrix, with the matrix bed depth of 200 mm. A similar trend can be observed for the steel ball matrix, as illustrated in Fig. 3.34. With decreasing velocity the probability of collision rapidly increases, as shown in Fig. 3.35. The retention of particles For a particle to be retained on the matrix after a collision, the total interaction between the particles and the matrix and the ﬂuid medium must be attractive. For su!ciently large particles the surface forces can be neglected and the magnetic dipolar and the hydrodynamic interactions are decisive. The mean free magnetic energy for the interaction of a spherical paramagnetic particle of susceptibility with a ferromagnetic sphere of saturation magnetization Pv > placed in an external magnetic ﬁeld E can be written [S1] as 4E 2 e2 32 2 e3 d3 EPv Yp = (3.106) 30 9u3 where u is the distance between the interacting bodies. Since d AA e and u = d + e, eq. (3.106) gives [S31] Yp =

32 2 3 e EPv 9

(3.107)

The hydrodynamic potential energy of a particle captured on the surface of a

206

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

collector is assumed to be Stokesian: Yg = 6yde

(3.108)

A particle will remain attached to the matrix if Yp + Yg ? 0. Therefore, for a particle to be retained by the matrix, the magnetic induction must be greater than the threshold magnetic induction that can be determined from the steadystate condition Yp + Yg = 0. Therefore, [S33]: EA

27yd 16e2 Pv

(3.109)

It is evident from eq. (3.109) that, for given conditions of separation, i.e. particle size and susceptibility, ﬂow velocity and size of matrix elements, an increase in strength of the applied magnetic ﬁeld beyond the threshold value will not increase the retention of particles on the matrix. It might appear from eq. (3.109) that by increasing the magnetic ﬁeld strength it is possible to increase the ﬂow velocity and thus the throughput of a separator, and still maintain the required rate of particle retention. However, if the particle velocity is too high, the particles will never collide with the matrix bed and will thus not be available for retention. This scenario is illustrated in Fig. 3.35. Furthermore, the selectivity of the separation process is be determined by the e!ciency with which the "non-magnetic" particles are being swept away from the matrix by the erosive force of the ﬂuid. Consequently, for particles that are supposed to report into the non-magnetic fraction, the inequality inverse to that given by eq. (3.109) should apply. This is in contrast to the trajectory models, in which the non-magnetic particles never reach the matrix surface.

3.5

Linear open-gradient magnetic separation

The concept of separation in a magnetic ﬁeld with open gradient of the ﬁeld is widely practised in drum and roll magnetic separators. Paradoxically, it is the linear multipole open-gradient magnetic separation (OGMS) that received considerable attention from the theoretical point of view, in spite of its failure to prove its advantages on the production scale. It has been explained in Section 2.5.3, that the linear multipole OGMS consists of an array of vertically positioned coaxial coils energized in opposite directions. The concept is schematically shown in Figs. 2.85(a) and (b) and in Fig. 3.36. The magnetic force directed radially inwards diverts the free-falling magnetic particles inwards while the feebly magnetic particles fall vertically, unaected by the magnetic force. The main advantage of open-gradient separators, in comparison with HGMS, is the absence of matrix which allows the elimination of the blockage problem. Another advantage of OGMS is the use of superconducting magnets which lend themselves easily to scale-up. This is because in resistive magnetic systems the

3.5. LINEAR OPEN-GRADIENT MAGNETIC SEPARATION

207

Feeder

Splitter Cryostat with superconducting coils

Figure 3.36: Schematic diagram of a linear multipole open-gradient magnetic separator. magnetic ﬁeld in the separation space is limited by the non-linear saturation eects in steel [G5]. On the other hand, systems consisting of superconducting magnets are linear as far as the magnetic ﬁeld generation is concerned, and the electric power consumption, which is spent mostly for cryogenic purposes, increases only moderately with their size. It was also found by Gerber et al. [G8] that the metallurgical e!ciency of the superconducting OGMS is superior to the conventional OGMS as a result of considerably larger particle deﬂections achievable in various designs of coil conﬁgurations. A detailed analysis of particle trajectories in dry OGMS was made by Collan et al. [C13], while Kopp [K10, K11] developed a simple kinetic model of the separation process. These models were subsequently reﬁned by numerous authors [B16 , G9, J3, B17, P6, G5]. Particle trajectories and particle deﬂections as a function of particle properties, particle collisions, electric current densities in the coils and the separator geometry were determined. Diamagnetic mode of OGMS was also described theoretically and conﬁrmed experimentally by Krist et al. [K12]. Considerable eort was also devoted to the optimization of the design parameters of the superconducting coils for OGMS [G10, G11, K13, J4, P7]. Although theoretical analyses of particle motion in OGMS are of considerable mathematical elegance, their applicability to practical problems of material separation is limited. In view of a somewhat esoteric character of the subject and as a result of the failure of several eorts to industrialize the concept of

208

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

OGMS [G3, K9, A8, S17] and to achieve commercial success, detailed description is beyond the scope of this monograph. The interested reader is referred to the literature listed above.

3.6

Magnetic ﬂocculation

The demand for mineral products is subject to two factors aecting the e!ciency of beneﬁciation: a decrease in the quality of economically accessible ores and an increase in the degree of ﬁneness of their valuable components. Since the recovery of ﬁne particles is still very ine!cient, vast quantities of valuable minerals are often lost in the form of slimes. Unless new technologies are developed, the increasing amount of ﬁnely-dispersed minerals that being mined and processed, will lead to increased volumes of waste. This will result in a substantial loss of valuable components and in environmental problems. Methods for the treatment of ﬁne particles are still in the early stages of development, and conventional methods are usually ine!cient for particles smaller than 20 m. Particles smaller than 5 m can be manipulated only by HGMS, a rather specialized technique applicable to a limited range of materials. A more general solution to the problem may lie in the formation of aggregates comprising ﬁne particles. In the past, ﬂocs were successfully formed by the addition of inorganic electrolytes or polymers, for instance for the removal of colloidal particles from e"uents. Flocculation can also be induced by the application of external forces to a system of particles, e.g. by stirring, or by the application of magnetic or electrical ﬁelds. Magnetic ﬂocculation has been used for some time to create ﬂocs of ferromagnetic particles. To induce this process, a magnetic induction of the order of 0.01 T is required. Experimental observations of magnetic ﬂocculation of strongly magnetic minerals and its application to the mining industry have been described in numerous publications [B18, B19, B20, B21, L9, K14, K2]. The theoretical description of mutual coagulation of ferromagnetic particles is also well established [D9, J5, L10, L9]. Although investigations into the magnetic ﬂocculation of paramagnetic and diamagnetic particles started much later [H16, W16, S34], systematic studies of the theoretical and experimental aspects [S35, P8, S36, P9, S37, S38, W17, W18, W19, P10, T5, S39, S40, S41] show that ﬂocculation of ﬁne, feebly magnetic, particles can be induced in magnetic systems that are presently available. In the following sections the present status of the theory of magnetic ﬂocculation of strongly and weakly magnetic materials will be brieﬂy outlined.

3.6.1

Magnetic ﬂocculation of strongly magnetic materials

The tendency of an assembly of ferromagnetic particles in the magnetic ﬁeld of a magnetic separator to reduce its magnetostatic energy often results in the formation of aggregates of the particles. The eect of magnetic ﬂocculation

3.6. MAGNETIC FLOCCULATION

209

is the inherent part of any process of manipulation of ﬁnely ground strongly magnetic materials and directly aects the e!ciency of material separation. In magnetic separation the process of magnetic ﬂocculation can often play a positive role by increasing the recovery and/or throughput. In other processes, such as recovery of dense medium, magnetic ﬂocculation is detrimental to the e!ciency of dense medium separation. Theory of magnetic ﬂocculation We shall consider a suspension of identical spherical ferromagnetic particles in a non-magnetic ﬂuid. Under the inﬂuence of a su!ciently strong external magnetic ﬁeld such particles tend to associate in long chains. Each particle s. of volume Ys and magnetization Ps carries a magnetic moment P = Ys P The energy of magnetic interaction between particles (1) and (2) separated by a distance u is YP =

1 P (1)P (2) 3[P (1)u][P (2)u] { } 0 u3 u5

(3.110)

If magnetization of the particles is su!ciently large, the electrical double layer interaction and the van der Waals interaction can be neglected. Total interaction energy, therefore, consists of the magnetic dipolar term only (eq. (3.110)). Eective magnetic interaction in the suspension can be obtained by averaging YP over all orientations of the colloidal particles. Thus [C14, C15] YP Y¯P = nW ln ? exp( )A nW

(3.111)

where n is the Boltzmann constant and W is the absolute temperature and Z YP 1 YP (3.112) exp( ) A= )g 1 g 2 g 3 ? exp( 3 nW 64 nW where g l (l =1,2,3) represents an element of a solid angle describing the orientation of each of the dipoles (1, 2) and that of the external magnetic ﬁeld (3). It was shown by Chan et al. [C14, C15] and by Scholten et al. [S42] that in the weak interaction limit, i.e. when 2P @0 u3 ? nW , the average interaction energy can be written as 4 Y¯P = 2 P6 (3.113) 30 u nW while in the strong interaction limit (2P @0 u3 A nW ) 2

2 Y¯P = P3 0 u

(3.114)

It can thus be seen that although the magnetic dipole-dipole interaction (eq. (3.110)) can be either attractive or repulsive, depending on the relative orientation of the dipoles, the orientational averaging process gives the energetically favourable (attractive orientation) heavy weighing.

210

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.37: The eect of the magnetic ﬁeld strength on the degree of ﬂocculation of strongly magnetic particles (adapted from [K14, K2]). A condition for magnetic ﬂocculation to take place can be expressed as Ip A Ig + Ih

(3.115)

where Ih is the electric force as a result of electrical double layer. Since Ip AA Ih for ferromagnetic particles at reasonably strong magnetic ﬁeld, the probability of ﬂocculation is determined by the interplay between the magnetic and hydrodynamic forces. As a function of the magnetic ﬁeld strength, the process of magnetic ﬂocculation proceeds through several stages, as is shown in Fig. 3.37. In stage 1, which corresponds to the steady-state phase of the process, in which Ip 6 Ig , the degree of ﬂocculation # i is proportional to Ip and, therefore, # i = nK 2 = At this phase the grade of the ﬂocs is high and ﬂocculation is selective. With further increase in the magnetic ﬁeld strength the magnetic interaction becomes dominant and the ﬂocculation enters phase 2. The process proceeds non-selectively at a very high rate and the grade of the ﬂocs is reduced. When the concentration of solids in a suspension is reduced below a certain threshold value, the mean distance between the particles and their characteristic ﬂocculation time increase and the process enters an equilibrium phase 3.

3.6.2

Magnetic ﬂocculation of weakly magnetic minerals

In contrast to strongly magnetic materials, the magnetic ﬂocculation of paramagnetic and diamagnetic materials is a considerably more complex process. In spite of its signiﬁcant potential, the process has not found any application on industrial scale as yet. Although several theoretical models that predict the behaviour of weakly magnetic particles of quasi-colloidal dimensions, in the

3.6. MAGNETIC FLOCCULATION

211

presence of the external magnetic ﬁeld, have been developed over the last twenty years, their experimental veriﬁcation is still limited and is mainly of qualitative character. Stability of colloidal suspensions The criteria of the stability of colloidal suspensions are governed largely by the interplay of repulsive and attractive forces between the particles. A detailed description of this interplay is the basis of the theory of stability of hydrophobic colloids as proposed by Derjaguin and Landau [D14] and Verwey and Overbeek [V1] (DLVO theory). The DLVO theory views the stability of colloids as arising from electrical charges on identical particles and a consequent electrical repulsion between them. Opposing this repulsion are the attractive forces of the universal London-van der Waals type. If the repulsion force can be su!ciently reduced so that the attractive interaction becomes dominant then the particles colliding with one another will stick together to form quasi-stable aggregates. The charge on a particle, together with the equal and opposite charge in a suspension, comprise the electrical double layer (EDL). Hogg et al. [H17] showed that the interaction of EDL between two dissimilar particles, under the condition of low surface potential and small thickness of EDL compared to the particle size, is given, under the assumption of a constant surface potential, by ¸ · u e1 e2 (# 21 + # 22 ) 2# 1 # 2 1 + exp([k) 2[k YU = ) (3.116) ln + ln(1 h 4(e1 + e2 ) (# 21 + # 22 ) 1 exp([k) where e1 > e2 and # 1 > # 2 are the radii and surface potentials of particles, respectively, u the dielectric constant of the medium, [ the Debye-Hückel reciprocal length parameter, and k their distance between the surfaces of the interacting particles. [ is related to the ionic strength Lp of the medium by the expression [=

[email protected]

8h2 Lp u nW

(3.117)

In the case of identical spherical particles eq. (3.116) reduces to u e# 2 (3.118) ln(1 + h[k ) 2 When the thickness of EDL is not small (i.e. when e[ ? 1), YU can be expressed in a simple approximate form: YU =

YU = u e2 # 2

exp([k) (2e + k)

(3.119)

Similarly, the London - van der Waals interaction for dissimilar spheres can be written as 6 5 2e1 e2 2e1 e2 + + D 9 k2 + 2(e1 + e2 )k k2 + 2(e1 + e2 )k + 4e1 e2 : : (3.120) YD = 9 8 k2 + 2(e1 + e2 )k 6 7 ln 2 k + 2(e1 + e2 )k + 4e1 e2

212

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where D is the Hamaker constant. For identical particles, eq. (3.120) simpliﬁes to ¸ · D k2 + 4ek 2e2 2e2 YD = (3.121) + ln 2 + 6 k2 + 4ek k2 + 4ek + 4e2 k + 4ek + 4e2 When the London forces operate over distances comparable to or larger than 0.1> where is the wavelength of the intrinsic electronic oscillations of the atoms, the interaction is reduced by the retardation eect [S43, R15]. Flocculation in a magnetic ﬁeld When a suspension of colloidal particles is placed in an external magnetic ﬁeld there is, in addition to the interactions considered so far, a magnetic dipolar interaction, described by eq. (3.110). In the strong interaction limit [C14, S34], the mean magnetic interaction energy can be written as YP =

80 1 2 e31 e32 K 2 9(k + e1 + e2 )3

(3.122)

where l are volume magnetic susceptibilities of particles and K is the magnetic ﬁeld strength. In agreement with the assumption of the DVLO theory that double layer and van der Waals forces are independent and additive, Svoboda [S34] supposed that the total energy of interaction of colloidal particles in the external magnetic ﬁeld is, therefore, given by the sum of electrical double-layer energy, van der Waals interaction energy and magnetic dipolar interaction energy YW = YU + YD + YP

(3.123)

Generally, the total interaction energy YW can be either attractive or repulsive depending on the sign of the individual terms on the right-hand side of eq. (3.123). Electrical double layer energy is repulsive for interaction of particles of the same material, while it can be attractive or repulsive for interaction of unlike materials (e.g. between a valuable mineral and gangue). The van de Waals interaction is usually attractive, but under certain conditions [V2], determined by relative values of the Hamaker constant of the interacting particle and the medium, the interaction becomes repulsive. Magnetic interaction can be either attractive or repulsive, depending on the signs of the magnetic susceptibilities of the interacting particles. It is clear that interaction between diamagnetic and paramagnetic particles is repulsive. On the other hand, magnetic interaction of identical materials, whether paramagnetic or diamagnetic, is always attractive. Magnetic ﬂocculation of diamagnetic particles is, therefore, possible, in principle. A curve of the total interaction energy YW as a function of the interparticle distance is shown in Fig. 3.38. A potential barrier Ymax separates two minima: a closer and deeper primary minimum and a more distant and shallow secondary

3.6. MAGNETIC FLOCCULATION

213

VT

Vmax Vmin 0

r

2b

r

Figure 3.38: The general form of the total potential energy for a pair of interacting colloidal particles of radius e= minimum of depth Ymin . The individual potential energy contributions are aected by the properties of a suspension in dierent ways. The magnitude and range of the electric double layer interaction YU are sensitive to # and [, which are controlled by the solution conditions (i.e. ionic strength and pH), whereas the van der Waals and magnetic contributions YD and YP are independent of these parameters. The magnitudes of the individual potential energy components have a dierent dependence on the particle size: YP is proportional to the cube of the radius while YU and YD are much less sensitive to particle size as they are proportional to the ﬁrst power of particle size. The height of the barrier determines the stability of a suspension. If the barrier is very low, there is nothing to prevent contact between the particles, and ﬂocculation will take place at a rate governed by the frequency with which the particles collide. If there is a secondary minimum in the curve of a potential energy, particles can ﬂocculate into this potential well. In this instance, the potential barrier need not be suppressed. Flocs thus formed will have a rather loose structure as a result of large interparticle distance at which the secondary minimum is created. The existence and position of the primary and secondary minima can be aected by changes in the magnetic ﬁeld, the magnetic susceptibility of the particles and the pH value of the suspension. The total interaction energy YW is shown in Fig. 3.39 as a function of magnetic induction and particle size. In region I the potential barrier is present and the secondary minimum is su!ciently close, while in region II the secondary minimum is too distant. In regions III and IV, in which, owing to high magnetic induction, the potential

214

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.39: Regions in which primary and secondary minima are found in the (a,B) plane, for hematite (# = 30 mV, [ = 105 m1 ), d - particle radius, E - magnetic induction (after [S36, S37]).

barrier is suppressed and the total interaction becomes attractive, and particles can ﬂocculate into the primary minimum. It follows from Fig. 3.39 that, for any particle size, a value of the magnetic induction can be found at which the potential barrier disappears. Wang et al. [W17] calculated the potential energy of interaction of particles of hematite and chromite in a magnetic ﬁeld. Typical curves shown in Fig. 3.40 illustrate that at moderate magnetic ﬁeld strength the potential barrier is eliminated and ﬂocculation into the primary minimum could take place. A deep secondary minimum is created at even lower magnetic ﬁeld. A threshold magnetic ﬁeld, at which the ﬂocculation into the primary minimum starts, can be determined provided that the total potential energy of interaction YW is negative [S34], or that the stability ratio Zs , which is given by eq. (3.124), is smaller than, or equal to, unity [S35]. The stability ratio is the ratio of the initial rate of ﬂocculation to that which would occur if the process was only diusion controlled (in the absence of an energy barrier) [P11]. µ

Z Zs = 2

exp

YW nW

¶

gv v2

(3.124)

3.6. MAGNETIC FLOCCULATION

215

Figure 3.40: The potential energy as a function of interparticle distance for 4 m hematite particles, [ = 108 m1 (adapted from Wang et al. [W17]).

Figure 3.41: Threshold magnetic ﬁeld, at which ﬂocculation into a primary minimum begins, as a function of particle size (adapted from Svoboda [S35]).

216

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The values of the threshold magnetic ﬁeld Es , at which magnetic ﬂocculation into the primary minimum begins, are shown in Fig. 3.41, as a function of particle size, for various minerals. It can be seen that as the particle size and magnetic susceptibility increase, the threshold magnetic ﬁeld decreases. For ﬁne particles with a volume magnetic susceptibility smaller than 103 (SI), the threshold magnetic ﬁeld is too high for magnetic ﬂocculation to be practicable. This is particularly true for the magnetic ﬂocculation of diamagnetic materials, which require a magnetic induction of the order of tens of hundreds of Tesla. Flocculation in the secondary minimum As shown in Fig. 3.39, there is a secondary minimum (SM) in addition to the primary minimum in regions I, II and III. Although in regions I and II the potential barrier prevents particles from ﬂocculating into the primary minimum, particles can ﬂocculate into the secondary minimum. The secondary minimum in region II is too distant from the origin, and consequently, the aggregates will be packed too loosely. Furthermore, the secondary minimum is too shallow and the stability of the ﬂocs will be low. However, in region I, the secondary minimum can be deep enough and close enough to the origin to render it suitable for practical ﬂocculation. The mere existence of a secondary minimum does not imply an observable destabilization of a suspension. The other condition to be satisﬁed is su!cient depth of SM; the analysis indicates [S36] that, for Ymin A 1 kT (where kT is the unit of thermal energy), the value of the stability ratio Zv for ﬂocculation in a secondary minimum, as given by eq. (3.125), will be close to unity, and the ﬂocculation into SM will be rapid.

Zv =

R4

YW gv ) nW v2 Ymin 1 exp( ) nW

vp

vp

exp(

(3.125)

where vp is the position of the secondary minimum. The threshold magnetic ﬁeld Ev required to commence the ﬂocculation into SM can be determined from the condition Zv = 1. The dependence on a particle radius of threshold magnetic ﬁeld Ev in SM, which was determined from the condition of rapid ﬂocculation (Zv = 1), is shown in Fig. 3.42. A comparison of these values with those of the threshold magnetic ﬁeld Es for ﬂocculation into the primary minimum (Fig. 3.41) indicates that the magnetic ﬁeld needed to induce rapid ﬂocculation in SM is substantially lower. This conclusion has been conﬁrmed by detailed calculations by Wang et al. [W17], an example of which is presented in Fig. 3.40. Experimental conﬁrmation of the magnetic ﬁeld-induced ﬂocculation is depicted in Fig. 3.43. Figure 3.44 illustrates the experimentally determined onset of rapid ﬂocculation of hematite and chromite at threshold magnetic ﬁeld of about 0.5 T [W17].

3.6. MAGNETIC FLOCCULATION

217

Figure 3.42: Threshold magnetic ﬁeld for ﬂocculation into a secondary minimum, as a function of particle diameter (adapted from Svoboda [S35]).

Figure 3.43: The magnetic ﬁeld-induced ﬂocculation of hematite particles at various values of magnetic induction. pH = 7.8, # 45 mV, g50 = 3.9 m (adapted from Wang et al. [W17]).

218

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.44: The onset of the magnetic ﬁeld-induced ﬂocculation of hematite (g50 = 3.9 m) and chromite (g50 = 3.6 m) particles (adapted from Wang et al. [W17]). We have seen that under suitably chosen conditions, the interaction potential between a pair of colloidal particles can develop a signiﬁcant (> 1 kT) secondary minimum, while maintaining a large (AA 1 kT) primary maximum. Although the primary maximum will prevent irreversible coagulation into the primary minimum, the particles can undergo reversible ﬂocculation into the secondary minimum. The above treatment of the ﬂocculation process is applicable only to colloidal particles. For particles greater than the colloidal range, the thermal motion and the surface forces play only a limited role, and the process of ﬂocculation will be governed mainly by the gravitational and hydrodynamic forces. The kinetics of ﬂocculation It has been shown that the stability of suspensions depends on the magnitude of the potential barrier and on the existence and depth of the secondary minimum. In addition, however, determination of how quickly ﬂocculation will take place is necessary. Fuchs [F13] showed that the time taken for the number of particles to be halved is given by the relation [email protected] =

3Z 4nW Q0

(3.126)

where is the viscosity of the medium and Q0 is the initial concentration of the particles.

3.6. MAGNETIC FLOCCULATION

219

Figure 3.45: Dependence of the stability ratio Zs (as log Zs ) on magnetic induction for assorted sizes of hematite particles (adapted from Svoboda [S35]). It can be seen that the half-time of ﬂocculation is directly proportional to the stability ratio and indirectly proportional to the initial concentration of the particles. To achieve a reasonably short ﬂocculation time, low values of Z and high values of Q0 must be used. In chemical ﬂocculation, the values of Z smaller than 101 are reached with di!culty [V1]. This signiﬁcantly restricts the possibility of accelerated ﬂocculation. On the other hand, it was shown by Svoboda [S35], that in magnetic ﬂocculation, the values of the threshold magnetic ﬁeld determined from the condition Z = 1 for rapid ﬂocculation, allow reasonably short ﬂocculation time to be achieved. As is shown in Fig. 3.45, the values of Zs , of the order of 103 > can be achieved at reasonably low magnetic ﬁelds so that the ﬂocculation time into the primary minimum can be realistically short. Magnetic-hydrophobic ﬂocculation In order to explain situations in which the original DLVO theory failed, numerous ”non-DLVO” forces have been invented. A variety of forms of long-range forces such as hydrophobic/hydrophilic interaction have been introduced. For example, surface-active agents can adsorb at the mineral-water interface and render the solid hydrophobic. Particle-particle adhesion is favoured by the attraction between the hydrophobic coatings on dierent particles and the resultant reduction in the area of hydrophobic mineral-water surface. A critical review of such extensions of DLVO theory to include ”non-DLVO” interactions was published by Ninham [N6] who argued that confusion created

220

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.46: The potential energy curves for hydrophobic and magnetic ﬂocculation of rhodochrosite (2e50 = 2.25 m) hydrophobized by sodium oleate, at a magnetic induction of 0.9 T (adapted from [L11]).

by introduction of plethora of hydrophobic phenomena observed in the stability studies can, in principle, be explained by capillary condensation, i.e. thermodynamics. Several authors have shown that the stability of a colloidal suspension can be controlled, in addition to the electrostatic surface potential and the magnetic interaction, by such a hydrophobic interaction. Lu et al. [L11] included the energy of hydrophobic interaction YK as an additive term in the expression of the total interaction energy (eq. (3.123): YW = YU + YD + YP + YK

(3.127)

The hydrophobic interaction energy was expressed by two terms, each representing dierent mechanism of the hydrophobic interaction. The potential energy curves of three possible ﬂocculation mechanisms for paramagnetic rhodochrosite were calculated and are shown in Fig. 3.46. It can been seen that the potential energy of magnetic interaction exhibits a deep secondary minimum and a primary minimum barrier. In hydrophobic aggregation, a relatively low potential barrier partially prevents particles from rapid ﬂocculation into the primary minimum. On the other hand, the potential energy curve for combined magnetic and hydrophobic ﬂocculation shows deep primary and secondary minima, with no potential barrier. The experimentally determined rates of ﬂocculation in these three regimes are illustrated in Fig. 3.47. It is clear that the combined ﬂocculation by a

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION

221

Figure 3.47: Flocculation of rhodochrosite by magnetic (B = 0.85 T), hydropohobic (sodium oleate + kerosene) and combined mechanisms (adapted from [L11]). combination of magnetic and hydrophobic processes was more eective than aggregation induced by sodium oleate or magnetic ﬁeld alone. Škvarla and Zeleˇ nák [S41] developed a simple model of magnetic-hydrophobic ﬂocculation, as a variation of Lu’s model [L11]. They assumed that the potential of the hydrophobic interaction was of the short range and it was approximated by a single exponential YK = 2e VO exp(

kf k )

(3.128)

where VO is the solid/water interfacial energy of the spherical particles, kf is the contact separation distance of the spheres ( = 0.2 nm), and is the empirical constant ( = 1 nm). The model was veriﬁed by experimental observation of magnetic-hydrophobic ﬂocculation of siderite. A satisfactory correlation between the measured and calculated potential energy maxima was observed for the hydrophobic process. The prediction of the model of magnetic ﬂocculation alone was not satisfactory.

3.7

Magnetic separation by particle rotation

Motion of magnetizable particles in alternating or rotating magnetic ﬁelds is a well established research ﬁeld. In 1925 Koizumi [K15] designed a magnetic separator with a rotating magnetic ﬁeld, to eliminate entrapment of non-magnetic

222

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.48: Schematic diagram of a separator with rotating magnetic ﬁeld (courtesy of N. Allen [A17]).

particles in the magnetic concentrate. Similar approach was taken more recently by other researchers to improve the quality of magnetic concentration [T3, D1, F1, G12, G13, L9]. Although the results of these investigations had been positive, the technique did not appear to be accepted and developed further. Recently, Allen [A9] employed the concept of the eect of a rotating magnetic ﬁeld on magnetizable particles and developed rotating magnetic ﬁeld (RMF) separators, described in Section 2.6.3. The rotation separation is based on magnetic anisotropy of particles, which is present in ferromagnetic as well as paramagnetic materials. However, in paramagnetic minerals the magnetic anisotropy is generally too weak to be of practical use for particle separation. In general, ferromagnetic particles will rotate if they are placed in a rotating external magnetic ﬁeld, while paramagnetic particles will not. An RMF is generated by a rotating magnetic drum ﬁtted, around its circumference, with magnets, with alternate polarity. As is schematically illustrated in Fig. 2.95, the external magnetic ﬁeld exerts a torque on a magnetically anisotropic particle and makes it rotate and move it in the direction opposite to that of the rotating ﬁeld. A schematic diagram of such an RMF separator is shown in Fig. 3.48.

3.7.1

RMF rotation separation

In the RMF separator a particle is placed on a non-magnetic surface in a rotating magnetic ﬁeld, as shown in Fig. 3.49. If the particle is capable of rotation in the

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION x

223

Direction of particle rotation

Particle Direction of drum rotation

Magnet N S

S

N

N

Drum Fg,FgFm

Figure 3.49: Schematic diagram of a particle placed on a rotating magnetic drum. ﬁeld, it will experience a torque in order to align its axis of easy magnetization with the direction of the external magnetic ﬁeld. The torque, which thus arises when the direction of the magnetization of a particle and the external magnetic ﬁeld do not coincide, will force the particle to roll. The rolling is opposed by the force of gravity and magnetic traction force acting on the particle. The particles to be separated by rotation will, in general, contain ferromagnetic and paramagnetic regions. While the paramagnetic regions will make limited contribution to the particle rotation, they will contribute to the magnetic traction (holding) force. This traction force can, therefore, be written [A17] as: 1 Ip = s Yss EuE + Psi Ysi uE (3.129) 0 where Yss and Ysi are the volumes of the paramagnetic and ferromagnetic regions of the particle, respectively. Psi is the magnetization of the ferromagnetic components while s is the volume magnetic susceptibility of the paramagnetic contribution. The magnitude of the torque of the force I , required to rotate a particle, is the product of the magnitude of the force and the moment arm g; that is W = Ig (3.130) The particle will not start rotating unless the initial magnetic rotational torque exceeds the initial gravitational and magnetic traction force torques (case (a) in Fig. 3.50). The cubic shape of the particle is usually used to demonstrate the

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

224

(b)

(a)

( c)

B L

ș

M L

d

Fg Fm

Fg , Fm

Figure 3.50: Forces acting on a cubic particle in traction and rotating magnetic ﬁelds. case [A17, A18] and we have Wlqlw =

O (Ij + Ip ) 2

(3.131)

where O is the length of the cube edge and the force of gravity Ij is given by eq. (1.14). For a cubic ferromagnetic particle, under the assumption that the ﬁrst term on the right-hand side of eq. (3.129) can be neglected, the initial gravitational + magnetic holding torques (that is, when the particle is resting ﬂat on the surface) can be written Wlqlw = O3 s j

3.7.2

O O + Ps O3 uE 2 2

(3.132)

Magnetic torque on a particle and condition for separation by rotation

The application of an external magnetic ﬁeld to a ferromagnetic crystal, at a certain angle + to a direction of easy magnetization, causes a deviation of the magnetization, as indicated in Fig. 3.51. The external magnetic induction E applies a torque to the particle magnetization Ps and causes it to deviate from the direction of easy magnetization {. As a result, the magnetocrystalline forces apply a torque on the magnetization to return it to the direction of easy

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION

B

225

M ș

į

x

y

Figure 3.51: The torque experienced by an anisotropic magnetizable particle placed in an external magnetic ﬁeld. magnetization. This situation can be described by a relationship Ps E sin = Ps D sin

(3.133)

where D represents the anisotropy ﬁeld. If the external ﬁeld is very low, then the angle is small. If the external ﬁeld is very high, then is small [A17]. For a cubic particle, the magnetic torque given by eq. (3.48), can be rewritten as: Wpdj = Ys Ps E sin = O3 Ps E sin (3.134) where is the angle between the directions of the magnetic ﬁeld and particle magnetization, as can be seen in Figs. 3.50(b) and 3.51. Therefore, a particle will start rotating when Wpdj A Wlqlw (3.135) or, explicitly, E sin A

O s j + uE) ( 2 Ps

(3.136)

Coercive forces are very low for many ferromagnetics (s.l.), such as magnetite and steel, while anisotropy forces are high. If the external ﬁeld is smaller than the coercive force (E ? 0 Kf ), angular deviations from directions of easy magnetization are also small. Maximum torque is then applied when the external ﬁeld is very close to 900 to the particle magnetization. [A17]. Although the angle between the magnetization and the external ﬁeld has been maximized, the external ﬁeld is very low for most materials and, therefore, the torque is small. However, for materials of very high coercive force, such as roasted ilmenite, this is an advantageous situation for magnetic separation by rotation.

226

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

In a magnetic ﬁeld that exceeds the coercive force Kf of the material, the movement of domain walls within the solid substitutes for the movement of particles. The overall magnetization of a ferromagnetic particle is able to change direction in response to the direction of the external ﬁeld. However, while the changes of the direction of the domain magnetization may occur freely between directions of easy magnetization within a crystal, they are restrained for intermediate angles by magnetocrystalline anisotropy. In this case the maximum torque angle is approximately one quarter of the angle between directions of the external ﬁeld and the particle magnetization [A20, A17].

3.7.3

Rotation of particles in a liquid

It has been assumed, so far, that the particles to be rotated are suspended in air. If the particles are suspended in water, they are exposed, in addition to the force of gravity and the magnetic traction force, to hydrodynamic forces. These hydrodynamic forces are associated with a torque acting in the opposite direction [L9]. It was shown by Lantto [L9] that the hydrodynamic torque at a high Reynolds number is approximately given by Wk|gur =

1 $ 2 f4 e5 2 i

(3.137)

where $ is the frequency of the rotating magnetic ﬁeld, e the radius of the cylindrical particle, the length of which is fe (where f AA1). The magnetic torque is Wpdj = 2fe3 Ps E sin

(3.138)

Therefore, a cylindrical rod-like body will be brought into rotation when Wpdj A Wk|gur . This condition is met when EA

i $ 2 f3 e2 4Ps sin

(3.139)

It can be seen that rotation is more easily accomplished for small particles with large values of magnetization and large anisotropy angle . On the other hand, an increase in frequency of the rotating ﬁeld hampers the ability of particles to rotate. It has to be stressed, however, that if the value of the magnetic induction given by eq. (3.139) exceeds that corresponding to the coercive force (E A 0 Kf ) for the particle material, the particles will either cease to rotate and may become demagnetized. If the particles are still rotating, the angle will be reduced. In laminar ﬂow, with small Reynolds numbers, the viscosity of the liquid will play an important role; otherwise the general character of the phenomenon is the same as that at high Reynolds numbers [L9].

3.8. SEPARATION IN MAGNETIC FLUIDS

3.8

227

Separation in magnetic ﬂuids

The sink-and-ﬂoat technique of gravity separation relies on selective levitation and sinking of materials based on their relative densities and that of the separating medium. The scope of the sink-and-ﬂoat technique is restricted by a limited range of densities of the separating medium, the upper limit of ferrosilicon medium being approximately 3500 kg/m3 and that of Clerici solution about 4200 kg/m3 at room temperature. In the mid sixties of the last century the application of magnetic ﬂuids as a heavy medium, had been investigated, and it was established that by exposing a magnetic ﬂuid to a non-homogeneous external magnetic ﬁeld the ﬂuid exhibited an apparent density exceeding densities obtainable with conventional heavy liquids. Two broad classes of magnetic ﬂuids were investigated at that time, namely paramagnetic liquids [A1, A12, A19] and ferroﬂuids [R1, R7, R8, R16, G4, K16, F8]. Paramagnetic liquids are solutions of paramagnetic salts, such as MnCl2 and Mn(NO3 )2 . These liquids are paramagnetic in their behaviour: their magnetization increases linearly with an increasing magnetic ﬁeld and their susceptibility is low, of the order of 6×107 m3 /kg. On the other hand, a ferroﬂuid is a stable colloidal suspension of sub-domain ferromagnetic (s.l.) particles, for example magnetite, in a liquid carrier. The behaviour of ferroﬂuids is superparamagnetic, characterized by the absence of hysteresis and coercivity. Ferroﬂuids dier from paramagnets in having quite large magnetic susceptibilities and being able to become saturated in moderate magnetic ﬁelds. Saturation polarization of a ferroﬂuid can be as high as 0.1 T (1000 G) The concept of separation of non-magnetic particles suspended in a magnetic ﬂuid is based on the generalized Archimedes law whereby, in addition to the conventional force of gravity acting on the ﬂuid, also a magnetically induced force acts on the ﬂuid. This additional magnetic pull creates a magnetically induced buoyancy force on a particles immersed in the ﬂuid. This buoyancy force can be controlled in a wide range of values and materials as dense as 20 000 kg/m3 or higher can ﬂoat in such a ﬂuid. A schematic diagram of the process of separation in magnetic ﬂuids is shown in Fig. 3.52, while a general diagram of a magnetic circuit used in separation in magnetic ﬂuids in shown in Fig. 3.53. Permanent magnets or electromagnets are used to generate a non-homogeneous magnetic ﬁeld in the separation gap. The desired pattern of the magnetic ﬁeld and its gradient is achieved by shaping the pole tips. A separation chamber placed between the pole-pieces of the magnetic circuit is ﬁlled with a magnetic ﬂuid.

3.8.1

Apparent density of a magnetic ﬂuid

There are two dominant forces acting on a volume of the magnetic ﬂuid, placed in an external non-homogeneous magnetic ﬁeld, namely the force of gravity and the magnetic traction force. The situation is schematically depicted in Fig. 3.52.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

228

Ferrofluid Floating particles

Element of ferrofluid

Magnet

Fg

S Fm

N

Sinking particles

Figure 3.52: Schematic diagram of the process of separation in magnetic ﬂuids.

Figure 3.53: Schematic diagram of a magnetic circuit used in separators with magnetic ﬂuids.

3.8. SEPARATION IN MAGNETIC FLUIDS

229

The total force on the magnetic ﬂuid of volume Yi can be written as: 1 Ii = Ij + Ip = i Yi j + i Yi EuE 0

(3.140)

where i and i are the physical density and volume magnetic susceptibility, respectively, of the magnetic ﬂuid. For a ferromagnetic (s.l.) ferroﬂuid, the magnetic force can be expressed as 1 Ip = Mi Yi uE 0

(3.141)

where Mi is the magnetic polarization of the ferroﬂuid. When the ﬁeld gradient is parallel with the gravitational force and of the same sense, eqs. (3.140) and (3.141) can be rearranged, as

and

i Ii = Yi j (i + EuE) 0 j

(3.142)

Mi Ii = Yi j (i + uE) 0 j

(3.143)

The expressions in parentheses can be viewed as an apparent density d of a magnetic medium exposed to an external non-homogeneous magnetic ﬁeld: d = i +

i EuE 0 j

(3.144)

Mi uE 0 j

(3.145)

and d = i +

In a more general case, when the ﬁeld gradient makes an angle with gravity, eq. (3.145) becomes Mi d = i + uE cos (3.146) 0 j Equations (3.143) and (3.145) form the basis of ferrohydrostatic separation (FHS). In a typical case, a water-based ferroﬂuid with polarization of 0.02 T (200 G), placed in a magnetic ﬁeld of gradient of 2 T/m (200 G/cm) will exhibit an apparent density of approximately 4200 kg/m3 . Figure 3.54 illustrates the apparent density as a function of the ﬁeld gradient for two types of kerosenebased ferroﬂuid.

3.8.2

A particle suspended in a magnetic ﬂuid

A particle suspended in a magnetic ﬂuid is acted upon by several forces illustrated in Fig. 3.55. The force of gravity is given by Isj = s Ysj

(3.147)

230

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.54: The apparent density as a function of the gradient of the magnetic ﬁeld for two types of kerosene-based ferroﬂuid, of dierent densities and magnetic polarizations. while the magnetic traction force is 1 s Ys EuE Isp = 0

(3.148)

where s is the volume magnetic susceptibility of the particle. Such a particle experiences a loss of its weight as a result of two buoyancy forces acting on the particle. The ﬁrst buoyancy force is the classical Archimedes gravity-related force: Isje = i Ysj (3.149) The other force is the magnetically induced buoyancy force due to the magnetic traction force acting on the ferroﬂuid: 1 Ispe = Ys Mi uE 0

(3.150)

The net vertical force on a particle suspended in a ferroﬂuid and acted upon by a non-homogeneous magnetic ﬁeld with vertical gradient can thus be written: Is = Isj + Isp + Isje + Ispe

(3.151)

uE Ys (s E Mi ) Is = Ys (s i )j + 0

(3.152)

or, in an explicit form:

3.8. SEPARATION IN MAGNETIC FLUIDS

231

Fpd (1)

Fpmb

Fpgb Solid particle

Pool of ferrofluid Gradient of the magnetic field

Fpg Magnetic field Fpd (2) Fpm

Figure 3.55: Forces acting on a particle in a stationary ferroﬂuid, placed in a non-homogeneous magnetic ﬁeld. Deﬁning the eective cut-point density fs for separation as that particle density s for which Is = 0 (i.e. equilibrium of the forces acting on the particle), eq. (3.152) yields: uE fs = i + (3.153) (Mi s E) cos j For non-magnetic particles s = 0 and eq. (3.153) reduces to fs = i +

Mi uE cos 0 j

(3.154)

where is the angle between the vectors of the gravitational force and the ﬁeld gradient. When the force of gravity and the gradient of the magnetic ﬁeld are parallel, eq. (3.154) becomes fs = i +

Mi uE 0 j

(3.155)

which is equivalent to eq. (3.145). It can be seen that for non-magnetic particles, the density cut-point is equal to the apparent density of the ferroﬂuid. Particles whose densities s are smaller than the apparent density of the ferroﬂuid (s ? d ) will ﬂoat in ferroﬂuid, while particles with density greater than the apparent density of the ferroﬂuid (s A d ) will sink. Trajectories of sink and ﬂoat particles in a stationary ferroﬂuid placed in a non-homogeneous magnetic ﬁeld are shown in Fig. 3.56.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

232

Particles enter a pool of ferrofluid

Float particles Field gradient

Sink particles

Į Pool of ferrofluid

Figure 3.56: Trajectories of ﬂoat and sink particles in a stationary ferroﬂuid placed in a non-homogeneous magnetic ﬁeld.

Figure 3.57: The eect of hydrodynamic drag on cut-point density, for two particle velocities. The nominal "large-particle" (eq. 3.155) cut-point density fs = 3500 kg/m3 .

3.8. SEPARATION IN MAGNETIC FLUIDS

233

Figure 3.58: The inaccuracy in cut-point density introduced by ignoring hydrodynamic drag, for two dierent particle velocities. The nominal cut-point density fs = 3500 kg/m3 .

3.8.3

The eect of the hydrodynamic drag

In many applications of ferrohydrostatic separation it is legitimate to ignore the eect of the hydrodynamic drag. For small particles, however, the inﬂuence of the drag on the cut-point density can be signiﬁcant. If we assume that the Stokes law applies, the hydrodynamic drag is given by eq. (1.16). By including this drag in the expression of the total force (eq. (3.151)), the equilibrium of forces on a non-magnetic particle yields fs = i +

Mi 9y uE + 0 j 2je2

(3.156)

Equation (3.156) applies to a particle that is moving vertically downwards, i.e. the hydrodynamic drag Isg (1) acts on the particle. Such a particle is either a sink particle, i.e. a particle whose density is greater than d , or a ﬂoat particle that is temporarily moving downwards because of the non-zero initial velocity with which it entered the ﬂuid, as shown in Fig. 3.56. Once a ﬂoat particle reaches its terminal velocity (equal to zero), it will reverse the direction of its motion and will start moving upwards. At that point the opposite hydrodynamic drag Isg (2) will be acting on the particle and the particle will experience an apparent density given by d = i +

Mi 9y uE 0 j 2je2

(3.157)

234

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.59: Density increment, for paramagnetic particles, as a function of magnetic susceptibility, at three dierent values of the applied magnetic ﬁeld. uE = 2 T/m. Therefore, it becomes clear that, in general terms, the presence of the hydrodynamic drag increases the cut-point density for sinking particles, i.e. sink particles or ﬂoat particles in their initial phase of motion within the ferroﬂuid. For particles reporting to the ﬂoat fraction, however, the hydrodynamic drag decreases the cut-point density. It can be found from eq. (3.156) that for particles greater than, for example, 1 mm the hydrodynamic drag can be neglected and the cut-point density is independent of particle size, and is given by eq. (3.155). However, by inclusion of the hydrodynamic drag, the cut-point density begins to deviate, for particles smaller than 1 mm, from its "large particle value", as is illustrated in Fig. 3.57. Figure 3.58 shows the inaccuracy in the cut-point density introduced by ignoring the hydrodynamic drag.

3.8.4

The eect of particle magnetic susceptibility

A magnetic particle (s 6= 0) will exhibit an eective density hi i dierent from its natural (true) density s , as a result of its attraction (or repulsion) in the direction of the ﬁeld gradient. This eective density can be written: hi i = s +

s E uE cos 0 j

(3.158)

It can be seen that the dierence between the eective and true densities s = hi i s increases, for paramagnetic particles, with increasing magnetic

3.8. SEPARATION IN MAGNETIC FLUIDS

235

susceptibility, magnetic ﬁeld strength and the ﬁeld gradient. A relative density increment as a result of non-zero magnetic susceptibility of a particle, follows from eq. (3.158) hi i s "s E = uE (3.159) s 0 j where "s is the mass magnetic susceptibility of the particle. A typical dependence of the density increment as a function of magnetic susceptibility of paramagnetic particles is shown in Fig. 3.59. It is evident that the density increment increases with increasing magnetic susceptibility of the particle and the ﬁeld strength. This is a very important implication that aects the accuracy of separation of materials of non-zero magnetic susceptibility. On the other hand, the eective density of diamagnetic particles decreases, as a result of their negative magnetic susceptibility. In view of the low values of diamagnetic susceptibility, the density decrease is very small; at the magnetic induction of 2 T, the decrease is approximately 0.2%. For example, the eective density of quartz (" = - 6.0×109 m3 /kg) is reduced, at 2 T, from its physical density of = 2700 kg/m3 to approximately 2695 kg/m3 . The validity of eq. (3.159) has been tested using magnetic tracers, particles of constant density and of dierent values of magnetic susceptibility [R31]. Magnetic tracers, 5 mm in size, and of density 3550 kg/m3 , with mass magnetic susceptibility ranging from 2.5×107 m3 /kg (20×106 cm3 /g) to 1.25×105 m3 /kg (1000×106 cm3 /g), were separated in a ferroﬂuid the apparent density of which was varied from 3600 kg/m3 to 4200 kg/m3 . The magnetic induction to which the ferroﬂuid was exposed in the separation region was 0.2 T and the ﬁeld gradient was 1.5 T/m. Partition curves thus obtained are shown in Fig. 3.60. It can be seen that 50% of tracers with density of 3550 kg/m3 sank in a ferroﬂuid of apparent density of 3700 kg/m3 only when their susceptibility was greater than 1.25×106 m3 /kg. When the density of the ferroﬂuid was set to 4200 kg/m3 , 50% of magnetic tracers of density 3550 kg/m3 sank when their magnetic susceptibility was greater than 8.2×106 m3 /kg. This experimental observation can be compared with the theoretical prediction expressed by eq. (3.159). Using the above values of particle susceptibility, and taking into account that E = 0.2 T and uE = 1.5 T/m, the right-hand side of eq. (3.159) is equal to 0.19. This value agrees well with the relative density increment (4200 - 3550)/3550, obtained from the left-hand side of eq. (3.159).

3.8.5

Motion of particles in a ferroﬂuid

The equation of motion of non-magnetic particles The equations of motion of a non-magnetic particle suspended in a stationary ferroﬂuid, as depicted in Fig. 3.61, can be expressed [M18] as: gy{ 1 g2 { { { = (I { + Isp + Isg ) = gw2 gw s Ys se

(3.160)

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

236

Figure 3.60: The partition curves for magnetic tracers of density 3550 kg/m3 , as a function of their mass magnetic susceptibility, separated in a ferroﬂuid of dierent apparent densities [R31]. z h

Fzpmb, Fpgb

v0

Fpmb

grad B x

F

pmb

į

Fpg,

Į

x

Figure 3.61: Section through a pool of ferroﬂuid of depth , inclined at an angle =

3.8. SEPARATION IN MAGNETIC FLUIDS gy} g2 } 1 } } = (I } + Isg + Isp Ij ) = 2 gw gw s Ys se

237 (3.161)

These equations can be re-written gy{ + Ny{ = Z gw

(3.162)

gy} + Ny} = Z 0 gw

(3.163)

where parameters N> Z and Z 0 have the following forms: N=

d i d cos s + 2i sin2 (@2) 6e >Z = j sin > Z 0 = j (3.164) s Ys s s

The initial conditions for eqs. (3.162) and (3.163) are: for w = 0 y{ = 0 and y} = y0

(3.165)

The initial velocitys of a particle that is being dropped into the ferroﬂuid from height k is y0 = 2jk. Dierential equations (3.162) and (3.163) can be solved analytically and the solutions are [M18]: g{ Z (3.166) = y{ = (1 hNw ) gw N Z” g} = y} = y0 hNw + (1 hNw ) gw N

(3.167)

The initial conditions for eqs. (3.166) and (3.167) are for w = 0 { = 0 and } =

(3.168)

Equations (3.166) and (3.167), with these initial conditions, yield the following solutions: Z Z (3.169) w 2 (1 hNw ) {= N N } =+(

Z0 y0 Z ” 2 )(1 hNw ) + w N N N

(3.170)

Particle trajectories can be obtained from these parametric equations by calculating pairs of coordinates ({> }). Typical trajectories of non-magnetic particles of dierent densities are shown in Fig. 3.62. It can be seen that when k = 0 then y0 = 0 and the trajectory of a particle is a straight line.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

238

z (cm)

10 3300 3400

5

3500 3600

x (cm)

0 0

5

10

15

20

-5

Figure 3.62: Trajectories of non-magnetic particles of various densities: d = 3500 kg/m3 , k = 3 mm, i = 990 kg/m3 , = 1.65×103 Pa×s, = 20 . The straight dashed lines are trajectories of particles of densities of 3500 kg/m3 and 3550 kg/m3 for k = 0 (adapted from [M18]).

z (cm)

10

0

5

40 60 70

0 0

5

10

15

x (cm) -5

Figure 3.63: Trajectories of magnetic particles of various mass magnetic susceptibilities (×108 m3 /kg): d = 3500 kg/m3 , s = 3300 kg/m3 (adapted from [M18]).

3.8. SEPARATION IN MAGNETIC FLUIDS Repulsion

Attraction

N

N

239

S

S

N

S

N

Particle

Magnetic fluid

S

Magnet

Figure 3.64: Interaction between non-magnetic particles in a magnetized magnetic ﬂuid (adapted from Fujita et al. [F14]). The equation of motion of a magnetic particle As has been discussed in Section 3.8.4, a magnetic particle suspended in a ferroﬂuid placed in a non-homogeneous magnetic ﬁeld will exhibit an eective density hi i (given by eq. (3.158)) dierent from its natural density. Trajectories of magnetic particles can be obtained by replacing the natural density s of the particles by eective density. As a result of the non-uniformity of the magnetic ﬁeld, the eective density is dierent at dierent positions of the particle along the vertical axis, being the greatest where the pole tips of the magnet are closest to one another, as shown in Fig. 3.52. The mean eective density can be calculated, for example, by replacing E in eq. (3.158) with the mean magnetic induction Emean = Emin + Emax . In this situation the equations of motion remain the same as parametric equations (3.169) and (3.170). Typical trajectories of magnetic particles are shown in Fig. 3.63. Interaction of particles during separation The analysis of the particle motion in a ferroﬂuid assumed that particles were non-interacting. This simpliﬁcation ignores, however, the fact that non-magnetic particles suspended in a magnetic ﬂuid possess surface magnetic charges as a result of magnetization of the surrounding ﬂuid. Fujita and Mamiya [F14] determined, theoretically and experimentally, that non-magnetic particles, placed in a magnetized ferroﬂuid, attracted one another in the direction parallel to the direction of magnetic ﬁeld and repelled one another in the perpendicular direction. The situation is depicted in Fig. 3.64. The attractive force increases with increasing density of the ferroﬂuid and magnetic ﬁeld strength. The attractive interaction was found to reduce the selectivity of separation of non-magnetic particles in a magnetic ﬂuid.

240

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Magnet

Fpm

Fpmb

N Fpc

Fg

Fpd

Rotating ferrofluid

Figure 3.65: Forces acting on a particle in a rotating ferroﬂuid in a nonhomogeneous external magnetic ﬁeld.

3.8.6

Separation in a rotating ferroﬂuid

In order to overcome certain practical limitations of gravity-based ferrohydrostatic separation, particularly treatment of ﬁne particles, several proposals were made [R11, A14, W7] to replace the force of gravity by the centrifugal force. Work carried out at Intermagnetic Corp.(USA) in early nineteen eighties resulted in a new rotation-based separation process called Magstream. The theory and the practice of separation in a rotating ferroﬂuid have been described in several publications [W20, W21, W22, B22, B23, S44]. Forces acting on a particle suspended in a rotating ferroﬂuid exposed to a non-homogeneous magnetic ﬁeld are illustrated in Fig. 3.65. Walker and Devernoe [W22] assumed that the axis of the separator was vertical and ignored the force of gravity and the hydrodynamic drag acting on the particle. In this scenario only the radially outward centrifugal force Isf , magnetic traction force Isp and the inward buoyancy force Ispe resulting from the outward attraction of the magnetic ﬂuid by the magnetic ﬁeld were included. The centrifugal force can be written Isf = Ys (s i )$ 2 u

(3.171)

where u is the radial position of the particle and $ is the rotational velocity of the ferroﬂuid. The magnetic buoyancy force is given by eq. (3.150) while the magnetic traction force is given by eq. (3.148). The total force Isu acting on a particle in the horizontal direction, along the

3.8. SEPARATION IN MAGNETIC FLUIDS

241

radius of the rotating device, can be expressed as: Isu = Ys (s i )$ 2 u +

1 1 s Ys EuE Ys Mi uE 0 0

(3.172)

In equilibrium Isu = 0 and the cut-point density for non-magnetic particles (s = 0) can be determined from the above equation as: µ fs = i +

N Q

¶2 Mi uE

(3.173)

where Q is the number of revolutions of the rotating device per minute (Q = 60$/2), and N is a parameter determined by the design of the magnetic system of the rotating separator: µ N = 15

1 107 3 u

¶[email protected] (3.174)

Equation (3.173) is used to calculate the operating conditions in the Magstream separator [W22]. It is apparent from eqs. (3.173) and (3.174) that if the pattern of the magnetic ﬁeld is designed in such a way that the ﬁeld gradient is a linear function of the radial position u, then N = const. and the cut-point density is determined solely by the polarization and the rotational velocity of the ferroﬂuid. This condition is satisﬁed, for instance, for the magnetic ﬁeld generated by a sextupole magnet, such that the ﬁeld magnitude is given by E = E0 ([email protected] )q1 , where 2q = 6, and E0 is the magnetic induction at u0 , the outside wall of the separation annulus [W20]. Equation (3.173) is equivalent to eq. (3.154) derived for ferrohydrostatic separation. It can, therefore, be seen that the cut-point density in a rotating ferroﬂuid can be controlled, in a wide range, by varying the rotational velocity and the ﬁeld gradient. The operating density range of the ﬂuid in a ferrohydrostatic separator is, in contrast, controlled by adjusting the ﬁeld gradient only. However, in most Magstream models the magnetic ﬁeld is generated by permanent magnets and the ﬁeld gradient is given by the design of the magnetic system. For instance, in Magstream Model 200 the ﬁeld gradient is equal to uE = 13.2u T/m (1320u G/cm). Simplifying assumptions introduced by Walker and Devernoe [W22], when deriving eq. (3.173), reﬂect themselves in limited accuracy of determination of the cut-point density and thus in reduced e!ciency of separation. Bunge and Fuerstenau [B22], in order to account for the dispersion component of particle behaviour, developed a diusion model of separation. They concluded that the primary cause of non-ideal separation in a rotating ferroﬂuid is the dispersion of the settling particles. This fuzzy behaviour was ascribed to the eect of turbulence, particle shape and interparticle interactions. The model of Bunge and Fuerstenau, however, was not able to explain the dependence of the separation e!ciency on particle size and ﬂuid viscosity [B22, B23].

242

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.66: The cut-point density of non-magnetic particles in Magstream, as a function of density. u = 2.1 cm, = 5×103 Pa×s, fs (no drag) = 3130 kg/m3 (adapted from [S44]).

Svoboda [S44] included the horizontal hydrodynamic drag (eq. (1.16)) into the balance of forces and obtained, for the cut-point density,

fs = i +

1 Mi s 9ys E)uE + 2 2 ( 2 $ u 0 0 2$ e u

(3.175)

This more general expression shows that the hydrodynamic interaction of particles with the ferroﬂuid contributes to the determination of the cut-point density. The most signiﬁcant consequence of the hydrodynamic contribution is that the cut-point density depends on particle size, in contrast to eq. (3.173). It transpires from eq. (3.175) that the correction hydrodynamic term gains importance for weakly magnetic and/or highly viscous ferroﬂuids (low Mi and high ), and for small particles. In addition, the hydrodynamic term depends on the position of a particle within the separation space. The eect of particle size on the cut-point density of non-magnetic particles is illustrated in Fig. 3.66. It can be seen, for example, that a cut-point density of 3130 kg/m3 , determined by ignoring the hydrodynamic drag, is accurate down to particle size of 2 mm. For particle diameters smaller than 2 mm the relative importance of the hydrodynamic interaction steeply increases and separation becomes inaccurate.

3.9. EDDY-CURRENT SEPARATION

3.9

243

Eddy-current separation

It has been stated in Section 2.7 that when conducting particles move through a region of spatially varying magnetic ﬁeld, then an electromagnetic force, and hence eddy currents, are induced in such particles. The eddy currents are caused by time-dependent changes of the magnetic induction acting on a particle and are given by the Faraday induction law: × m = s C E u Cw

(3.176)

where m is the current density and s is the speciﬁc electrical conductivity of the particle. These eddy currents generate a magnetic ﬁeld opposed to the external magnetic ﬁeld. This opposite ﬁeld then produces a repulsive Lorentz force on a linear element gv of the conductor [S47] IO = Lgv × E

(3.177)

where L is the current carried by the conductor. This force can be made lateral to the motion of the particles and so to deﬂect them. Negligible eddy currents develop in non-conducting elements, which, therefore, experience no deﬂection. In this way it is possible to separate conducting particles from non-conducting and this method has been developed into an e!cient technique for the recovery of non-ferrous metals from streams of industrial or municipal waste. The varying magnetic ﬁelds can be generated in several ways. In linear motors, the magnetic ﬁelds are generated by electromagnets with alternating currents. The repulsive force can also be generated by moving particles through a non-homogeneous static or rotating magnetic ﬁelds. These ﬁelds can be conveniently generated by permanent magnets.

3.9.1

Static ramp eddy-current separator.

The simplest design of an eddy-current separator (ECS) proposed by Schloemann [S45] comprises a long ramp, as shown in Fig. 3.67. The ramp consists of permanent magnet strips of alternating polarity, mounted on a mild steel base plate inclined at an angle of about 450 to the ramp axis. A stream of particles is allowed to slide down the ramp. The non-conducting particles are not aected by the magnetic ﬁeld and travel straight down the ramp. The conducting particles, under the inﬂuence of the eddy-current-induced repulsive Lorentz force perpendicular to the magnet strips, are deﬂected from the stream of non-conducting particles, as shown in Fig. 3.67. The magnitude of the lateral deﬂection depends, among other things, on the electrical conductivity, density, size and shape of the particles and the strength and the periodicity of the magnetic ﬁeld.

244

CHAPTER 3. THEORY OF MAGNETIC SEPARATION Feed

Y

+ -

Magnet strips of alternating polarity

+ + -

Z

Mild steel base

ș

X Conducting particles

Non-conducting particles

Figure 3.67: Schematic diagram of a ramp eddy-current separator (adapted from Schloemann [S45]). Schloemann [S45] found that the component of the repulsive force in |direction acting on a conducting particle is given by: | IOs = ps y{

(3.178)

where ps and y{ are the mass and velocity in the { - direction of the particle, respectively. The coe!cient is a function of particle shape, and for a thin disc of diameter gs , it is given by [S45]: =

1 2 s CE} 2 ( g ) 32 s s C{

(3.179)

and approximate expression for the repulsive force (eq. (2.6)) is quoted by Schubert [S22]: s gs 2 | IOs ' ps (3.180) E y{ s 2i where i is the period of the magnetic ﬁeld. This equation, supported by additional calculations of the repulsive force on particles of various shapes [S46, V3, V4] shows that the repulsion force is a function of the material parameter s @s , given in Table 2.1, and of the square of the magnetic induction. Schloemann [S45] calculated trajectories of disc-shaped particles in a ramp eddy-current separator from the following equations of motion: gy{ gy| = j sin and = y{ gw gw

(3.181)

3.9. EDDY-CURRENT SEPARATION

245

It follows from eqs. (3.181) that {(w) =

1 2 w j sin + y0 w 2

1 1 |(w) = ( w3 j sin + y0 w2 ) 6 2 where y{ (0) = y0 . The particle trajectory, in a frictionless situation, is then: s ·³ ³ { ´[email protected] ¸ 2 {0 ´ ³ {[email protected] {0 ´[email protected] 0 |({) = + 2 1 2 1 + 3 (j sin )[email protected] { { {

(3.182) (3.183)

(3.184)

where {0 is the distance along the ramp after which a particle starting at rest has attained the velocity y0 = Therefore, {0 = y02 @2j sin . A more detailed analysis of the eect of friction on particle motion can be found in [S45]. Although ramp eddy-current separators were used in several industrial installations [S46], their commercial success was limited. Poor selectivity, particularly for small particles, and low throughput were responsible for the failure of ramp separators to ﬁnd a long-term production application. Further development of the ramp concept resulted in the design of a vertical eddy-current separator [V4, V3], in which the deﬂection occurred in a vertical channel between two arrays of magnet strips mounted on the inside of two vertical parallel mild steel plates. The strips of alternating polarity were also oriented at an angle to the base plate and, in addition, the magnets on the opposite plate were also arranged with opposite polarity. These static gravitybased separators also failed to gain industrial acceptance and were replaced by dynamic rotating drum eddy-current separators. A detailed study of the separating Lorentz force, by eliminating the competing forces such as gravity and frictional forces, was conducted theoretically by Fletcher et al. [F15, F16, F17]. These idealized physical models of separation of conducting and non-conducting elements moving in a horizontal plane and incident on a single boundary of a semi-inﬁnite magnetic ﬁeld were compared with the experimental results. Theoretical trends of the metal recovery with particle size, splitter position and boundary ﬁeld proﬁle were in good agreement with experimental observations. Although the ﬁeld geometry and the separation arrangement in these studies diered from those used in practical applications, the methodology used can serve as a starting point for more fundamental research into the mechanisms of eddy-current separation.

3.9.2

Rotating drum eddy-current separators

Presently, the eddy-current separators most frequently used in industrial practice are based on a rotating drum concept. The active part of such a separator is a drum containing rapidly rotating magnetic system. Permanent magnets are arranged, with alternating polarity, along the circumference of the magnetic system. This concept is schematically described in Figs. 2.100 and 3.68.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

246

Drum rotation Eddy current S

Belt

N

Particle S

N

S

Lorentz force N S

N Particle

Figure 3.68: A top view of an eddy-current separator based on a rotating drum. The particles are expelled by the Lorentz force in the direction of the direction of drum rotation (adapted from [R17]). In order to calculate the forces acting on particles due to eddy current, a dipole model was developed by Rem et al. [R17, R18]. It was assumed that the magnetic ﬁeld induces eddy currents within a particle, which in turn generate a magnetic moment in that particle. The interaction between the magnetic moment P and the external magnetic ﬁeld E results in eddy current forces. The force can then be expressed as: IOs = P uE

(3.185)

where P = Ps Ys . The torque on the particle is given by eq. (3.48). In order to determine the force acting on a particle, given by eq. (3.185), a magnetic ﬁeld generated by the magnetic system must be calculated. Rem et al. [R17] have shown that the components of the magnetic induction in the cylindrical coordinate system (u> !> }) relative to the drum axis can be written: Eu =

4 X

eq ([email protected] )(2q+1)n1 sin[(2q + 1)n(! $ guxp w)]

(3.186)

eq ([email protected] )(2q+1)n1 cos[(2q + 1)n(! $ guxp w)]

(3.187)

q=0

E! =

4 X q=0

where eq are the Fourier coe!cients, Uguxp the radius of the drum, n the number of pairs of the magnets used in the drum and $ guxp the angular velocity of the drum. The Fourier coe!cients can be determined by measuring the magnetic ﬁeld strength as a function of distance from the magnetic pole surface. Based on eqs. (3.186) and (3.187), Zhang et al. [Z4] obtained the following expressions for the tangential Isw and radial Isu eddy-current forces acting on the particle: (n$ guxp + ) 2vYs E2 (3.188) IOsw = 0 z 1 + (n$ guxp + )2 2

3.9. EDDY-CURRENT SEPARATION IOsu =

2vYs (n$ guxp + )2 2 E2 0 z 1 + (n$ guxp + )2 2

247 (3.189)

where z is the width of one pair of magnets, v is the shape factor of the particle and is the angular velocity of particle rotation. is a characteristic time with which the induced magnetic ﬁeld decays in the particle given by [Z4]: = 0 s ve2

(3.190)

where e is the particle radius. The torque on the particle was found to be [Z4]: W =

vYs (n$ guxp + ) E2 0 1 + (n$ guxp + )2 2

(3.191)

It can be seen that the eddy-current forces and the torque depend on the square of the magnetic ﬁeld strength. By replacing ceramic ferrite permanent magnets by rare-earth magnets, a considerable increase in the separating force can be, therefore, achieved. Competing forces Gravitational, centrifugal, frictional and aerodynamic forces compete with eddycurrent forces and their relationship determines the particle trajectories in an eddy-current separator. Eddy current forces and a wide spectrum of competing forces and their various dependencies on particle size and shape, electrical conductivity, magnetic ﬁeld strength and its frequency (or the angular velocity of the rotating drum) make the determination of particle trajectories and thus the e!ciency of separation a problem of considerable complexity. Only rudimentary eorts have been made the develop the balance of forces in a rotating drum eddy-current separator [Z4, R17, R18]. Rem et al. [R18] developed a model for simulation of such a rotating drum ECS. The eddy-current forces and some of the competing forces were included in the model and particle trajectories were calculated. Typical trajectories, shown in Figs. 3.69 and 3.70, comprise the rolling, sliding and ﬁnally ﬂying stages. It can be seen that at low belt velocities (Fig. 3.70) light particles tend to lose contact with the belt at an early stage and they collide with the belt at a later stage. As a result of the dependence of the eddy-current forces and other forces on the cube of the particle size, the particle size is the most signiﬁcant variable aecting the performance of a separator. It transpires from the above equations that also the particle shape plays an important role in the separation process. For instance, it was observed that ﬂat particles exhibit much greater displacement by eddy-current forces than spherical particles. In spite of considerable complexity of the process, some general rules that govern the e!ciency of separation in a drum ECS can be formulated. In order to achieve a high recovery of conducting particles, the eddy-current separating force must be greater than

248

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.69: Particle trajectories in a rotating drum ECS. Three stages of particle motion, namely rolling, sliding and ﬂying are apparent. Operating conditions: belt speed: 1.5 m/s, drum angular velocity: 35 s1 , material: aluminium particles 15 mm in diameter, 45 mm long (courtesy of P.C. Rem).

Figure 3.70: Particle trajectories in a rotating drum ECS, at low belt velocity. Belt speed: 0.5 m/s, drum angular velocity: 35 s1 , material: aluminium particles of diameter of 10 mm, 2 mm thick (courtesy of P.C. Rem).

3.9. EDDY-CURRENT SEPARATION

249

Figure 3.71: Frequencies required to rotate metal particles of various diameters (adapted from Allen [A21]). the sum of the competing forces: Ivhsdu A Ifrps

(3.192)

If, however, Ivhsdu AA Ifrp , selectivity of separation will be low, as no distinction will be made between various classes of conducting particles. Selective separation of one metal from another is determined by the interplay between corresponding eddy-current and competing forces. Selective separation of metal (1) from metal (2) will be achieved when the following relationship is met: (1) (2) Ivhsdu A Ifrps A Ivhsdu

(3.193)

However, when Ivhsdu ? Ifrps , no separation based on the characteristic property, such as electrical conductivity in ECS, will take place.

3.9.3

Eddy-current separation by particle rotation

With decreasing particle size, the torque on the particle become an important separating force. Also, when the particle size becomes much smaller than the width of the magnet strips used in the rotating drum eddy-current separators, the particles increasingly respond to the ﬁeld changes by rotation rather than by repulsion [A21]. As a result of decrease in the particle throw and increase of particle rotation as particle size decreases, Allen [A21, A22] proposed to use particle rotation as the separating mechanism of conducting particles.

250

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Allen found that the magnitude of the torque acting on a cubic conducting particle by a rotating ﬁeld is Wf =

E 2 O5 z 8(s

(3.194)

where O is the length of the cube edge, z is the magnetic ﬁeld rotation frequency and (s is the resistivity of the material. For a sphere of diameter gs , the torque is given by E 2 g5s z (3.195) Wf = 60(s If such a torque is exerted on a particle by a rotating magnetic ﬁeld, and the particle is resting on a surface, the particle will be rolled when the torque becomes greater than the gravitational force holding the particle against the surface. The gravitational torque preventing a cubic-shaped particle from rolling can be written: O4 Wj = (3.196) j 2 s Combining eqs. (3.195) and (3.196) an estimate of the minimum size of a cubic particle that could be rolled at a given magnetic ﬁeld strength is obtained [A21]: Omin =

4s (s j E 2 z

(3.197)

Equation (3.197) gives a reasonable estimate of the minimum size of a ”rollable” cubic particle when the rotating magnetic ﬁeld has its rotation axis at the centre of the particle. In a more practical situation of a rotating drum eddy-current separator, the magnetic ﬁeld not only rotates the particle, but it is also moving through the particle. This moving ﬁeld produces a ﬁeld which rotates in the opposite direction, at half the ﬁeld rotation frequency [A21]. The minimum ”rollable” cubic particle size, ignoring inter-particle interactions, can, therefore, be estimated as 8s (s j Omin = (3.198) E 2 z The rotating frequencies of the magnetic ﬁeld, required to rotate and thus to separate particles of various metals and various sizes in a magnetic ﬁeld of 0.45 T, are shown in Fig. 3.71 [A21]. It can be seen, for example, that particles of gold, as small as 60 m, could be separated by rotating them at the frequency of 1000 s1 = The concept has been demonstrated by separating aluminium particles from their mixture with sand, with the recovery of 86% and the concentrate grade of 95 % Al, at the feed rate of 5 t/h/m [A17].

Chapter 4

Elements of Design of Magnetic Separation Equipment 4.1

Introduction

The design of a magnetic circuit for a magnetic separator is based on the need to optimize the magnetic force required to separate e!ciently, and selectively, particles of dierent magnetic susceptibilities. As transpires from eq. (1.8), the magnetic force is the product of the magnetic ﬁeld strength and of the ﬁeld gradient. The desired magnetic ﬁeld strength, the ﬁeld gradient and their combination are a function of the type of material to be separated, mode of separation, required metallurgical performance and economic criteria. In this chapter the basic design criteria and techniques of the generation of the magnetic ﬁeld and its gradient, as used in magnetic separation, will be reviewed. Magnetic circuit design has been traditionally di!cult because of the usual non-analytic nature of the solutions for ﬁelds emanating from arbitrary sources. Further, unlike currents in electric circuits, magnetic ﬂux is not conﬁned to the wires but passes through various components of the circuit, including the air. Over the years, several analytical techniques have been used to give approximate solutions to magnetic design problems. In the simplest cases, the analytical solution can be exact, but in general for any practical problem, analytical solutions lead to large errors. Most designs are optimized by measurement and extrapolation, and experience of working with a particular type of a magnetic circuit is important. The advent of powerful computational techniques, such as ﬁnite element analysis, allows us to ﬁnd accurate solutions for two- or three-dimensional ﬁeld distributions in complex geometries, which in turn may be used to predict device performance with similar precision. However, these modelling techniques 251

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

252

require a detailed deﬁnition of the geometry and boundary conditions to be solved, which assumes that an initial design already exists. While providing an accurate ﬁeld solution for a given geometry, these techniques will not optimize it. Suggestions for changes in dimensions, materials etc. must come from the designer. Consequently, while computer-based ﬁeld analysis is an eective tool for simulating a known device, it is too cumbersome for design optimization [C16]. Field equations Calculation of the ﬂux in a magnetic circuit is based on two Maxwell’s equations. The ﬁrst, in its dierential form is: ×K = m u

(4.1)

where m is the current density. After integrating over an arbitrary surface V we obtain the above equation in the integral form: Z Z × K) · gd = m · gd (4.2) (u V

V

Then, using Stokes’s theorem, the left-hand side of this equation can be transformed into a line integral around a closed path F, which bounds the surface V, and I Z (4.3) K · go = m · gd = L F

V

where L is the total current. This is Ampere’s circuital law: the line integral of K around a closed path is equal to the total current crossing any surface bounded by the line integral path. The left-hand side of eq. (4.3) is known as magnetomotive force or ppi . The second fundamental relationship required for a magnetic circuit design expresses the fact that ﬂux must be conserved through any closed volume, or, that the total ﬂux ﬂowing out of any volume must be zero. Therefore Z · gd = 0 or u ·E =0 E (4.4) V

Equations (4.3) and (4.4) are two basic equations used for magnetic circuit design.

4.2 4.2.1

Design of circuits with permanent magnets Basic concepts and ﬁgures of merit

The general relationship between magnetic induction and intrinsic material magnetization or polarization is given by = 0 (K +P ) = 0 K + M E

(4.5)

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS B

253

B

Jr,Br

(BH)max

BH

Hc

H Hci i

(BH) max

(BH)max

Figure 4.1: The maximum energy products of permanent magnets. The relationship between E and K is illustrated by the hysteresis curve shown in Fig. 1.7. The second (demagnetization) quadrant of such a hysteresis curve is important for description of the quality of a permanent magnet material. Relative contributions of M and K greatly inﬂuence the magnetizing, demagnetizing and stability properties of permanent magnets. For instance, the coercive force Kf can never exceed the remanent magnetic induction Eu : 0 Kf Eu

(4.6)

while the intrinsic coercive force Kfl is not under such a restraint. There is clearly one point between Eu and Kf for which the product of E and K has a maximum value. The optimum operation of a magnet corresponds to conditions under which this EK product is maximum. This maximum value of the energy product is given by (EK)lim max =

Mv2 P2 = 0 v 4r 4

(4.7)

where Mv (or Pv ) is the saturation polarization (or magnetization) of the magnet material. It transpires from this equation that, in order to establish the maximum capability of a permanent magnet, one has to know only the value of the saturation polarization. The maximum value of the energy product corresponds to the largest rectangle which can be drawn under the demagnetization curve corresponding to the magnetic induction, as shown in Fig. 4.1. Another important ﬁgure of merit is the intrinsic energy product (EK)lmax . This quantity is of importance when the magnet is subjected to large demagnetizing inﬂuences in its operating environment. The maximum intrinsic energy product corresponds to the largest rectangle that can be drawn under the demagnetization curve

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

254

Table 4.1: Relative permeabilities of permanent magnet materials. Material Alnico 6 Ferrimag 5 NdFeB

Permeability 4.2 1.06 1.08 - 1.1

µ1

N Alnico

µ2

S

µ2>>µ1

S

N Ferrite or NdFeB

µ2 ≅ µ1

Figure 4.2: Flux leakage in two dierent types of permanent magnets.

corresponding to the material polarization. The situation is depicted again in Fig. 4.1. Dierent types of permanent magnets can dier considerably in their magnetic behaviour. For instance, the two energy products of an Alnico magnet are very similar, namely (EK)lmax = (EK)max , while for ferrite and rare-earth magnets (EK)lmax AA (EK)max = The permeability of Alnico magnets diers considerably from that of the air, namely pdwhuldo A dlu , while for ferrite and rare earth magnets these permeabilities are similar, so that pdwhuldo = dlu . Typical values of magnetic permeabilities are shown in Table 4.1. As a result of the above dierences, the patterns of the magnetic ﬂux around a magnet also dier. As is shown in Fig. 4.2, the ﬂux lines in Alnico magnets leave the magnet limb perpendicularly, since the poles of the magnet are not at the terminals, but appear to be spaced at about 0.7 of the length of the bar [P4]. On the other hand, in ferrite and rare-earth magnets the ﬂux lines tend to reach the terminal and the pole spacing is, therefore, the full length of the bar. In a long bar of Alnico 5, only 45% of the lines in the neutral section of the magnet reach the end of the bar. Therefore, a high percentage of the total energy is

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

Ag

255

Iron pole-pieces

Lg

Lm

Am

Permanent magnet

Figure 4.3: Magnetic circuit with a permanent magnet. stored in leakage ﬁelds. On the other hand, in a ferrite bar approximately 95% of the ﬂux at the neutral section reaches the end of the magnet. These magnets, therefore, store most of their energy within their volume and their useful energy approaches (EK)max [P4].

4.2.2

The static gap design

In a circuit with permanent magnets there are no currents, L = 0, and eq. (4.3) reduces to I · go = 0 K (4.8) In a simple magnetic circuit of Fig. 4.3, with a permanent magnet and an air gap, under static conditions, in which the dimensions of the air gap are constant, eq. (4.8) can be re—written Z Z · go + · go = 0 K K (4.9) jds

pdjqhw

Therefore, the sum of the magnetomotive force (mmf) in the magnet and the magnetomotive force in the air gap equals zero: Kj Oj + Kp Op = 0 or Kj Oj = Kp Op

(4.10)

assuming that the soft-iron parts have inﬁnite magnetic permeability. Also, because the ﬂux is continuous Ej Dj = Ep Dp

(4.11)

256

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

In the above equations Oj , Dj and Ej are the length, cross-sectional area and the magnetic induction of the air gap, respectively, while Op , Dp and Ep are the length, cross-sectional area and magnetic induction of the magnet. It can be seen from eq. (4.9) that the magnetomotive force inside the magnet is in the opposite direction to the magnetomotive force in the air gap. Permanent magnets thus operate in the top left-hand quadrant (demagnetization quadrant) of the hysteresis curve. By multiplying eq. (4.10) by eq. (4.11) we get Kj Ej Yj = Kp Ep Yp

(4.12)

where Yj and Yp are the volumes of the gap and magnet, respectively. This equation can be re-written as 1 2 E Yj = Kp Ep Yp 0 j

(4.13)

These equations illustrate that the larger the product Kp Ep and/or the volume of the magnet, the greater the magnetic induction in the air gap. It is also possible to determine, from the above equation, the volume of the magnet required to generate a desired ﬂux density in a given air gap: Yp =

Ej2 Yj 0 Kp Ep

(4.14)

By combining eqs. (4.12) and (4.13) we can also write Ep Dj Op Op = 0 = Sj Kp Dp Oj Dp

(4.15)

where Sj = 0 Dj @Oj is the so-called permeance of the air gap, while the permeance of the magnet can be deﬁned as Sp = 0 Dp @Op . Permeance is a measure of magnetic conductance which, if known, enables an accurate prediction to be made concerning how much of the total ﬂux of a magnet will reach the air gap. The reciprocal of permeance is called reluctance, = [email protected] . It can be seen from eq. (4.15) that by increasing the air-gap area and/or reducing the air gap length the ease with which ﬂux travels across this gap will increase. Equation (4.15) can be plotted as a straight line with a negative slope on a demagnetization curve. The intersection of this so-called load line with the demagnetization curve represents the operating point of the magnet, as shown in Fig. 4.4. The slope of the load line is equal to 0 Dj Op @Dp Oj = For a very small air gap, in the limit Oj $ 0> the magnet is short-circuited and Ep @0 Kp $ 4> as shown in Fig. 4.4. In the opposite case, if the soft iron pole pieces are removed and the magnet stands alone, the air gap becomes large and the magnet operates in the open circuit regime. The optimum operation of the magnet is obtained when the working point on the demagnetization curve corresponds to the maximum value of the product (EK), as illustrated in Fig. 4.1.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

Load line

257

Bm

Operating point

Open circuit

Hm Figure 4.4: The load lines of permanent magnets operating in dierent regimes.

4.2.3

Leakage factors

In all practical situations the pole pieces will have ﬁnite magnetic permeability and even more importantly, there will be a considerable leakage of the magnetic ﬂux. Allowance for these imperfections can be made by introducing correction factors N1 (leakage coe!cient) and N2 (loss factor) [P4]: N1 =

Total ﬂux in circuit Useful ﬂux + Leakage ﬂux = Useful ﬂux Useful ﬂux N2 =

magnet mmf useful mmf

(4.16)

(4.17)

The equation for the load line then becomes N1 Dj Op Ep = 0 Kp N2 Dp Oj

(4.18)

It is of interest to note that the Ep @Kp ratio is entirely determined by the physical relationships between the permanent magnet and the entire magnetic circuit within which it functions. This ratio is independent of the material from which the magnet is made. Although the correction factor N1 is rarely smaller than 2 and has no upper limit, for reasonably e!cient permanent magnets it is in the range from 2 to 3. The loss factor N2 is generally much smaller than N1 , usually within the range 1.05 to 1.45 [H18].

258

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Dynamic operation If the magnetic circuit geometry does not remain unaltered, then the load line slope in eq. (4.18) will change through any of the parameters Oj , Dj , N1 and N2 = The operating point of the magnet may undergo an excursion within the short and open-circuit limits shown in Fig. 4.4. A portion of the ﬂux changes from the leakage paths to the useful paths and back again, as the useful permeance is changed. The operation of a lifting magnet is a typical situation in which the magnetic system undergoes dynamic changes.

4.2.4

Determination of permeance and leakage factors

The primary requirement for magnetic circuit design, and therefore the design of the basic magnet used in the circuit, is to be able to calculate the relationships between ﬂux paths. As pointed out in the previous section, the easiest approach to such calculations is by means of permeances. In general, the permeance of the ﬂux paths varies from a minimum near the neutral section of the magnet to a maximum for zones at the end of the magnet or close to the air gap. Relatively simple formulae for various circuit geometries are available in the literature [T6, P4, M19, H18, M20]. Adding the gap and leakage permeances using these relationships is one of the methods of estimating the total permeance. For instance, permeance of the air gap between rectangular surfaces of width d and thickness e (Fig. 4.5) is given by S =

0 de Oj

(4.19)

This equation is a special case of a more general expression S =

0 Dj Oj

(4.20)

which is valid for any shape of the air gap. The leakage permeance of the geometry shown in Fig. 4.5 is given by an approximate formula [H18] S =

0 d 2e + 1) ln( Oj

(4.21)

In order to demonstrate the di!culties facing a designer, Parker and Studders [P12] quote, for the same geometry, another formula that leads to values of S about 20% to 30% higher. For a bar magnet that operates in the open-circuit mode, the permeance is the permeance from one limb of the magnet to the other, since there are no pole pieces or a well-deﬁned air gap. Permeance of such magnets, of various shapes such as bars, rods and rings, is s S = 1=77 D (4.22)

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

259

a

Lg

b

Figure 4.5: Geometry of a magnetic circuit for calculation of the leakage permeance. where D is the cross-sectional area of the pole. This relationship is applicable to ferrite and rare-earth magnets, while for Alnico magnets the relation is s (4.23) S = 1=77 × 0=7 D This equation takes into account the fact that for Alnicos the eective spacing of the poles is only 0.7 of the total length, as shown in Section 4.2.1. It is clear that the calculation of individual permeances is very laborious and various empirical formulae have been developed for the determination of the total leakage. A very simple example of such a formula [H18] is an expression for the leakage factor N1 for a gap of length Oj between circular pole-pieces of diameter g : 7Oj N1 = 1 + (4.24) g Comprehensive sets of formulae, usually attributed to Tenzer [e.g. T6], are available in the literature [e.g. H18]. For instance, in a magnetic circuit shown in Fig. 4.6, in which the permanent magnet material is adjacent to the gap, leakage from the sides and base, which are at the same potential, can be ignored. The correction factor N1 is then given by [H18, M19]: N1 = 1 +

0=67d Oj Oj (1=1Xd )(1 + ) Dj 0=67d + Oj d

(4.25)

where Xd is the perimeter of a part shown as length d= Similar equations are available for other geometries [H18, M19].

4.2.5

Magnetic ﬁeld around a permanent magnet

The distribution of the magnetic induction at various points of magnets operating in the open-circuit regime is shown in Fig. 4.7 and Table 4.2. The long thin bar is magnetized along its long axis while the thin disc is magnetized along its short axis. The sphere is magnetized along its diameter. It is of interest to

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

260

Permanent magnet

Ag

Lg

a

Mild steel yoke

Figure 4.6: A permanent magnet circuit for the calculation of the leakage coefﬁcient.

note that a thin disc magnetized through its thickness produces no magnetic ﬂux density although the magnetic ﬁeld strength K at point C is equal to [email protected]0 . Calculation of the magnetic ﬁeld around a permanent magnet can be performed either using the pole concept or the surface current models. In the former approach a magnet is treated as having a uniform distribution of poles on the ends of the magnet. Using this assumption, magnetic induction on the } axis of a circular inﬁnitely long magnet, as a function of the distance from the

H

A

B

C

D

E

A B

C

D

E

A

C

E

Figure 4.7: Distribution of magnetic induction inside and outside magnets of various shapes.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

261

Table 4.2: Distribution of magnetic induction B inside and outside magnets of various shapes [H18]. Point A B C D E

Bar J/2 J/2 J J/2 J/2

Sphere 2J/3 2J/3 2J/3 2J/3 2J/3

Disc 0 0 0

R ș2 ș1

P

z

P

(a)

(b)

Figure 4.8: Calculation of magnetic induction on the axis of a cylindrical magnet.

magnet (Fig. 4.8), is given by 5 E} =

M 2

6

9 : }@U 9 : 91 µ : ¶ 2 [email protected] 8 7 } 1+ 2 U

(4.26)

where U is the radius of the magnetic cylinder. By symmetry, E has no components perpendicular to }= It can be seen that on the surface of the magnet (} = 0) the magnetic induction E = [email protected], as shown in Table 4.2. Numerical computations are required to determine the magnetic induction o the axis. Expressions similar eq. (4.26) can also be obtained for the components of magnetic induction generated by rectangular surfaces [M19]. A uniform solenoid of rectangular or circular cross-section with surface current density mv (A/m) is equivalent, for the purpose of calculating magnetic induction, to a bar with uniform magnetization P = mv = [email protected]0 . If a solenoid has a circular cross-section, magnetic induction E> at point S on its axis, is

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

262

z

2R

z

L

L

D

W

Figure 4.9: Deﬁnition of geometrical parameters of a cylindrical and a rectangular permanent magnets for calculation of the magnetic ﬁeld. given by

mv (4.27) (cos 1 cos 2 ) 2 It can be seen that on the surface of an inﬁnitely long solenoid (1 = 0, 2 = 900 ) E = 0 [email protected], as could have been expected. Selvaggi and Selvaggi [S48] developed mathematical equations that allow the external and internal magnetic ﬁelds of cylindrical and rectangular permanent magnets of ﬁnite dimensions to be determined. These magnets are shown schematically in Fig. 4.9. The authors assumed that the surface charge density at the poles is equal to Mu and that only two parallel faces contribute to the ﬁeld. The equation for the external ﬁeld at distance } from the face of a circular magnet of radius U and length O is ) ( Mu } }+O Eh{w = (4.28) 2 [U2 + (} + O)2 ][email protected] [U2 + } 2 ][email protected] E = 0

The equation of the internal ﬁeld, at the centre of the magnet is Elqw = {

Mu 2

O (U2 +

O2 ) 4

}

(4.29)

Clearly, for O $ 4, Elqw $ Mu . It can be seen that both terms in parentheses in eqs. (4.28) and (4.29) are dimensionless and thus any system of units can be used.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

263

Similar expressions were derived for a rectangular permanent magnet of ﬁnite dimension, as deﬁned in Fig. 4.9. The equation for the external ﬁeld is

Eh{w

; ZG A A arcsin · A ¸[email protected] A 2 A Z G2 A 2 2 A 4 ( + } )( +} ) Mu ? 4 4 = ZG A A arcsin · A ¸[email protected] A 2 A Z G2 A A 2 2 = 4 ( + (} + O) )( + (} + O) ) 4 4

while the expression for the internal ﬁeld is given by ; 5 6< A A ? @ ZG Mu 9 : Elqw = 2 arccos 7 8 2 2 2 2 A Z O G O [email protected] A = > 4[( + )( + )] 4 4 4 4

< A A A A A A A @ A A A A A A A >

(4.30)

(4.31)

Considerably more complicated expressions for the o-centre magnetic ﬁeld can also be found in [S48]. Good agreement between the measured values and those determined from eqs. (4.28) to (4.31) was found.

4.2.6

Magnetic forces

Permanent magnet circuits can be designed either for holding magnetic bodies or for attracting them. The distinction is that the holding magnet has to exert a magnetic force on a material with which it makes a good contact, while the attracting magnet has to exert a force on a magnetic body at a considerable distance. The distinction is important, because the optimum design for the two purposes diers considerably. While the attraction force is essential in many forms of magnetic separators, such as suspended magnets or wet low-intensity drum magnetic separators, in other types of separators it is the holding force that plays a decisive role. The correct compromise between holding and attracting particles from a distance must be achieved. A force between two magnetic charges T1 and T2 separated by a distance u is given by Coulomb’s magnetostatic law: T1 T2 I = u0 40 u2

(4.32)

where u0 is the unit vector in the direction of u= For a thin cylindrical magnet T = MD where M is the magnetic polarization and D is the cross-sectional area of the magnet. We can then write, for semi-ﬁnite magnetic bars of the same cross-sectional area D 1 I = Md Me D2u0 (4.33) 40 u2

264

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

where Md and Me are magnetic polarizations of bars d and e, respectively. When these bars are in contact, eq. (4.33) reduces to: I =

1 Md Me D 20

(4.34)

As an example, magnetic polarization of 1 T produces a pull of 40 N/cm2 , or approximately 4 kg/cm2 , while 0.2 T creates a pull of a mere 0.16 kg/cm2 . Equation (4.34) is often simpliﬁed even further, under the assumption Md = Me = E> into the form 1 2 I = E D (4.35) 20 which is incorrect in many instances [M19]. For instance, if Me = 0, then correctly I = 0> according to eq. (4.34). The simpliﬁed formula would incorrectly yield I = Md2 [email protected]0 . Generally, eq. (4.35) is valid only when bars d and e are of the same material and when there is no source of external magnetic ﬁeld. It is obvious from eqs. (4.34) and (4.35) that the holding force is proportional to the square of ﬂux density and only to the ﬁrst power of the magnet area. By using tapered soft-iron pole-tips it is possible to concentrate the ﬂux to a higher density than the magnets themselves can provide. Although the cross-sectional area of the magnet would decrease somewhat, the holding force will increase nevertheless. Although by increasing the magnetic ﬂux it is possible to increase the holding force for zero air gap, the reach of the magnetic force would decrease once the air gap is introduced. The force of attraction would thus decrease. Therefore, in those magnetic separators in which a pull at a distance (traction force) is important, wide pole-pieces working at a low induction and allowing high force penetration into the air gap, are required. On the other hand, closely spaced poles that produce high holding force are incorporated into those magnetic separators that rely on the holding force rather than traction force. Dry drum and roll magnetic separators are an example of such machines.

4.2.7

Soft iron components of the magnetic circuits

Pole-pieces of a solid or laminated soft iron or mild steel , or occasionally cobaltiron, are an essential part of magnet design. These ﬂux-conducting members are used to complete a return path for the ﬂux and to concentrate or change the ﬂux density in a circuit. Cost is usually an important factor in the choice and majority of magnetic circuits use ordinary cold-rolled steel for these components. Cobalt-iron alloy is used in some high-performance circuits. It is a good practice to operate these materials near their maximum permeability, as shown in Fig. 1.9. This will ensure the maximum ﬂux-carrying capacity of the circuit. Magnetization curves for some high-permeability materials is shown in Fig. 4.10. Relative position of permanent magnets and mild steel components is also of signiﬁcant importance. Figure 4.11 illustrates three possible arrangements

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

265

Figure 4.10: Magnetization curves for several high-permeability materials.

Three positions of permanent magnets in a circuit

(a)

(b)

(c )

Figure 4.11: Three arrangements of a circuit with permanent magnets.

266

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Table 4.3: Reversible temperature coe!cients of permanent magnetic materials. Material Ferrite SmCo5 NdFeB

(Bu ) [%/0 C] - 0.20 - 0.04 - 0.12

(Hfl ) [%/0 C] + 0.40 - 0.30 - 0.60

of a circuit with permanent magnets. Arrangement (a) is the least e!cient as the leakage between the circuit elements is very high. On the other hand, arrangement (c) is the most e!cient as a result of low leakage. Analysis of these circuits with an Alnico 5 magnet showed that the ratio of the gap ﬂux to the total ﬂux in the arrangement (c) is three times higher than in arrangement (a) [P12]. It is clear that permanent magnets should be placed as close to the air gap as possible. A valuable advantage can be obtained by placing a magnet, magnetized through its thickness, on a ferromagnetic plate. Then the magnet behaves like one of twice its thickness.

4.2.8

Stability of permanent magnets

Permanent magnets are expected to maintain a constant ﬂux output over a long period of time, although any magnet, after being fully magnetized, is likely to lose strength slowly with time. In nearly all applications the magnet is subject to inﬂuences that tend to alter the magnet ﬂux. However, in contrast to early permanent magnets, the modern materials exhibit remarkable stability, sometimes as high as 106 . Reversible changes The magnetization changes fall into two classes, namely reversible changes and irreversible changes. The reversible changes in the magnetic properties, as a function of temperature, originate in the change in spontaneous magnetization. Reversible changes are functions of temperature and circuit loading and are time-independent. They disappear completely without need for remagnetization when the permanent magnet is returned to its initial temperature. Figure 4.12 illustrates the dependence of the remanent magnetization on temperature for three types of permanent magnet materials. The reversible changes resulting from temperature changes can be represented by temperature coe!cients, expressed as a percentage change in M or E per 0 C. A summary of the temperature coe!cients of Eu and Kfl for several permanent magnet materials is given in Table 4.3. In addition, Table 1.18 summarizes the Curie temperatures and maximum operating temperatures of various permanent magnet materials. In many instances the temperature coe!cients of magnetization and coercive force do not give enough information about how a magnet will respond to temperature changes. Changes in the shape of a demagnetization curve and the

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

267

Figure 4.12: Temperature dependence of remanent magnetization of various permanent magnetic materials (adapted from [P4]). position of the load line and the working point can only be seen from a complete set of demagnetization curves, measured at dierent temperatures. Figures 4.13 and 4.14 illustrate families of demagnetization curves at various temperatures for ferrite and NdFeB permanent magnets. Such curves are useful for graphical design of magnets operating under various temperature conditions. Complete sets of such demagnetization curves are available either in the literature (e.g. [P4]) or the most recent data can be obtained directly from magnet manufacturers. Irreversible changes In the case of irreversible changes, after the removal of the disturbing inﬂuence, the magnetization does not return to its original value. In certain types of changes however, the magnetization can be fully restored by re-magnetization. Such changes are, for instance, ambient temperature changes and exposure to an external magnetic ﬁeld. Upon exposure to an external ﬁeld, the operating point moves down the demagnetization curve and the intrinsic magnetization of the magnet shows a corresponding change. When the external ﬁeld is removed, the magnetization recovers only partially. This loss is recoverable by re-magnetization. The loss will be greater when a magnet is operating in the steepest part of the demagnetization curve. Although mechanical shock and vibration contribute energy to a permanent magnet, changing its magnetization, modern materials with high coercive forces seem to be resistant to changes by mechanical eects. At the same time, however, ﬁeld exposure is not able to completely eliminate changes that might have occurred.

268

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.13: Demagnetization curves of a ferrite magnet at dierent temperatures.

Figure 4.14: Demagnetization curves of an NdFeB magnet at various temperatures.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

269

Table 4.4: Magnetic induction required to magnetize permanent magnet materials. Material Alnico 5 Alnico 8 Ferrite RECo5 NdFeB

Bvdw [T] 0.3 0.8 1.0 2.0 to 3.0 2.5 to 3.0

While Alnico and ferrite magnets are stable and not subject to corrosion, rare-earth magnets have oxidation problems that limit their maximum operating temperature. If no coating is provided for protection, oxygen diuses into such a magnet, causing a metallurgical change in a surface layer. The surface layer will have a lower Kfl , which will allows this region of the magnet to be demagnetized more easily. Surface oxidation thus leads irreversibly to a reduction in the magnetic properties. Irreversible changes, resulting from permanent changes in the structural or metallurgical state, are usually time-dependent and re-magnetization does not restore the original state of magnetization. The temperature at which changes in properties ﬁrst become noticeable corresponds to the maximum operating temperature. Temperature-induced irreversible losses in permanent magnets are shown in Table 1.17.

4.2.9

Magnetization of permanent magnets

It is generally accepted that to magnetize a permanent magnet to saturation, an external magnetic ﬁeld three to ﬁve times its intrinsic coercivity Kfl must be applied. Typical values of the magnetic induction required to magnetize various permanent magnet materials are summarized in Table 4.4. Simple bar or ring-shaped magnets may be magnetized by a larger permanent magnet, a solenoid or an electromagnet. To magnetize rare-earth magnets, very high ﬁelds are required and magnetization is often performed with small coils or solenoids energized by large current pulses of short duration. Large magnets cannot be magnetized by a pulse of short duration, because eddy currents prevent the ﬂux reaching the centre of the magnet. In general, the frequency i of the pulse must be chosen so that the magnetizing pulse lasts longer than the eddy current. The depth of penetration, or the skin depth , is given by µ ¶[email protected] ( = (4.36) 0 i where ( is the resistivity of the material. Resistivity plays a very important role since most permanent magnets have very low permeabilities . Ceramic ferrite magnets have high resistivity ( A 104 m and full penetration of a pulse is easy. On the other hand, Alnico and

270

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Pole

Coil

B

A

Lg Pole-piece

C Path of integration

Yoke

Figure 4.15: Schematic diagram of an electromagnet with iron yoke. rare-earth magnets, with ( 100×108 m, pose a problem and a pulse width of at least 10 ms must be used [P4].

4.3

Design of iron-core electromagnets

In section 1.7.2 the position of electromagnets with an iron yoke as a source of magnetic ﬁeld in magnetic separation was outlined. Although the iron-core electromagnets have been recently replaced by rare-earth permanent magnets in several types of magnetic separators, they still play an important role in various designs of magnetic separators. In those applications where variable magnetic ﬁeld of moderate strength in a relatively large volume is required, electromagnets with an iron yoke are the ﬁeld source of choice. In spite of availability of powerful modelling techniques for optimization of electromagnet design, the initial design ought to be created based on experience and, to some degree, on guesswork. In this section general principles of design of electromagnetic circuits with an iron core will be described. The design of such a circuit, schematically shown in Fig. 4.15, is governed by Ampere’s law given by eq. (4.3). If we suppose that coils with a total number of turns Q are wound onto the circuit, then Ampere’s law can be re-written as I · go = Q L K (4.37) F

The path of integration extends around the magnetic circuit as shown in Fig. 4.15. The magnetic induction Ej in the air gap of length Oj is, therefore, given by Z Ej = 0 (Q L Kgo) (4.38) Oj EFD

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

271

By calculating the actual ﬁeld E inside the iron part of the circuit, we can then determine the magnetic induction in the air gap from the value of the magnetomotive force (or number of ampere-turns) Q L= We can deﬁne reluctances of the air gap j and of the iron part of the circuit p as Oj (4.39) j = 0 Dj Z 1 go (4.40) p = EFD Dp where Dj and Dp are cross-sectional areas of the air gap and iron and is the permeability of iron. If the magnetization of the iron is much less than saturation, then AA 0 and j AA p = Then we have E0 = 0

QL Oj

(4.41)

This equation expresses a linear relationship between E0 and L, which is observed for any type of electromagnet at low magnetic ﬁelds. If, however, the magnetization of the iron approaches saturation, the permeability of the iron is greatly reduced. Under these conditions eq. (4.41) is not valid and we must use the following, more general equation to calculate Ej Ej =

QL (j + p )Dj

(4.42)

For this purpose we must calculate p from eq. (4.40), which is a di!cult task as we have no straightforward way of determining the value of as a function of position o= Furthermore, the leakage of the ﬂux will increase as becomes small [I1].

4.3.1

Calculation of the magnetic ﬁeld

The magnetic ﬁeld produced in an air gap of an electromagnet can be calculated by integrating contributions of the magnetic charges on the pole surface. For cylindrical ﬂat poles, as shown in Fig. 4.16, the magnetic induction in the gap is given by [M21] · ¸ { Ej = Mv f (1 cos ) = Mv f 1 2 (4.43) (u2 + {2 )[email protected] where f is a correction factor. For tapered poles with coinciding apexes (Fig. 4.16) the magnetic induction becomes u2 Ej = Mv f (1 cos + cos sin2 ln ) = (4.44) u1 · ¸ {u12 u2 { + ln (4.45) Mv f 1 2 2 2 [email protected] 2 [email protected] u1 (u1 + { ) (u1 + { )

272

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Lp

ș r2

x

ș r1

r2

Figure 4.16: Cylindrical ﬂat poles and tapered poles with coinciding apexes. It can be seen that in this case the magnetic induction consists of two terms, the ﬁrst term being the magnetic induction for cylindrical ﬂat poles. The second term is greater than zero (provided that ? 900 and u2 A u1 ), and magnetic induction generated by tapered poles, therefore, generates a greater magnetic ﬁeld than ﬂat poles. This second term achieves its maximum for = 54.70 . It was shown by Montgomery [M21] that eq. (4.43) gives good results if f = 0=7 for 1, while for = 0=5 the correction factor f = 1 gives a good agreement between calculated and measured values of magnetic induction. is a geometrical factor deﬁned as = Os @2u2 and Os is deﬁned in Fig. 4.16. In magnets with tapered pole-pieces eq. (4.45) has very good predictive capability for f = 1.

4.3.2

Shape of iron parts of the circuit

The yoke, as shown in Fig. 4.15, serves to transport the magnetic ﬂux from the end of one pole to the end of the other pole. The presence of iron permits useful values of the magnetic induction (for example, up to 2 T) to be reached with modest investments in ampere-turns. The iron yoke also conﬁnes the stray ﬂux to the immediate vicinity of the magnet gap. The yoke should, therefore, have reasonably high permeability, even when the poles and pole pieces are saturated. Since the magnetization curve of soft iron has a knee at [email protected] = 70% to 80%, it is recommended to make the cross section of the yoke about 1.2 to 1.4 times that of the poles [I1]. In modern magnets the yokes and the poles are made of laminations. In order to attain the strongest possible magnetic ﬁeld, the shape of the poles and pole pieces must be determined to satisfy the following two requirements:

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

r3

r2

x1

273

r1

x2 x3

ș1 ș2

Figure 4.17: Shape of a pole with two conical pole-pieces.

(a) The magnetization of the poles and pole pieces must produce the maximum possible ﬁeld when they are saturated. (b) Saturation should be achieved simultaneously throughout the volume of the poles and the pole pieces. In view of increasing leakage from the poles, as their magnetization approaches saturation, the cross-section of the poles must be reduced as the tip of the pole is approached. The ﬂux density will thus be maintained constant and the requirement (b) will be met. In order to satisfy the requirement (a), Ewing [E2] showed, as early as the end of the nineteenth century, that the shapes of the pole pieces must be conical, preferably with the vortex angle of 54.70 . In an actual electromagnet, however, this conical shape must be modiﬁed, in order to secure homogeneity of the ﬁeld in the air gap and to ensure that permeability is constant throughout the pole and the pole piece [I2]. Analyzing eqs. (4.43) and (4.45), Ishikawa and Chikazumi [I2] showed that the pole shape that satisﬁes the above requirements can be approximated by the shape shown in Fig. 4.17. This shape is composed of a pole-tip of radius u1 , a conical part of radius u2 and another conical part of radius u3 . Analysis of this shape indicates that that the maximum ﬁeld in the air gap depends on the value of u2 @{1 and not on u1 @{1 > while the homogeneity of the ﬁeld is determined by the value of u1 @{1 . The issue of the ﬁeld homogeneity is not critically important in magnetic separation and the parameter u1 @{1 is, therefore, of limited relevance for the design of a circuit of a magnetic separator.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

274

B0

B C A (NI)A

(NI)B

(NI)c

NI

Figure 4.18: The excitation curve of an electromagnet showing the unsaturated zone (A), transition zone (B) and saturated zone (C).

4.3.3

Practical procedure for design of the poles

The design of an electromagnet for a magnetic separator is based on two fundamental speciﬁcations, namely the required magnetic ﬁeld strength Ej and the length (2{1 ) and the depth (2u1 ) of the air gap. The former parameter is determined by the required separation e!ciency while the latter mainly by the desired throughput of the separator. In wet high intensity magnetic separators the depth of the air gap determines the depth of the matrix bed, which in turn also aects the eectiveness of separation. From an economic point of view, the size and thus the price of the magnet depends strongly on the length of the air gap Oj = 2{1 = The volume of the magnet is approximately proportional to (2{1 )3 . Contribution of iron to the magnetic ﬁeld The contribution of the iron circuit to the magnetic induction in the air gap can be divided into three regions, as illustrated by the excitation curve shown in Fig. 4.18. In the unsaturated zone D the reluctance of the air gap is much greater than the reluctance of the rest of the circuit so that almost the entire magnetomotive force appears across the gap. Once the transition zone sets in, the ﬂux that reaches the air gap is reduced. In order to achieved the desired magnetic induction, the number of ampere-turns must be increased, as shown in Fig. 4.18. It was reported by Montgomery [M21] that usually (Q L)E @(Q L)D 1.1 at 60% of the maximum magnetic ﬁeld, while a typical value of this ratio at 85% of the maximum ﬁeld is about 2. A plot of this ratio against the percentage

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

275

Figure 4.19: Ampere-turns needed to achieve a required magnetic ﬁeld.

of the maximum induction, for a typical magnet, is shown in Fig. 4.19. With the number of ampere-turns known at 60% and 85% of the maximum ﬁeld, a satisfactory curve can be drawn representing the magnetization of iron from 0 to 100% [M21]. Figure 4.20 shows the number of ampere-turns required to obtain 85% of the maximum ﬁeld, as a function of the geometry of the magnet. Design of coils Coils in an iron-core electromagnet serve two functions: they provide the electromagnetic force to magnetize the iron, and they contribute a certain magnetic ﬁeld in the air gap. The magnetic induction generated by a coil, the geometry of which is shown in Fig. 4.21, at the centre of the coil, is given by [M22]: Ej =

QL I (> ) 20 d1 ( 1)

(4.46)

where = d2 @d1 , = [email protected] and I (> ) is the ﬁeld factor deﬁned (in SI units) as + (2 + 2 )[email protected] I (> ) = ln (4.47) 1 + (1 + 2 )[email protected] The ﬁeld along the axis } of a coil of axially uniform excitation can be written [M22]: · ¸ } I (> + }@d1 ) + I (> }@d1 ) E} ( ) = E} (0) (4.48) d1 2I (> )

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

276

Figure 4.20: Ampere-turns required to reach 85% of the maximum magnetic ﬁeld in the air gap, as a function of the ratio of the pole face diameter and the gap length, u1 /{1 , for several u3 @u1 ratios (adapted from [M21]).

2b

a2 a1

z

Figure 4.21: Deﬁnition of geometrical parameters of a solenoid coil.

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

277

Figure 4.22: Empirically obtained curve expressing the maximum magnetic ﬁeld as a function of ratio of the pole diameter to air gap length (adapted from [I1]). If the point at which this ﬁeld is measured lies outside the coil (e.g. in the air gap of an electromagnet) the following relationship should be used in eq. (4.48): I (> }@d1 ) = I (> }@d1 )

(4.49)

Practical rules for the design Taking into account the above analysis, the following rules should be followed in the design of an electromagnet: (1) Although the ﬁeld homogeneity is not critical in magnetic separation, a suitable choice of the pole radius u1 , in such a way that u1 = 2{1 , usually ensures the ﬁeld homogeneity within 103 = (2) The maximum magnetic ﬁeld is a function of the maximum pole diameter 2u3 , irrespective of dierences in pole shapes [I1]. Using Figs. 4.20 and 4.22, approximate value of the maximum diameter of the pole from the selected values of Ej and {1 can be determined. (3) The optimum value of angle 1 depends on the value of u1 @{1 which again is not of major importance in magnetic separators. 1 usually ranges from 500 to 600 . (4) A generally accepted rule is that u3 = 1.2u2 to 1.4u2 = (5) The number of ampere-turns should be selected in such a way that (Q L)E = 1=1(Q L)D or 2(Q L)D , if 60% or 85% of the maximum ﬁeld is to be achieved, respectively. Figure 4.23 illustrates modelling of the magnetic ﬂux in a iron-core electromagnet.

278

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.23: Modelling of an iron-core electromagnet.

4.4

Design of solenoid magnets

As has already been discussed in Section 1.7.3, generation of magnetic induction by iron-core electromagnets is limited by the saturation of the iron. In order to overcome this limitation, Bitter [B24] proposed the use of a magnetizing solenoid surrounded by steel cladding. The magnetic induction in the working volume of such a magnet is given by the sum of the contribution from the coil and from the magnetized iron, as expressed by eq. (1.50). Figure 1.40 illustrates the relative contributions from these two components of the magnet. The idealized circuit of the iron-clad solenoid is shown in Fig. 4.24. The magnetic induction in the air gap is given by Ampere’s law (eq. (4.41)). If the magnetic reluctance of the iron frame cannot be neglected, eq. (4.42) must be used. In a more practical form, a leakage factor N can be included in eq. (4.42), and we can write: QL Ej = 0 (4.50) Oj (1 + N) The leakage factor N is often taken equal to 0.2 [T6, M23]. It transpires from eq. (4.50) that the number of ampere-turns required to generate a given magnetic induction is determined solely by the length of the ﬁeld (or the length of the air gap) Oj and is independent of the radius d1 of the working volume. Solenoids shown in Fig. 4.25 have the same length of the air gap, while their radii dier, and the number of ampere-turns required to generate a required magnetic induction is the same for both solenoids. This feature is extremely useful in the scale-up of magnetic separators. In iron-core electromagnets a higher throughput of separators is achieved by increasing the

4.4. DESIGN OF SOLENOID MAGNETS

279 t

Lg

a1 a2

Figure 4.24: Schematic diagram of an iron-clad solenoid.

length of the air gap. This requires an increased number of ampere-turns, as follows from eq. (4.41). This, in turn, results in an increase in the mass, size and cost the magnet. On the other hand, the scale-up of a magnetic separator based on an ironclad solenoid is achieved by increasing the diameter of the solenoid, keeping the length of the air gap constant. The number of ampere-turns will be constant, only the length of the conductor, and thus its resistance will increase.

Lg

2a1

Figure 4.25: Two iron-clad solenoids having the same length of the air gap and dierent radii.

280

4.4.1

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

The power requirements

The magnetic induction generated directly by the coil itself can be calculated using eqs. (4.46) and (4.48). The power Z (in watts), required to generate a given magnetic induction, is then given by: Z =

(d21 (2 1)(Q L)2 2e(d2 d1 )2

(4.51)

where ( is resistivity of the conductor and is the ﬁlling factor of the winding deﬁned as active section of the winding (4.52) = total section of the winding Combining eqs. (4.41) and (4.51) it can be seen that the power is proportional to the square of the number of ampere-turns and thus of magnetic induction, Z Ej2 . While the electric current L and the number of turns Q are related by eq. (4.41), the necessary voltage can be found from Y = LU> where the resistance of the winding can be calculated from: U=

2(Q (( + 1) Q2 Gphdq = D 2( 1)d1

(4.53)

where D is the cross-section of the winding and Gphdq is the mean diameter of the winding.

4.4.2

The choice of the conductor

The choice of the conductor, between copper and aluminium, determines the maximum current density, the mass and the volume of the coil and the cost of the magnet. Copper is 3.3 times denser than aluminium (8960 kg/m3 vs 2699 kg/m3 ) and for equal coil sizes aluminium will make a much lighter coil. On the other hand, resistivity of aluminium is about 1.58 times greater than resistivity of copper (2.45×108 m vs 1.555×108 m at 0 0 C), 1.58 time more power is required by the aluminium coil to generate the same ﬁeld. Detailed analysis of the relative merits of aluminium and copper coils, as a function of coil geometry, mass and cost can be found in [M22].

4.4.3

The cooling of coils

The removal of the Joule heat generated inside the winding can be accomplished in several ways. Indirect air cooling can be applied to magnets operating at low current densities, generally not exceeding 3 A/mm2 for a copper conductor. Direct immersion of the coil into the circulating oil or water greatly improves heat conduction and transfer and higher current densities can be used. The operating current density can be increased considerably by using hollow conductors through which the cooling liquid circulates. Water is a very e!cient

4.4. DESIGN OF SOLENOID MAGNETS

281

coolant in removing heat at conventional temperatures. The oils, for example, have heat-transfer characteristics about one-ﬁfth that of water [D11]. Coils with low resistance, operating at low voltage, are almost always cooled with deionized or demineralized water, mains water causing electrolysis even at low voltage. The cooling water is circulated through the coil, a heat-exchanger, a ﬁlter and a deionizer. In the heat-exchanger the heat is carried o by tap water. The ﬂowrate of water T (in cm3 /s or m3 /h) required to restrict the temperature rise to W (in 0 C) in a magnet with power input of Z (in watts) is given [M22] by: Z Z (fjv) = (VL) (4.54) T= 4=186W 1163=7W For instance, for a 250 kW magnet, with temperature rise of W = 30 0 C, the required ﬂowrate is approximately 2000 cm3 /s, or 7.2 m3 /h. The operating temperature of a magnet aects the resistance of the winding and thus the power needed to achieve the required magnetic ﬁeld. The hotter the coil, the higher the resistance will be and the more power will be needed. The temperature dependence of resistivity of conductors can be written (W = (20 [1 + (W 200 F)]

(4.55)

where (W and (20 are resistivities at temperature W and 20 0 C, respectively and is the temperature coe!cient. For copper (20 = 1.72×108 m and = 0.0041/0 C, while for aluminium (20 = 2.7×108 m and = 0.0045/0 C. Therefore, a copper conductor operating at 60 0 C has resistivity of 2×108 m, while an aluminium conductor has resistivity of 3.2×108 m. Whether or not the amount and ﬂow velocity of the coolant, as determined by eq. (4.54), can be forced through the winding of the magnet depends on the pumping power available and on the detailed structure of magnet. The pressure drop across a tube is the sum of the entrance and exit losses and frictional drop in the tube. The total pressure drop S (in Pa) becomes O S = (0=74 + 0=015 )103 y 2 g

(4.56)

where O and g are the length and diameter of the cooling path (in m), and y is the coolant velocity (in m/s). A typical pressure drop for copper hollow conductors is 0.5 to 0.8 MPa.

4.4.4

Thickness of the iron cladding

The basic requirement for the iron cladding is that it must not be saturated. The magnetic ﬂux in the cladding is Mv Df where Df is the cross-sectional area of the cladding. In order to avoid oversaturation of the cladding, the following inequality must be satisﬁed: Ej Dj 5 Mv Df (4.57) where Ej is the magnetic induction in the air gap of cross-sectional area of Dj . The thickness of the cladding can thus be found from this equation.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

282

Table 4.5: Properties of decarburized steel for high-ﬁeld magnets [B1]. Chemical composition Coercivity Hmax f Permeability

0.05 - 0.02% C, 0.2% Mn, 0.02% S 0.05% Cu, 0.01% P, 0.02% Ni 60 to 80 Am1 B A 0.04 T at H = 40 Am1 B A 1.5 T at H = 1200 Am1 B A 2.0 T at H = 2400 Am1

The choice of the value of Mv is important for correct dimensions of the iron cladding. The values of saturation polarization for commercial steels are usually not available and the value of 1.5 T or less should be used. Low-carbon decarburized steel is frequently used in high-ﬁeld magnets and typical speciﬁcations are shown in Table 4.5 [B1]. Several important rules relating to the usage of iron cladding can be outlined: • Magnets for which the length of the air gap is greater than the inner diameter of the solenoid, i.e. Oj A 2d1 , do not require the iron pole above and below the working volume. On the other hand, when Oj ? 2d1 , the presence of iron cladding in the vicinity of the working space is necessary. • By replacing the external air path with a magnetic circuit of low reluctance, the most signiﬁcant increase in the magnetic induction, for a given magnetomotive force, can be obtained for solenoids of small axial length. Therefore, the contribution of the iron is largest if the coil has a considerable stray magnetic ﬁeld. In the case of a long thin solenoid, in which the stray ﬁeld is small, the eect of an external iron circuit is negligible.

4.5 4.5.1

Design of drum magnetic separators The basic magnet arrangements

The basic design of the magnetic circuit of drum magnetic separators is common to most commercially available models. Permanent magnet blocks are stacked on top of each other in a speciﬁc geometrical arrangement. The simplest arrangement is shown in Fig. 4.26. Strontium or barium ferrite blocks, usually magnetized through their thickness are frequently arranged radially in low-intensity drums. The frequently used size of the blocks is 150 mm long, 100 mm wide and 25 mm thick. The number of blocks per stack is determined by the diameter of the drum. These radially magnetized stacks are most often arranged in rows parallel with the axis of the drum, separated by an air gap. A radial arrangement is also used, as discussed in Section 2.1.5. and as shown in Fig. 2.12. Figure 4.27 illustrates the axial arrangement of magnet blocks in a magnetic drum.

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

a

283

b S

N

N S

L

Figure 4.26: Schematic diagram of radially magnetized magnets in a magnetic drum with axial arrangement of the poles.

Figure 4.27: Axial arrangement of magnet blocks in a magnetic drum.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

284 N

N

S

S

S

N

Figure 4.28: Position of a backing magnet (cross pole) in a drum magnetic separator. High-intensity drum separators employ rare-earth magnets, usually NdFeB, and it is a common practice to simply replace ferrite magnets with rare-earth blocks, with the intent to achieve a higher magnetic ﬁeld [A13]. The rare-earth blocks are smaller than the ferrite blocks, for example 50×50×15 mm. Another arrangement of permanent magnets which is frequently employed is shown in Fig. 4.28. A ferrite magnet, magnetized in a transverse direction is inserted between the radially magnetized stacks of permanent magnets. Explanations of the function of this "backing" of "blocking" magnet (or "cross pole") are as numerous as its names. Reduction of the leakage ﬂux between the adjacent main stacks and addition of extra ﬂux [M19] are the most likely explanations of the beneﬁt that this arrangement oers.

4.5.2

Geometry of the magnet assembly

Although drum magnetic separators are one of the oldest types of magnetic separators, and certainly the most widely used, design of the magnetic circuit is still to a great extent empirical. A simple rule for geometrical arrangement of the magnet blocks that was used for many decades states that the ratio of the magnet block width e and the width of the air gap d should be [email protected] = 3 to 5 for ferrite and rare-earth magnets and [email protected] = 1.2 for Alnico magnets and electromagnets [D4]. The design dierence is the result of dierent demagnetization behaviour of the permanent magnet materials, as shown in Fig. 4.2. Using computer modelling, this design rule has been revised, as will be discussed later. A typical distribution of the ﬁeld pattern along the circumference of a drum with axial pole arrangement is shown in Fig. 4.29. The maxima in the magnetic induction occur at the centres of the air gaps while the minima occur at the centre of the magnet block. Comparison of the magnetic induction generated by dierent magnet arrangements in a drum is given in Fig. 4.30. The relative values of the magnet and air gap widths aect the magnetic ﬁeld and force distribution around the drum. For instance, by reducing the distance between the magnet blocks, or the so-called pole pitch (deﬁned either

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

285

Figure 4.29: Distribution of the magnetic induction along the circumference of an NdFeB drum with axially arranged poles. The width of the radially magnetized magnets e = 100 mm and the air gap width d = 10 mm [M24].

Figure 4.30: The maximum magnetic induction generated by dierent magnet arrangements in an axial drum with radial magnetization of the magnet blocks (adapted from [M10]).

286

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.31: Magnetic ﬁeld and force index (in arbitrary units) as a function of distance from the drum surface, for dierent distances between the poles (adapted from [S13]).

Shell

Steel pole

Magnet block

Figure 4.32: Steel poles sandwiched between azimuthally arranged magnet blocks.

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

287

Figure 4.33: Magnetic induction generated by magnetic drums, with three different magnet arrangements, as a function of distance from the drum surface (adapted from [F19]).

Figure 4.34: Dependence of the magnetic induction on the surface of the drum, on the width e of the NdFeB magnet, for d = 10 mm. Three dierent conﬁgurations are shown [M24].

288

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.35: Dependence of the force index at 15 mm from the drum surface, on the width e of the NdFeB magnet, for d =10 mm. Three dierent conﬁgurations are shown [M24].

Figure 4.36: Magnetic induction as a function of the width d of the air gap, for an NdFeB magnetic drum, for e = 100 mm [M24].

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

289

Figure 4.37: Force index for an NdFeB drum, as a function of the width d of the air gap, for e = 100 mm [M24]. as d or d + e in Fig. 4.26), it is possible to increase the ﬁeld gradient. Although the ﬁeld strength is reduced, the increase in the ﬁeld gradient is su!cient to result in the increase of the force index. The situation is depicted in Fig. 4.31. It can be seen that the increase in the force index by reducing the pole pitch takes place only in the proximity of the drum surface and that the force index decreases rapidly away from the drum. In other words, the smaller the pitch, the higher the force index on the drum surface and the shorter the reach of the magnetic force. In the nineteen eighties the Fives-Lille group developed drum magnetic separators with steel poles sandwiched between ferrite magnet blocks with azimuthally arranged direction of magnetization, as shown in Fig. 4.32. As a result of their superior performance, compared to the conventional design, in terms of magnetic force and metallurgical performance, the azimuthal concept was commercially accepted for some applications. Comparison of the magnetic ﬁeld strength achievable by the conventional and azimuthal designs is shown in Fig. 4.33.

4.5.3

Electromagnetic modelling of the design

Electromagnetic modelling software that has become available in recent years allows for the optimization of the design of conventional magnetic circuits. The modelling allows the investigation of the eect of various geometrical parameters of the drum on the magnetic ﬁeld and magnetic force. For instance, Fig. 4.34

290

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.38: The dependence of the magnetic induction generated by a strontium ferrite block 100×150 mm, on its depth O, on the surface of the block and at 15 mm from the surface. illustrates the variation of the magnetic induction on the surface of a drum with the width e of the magnet block. It can be seen that for a constant width d = 10 mm of the gap, the maximum magnetic induction is achieved for the magnet width of 100 mm. The ratio [email protected] = 10 is thus in disagreement with the empirical rule-of-thumb mentioned earlier. Figure 4.34 also shows that replacement of the air gap with a steel block results in the reduction of the magnetic ﬁeld. Similar conclusions can be drawn from Fig. 4.35, which displays the eect of the magnet width on the force index. The eect of the width d of the air gap on the ﬁeld at various distances from the drum surface is illustrated in Fig. 4.36. It can be seen that by increasing d, for a constant value of the width of the magnetic block (i.e. with the ratio [email protected] decreasing), the magnetic induction decreases, at least in the proximity of the drum surface. At larger distances from the drum surface, e.g. at 50 mm, the eect of the value of d (and thus of [email protected]) is diminishing. Similar trends can be observed for the force index as shown in Fig. 4.37. The results illustrated in Fig. 4.30 and Figs. 4.34 to 4.37 were obtained for a drum with axial pole arrangement and with magnets magnetized radially. The diameter of the drum was 600 mm and the depth O of the magnet stack was 100 mm. The eect of the depth of the magnet stack can be determined by using eq. (4.30), which allows for the variation of the depth O , as shown in Fig. 4.9, and for the calculation of the magnetic ﬁeld generated by such a magnet block, at dierent distances }. Figure 4.38 illustrates such a dependence for a strontium

4.6. DESIGN OF A MAGNETIC ROLL

291

Figure 4.39: Magnetic induction on the roll surface, as a function of the magnet ring thickness. The values of magnetic induction were obtained by computer modelling [F18]. ferrite block, of dimensions 150 mm (Z ) × 100 mm (G). It can be seen that the beneﬁt of increasing the depth of the magnet stack above 140 mm is limited. The computer modelling also allowed for the development of new geometries of the magnet arrangement, capable of producing a higher magnetic strength and magnetic force [A13, S8]. Some of these new designs are proprietary and the patents are still pending. Comparison of one such a design, with conventional designs, is shown in Figs. 4.34 and 4.35.

4.6 4.6.1

Design of a magnetic roll Basic concepts of design

The overall view of a magnetic roll separator is shown in Figs. 2.30 and 2.31. The magnetic roll itself forms a part of a short conveyor fed by a vibratory feeder. The conveyor belt is made of a thin high-tensile material, often with antistatic coating. The belt is supported by second roll (idler). Roll separators are usually of modular design allowing them to be stacked in any number of passes of material. Typical speciﬁcations of such a roll separator are shown in Table 4.6. The e!ciency of separation is aected by the roll design and by several operating variables: the number of separation stages, belt speed, splitter position and belt loading. Most of these variables are determined by particle size

292

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.40: Force index as a function of the magnet ring thickness, for thickness of steel rings equal to 1 mm and 1.75 mm, on the roll surface and at 15 mm from the surface.

Figure 4.41: Magnetic induction on the surface of a roll, as a function of thickness of steel rings, for several thicknesses of permanent magnet rings.

4.6. DESIGN OF A MAGNETIC ROLL

293

Table 4.6: Typical speciﬁcations of a permanent roll magnetic separator. Parameter Belt thickness Roll diameter Roll length Max. magnetic induction

Speciﬁcation minimum 0.12 mm 72, 76, 100, 220 & 300 mm 250, 500, 1000 and 1500 mm NdFeB: 1.9 T, SmCo: 1.5 T, SrFe: 0.5 T

distribution and magnetic properties of the feed and by the recovery vs grade requirement.

4.6.2

Design parameters

Thicknesses of magnet and steel rings As has been discussed in Section 2.3.3 and shown in Fig. 2.28, the roll consists of discs or rings of permanent magnets, interleaved with mild steel rings. The adjacent permanent magnet rings are arranged with the same polarity facing one another, i.e. rings are arranged in a repulsive mode. The relative thicknesses of the magnets and the steel rings aect the magnetic ﬁeld strength and its pattern around the roll. This situation is depicted in Figs. 4.39, 4.40 and 4.41. It can be seen that the magnetic induction on the surface of a roll increases with increasing thickness of the magnet ring. At the same time it achieves the maximum value for a certain, rather small, thickness of the steel rings. With further increase in the thickness of the steel rings the magnetic induction decreases. This is a consequence of the fact that the saturation magnetization of steel is much greater than that of the permanent magnet material. If the thickness of the steel exceeds a certain optimum value, the magnet ring does not succeed in saturating the steel, as transpires from eq. (4.12). As can be seen in Figs. 4.42 and 4.43, for thin steel and magnet rings, which generate a high force index close to the roll surface, the reach of the magnetic force drops dramatically away from the surface. The rate of decrease is much smaller for thicker magnet rings and even more so for an NdFeB drum. Optimization of the design of the magnetic roll consists not only of maximizing the magnetic induction and force index on the roll surface and at a suitable distance from the roll, but also of matching the dimensions of the magnet and steel rings thicknesses to the particle size distribution of the material to be separated. Distributions of the magnetic induction along the axes of NdFeB and SrFe rolls are shown in Figs. 4.44 and 4.45. The magnetic ﬁeld (and magnetic force) on the roll surface are the greatest in a relatively narrow region at the interface between the magnet and steel rings. It can also be seen that the ﬁeld and the force along the circumference of the magnet rings are very feeble, and it is imperative, therefore, that no particles are continuously exposed to this region of the roll. The thickness of the magnet rings should thus be of magnitude similar to the

294

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.42: Force index as a function of distance from the roll surface, for various thicknesses of magnet rings. Steel ring thickness equals 1 mm.

Figure 4.43: Force index (in arbitrary units), for two conﬁgurations of NdFeB rolls and an NdFeB drum, as a function of the distance from the surface of the roll [F18].

4.6. DESIGN OF A MAGNETIC ROLL

295

Figure 4.44: Distribution of the magnetic induction on the surface on an NdFeB roll with 3/1 conﬁguration (magnet thickness: 3 mm, steel thickness: 1 mm).

Figure 4.45: Distribution of the magnetic induction on the surface of a SrFe roll with 6/2 conﬁguration (magnet thickness: 6 mm, steel thickness: 2 mm).

296

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.46: The partition curves for the recovery of 4 mm magnetic tracers by NdFeB rolls of dierent conﬁgurations [F20]. mean particle size of the material to be separated. Thin magnet rings should be used to separate ﬁne particles, while for larger particles a thicker magnetic ring oers a larger contact area with the roll, and a longer reach of the magnetic force, of the order of the radius of the particles. It transpires from the above discussion that the design of the roll, and specifically the thicknesses of the magnetic and steel rings, is dictated by the magnetic properties and size distribution of the feed. The roll design must be optimized in order to maximize the magnetic force and its reach and to match the dimensions of the particles with the magnet thickness. A speciﬁc conﬁguration expressed as magnet thickness/steel ring thickness is suitable only for a narrow size fraction and typical conﬁgurations are summarized in Table 4.7. The optimum conﬁguration obtained by electromagnetic modelling can be validated experimentally using magnetic tracers of suitable sizes and accurate values of magnetic susceptibility. Magnetic partition curves can then be constructed, the probable error Hs can be calculated and a conﬁguration with the lowest Hs can be determined. Hs for a magnetic separator can be deﬁned as Hs =

"75 "25 2

(4.58)

where "75 and "25 are the mass magnetic susceptibilities of particles 75% and 25% of which, respectively, report to the magnetic fraction. Typical partition curves, for 4 mm particles, are shown in Fig. 4.46. It can be seen that the partition curve for the roll conﬁguration 4/2.5 is steeper than that for 4/1

4.6. DESIGN OF A MAGNETIC ROLL

297

Table 4.7: Various conﬁgurations of NdFeB magnetic rolls. Conﬁgurations are expressed as the ratio magnet thickness/steel thickness. Conﬁguration 3/1, 4/1 or 4.1.5 6/1.5, 6/2, 6/3 8/2, 8/3

Size fraction - 5 + 0.1 mm - 10 + 5 mm + 10 mm

Comment Short reach, high ﬁeld Longer reach, lower ﬁeld For large particles

Figure 4.47: Force index for NdFeB rolls of dierent diameters, as a function of distance from the roll surface. Roll conﬁguration: 12/7.5. The data were obtained by computer modelling (adapted from [F18]). conﬁguration and Hs is correspondingly lower. Conﬁguration 4/2.5 is, therefore, more selective in separating 4 mm particles of dierent magnetic susceptibilities.

Diameter of magnet rings In the past, the diameter of a rare-earth magnetic roll was dictated by availability of the largest magnetic rings. While the ﬁrst commercial rolls had diameters of 72 and 76 mm, recent progress in manufacture of rare-earth permanent magnet rings and segments allows for the manufacture of rolls with diameter of 100, 220 and 300 mm. The choice is determined by a combination of throughput, performance and cost considerations. The present advantageous cost situation favours larger diameter rolls, particularly when large throughputs are required [A13]. In a simpliﬁed assumption of a constant magnetic force and constant resi-

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

298

2a1

h H

2a3

2a2

z

P

Figure 4.48: Schematic diagram of a suspended magnet. dence time, a throughput increase by increasing the roll diameter, follows the ratio G1 /G2 , where G1 and G2 are the roll diameters, as follows from eq. (5.4). It is sometimes argued that by increasing the magnet diameter the magnetic force also increases and an even higher throughput can be expected. It appears, however, that the increase in the magnet ring diameter above 100 mm brings only negligible increase in the force index, as is illustrated in Fig. 4.47. On the other hand, a longer retention time of particles in a larger-diameter roll, as a result of a longer arc of the magnet ring, to which the particles are exposed, allows for the increase of speed of rotation of the roll and thus for the increase of the throughput, while maintaining constant residence time. Experience indicates that a throughput increase by factor of two to ﬁve, maintaining the same performance, can be obtained with larger diameter rolls [A23, A13].

4.7

Design of a suspended magnet

Suspended magnets are usually installed over conveyor belts, discharge ends of feeders or screens and above chutes or launders. Their design is dictated by the burden depth, the belt speed, the clearance required over the burden and the size, shape and mass of the tramp iron that is being removed. Strength and reach of the magnetic ﬁeld and of the magnetic force must, therefore, be maximized for high e!ciency of the material removal. A schematic diagram of an electromagnet-based rectangular suspended magnet is shown in Fig. 4.48. The magnet consists of an iron yoke and a coil, which magnetizes the yoke. The magnetic ﬁeld generated at point S , at distance } from the magnet, is the sum of contributions from the magnetized steel and

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

299

Figure 4.49: Pattern of magnetic ﬂux around a suspended magnet. the coil. Dimensions of individual parts of the yoke determine the distribution of the magnetic ﬁeld and magnetic force, their value and reach. Using computer modelling, it is possible to investigate the inﬂuence of these dimensions and to determine the optimum design for a given application. The distribution of magnetic ﬂux around a suspended magnet is shown in Fig. 4.49, while a three-dimensional image is presented in Fig. 4.50. In commercially available suspended magnets, the width 2d1 of the magnet typically ranges from 900 mm to 1400 mm, the depth ranges from 700 mm to 1250 mm and the height K is around 500 mm. Aluminium is the preferred conductor materials, mainly because of its lower density. For the same electric power, the mass of the aluminium coil can be approximately halved, compared with the copper coil [K36]. In addition, the use of the aluminium foil, rather than of the wire, allows for the increase in the ﬁlling factor of the winding, by about 40% [K36]. As a result, the number of ampere-turns can be reduced, or, alternatively, at the constant number of ampere-turns, a more powerful magnet can be constructed.

4.8

Design of a ferrohydrostatic separator

Commercial and laboratory ferrohydrostatic separators use either an electromagnet or permanent magnets to generate the magnetic ﬁeld in the working space. Of fundamental importance in the operation of separators with magnetic ﬂuids are the characteristics of the magnetic levitation force, expressed by the second term on the right-hand side of equation (2.9), namely by Mi EuE. These characteristics are determined by the pattern of the gradient of the magnetic

300

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.50: A three-dimensional image of the magnetic ﬁeld around a suspended magnet. ﬁeld and, therefore, by the shape of the pole tips. The shape of the pole tips is determined by several factors, namely by the choice of the magnetic ﬂuid and the number of density fractions that are to be produced. If paramagnetic liquids are to be used, the constant apparent density of separation in the entire volume of the ﬂuid will be obtained if the force acting on a particle is constant, I = const., which corresponds to EuE = const., as transpires from eq. (3.144). This condition can be re-written as CE 2 = frqvw= C|

(4.59)

where | is the vertical axis, as shown in Fig. 4.51. This requirement is the result of the linear dependence of the ﬂuid polarization, namely i E, on the external magnetic ﬁeld. The ﬁeld that satisﬁes condition (4.59) is the isodynamic ﬁeld. As can be seen from eq. (3.145), the situation is somewhat dierent with ferroﬂuids: if the ferroﬂuid is magnetically saturated, a constant density of separation will be obtained by maintaining the constancy of the force acting on the particles by satisfying the condition uE = const. In other words, the condition CE = frqvw= (4.60) C| should be satisﬁed in a su!ciently large region of the magnetic ﬁeld. Two basic shapes of pole tips have been used in ferrohydrostatic separators, namely a simple wedge geometry of the working space, and pole tips with hyperbolic shape.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

301

y S

N

Permanent magnet

lg ș Iron yoke

Figure 4.51: Schematic diagram of an FHS magnetic circuit with a wedgeshaped working gap.

4.8.1

FHS separators with a wedge-shaped working gap

Wedge-shaped working space was used in separators with permanent magnets, such as those built by Tohoku University [S50], Nittetsu Mining Co. (Japan) [S51] and the Too Geos (Russia) [S52] machines. A schematic diagram of such a magnetic circuit is shown in Fig. 4.51. Since the gradient of the magnetic ﬁeld, in this design, is not constant along the vertical ([email protected]| 6= frqvw=), the apparent density of the ferroﬂuid along the vertical will also vary. A typical distribution of apparent density of the ferroﬂuid in a separator with wedge-shaped working space, used for recovery of non-ferrous metals, is shown in Fig. 4.52. It can be seen that essentially a continuous spectrum of densities is present in the pool of the ferroﬂuid. The usefulness of this density distribution is very limited as inter-particle collisions and interactions do not allow accurate and selective separation of individual metals into individual density fractions. Distributions of the magnetic induction and the apparent density of the ferroﬂuid along the vertical axis for the Too Geos separators with ferrite permanent magnet-based wedge-shaped pole tips were reported by Solodenko [S52]. The results are summarized in Fig. 4.53. Shimoiizaka et al. [S50] obtained a similar pattern in a separator that used SmCo permanent magnets (see Fig. 4.54). It can be seen again that a magnetic system with wedge-shaped poles creates a plurality of values of the ﬁeld gradient, and, therefore, of the apparent density of the ferroﬂuid along the vertical axis of the magnet gap. It is clear that such patterns of the apparent density can be used only for density separation of mixtures of materials with large density dierential. Speciﬁcations of the Tohoku University FHS separator, as reported by Shi-

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

302

Feed point

Surface of ferrofluid 5 g/cm3 Al

Pool of ferrofluid

6

V

8

Zn

9

Cu

10

Bi

8 6

Bottom of the magnetic pole Pb

Figure 4.52: Distribution of the apparent density of ferroﬂuid in an FHS with a wedge-shaped working space. Recovery of various non-ferrous metals at dierent positions along the vertical axis is indicated.

Figure 4.53: The apparent density and magnetic induction in a permanent magnet-based ferrohydrostatic separator with wedge-shaped pole tips, as a function of distance from the base of the pole tips (adapted from [S52]).

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

303

Figure 4.54: Magnetic induction and its gradient in the gap of a SmCo magnet-based ferrohydrostatic separator with wedge-shaped pole tips (adapted from [S50]). Table 4.8: Speciﬁcations of the Tohoku University FHS separator for the recovery of non-ferrous metals, for three dierent values of the width of the magnet gap [F21]. Parameter Magnetic ﬁeld [T] Field gradient [T/m] Apparent density [kg/m3 ]

lj = 60 mm 0.362 3.5 9600

lj = 80 mm 0.314 3.0 8200

lj = 100 mm 0.265 2.5 6900

moiizaka et al. [S50] and Fujita [F21], are summarized in Table 4.8. SmCo permanent magnets were used to generate the magnetic ﬁeld in the working space. The height of the ferroﬂuid pool was 120 mm and the angle between the pole tips amounted to 300 . Water-based ferroﬂuid of density approximately 1400 kg/m3 and magnetic polarization of 0.028 T was used. Another disadvantage of the permanent magnet-based FHS is that the value of the magnetic induction and of the ﬁeld gradient cannot be easily varied. The magnetic induction can be varied only by changing the distance between the pole tips using a mechanical device that can slide one of the poles against the other. The ﬁeld gradient can be varied by adjusting the angle = As a result of the absence of constancy of the apparent density of the ferroﬂuid and of any meaningful control of the operating magnetic ﬁeld and its gradient, the permanent magnet-based wedge-shaped ferrohydrostatic separators are suitable only for separation of materials that dier in density by at

304

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.55: Hyperbolic pole proﬁle with a mirror plate. least 2000 kg/m3 . Recovery of platinum-group metals [S53, S54, G4] and possibly separation of non-ferrous metals [S50] are applications where the limited accuracy of such separators can be tolerated. For more accurate separation of materials with small density dierences, hyperbolic pole tips must be used.

4.8.2

Separators with hyperbolic pole tips

A common objective of sink-and-ﬂoat separation is usually a production of two density fractions selectively and accurately. In order to achieve such a goal in ferrohydrostatic separation, it is necessary for the apparent density of the ferroﬂuid to be constant throughout the volume of the ferroﬂuid. As follows from eq. (3.145), this can be achieved by ensuring that the ferroﬂuid is magnetically saturated and by designing the shape of the pole tips in such a way that the ﬁeld gradient along the vertical axis is constant, namely [email protected]| = const. An additional constraint on the desired ﬁeld pattern is that the horizontal gradients, i.e. [email protected]{ and [email protected]}, are as small as possible. Therefore, for ideal density separation in ferrohydrostatic separators, the following conditions should be met: CE CE CE = frqvw 6= 0> = =0 (4.61) C| C{ C} Such a pattern of the magnetic ﬁeld can be achieved by a hyperbolic shape of the pole tips [K18], as shown in Fig. 4.55. In deriving the above conditions (eq. (4.61)), it was assumed that the branches of hyperbola forming the pole proﬁle extend to inﬁnity and that their asymptotes ({-axis) are at equal potential [G14]. The latter condition is satisﬁed in magnetic systems, in which the upper

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

305

Figure 4.56: GMUO ferrohydrostatic separator with hyperbolic pole tips. half of the hyperbolic surface is replaced by a ferromagnetic plate, coincident with the { axis, and perpendicular to the | axis, as shown in Fig. 4.55 [K18]. It was shown [K18, G15] that conditions given by eqs. (4.61) cannot be satisﬁed at all points in the working zone of the magnetic system. These conditions can be met only in the plane of symmetry passing through the centre of the interpolar gap deﬁned by the | axis in Fig. 4.55. The situation is further complicated by the fact that, in practice, the poles have ﬁnite dimensions. The hyperbolic surfaces are, therefore, terminated at some ﬁnite values of {> | and }. Such a truncation of the ideal hyperbolic shape necessitates corrections to the shape of the pole tips, in order to meet the conditions expressed by eqs. (4.61). The surfaces of the poles are shaped in such a way that they coincide with one of the elementary solutions of the Laplace equation. A powerful method for the analytical solution of Laplacian ﬁelds, namely conformal transformation, was used to calculate the magnetic ﬁeld generated by poles of ﬁnite size and of hyperbolic proﬁle [G14, G15, G16, S55]. This approach is the basis of the design of the GMUO ferrohydrostatic separators, as described in Section 2.8 and

306

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.57: The gradient of the magnetic ﬁeld along the vertical axis of the GMUO FHS-40M separator, as a function of distance from the base of the magnet pole tips.

shown schematically in Fig. 4.56. Similar design of the pole tips was used by the US Bureau of Mines [R9, K17] in their equipment for separation of non-ferrous metals. The distribution of the magnetic ﬁeld gradient along the vertical | axis in the GMUO FHS-40M separator is shown in Fig. 4.57. It can be seen that in a 40 mm long region along the vertical the gradient is constant. The apparent density of the ferroﬂuid is, therefore, also constant and selective and accurate density separation is possible in that region. It is found, using eq. (3.145), that a ﬁeld gradient of 2.5 T/m generates an apparent density of approximately 4200 kg/m3 , using, for example, a kerosenebased ferroﬂuid with magnetic polarization of 0.02 T. The apparent density can be varied by varying the electrical current in the coils and thus varying the magnetic ﬁeld in the working gap. The availability of computer electromagnetic modelling software has changed the speed and accuracy of the design of suitable proﬁles of the pole tips considerably. Although the initial proposal and design of the proﬁles still has to be worked out from ﬁrst principles of the magnet design, computer-based ﬁeld analysis can be used to verify and ﬁne-tune the design. Computer modelling, therefore, allows the pole proﬁles to be optimized so that the required density range and its accuracy are obtained. An example of the optimized hyperbolic proﬁle of pole tips of FHS is shown in Fig. 4.58 and a general view of a ferrohydrostatic separator with hyperbolic pole tips is shown in Fig. 4.59.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

307

Figure 4.58: Hyperbolic pole tips in FHS, as obtained by computer modelling.

Figure 4.59: Ferrohydrostatic separator with hyperbolic pole tips.

308

4.8.3

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Calculation of proﬁles of pole tips in FHS

Although computer modelling facilitates optimization and ﬁne-tuning of the pole proﬁles, the ﬁrst step in the design of a magnetic system of a ferrohydrostatic separator is, as a rule, the calculation of the ﬁeld and of the pole proﬁle from ﬁrst principles. The magnetic ﬁeld between the poles of the magnet can be represented by a scalar magnetic potential X : K = uX

(4.62)

Since the electrical currents are absent in this system, the magnetic potential satisﬁes the Laplace equation u2 X = X = 0

(4.63)

which can be written in polar coordinates u2

CX C2X C2X + u =0 + Cu2 Cu C2

(4.64)

A possible solution of the Laplace equation is the potential function X (u> ) = U(u)V()

(4.65)

where U is a function of u only and V is a function of only. It can be shown that these functions have the following form [B25]: U = fup + gup

(4.66)

V = j cos p + k sin p

(4.67)

and where f> g> j and k are constants. A particular solution to the Laplace equation can, therefore, be written in the form of a circular harmonic of order p as X (u> ) = (fup + gup )(j cos p + k sin p)

(4.68)

Of practical interest are, for example, solutions of the form [G17, Z7]: X0 = D0

(4.69)

Xp = Dp up sin p

(4.70)

and If the surfaces of the poles of the magnet are made to coincide with a given pair of equipotential surfaces (the proﬁle of which is independent of the third dimension), the ﬁeld between them and the proﬁle of the pole tips are described by eqs. (4.69) and (4.70).

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

309

Table 4.9: Properties of pole proﬁles. Value of m 2 3/2

Up /A u2 sin 2 = frqvw= [email protected] sin 32 = frqvw= = frqvw=

Comment constant gradient isodynamic ﬁeld, I = frqvw= wedge conﬁguration

Taking into account that K = uX , the modulus of the magnetic ﬁeld intensity is |K| = pDup1 (4.71) The gradient of the magnetic ﬁeld along the vertical (| axis) then has the form CK (4.72) = (p 1)pDup2 sin p C| while the product of the magnetic ﬁeld and its gradient (force index) are expressed as CK (4.73) = (p 1)p2 D2 u2p3 sin p K C| These equations can be used to evaluate and design various shapes of the pole proﬁles. For p = 1, [email protected]|, or the magnetic force, is zero. The simplest practical case of a wedge pattern is expressed by eq. (4.69). The wedge conﬁguration is represented by a straight line described by the equation = const= The isodynamic proﬁle, in which [email protected]| = const=> can be obtained from eq. (4.73) when p = 3/2. The isodynamic proﬁle of the pole tips is then given by 3 Xp = [email protected] sin = frqvw= (4.74) 2 and 3 CK = D2 sin (4.75) K C| 2 Pole proﬁles that generate a magnetic ﬁeld whose gradient in constant along the vertical axis can be obtained from eq. (4.72) when p = 2 and the equations of the proﬁle are as follows:

and

Xp = Du2 sin 2 = frqvw=

(4.76)

CK = 2D sin 2 C|

(4.77)

Equations (4.74) to (4.77), in which p determines the geometrical features of the ﬁeld and D describes the magnetic characteristics of the system, provide the full description of the proﬁle of the pole tips. Properties of these conﬁgurations are summarized in Table. 4.9.

310

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Design procedure We will assume that we want to design the pole proﬁles for a ferrohydrostatic separator operating with a ferroﬂuid. In order to obtain selective and accurate separation of the feed material into two density fractions, the apparent density of the ferroﬂuid in the working volume of the separator must be constant. This condition will be met if the ﬁeld gradient along the vertical axis is constant, i.e. if conditions (4.61) are met. Therefore, the proﬁle pattern must satisfy eq. (4.77). The practical procedure of designing the pole proﬁle and the magnetic ﬁeld characteristics is as follows: 1. Determine, from eq. (3.145), what ﬁeld gradient [email protected]| is needed to obtain the required density of separation, i.e. the apparent density of the ferroﬂuid. 2. Using [email protected]| = 2D (eq. (4.76)) calculate D= 3. From K = 2Du (eq. (4.71)) calculate K, for a given value of u= The length of the pole tips and the width of the gap between the pole tips are determined by u. The simplest approach would thus be to take u to represent the radius vector of the point of the closest distance O between the pole tips. 4. Based on the condition X = Du2 sin 2 = frqvw., it is possible to calculate the constant from frqvw u0 = (4.78) (sin 20 )[email protected] where u0 is the starting radius vector and 0 is the starting azimuthal angle, as shown in Fig. 4.55. Using this constant, the pole proﬁle is then given by u=

frqvw (sin 2)[email protected]

(4.79)

A similar procedure can be used to construct other pole proﬁles, for instance the isodynamic shape. The role of the mirror plate It follows from the pioneering work of Kaiser and Mir [K18] that a ferromagnetic mirror plate simulates the role of the upper half of the hyperbolic surfaces. Computer modelling of the hyperbolic pole proﬁles has shown [F20] that the presence of the mirror plate negatively aects the constancy of the vertical ﬁeld gradient for the isodynamic ﬁeld pattern. On the other hand, the constancy of the ﬁeld gradient in a magnetic system with constant vertical gradient improved by including the mirror plate. The position of the plate was found to have an inﬂuence on the magnetic characteristics of the circuit, particularly the constancy of the vertical ﬁeld gradient. For the GMUO FHS-40M separator, shown in Fig. 4.60, the optimum distance of the plate from the top of the pole pieces was about 28 mm. On the other hand, the thickness the plate did not aect the magnetic parameters.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

311

Figure 4.60: GMUO FHS-40M ferrohydrostatic separator with a mirror plate.

4.8.4

Scale-up of ferrohydrostatic separators

The application of ferrohydrostatic separation on production scale, particularly for the recovery of non-ferrous metals from automobile or electronic scrap, requires that separators with throughputs of at least 1 t/h, but preferably more, are available. In existing models of FHS, that are based on the iron-yoke concept with the air gap between the pole pieces, the increase in throughput can be accomplished by increasing the gap between the pole pieces. As has been discussed in Section 4.3, the increase in the length of the air gap results in an increase in the ampere-turns and thus of the mass, size and cost of the magnet. With ferrohydrostatic separators, the situation is aggravated even further by the fact that in order to maintain the required ﬁeld gradient, the necessary magnetic ﬁeld increases linearly with dimensions of the air gap. In other words, CK since = 2D for p = 2 (the constant gradient ﬁeld pattern), the magnetic C| ﬁeld strength, given by K = 2Du (eq. (4.71)), required to maintain this gradient, increases with u= The scale-up of a ferrohydrostatic separator by increasing the width of the air gap thus results not only in an increase in the magnetic ﬁeld, with attendant uneconomical increase in the volumes of iron and copper, but also in the increase of the height of the pole pieces well beyond the height of the pool of the ferroﬂuid required for e!cient separation.

312

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS y Separation chamber with ferrofluid

Feed x

z

Solenoid winding

Float

Sink

Figure 4.61: Schematic diagram of a ferrohydrostatic separator with a solenoid magnet [S56].

Solenoid-based FHS It is clear that the design of a large-throughput ferrohydrostatic separator must not be based on a simple increase of the air gap between the pole pieces. A natural approach to the scale-up of FHS would thus be to replace an iron-core magnet by a solenoid magnet as was proposed by Svoboda [S56]. Figure 4.61 illustrates such a solenoid-based FHS separator. A solenoid, and particularly an iron-clad solenoid, has numerous advantages compared to an iron yoke magnet. While it is necessary to increase the air gap in an iron yoke magnet in order to achieve an increase in throughput of material to be separated, with the attendant drawbacks mentioned above, the throughput of a solenoid-based separator can be increased by merely increasing the relevant transverse dimension (diameter) of the solenoid. The axial length (along the | - axis, as shown in Fig. 4.61) of the air gap and thus the number of ampere-turns required to generate a given magnetic ﬁeld remain constant. A solenoid allows the design of the magnetic ﬁeld pattern to be achieved in a simple and accurate manner. Such an approach facilitates the provision of a magnetic ﬁeld gradient which is constant, thereby enabling close control to be maintained over the apparent density of the ferroﬂuid and accordingly over the cut point density. This can be achieved, for example, by precisely designing the winding of the solenoid, or by varying the current density at dierent positions in the winding, or by using a multiple winding arrangement. This is in contrast

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

313

Feed Float 1

FHS 1

Sink 1

Float 2

FHS 2 Sink 2

Figure 4.62: A two-stage ferrohydrostatic separator with solenoid windings [S56]. to iron-core magnets, where approximate solutions of the Laplace equation are used to design approximate shape of pole tips, a task that is further complicated by non-linear magnetization characteristics of iron. The magnetic ﬁeld across the transverse dimension of a solenoid (along the { - axis) is homogeneous in a large region within the solenoid, which means that the same constant apparent density of ferroﬂuid can be achieved across the essentially full transverse dimension. Therefore, almost the entire diameter of the solenoid can be used for separation. This is in contrast to iron-core magnets where the constant gradient exists only at the plane deﬁned by the | - axis and considerable deviations from a constant gradient exist in the proximity of the pole tips. Because of the relatively small mass and size of a solenoid compared to an iron-yoke magnet, it is possible to arrange for two or more FHS units to provide for multi-stage separation, as shown in Fig. 4.62. In this arrangement the top unit, operating, for example, at the apparent density of 8000 kg/m3 > can ﬂoat zinc and sink copper and lead, while copper could be separated from lead into the ﬂoating fraction in the bottom separator operating at the apparent density of 9500 kg/m3 . Computer modelling of the solenoid-based FHS [S8] showed that it is fairly simple to achieve ﬁeld gradients of the order of 3 T/m in su!ciently large volumes of ferroﬂuid. It was also shown that the use of steel cladding considerably

314

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Grad B B B Grad B

Conventional U-dipole FHS

C-dipole FHS

Figure 4.63: U-dipole magnetic circuit versus C-dipole circuit.

increased this volume in both axial and radial directions. The modelling also conﬁrmed the technical and economic advantages of this design by the use of a superconducting solenoid.

C-dipole-based FHS The scale-up of a conventional iron-yoke-based ferrohydrostatic separator can also be accomplished by re-orienting the U-shaped magnet (Fig. 3.53), to form a C-dipole circuit, as shown in Fig. 4.63. Svoboda [S57] proposed the use of Cdipole magnet to generate a vertical magnetic ﬁeld, the pattern of which can be controlled by appropriate design of the magnetizing coils on upper and/or lower legs of the C-dipole, and/or by controlling the relative polarity of the electrical current ﬂowing through these coils. Appropriate shaping of the pole-tips of the upper and lower pole pieces can also be employed to create a required ﬁeld pattern. The scale-up of such a C-dipole-based separator can be accomplished by merely increasing the length of the magnet Op , and maintaining a constant length of the air gap Oj between the pole-pieces, as shown in Fig. 4.64. The magnetic ﬁeld along the length of the C-dipole is homogeneous, and the same magnetic ﬁeld pattern and apparent density of the ferroﬂuid, along the vertical axis, can be maintained along the full length of the magnet. One possible embodiment of such a concept of the C-dipole FHS is shown in Fig. 4.65.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

315

Figure 4.64: Schematic diagram of a ferrohydrostatic separator based on a Cdipole magnet [S57].

Figure 4.65: Schematic diagram of a ferrohydrostatic separator based on a Cdipole magnet [S57].

316

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.66: Magnetic circuit of an FHS separator with across-the-pole feeding system.

Figure 4.67: Separation process in the across-the-pole FHS concept [K19].

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

317

Figure 4.68: Layout of the ATP ferrohydrostatic separator [K19].

Figure 4.69: A pilot-plant ATP ferrohydrostatic separator (De Beers Consolidated Mines (Pty.) Ltd.)[K19].

318

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

"Across-the-pole" FHS An even simpler concept for overcoming the throughput limitation of the conventional U-pole design of FHS was developed at De Beers Consolidated Mines (Pty.) Ltd. [S8, K19]. By rotating the feed direction through 900 , the throughput increase could be achieved by lengthening the pole pieces rather than increasing the width of the air gap. Figure 4.66 gives a three-dimensional impression of this across-the pole (ATP) concept, while Fig. 4.67 gives a schematic description of the separation process. As can be seen, instead of feeding the material across the width of the air gap of the magnet, the particles are introduced into the ferroﬂuid across the poles. The ﬂoat fraction passes over one of the pole pieces, while the sink fraction is collected underneath in the bottomless separation chamber. An illustration of the layout of the separator is shown in Fig. 4.68. The width of the air gap is determined by the required residence time of material in the ferroﬂuid and remains the same for any length of the pole-pieces, and, therefore, for any throughput of the separator. The magnetic pattern and the apparent density of the ferroﬂuid are determined by the proﬁle of the pole tips, in the same way as in conventional FHS units. A view of the pilot-scale ATP separators is shown in Fig. 4.69.

Chapter 5

Practical Aspects of Magnetic Methods for Materials Treatment Magnetic separation is used in a wide spectrum of areas of material handling whose requirements dier considerably. In general terms, magnetic methods of separation are used in several distinct processes: • Magnetic ﬁltration - recovery of liquid (the magnetizable solids are discarded) - recovery of magnetizable solids (liquid is discarded). • Concentration of a valuable "non-magnetic" component of a mixture by discarding the magnetizable component recovered into the magnetic fraction. • Concentration of magnetizable component into the magnetic fraction and rejection of the "non-magnetic" waste. • Concentration of non-ferrous metals by discarding the non-metallic component of a mixture, and separation of individual non-ferrous metals into individual fractions. • Separation of materials into individual density fractions. The selection of the most appropriate magnetic technique to be used in a given application is a formidable task, and clear deﬁnition of the objective of the process is an important prerequisite for successful choice of the separation technique. 319

320

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

5.1

Selection of magnetic separation technique

There are numerous types of magnetic separators, each one being suitable for only a limited range of applications. The choice is inﬂuenced by a wide variety of factors and the successful operation of a magnetic separator depends, to a great degree, on practical experience. The results of separation cannot generally be accurately predicted. As with most other physical techniques of material treatment, magnetic separation cannot be successfully performed simply on the basis of theoretical models and experience is still the foundation. At present, there is no branch of magnetic separation where theoretical treatment of the subject could be considered entirely adequate. Each magnetic separation technique has its merits as well as limitations; no single technique is applicable to all applications of magnetic separation. The evaluation of magnetic separation as a means of beneﬁciation, or generally of recovering solids, liquids or gases, is often based solely on the data collected from a few brief tests, not always carried out in a suitable magnetic separator. The likelihood of disappointing results and even of rejection of the technique is high, in spite of adaptability and large scope of the magnetic methods of materials manipulation. The choice of magnetic equipment, and the selection of appropriate operating conditions dier widely between these processes. The mode of operation, namely wet or dry, and the throughput requirements impose additional complicating restrictions on the selection of the most suitable magnetic technique. Since particle size of the material to be treated is the most important variable that determines the selection of the magnetic separation technique, the general guidelines of the process selection are based on particle size distribution, as shown in Fig. 5.1. If the size of particles to be manipulated by magnetic separation is greater than, for example, 75 m, we have an option of a dry or wet process. If, however, the particles are ﬁner than 75 m, the wet technique is more appropriate, although this threshold particle size can be smaller or greater than 75 m, depending upon the amounts of the ﬁnes present in the feed and on the physical properties of the feed. The subsequent choice of the magnetic separation technique depends on the magnetic properties of the material. If a strongly magnetic component is present in the feed, low-intensity drum magnetic separators can be used, either in wet or dry modes of operation. Coarse, weakly magnetic materials can be treated by wet roll magnetic separators, rare-earth drum separators and possibly by wet high-intensity highgradient magnetic separators. In the latter technique, there is an upper limit imposed on the particle size by the type of the matrix and particles greater than 1 mm usually cause clogging, even of a coarse matrix. In a dry mode, coarse weakly magnetic particles can be recovered by a variety of high-intensity magnetic separators, including induced magnetic roll, cross-

5.2. DRY MAGNETIC SEPARATION

321

Strongly magnetic

LIMS, Chute

Weakly magnetic

Wet roll MS, WHIMS, HGMS, REDs

Strongly magnetic

LIMS, Suspended, Pulley, Grate, Roll MS

Weakly magnetic

Roll, REDS, Cross-belt, IMR, OGMS, HGMS

Strongly magnetic

LIMS

Weakly magnetic

REDS, WHIMS, HGMS

Wet

> 75 µm

Dry Particle size

< 75 µm

Wet

Figure 5.1: Classiﬁcation of magnetic separation processes (adapted from Svoboda [S1]). belt separator, permanent magnet roll separator, rare-earth drum separator and open-gradient magnetic separator. If the particles are ﬁner than 75 m, the best approach is to use wet magnetic separation. Fine, strongly magnetic particles are usually recovered by wet lowintensity drum separators, while for weakly magnetic materials the wet highintensity or high-gradient magnetic separation is appropriate. The decision making process for selection of the magnetic separation technique is schematically shown in Fig. 5.2.

5.2

Dry magnetic separation

Dry magnetic separation is a technique dating back to the beginning of the last century. It has been practiced successfully in the removal of tramp iron from process streams, in beneﬁciation of strongly magnetic minerals, as well as feebly magnetic minerals such wolframite, cassiterite or ilmenite. Puriﬁcation of numerous industrial minerals, such as andalusite, glass sand, ﬂuorspar, feldspar, diamonds and others, by removing ﬁne strongly magnetic impurities, is very often carried out in a dry mode. More recently developed eddy-current separators also operate in a dry mode. For dry magnetic separation to be successful, the material must be com-

322

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Magnetic separation

Yes Wet MS

Particle < 75 um No

No

Strongly magnetic?

Is dry process required?

Yes

Yes Dry MS

No LIMS

Yes Wet MS

WHIMS HGMS

Strongly magnetic? No

Yes

Strongly magnetic? No

LIMS Plate Chute

WHIMS HGMS REDS Wet roll

IMR Roll REDS Cross-belt Disc OGMS HGMS

LIMS Pulley Suspended Grate Plate Roll

Figure 5.2: Selection of magnetic separation techniques (adapted from Svoboda [S1]).

5.2. DRY MAGNETIC SEPARATION

323

pletely dry, which sometimes involves an expensive heating stage. For particles smaller than a certain threshold size (for instance 75 m), the attractive electrostatic and van der Waals forces will cause sticking and the formation of aggregates. Selectivity of separation can thus be severely aected. Dry processes often require the material to be sized into several rather narrow size fractions, each of which must be spread in a monolayer over the separating surface. It is a well-established fact that when magnetic separation is performed on materials sized into, for example, three or more fractions, the e!ciency of separation is usually much improved in comparison with unsized samples. The loading of the separating surface, such as belt or drum, inﬂuences the throughput and the e!ciency of the separation, and a compromise must be found between these contradictory requirements. As a rule of thumb, when the particles are introduced onto a belt in a monolayer, a safe belt loading (portion of the belt covered with feed particles) should be approximately 25%, even when the feed contains a high percentage of the magnetic material. As a rule, a larger proportion of dry ﬁnes necessitates higher rotating speeds of a roll or drum. Although increase in speed will improve the grade of the magnetic product and the throughput of the separator, it will also increase the losses of the magnetic component. The recovery can be improved by re-treating the non-magnetic fraction in a second stage. On the other hand, when the valuable product is the non-magnetic fraction, high speed of rotation will result in high recovery and poor selectivity of separation. The grade of the concentrate can be improved by cleaning the non-magnetic fraction in the second pass.

5.2.1

Electrostatic phenomena in dry separation

During dry material handling operations, the dielectric particles invariably become electrostatically charged. The dominant charging mechanisms are triboelectriﬁcation (or frictional charging) and contact charging. These mechanisms can happen during any dynamic contact of surfaces, such as sliding, rolling and vibration of surfaces at contact. When two dissimilar dielectric materials make and then break contact, charge transfer from one of the materials to the other takes place. This is not to say that conductors will not charge by contact electriﬁcation - they usually charge - but since they are conductors, they often lose their charge quickly. While physical mechanisms of contact charging are well understood, triboelectriﬁcation, the oldest form of charging, is poorly understood and explanations are of phenomenological nature. One of the controversial rules of thumb often used for predicting the sign of the surface charge resulting from contact electriﬁcation is Coehn’s rule, which states that "when two dielectric materials are contacted and separated, the material with the higher dielectric constant becomes positively charged" [L12]. Coehn’s rule was quantitatively formulated as v = 15 × 106 (u1 u2 ) (5.1) where v is the surface charge density (in [F/m2 ]) and u1 and u2 are dielectric

324

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.1: Dielectric constants of selected materials. Material Water TiO2 Barium titanate Carbon Ilmenite Chromite Rutile Zircon Glass Quartz Hematite Limestone Fluorspar Bakelite Perspex

Dielectric constant u 80.4 90 1200 5.7 33.7 to 81 11 89 to 173 12.6 4 to 6 4.3 25 6.1 7.4 4.9 3.4

constants (relative permittivities). Although Coehn’s rule is reported to have been veriﬁed for more then 400 substances [L12], it is of limited value to the metallurgist because of the difﬁculty in determining the relative permittivities of the surface layers of two materials that are to make contact. Typical values of dielectric constant of selected materials are shown in Table 5.1. Sometimes several materials can be arranged into the so-called triboelectrical series such that each material is charged positively when it is rubbed against the previous one. Examples of such series are: • zinc-glass-cotton-ﬁlter-paper-silk-zinc [B26] and • teﬂon-metals-resins-wood-mica-quartz-glass [H19]. The triboelectric charging behaviour of materials is generally sensitive to an atmospheric environment. At high values of relative humidity, considerable negative charging takes place. At low values of relative humidity, although ﬁne particles still charge negatively, the coarse particles show a change of charging polarity such that the net charge conveyed by the powder material is positive [B27]. When a particle undergoes charging during handling, the charge transferred at the particle contact point will re-distribute itself over the particle surface by electrostatic forces. The rate at which re-distribution proceeds depends on the relaxation time h (in [s]) given by h = u 0 (

(5.2)

5.2. DRY MAGNETIC SEPARATION

325

Figure 5.3: The eect of moisture on the grade of the magnetic concentrate obtained from - 2 mm magnetite and martite ores treated by crossbelt and induced magnetic roll separators (adapted from [D4]). where ( is the resistivity of the material (in [ m]) and u its relative permittivity (dielectric constant) and 0 = 8.85×1012 F/m is permittivity of vacuum. The time dependence of the surface charge density, after completion of the charge transfer, is given by: v = 0 exp([email protected] h )

(5.3)

where 0 is the surface charge density at w = 0. As a general rule, if electrostatic phenomena arise in a material handling situation, they are likely to become increasingly signiﬁcant as particle size decreases. Particles charged triboelectrically, either positively or negatively, may adhere strongly to surfaces. Moisture contributes to the strength of adhesion and Fig. 5.3 illustrates the eect of moisture on selectivity of dry magnetic separation. It can be seen that the grade of the magnetic concentrate is seriously impaired by the presence of moisture and the permissible moisture content decreases with decreasing particle size. For instance, if an ore with size distribution - 20 mm can tolerate 4% of moisture, then the maximum moisture content in a ﬁne ore - 2 mm should not exceed 1% [D4]. The eect of air humidity The moisture concentration in an ore is also inﬂuenced by the relative humidity of the air. This is a consequence of the capillary attraction between particles, which results in adsorption and subsequent capillary condensation of the water vapours in the particle contact area. If the force of capillary attraction Ik

326

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.4: The eect of air humidity on dry magnetic separation of magnetitequartz mixtures, for dierent values of particle radii (adapted from [V10]). between a non-magnetic particle and a magnetic particle is greater than its weight J, the non-magnetic particle will report in the magnetic fraction. The force Ik is the sum of of the surface tension and the Laplace pressure force: Ik = 8u1 + 4u22 (

1 1 ) u2 u1

where ul (l = 1 and 2) are the radii of the curvatures of the meniscus between the contacting particles 1 and 2, and is the surface tension (in N/m) of the ﬂuid. Experimental investigation [V10] of the eect of the air humidity on dry magnetic separation of magnetite-quartz mixtures, as a function of particle size, conﬁrmed that the e!ciency of separation varies linearly with the ratio J/Ik = It can be seen from the results illustrated in Fig. 5.4 that with increasing humidity, the separation e!ciency decreases steeply. The eect of the air humidity becomes particularly pronounced with decreasing particle size.

5.2.2

Density and magnetic tracers

The use of the Tromp curve, or partition curve, is a well established practice for the evaluation and representation of gravity concentration processes. The partition curve can be conveniently constructed with the aid of density tracers [N15]. The density tracers are manufactured as cubes in sizes ranging from 0.8

5.2. DRY MAGNETIC SEPARATION

327

to 20 mm. They are colour-coded according to the magnitude of their density and are commercially available, for example from Bateman Engineering (Pty.) Ltd. (South Africa), in the density range from 1300 kg/m3 to 4000 kg/m3 , with density interval of 50 kg/m3 . Partition Enterprises (Pty.) Ltd. (Australia) supply density tracers that are strongly magnetic for easy recovery, by magnetic means, from density separation products. The partition number, or the percentage recovery U into the concentrate, for each size and density fraction, is usually determined as U = 100

qf qf + qw

where qf and qw are the numbers of tracers in the concentrate and in the tailings, respectively. Magnetic tracers, which have become commercially available only recently, can be used, in a fashion similar to the way density tracers are used in gravity concentration, to determine and optimize the separation e!ciency of magnetic separators. A magnetic tracer is a simulant designed to have the same size and magnetic susceptibility as the material which is being recovered or removed in a magnetic separator. Magnetic tracers of mass magnetic susceptibility ranging from 2.5×107 m3 /kg to 125.5×107 m3 /kg (20×106 cm3 /g to 1000×106 cm3 /g), in steps of 2.5×107 m3 /kg, for low-susceptibility tracers, and 12.5×107 m3 /kg for high susceptibility tracers, are available from Bateman Engineering (Pty.) Ltd., South Africa [D12]. These tracers, whose size ranges from 1 mm to 20 mm, are colour- and shape-coded, according to the magnitude of their magnetic susceptibility for easy evaluation of the separation process. Tracers smaller than 1 mm are impractical as they cannot be easily identiﬁed among the mineral particles. The magnetic partition curve can be constructed using the partition numbers, or percentage recovery into magnetic or non-magnetic fractions. In terms of the recovery of the tracers into the magnetic fraction, for example, the partition number, for a given size and magnetic susceptibility, is expressed as: U = 100

qpdj qpdj + qqrqpdj

where qpdj and qqrqpdj are the numbers of tracers in the magnetic and nonmagnetic fractions, respectively. The probable error of separation is given by eq. (4.58). While magnetic tracers are ideally suited for quantiﬁcation of the e!ciency of a magnetic separation process, their practical use is restricted to the separation of materials coarser than 1 mm. Although they can be used to evaluate the e!ciency of separation of even ﬁner materials in dry separators such as roll and drum, the particle-size dependence of the magnetic susceptibility cut point can result in considerable inaccuracy of the audit. In wet separators, such as low-intensity drum separators or WHIMS or HGMS, even the smallest 1 mm magnetic tracers would interfere with the separation process

328

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.5: Comparative metallurgical e!ciencies of various dry magnetic separators as applied to apatite recovery (adapted from Roux et al. [R19]).

5.2.3

Comparison of dry magnetic separation techniques

The minerals industry has always had a great need to beneﬁciate coarse, weakly magnetic minerals and a wide spectrum of dry magnetic separators has been developed over the years. The range of various types of separators, based on dierent principles of the generation of the magnetic ﬁeld, makes a correct choice of the most suitable technique a di!cult task. Comparisons of the separation e!ciencies of dierent techniques are usually not published and if they are, caution should be exercised when taking these comparisons at face value. Every comparison is only conditional since the relative merit of each technique is a function of the mineral to be treated and its physical properties. Sometimes comparisons are oered by manufacturers of magnetic separators who might be biased towards their own product. Comparison of dry separators for beneﬁciation of the pyroxenite ore One of the rare comprehensive comparative production-scale exercises was conducted by Roux et al. [R19]. In order to beneﬁciate pyroxenite ore to yield apatite concentrate, several dry magnetic separators were tested at Foskor (South Africa). Figure 5.5 summarizes the metallurgical e!ciencies of dierent types of separators, while Fig. 5.6 shows the relationship between phosphate recovery and particle size for IMR, HGMS and OGMS machines. A thorough practical experience with these magnetic separators was gained at Foskor and their

5.2. DRY MAGNETIC SEPARATION

329

Figure 5.6: Phosphate recovery as a function of particle size for various magnetic separators (adapted from Roux et al. [R19]). comparison is summarized in Table 5.2. A gradual deterioration in the results was observed with IMR, caused by abrasive wear on the epoxy ﬁller between the steel discs of the rolls. Furthermore, because the separation distance between the magnetics and non-magnetics is very small, a precision setting of a splitter was required. As the mineralogy of the ore varies, constant attention to the optimization of roll speed and splitter settings was required, which made it di!cult to maintain good metallurgy [R19]. A Sala HGMS 120-15 operated reliably and well for 1000 hours and it was found that single-stage separation yielded metallurgical results equivalent to that of two stages of IMR separation. The expanded metal matrix showed no measurable wear, while the metallurgy was shown to be adversely aected by oversize material, which gradually accumulated in the matrix. In order to keep coarse particles out of the feed, and to avoid the onerous task of cleaning the matrix chambers, it became necessary to ﬁt a second screen which could be kept under continuous visual observation. An extensive series of experiments with SmCo permanent roll separators showed that the feed rate, roll speed and thickness of the magnet and steel rings must be optimized for each separation stage. The open-gradient, split-coil superconducting magnet separator was tested in two modes, shown in Chapter 2 in Fig. 2.85(a) and (b). The free-fall system gave acceptable metallurgical results only at very low feed rates. A much more satisfactory ore presentation system was found to be the one in which the ore slid down a ramp, as shown in Fig. 2.85(b). The ramp imparts an outward

330

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.2: Comparison of dierent types of dry magnetic separators, as applied to phosphate recovery (after Roux et al. [R19]). Parameter Capacity Power input Ore distribution Mass [kg] per t/h of feed Sensitivity to ore variation Recovery of the ﬁnes

IMR Low, 4 t/h/m 2 kW/t Complex 2200

RE Roll Low, 8 t/h/m 0.6 kWh/t Complex 440

HGMS High, 400 t/h 5.6 kWh/t Simple 4100

OGMS High, 60 t/h

High

Low

Low

Very high

Poor

Very poor

Good

Very poor

0.5 kWh/t Simple 41

Table 5.3: Comparison of IMR and RE roll in ilmenite-rutile separation (after Arvidson [A26]). Product Magnetics (mass %) Non-mags in mags (%) Middlings (%) Non-magnetics (%) Mags in non-mags (%)

IMR @ 2.5 t/m/h 25 2.5 10 65 0.5

RE roll @ 4 t/h/m 30.5 0.46 0.8 68.7 0.28

velocity to the particles, thereby counteracting, to a considerable extent, the sweeping across of non-magnetic particles by the magnetic ones. This approach made it possible to obtain metallurgical results comparable with those of IMR separators, at feed rates of up to 6 t/h per meter width, or 3.5 times the optimum feed rate of an IMR. Comparison of dry separators for beneﬁciation of beach sands and other industrial minerals. High-intensity magnetic separation has been a standard beneﬁciation method for heavy mineral sands and various industrial minerals, and a variety of dry magnetic separators has been used. With the advent of aordable rare-earth permanent magnets, and as a result of design improvements, the conventional dry separators, such as induced magnetic roll and cross-belt separators are being replaced by reliable and economical rare-earth roll and drum separators [A24, A25, A26]. Although the plant data are usually conﬁdential, comparative studies indicate superior performance of the rare-earth-based separators. An example is shown in Table 5.3, which compares the separation e!ciency of IMR and RE roll separators as applied to ilmenite and rutile separation. A similar improvement in the e!ciency of separation after replacing the induced magnetic roll with a permanent magnetic roll, was obtained with feldspar.

5.2. DRY MAGNETIC SEPARATION

331

Table 5.4: Comparison of IMR and RE roll magnetic separation as applied to beneﬁciation of feldspar [A24]. Product Magnetic fraction Non-magnetic fraction

IMR 12% - 14% 86% - 88%

RE Roll 4% - 4.5% 95.5% - 96%

Table 5.5: Reduction of the iron content in various size fractions of feldspar, by IMR and roll permanent magnetic separators. IMR was operated at 1.8 T [A27]. Separator

Fraction [m]

Fe oxides in feed [%]

IMR

- 500 + 212 - 212 + 106 - 106 + 74 - 500 + 212 - 212 + 106 - 106 + 74

0.20 0.43 0.45 0.20 0.43 0.45

Roll

Yield into non-mags [%] 95.5 93.0 82.3 86.6 85.8 79.5

Fe oxides in non-mags [%] 0.04 0.06 0.07 0.08 0.10 0.11

This is shown in Table 5.4. On the other hand, results of another comparative study [A27], summarized in Table 5.5, indicate a superior performance of an induced magnetic roll, in the entire range of particle sizes. Dry magnetic separators can also be e!ciently used to recover metal from slags. Comparison of several dry separation techniques to recover ferrochrome from coarse slag is shown in Table 5.6 [S58]. A dry ferrite roll separator was also successfully applied to the recovery of the ferrochrome metallics from a ﬁne fraction (- 0.8 mm) of slag. Comparison of its performance with a wet rare-earth drum separator is shown in Table 5.7. Replacement of conventional electromagnet-based separators by rare-earth permanent magnet units also often results in economic advantages. Improved quality of the ilmenite concentrate and reduced operating costs contribute to improved plant e!ciency, as shown in Table 5.8. Additional cost savings result

Table 5.6: Recovery of ferrochrome metal from slag (- 15 + 2 mm) by magnetic separation [S58]. Separator Dry LIMS Lifting IMR Ferrite roll

Head grade [ FeCr %] 22.7 20.1 27.1

Mags grade [ FeCr %] 60.6 77.6 45.7

Recovery [%] 85.0 85.8 97.5

332

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.7: Recovery of ferrochrome metal from ﬁne slag (- 0.8 mm) by magnetic separation [S58]. Separator Ferrite roll Wet RE drum

Head grade [ FeCr %] 4.4 4.7

Mags grade [ FeCr %] 16.9 17.3

Recovery [%] 65.6 70.2

Table 5.8: Comparison of the operating costs of various dry magnetic separators applied to ilmenite beneﬁciation, in relation to a cross-belt separator [A24]. Magnetic separator Cross-belt IMR RE drum separator RE roll (short belt life) RE roll (long belt life)

Cost 100 42 to 53 17 21 to 42 11 to 15

from a smaller size of the plant for a given throughput. Since a plant with rare-earth magnetic separators would use between 6% and 20% of a cross-belt plant space [A24], the cost saving can be considerable. Compared to IMR for non-magnetic cleaning applications, the space saving can be 50% to 70% [A24]. Improved performance can be also obtained by implementing multiple-stage separation, as is demonstrated in Fig. 5.7. Combined with higher roll speeds, the selectivity of separation increases in addition to a higher throughput. In some applications, it was found advantageous to combine rare-earth roll separators with rare-earth drum separators. While roll separators tend to be more e!cient, more selective and can be more readily adjusted to feed variations, drum separators have a higher throughput and are less demanding from the maintenance point of view. Comparison of the roll and roll+drum options is shown in Table 5.9.

Table 5.9: Comparison of roll and roll+drum alternatives for treatment of ilmenite gravity concentrate (- 0.9 + 0.1 mm), at 30 t/h, in 1999 prices [A25]. Parameter Stages required Capacity Quantity Price per unit [US$] Total price [US$]

Drum + Roll 1 drum + 2 rolls 7 t/h/m 3 $114 000.00 $342 000.00

Roll separator only 3 stages 4 t/h/m 5 $65 000.00 $325 000.00

5.2. DRY MAGNETIC SEPARATION

333

Figure 5.7: Comparison of single and multiple-pass separation of ilmenite, by a roll separator, at dierent feed rates (adapted from Arvidson [A26]). Comparison of roll and matrix separators Jirestig and Forssberg [J7] carried out a detailed comparative study of four dry high-intensity magnetic separators. Three of these separators were roll units: R R ° ° Permroll (E.L. Bateman) with Kevlar belt, High Force (Inprosys) with polyurethane belt, induced magnetic roll (Humboldt Wedag) and dry HGMS (Sala). An expanded metal matrix, with and without spacers, was used in the Sala HGMS and particles were propelled through the matrix by a compressed air-driven vacuum pump. Various size fractions of calcite and dolomite samples were used as test materials. Permroll, High force and dry HGMS, operating at 2 T yielded products of similar brightness for ﬁne to medium-size (- 450 + 38 m) particles, as can be seen in Fig. 5.8. For particles larger than 450 m, the Sala HGMS machine experienced problems with matrix clogging, while the e!ciency of the induced magnetic roll was slightly inferior. The signiﬁcant advantage of the matrix separator, compared to belt-type separators, is its high selectivity of separation of ﬁne particles, smaller than 100 m. The high brightness of products from belt separators was achieved at great cost to the recovery. Only about 5% of 38 m material reported to the magnetic fraction in the matrix separator, while Permroll and High Force machines experienced signiﬁcant losses (35% to 80 %) of the valuable material into the magnetic tailings. The dierent performances of the two belt separators are probably due to dierent types of belts used and the results indicate the importance of controlling electrostatic properties of the belt material, as discussed in Section 5.2.1.

334

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.8: Brightness of various size fractions of the calcite non-magnetic product, as obtained in several dry magnetic separators (adapted from Jirestig and Forssberg [J7]). Comparison of rolls of dierent diameters Magnetic rolls of diameter ranging from 72 mm to 300 mm are commercially available and judicious selection of the most suitable unit is essential for optimum metallurgical results and operating costs. Figures 5.9 and 5.10 illustrate that magnetic rolls of larger diameter (300 mm) can operate at higher feed rates than standard 76 and 100 mm diameter rolls. By increasing the speed of rotation the same performance can be maintained. As has been discussed in Section 4.6.2, the magnetic force is practically independent of the magnetic ring diameter. The increase in the rotational speed of the roll, maintaining the same residence time of particles in the magnetic ﬁeld as in a smaller diameter roll, results in the increase of the centrifugal force on a particle. In turn, this results in a closer balance of the magnetic and competing forces and better selectivity of separation can thus be obtained. This additional beneﬁt of larger ring diameters is depicted in Fig. 5.10. Comparison of RE roll and RE drum separators Rare-earth roll separators and rare-earth drum separators are designed to address similar beneﬁciation applications. The choice between these two types of separators is rarely made on the basis of comprehensive comparative tests. Since the pattern of the magnetic force around the roll and drum dier considerably, correct systematic evaluation of the operation is essential. As has been discussed in Section 4.6.2, magnetic roll separators generate a much higher mag-

5.2. DRY MAGNETIC SEPARATION

335

Figure 5.9: Comparison of separation e!ciencies of magnetic rolls of diameters 100 and 300 mm, at dierent throughputs, as applied to beneﬁciation of - 3 mm iron ore (adapted from Arvidson and Dillé [A23]).

Figure 5.10: Comparison of performances of 76 mm and 300 mm rolls at dierent speeds of rotation, applied to puriﬁcation of - 600 + 800 mm silica sand (adapted from Dobney [D8]).

336

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.11: Magnetic partition curves. The ideal curve corresponds to a magnetic susceptibility cut-point of "50 = 80×106 cm3 /g (10×107 m3 /kg) [M24].

netic force, which, however, is of short reach. On the other hand, the magnetic force on the surface of a drum separator is much lower, as a result of a considerably lower magnetic ﬁeld gradient. The reach of the force is, however, much longer than that in a roll separator. The behaviour of particles in these two types of separator is dierent and the settings of the optimum operating conditions dier widely. Detailed comparative tests on rare earth roll and drum separators were conducted by Murariu and Svoboda [M24]. Magnetic tracers of various sizes and mass magnetic susceptibilities were used to set the optimum operating conditions, and magnetic partition curves were generated. The values of Hs, given by eq. (4.58), of these curves were compared. Figure 5.11 illustrates such a partition curve for the cut-point magnetic susceptibility of 80×106 cm3 /g (10×107 m3 /kg). The cut-point is deﬁned as the value of magnetic susceptibility ("50 ), for which the particles having this susceptibility split equally into the magnetic and non-magnetic fractions. It was observed that the same cut point could be obtained using dierent combinations of the speed of rotation of the drum or roll and of the position of the splitter. However, not all combinations of these parameters give the same optimum e!ciency of separation, as is demonstrated by Fig. 5.12. It can be seen that, for a drum separator, a lower speed and a closer position of the splitter between the magnetic and non-magnetic fractions, result in lower Hs and thus

5.2. DRY MAGNETIC SEPARATION

337

Figure 5.12: Experimental partition curves for an NdFeB drum magnetic separator. The curves were obtained for the same value of the cut point, but for dierent positions of the splitter and the rotational speed of the drum. Drum diameter: 600 mm, magnetic induction on the drum surface: 0.9 T [M24]. a more e!cient separation. However, with a roll separator (diameter 100 mm), a more selective separation was achieved at a high roll speed and with a splitter far from the roll. This dierence in the optimum operations of drum and roll magnetic separators results from the fact that the magnitude of the magnetic force acting on a particle in a drum is much smaller than that in a roll separator. As discussed in Section 1.2, the separation is selective when the magnitudes of the magnetic force and the competing forces are of comparable magnitudes. The magnetic roll, which generates a higher magnetic force than the drum, requires a higher centrifugal force (i.e. a higher roll speed) and a more distant position of the splitter. Tracer tests showed that the setting of the cut point, that is of the rotation speed of the roll or drum and position of the splitter, is dependent on particle size. The size dependence was found to be approximately linear for both separators, as is illustrated in Fig. 5.13. The slope of the plots indicates sensitivity of a separator to the size of the tracers. It can be seen that roll magnetic separators are considerably more sensitive to particle size and the sensitivity increases with decreasing thicknesses of the magnet and steel rings. A roll separator of a given conﬁguration is, therefore, suitable for accurate separation of only a narrow size range of the feed particles. For example, if the cut point is set to 10×107 m3 /kg (80×106 cm3 /g) and the required accuracy is ± 10% (two horizontal lines in Fig. 5.13), a roll separator with conﬁguration 12/7.5 will satisfy the accuracy

338

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.13: Variation of the cut-point magnetic susceptibility with the size of magnetic tracers, for roll and drum magnetic separators of dierent conﬁgurations [M24].

requirement for a size fraction - 6 + 4 mm. A roll separator with conﬁguration 4/2.5 will meet this requirement only for particle size of 2 mm. On the other hand, the drum separator will be able to treat selectively a size fraction of - 16 + 8 mm.

The loading of the belt or the drum The loading of the drum and of the belt of the roll separator, inﬂuences the throughput and the e!ciency of separation, and a compromise must be found between these two contradictory requirements. As a result of a short residence time of particles on the roll surface, the feed material must be distributed evenly over the belt in a monolayer and a safe belt loading is approximately 25%. Lower belt loadings lead to a low throughput and generally cannot be justiﬁed in view of a limited beneﬁt and high cost of the separator. In drum separators, the residence time is much longer and if the feeding system is optimized and the feeder tray is su!ciently close to the drum, to avoid particle bouncing, the particles usually spread evenly on the drum surface even when particles ﬂow in a thicker layer on the feeder tray. Typical ﬂow of material onto a drum surface is shown in Figs. 5.14 and 5.15. However, adherence of strongly magnetic particles on the drum surface can be a problem, as shown in Fig. 5.16.

5.2. DRY MAGNETIC SEPARATION

339

Figure 5.14: Flow of the - 2 + 1 mm material on the surface of an NdFeB drum magnetic separator.

Figure 5.15: Flow of the - 16 + 8 mm material on the surface of an NdFeB drum magnetic separator.

340

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.16: Attachment of strongly magnetic particles to the surface of a drum magnetic separator. Throughput of a roll separator The throughput of a roll separator is determined by a variety of factors and only experimental determination can give reliable information on this important speciﬁcation. The general formula for throughput calculation is Ys s zyi F= (5.4) Ds where F is the throughput (in [kg/s]), Ys is the particle volume (in [m3 ]), s is the particle density (in [kg/m3 ]), z is the belt width (in [m]), y is the belt speed (in [m/s]), Ds is the cross-sectional area of a particle (in [m2 ]) and i is the ﬁlling factor of the belt. It is evident from this equation that the shape of the particles must be known before the throughput can be calculated. Belt tracking As the belts used in roll magnetic separators are frequently very thin, usually between 0.13 mm and 0.25 mm, they are prone to wear and their life time is often short. Accumulation of dust and magnetic particles underneath the belt and misalignment of the belt, result not only in impaired separation performance but also cause damage to the belt. Various manufacturers of roll separators use dierent mechanisms for the belt tracking, with dierent levels of resistance to misalignment. Considerable eort has been expended to extend the wear life by developing and applying correct tracking system. Crown idler rolls have been used successfully for many years, particularly for small diameter rolls and for separators with a large distance between the

5.2. DRY MAGNETIC SEPARATION

341

Figure 5.17: The temperature of the shell of an NdFeB drum magnetic separator, as a function of time. Drum diameter: 600 mm, magnetic induction on the shell: 0.9 T, speed of rotation: 50 rpm [M24]. roll and the idler. With the advent of large diameter rolls (e.g. 300 mm), the conventional crowned idler system has been replaced, for rolls longer than 0.5 mm, by a self-adjusting roller system [A23, A13]. Depending on the application, the average lifetime of a thin belt (0.13 mm) ranges from one month to six months, while a thicker belt (0.25 mm) can last as long as 12 months [A24]. The changing of a damaged belt can also be an onerous and time-consuming exercise. It is claimed, however, that the belt changing time for a one meter long roll can be shorter than 5 minutes [D8]. Eddy currents and temperature increase in the drum shell It has frequently been observed that the temperature of the shell of drum magnetic separators increases during operation. This phenomenon is based on the fact that as the metallic shell of a drum separator rotates around a stationary magnetic system, eddy currents are developed in the shell. These eddy currents are generated in such a way that the magnetic ﬁeld they produce opposes the external magnetic ﬁeld, as discussed in Section 2.7. This interaction energy is converted into heat which might be detrimental to operation of a drum magnetic separator and it could reduce the lifetime of the permanent magnet material. This is of particular importance for high-ﬁeld rare-earth drum separators which are often operated at higher rotational speeds than low-intensity magnetic drum separators. Figure 5.17 illustrates the temperature development on the surface of the shell of an NdFeB drum separator [M24]. The temperature was measured by

342

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

a thermocouple as a function of time over a period of eight hours. The temperature increased rapidly within the ﬁrst 30 minutes of operation from the room temperature of 24 0 C to 36 0 C. Afterwards, the temperature kept increasing asymptotically to the temperature of 45 0 C, which remained constant after eight hours. While the temperature within the permanent magnet material inside the drum will be higher than on the shell surface, it is probably still well below the critical operational temperature of the permanent magnet material. Nevertheless, caution should be exercised in this aspect. The eect of the increased temperature of the magnetic system on the separation e!ciency was investigated using 8 mm magnetic tracers and - 4 + 2 mm kimberlite gravel [M24]. It was found that the experimental partition curves determined at room temperature and after six hours of the drum operation, exhibited the same cut-point magnetic susceptibility. Also, the mass recoveries of the gravel into the magnetic fraction were identical, indicating that the separation e!ciency was not aected by the increased temperature of the drum.

5.3

Wet magnetic separation

As shown in Fig. 5.1, wet magnetic separation can be applied to coarse as well as ﬁne particles, that are either strongly or weakly magnetic. Strongly magnetic materials can be recovered by wet low-intensity machines, which are by far the most common in use. Weakly magnetic particles, coarse or ﬁne, can be treated by rare-earth drum magnetic separators, while wet high-intensity magnetic separators (WHIMS) and high-gradient magnetic separators (HGMS) are applied, as a rule, to ﬁne weakly magnetic materials only.

5.3.1

Wet low-intensity drum magnetic separation

Wet low-intensity drum magnetic separators (LIMS) are used to recover strongly magnetic solids from a slurry feed. The major areas of application are media recovery in dense media separation plants (DMS) and in magnetite ore beneﬁciation. Physical construction of wet drum separators is slightly dierent for the two applications, with the ore concentrator being more rugged in construction and subject to more detailed speciﬁcations than the media recovery units. This is particularly true with reference to feed and collection tank design, bearing construction, wear covers on the drums, magnet assembly design and magnetic ﬁeld strength rating. On the other hand, modern LIMS machines for DMS plant operation have a longer pick-up zone [D13], compared to the conventional separators. Wet magnetic drum separators for media recovery In media recovery application the particle size of the feed, particularly the magnetic portion, is quite ﬁne and drum wear is not a serious problem. Maximum magnetic recovery is important, and the highest magnetic purity and solids content in the magnetic concentrate is desired.

5.3. WET MAGNETIC SEPARATION

343

Table 5.10: Maximum concentration of solids in the feed into LIMS for dense media recovery [S59]. Separator Con-current Counter-rotation Double drum

Max. solids concentration [% by weight] 20 25 50

Factors that are considered in selecting a wet drum separator for media recovery are: • Percentage of solids in the feed slurry • Percentage of magnetics in the feed solids • Grade of the media used • Feed volume (m3 @h) to the separator • Magnetic discharge rate (t/h) from the separator • Desired magnetic recovery. Media recovery magnetic drums are available in diameters of 762 mm (30"), 914 mm (36") and 1219 mm (48"), and in drum widths up to 3050 mm (120"). A 1200 mm diameter magnetic separator has approximately twice the capacity of a 900 mm unit. This allows circuits to be designed with fewer magnetic separators and therefore with reduced vulnerability to mechanical failure, uneven feed distribution and poor control [D13]. Both con- and counter-current feed arrangements have been used. The concurrent drum arrangement usually gives the highest magnetic content in the magnetic discharge and provides the highest percentage of solids in the discharge. The overwhelming majority of the magnetic separators installed in DMS plants has been of the con-current design. The counter-rotation units have been used successfully as secondary separators [D13]. Solids content in the feed For e!cient operation of the DMS plant it is desirable to keep the media as free of ﬁnes as possible. The reduced concentration of ﬁnes limits the viscosity problem and results in sharper separation. It also improves the magnetic recovery by the magnetic drum and gives a cleaner magnetic concentrate. Typically, a single LIMS will be used in plants where the feed solids are in the 10% to 15% range. It is signiﬁcant to note that an extremely dilute feed makes the magnetic recovery more di!cult and the feed volume should be reduced by a factor of 0.5 to 0.75 for such a dilute feed [B28, M26]. For solids in the 20% to 25% range, either 900 mm diameter single drum or 760 mm diameter double drum units are recommended. Above 25% solids, 900

344

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.11: Recovery of ferrosilicon in a magnetic separator at low concentration of the magnetics in the feed [D13]. Mags in the feed [g/c] 55 38 5 2 0.5

Recovery [%] 98.8 98.0 92.0 67.0 56.0

Mags in e"uent [%] 0.83 0.76 0.40 0.67 0.22

Table 5.12: Suggested feed volumes into LIMS for dense media recovery [B28, M26]. Separator 762 mm single drum 914 mm single drum 762 mm double drum 914 mm double drum

Feed rate [m3 /h/m] 50 - 55 55 - 70 55 - 70 70 - 95

mm diameter double drum are advised. The suggested maximum concentrations of solids in the feed are shown in Table 5.10. Magnetic content of the feed solids Typically, the magnetic content of solids will be 60% or higher. When the magnetic content of the solids falls below 60%, the feed volume should be reduced and multi-drum arrangement considered, in order to maintain a high magnetic recovery. Table 5.11 illustrates the detrimental eect of low concentrations of the magnetics on their recovery. It is well established that the magnetics-to-ore ratio and the solids content are two parameters that control concentrate purity most eectively [S59]. Recommended feed volume and discharge rate of the magnetics In selecting drum size for media recovery, the feed volume and magnetic solids discharge should be balanced. In Table 5.12. typical feed rates are suggested for various single and double wet low-intensity magnetic separators. Magnetic discharge rates should not exceed the rates given in Table 5.13, in order to maintain high magnetic media recovery. The eect of the magnet position Plant experience conﬁrms that the initial settings of a drum magnetic separator, recommended by manufacturers, are only a rough guide. Settings of such parameters as the magnet position and drum-to-tank clearance should be optimized based upon the plant experience. For instance, it was found by Dardis [D13] that the magnet position signiﬁcantly inﬂuenced tailings losses and the return density of the concentrate. Two minima in the loss curve were observed [D13], corresponding to the minima in the proﬁle

5.3. WET MAGNETIC SEPARATION

345

Table 5.13: Recommended maximum discharge rates of the magnetics [M26, S59]. Separator 762 mm drum 914 mm drum 1200 mm drum Double 762 mm Double 914 mm Double 1200 mm

Max. discharge rate [t/h/m] 10 15 24 18 30 48

of the magnetic force (or force index) shown in Fig. 4.29. Similarly, the critical role of the magnetic position on the recovery of magnetite was reported by Howell et al. [H21]. On the other hand, Rayner and Napier-Munn reported [R20] that the magnet position had no signiﬁcant eect on the performance of the drum separator. The distance between the drum and the tank has a two-fold eect on the separation e!ciency. With increasing clearance between the drum and the tank, the magnetic ﬁeld strength and the magnetic force are reduced in the areas furthest from the drum. This negatively aects the e!ciency of separation, particularly of ﬁne particles. On the other hand, by increasing the clearance, the velocity of ﬂow through the separation zone decreases and so does the hydrodynamic drag on particles. This results in a more e!cient attraction of magnetic particles to the drum and in reduced shear stress acting on particles already captured on the drum. The combined eect of these two contradictory phenomena can lead to improved recoveries when the clearance is increased [D13]. Media types and size The most common medium for separation is a suspension in water of ﬁne magnetite, ferrosilicon (FeSi), or a mixture of the two, depending on the separation density required. Magnetite alone is used when a density is required in the range 1250 to 2200 kg/m3 , a mixture for 2200 to 2900 kg/m3 and ferrosilicon alone for 2900 to 3700 kg/m3 . Magnetite, the density of which ranges from 4800 to 5200 kg/m3 > is the most popular choice for medium solids used in coal preparation, while ferrosilicon is invariably used, for instance, for the concentration of diamonds, for the recovery of aluminium in recycling plants, and for beneﬁciation of iron and manganese ores. Ferrosilicon containing between 14% to 16% silicon has a density ranging from 6700 to 7100 kg/m3 . It is non-rusting and strongly magnetic. With concentrations of silicon greater than 22% the material is feebly magnetic, while with concentrations of silicon lower than 15%, it is prone to rusting. Magnetite and ferrosilicon are thus selected as media because they meet a number of essential criteria: they are physically stable and chemically inert, easily removable from the products and are readily recovered for re-use by magnetic

346

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.14: Particle size distribution of magnetite for DMS [M26]. Size fraction [m] - 300 + 212 - 212 + 150 - 150 + 106 - 106 + 75 - 75 + 45 - 45

Fine grade [%] 3.8 4.4 6.2 7.6 13.5 64.5

Coarse grade [%] 8.2 4.3 14.1 12.0 19.9 32.7

Table 5.15: Particle size distributions of selected grades of milled and atomized ferrosilicon (Samancor, South Africa). Size fraction [m] + 212 + 150 + 106 + 75 + 45 - 45

48D 0-2 4-8 12 - 18 19 - 27 27 - 35 27 - 35

100D 0-1 0-1 1-4 5 - 10 28 61 - 69

270D 0 0 0-1 0-3 7 - 11 85 - 93

Cyclone 60 0 0-2 0-4 2-6 18 - 26 65 - 78

separation. Media is supplied in several size grades and the grade used will vary with each individual plant. While ﬁner grades improve stability, ﬁne particles, in addition to possible viscosity problems, are more di!cult to recover and the feed into LIMS should then be reduced by a factor of 1.5 to 2, to maintain the magnetic recovery. A typical particle size distribution of ground magnetite is shown in Table 5.14, while size distributions of several grades of ferrosilicon are listed in Table 5.15. There are two basic types of ferrosilicon available to the operators of dense medium plants, namely milled (e.g. 270D) and atomized spherical grades (e.g. Cyclone 60). There is a marked dierence in both the shape and nature of ferrosilicon particles produced by grinding and atomizing. Particles produced by grinding are rough and angular in shape, whereas particles produced by atomizing are smooth and largely spherical or rounded. This dierence in the particle shape has marked eects on the rheological properties of aqueous suspensions of the two types of ferrosilicon [C7]. The critical value of slurry density for atomized grades is much higher than for the milled grades. At densities above 3000 kg/m3 , the viscosities of suspensions of atomized ferrosilicon are signiﬁcantly lower than those of the milled grades, owing to the greater friction among the colliding irregularly shaped milled particles [C17]. This superior property of atomized ferrosilicon allows very high suspension densities to be obtained (up to 3800 kg/m3 ) and this has made possible the heavy-medium separation of certain ores that were not

5.3. WET MAGNETIC SEPARATION

347

previously amenable to the treatment. On the other hand, grades of milled ferrosilicon show greater stability than grades of atomized ferrosilicon of equivalent size distribution. Since the desired conditions of separation are those of minimum viscosity with maximum stability, selection of the grade of ferrosilicon is based on a trade-o between these contradictory requirements and on cost considerations. Viscosity of dense medium suspensions Magnetite media are characterized by high apparent viscosities, extremely sensitive to rate of shear. Viscosities of the magnetite medium ranging from 700 cP (0.7 Pa×s) at the shear rate of 1000 s1 to 2740 cP (2.74 Pa×s) at 1000 s1 were reported at the operating density of 2800 kg/m3 [G18]. Viscosities of ferrosilicon under similar conditions ranged from 84 cP (0.084 Pa×s) to 200 cP (0.2 Pa×s). Similar results were obtained for various grades of ferrosilicon [D14]. The modelling data and their veriﬁcation by experimental measurements show that the apparent viscosity of atomized ferrosilicon (e.g. Cyclone 60), at the operating density of 3800 kg/m3 ranged from 0.025 Pa×s at the shear rate of 150 s1 to 0.3 Pa×s at 10 s1 . Media losses Historically, media losses have frequently been the largest single component of the operating costs of dense medium separation plants. Losses of magnetite in coal washing plants range from 0.4 kg to 2 kg per tonne of raw coal. In modern large cyclone plants treating - 45 + 0.5 mm material, the average losses amount to 0.45 kg/t [E3]. In DMS plants that use ferrosilicon, the losses amount to 20% to 40% of the DMS plant operating costs [D13] and may range widely, from 0.1 to 2.8 kg/t [H20], although in modern plants they do not exceed 0.25 kg/t [D13]. In an iron ore cyclone plant, the ferrosilicon losses are reported to be 0.12 kg/t and 0.15 kg/t, for intermediate and ﬁne ore fractions, respectively [K20]. It is generally claimed that the losses in the magnetic circuit usually represent the major component of the total loss. For instance, Hunt et al. [H20] report that, excluding plant housekeeping, the average losses attributable to magnetic separation, adhesion and corrosion occur in the ratio 6:3:1. In another investigation, however, magnetic losses not exceeding 30% of the total loss were observed [N7]. Magnetic properties of ferrosilicon and magnetite The magnetic properties of magnetite and ferrosilicon are important for easy recovery and cleaning of the medium in the circuit. The running costs of a DMS plant are also aected by the magnetic properties. Baran and Svoboda [B29] conducted an extensive study of magnetic properties of both magnetite and ferrosilicon of various grades. A typical hysteresis curve of 270D milled ferrosilicon is shown in Fig. 5.18. Table 5.16 summarizes the magnetic characteristics of ferrosilicon and magnetite, as determined from measurements by a vibrating sample magnetometer. It can be seen that atomized grades of FeSi exhibit slightly higher values of the saturation polarization (by 5% to 7%) compared to the milled grades. The saturation polarization of magnetite (0.45 T) is lower than that of FeSi by factor

348

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Magnetisation of 270D FeSi 8000 6000 4000 2000 0 -2000 Magnetisation (G)

-4000 -6000 -8000 -15000

-10000

-5000

0

5000

10000

15000

Magnetic Field (Oe)

Figure 5.18: A hysteresis curve of 270D ferrosilicon as measured by a vibrating sample magnetometer [B29].

Table 5.16: Saturation polarization Js, remanent polarization Jr and coercive force Hc of various grades of ferrosilicon (Samancor) and magnetite (Amcoal), as measured by a vibrating sample magnetometer [B29]. Material Cyclone 60 48D 65D 100D 150D 270D Magnetite

Jv [T] 0.93 0.83 0.87 0.87 0.86 0.83 0.45

Ju [T] 0.047 0.052 0.055 0.048 0.048 0.051 0.063

Hf [kA/m] 9.96 10.2 10.6 9.33 9.89 9.89 14.3

5.3. WET MAGNETIC SEPARATION

349

Figure 5.19: Relationship between the Si concentration and the saturation polarization of FeSi (after [B29]). of two, and it was found to be by about 25% lower than the literature value of 0.6 T, as a result of the presence of weakly magnetic impurities. The coercive force of magnetite is 50% higher than that of ferrosilicon. This might indicate a need for a higher demagnetization ﬁeld for magnetite. Although the milled grades of FeSi were found to be much more susceptible to corrosion than the atomized grades, no substantial eect of corrosion on the magnetic properties was observed. Also, no signiﬁcant dierences in the magnetic behaviour of various size fractions of FeSi were observed. Only a slight reduction (less than 5%) in the saturation polarization values for fractions smaller than 106 m was observed. Losses of ﬁne FeSi in DMS plants can thus be ascribed to the reduced e!ciency of magnetic separators to recover ﬁne particles rather than to reduced magnetization. The initial magnetic susceptibility of all grades of FeSi was approximately 2.8×104 m3 /kg, while that of magnetite was found to be equal to 3.5×104 m3 /kg. It was also observed that a substantial increase in the saturation polarization of FeSi could be achieved by decreasing the concentration of Si as is illustrated in Fig. 5.19. It was found that the saturation polarization changed by 0.16 T for every 1% in the Si content, in the range 14% to 16%. Demagnetization The passage of heavy medium through magnetic separators in the medium recovery circuit induces remanent magnetization of the medium. This may result in the formation of magnetic ﬂocs with subsequent deterioration of the medium properties, such as stability and viscosity.

350

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.20: The eect of the demagnetizing magnetic induction on FeSi viscosity in a cone circuit at Premier Diamond Mine, South Africa (adapted from [C17]).

It is common practice at DMS plants to install demagnetization coils on the magnetic separator return lines. Although the need to demagnetize media has been recognized in the static-bath processes, the usefulness of demagnetization coils in cyclone plants has been a subject of dispute. The views range from outright rejection to unconditional acceptance. These polarized views are part of the DMS plant folklore, although there is an overwhelming scientiﬁc and engineering evidence of the beneﬁcial eect of media demagnetization. In general, the installation of demagnetization coils in DMS cyclone plants is recommended (e.g. [N8]). The inverse relationship between the magnetic ﬁeld strength in a demagnetization coil and the viscosity of the circulating medium FeSi medium in the cone circuits is illustrated in Fig. 5.20. A similar beneﬁcial eect of FeSi demagnetization, in a cyclone plant, was reported by Napier-Munn and Scott [N7]. They observed that the coil had a rapid and substantial eect on the viscosity and the results are summarized in Fig. 5.21. The viscosity had started to drop shortly after the coil was activated and to rise again after the coil was de-activated. Measurements of the magnetic susceptibility of magnetized samples of ferrosilicon showed that the values of magnetic susceptibility were higher than those of unmagnetized samples [B29]. After demagnetization by a coil generating the a.c. magnetic induction of 0.06 T, the magnetic susceptibility returned to its original value. Practical aspects of demagnetization are discussed in Section 5.5.

5.3. WET MAGNETIC SEPARATION

351

Figure 5.21: The eect of demagnetization on the viscosity of 150D FeSi medium at the cyclone plant of the Mount Isa Mines lead-zinc concentrator, Australia, (adapted from [N8]). Wet magnetic drum separators for ore concentration Wet low-intensity drum magnetic separators are also used for the concentration of magnetite ore or other strongly magnetic minerals. Most of the low-intensity magnetic separation technology used today was developed during the 1960s with no signiﬁcant changes taking place. The most noticeable changes over the years have occurred with the increased diameter and length of the drum. With each increase of the drum diameter, the process capacity of units increased and throughputs as high as 160 t/h per meter length of the drum were recorded. However, tests with 1500 mm diameter drum separators could not reproduce this trend for the capacity increase, and currently not many concentrators of this size have been installed [S13]. The improved design and more e!cient permanent magnetic materials allowed the magnetic ﬁeld rating of the drum magnetic separators, traditionally expressed as the magnetic induction at 50 mm (or 2 inches), to be increased, from 0.05 T to about 0.12 T available today. In the ore concentration applications, the separators are designed for three basic operations, namely as cobbers, roughers (cleaners) and ﬁnishers. Cobbers Drum separators used in cobbing operations are designed to obtain maximum rejection of a non-magnetic fraction and maximum recovery of the magnetic material. Most iron-ore concentrating drum separators are applied in multi-drum, usually con-current, conﬁgurations so that the high-grade magnetic concentrate is obtained. In cobbing operations, two drums are typical, but as

352

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

many as four drums have been used. The diameter of the drums is either 900 or 1200 mm and the magnetic ﬁeld rating, at 50 mm, of 0.1 T is standard for cobbers. Roughers Drum magnetic separators used in roughing or cleaning are applied after the size of the cobber concentrate has been further reduced. Because the cobbing has signiﬁcantly upgraded the ore, magnetic loading of the drum is usually increased considerably. The objective of roughing is to obtain a highgrade magnetic concentrate, while maintaining high recovery. Double-drum separators, in con- or counter-current modes of operation are typically used in roughers and the required magnetic ﬁeld at 50 mm is, as a rule, 0.07 T to 0.09 T. Finishers Finishing drum magnetic separators are designed to produce the highest possible iron content in the concentrate. The feed tank and feed arrangements are usually of semi-counter-current design, with the objective of dispersing the feed particles in order to obtain maximum rejection of non-magnetic particles. Both 760 and 900 mm-diameter drums are used in the ﬁnisher applications, with the magnetic ﬁeld strength at 50 mm lower (e.g. 0.05 T) than in a rougher, to improve selectivity of separation. The feed size is usually reduced to less than 75 m or 45 m. Variables in low-intensity magnetic separation of ores Factors associated with the properties of the feed, to be considered in the selection of a wet drum magnetic separation applied to the ore beneﬁciation, are [M26]: • Feed rate (t/h/m) • Feed particle size (max. 10 mm) and size distribution • Feed volume (m3 /h) • Concentration of magnetic particles • Degree of liberation • Desired recovery into the magnetic fraction. As shown in Table 5.17, the maximum feed rate varies with the type of separator considered; maximum and recommended feed volumes are also given. Typical sizes of feed particles for the three modes of operation are: Cobbers: - 6 mm + 850 m Roughers: - 500 m + 300 m Finishers: - 75 m + 45 m.

5.3. WET MAGNETIC SEPARATION

353

Table 5.17: Feed rates and feed volumes in LIMS, as applied to ore beneﬁciation [M26]. Application Cobber Rougher Finisher

Feed rate [t/h/m] Max. Recommended 75 45 60 45 15 15

Feed volume [m3 /h/m] Max. Recommended 100 70 100 70 35 20

Table 5.18: Number of drums and magnetic poles used in LIMS for ore beneﬁciation [M26]. Separator Cobbers Roughers Finishers

Number of drums 2 to 4 1 or 2 2 or 3

Number of poles 5 or 6 5 or 6 4 to 10

Magnetic content and degree of liberation The magnetic content of iron ores to be concentrated by LIMS varies over a fairly wide range. Ores with iron concentrations from 10% to 50% or more have been successfully treated. Since liberation is not complete at the cobber stage, a substantial amount of gangue is carried into the cobber concentrate. Typically, the cobber concentrate contains 50% Fe or more and, accordingly, the magnetics content of the rougher feed is quite high. The ﬁnisher feed contains 2% to 5% of non-magnetics and thus has a very high concentration of the magnetic material. Complete liberation of most iron ores that are being treated by LIMS is usually at sizes ﬁner than 150 m, although some ores have to be reduced to 45 m. Magnetic ﬁeld strength and number of poles Increased magnetic ﬁeld strength achievable in modern low-intensity drum magnetic separators allows not only more e!cient recovery of ﬁne particles, but also the throughput of a separator can be increased without losing recovery. Such an eect of magnetic ﬁeld strength on throughput and recovery is illustrated in Fig. 5.22. The number of drums used in various applications varies with the individual ores and the choice is determined by the results of pilot-plant or laboratory tests. In addition, various types of magnetic assemblies and pole combinations have been successfully used. Typical magnetic pole speciﬁcations and number of drums are shown in Table 5.18. Throughput The feed rate in a low-intensity magnetic separator aects its metallurgical performance, as can be seen in Figs. 5.22 and 5.23. With increasing feed rate, the recovery of magnetic particles into the magnetic fraction decreases, the rate of decrease being strongly dependent on the magnetic ﬁeld

354

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.22: Recovery of iron by LIMS, as a function of throughput, for dierent values of magnetic induction at 50 mm (adapted from Sundberg [S13]). strength generated by the magnetic drum.

5.3.2

Wet high-intensity magnetic separation

Wet high-intensity magnetic separation is used in three dierent technological processes, as shown in Fig. 5.24. These separators can thus be used either as a magnetic ﬁlter to remove a single solid component from a suspension, or as a magnetic separator to remove an unwanted magnetic component from a mixture of materials, or for a concentration of valuable weakly magnetic materials from a mixture. The high intensity of the magnetic ﬁeld in these separators is generated either by rare earth or ferrite permanent magnets (for example in RE drum separators or in a Ferrous Wheel separator), or by resistive electromagnets or superconducting magnets. Magnetic ﬁeld gradient, an equally important parameter in magnetic separation, is generated by three dierent methods. Close-gradient, open-gradient and matrix (polygradient) techniques produce magnetic ﬁeld gradients of widely dierent magnitudes, as can be seen in Table 1.20. As a result of these dierent attributes of high-intensity magnetic separators, a plethora of names and terms is being used to classify them, although the operating principle of many of them are the same or, at worst, they can address similar separation objectives. The resulting chaos is further magniﬁed by the advent of new magnetic materials and advanced magnet designs that allow new approaches to high ﬁeld and high

5.3. WET MAGNETIC SEPARATION

355

Figure 5.23: The eect of feed rate on the recovery of magnetite, in a lowintensity magnetic drum separator. Drum length: 1.2 m, drum diameter: 900 mm (adapted from [K14]).

< 1% solids

Cyclic

> 1% solids

Continuous

< 1% solids

Cyclic

> 1% solids

Continuous

Filtration

Wet highintensity magnetic separation

Removal from mixture

High recovery Concentration from mixture

Continuous separation

High grade High grade and recovery

Figure 5.24: The range of applications of wet high-intensity magnetic separation (adapted from Svoboda [S1]).

356

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.19: Nomenclature for wet high-intensity magnetic separators. Separator Rare-earth drum separator Linear multipole open-gradient separator Matrix continuous separator Matrix cyclic separator Matrix cyclic magnetic ﬁlter

Acronyms REDS, REDMS, MIMS OGMS WHIMS, HGMS, HIMS HGMS HGMF, HIMF

gradient generation. A summary of the terms most frequently used to describe wet high-intensity magnetic separators is given in Table 5.19. A schematic diagram of dierent technological processes, in which wet highintensity magnetic separators are used, is shown in Fig. 5.24. It is clear that conditions for successful separation in these three categories can dier widely. Their correct selection must be based upon proper identiﬁcation of the target of the process and the deﬁnition of criteria that would distinguish successful separation from unsuccessful. The decision-making process in such a selection is outlined in Fig. 5.25 and its detailed discussion will be presented in subsequent sections. Wet rare-earth drum magnetic separators Although dry rare-earth drum magnetic separators have been readily accepted by the mining industry, it has taken somewhat longer to develop and implement wet RE drum separators. One of the reasons for reluctant acceptance of wet RE drums by the industry is the onerous problem with the removal of strongly magnetic material from the drum, even when these particles are present in trace concentrations. Conventional high-pressure spraying or scraping methods are not su!ciently eective in overcoming the strong magnetic force holding the particles on the drum, and new approaches to this problem are being investigated [A23]. Magnetic ﬁltration Magnetic ﬁltration is used primarily for the removal of ﬁne and quasi-colloidal particulates from dilute ﬂuid suspensions. Removal is carried out by passing suspensions through a magnetized matrix, which leads to the retention of particles throughout the matrix. The ﬂuid stream may be either liquid or gas. The process of magnetic ﬁltration is analogous to that of deep bed ﬁltration, the dierence being that an additional external force, namely the magnetic force, contributes to the ﬁltration e!ciency in magnetic ﬁltration. Although the magnetic force does not signiﬁcantly increase the probability of particle collision with the matrix [S31, S33], the enhanced e!ciency of particle attachment caused by the presence of strong, static dipolar magnetic interaction between the matrix and a colliding particle increases signiﬁcantly the e!ciency of the

5.3. WET MAGNETIC SEPARATION

357

HGMS

Yes Single solid component?

Magnetic filtration

No

Continuous MS

Magnetic component valuable?

No

Magnetic Techniques for the Treatment of Materials by

Jan Svoboda Formerly Research Programme manager and Principal Technology leader, De Beers Diamond Research Laboratory, De Beers Consolidated Mines (Pty.) Ltd., Johannesburg, South Africa

KLUWER ACADEMIC PUBLISHERS NEW YORK, BOSTON, DORDRECHT, LONDON, MOSCOW

eBook ISBN: Print ISBN:

1-4020-2107-0 1-4020-2038-4

©2004 Springer Science + Business Media, Inc.

Print ©2004 Kluwer Academic Publishers Dordrecht All rights reserved

No part of this eBook may be reproduced or transmitted in any form or by any means, electronic, mechanical, recording, or otherwise, without written consent from the Publisher

Created in the United States of America

Visit Springer's eBookstore at: and the Springer Global Website Online at:

http://www.ebooks.kluweronline.com http://www.springeronline.com

Contents Contents

v

Preface

xi

1 Principles of Magnetic Treatment 1.1 Magnetic separation and innovation . . . . . . . . . . . . . . . . 1.2 Principles of magnetic separation . . . . . . . . . . . . . . . . . . 1.2.1 Magnetic force on a magnetizable particle . . . . . . . . 1.2.2 Competing forces in a magnetic separator . . . . . . . . . 1.3 Fundamental quantities of magnetism . . . . . . . . . . . . . . . 1.3.1 Magnetic ﬁeld and magnetization . . . . . . . . . . . . . . 1.3.2 Magnetic susceptibility and permeability . . . . . . . . . 1.3.3 Magnetic units . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Magnetic properties of materials . . . . . . . . . . . . . . . . . . 1.4.1 Diamagnetism . . . . . . . . . . . . . . . . . . . . . . . . 1.4.2 Paramagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.3 Ferromagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.4 Antiferromagnetism . . . . . . . . . . . . . . . . . . . . . 1.4.5 Ferrimagnetism . . . . . . . . . . . . . . . . . . . . . . . 1.4.6 Demagnetization . . . . . . . . . . . . . . . . . . . . . . . 1.4.7 Mixtures containing ferromagnetic (s.l.) materials . . . . 1.5 Magnetic properties of minerals . . . . . . . . . . . . . . . . . . . 1.5.1 The classiﬁcation of minerals according to their magnetic properties . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.2 Magnetite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.3 Titanomagnetites . . . . . . . . . . . . . . . . . . . . . . . 1.5.4 Ilmenohematites . . . . . . . . . . . . . . . . . . . . . . . 1.5.5 Maghemite . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.6 Hematite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.7 Goethite . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.8 Siderite . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5.9 Iron sulphides . . . . . . . . . . . . . . . . . . . . . . . . 1.5.10 Chromites . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 Measurement of magnetic properties . . . . . . . . . . . . . . . .

1 1 3 5 6 9 9 10 10 11 13 14 15 21 21 21 24 25

v

25 26 27 29 31 31 32 33 33 34 34

CONTENTS

vi

1.7

1.6.1 Measurement of the magnetic ﬁeld strength 1.6.2 Measurement of magnetic susceptibility and Sources of magnetic ﬁeld . . . . . . . . . . . . . . . 1.7.1 Permanent magnets . . . . . . . . . . . . . 1.7.2 Iron-core electromagnets . . . . . . . . . . . 1.7.3 Solenoid electromagnets . . . . . . . . . . . 1.7.4 Superconducting magnets . . . . . . . . . . 1.7.5 Generation of the magnetic ﬁeld gradient .

. . . . . . . . magnetization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 Review of Magnetic Separators 2.1 Dry low-intensity magnetic separators . . . . . . . . . . . . 2.1.1 Magnetic pulleys . . . . . . . . . . . . . . . . . . . . 2.1.2 Plate magnets . . . . . . . . . . . . . . . . . . . . . 2.1.3 Grate magnets . . . . . . . . . . . . . . . . . . . . . 2.1.4 Suspended magnets . . . . . . . . . . . . . . . . . . 2.1.5 Drum magnetic separators . . . . . . . . . . . . . . . 2.2 Wet low-intensity drum magnetic separators . . . . . . . . . 2.2.1 Concurrent tank . . . . . . . . . . . . . . . . . . . . 2.2.2 Counter-rotation tank . . . . . . . . . . . . . . . . . 2.2.3 Counter-current tank . . . . . . . . . . . . . . . . . . 2.2.4 Design of the drum . . . . . . . . . . . . . . . . . . . 2.3 Dry high-intensity magnetic separators . . . . . . . . . . . . 2.3.1 Cross-belt magnetic separator . . . . . . . . . . . . . 2.3.2 Induced magnetic roll separator . . . . . . . . . . . . 2.3.3 Permanent magnetic roll separator . . . . . . . . . . 2.3.4 High-intensity drum separators . . . . . . . . . . . . 2.4 Wet high-intensity magnetic separators . . . . . . . . . . . . 2.4.1 Dry separation versus wet separation . . . . . . . . . 2.4.2 Iron core-based wet high-intensity separators . . . . 2.4.3 Solenoid-based magnetic separators . . . . . . . . . . 2.5 Superconducting magnetic separators . . . . . . . . . . . . . 2.5.1 Cyclic superconducting HGMS . . . . . . . . . . . . 2.5.2 Reciprocating superconducting HGMS . . . . . . . . 2.5.3 Open-gradient superconducting magnetic separators 2.6 Laboratory magnetic separators . . . . . . . . . . . . . . . . 2.6.1 Davis Tube . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Frantz isodynamic separator . . . . . . . . . . . . . 2.6.3 Separators with a rotating magnetic ﬁeld . . . . . . 2.7 Eddy-current separators . . . . . . . . . . . . . . . . . . . . 2.8 Separators with magnetic ﬂuids . . . . . . . . . . . . . . . . 2.8.1 Basic concept . . . . . . . . . . . . . . . . . . . . . . 2.8.2 Ferrohydrostatic separators . . . . . . . . . . . . . . 2.8.3 Magstream separator . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

35 39 45 47 53 56 57 59 67 69 70 72 72 73 78 81 82 82 84 84 86 86 88 89 94 96 96 97 112 128 131 132 136 138 139 141 146 147 153 153 156 159

CONTENTS

vii

3 Theory of Magnetic Separation 3.1 The forces and the equations of particle motion . . . . . . . . . . 3.2 Particle motion in drum and roll separators . . . . . . . . . . . . 3.2.1 Motion of a particle on the drum or roll surface . . . . . . 3.2.2 Motion of the particle after it leaves the roll . . . . . . . . 3.3 Separation of particles by a suspended magnet . . . . . . . . . . 3.3.1 Magnetic force in a suspended magnet . . . . . . . . . . . 3.3.2 Torque on a magnetizable body . . . . . . . . . . . . . . . 3.3.3 Demagnetization factors . . . . . . . . . . . . . . . . . . . 3.3.4 The eect of the burden . . . . . . . . . . . . . . . . . . . 3.4 High-gradient magnetic separation . . . . . . . . . . . . . . . . . 3.4.1 Theory of particle capture by a single-collector . . . . . . 3.4.2 Capture of particles in multi-collector matrices . . . . . . 3.5 Linear open-gradient magnetic separation . . . . . . . . . . . . . 3.6 Magnetic ﬂocculation . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 Magnetic ﬂocculation of strongly magnetic materials . . . 3.6.2 Magnetic ﬂocculation of weakly magnetic minerals . . . . 3.7 Magnetic separation by particle rotation . . . . . . . . . . . . . . 3.7.1 RMF rotation separation . . . . . . . . . . . . . . . . . . 3.7.2 Magnetic torque on a particle and condition for separation by rotation . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.3 Rotation of particles in a liquid . . . . . . . . . . . . . . . 3.8 Separation in magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . 3.8.1 Apparent density of a magnetic ﬂuid . . . . . . . . . . . . 3.8.2 A particle suspended in a magnetic ﬂuid . . . . . . . . . . 3.8.3 The eect of the hydrodynamic drag . . . . . . . . . . . . 3.8.4 The eect of particle magnetic susceptibility . . . . . . . 3.8.5 Motion of particles in a ferroﬂuid . . . . . . . . . . . . . . 3.8.6 Separation in a rotating ferroﬂuid . . . . . . . . . . . . . 3.9 Eddy-current separation . . . . . . . . . . . . . . . . . . . . . . . 3.9.1 Static ramp eddy-current separator. . . . . . . . . . . . . 3.9.2 Rotating drum eddy-current separators . . . . . . . . . . 3.9.3 Eddy-current separation by particle rotation . . . . . . .

163 164 166 169 170 172 173 175 178 179 181 181 198 206 208 208 210 221 222

4 Design of Magnetic Separators 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Design of circuits with permanent magnets . . . . . . . 4.2.1 Basic concepts and ﬁgures of merit . . . . . . . . 4.2.2 The static gap design . . . . . . . . . . . . . . . 4.2.3 Leakage factors . . . . . . . . . . . . . . . . . . . 4.2.4 Determination of permeance and leakage factors 4.2.5 Magnetic ﬁeld around a permanent magnet . . . 4.2.6 Magnetic forces . . . . . . . . . . . . . . . . . . . 4.2.7 Soft iron components of the magnetic circuits . . 4.2.8 Stability of permanent magnets . . . . . . . . . . 4.2.9 Magnetization of permanent magnets . . . . . .

251 251 252 252 255 257 258 259 263 264 266 269

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

224 226 227 227 229 233 234 235 240 243 243 245 249

CONTENTS

viii 4.3

. . . . . . . . . . . . . . . . . . . . . .

270 271 272 274 278 280 280 280 281 282 282 284 289 291 291 293 298 299 301 304 308 311

5 Practical Aspects of Magnetic Methods 5.1 Selection of magnetic separation technique . . . . . . . . . . . . . 5.2 Dry magnetic separation . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Electrostatic phenomena in dry separation . . . . . . . . . 5.2.2 Density and magnetic tracers . . . . . . . . . . . . . . . . 5.2.3 Comparison of dry magnetic separation techniques . . . . 5.3 Wet magnetic separation . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Wet low-intensity drum magnetic separation . . . . . . . 5.3.2 Wet high-intensity magnetic separation . . . . . . . . . . 5.3.3 Magnetic ﬁeld in high-intensity magnetic separators . . . 5.3.4 Matrix in high-gradient magnetic separators . . . . . . . . 5.3.5 Flow velocity of the slurry . . . . . . . . . . . . . . . . . . 5.3.6 Slurry density . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.7 Feed rate . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.8 The eect of particle size . . . . . . . . . . . . . . . . . . 5.3.9 Pre-treatment of slurry . . . . . . . . . . . . . . . . . . . 5.3.10 The selectivity of separation . . . . . . . . . . . . . . . . . 5.3.11 Comparative tests with wet high-intensity magnetic separators . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Magnetic ﬂocculation . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Magnetic ﬂocculation of ferromagnetic materials . . . . . 5.4.2 Magnetic ﬂocculation of weakly magnetic minerals . . . . 5.5 Demagnetization . . . . . . . . . . . . . . . . . . . . . . . . . . .

319 320 321 323 326 328 342 342 354 360 375 396 399 402 403 405 411

4.4

4.5

4.6

4.7 4.8

Design of iron-core electromagnets . . . . . . . . . . 4.3.1 Calculation of the magnetic ﬁeld . . . . . . . 4.3.2 Shape of iron parts of the circuit . . . . . . . 4.3.3 Practical procedure for design of the poles . . Design of solenoid magnets . . . . . . . . . . . . . . 4.4.1 The power requirements . . . . . . . . . . . . 4.4.2 The choice of the conductor . . . . . . . . . . 4.4.3 The cooling of coils . . . . . . . . . . . . . . . 4.4.4 Thickness of the iron cladding . . . . . . . . . Design of drum magnetic separators . . . . . . . . . 4.5.1 The basic magnet arrangements . . . . . . . . 4.5.2 Geometry of the magnet assembly . . . . . . 4.5.3 Electromagnetic modelling of the design . . . Design of a magnetic roll . . . . . . . . . . . . . . . . 4.6.1 Basic concepts of design . . . . . . . . . . . . 4.6.2 Design parameters . . . . . . . . . . . . . . . Design of a suspended magnet . . . . . . . . . . . . . Design of a ferrohydrostatic separator . . . . . . . . 4.8.1 FHS separators with a wedge-shaped working 4.8.2 Separators with hyperbolic pole tips . . . . . 4.8.3 Calculation of proﬁles of pole tips in FHS . . 4.8.4 Scale-up of ferrohydrostatic separators . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . gap . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

417 420 420 422 422

CONTENTS 5.6

5.7

ix

Separation in magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . 425 5.6.1 Magnetic ﬂuids . . . . . . . . . . . . . . . . . . . . . . . . 426 5.6.2 Ferrohydrostatic separation . . . . . . . . . . . . . . . . . 440 5.6.3 Ferroﬂuid recovery and recycling . . . . . . . . . . . . . . 454 5.6.4 Separation in a rotating ferroﬂuid . . . . . . . . . . . . . 458 Magnetism in other areas of material handling . . . . . . . . . . 459 5.7.1 Magnetic cyclone . . . . . . . . . . . . . . . . . . . . . . . 460 5.7.2 Magnetic gravity separation, ﬂotation and vacuum ﬁltration466 5.7.3 Magnetic jigging . . . . . . . . . . . . . . . . . . . . . . . 467

6 Industrial Applications 6.1 Treatment of minerals . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Recovery of grinding ball fragments from SAG and ball mills . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.2 Heavy medium recovery circuits . . . . . . . . . . . . . . 6.1.3 Beneﬁciation of iron ores . . . . . . . . . . . . . . . . . . 6.1.4 Beneﬁciation of manganese ores . . . . . . . . . . . . . . . 6.1.5 Beneﬁciation of ilmenite ores . . . . . . . . . . . . . . . . 6.1.6 Beneﬁciation of ores of non-ferrous metals . . . . . . . . . 6.1.7 Mineral sands . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.8 Industrial minerals . . . . . . . . . . . . . . . . . . . . . . 6.1.9 Magnetic beneﬁciation of coal . . . . . . . . . . . . . . . . 6.2 Nuclear industry . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Removal of solids from fuel dissolver liquor . . . . . . . . 6.2.2 Removal of ferric hydroxide ﬂocs . . . . . . . . . . . . . . 6.2.3 Soil decontamination . . . . . . . . . . . . . . . . . . . . . 6.3 Waste water treatment . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Steel industry . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Thermal power plants . . . . . . . . . . . . . . . . . . . . 6.4 Magnetic carrier techniques . . . . . . . . . . . . . . . . . . . . . 6.4.1 General principles . . . . . . . . . . . . . . . . . . . . . . 6.4.2 E"uent processing and metal ion removal . . . . . . . . . 6.4.3 Biomagnetic extraction of heavy metals . . . . . . . . . . 6.5 Magnetic carriers and separation in biosciences . . . . . . . . . . 6.5.1 Principles of biomagnetic separation techniques . . . . . . 6.5.2 Magnetic separators in biosciences . . . . . . . . . . . . . 6.5.3 The application of magnetic separation . . . . . . . . . . 6.5.4 Separation of red blood cells by HGMS . . . . . . . . . . 6.6 Recovery of metals from wastes . . . . . . . . . . . . . . . . . . . 6.6.1 The separation processes in metal recycling . . . . . . . . 6.6.2 Sorting of heavy non-ferrous metals . . . . . . . . . . . . 6.7 The applications of ferrohydrostatic separation . . . . . . . . . . 6.7.1 Recovery of gold and other platinum-group metals . . . . 6.7.2 Applications in the diamond winning industry . . . . . . 6.7.3 The fractionation analysis of coal . . . . . . . . . . . . . .

469 470 470 472 472 488 489 494 498 504 507 510 510 511 511 514 514 517 519 519 520 524 525 525 528 530 533 534 535 539 542 543 545 546

x

CONTENTS

7 Innovation and future trends 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Science and technological innovation . . . . . . . . . . . . . . . 7.3 Magnetic separation and innovation . . . . . . . . . . . . . . . 7.3.1 Reliance on an empirical approach? . . . . . . . . . . . 7.3.2 A walk through innovation in magnetic separation . . . 7.4 The current status of magnetic separation technology . . . . . . 7.5 What the future holds? . . . . . . . . . . . . . . . . . . . . . . 7.5.1 Mineral processing . . . . . . . . . . . . . . . . . . . . . 7.5.2 Biomedical applications . . . . . . . . . . . . . . . . . . 7.5.3 Recycling and waste processing . . . . . . . . . . . . . . 7.5.4 Prospects for superconductivity in magnetic separation 7.6 Research and development needs . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

551 551 552 555 556 556 567 567 568 569 569 570 573

List of Symbols

577

Bibliography

583

Index

629

Preface In the years following the publication of Magnetic Methods for the Treatment of Minerals by Elsevier in 1987, many changes have taken place in magnetic technology. While fundamental and thorough, the above treatise reﬂected preferences and philosophy of research and the development and application of magnetic methods as they were practiced in the second half of the last century. Although demand for metals and minerals has not diminished, the dominant drivers of the early 21st century dier signiﬁcantly from those of the late 20th. The priorities of nuclear power, defence, and energy-demanding and waste-generating beneﬁciation of mineral resources are being replaced by those associated with technology sustainability, environmental and knowledge management, recycling, and health care. Research priorities and product development of the last century cannot, therefore, satisfactorily meet criteria of the 21st century. Considerable technological progress has been achieved in areas such as automation, computerization, sustainable material science, laboratory and plant practices and separation equipment. New permanent magnetic materials, advances in practical applications of superconductivity and availability of sophisticated modelling tools have changed the technological landscape. As a result, innovation and technology transfer in magnetic technology have been remarkably successful during the last two decades. The title of this monograph reﬂects the fact that the book covers not only the application of magnetic techniques in the minerals industry, but also in recycling, environmental engineering and biomedical sciences. The goal of the book is to reﬂect the current technological trends and to re-position the research, development and practice of magnetic methods of material manipulation, according to current needs and strategic thinking. The book is intended for researchers, students, development workers and consulting metallurgists, as well as plant practitioners and equipment manufacturers who wish to acquire comprehensive knowledge of magnetic separation technology. The book is based on work of numerous scientists and engineers. I am grateful to many of my colleagues and friends at universities, research organizations, and mining and manufacturing companies around the world, for their contribution in advancing magnetic separation technology. Interaction and collaboration with them over the years has been enriching and rewarding and they will be identiﬁed in this monograph by citation of their published work. I am xi

PREFACE

xii

also indebted to many individuals and companies who have given me invaluable help by providing data and photographs for reproduction. Their important contributions have been acknowledged directly in the text. I am grateful to Mr. E. H. Roux and Drs. D. Slatter, G. Hill and N. Allen for their kindness in reading portions of the manuscript and suggesting improvements. I also wish to express my appreciation to my colleagues Drs. V. Murariu and L. Krüger and Mr. A. Sarelis for assistance with various aspects of this book. Jan Svoboda Johannesburg, South Africa February 2004

Chapter 1

Principles of Material Treatment by Magnetic Means 1.1

Magnetism and the innovation milestones in magnetic separation

Magnetic phenomena have been known and exploited for many centuries. The earliest experiences with magnetism involved magnetite, the only material that occurs naturally in a magnetic state. Thales of Miletus stated that the magnetic interaction between lodestone, or magnetite, and iron was known for at least as long ago as 600 B.C. That magnetite can induce iron to acquire attractive powers, or to become magnetic, was mentioned by Socrates. Permanent and induced magnetism, therefore, represents one of man’s earliest scientiﬁc discoveries. Practical signiﬁcance of magnetic attraction as a precursory form of magnetic separation was recognized in 1792, when W. Fullarton obtained an English patent for separating iron ore by magnetic attraction [D1]. Since that time the science and engineering of magnetism and of magnetic separation have advanced rapidly and a large number of patents have been issued. While separation of inherently magnetic constituents was a natural early application of magnetism, Wetherill’s separator, devised in 1895, was an innovation of signiﬁcant proportions. It demonstrated that it was possible to separate two components, both of which were commonly considered to be non-magnetic. In the ensuing time various types of disk, drum and roll dry magnetic separators were developed although the spectrum of minerals treatable by these machines was limited to rather coarse and moderately strongly magnetic materials. Since the end of the nineteenth century there has been a steady expansion of both the equipment available and the range of ores to which magnetic separation is applicable. The development of permanent magnetic materials and improvement in their 1

2

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.1: Development of permanent magnet materials.

magnetic properties have been main drivers of innovation in magnetic separation. Figure 1.1 illustrates the history of improvement of the maximum energy product (EK)max of permanent magnets. Three innovation milestones can be identiﬁed in the graph. At the end of the nineteenth century very feeble steelbased magnets were employed, while in the 1940s permanent magnets that were able to compete with electromagnets, were developed. Probably the most important innovation step was made in the late seventies of the last century when rare-earth magnets became available. These magnets allowed new solutions for challenges that were not possible or feasible with electromagnets. Another signiﬁcant driver of innovation in magnetic separation was the introduction of ferromagnetic bodies (such as balls, grooved plates or mesh) into the magnetic ﬁeld of a separator. In 1937 Frantz developed a magnetic separator consisting of an iron-bound solenoid packed with ferromagnetic steel ribbons [F1] and this proved to be an important milestone in the development of the present high-intensity and high-gradient magnetic separators. This innovation extended the range of applicability of magnetic separation to many weakly magnetic and even to diamagnetic minerals of the micrometer size. Although the signiﬁcance of the discovery of superconductivity has been equated with the invention of the wheel [K1], its importance for magnetic separation does not seem to represent a major breakthrough. The need for magnetic induction greater than 2 T has never been convincingly demonstrated in matrix separators [S1, S2] and the main advantage of superconducting magnets is, therefore, the reduced energy consumption and the possibility of generating a high magnetic force in large volumes, even without using matrices. The concentration of various ferrous and non-ferrous minerals has been an

1.2. PRINCIPLES OF MAGNETIC SEPARATION

3

Feed Magnetic force

Competing forces

Non-mags

Mags Middlings

Figure 1.2: Schematic representation of the process of magnetic separation. important application of magnetic separation, as has the removal of low concentrations of magnetizable impurities from industrial minerals. In recent years, as a result of numerous economic, environmental and social challenges, the recycling of metals from industrial wastes and the concentration or removal of biological objects in medicine and biosciences have become important areas of application of magnetic technology. Recent research and development of eddycurrent separators, magnetic ﬂuids and magnetic carriers illustrate the enormous eort that has been expended over the last twenty years in order to convert a wealth of novel ideas into workable techniques and introduce them into material manipulation operations.

1.2

Principles of magnetic separation

Magnetic separation is used for the concentration of magnetic materials and for the removal of magnetizable particles from ﬂuid streams. The separation is achieved by passing the suspensions or the mixtures of particles through a non-homogeneous magnetic ﬁeld. This process leads to preferential retention or deﬂection of the magnetizable particles. The same objective is often achieved in a very dierent fashion, the common features being a competition between a wide spectrum of forces of various magnitudes and ranges. In magnetic separation the separating (dierentiating) external force is the magnetic force. The separation of one material from another or the removal of magnetizable particles from streams depend upon their motion in response to the magnetic force and to other competing external forces, namely gravitational, inertial, hydrodynamic and centrifugal forces. Interparticle forces of electromagnetic and electrostatic origin contribute to the overall scenario, which is depicted in Fig. 1.2. It is thus clear that a necessary (but not su!cient) condition for a successful

4

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

separation of more strongly magnetic from less strongly magnetic particles in a p magnetic ﬁeld is that the magnetic force Ipdj acting on more magnetic particles lp . Simultaneously, must be greater than the sum of all the competing forces Ifrps q a magnetic force acting on less strongly magnetic particles, Ipdj must be smaller than the sum of the corresponding competing forces. Therefore, the following conditions must be met in a magnetic separator: p Ipdj

X l

lp Ifrps

and

q Ipdj

X

lq Ifrps

(1.1)

l

For dierent objectives eqs. (1.1) will have speciﬁc forms. For instance, in order to achieve high recovery of magnetic particles, the magnetic separating force must be greater than the sum of the competing forces as shown in eqs. (1.1). If, however, the magnetic force is much greater than the competing forces, i.e. Ipdj AA Ifrps (1.2) selectivity of separation will be poor, as no distinction will be made between magnetizable species of dierent values of magnetic susceptibilities. High selectivity of the separation process can thus be obtained when the magnitudes of the magnetic and competing forces are of comparable magnitudes, compatible with conditions given by eqs. (1.1). The selectivity of the process will be, therefore, critically determined by the relative values of the magnetic and competing forces. And these are aected by the correct choice of a separator and its operating conditions. For instance, selective separation of a magnetizable material (1) from magnetizable material (2) will be achieved when the following relationship is met: (1) (2) Ipdj A Ifrps A Ipdj (1.3) If the non-magnetic fraction is the valuable product, the ”brute force” approach to separation, expressed by relationship (1.2), will result in poor yield of the non-magnetic product, as a result of mechanical and magnetic entrainment of the non-magnetic material in the magnetic tailings. In general, a mixture of particles introduced into the magnetic separator will be split into two or more components. However, in any real separation, both magnetic and non-magnetic particles can be found in the magnetic fraction, non-magnetic fraction and the middling fractions. The e!ciency of separation is usually expressed by the recovery of the magnetic component, and by the grade of the magnetic product. However, these criteria are not unique and they must be selected on the basis whether the useful product is the magnetic or non-magnetic fractions. Since all materials are magnetic to some extent, methods of separation that use magnetic force oer a unique approach to material manipulation in a wide array of industries. One of the main advantages of material treatment in a magnetic ﬁeld is that the magnetic force can be applied in a controlled manner, in a wide range of values. Moreover, this force can be superimposed on other physical forces and several physical properties of materials can thus be exploited

1.2. PRINCIPLES OF MAGNETIC SEPARATION

5

simultaneously. In addition, magnetic separation can treat a wide range of types of materials, ranging from colloidal to large sizes and from ”non-magnetic” to strongly magnetic. Magnetic separation is an environmentally friendly technique and it can operate in wet and dry modes, making it a technique of choice for arid or arctic regions.

1.2.1

Magnetic force on a magnetizable particle

The density of the magnetic energy zp in a linear isotropic medium is given by: 1 K ·E (1.4) 2 where K and E are, respectively, the magnitudes of the magnetic ﬁeld and the magnetic ﬂux density (magnetic induction). It transpires from eq. (1.4) that the magnetic energy Xps of a magnetizable particle of volume Ys placed in the magnetic ﬁeld is: zp =

1 Ys K 2 2 s while the magnetic energy of a ﬂuid of the same volume is given by Xps =

Xpi =

1 Ys K 2 2 i

(1.5)

(1.6)

In eqs. (1.5) and (1.6), s and i are magnetic permeabilities of the particle and the ﬂuid, respectively. The energy increment X of the system (particle + ﬂuid) is given, to ﬁrst order, as the dierence between the energies given by eqs. (1.5) and (1.6). For weakly magnetic particles this is a good approximation [G1]. Thus: X=

1 ( s )Ys K 2 2 i

(1.7)

In general, a force can be expressed as I = uX , where u is the operator of the gradient. Taking into account that m = 0 (1 + m ) , where m is the volume magnetic susceptibility of material m and 0 is the magnetic permeability of vacuum, the magnetic force can be written (in SI units): 1 Ip = 0 (s i )Ys uK 2 2

(1.8)

In practical situations the magnetic ﬂux density E is frequently used, rather than the magnetic ﬁeld strength K, and eq. (1.8) can then be expressed as: 1 (s i )Ys EuE Ip = 0

(1.9)

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

6

For su!ciently strongly magnetic particles (s AA i ) it is advantageous to re-write eq. (1.8) as: Ip = 0 Ys P uK

(1.10)

where P is the magnetization of the particle. Researchers as well as practitioners of magnetic separation sometimes use old cgs system of units, in which eq. (1.9) can be written Ip = (s i )Ys EuE

(1.11)

In practice it is easier to measure speciﬁc (mass) magnetic susceptibility " rather than volume susceptibility and eq. (1.9) can be re-written, assuming that "i ?? "s : 1 (" "i )ps EuE Ip = 0 s

(1.12)

where ps is the mass of the particle. It can be seen from eqs. (1.8) to (1.12) that the magnitude of the magnetic force is proportional to the product of the magnetic ﬂux density and its gradient. This force is in the direction of the ﬁeld gradient, not of the magnetic ﬁeld. It is also clear that in a homogeneous magnetic ﬁeld, i.e. when uE = 0, the force on a particle is zero. It can also be seen from the above equations that Ip e3

(1.13)

where e the particle radius.

1.2.2

Competing forces in a magnetic separator

As has been mentioned above, magnetic force in a magnetic separator competes with various external forces such as forces of gravity and inertia, centrifugal force and hydrodynamic drag. The importance of each force is a function of the type of the separator and of the mode in which it operates. For a spherical particle of density s the gravitational force is given by: Ij = (s i )Ysj

(1.14)

where i and j are the density of the ﬂuid medium and the acceleration by gravity, respectively. The centrifugal force can be expressed as: If = (s i )$Ysu

(1.15)

where u is the radial position of the particle and $ is the angular velocity. The hydrodynamic drag force can be obtained from Stokes’s equation:

1.2. PRINCIPLES OF MAGNETIC SEPARATION

7

Figure 1.3: Hydrodynamic drag and force of gravity, as a function of particle diameter, for particles of density 5000 kg/m3 (e.g. hematite), moving in water ( = 103 Pa×s), with relative velocity y..

Ig = 6e(yi ys )

(1.16)

where is the dynamic viscosity of the ﬂuid and yi and ys are velocities of the ﬂuid and the particle, respectively. It can be seen from the last three equations that: Ij e3 > If e3 and Ig e1

(1.17)

Because some of the forces have dierent dependence on particle radius, their relative importance will vary with particle size. The dependence of the force of gravity on the third power of the particle radius means that the force of gravity will be signiﬁcant for large particles, On the other hand, the hydrodynamic drag, which in the Stokes regime depends on the ﬁrst power of particle size, will be important for small particles. This situation in depicted in Fig. 1.3 and demonstrates that the force of gravity, for this speciﬁc case, is dominant for particle diameter greater than 500 m, while for particle diameter smaller than 50 m the hydrodynamic drag is the main competing force. The magnetic force depends on the cube of particle radius and its relative importance in the process of magnetic separation is determined by the magnetic properties of the particles and by technical parameters of the magnetic separator (i.e. magnetic ﬁeld strength and its gradient). Figure 1.4 illustrates the dependence of the magnetic force on a hematite particle of magnetic susceptibility = 9.4×103 (SI) (" = 188×108 m3 /kg), as a function of particle size,

8

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.4: Magnetic force on a hematite particle in several types of magnetic separators, as a function of particle size. Table 1.1: Typical values of BuB for selected magnetic separators.

Suspended magnet 0.05

EuE[T2 /m] Nd drum Nd roll magmagnetic netic separaseparator tor 80 300

HGMS with steel wool matrix 5×104

for various types of magnetic separators. The values of the product EuE used in construction of the graph are summarized in Table 1.1. It is clear from eq. (1.9) and from Fig. 1.4 that the particle size is a more important discriminating factor in magnetic separation than the magnetic susceptibility. Since Ip e3 , even a large dierence in magnetic susceptibilities of components of a poorly classiﬁed mixture to be separated will not necessarily result in selective separation. As can be seen in Table 1.2, a particle characterized by magnetic susceptibility of 1 a.u. (arbitrary unit) and size 10 a.u. will be acted upon by the same magnetic force as a particle with susceptibility of 1000 a.u. and size 1 a.u. Selectivity of separation will be determined by the balance of the magnetic and competing forces acting on these two components. It is evident from the above discussion that the subject of magnetic separation cannot be treated without ﬁrst deﬁning the physical quantities usually encountered in magnetism, and the units in which these quantities are measured. The next sections will be devoted to these issues.

1.3. FUNDAMENTAL QUANTITIES OF MAGNETISM

9

Table 1.2: Magnetic force vs particle size. Particle size [a.u.] 10 1

1.3 1.3.1

Magnetic susceptibility [a.u.] 1 1000

Magnetic force [a.u.] 1000 1000

Fundamental quantities of magnetism and their units Magnetic ﬁeld and magnetization

When we describe a magnetic ﬁeld, we employ two dierent quantities, namely magnetic ﬁeld strength K and magnetic ﬂux density (or magnetic induction) E. K and E are both vector quantities having direction as well as magnitude. In vacuum E and K are not independent and are related by the equation = 0 K E

(1.18)

where the magnetic permeability of vacuum 0 is numerically equal to 4 ×107 H/m. In a magnetic material of magnetization P , the total magnetic induction becomes, in Sommerfeld convention, adopted by IUPAP: = 0 (K +P ) E

(1.19)

In the cgs system, since 0 = 1, eq. (1.19) becomes =K + 4 P E

(1.20)

Magnetization is deﬁned as the total magnetic moment P of dipoles per unit volume Y , i.e. P = P @Y . The factor 4 arises from the fact that a unit pole produces a unit ﬁeld everywhere on the surface of a sphere of unit radius (1 cm) enclosing the pole, and the surface of this sphere is 4 cm2 = In the Kennelly system, which is traditionally favoured by electrical engineers, E is given in SI by:

= 0 K + M E where M is the magnetic polarization. M and P are related by equation: M = 0 P

(1.21)

The magnetic induction thus includes contributions from the magnetization P , which is deﬁned as the magnetic dipole moment of a body per unit volume, or polarization M deﬁned by eq. (1.21).

10

1.3.2

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Magnetic susceptibility and permeability

The magnetization of a material, in general, depends on the magnetic ﬁeld acting on it. For many materials, P is proportional to K (at least when K is not too large) and we may write: = K P

(1.22)

where , the volume magnetic susceptibility, is a property of the material. Since P and K have the same dimensions, is dimensionless. We can combine eq. (1.22) with eq. (1.19) to get = 0 (1 + )K = 0 u K = K E

(1.23)

u = 1 + and

(1.24)

where = 0 (1 + )

The quantity u is called relative magnetic permeability and is dimensionless, while is called magnetic permeability and has a unit of H/m. While eq. (1.19) is general, eqs. (1.23) and (1.24) are based on assumption that the material is both isotropic and linear. In other words, that P is proportional to H and in the same direction. This assumption is never completely true for ferromagnetic materials. Either u or may be used to characterize a material. Volume magnetic susceptibility ranges from values close to 0, both positive and negative, to positive values greater than 1, for dierent materials. For materials that have very small susceptibilities, it is much more convenient to use than u . For instance for = 106 , u = 1.000001, and for = - 106 , u = 0.999999. Magnetic susceptibility can also be expressed with respect to the unit mass of material of density , and then "=

(1.25)

where " is the mass, or speciﬁc, magnetic susceptibility. Since a sample mass p is usually better known than its volume, mass magnetic susceptibility is very commonly employed. For the same reason the mass magnetization rather than magnetization P is often used to characterize materials. The mass magnetization is deﬁned as =

1.3.3

P thus P = p

(1.26)

Magnetic units

The units and symbols used in this book are those of the Système International d’Unités, designated SI. This system, which is based on the meter, kilogram, second, ampere, kelvin and candela, is essentially the same as the Giorgi, or MKSA, system in the ﬁeld of electromagnetism.

1.4.

MAGNETIC PROPERTIES OF MATERIALS

11

Essentially all students today are taught in SI units and most scientiﬁc journals require their contributors to use SI units. Nevertheless, many papers on magnetism - and magnetic separation is no exception - are still published in cgs units. Occasionally, the cgs system is polluted with the emu ”unit”, which is not really a unit to which dimensional analysis can be applied [S3]. Therefore, even today the ﬁeld of magnetism is not blessed with a lucid system of quantities and units and numerous panel discussions and articles on the subject illustrate the reigning chaos [C1, S4, G2]. Those authors who follow the current trend and convert cgs units to SI units ﬁnd that the task of conversion is gigantic and that errors almost always creep in. Table 1.3 lists the SI units in use for most important quantities, together with their conversion factors to electromagnetic cgs units. Conversion of magnetic induction in the cgs unit of Gauss into the SI unit of Tesla should present no di!culty, with the values in Gauss divided by 104 . When the magnetic ﬁeld strength is used, Oersted multiplied by 103 @4 (approximately 79.58) will give the value in the SI unit of A/m. Magnetic susceptibility is a more complicated quantity. It is the volume magnetic susceptibility that enters most equations used in magnetic separation. Although dimensionless in both systems of units, volume magnetic susceptibility diers by a factor of 4 in the systems of units, as can be seen in Table 1.3. Experimentally, it is easier to determine the mass magnetic susceptibility and therefore most values of magnetic susceptibility that can be found in the literature are those of mass susceptibility, often in cgs units. Various names are used for this unit, e.g. emu/cm, emu/g×Oe and cgs, but all of them usually represent the same unit, namely cm 3 /g. Thus in SI the unit is m 3 /kg and conversion factor from cgs to SI is 4×103 . The following equations summarize relationships between volume and mass magnetic susceptibilities, in both SI and cgs systems of units (density is expressed in g/cm3 ).

1.4

(VL) = 4(fjv)

(1.27)

(fjv) = "(fjv) and (VL) = 103 "(VL)

(1.28)

(VL) = 4"(fjv)

(1.29)

"(VL) =

4 "(fjv) 103

(1.30)

"(fjv) =

103 "(VL) 4

(1.31)

Magnetic properties of materials

It has been stated at the outset that all materials display certain magnetic properties, regardless of their composition and state. According to their magnetic

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

12

Table 1.3: Units of important magnetic quantities. The quantity is cgs units is obtained by multiplying the quantity in SI by the conversion factor. For instance, 1 G = 10e-4 T. Quantity Magnetic ﬁeld strength Magnetic induction (ﬂux density) Magnetization Mass magnetization Magnetic ﬂux

Symbol

SI unit

cgs unit

H

A/m

Oersted (Oe)

B

Tesla (T)

Gauss (G)

104

M

A/m

103

Am2 /kg

Oe, erg/Gcm3 emu/g

Wb (Weber)

Mx (Maxwell) G erg/G

108

Polarization Magnetic moment Volume magnetic susceptibility Mass (speciﬁc) magnetic susceptibility Demagnetization factor Energy product Permeability of vacuum Bohr magneton

J P

Nuclear magneton Anisotropy constant

Q

Tesla (T) Am2

dimensionless dimensionless, emu/cm3 Oe

"

m3 /kg

N

dimensionless dimensionless

BH 0

J/m3 H/m

E

9.274×1024 Am2 5.051×1027 Am2 J/m3

K

cm3 /g

GOe 1 (dimensionless)

erg/cm3

Conversion factor 103 @4

1

104 103 4 4 · 103

1/4 1/40 4 · 107

101

1.4.

MAGNETIC PROPERTIES OF MATERIALS

Paramagnetic

Ferromagnetic

Antiferromagnetic

Ferrimagnetic

13

Figure 1.5: Schematic diagram of the alignment of magnetic moments. properties, materials can be divided into ﬁve basic groups: diamagnetic, paramagnetic, ferromagnetic, antiferromagnetic and ferrimagnetic. The last three groups have generally higher magnetic susceptibilities than the other groups and are frequently termed ”ferromagnetic” sensu lato (s.l.). This broad deﬁnition must be distinguished from one of its subdivisions, ferromagnetic sensu stricto (s.s.) [T1] as discussed below. The alignment of magnetic moments in each type of material is shown in Fig. 1.5. The classiﬁcation of magnetism in terms of magnetic permeability is given in Table 1.4.

1.4.1

Diamagnetism

Diamagnetism has its origin in the modiﬁcation of the electron orbit magnetic moment by an external magnetic ﬁeld. The currents thus induced give rise to an extra magnetic moment. However, according to Lenz’s law, the resulting magnetic moment is in the opposite direction to the ﬁeld that has induced the current. Therefore, approaching a source of the magnetic ﬁeld, a diamagnetic material is repelled from it. This eect is present in all materials, independently of temperature. Diamagnets have a very small and negative volume magnetic susceptibility, of the order of - 105 (SI). While many inorganic and almost all organic molecules are diamagnetic, in many materials their diamagnetism is hidden by a much stronger paramagnetic/ferromagnetic (s.l.) eect. This is, for instance, the case of metals that are normally associated with small negative susceptibility, often overwhelmed by positive paramagnetic or ferromagnetic contribution. The values of selected diamagnetic metals and non-metallic compounds are given in Table 1.5. Table

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

14

Table 1.4: Magnetic susceptibility in various types of magnetism. Parameter

Diamagnetism

Susceptibility Relative permeability

?0 ?1

Paramagnetism Ferromagnetism Antiferromag- Ferrimagnetism netism 0 AA 0 1 AA 1

Table 1.5: Magnetic susceptibilities of diamagnetic materials. [SI] × 105 -1.0 -1.4 -3.6 -1.56 -2.0 -0.9 -0.73

Material Copper Zinc Gold Lead Diamond Water Ethylalcohol

"[m3 @kg] × 109 -1.1 -1.96 -1.86 -1.38 -5.6 -9.0 -9.3

1.6 summarizes the magnetic susceptibilities of various diamagnetic minerals.

1.4.2

Paramagnetism

In paramagnetic materials the magnetic atoms or ions have permanent intrinsic magnetic moments and occur in low concentrations. Susceptibility arises from the competition between the aligning eect of the applied magnetic ﬁeld and the randomizing eect of thermal vibrations. In zero applied magnetic ﬁeld, the moments point in random directions. When a ﬁeld is applied, a small magnetization develops, but the magnetic susceptibility is very small and is inversely proportional to the absolute temperature. In the presence of the external magnetic ﬁeld, and under standard practical conditions (i.e. when P [email protected] ?? 1, where P is the magnetic moment, n is the Boltzmann constant and T is the absolute temperature) the magnetization of a paramagnetic material is f q2 K P (1.32) = 0 P nW where f is a constant and q is the number of magnetic dipoles. The susceptibility of paramagnetic materials is then given by =

F f0 q2P = nW W

(1.33)

1.4.

MAGNETIC PROPERTIES OF MATERIALS

15

Table 1.6: Mass magnetic susceptibilities of assorted diamagnetic minerals. Mineral

Quartz Calcite Sphalerite Galena Baddeleyite Barite Magnesite Apatite Fluorite Halite Kaolinite

Chemical formula

SiO2 CaCO3 ZnS PbS ZrO2 BaSO4 MgCO3 Ca5 [PO4 ]3 (F,Cl) CaF2 NaCl Al4 Si4 O10 (OH)8

Mass magnetic susceptibility [m3 /kg]×109 - 6.0 - 4.8 - 3.2 - 4.4 - 1.4 - 3.8 - 6.4 - 3.3 - 7.9 - 9.0 - 20.0

where F is the Curie constant. Equation (1.33) is called the Curie law, which states that magnetic susceptibility of the paramagnetic substance is inversely proportional to the temperature. The paramagnetic susceptibility is always small ( 105 to 103 (SI)), although paramagnetism can be several orders of magnitude larger than diamagnetism. As follows from eq. (1.32), the dependence of the magnetization of a paramagnetic material on the ﬁeld strength is expressed by a straight line. In most cases, in standard conditions such as W = 300 K and E = 1 T, the above formulae apply. In extreme conditions, such as at cryogenic temperatures and very high magnetic ﬁeld, a saturation eect appears. Taking into account eq. (1.23), it transpires from eq. (1.32) that for paramagnetic materials the magnetic susceptibility is independent of the magnetic ﬁeld. Table 1.7 summarizes the values of magnetic susceptibility for selected paramagnetic metals and compounds, while Table 1.8 lists susceptibilities of assorted paramagnetic minerals. Compilations of susceptibility of minerals are numerous [A1, S1, K2, D2] and large variations can be observed. Conﬂicting data can be explained by the inherent variability in mineral composition and the presence of inclusions and contaminants. Dierent measuring techniques tend to give diering values of susceptibility [M1] and the usage of dierent systems of units also contributes to frequent inconsistency of the values of magnetic susceptibility found in the literature.

1.4.3

Ferromagnetism

In ferromagnetic materials (s.s.) interaction between neighbouring atoms is strong so that the magnetic moments of all atoms are aligned parallel to each other against the randomizing force of thermal motion. The strong internal

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

16

Table 1.7: Magnetic susceptiblities of paramagnetic materials. Material

Aluminium Chromium Titanium Vanadium Platinum Zirconium CuSO4 ·5H2 O NiSO4 ·7H2 O MnO

Mass magnetic susceptibility [m3 /kg]×109 7.67 42.0 42.2 73.0 12.3 16.7 76.7 201 860

Volume magnetic susceptibility [SI]×105 2.1 30.2 19.0 44.5 26.4 10.8 17.5 39.8 445.5

Table 1.8: Magnetic susceptibilities of paramagnetic minerals. Mineral

Chemical composition

Hematite Siderite Goethite Ilmenite Rutile Wolframite Pyrite Limonite Manganite Pyroxene Dolomite

Fe2 O3 FeCO3 FeOOH FeTiO3 TiO2 (Mn,Fe)WO4 FeS2 Fe2 O3 ·nH2 O MnO2 ·Mn(OH)2 (Mg,Fe)2 Si2 O6 CaMg(CO3 )2

Mass magnetic susceptibility [m3 /kg]×109 250 - 3800 350 - 1500 250 - 400 200 - 1500 10 - 50 350 - 1200 3 - 200 100 - 400 100 - 500 40 - 1000 5 - 20

ﬁelds, which align the spins, are called molecular or Weiss ﬁelds. These ﬁelds are the result of a quantum mechanical process called exchange interaction. Weiss assumed that the molecular ﬁeld is very large, its magnitude independent of external magnetic ﬁeld, and its direction not ﬁxed, but always parallel to the magnetization. The Weiss hypothesis predicts that a material can be spontaneously magnetized even in the absence of an applied magnetic ﬁeld at temperatures below the Curie temperature, at which the thermal agitation overcomes the molecular ﬁeld. This tendency aids the external ﬁeld in producing saturation, i.e. complete alignment. There is an apparent contradiction between theory, which explains that magnetic materials are fully magnetized even in the absence of an external ﬁeld, and practice, which generally shows that such materials exhibit no magnetization or magnetization much smaller than saturation. In fact, theory is correct at a mi-

1.4.

MAGNETIC PROPERTIES OF MATERIALS

17

Figure 1.6: Temperature behaviour of various classes of magnetic materials. croscopic level, but at a macroscopic scale the ferromagnetic body is subdivided into Weiss domains, each of which is spontaneously magnetized to saturation, but not in the same direction, by virtue of a strong exchange magnetic ﬁeld. Inside a domain the magnetization is at a maximum (saturation), but as all domains compensate each other, on macroscale the mean magnetization is nil. The value of the saturation magnetization varies with temperature, decreasing from a maximum value at W = 0 K, becoming zero at the Curie temperature Wf . Above Wf , the behaviour is similar to that of a paramagnetic material, with the magnetization being proportional to the ﬁeld and the susceptibility decreasing with increasing temperature. However, the susceptibility does not follow the Curie law, eq. (1.33), but varies as =

F W Wf

(1.34)

Equation (1.34) is called the Curie-Weiss law. The temperature behaviour of various types of magnetism is shown in Fig. 1.6. In contrast to diamagnetic and paramagnetic materials, magnetization of ferromagnetic materials (v=o=) depends not only on the ﬁeld strength, but also on the shape and the magnetic history of the sample. For instance, a ferromagnetic material can remain magnetized after removal of the external ﬁeld. The ferromagnetics (s.l.) are thus characterized by hysteresis as is illustrated in Fig. 1.7.

18

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.7: Hysteresis loop of a ferromagnetic (s.l.) material.

It can be seen in Fig. 1.7 that two kinds of the magnetic curve (or hysteresis loop) can be determined. The induction curve is E = E(K)> while the magnetization (or intrinsic) curve illustrates the P = P (K) dependence. Since E = 0 (P + K), and since P is much greater than K in most parts of the initial magnetization curve (curves OP and OQ, respectively, in Fig. 1.7), both curves are comparable. The dierence occurs mainly in the saturation region where P (K) is asymptotic to Pv , while E(K) approaches 0 (Pv + K). It can be seen in Fig. 1.7 that after the initial (or virgin) magnetization reaches its saturation value Ev or Pv , (points P and Q, respectively), irreversibility, resulting from imperfections in the material, prevents the magnetization (or the induction) from returning to zero when the external ﬁeld is removed. Magnetization and induction at K = 0 are called remanent magnetization, or remanent induction, respectively. By reversing the direction of the external ﬁeld K, the residual induction and magnetization decrease to zero for particular ﬁelds Kf and Kfl called coercive force and intrinsic coercive force, respectively. As can be seen in Fig. 1.7, Kf is not the same for P (K) and E(K) curves. For low-Kf materials (soft magnetic materials) the dierence is generally negligible, while for hard material or permanent magnets (high Kf ) the dierence becomes signiﬁcant. Magnetic permeability, deﬁned as = [email protected], can vary widely at various points on the magnetizing and demagnetizing portions of the hysteresis loop. The initial permeability l and the maximum permeability max are important

1.4.

MAGNETIC PROPERTIES OF MATERIALS

19

Figure 1.8: The initial magnetization curve and permeabilities of a ferromagnetic material.

parameters that can be determined as the slopes of the magnetization curve as shown in Fig. 1.8. The initial permeability illustrates the behaviour of the permeability when the external magnetic ﬁeld approaches zero. With increasing magnetic ﬁeld the permeability of the ferromagnetics (s.l.) increases and reaches its maximum. With further increase of the magnetic ﬁeld permeability decreases and the relative permeability asymptotically approaches unity. This trend is shown in Fig. 1.9 which illustrates the dependence of the relative permeability on the external magnetic ﬁeld for decarburized steel used for magnetic yokes [B1]. In a similar way we can deﬁne magnetic susceptibility of a ferromagnetic material, taking account relationship (1.24). Magnetic susceptibility has a similar trend as permeability, and at a high magnetic ﬁeld it asymptotically approaches zero. Ferromagnetism occurs in nine elements: three transition metals, iron, cobalt and nickel, and six rare earth metals, gadolinium, terbium, dysprosium, holmium, erbium and thulium. Most alloys consisting of the three transition metals are ferromagnetic, and so are many of their alloys with non-magnetic elements. Many alloys of manganese with non-magnetic elements are also ferromagnetic, although manganese is not ferromagnetic in the pure state. On the other hand, there is no mineral that would possess ferromagnetic properties. The values of magnetization and of the Curie temperature for three ferromagnetic elements (v=v) and other ferromagnetic materials are given in Table 1.9.

20

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.9: Permeability of decarburized steel used for manufacture of magnet yokes [B1].

Table 1.9: Magnetization and Curie temperatures of ferromagnetic materials. Material Iron Nickel Cobalt Armco Si-Fe Permalloy 45 Permendur Mumetal

Magnetization 0 Pv [T] at 0 K 2.18 0.64 1.81 2.11 1.97 1.6 2.45 0.8

Curie temperature Tf [0 C] 770 358 1120

1.4.

MAGNETIC PROPERTIES OF MATERIALS

1.4.4

21

Antiferromagnetism

Antiferromagnetic materials were originally thought of as a class of anomalous paramagnets, since they have small positive susceptibilities of similar magnitude to many materials of the latter class. However, their magnetic susceptibility does not increase steadily as the temperature decreases all the way to absolute zero. At high temperatures they follow the relationship =

F W + WQ

(1.35)

where WQ is the so-called Néel temperature. At this critical temperature the susceptibility ceases to obey eq. (1.35) and below WQ the susceptibility generally decreases with decreasing temperature. The situation is depicted in Fig. 1.6. In the original Néel’s theory, an antiferromagnetic substance was envisaged as composed of two sublattices, one of whose spins tend to be antiparallel to those of the other. Néel assumed the magnetic moments of the two sublattices to be equal, so that the net moment of the material was zero, as is schematically shown in Fig. 1.5. Since Néel’s original hypothesis the term antiferromagnetism has been extended to include materials with more than two sublattices and those with triangular, spiral and canted spin arrangements. Antiferromagnetism occurs mostly in transition metal oxides, such as MnO, CoO and NiO, as well as in other similar compounds such as sulphides and selenides. Antiferromagnets have small (1010 to 108 m3 /kg) positive susceptibilities and hematite is one of the minerals that possess antiferromagnetic properties.

1.4.5

Ferrimagnetism

In a ferrimagnetic material magnetic moments are ordered regularly in an antiparallel sense, but the sum of the moments pointing in one direction exceeds those pointing in the opposite direction. This situation is illustrated in Fig. 1.5. The magnetic properties of ferromagnets and ferrimagnets are generally similar: both exhibit saturation and their magnetization is much greater than that of other magnetic classes. Ferrimagnetism occurs mainly in ferrites, mixed oxides of iron and of other elements, and also in two of the oxides of iron, namely magnetite Fe3 O4 and maghemite Fe2 O3 . The shapes of magnetization curves of various classes of materials are shown in Fig. 1.10 and a summary of magnetic properties of materials is given in Table. 1.10.

1.4.6

Demagnetization

It was previously stated that the magnetic properties of ferromagnetic (v=o=) particles also depend on the shape of the body. The magnetic ﬁeld Kl inside a magnetized body is not equal to the ﬁeld applied to it (K0 ). The magnetization of a ferromagnetic body of a ﬁnite size will produce a magnetic ﬁeld inside the

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

22

Table 1.10: Classiﬁcation of materials according to their magnetic properties. Class Diamagnetic

Critical temperature None

Paramagnetic

None

Ferromagnetic

Curie temperature Wf Néel temperature WQ

Magnitude of [SI] Approximately 106 to 5 - 10 Approximately + 105 to + 103 Large, e.g. A 1 (below Wf ) As paramagnetic

Curie temperature Wf

As ferromagnetic

Antiferromagnetic

Ferrimagnetic

Temperature variation of Constant = [email protected] Above Wf F W Wf

=

Above WQ F = (W ±W with l) Wl 6= WQ below WQ decreases, anisotropic Above Wf F (W ±Wl ) with W 6= Wl

body in a direction opposite to that of the magnetization. The induced ﬁeld is called the demagnetizing ﬁeld Kg because it always tends to oppose the applied ﬁeld K0 . The situation is depicted in Fig. 1.11. The magnitude of Kg is proportional to that of magnetization P : g = Q P K

(1.36)

where Q is the dimensionless constant of proportionality called the demagnetization factor. The value of Q varies from zero to unity, depending upon the shape of the material and the direction of magnetization. The resulting magnetic ﬁeld inside the body is given by l = K 0 + K g = K 0 QP K

(1.37)

In general, the calculation of Q is quite complex and numerical values for various shapes can be found e.g. in [B2, B3, D3]. With increasing aspect ratio, with the major axis parallel to the ﬁeld, the demagnetization factor decreases. For a sphere Q = 1/3, while for the inﬁnitely long cylinder whose axis coincides with the direction of the ﬁeld, Q = 0. For a thin disc, perpendicular to the ﬁeld, the demagnetization factor achieves its maximum value, Q = 1. For a linear soft magnetic material, for which P = K> eq. (1.37) can be re-written l = K

1 0 K 1 + Q

l = 0 and E

1 0 K 1 + Q

(1.38)

1.4.

MAGNETIC PROPERTIES OF MATERIALS

23

Figure 1.10: Shapes of the magnetization curves of various classes of materials (not in scale).

Figure 1.11: The demagnetizing ﬁeld in a short magnetic sample.

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

24

In the studies of mineral magnetism it is important to distinguish extrinsic susceptibility h , which is the susceptibility that is conventionally measured by most instruments, from intrinsic susceptibility lq > which is the true susceptibility after removal of the eects of internal demagnetizing ﬁelds [T1]. These susceptibilities are related by the following equation: h =

1.4.7

lq 1 + Q lq

(1.39)

Mixtures containing ferromagnetic (s.l.) materials

In magnetic separation, many weakly magnetic materials contain ferromagnetic (v=o=) impurities. As a result of a high magnetic permeability of most ferromagnetic (v=o=) materials, the bulk magnetic susceptibility of a weakly magnetic mineral will be determined by the concentration of ferromagnetic impurities. For such a mixture the observed magnetic susceptibility is given by h =

flq (1 + Q lq )

(1.40)

where f is the volume concentration of the ferromagnetic (v=o=) material. Contributions of various ferromagnetic (v=o=) and paramagnetic minerals to the total susceptibility of a mixture is shown in Fig. 1.12 [T1]. Since the magnetic permeability and susceptibility of a ferromagnetic (v=o=) material is a function of the magnetic ﬁeld, the deﬁnition of magnetic susceptibility is determined by measuring techniques used to determine the susceptibility. The most frequently quoted value is the initial susceptibility (or permeability) l as shown in Fig. 1.8. For strongly susceptible materials, such as magnetite, h = [email protected] , and the initial susceptibility can be written: f Q For spherical particles Q = 1/3 and thus l =

(1.41)

l 3f

(1.42)

while for ovoid particles, with the ratio of long and short axes of 10, the susceptibility is [L1, T1]: l 18f

(1.43)

Although the magnetic susceptibility of paramagnetic material is independent of the magnetic ﬁeld, minerals displaying various forms of magnetic order (i.e. ferromagnets (v=o.)), or paramagnetic minerals containing the admixtures of the magnetically ordered materials, exhibit a ﬁeld-dependent magnetic susceptibility. This phenomenon can seriously alter the predictions of the results of magnetic separation based on the ﬁeld-independent magnetic susceptibility. The measured magnetic susceptibility, in a relatively low applied magnetic ﬁeld (E? 0.6 T), can be represented by the Owen-Honda equation [O1, H1]:

1.5. MAGNETIC PROPERTIES OF MINERALS

25

Figure 1.12: Contribution of various minerals to the total susceptibility of a mineral mixture [T1].

Pv Pv = 4 + (1.44) K K where s and g are paramagnetic and diamagnetic susceptibilities, respectively, 4 is the magnetic susceptibility extrapolated to the inﬁnite magnetic ﬁeld, and Pv is the saturation magnetization of the ferromagnetic (v=o=) component of the mixture. It has been experimentally determined ([N2, P2]) that 4 is characteristic of a mineral, and is nearly constant for samples of the same mineral from dierent localities. On the other hand, saturation magnetization Pv , which indicates the degree of weak ferromagnetism, varies widely between samples from diering localities and between size fractions of the same sample. = s + g +

1.5 1.5.1

Magnetic properties of minerals The classiﬁcation of minerals according to their magnetic properties

Although all matter responds to the presence of the external magnetic ﬁeld, the degree of this response varies widely. For practical reasons the technical classiﬁcation of materials, and particularly of minerals, diers from physical

26

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

categorization discussed in previous sections. For the purposes of magnetic separation, materials can be divided into three basic groups: Strongly magnetic materials can be recovered by a magnetic separator with the use of a relatively weak magnetic ﬁeld, up to, for example, 0.15 T, with a modest ﬁeld gradient of the order of 0.5 T/m. The magnetic susceptibility that responds to such a low magnetic ﬁeld is generally greater than 104 m3 /kg and ferromagnetic and ferrimagnetic materials like mild steel, iron, magnetite, maghemite and pyrrhotite fall under this group. Weakly magnetic materials can be recovered by a magnetic separator that generates magnetic induction up to 1.0 T, and the ﬁeld gradient in the range from 50 to 500 T/m. This broad group of materials includes antiferromagnetic, paramagnetic and some ferrimagnetic minerals. The group comprises iron and manganese oxides and carbonates, ilmenite, wolframite and other materials. Magnetic susceptibility of these materials ranges from 107 m3 /kg to 5×106 m3 /kg. ”Non-magnetic" materials are those materials that cannot be easily recovered by conventional magnetic separators. They include very weakly paramagnetic and antiferromagnetic materials with magnetic susceptibility smaller than, for example, 107 m3 /kg. Austenitic stainless steel, aluminium, rutile, pyrite, garnet and red blood cells belong to this group. Diamagnetic materials, with their negative magnetic susceptibility are also included. This classiﬁcation is only conditional as it does not take into account such an important variable as particle size, which, as we have seen in Section 1.2.2, is as important as magnetic susceptibility in determining the e!ciency of magnetic separation. Recent developments and innovation in magnetism extended the range of materials that can be treated by the magnetic means to such a degree that all classes of matter are included, down to the submicrometer or even nanosize range.

1.5.2

Magnetite

Magnetite Fe3 O4 is the most fundamental and important magnetic mineral. It has a cubic crystalline structure in which Fe3+ and Fe2+ cations form two distinct lattices. Each of the lattices is magnetized in opposite directions and magnetite behaves as a ferrimagnetic mineral . The saturation polarization of magnetite at room temperature ranges from 0.55 T to 0.61 T and the Curie temperature is 575 0 C. The density of pure Fe3 O4 is 5200 kg/m3 , calculated from the cell dimensions [N1]. As has been mentioned earlier, magnetic properties of magnetically ordered mineral grains depend, among other things, on the grain size. The most important distinction is between very small particles, each of which is a single domain, and large grains, which are multidomain. For any material there is a maximum size for spherical simple domain, referred to as the critical size. For magnetite this critical size is about 0.05 m [S5], while for hematite, for instance, this value is much higher, of the order of 200 to 300 m [N1].

1.5. MAGNETIC PROPERTIES OF MINERALS

27

Figure 1.13: Magnetic susceptibility and coercive force of ferromagnetic particles, as a function of grain size. The variation of the coercive force Kf with particle diameter g, in granular magnetic materials and over a wide range of grain sizes, is well represented by the relationship Kf gq

(1.45)

The value of q is usually in the range between 0.25 and 1. The eect of transition from single domain to multidomain structure, on magnetic properties of a ferromagnetic grain, is illustrated in Fig. 1.13. This Figure shows that, at the transition between multidomain and single domain arrangement, magnetic susceptibility achieves its minimum, while the coercive force is maximum. A simpliﬁed dependence of the coercive force and mass magnetic susceptibility on particle diameter is shown in Fig. 1.14. Fig. 1.15 illustrates the dependence of the mass magnetic susceptibility of magnetite on the external magnetic ﬁeld, ranging from 0 to 240 kA/m (0 to 3 kOe). The data reported in [P1] were obtained with size fraction - 74 + 53 m.

1.5.3

Titanomagnetites

Titanomagnetites Fe3{ Ti{ O4 are one of the most common magnetic minerals. Magnetic susceptibility, saturation magnetization and Curie temperature vary in a regular manner with the composition parameter { from { = 0 (magnetite)

28

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.14: Dependence of the coercive force and magnetic susceptibility of magnetite on the particle size (after Derkach [D4]).

Figure 1.15: The ﬁeld dependence of the magnetic susceptibility of magnetite (adapted from Derkach [D4]).

1.5. MAGNETIC PROPERTIES OF MINERALS

29

Figure 1.16: Variation of the room temperature magnetic susceptibility with composition, for titanomagnetites (after [O1]).

to { = 1 (ulvöspinel). The variation of the initial magnetic susceptibility with composition, for three size fractions, is shown in Fig. 1.16 [O1]. Fig. 1.17 illustrates the dependence of the initial magnetic susceptibility on particle size, for assorted compositions of titanomagnetites.

1.5.4

Ilmenohematites

Titanium-rich ilmenohematites Fe2| Ti| O3 are signiﬁcant magnetic minerals, as their susceptibilities are more than two to three orders of magnitude greater than those of paramagnetic minerals. Ilmenite FeTiO3 is antiferromagnetic below the Néel temperature of 55 K. Above the Néel temperature ilmenite is paramagnetic [N1] and its magnetic susceptibility (approximately 5×103 (SI) or 10×107 m3 /kg) is somewhat lower than for other members of the series [T1, D2], and was found to be essentially independent of the magnetic ﬁeld strength in the range from 0.1 T to 9 T [D2]. Magnetic susceptibility measured below the Néel temperature (at 4.3 K) was found to be equal to 150×107 m3 /kg at magnetic ﬁelds smaller than 0.6 T. At higher magnetic ﬁelds the value of the susceptibility dropped to about 100×107 m3 /kg [D2]. Figure 1.18 illustrates the variation of the saturation magnetization of ilmenohematite samples of particle size of 9.8 m, at room temperature, with composition [O2]. It can be seen that ilmenite (| = 0) is one of the magnetically weakest members with saturation polarization of approximately 0.012 T.

30

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.17: Variation of the initial magnetic susceptibility, at room temperature, with grain size, for titanomagnetites (after [O1]).

Figure 1.18: Saturation magnetization of ilmenohematites as a function of their composition (after [O2]).

1.5. MAGNETIC PROPERTIES OF MINERALS

31

Figure 1.19: Magnetic susceptibility of hematite as a function of the applied magnetic ﬁeld (after [N2]).

1.5.5

Maghemite

The magnetic properties of maghemite (-Fe2 O3 ) are very similar to those of magnetite (albeit slightly less pronounced). Both minerals have fundamentally the same spinel structure, although the composition of maghemite is essentially that of hematite. Maghemite is metastable and converts to hematite at temperatures in the range from 300 0 C to 350 0 C. The saturation polarization at room temperature ranges from 0.48 T to 0.51 T.

1.5.6

Hematite

Pure hematite -Fe2 O3 has antiferromagnetic structure above the Néel temperature of approximately 680 0 C. Between the Néel temperature and the Morin temperature WP = - 100 0 C hematite is a canted antiferromagnet (”weak ferromagnet”). At room temperature, the magnetic polarization is about 0.5 % that of magnetite, i.e. between 15×104 to 30×104 T. The weak ferromagnetism (v=o=) of hematite is not fully understood because of its complex and contradictory behaviour. The properties vary from sample to sample and depend on their origin. For instance, the ratio of the remanent polarization to saturation polarization MU @MV for ﬁne hematite, ranges from close to zero to about 0.8 [A2]. The coercive force of ﬁne hematite is very high, up to 2.5×105 A/m, in contrast to the low values of the order of 8×102 A/m [S5, D5], observed with crystals, which were a few millimeters in size.

32

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.20: The eect of temperature and magnetic ﬁeld on the magnetic susceptibility of specularite (after [P2]). Hematite is also strongly anisotropic, i.e. crystals can be magnetized by magnetic ﬁelds applied along the basal plane, but are almost unaected by ﬁelds perpendicular to this plane, unless extremely strong ﬁelds are employed [T1]. Hematite also tends to ﬂake parallel to its basal plane and the ﬂakes are often termed specularite. The magnetic susceptibility of pure hematite is a complicated function of particle size, magnetic ﬁeld, and temperature, determined by the interplay between contributions from weak ferromagnetism and antiferromagnetism [D5]. The eects of magnetic ﬁeld strength and temperature on magnetic susceptibility are shown in Figs. 1.19 and 1.20, respectively. A signiﬁcant change in magnetic susceptibility for magnetic ﬁelds smaller than 8×105 A/m (10 kOe) can be seen in Fig. 1.19. The ﬁeld-independent magnetic susceptibility 4 was found to be equal to 1.43×103 (SI) [N2]. Pastrana and Hopstock [P2] investigated the eect of temperature and magnetic ﬁeld on magnetic susceptibility in terms of eq. (1.44). They found that 4 increased only slightly with temperature but the eect of temperature on was dramatic, as illustrated by Fig. 1.20.

1.5.7

Goethite

Goethite (FeOOH) is an antiferromagnetic mineral, which ideally should have perfectly compensated spins, and hence no net spontaneous magnetic moment. It appears, however, that one of the sublattices is usually canted; as a result the mineral behaves ferrimagnetically. It has a magnetization greater

1.5. MAGNETIC PROPERTIES OF MINERALS

33

Table 1.11: Some physical properties of ferromagnetic (s.l.) minerals. Mineral

Magnetite Maghemite Hematite Goethite Pyrrhotite Chromite

Composition

Fe3 O4 Fe2 O3 Fe2 O3

Curie/Néel temperature [r C] 575 350 680

FeOOH

120 - 130

FeS FeCrO4

320 - 84

Saturation polarization [T] 0.59 - 0.61 0.48 - 0.51 10×104 to 30×104 50×107 to 50×104 0.1 1.9×105

Density [kg/m3 ] 5200 4800 5300 4300 4600 5090

than that of hematite but weaker than that of magnetite. Goethite also has a high coercivity, comparable to that of hematite. The mass magnetic susceptibility ranges from 2.5×107 m3 /kg to 6×107 m3 /kg [A1, P2]. The temperature and the magnetic ﬁeld dependence of the magnetic susceptibility of goethite, as reported by Pastrana and Hopstock [P2] is shown in Fig. 1.21. Physical properties of selected ferromagnetic (v=o) minerals, including goethite, are summarized in Table 1.11.

1.5.8

Siderite

Siderite FeCO3 undergoes an antiferromagnetic transition at the Néel temperature of about 14 K. When heated under oxidizing conditions, it decomposes into minerals such as maghemite, magnetite and iron hydroxide. The ﬁnal decomposition product is hematite [B4]. Results of extensive measurements of magnetic susceptibility of samples of siderite (- 150 + 105 m) at room temperature [P3] show that the susceptibility does not vary with the applied magnetic ﬁeld. The susceptibility ranges from 8×107 m3 /kg to 11×107 m3 /kg and similar values were reported in [T1, M2].

1.5.9

Iron sulphides

Iron sulphides exhibit magnetic properties over a narrow range of speciﬁc compositions, but these are strongly aected by impurities, grain size and similar factors. Pyrrhotite (FeS1+{ for 0.10 ? { ? 0.14) is the most common ferromagnetic (v=o=) iron sulphide. Most of these minerals are chemically unstable on heating and the Curie temperature of pyrrhotite, 320 0 C, is almost the same as the temperature at which is decomposes to magnetite [T1]. As in hematite, the spin structure consists of ferromagnetic order, the magnetic moments of adjacent planes being coupled parallel. Unlike hematite, the moments of the planes dier in magnitude and a strong ferrimagnetism results [O2]. Pyrrhotite is generally more strongly magnetic than hematite and the

34

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.21: Magnetic susceptibility of goethite as a function of magnetic ﬁeld strength and temperature (after [P2]). saturation polarization, at room temperature, is about 0.12 T [O2], although smaller values are often found in literature (e.g. [T1]). The magnetic ﬁeld dependence of the mass magnetic susceptibility is shown in Fig. 1.22 [D4].

1.5.10

Chromites

The magnetic properties of natural chromium-bearing spinels or chromites (Fe, Mg)(Cr,Al,Fe)2 O4 are highly variable, the variation being closely related to the variation in their chemical composition. It is frequently assumed that the magnetic susceptibility and the hysteresis behaviour of chromites is controlled by the end-member magnetite [H2, S6]. The magnetic susceptibility is reported to range from 6×107 m3 /kg to 30×107 m3 /kg at 4.3 K [D2] and from 5×107 m3 /kg to 12×107 m3 /kg at elevated temperatures (78 and 136 K) [D2, S6].

1.6

Measurement of magnetic properties

This section brieﬂy describes experimental techniques used for the measurement of magnetic quantities. There are hundreds of dierent techniques and their modiﬁcations, each having distinct merits as well as limitations. There is no single technique which is universally applicable to all types of measurements. There are several comprehensive sources of information [Z1, F2, B5, B6, C2] that provide a good starting point in the pertinent literature. It is interesting

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

35

Figure 1.22: Mass magnetic susceptibility of pyrrhotite as a function of the magnetic induction (after [D4]). to note that while the measurement methods have remained virtually unchanged for a long period, the equipment has been subjected to continuous development. Practitioners as well as researchers who use magnetic techniques as a tool for mineral beneﬁciation, material concentration or removal will be interested primarily in the measurement of the magnetic ﬁeld strength and its gradient and of magnetic susceptibility. There is a wide range of measuring instruments commercially available, some of them easily aordable and suitable for ﬁeld applications.

1.6.1

Measurement of the magnetic ﬁeld strength

There are several ways of measuring the magnetic ﬁeld strength or magnetic induction. The choice of the measurement method depends on several factors. The ﬁeld strength, its non-homogeneity, as well as the required accuracy all need to be considered. Figure 1.23 shows the accuracy of absolute measurements of magnetic ﬁeld strength for a few commonly used methods. The ﬂuxmeter method This method, which is based on Faraday’s induction law, is one of the oldest, and still very accurate, techniques of the ﬁeld measurement. It consists of placing a coil in the magnetic ﬁeld so that part of that ﬁeld is enclosed as a magnetic ﬂux through the coil area. Switching o the ﬁeld or removing the coil from the ﬁeld gives rise to an induction voltage across the coil terminals. The ﬂux is

36

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.23: Measurement of the magnetic ﬁeld strength: accuracies and ranges of various methods [H3]. then measured as the time integral of the voltage produced. Measurements are performed either by using ﬁxed coils in a dynamic magnetic ﬁeld, or by moving the coils in a static ﬁeld. The Hall Eect method E.H. Hall discovered in 1879 that a metal strip immersed in a transverse magnetic ﬁeld and carrying a current developed a voltage mutually at the right angle to the current and the voltage that opposed the Lorentz force on the electrons. The Hall-probe meters, known as gaussmeters, use very simple electronic instrumentation and provide an instant measurement. The small size of the probe sensing area (1 mm2 and less), its static physical characteristics, as no motion of the probe is required, and there are no moving parts, make gaussmeters very useful instruments. The basic premise of the Hall probe is that when a current L is ﬂowing along one axis of a conductor or semiconductor, and when the magnetic ﬁeld E is applied perpendicularly to the plane of the probe (or generator), then the Hall voltage XK given by eq. (1.46) is generated perpendicular to both the current and the magnetic ﬁeld. The situation is depicted in Fig. 1.24. L ·E (1.46) g where g is the thickness of the Hall generator and UK is the Hall constant. The Hall voltage is thus, in the ﬁrst approximation, proportional to the XK = UK

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

37

B FL

UH v

B

d

I +

Figure 1.24: Schematic representation of the Hall-eect probe.

ﬂux density. The Hall constant depends on various material parameters as well as temperature and, to a small extent, on the ﬂux density E. The resulting linearity error is kept as small as possible by applying an appropriate ohmic resistor to the Hall voltage. This allows the construction of measuring devices that are linear to within ±1 % for a ﬂux density of about 1 T. Equally important for accuracy is the eect of the temperature coe!cient of the Hall voltage. The Hall probes, usually made using indium arsenide, are very fragile. The Hall element is generally only a few hundredths of a millimeter thick and needs mechanical support. Aluminium is usually used as a substrate. The Hall probes can be used to measure d.c. ﬁelds, a.c. ﬁelds and pulsed magnetic ﬁelds. The probes are available in various shapes and their use depends on the direction of the magnetic ﬁeld to be measured. The probes are either transverse or axial. With the transverse probe, the ﬂux density is measured perpendicular to the probe rod, while with the axial probe the measured magnetic ﬁeld is in the direction of the probe axis. The overall views of hand-held and bench-scale gaussmeters are shown in Figs. 1.25 and 1.26. In order to generate a high magnetic force on particles to be separated, the magnetic ﬁeld in magnetic separators is generally very non-uniform. The value of the magnetic ﬁeld thus changes considerably, often over a scale of several hundreds of micrometers, particularly in high-gradient type magnetic separators such as HGMS, or permanent magnet roll separators. In view of the ﬁnite size of the Hall sensing element, it is the mean magnetic ﬁeld over the relatively large cross-sectional areas of the sensor, and not the maximum ﬁeld, that is being measured by the Hall probe. With common commercially available Hall probes the measured magnetic ﬁeld is usually much less than the maximum ﬁeld. For instance, magnetic induction usually measured in an NdFeB permanent magnetic roll separator rarely exceeds 1 T, while a special Hall microprobe can

38

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.25: A portable hand-held gaussmeter (courtesy of Walker LDJ Scientiﬁc, Inc.).

Figure 1.26: A precision laboratory gaussmeter (courtesy of Walker LDJ Scientiﬁc, Inc.).

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

39

measure the ﬁeld as high as 1.9 T. Such values agree with the ﬁeld strength obtained in computer modelling. The above discussion indicates that it is rather di!cult to measure accurately the magnetic ﬁeld gradient in a magnetic separator. Although the knowledge of the spatial distribution of the magnetic ﬁeld and its proﬁle is important for serious understanding of the process of magnetic separation and of the design of magnetic separators, commercial Hall probes are usually unsuitable for this exercise. However, commercially available gaussmeters can be used for measurements of the magnetic ﬁeld gradient in a low-gradient class of magnetic separators, such as magnetic pulleys and suspended magnetic separators. Accuracy of the measurement can be enhanced by devising a measuring rig [S7].

1.6.2

Measurement of magnetic susceptibility and magnetization

All techniques for the determination of magnetic susceptibility fall into two principal categories. The ﬁrst is based on the measurement of a force that acts on a sample when it is placed in a non-uniform magnetic ﬁeld. The other method makes use of the electromagnetic force induced in a coil when the magnetic ﬁeld changes, or when there is a relative motion of the sample and the coil. The force methods The most familiar of the force techniques for measurement of magnetic susceptibility is the Gouy method. The sample under investigation is packed into a long cylindrical container, which is positioned so that one end is in a strong uniform magnetic ﬁeld E1 (near the centre of the magnet gap), while the other is in a much weaker ﬁeld E2 , e.g. outside the gap. The magnetic force acting on the sample is equal to Ip =

v p D(E12 E22 ) 20

(1.47)

where v and p are volume magnetic susceptibilities of the sample and of the surrounding medium, respectively, and D is the cross-sectional area of the sample. This force is detected as a weight dierential between the ﬁeld-on and ﬁeld-o conditions. The principal merit of the Guoy method lies in its simplicity - one needs only a balance, a sample container and the magnet [D6]. The Faraday method rests in the measurement of the force exerted on a small sample by a non-homogeneous magnetic ﬁeld. This can be achieved, for instance, by the use of special pole pieces. In this case the force on the sample can be written v p gE Ip = YE (1.48) 0 g} where } is the direction of the magnetic ﬁeld gradient and Y is the volume of the sample.

40

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.27: Magnetic susceptibility meter KLF-4 (courtesy of Agico Instruments). Magnetic induction methods In the simplest application of the induction principle, a sensing coil is wound around a sample. A second winding is used to generate variable magnetic ﬁeld, which produces a magnetization. There are several instruments based on the induction principle available commercially. They are essentially induction bridges that measure magnetic susceptibility of a sample of any shape and form while the mass of the specimens can range from a few grams to several tens of grams. Figure 1.27 illustrates such an automatic computer-controlled inductivity bridge, which is suitable for rapid laboratory measurement of magnetic susceptibility of rocks, soils, minerals and other materials. Sensitivity of the instrument is 1×106 (SI) and the measurement is conducted at the magnetic ﬁeld range from 10 A/m to 300 A/m (0.12 G to 3.8 G). A similar instrument with resolution of 2×106 (SI) is shown in Fig. 1.28. An even more sensitive instrument is the KLY-3 Kappabridge shown in Fig. 1.29. It employs a fully automatic zeroing system with autoranging and automatic compensation of the thermal drift and its sensitivity is speciﬁed as 2×108 (SI). While the above described laboratory susceptibility meters could be of considerable interest and use for practitioners and researchers in magnetic separation, they might not be easily aordable and su!ciently portable in plant operation. For ﬁeld operation there are several types of portable susceptibility meters commercially available. Figure 1.30 shows such an easily aordable pocket-size susceptibility meter. The instrument weighs 0.18 kg and has the measurement sensitivity of 1×107 (SI). The ﬁeld data can be stored in 250 memory registers and recalled later. The advantages of the induction bridge susceptibility meters are their high accuracy, fast measuring rate and automated computer-controlled mode of operation. High sensitivity enables one to measure the magnetic susceptibility of

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

41

Figure 1.28: Magnetic susceptibility meter MS2 (courtesy of Bartington Instruments).

Figure 1.29: Magnetic susceptibility meter Kappabridge KLY-3 (courtesy of Agico Instruments).

42

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.30: Pocket-size magnetic susceptibility meter SM-30 (courtesy of ZH Instruments). Table 1.12: Magnetic susceptibility of pyrrhotite measured by an induction bridge [S8]. Magnetic ﬁeld [G] 0.0256 0.9 5.36

Volume magnetic susceptibility ([SI]x103 ) 186 233 357

materials ranging from diamagnetic to ferromagnetic. The main drawback from the magnetic separation point of view is that these instruments operate at very low magnetic ﬁeld and do not allow measurement of the susceptibility as a function of the magnetic ﬁeld strength. The measurement of susceptibility at a low magnetic ﬁelds is only acceptable for paramagnetic and diamagnetic materials for which the susceptibility is ﬁeld-independent. For materials with ordered structures, such as ferromagnetic (v=o=) materials, magnetic permeability and magnetic susceptibility are strongly dependent on the external magnetic ﬁeld, as has been demonstrated in Figs. 1.9 and 1.15. Table 1.12 illustrates the dependence of the initial magnetic susceptibility on the magnetic ﬁeld strength, as measured by an induction bridge. It can be seen from Figs. 1.9 and 1.15 that the initial permeability or susceptibility is generally smaller than the eective permeability at the magnetic ﬁeld at which magnetic separation takes place, i.e. l ? hi i = If the external magnetic ﬁeld is su!ciently high then $ 1 and $ 0, and the magnetic force on a particle will be determined by the saturation magnetization Pv as follows from eq. 1.44. The value of Pv can be high or low, depending on the

1.6. MEASUREMENT OF MAGNETIC PROPERTIES

43

Figure 1.31: Vibrating sample magnetometer (courtesy of LDJ, Inc.). type of material, irrespective of what the value of the initial permeability (or susceptibility) is. It is thus clear that evaluation of separability of ferromagnetic (v=o=) materials based on the measurement of the initial magnetic susceptibility can lead to erroneous conclusions. Vibrating sample magnetometer A vibrating sample magnetometer (VSM), shown in Fig. 1.31, is one of the most popular techniques in magnetometry [F3]. The sample is vibrated at small amplitude with a known frequency and phase in a uniform applied magnetic ﬁeld. The ﬁeld distortion produced by the sample varies in an a.c. manner and is detected by a pick-up coil. Using a lock-in ampliﬁer to ﬁlter out signals at frequencies other than the sample vibration frequency, VSM is able to make highly sensitive measurements. The magnitude of the signal is dependent on the magnetic properties of the sample. The external magnetic ﬁeld can be produced by superconducting magnets, various types of electromagnets or Helmholtz coils, providing excitation ﬁelds from a fraction of milliTesla to many Tesla. For all magnetizable materials, the VSM test results are displayed as magnetization curves. For ferromagnetic (v=o=) materials the results are in the form of the simple hysteresis loop, with values provided for all of the critical parameters, such as coercive force, remanent and saturation magnetization, applied magnetic ﬁeld and others. VSM can be used to test magnetic properties of metal alloys, minerals, permanent magnets, thin ﬁlms, magnetic ﬂuids etc. A typical hysteresis curve, as obtained by VSM, is shown in Fig. 1.32. For purposes of evaluation of magnetic separability of materials, VSM is a very useful, albeit rather expensive instrument. Since susceptibilities of diamagnetic and paramagnetic materials do not depend on the strength of the

44

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.32: The hysteresis curve for mild steel, as obtained by VSM.

external magnetic ﬁeld, information obtained using inductive bridges is su!cient to access separability of such materials. For ferromagnetic (v=o=) materials, however, the magnetic susceptibility is strongly dependent on the ﬁeld strength and separability of such materials is determined by the magnetic properties at the operating magnetic ﬁeld strength of a given magnetic separator. Vibrating sample magnetometer allows the determination of the magnetic susceptibility at any point on the hysteresis curve (Fig.1.32), as the tangent to the curve. It is thus possible to determine the magnetic susceptibility at any value of the magnetic ﬁeld. This procedure is useful only in the linear part of the magnetization curve. Once the material begins to saturate magnetically, the susceptibility approaches zero and the magnetic force on a particles is determined by the saturation magnetization. A typical ﬁeld dependence of the magnetic susceptibility as determined from the magnetization curve obtained using VSM is shown in Fig. 1.33. As has been stated earlier, in magnetic separation many paramagnetic and diamagnetic materials, and minerals in particular, contain ferromagnetic (v=o=) admixtures. These admixtures can signiﬁcantly inﬂuence the values of magnetic susceptibility as a consequence of its dependence on magnetic ﬁeld, temperature and particle size. A correct evaluation of magnetic susceptibility in terms of eq. (1.44), under given experimental or operational conditions, can only be eected with instruments such as VSM. However, VSM is only rarely accessible to a practitioner or even researcher in magnetic separation and detailed information about magnetic properties of minerals available in literature is limited. An exception is the work of Dahlin and Rule [D2] who investigated the magnetic susceptibility of numerous minerals as a function of the magnetic ﬁeld strength.

1.7. SOURCES OF MAGNETIC FIELD

45

Figure 1.33: Volume magnetic susceptibility of magnetite and ferrosilicon 270D, as a function of magnetic ﬁeld, as measured by VSM [S8]. A vibrating sample magnetometer with a superconducting magnet capable of producing a magnetic ﬁeld of 7.16×106 A/m (90 kOe) was used. The results showed that magnetic susceptibility of most minerals that were investigated was essentially constant in magnetic ﬁelds above those needed to saturate the ferromagnetic constituents, in agreement with eq. (1.44). Figure 1.34 illustrates some of the results. Hysteresisgraphs Hysteresisgraphs are systems for testing and analyzing hysteresis properties (BH loop) of hard and soft magnetic materials. The commercially available units are usually precision personal computer-controlled systems. Designers of permanent magnet-based magnetic separators can use such instruments to test, analyze and quality-control hard magnetic materials such as ferrites, Alnico, samarium-cobalt and neodymium-iron-boron alloys. Figure 1.35 illustrates such a hysteresisgraph.

1.7

Sources of magnetic ﬁeld in magnetic separation equipment

The aim of magnetic separation is to recover or remove particles with sizes ranging from several tens of millimeters down to a fraction of micrometre, with a wide spectrum of magnetic susceptibilities, from ferromagnetic to weakly paramagnetic. Furthermore, it is frequently necessary to separate two or more ma-

46

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.34: Magnetic susceptibilities of various minerals, measured by VSM, as a function of magnetic ﬁeld strength (adapted from [D2]).

Figure 1.35: Hysteresisgraph Permagraph (courtesy of Magnet Physik GmbH) for quality control of permanent magnets.

1.7. SOURCES OF MAGNETIC FIELD

47

terial species, the magnetic susceptibilities of which do not dier very much, of a wide range of particle sizes. The magnetic ﬁeld strength needed to recover such particles, therefore, varies substantially from one application to another and dierent ways of generating the magnetic ﬁeld are employed. As can be seen from eq. (1.8), the magnetic force required to separate a magnetizable particle depends not only on the physical properties of a material, and on the magnetic ﬁeld strength, but also on the value of the gradient of the magnetic ﬁeld. Therefore, to achieve a selective separation of a valuable material from unwanted ones, a carefully selected combination of the magnetic ﬁeld strength and its gradient must be used to warrant a high recovery and simultaneously a high grade of the concentrate. Magnetic separation can be considered successful only if it produces the right quality of the concentrate with the right recovery. In some applications of magnetic separation, for instance in magnetic ﬁltration, the ”brute force” approach is often used to ensure a high degree of removal of magnetizable solids from suspension. Consequently an eort is usually made to maximize the external magnetic ﬁeld or the ﬁeld gradient, or both. This approach is also employed in some applications in mineral processing, for instance in removal of magnetic contaminants from industrial minerals. Such a combination of high magnetic ﬁeld and ﬁeld gradient often results in a high-quality non-magnetic product, at the expense of losses of the non-magnetic component into the magnetic fraction. Undue emphasis on the magnetic ﬁeld strength and/or ﬁeld gradient sometimes results in reduced recovery of the valuable components and reduced selectivity. Excessively high capital and operating costs are additional consequences of such an approach. In the majority of applications, only a moderate magnetic ﬁeld, combined with an optimized ﬁeld gradient, are required to achieve the optimum results. The desired magnetic induction and the ﬁeld gradient are thus a function of the type of application, required metallurgical performance and economic criteria. In the following section the basic methods of the generation of magnetic ﬁelds and their gradients, as used in magnetic separation, will be reviewed.

1.7.1

Permanent magnets

Recent years have seen a strongly increasing industrial demand for permanent magnet materials. Permanent magnets have become essential components in many electric, electronic and electromechanical devices, including magnetic separators. Although the earliest permanent magnet, lodestone, was known in ancient times, the greatest strides in magnet development have occurred only over the past hundred years. Each advance has been connected with the discovery of a new class of materials, characterized by ever more desirable properties. This evolution has been monitored generally by one ﬁgure of merit for a permanent magnet, the maximum energy product (EK)max , which provides a measure of the ﬁeld that can be produced outside a unit volume of magnet material. The so-called theoretical maximum energy product, the largest value realizable in

48

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT Table 1.13: Magnetic properties of Alnico alloys. Material

Alnico Alnico Alnico Alnico Alnico

5 5-7 5DG 8B 9

Bu [T]

Hf [Oe]

Hfl [Oe]

1.27 1.34 1.33 0.9 1.05

640 740 685 1600 1500

645 745 690 1640 1515

(BH)max [MGOe (kJ/m3 )] 5.5 (44.0) 7.5 (60.0) 6.5 (52.0) 6.75 (54.0) 10.5 (84.0)

principle, is an intrinsic quantity deﬁned by (EK)max =

1 Mv 2 ( ) 0 2

(1.49)

where Mv is the saturation polarization (in [T]). This maximum energy product (in [J/m3 ]) can be achieved only if the magnet retains Mv in a reverse ﬁeld at least as large as Mv @2 [H4]. The maximum energy product is thus limited, to perhaps 1.2×106 kJ/m3 (150×106 MGOe), by the maximum saturation polarization of elements and alloys of approximately 2.5 T. At the present time, one third of this maximum has been achieved with NdFeB material. The chronological trend of the maximum energy product achieved in various permanent magnet materials is shown in Fig. 1.1. It can be seen that there are four major families of permanent magnet materials: Alnico, ferrite, rare-earth-cobalt and rare-earth-iron.

Alnico A major advance in permanent magnet technology began in 1932 with the discovery of excellent magnetic properties of an aluminium-nickel-iron alloy, Alnico. Numerous subsequent investigations resulted in many variations in composition and properties. Alnico magnets are expensive when compared to ferrite magnets since they contain 20% to 40 % of cobalt in addition to other components. Alnico alloys have desirably high remanent magnetization, good thermal stability, but comparatively low coercivities. Curie temperature is about 900 0 C and the maximum recommended operating temperature is 500 0 C. Alnico magnets are very resistant to corrosion, nearly as resistant as stainless steel. Only slight discolouration of the surface is encountered when a magnet is heated in air to 450 0 C [P4]. The physical properties of Alnico alloys are rather poor. High coercivity is closely accompanied by extreme hardness and brittleness. Forming is by casting or sintering as close as possible to the desired size and shape. For close tolerance it is necessary to cut or wet-grind the magnet [P4]. Magnetic properties of several grades of Alnico are summarized in Table 1.13.

1.7. SOURCES OF MAGNETIC FIELD

49

Table 1.14: Magnetic properties of the ferrite magnets. Material Ferrite 5 Ferrite 7B Ferrite 8A Ferrite 8D Ferrite 8C

Bu [T] 0.395 0.38 0.39 0.40 0.43

Hf [Oe] 2200 3250 2950 3100 4100

Hfl [Oe] 2230 3800 3000 3000 2200

(BH)max [MGOe (kJ/m3 )] 3.6 (29.0) 3.3 (26.0) 3.5 (28.0) 3.8 (30.0) 4.3 (34.0)

Ferrite magnets A new class of permanent magnetic materials was announced in 1952. The materials were based on the crystal anisotropy of barium oxide. This class of magnets is generally known as ferrite, but is sometimes referred to as oxide or ceramic magnets. Today, ferrite magnets are by far the most widely used magnets. The success of ferrites is due to several reasons. The raw materials are inexpensive and non-strategic. Their high coercive force combined with reasonably high magnetic induction has allowed permanent magnets to be incorporated into many types of devices. Ferrites are mechanically hard and brittle and their magnetic properties are characterized by relatively low remanent magnetization while the coercive force is satisfactory. The Curie temperature is 450 0 C and the recommended maximum operating temperature is 250 0 C. At the same time, surfaces of ferrite magnets are stable and are not subject to oxidation. Ferrites are produced by powder metallurgy. Their chemical formula can be expressed as MO·6(Fe2 O3 ), where P is Ba, Sr or Pb. Strontium ferrite has a higher coercive force than barium ferrite and is produced on a larger scale [P4]. Ferrite magnets are available in isotropic and anisotropic grades. Magnetic properties of various grades of ferrites are shown in Table 1.14. Samarium-cobalt-based rare-earth magnets The family of rare-earth permanent magnets (REPM) has evolved in the last 35 years. The materials quickly surpassed all earlier magnets, with currently best values of energy product and coercivity, both being 5 to 10 times those of Alnico and ferrites. While they are rather costly for universal use, the REPM, together with the hard magnetic ferrites, are rapidly broadening applications of permanent magnets in general [S9]. Two major subgroups are being distinguished: rare-earth Co-based magnets (particularly Sm-Co) and rare-earth Fe-based magnets represented by Nd-Fe-B. The latter third-generation REPM, in rapid development since 1983, use cheaper, more plentiful raw materials than Sm-Co and oer still higher energy density at room temperature. Sm-Co-based rare earth magnets are of two types: the SmCo5 group and Sm2 Co17 group. These two groups constitute the ﬁrst and second generation rare-earth magnets, respectively [H5]. SmCo5 alloys are the most basic materials that make up rare-earth magnets. More advanced Sm2 Co17 alloys were devel-

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

50

Table 1.15: Magnetic properties of Sm-Co magnets [W1]. Material SmCo5 Sm2 O17

Bu [T] 0.90 1.10

Hf [kOe] 9.0 10.0

Hfl [kOe] 29.0 33.0

(BH)max [MGOe (kJ/m3 )] 20.2 (162.0) 37.5 (300.0)

oped following the success of SmCo5 , to obtain higher performance. In order to increase its rather low coercivity, the latter alloy is now based on Sm-Co-Cu composition. The general composition of this new class of Sm-Co magnets is R(Co,M)} , where U stands for at least one rare-earth element, P for a combination of transition metals and/or copper and } is between 6 and 8.5. These multicomponent magnet alloys are generally termed the 2:17 systems. They have the advantage of higher magnetization and use less Sm and Co. As a results of their high Curie temperature of 700 0 C to 800 0 C, Sm-Co-based permanent magnets satisfy the needs for applications with operating temperatures up to about 300 0 C. Further demand for operation at even higher temperatures has led to development of a new class of Sm-based alloys, which can operate at temperatures as high as 550 0 C [W1]. Magnetic properties of Sm-Co magnets are listed in Table 1.15. The samarium-cobalt materials are attractive replacements for electromagnets in many applications, but their use has been constrained by economic disadvantages. Samarium is the least abundant, and hence the most expensive, of the light rare earths, and this unfavourable circumstance is compounded by the fact that the price and availability of cobalt are subject to large, unpredictable excursions. The bulk of cobalt is mined in Congo and regional political instability in Africa resulted in diminished supplies and radically increased prices. This situation led to a continued eort to develop alternative high performance magnets not containing cobalt. Neodymium-iron-boron magnets Iron-based materials having the characteristics of Sm-Co had long been desired and in 1983 two dierent processing routes were announced. The standard powder metallurgy route (Sumitomo route) [S10] and the melt-spinning method (General Motors route) [C3] were proposed for the production of Nd-Fe-B permanent magnets. In the ensuing years production and application of this new type of magnet has been steadily increasing. It has been predicted that the NdFeB permanent magnet market will grow from the 2002 value of $2 billion to $4.8 billion in 2007 [B7]. Presently three common fabrication routes can be used to categorize NdFeB magnets: sintering, polymer bonding and hot deformation. The most successful procedure on the production scale is the powder metallurgical method. The reason is that sintered NdFeB magnets have outstanding magnetic properties, good productivity and superior energy e!ciency and cost performance. On

1.7. SOURCES OF MAGNETIC FIELD

51

Figure 1.36: Progress in development of NdFeB sintered permanent magnets (after [K4]). the other hand, sintered NdFeB magnets have certain disadvantages in terms of thermal and environmental stability. The theoretical value of the maximum energy product of the magnetic Nd2 Fe14 B phase is 512 kJ/m3 (64 MGOe) [S11]. So far, energy products exceeding 400 kJ/m3 have been achieved, with the latest record of 444 kJ/m3 (55.8 MGOe) [K4]. Progress in development of NdFeB sintered magnets is depicted in Fig. 1.36. Bonded magnets have intermediate energy products of 80 to 145 kJ/m3 (10 to 18 MGOe) and can be formed into intricate shapes. Hot deformed magnets possess intermediate to high energy product of 120 to 370 kJ/m3 (15 to 46 MGOe), isotropic and anisotropic properties and the potential to be formed into net shapes. Comparison of magnetic properties of several types of NdFeB permanent magnets is shown in Table 1.16. While NdFeB permanent magnets possess outstanding magnetic properties, they have insu!cient level of thermal and environmental stability. The Curie temperature of the NdFeB alloys is about 310 0 C. This proximity to the room temperature limits the practical range of applications of NdFeB magnets and causes appreciable changes in the ﬂux density as the temperature varies. Operation of a permanent magnet at elevated temperatures can result in structural changes, which in turn lead to irreversible losses of magnetic properties. Table 1.17 compares the loss of remanent magnetization, at 20 0 C, of various magnet materials, after exposure to the indicated temperature. Another study [F4] observed that after 30 minute exposure to the temperature of 220 0 C NdFeB magnets lost up to 80% of their magnetization. The maximum operating temperature of NdFeB magnets is about 150 0 C.

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

52

Table 1.16: Magnetic properties of NdFeB permanent magnets [B7]. Magnet

Sintered VCM Bonded MQ1-B Hot-pressed MQ2-E Die-upset MQ3-F Sintered (Sumitomo) [K4]

Bu [T]

Hfl [kOe]

1.31 0.69 0.825 1.31 1.51

14 9 17.5 16 8.68

(BH)max [MGOe (kJ/m3 )] 42 (336.0) 10 (80.0) 15 (120.0) 42 (336.0) 55.8 (445.0)

Table 1.17: Temperature-induced irreversible losses in permanent magnets [P4]. Magnet Alnico Ferrite SmCo5 NdFeB

-600 C -1.45% -27% 0 0

+1000 C 0.4% 0 0.5% 6.5%

+2000 C 0.8% 0 1.7% 65.0%

+3000 C 1.1% 0

Comparison of the Curie and maximum operating temperatures for various permanent magnets is given in Table 1.18. NdFeB permanent magnets are also sensitive to attack by both climatic and corrosive environments, resulting in a deterioration of the magnetic and physical properties. It appears that the susceptibility to corrosion is a problem that all NdFeB magnets experience, regardless of the fabrication process [H6]. It was found [C4] that the corrosion rate increases more with an increase in the humidity level than it does with an increase in the environmental temperature. It was also observed that nitrogen in the air retards the rate of corrosion. In practice, surface protection by epoxy resins or by Al coating, combined with chromating is applied. Typical coating thickness is from 10 m to 24 m for Al-chromated and about 25 m for electrically deposited epoxy [H6]. The application of two separate coatings, shot-peened and chromated aluminium deposited by ion vapour

Table 1.18: Curie and maximum operating temperatures of various permanent magnets. Magnet Ferrite Alnico RECo5 NdFeB

Curie temperature [0 C] 450 900 700 310

Maximum operating temperature [0 C] 350 500 250 150

1.7. SOURCES OF MAGNETIC FIELD

53

deposition and electropaint deposited cathodically have been shown to resist a variety of climatic and corrosive atmospheres [M3]. Permanent magnets in magnetic separation The early history of magnetic separation is closely associated with permanent magnets, which were used to remove strongly magnetic matter from wastes or to recover strongly magnetic (mostly iron) minerals from ores. With the development of powerful electromagnets the interest in permanent magnets as applied to magnetic separation temporarily diminished. In recent years, however, we have witnessed a remarkable renaissance of interest in permanent magnets, a phenomenon associated with the dramatic development of novel permanent magnets materials, based on rare earths. Although the magnetic induction that can be generated by permanent magnets rarely exceeds 1 T, the value that can be easily produced by electromagnetic coils, in a much larger volume, permanent magnets oer several advantages over electromagnets. In small devices, permanent magnets have major advantages over electromagnetism. Even in large systems, however, permanent magnets are a good solution, as a result of their advantageous volume e!ciency, low operating costs and simple support facilities. And very importantly, permanent magnets do not require a source of energy or a cooling ﬂuid.On the other hand, permanent magnets possess a few disadvantages, among them the fact that the magnetic ﬁeld is di!cult to vary and that it cannot be switched o. As a result of notable development of new permanent magnet materials during the last three decades, permanent magnets are currently used in a wide range devices for magnetic treatment of materials. In most applications, in which a relatively short reach of the magnetic force is required, permanent magnets replaced electromagnets. Permanent magnetic rolls, magnetic pulleys, suspended magnets, high-ﬁeld permanent drum magnetic separators and eddy-current separators are typical examples. Even in those applications of magnetic separation where the magnetic force must be generated in a relatively large volume, permanent magnets are employed. Multiple-ring high-gradient magnetic separators are an example. In the application of magnetic techniques in biosciences permanent magnets are an essential part of biomagnetic separators and devices for drug targeting and hyperthermia.

1.7.2

Iron-core electromagnets

Of the several ways of generating a magnetic ﬁeld in magnetic separation, the choice is dictated mainly by the required ﬁeld magnitude, by the volume in which a given magnetic ﬁeld is to be generated and by methods used to generate the ﬁeld gradient. An eective separation of weakly magnetic particles of a small size often requires an increase of both the magnetic ﬁeld and of its gradient beyond the values available with permanent magnets. Furthermore, as the magnetic ﬁeld falls very rapidly from the surface of a permanent magnet, the eective volume in which a su!ciently high magnetic force can be created is limited.

54

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT U - DIPOLE Coils

Iron Yoke

Figure 1.37: Schematic cross-section of the U-dipole iron-core electromagnet, with two possible positions of the magnetizing coils. Therefore, in order to generate a su!ciently high magnetic ﬁeld in a large volume that would guarantee a large throughput of a magnetic separator, an electromagnet must be used. Of the several ways of generating a magnetic ﬁeld by an electromagnet, the choice is dictated by consideration of the required ﬁeld magnitude, the volume in which the ﬁeld is to be generated and by the duty cycle of the separation process. The relative importance of these considerations usually determines the method with little overlapping of choice. For example, if the separation process requires a magnetic ﬁeld less than 2 T in a relatively small volume, an iron-core electromagnet is a good choice. For the ﬁeld of 2 T or less, in a large volume, a water-cooled iron-clad solenoid should be used, although a superconducting magnet could also be a choice. Magnetic ﬁelds in excess of 2 T will undoubtedly dictate the use of superconducting solenoids. In iron-core electromagnets, the electric current passing through the windings magnetizes a great mass of iron, which in turn produces a ﬁeld in the working volume. Judicious location of the iron and of the windings may increase considerably the e!ciency of the magnet. Although the ﬁeld strength obtained in this way is limited by the saturation magnetization of iron, for most large-scale applications of magnetic separation for the recovery of weakly magnetic materials, the magnetic force generated by such iron-core electromagnets is usually su!cient. Design of iron-core electromagnets is largely a matter of practical experience, and it is generally considered impossible to predict accurately the ﬁeld which a particular magnet will produce [I1]. The situation has improved recently, when modern computer modelling software has been made available to magnet de-

1.7. SOURCES OF MAGNETIC FIELD

55

C DIPOLE Iron yoke Coils

Figure 1.38: Schematic cross-section of the C-dipole iron-core electromagnet.

signers. The fact that the ﬁeld magnitude and conﬁguration is almost always determined by the iron pole pieces has both advantages and disadvantages. On the one hand, the presence of iron permits useful values of the magnetic induction (say, up to 2 T) to be reached with modest investments in magnetomotive force (ampere-turns). Iron also conﬁnes the stray magnetic ﬂux to the immediate vicinity of the gap of the magnet. On the other hand, numerous drawbacks are due to the properties of iron such as nonlinearity, saturation, hysteresis and remanent ﬁeld. Figures 1.37 and 1.38 schematically illustrate cross-sections of the U-dipole and C-dipole electromagnets. These conﬁgurations are frequently used in the design of magnets for magnetic separators. The U-dipole design has been employed in conventional wet high-intensity magnetic separators (WHIMS) such as Jones (Humboldt Wedag), Eriez Magnetics or Boxmag-Rapid. On the other hand, the C-dipole conﬁguration is used, for instance, in induced magnetic roll separators. A detailed description of such units will be given in Chapter 2, while the fundamentals of the design of iron-core magnets will be discussed in Chapter 4. It is clear from Figs. 1.37 and 1.38 that as the working space of the magnet becomes larger, the iron core and the coils also become larger and therefore require increasing amount of power to generate the required magnetizing ﬁeld. There is a deﬁnite crossover point at which a greater magnetic ﬁeld can be generated for the same power in a solenoid of bore equal to the gap of the ironcore magnet [M4]. Iron can still be used in the form of a cladding surrounding the magnet.

56

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT Energising coils

Iron cladding

Working volume

Figure 1.39: Comparison of a solenoid magnet (solid lines) and an iron-core electromagnet (dotted lines).

1.7.3

Solenoid electromagnets

As has been already mentioned, the magnetic induction obtained with iron-core electromagnets is limited by the saturation of the iron. To obtain still stronger ﬁelds, at even larger volume, one has to return to the original technique of the magnetic ﬁeld generation, namely the construction of a solenoid. Instead of making use of the magnetization of iron, the ﬁeld should be obtained directly from the current in the electrical conductor. Hence the magnet must be constructed in such a way that the windings are as close as possible to the ﬁeld space, and the current through them must be as high as possible. Thus we come to a magnet consisting of a short coil, usually clad with a steel return frame which facilitates the passage of the magnetic ﬂux. Comparison of ironcore electromagnet with an iron-clad solenoid both having the same width of the working space is shown in Fig. 1.39. The total magnetic induction in the working volume of a magnet is equal to the sum of the contribution from the coil (Ef ) and of the contribution from the magnetized iron (El ) Ewrw = Ef + El (1.50) Approximately 75% to 90% of El comes from the iron in the proximity of the working volume. Therefore, approximately the same portion of iron of the yoke could have been eliminated without reducing El [M5]. Contribution from the coils to the ﬁeld in the working gap in iron-core conﬁgurations (Figs. 1.37 and 1.38) is thus generally rather small. The coils are used mainly to magnetize

1.7. SOURCES OF MAGNETIC FIELD

57

Figure 1.40: Contribution from iron cladding and from the coil to the total magnetic induction in the iron-clad solenoid. iron and to generate high El . Nevertheless, if the iron-clad solenoid is used, the contribution from the coil to the magnetic induction Ef from the coil is much higher than in the iron-core magnet, while El remains the same. Comparison of the magnetization curves for these two magnetic circuits is shown in Fig. 1.40. It can be seen that El (iron-core magnet) u El (iron-clad solenoid) and Ef (iron-core magnet) ?? Ef (iron-clad solenoid). It is thus clear that the iron-clad solenoid uses much less material and exhibits better parameters. The concept of iron-clad solenoids has been used successfully in the design of magnetic separators. Design of conventional high-gradient magnetic separators that operate in a cyclic mode, such as those used to beneﬁciate kaolin, is based on an iron-clad solenoid. Several designs of continuous HGMS machines, such as Sala-HGMS carousel separator, VMS and SLON separators also use the ironclad solenoid approach.

1.7.4

Superconducting magnets

Superconductivity is a remarkable phenomenon whereby certain metals and other compounds, when cooled to very low temperatures, become perfect conductors of electricity. Unlike the gradual changes in electrical resistance shown by all metals at more familiar temperatures, the superconducting state appears quite abruptly at a critical temperature Wf , which is characteristic of the metal in question. It is accepted that below this temperature the resistance of conventional class II superconductors suitable for magnet manufacture is indeed zero [H7]. Critical temperatures of these superconductors are very low, a few Kelvin (K), and the use of liquid helium as a refrigerant is essential. In recent

58

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Table 1.19: Critical temperatures and magnetic induction of assorted superconductors. Material Nb3 Sn NbTi V3 Ga Nb3 Al Y-Ba-Cu-O Hg-Ba-Ca-Cu-O

Tf [K] 18.0 10.6 15.0 16 - 20 92 135 - 160

Bf [T] at 0 K 28 15 26 35 140 (k)> 29 (B) 1150 (k), 149 (B)

years, however, remarkable progress has been achieved in developing materials that become superconducting at temperatures as high as 160 K [M6, F5, C5]. After the discovery of superconductivity in 1911, it was recognized that large electromagnets, capable of generating high magnetic ﬁelds and consuming no power, could be built. However, these hopes were quickly dashed when it was discovered that superconductors, in addition to their critical temperature, have a critical ﬁeld Ef , above which they revert from the superconducting state to a normal resistive state. Metals that were investigated at those times, i.e. mercury, lead and tin, the so—called class I superconductors, exhibited very low critical ﬁeld, of the order of 0.05 T. The era of superconducting magnets started only in 1960 after the discovery of the high-ﬁeld properties of new class II superconductors, namely Nb3 Sn and NbTi. During the following years, the search for new materials of ever higher performance was actively carried out and a multitude of composites, such as V3 Ga and Nb3 Al, were investigated. Most of these materials proved to be di!cult to prepare in the form of conductors and progressively disappeared [D7]. The only materials available commercially at present are the two very ﬁrst Nb3 Sn and NbTi. The latter is by far the most widely used because of its excellent mechanical properties, while the former one, although di!cult to work with, is the only choice for ﬁelds exceeding 10 T [D7]. Critical temperatures Wf and critical magnetic induction Ef of assorted superconducting materials are summarized in Table 1.19. There are three obvious areas where superconducting magnets will have considerable impact. The ﬁrst area covers all applications which will beneﬁt from a signiﬁcant reduction in the consumption of electrical energy. The second area includes those applications in which the reduction of the mass and size of the magnet is important. The third area is the market for very high ﬁeld magnets where there is no viable alternative, or the magnets that can generate magnetic ﬁeld in a large volume. An example of a superconducting solenoid is shown in Fig. 1.41. As discussed above, conventional magnets make use of iron yoke or cladding to reduce magnetic reluctance, thereby minimizing the number of ampere-turns required. Superconducting magnets do not suer from this constraint because additional ampere-turns are to be had relatively cheaply and do not signiﬁcantly

1.7. SOURCES OF MAGNETIC FIELD

59

Figure 1.41: A superconducting solenoid for high-energy experiments (courtesy of Ansaldo spa.). aect the refrigeration power load. For this reason iron core or cladding are seldom used to augment the working ﬁeld, but they are often used for shielding, to reduce stray magnetic ﬁelds [W2]. All these three areas play a role in the application of superconductivity to magnetic separation. With the use of a superconducting magnet in material separation it should be possible to generate very high magnetic ﬁelds at low input power, in large volumes. On the other hand, the need for these very high magnetic ﬁelds in material separation has not been su!ciently convincingly demonstrated. Although it was envisaged [K1] that magnetic separation will be the ﬁrst industrial application of superconductivity, superconducting magnets have not yet made a signiﬁcant impact in material processing. Superconductivity has found application in cyclically operating solenoidbased high-gradient magnetic separators for beneﬁciation of kaolin. Further development resulted in industrial-scale operation of continuous reciprocatingcanister HGMS. On the other hand, superconducting drum magnetic separators and open-gradient magnetic separators have not been, so far, successfully introduced into the material treatment industry.

1.7.5

Generation of the magnetic ﬁeld gradient

As transpires from eq. (1.8), the magnetic force acting on a magnetizable particle in a magnetic separator is determined not only by the strength of the magnetic ﬁeld but also by its gradient. A suitable combination of these parameters must be determined for each application. It is thus essential to provide

60

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.42: Pattern of the magnetic ﬁeld around a suspended magnet. not only a strong magnetic ﬁeld but also a non-uniform ﬁeld. A large variety of designs have evolved over the years to render the magnetic ﬁeld non-uniform and to produce suitable magnetic gradients. Separators based on these modes of the ﬁeld gradient generation can be classiﬁed into three basic categories: • Open-gradient separators • Closed-gradient separators • Matrix (polygradient) separators In open-gradient separators the ﬁeld gradient is generated in several ways: a. As a result of the natural non-homogeneity of the ﬁeld caused by the dependence of the ﬁeld on the distance from its source. Typical examples are overband, suspended, plate and grate magnets. The pattern of the magnetic ﬁeld around a suspended magnet as shown in Fig. 1.42 illustrates the formation of the ﬁeld gradient in the separation zone below the magnet. b. By special arrangements of permanent magnets or of the windings of electromagnets so that the patterns of alternate polarity are generated. Magnetic rolls, pulleys and drum separators use this type of the ﬁeld gradient. Multipolar windings of conventional or superconducting coils with alternating polarity are employed in open-gradient magnetic separators (OGMS). Fig. 1.43 illustrates the open-gradient magnetic system of a drum magnetic separator while Fig. 1.44 shows the 3D pattern of the ﬁeld around a permanent magnet roll. The magnitude of the gradient and the reach of the magnetic force are determined, among other things, by the dimensions of the permanent magnet elements or

1.7. SOURCES OF MAGNETIC FIELD

61

Figure 1.43: Pattern of the magnetic ﬁeld around a magnetic drum [U1].

electromagnetic winding relative to the dimensions of the spacers (either air or steel) between these magnetic elements. A schematic view of a linear multipole OGMS system is shown in Fig. 1.45. In closed-gradient separators a high ﬁeld gradient is usually achieved by a suitable shaping of the pole pieces of the opposing magnetic poles. Magnetic ﬁeld is thus focused on the working element of the separator and a high ﬁeld gradient is created. Assorted geometrical arrangements of poles and counterpoles is shown in Fig. 1.46. These dierent geometries, such as a hyperbolic pole facing a ﬂat pole (case A), or a grooved pole (case B), triangular pole and multi-tooth arrangement generate various patterns of the magnetic ﬁeld and its gradient [D4, S12]. The gradient of the ﬁeld and the reach of the magnetic force are the function of the curvature of the poles and the counter-poles, by the pitch of the teeth and by the width of the separation gap. Induced magnetic roll and wet high-intensity magnetic roll separators employ this type of closed-gradient arrangement. Ferrohydrostatic separators with magnetic ﬂuids also generate a closed gradient by a suitable shaping of the pole tips [R1]. Multipolar windings or multipolar arrangements of permanent magnets also generate closed gradient of the magnetic ﬁeld. A quadrupole geometry was used to build a magnetic separator for biomedical applications [Z2, H8]. A sextupole arrangement is employed in Magstream separator with magnetic ﬂuids [W9], while quadrupole magnets, either resistive [A3] or superconducting [C6] were also tested in magnetic separation. Figure 1.47 shows a schematic diagram of a pure quadrupole while the coil and pole arrangement in a conventional quadrupole magnet for physical experiments are illustrated in Fig. 1.48.

62

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.44: Pattern of the magnetic ﬁeld on the surface of a permanent magnetic roll.

Figure 1.45: A multipole open-gradient magnetic system.

1.7. SOURCES OF MAGNETIC FIELD

63

B

A

D

C

Figure 1.46: Shapes of poles and counter-poles in magnetic separators with closed gradient.

S pole

N pole F B B

F

F

B B

N pole

F

S pole

Figure 1.47: Magnetic ﬁeld and forces inside a quadrupole magnet. Particles are entering the paper.

64

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.48: A quadrupole resistive magnet for high-energy physics experiments (courtesy of Danfysik A/S).

Figure 1.49: Magnetization curves for bulk steel and steel wool (after [K5]).

1.7. SOURCES OF MAGNETIC FIELD

65

Table 1.20: Typical values of the gradient of the magnetic ﬁeld in magnetic separators. Separator Suspended magnet Nd magnetic roll Nd drum separator Davis tube Frantz isodynamic Belt separator Steel wool (HGMS) Steel balls (WHIMS) Expanded metal Grooved plates Split pair OGMS FHS Magstream

Gradient of the magnetic ﬁeld T/m kG/cm 0.8 0.08 200 20 80 8 10 1 20 2 1 - 10 0.1 - 1 2.5×104 2.5×103 3 1×10 100 4×103 400 2×103 200 40 - 100 4 - 10 2 0.2 30 3

In matrix (polygradient) magnetic separators, the gradient of the magnetic ﬁeld is generated by means of induced magnetic moment in the ferromagnetic bodies (called the matrix) and placed in the external magnetic ﬁeld. Strong magnetic ﬁeld gradient is generated in the close vicinity of these bodies and its magnitude depends on the size and the shape of the matrix elements. Ferromagnetic bodies of various shapes have been used in high-intensity magnetic separators (such as balls, grooved plates, mesh, expanded metal, steel wool, rods etc.) and a proper choice of the matrix is one of the crucial prerequisites for successful separation. Since the ﬁeld gradient is inversely proportional to radius d of the matrix element, i.e. uE [email protected], the magnetic force acting on the magnetizable particles is maximized by using as ﬁne a matrix as possible. On the other hand, the dimensions of the matrix elements must be selected taking into account particle size of the material to avoid straining and to ensure the selectivity of separation. At the same time, the dimensions of the matrix bodies must be chosen in such a way that the magnetic force is su!ciently strong to recover the magnetic fraction. On the other hand, the magnetic force must not be too strong to cause the matrix blockage and retention of the ”non-magnetic” component. In order to magnetize a ﬁne matrix, su!ciently strong external magnetic ﬁeld is required. This is because the ﬁlling factor of the matrix is often low and the matrix does not conduct magnetic ﬂux very well. Typically, the ﬁlling factor ranges from 0.04 (4%) for steel wool matrix to about 0.20 (20%) for expanded metal. The exception is the ball matrix where the ﬁlling factor can be as high 0.50, and grooved plates with the ﬁlling factor up to 0.80. Figure 1.49 illustrates that a background magnetic induction of at least 0.7 T is needed to saturate the steel wool matrix, compared to about 0.2 T that is necessary to

66

CHAPTER 1. PRINCIPLES OF MAGNETIC TREATMENT

Figure 1.50: The magnetic ﬁeld lines around a cross-section of a magnetized steel sphere or steel wire. saturate the bulk material. The large background induction needed to saturate steel wool is a result of demagnetization eects. A large proportion of ﬁlaments in the randomly orientated steel wool is arranged along the di!cult axis of magnetization and exhibits thus a large demagnetization factor. The pattern of the magnetic ﬁeld around a magnetized steel wire or steel sphere is shown in Fig. 1.50. Typical values of the gradient of the magnetic ﬁeld for various types of magnetic separators are given in Table 1.20.

Chapter 2

Review of Magnetic Separation Equipment and Techniques In reviewing magnetic separators, it is necessary to examine hundreds of patents and papers and it is not possible to give adequate coverage to all of these. Moreover, there appear to be more models and modiﬁcations of magnetic separators than there are applications. Since each embodiment of a magnetic separation technique possesses distinct merits as well as limitations, no single technique is universally applicable to all types of magnetic separation. Various classiﬁcation schemes exist by which magnetic separator can be subdivided into categories. These schemes are based upon the dominant physical or technological feature. Magnetic separators can thus be grouped as follows: a) Based upon the medium carrying the ore: • dry • wet b) Based upon the requirement of the system: • removal of iron and similar materials for the protection of machinery subjected to damage or wear • extraction of valuable magnetic constituents • removal of deleterious magnetic impurities • separation of materials based on properties other than magnetic (e.g. density, conductivity) • material handling 67

68

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS c) Based upon the way the magnetic ﬁeld is generated: • permanent magnets • electromagnets with iron yoke • resistive solenoids • superconducting magnets d) Based upon the magnitude of the magnetic ﬁeld and its gradient: • low-intensity magnetic separators • high-intensity magnetic separators • high-gradient magnetic separators.

Low-intensity separators are primarily used for the manipulation of ferromagnetic materials or paramagnetic materials of high magnetic susceptibility, and/or of su!ciently large particle size. These separators can operate either in dry or wet modes. High-intensity separators are used for treatment of weakly magnetic materials, coarse or ﬁne, in wet or dry modes. Very ﬁne, feebly magnetic materials can be treated in high-gradient magnetic separators. From the practical point of view, classiﬁcation according to the requirement of the system is the most illustrative. For example, the application of magnetic separation to iron removal is usually dictated by the material handling system involved. The most commonly used magnetic separators include: • Magnetic pulleys, applied in belt conveyor systems as head pulleys • Suspended magnets, applied over belt conveyor chutes or feeders • Magnetic drums • Plate magnets, applied in chutes • Grate magnets, applied in product streams. For concentration or removal of magnetizable particles, a wide spectrum of magnetic separators is used. These include: • Magnetic pulleys • Magnetic low-intensity or high-intensity drums • Induced magnetic rolls • Permanent magnet roll separators (IMR)

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

69

• Cross-belt and disk magnetic separators • Magnetic ﬁlters • Wet high-intensity magnetic separators (WHIMS) • High-gradient magnetic separators (HGMS) For magnetic material handling, the magnetic systems usually applied are: • Magnetic conveyors • Magnetic rolls • Lifting magnets

Magnets are also used in numerous special applications: • Separators with magnetic ﬂuids, in which material is separated mainly on the basis of its density (FHS, MHS) • Eddy-current separators for separation of non-ferrous metals (ECS) • Dense-medium separators, in which a magnet is used to control magnetic heavy medium • Demagnetizing coils • Magnetic ﬂocculators.

2.1

Dry low-intensity magnetic separators

Dry low-intensity magnetic separators are usually used to remove tramp iron, to concentrate coarse strongly magnetic iron ores, and to recover iron values from blast furnace and steel mill slag. Removal of strongly magnetic impurities from a variety of materials is also accomplished with dry low-intensity separators. Tramp iron magnetic separators are used to protect handling and processing equipment such as crushers and pulverizers. These separators are usually used on dry material or on material which contains only surface moisture. Tramp iron comes in many shapes and sizes. By conventional deﬁnition, tramp iron means that a particle has a signiﬁcant size, which is su!cient to cause damage. Iron of abrasion, or particles smaller than 3 mm in diameter, usually do not cause equipment damage although they can discolour or contaminate the product [D7]. As far as the top size is concerned, large pieces as long as 2 m can be successfully removed. The size and shape of the tramp iron, together with the material handling system used must be considered in selecting the protective magnet.

70

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.1: Magnetic pulley (courtesy of Steinert GmbH).

2.1.1

Magnetic pulleys

An easy and simple way to remove tramp iron from material on a conveyor belt is by means of a magnetic head pulley. These are available both in permanent magnet and electromagnetic construction. They are relatively inexpensive and easy to install, and accomplish continuous tramp iron removal. The magnetic pulley, shown in Figure 2.1, usually replaces the head pulley or the tail pulley of a belt conveyor, converting the conveyor into a magnetic separator. Material carried on the conveyor passes over the magnetic pulley which holds the magnetic particles until they leave the region of the magnetic ﬁeld while the non-magnetic material is discharged over the pulley. A typical installation is shown in Fig. 2.2, while Fig. 2.3 illustrates an actual process of separation by the pulley. The permanent magnetic pulleys can be manufactured with axial poles in which the polarity alternates along the circumference, or radial poles, in which the polarity changes across the width the of the belt. For large particles and elongated shapes, the radial pole design is more suitable. For ﬁnely divided material, the uniformity of the ﬁeld across the belt width makes the axial pole design more advantageous. Strontium ferrite magnets are usually used. Electromagnetic pulleys are used where control of the magnetic ﬁeld is required. The magnetic pulleys are manufactured in a range of diameters, from 500 mm to 1250 mm. The width of the magnetic pulley should be selected to match the belt width. The throughput of magnetic pulleys of dierent dimensions is shown in Figure 2.4. Standard belt speeds for which the throughputs were calculated are shown in Table 2.1. Inclined belts provide additional areas of contact with the magnetic ﬁeld of the pulley and can tolerate higher capacities.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

Figure 2.2: Principle of operation of a magnetic pulley.

Figure 2.3: Operation of a magnetic pulley (courtesy of Steinert GmbH).

71

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

72

Table 2.1: Standard belt speed for magnetic pulley operation. Pulley diameter [mm] 500 630 800 1000 1250

Belt speed [m/s] 1.1 1.45 1.7 2.0 2.2

Table 2.2: Recommended diameters of magnetic pulleys. Feed size [mm] 50 - 100 25 - 50 6 - 25

Pulley diameter [mm] 750 - 900 450 - 600 300 - 450

Throughput [t/h/m] 250 - 400 165 - 250 75 -135

Magnetic pulleys of special design are used in the concentration of magnetite and other ferromagnetic minerals. For the best results, the feed should be screened into sized fractions and each fraction treated on a separate pulley. Typical feed sizes would be - 100 mm + 50 mm, - 50 mm + 25 mm and 25 mm + 6 mm. The magnetic pulley is not suited for the treatment of - 6 mm material. Pulley diameters recommended for various feed sizes are given in Table 2.2 [M7].

2.1.2

Plate magnets

Where the amount of tramp iron contained in a product is reasonably small and where automatic removal is not required, plate and grate magnets can be incorporated in chutes and ducts to remove both tramp iron and iron of abrasion. Such a plate magnet is shown in Fig. 2.5. The plate consists of a series of alternating poles, uniform across the chute width and alternating along the chute length. As the material passes over the magnet face, tramp iron is trapped on the magnet face while the remaining nonmagnetic material proceeds down the chute. The plate magnets must be cleaned and inspected daily since they are not eective if the accumulated tramp iron is allowed to remain on the face. The magnetized plates are usually of permanent magnet type, either ferrite or rare earth. The eective depth of the magnetic ﬁeld can be as high as 200 mm, depending on the type of the magnetic material and on the shape of particles to be removed. A chute angle not exceeding 450 is recommended [M7].

2.1.3

Grate magnets

The grate magnet shown in Figs. 2.6 and 2.7, consists of a series of magnetic tubes, which have poles alternating between one another and along their length.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

73

Figure 2.4: Throughput of magnetic pulleys of various diameters, for dierent widths of the conveyor belt. Standard belt speeds were assumed (after [M7]).

These units are used for granular free-ﬂowing materials ﬁner than 12 mm and are typically mounted at the discharge of a hopper. A number of rows of tubes provide several passes of ﬁnely divided material and can remove essentially all the magnetic particles. The permanent magnets used in the grate magnets are either ferrites, which are suitable for temperatures up to 150 0 C, or NdFeB magnets, with operating temperature up to 90 0 C. For higher temperature applications, up to 350 0 C, the Alnico magnetic grates are also manufactured.

2.1.4

Suspended magnets

Suspended magnetic separators have been used over many decades to improve material purity and to protect processing machinery. Particularly when the belt speed is high and/or if large tramp iron objects are to be removed, suspended magnets are recommended. Suspended magnets are available in both circular and rectangular construction. The rectangular magnet is most commonly used and permits installation of self-cleaning construction. Units based on permanent magnets or electromagnets are manufactured, with the permanent magnet design being restricted to lighter burdens. Simple suspended magnets, designed to remove small amounts or occasional pieces of tramp iron, employ the manual cleaning mechanism. They must be periodically turned o in order to remove

74

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Cleaning position S N

Plate magnet

Figure 2.5: Plate magnet.

Figure 2.6: Grate magnet.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

Figure 2.7: Grate magnet.

Figure 2.8: Principle of operation of an in-line suspended magnet.

75

76

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.9: Installation of a cross-belt suspended magnet (courtesy of BoxmagRapid Ltd.).

iron accumulated on the face of the magnet. Where a large amount of tramp iron is expected, or where access to the magnet for cleaning is di!cult, selfcleaning magnets should be used. A belt driven across the magnet face allows continuous automatic removal of tramp iron. Suspended magnets can be installed at many points in a material handling system: at any point along a conveyor belt, at the discharge end of feeders or screens and above chutes or launders. The preferred location for a suspended magnet is at an angle over the conveyor belt as shown in Fig. 2.8. In this orientation the tramp iron is moving into the face of the suspended magnet and the load is breaking open, allowing easier tramp iron removal. Self-cleaning magnets can be operated across the belt, as shown in Fig. 2.9, and as inline units as illustrated in Fig. 2.10. In the cross-belt mode of operation, the magnet belt moves perpendicularly to the conveyor belt. Because the tramp iron must be attracted and turned by 900 from the movement of the conveyor belt, a cross-belt magnet is usually larger and stronger than an in-line magnet. Typical values of the magnetic ﬁeld as a function of suspension distance for oil-cooled suspended electromagnets, for dierent lengths of the magnet, are shown in Fig. 2.11 [M7]. The selection process for suspended magnets will be discussed in Chapter 5.

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

77

Figure 2.10: Installation of an in-line suspended magnet (courtesy of Steinert GmbH).

Figure 2.11: Magnetic ﬁeld as a function of the suspension distance for oil-cooled suspended electromagnets of dierent lengths.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

78

Figure 2.12: Pole conﬁgurations in drum magnetic separators [M8].

2.1.5

Drum magnetic separators

Drum magnetic separators are probably the most widely used type of magnetic separation equipment. The design of drum separators is predominantly based upon permanent magnet technology, although electromagnetic drums can also be occasionally found in industrial practice. Drum separators are applied to the treatment of particle sizes, which range from several centimeters down to several micrometers, and operate either in a dry or wet mode. While ferrite magnets are used in conventional low-intensity drum separators, recent progress in availability and aordability of rare-earth permanent magnets has resulted in the construction of powerful high-intensity drum separators. The basic design of all drum magnetic separators is essentially the same. Blocks of permanent magnets are arranged in a stationary position inside a non-magnetic rotating drum, as shown in Fig. 2.12. Drums are made in several conﬁgurations depending on the application. The magnet assembly, consisting of three to nine magnetic blocks of alternating polarity, covers an angle usually ranging from 900 to 1200 . As can be seen in Fig. 2.12, in the radial arrangement of the magnets, the polarity alternates across the width of the drum, and is the same along the drum circumference. Such an arrangement is suitable for the removal of elongated tramp iron or concentration of coarse particles when high recovery is required. In the axial arrangement, the polarity alternates along the circumference of the drum and is uniform across the width of the drum. This arrangement

2.1. DRY LOW-INTENSITY MAGNETIC SEPARATORS

79

Figure 2.13: A pattern of the magnetic ﬂux around a magnetic drum.

provides an agitating action enabling the release of entrained non-magnetic particles. The axial arrangement is used when a high quality magnetic concentrate is required, although sometimes at the cost of reduced recovery. The development of improved permanent magnet materials resulted in increased magnetic induction available on the drum surface and at a suitable operating distance from the drum. Conventional ferrite-based drums generate up to about 0.22 T on the drum surface and 0.10 T at 50 mm. In NdFeB-based drums a magnetic induction as high as 1 T can be reached on the drum surface. A pattern of the magnetic ﬂux around a magnetic drum is shown in Fig. 2.13. Drums are manufactured with dierent diameters and widths. While diameters of ferrite drums range from 600 mm to 1500 mm, rare-earth drum are generally smaller, with diameters from 380 mm to 1000 mm. The most common width of the low-intensity drums is 1500 mm, although units 3000 mm wide are also manufactured. Dry low-intensity drum magnetic separators are used mainly for tramp iron removal where magnetic pulleys and suspended magnets are not feasible. With rare-earth magnets, the drums are also able to separate stainless steel and ironbearing minerals. These separators can operate with top feed and bottom feed, as shown in Figs. 2.14 and 2.15. The material to be separated is fed at the top of the rotating drum surface, as shown in Fig. 2.16; the non-magnetic fraction leaves the drum, while the magnetic fraction is retained by the magnetic force at the drum surface until carried outside the eective magnetic ﬁeld. In bottomfeed drums, the magnetic component of the feed is picked up by the magnet while the non-magnetic fraction leaves the system unaected. Drums with top feed produce the highest magnetic removal and are suitable for materials that contain relatively small amount of magnetic particles. However, the drum with

80

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.14: Dry drum magnetic separator with top feed [M8].

Figure 2.15: Dry drum magnetic separator with bottom feed [M8].

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

81

Figure 2.16: Operation of a dry drum magnetic separator (courtesy of Steinert GmbH). bottom feed produces a clean magnetic concentrate with little non-magnetic carry-over and should be used to treat materials containing a high percentage of magnetic particles.

2.2

Wet low-intensity drum magnetic separators

Wet drum magnetic separators are used to recover ferromagnetic solids from a slurry feed. The major areas for their use are in media recovery in dense medium separation plants and in beneﬁciation of magnetite ore. Figure 2.17 shows the recovery of the magnetic particles by a wet drum magnetic separator. Physical construction of wet drum separators is slightly dierent for the two applications, with the ore concentrator being more rugged in construction and subject to more detailed speciﬁcations than the media recovery units. The drum is partially submerged in a tank of water and carries the material to be treated across the face of the magnetic system and the magnetic concentrate out of the tank. The size of the feed treated in these separators rarely exceeds 6 mm while the bottom size of the feed can be as small as 20 m= The design of the tanks for the drum separator is very important and is determined by the objectives of the separation process. There are three basic tank designs, based on the slurry ﬂow: • concurrent • counter-current

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

82

Figure 2.17: A wet drum magnetic separator. • counter-rotation.

2.2.1

Concurrent tank

The concurrent tank design is shown schematically in Fig. 2.18. The feed is introduced at one end of the separator through the feed box and ﬂows in the direction of drum rotation. Magnetic material is picked up by the magnet and the non-magnetic material is discharged at the bottom through the tailings discharge opening. Magnetic particles continue to adhere to the surface of the drum and pass through an opening between the drum shell and the tank wall. The magnetic fraction is then discharged down the discharge lip. The concurrent design of the tank is used mainly for treating coarser material in the size range 5 mm and below. High throughput and high quality of the magnetic concentrate are characteristic features of this design.

2.2.2

Counter-rotation tank

In the counter-rotation design of the tank (Fig. 2.19), the feed is introduced through a special feed box to the drum, which rotates in the opposite direction to the slurry ﬂow. Magnetic material is picked up by the drum and discharged almost immediately. Since the tailings ﬂow along the entire magnetic arc of the drum before being discharged, losses are minimum. This tank design is used

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

Figure 2.18: The concurrent tank.

Figure 2.19: The counter-rotation tank.

83

84

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.20: The counter-current (Steenson) tank. primarily where surges in throughput are experienced, possibly involving high content of the magnetic material. Very high recoveries can thus be achieved with this design, while the grade of the concentrate is of secondary importance only. The particle size can be up to 4 mm, but is preferably smaller than 0.5 mm.

2.2.3

Counter-current tank

The counter-current tank (Fig. 2.20) is used mostly for ﬁnishing where very thorough cleaning is required. The term ”counter-current” refers to the fact that the tailings must ﬂow counter to the rotation of the drum when leaving the separator. Feed is introduced near the bottom of the drum and agitated through wash-water jets. Tailings ﬂow out from the opposite end of the tank through a tailings discharge overﬂow, which also acts as the slurry level control. This ensures a high recovery of magnetic material and a high quality of the concentrate. These tanks are most suited to ﬁnely ground material of 100 m and less.

2.2.4

Design of the drum

The separating drum consists of two main parts: a stationary magnetic circuit and a shell, usually made of stainless steel and often protected by an anti-wear cover. The shell rotates freely around the magnets that cover an angle up to 1500 . The choice of the permanent magnet material and design of the magnetic circuit are the same as those for dry drum magnetic separators as discussed in Section 2.1.5. The drums are available in 760 mm (30”) to 1200 mm (48”) diameter; 900 mm (36”) drum diameters being the most frequently used. The drum width ranges from 610 mm to 3050 mm, usually in increments of 300 mm.

2.2. WET LOW-INTENSITY DRUM MAGNETIC SEPARATORS

85

Figure 2.21: Throughput of a drum magnetic separator, as a function of the drum diameter (after [K6], [S13]).

With increasing diameter of the drum, the throughput also increases. This is illustrated, for dierent types of tank design, in Fig. 2.21. It appears, however, that the 1200 mm diameter is the optimum size, as a further increase in diameter has not apparently resulted in the corresponding increase in processing capacity [S13]. The increased throughput with increasing drum diameter can be expected as the residence time of particles in the magnetic ﬁeld increases as the length of the magnetic arc increases. This increase in residence time results either in improved recovery of the magnetic particles (possibly with a reduced grade of the concentrate due to increased entrainment of non-magnetic particles) or, at constant recovery, in increased throughput. Large diameter drums usually incorporate a larger pitch of the magnetic poles [S13]. Such a modiﬁcation of the magnetic design then results in a deeper magnetic ﬁeld around the drum and in the ability to treat higher volumes of material. However, a larger pitch of the poles reduces the ﬁeld gradient and thus the magnetic force acting on the magnetizable particles. This could result in a reduced recovery. Figure 2.22 illustrates the operation of wet-intensity drum separators in an iron-ore beneﬁciation plant. A more detailed discussion of practical aspects of operation and selection of wet drum magnetic separators is given in Chapter 5.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

86

Figure 2.22: Wet drum magnetic separators in an iron-ore beneﬁciation plant.

2.3

Dry high-intensity magnetic separators

Weakly magnetic minerals can only be removed from a material stream in magnetic ﬁelds much greater than those available in low-intensity magnetic separators. Dry high-intensity magnetic separation has been used commercially since the beginning of the last century, while wet high-intensity high-gradient magnetic separators were developed only relatively recently. Five types of dry high-intensity magnetic separators are in use: • cross-belt separators • induced magnetic roll separators • permanent magnetic roll separators • magnetic ﬁlters • rare-earth drum magnetic separators.

2.3.1

Cross-belt magnetic separator

The cross-belt magnetic separator is one of the oldest types of separators used to concentrate moderately magnetic ores. The operating principle is shown in Fig. 2.23. Dry material is fed in a monolayer onto a conveyor belt and is carried between the poles of the magnetic system. The belt, with its load, passes

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

87

Figure 2.23: Cross-belt magnetic separator.

between the poles of two or more electromagnets. The lower pole-pieces are ﬂat and immovable, while the corresponding upper pole-pieces are shaped and may be raised or lowered as required for the material undergoing treatment. An endless cross-belt runs around a series of pulleys and across each upper poleface surface at right angles to the conveyor belt. As the material passes, the magnetic particles are attracted to the cross-belt, carried with it towards the discharge side and fall into a bin. The material may be passed successively between several pairs of magnet poles when it is desired to make several products in one pass. Non-magnetic tailings discharge as the conveyor belt passes over its end pulley. Machines with two to eight pairs of poles are available and each pair can be adjusted independently by regulating the position of the upper poles and by altering the current through the coils. The height of the upper pole-pieces above the belt should be set at least 2.5 times the size of the largest particle in the feed. The conveyor belt width ranges from 100 mm to 600 mm and particles ranging from 4 mm to 75 m may be treated, preferably sized into several fractions. Depending on the gap between the poles and on the current setting, the operating magnetic induction ranges from 0.2 T to 2.0 T. The main advantage of the cross-belt separator is that several types of magnetic products can be recovered in one pass. However, low throughput is a major drawback. A ﬁve-pole cross-belt separator is shown in Fig. 2.24.

88

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.24: A cross-belt separator (courtesy of Roche Mining).

2.3.2

Induced magnetic roll separator

The induced magnetic roll (IMR) separator shown in Figs. 2.25 and 2.26 consists of a revolving laminated roll formed of alternate magnetizable and non-magnetic discs. The roll is placed between shaped pole-pieces of an electromagnet. The electromagnet induces a magnetic ﬁeld in the magnetic lamination of the roll and generates regions of high magnetic ﬁeld gradient. Material to be treated is fed in a controlled thin stream by a vibratory feeder to the top of the roll. As the roll revolves, the material passes through a narrow gap between the pole of the magnet and the roll. Non-magnetic particles are discharged from the roll while the magnetic particles are attracted to the roll and report into a separate chute when they enter a region outside the sphere of inﬂuence of the magnet. Ferromagnetic material should be removed with a separate magnetic scalper before feeding to IMR, to prevent plugging the gap. The gap between the feed pole and the roll is adjustable and also the setting of the splitter is of great importance. Depending on the width of the separation gap and the current in the magnetizing coils, the magnetic induction in the gap can approach 2 T. The material to be treated must be dry, free-ﬂowing and for best results it should be in the size range - 2 mm + 100 m. The gap should be set to at least 2.5 times the average grain size. The throughput can range from 1 to 3 t/h per meter length of the roll. IMR separators have been extensively used for the beneﬁciation of beach sands and for the removal of weakly magnetic impurities from glass sand, andalusite, feldspar, wollastonite, magnezite and other industrial minerals. IMRs can also be used for concentration of materials such as chromite, monazite and wolframite. IMRs possess several limitations, namely relatively low throughput, limited particle size range and large mass. In recent years, much simpler and easier to operate permanent magnetic roll separators have replaced IMRs in numerous

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

89

Figure 2.25: Schematic diagram of an induced magnetic roll separator (courtesy of Roche Mining). applications. An induced magnetic roll with bottom feed was developed by Carpco, Inc. It is oered as a laboratory or pilot-scale separator for treatment of particles up to 1 mm in size, in throughputs up to 50 kg/h. The separator, shown in Fig. 2.27, achieves highly selective separation by magnetically lifting weakly magnetic particles against gravity. As no entrapment of unwanted material takes place, the separator is suitable in those applications where the grade of the magnetic concentrate or the recovery of the non-magnetic concentrate are of prime importance.

2.3.3

Permanent magnetic roll separator

Although the idea of a permanent magnetic roll separator, consisting of permanent magnet disks or rings interleaved with mild steel disks, as shown in Fig. 2.28, dates back to 1968 [A4], it was only the advent of rare-earth permanent magnet materials that spurred the rapid development of these machines. A patent by E.L. Bateman Ltd. [Y1] became a starting point for a productive period of competitive development of a wide array of roll separators. Initially Sm-Co permanent magnets were used but they were quickly replaced by NdFeB magnets when they became commercially available. The active part of this separator is a roll consisting of disks or rings of permanent magnets, sandwiched between mild steel rings. The adjacent per-

90

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.26: Reading induced magnetic roll separator (courtesy of Roche Mining).

Figure 2.27: An induced magnetic roll separator with bottom feed (courtesy of Outokumpu Technology, Carpco Division).

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

Permanent magnet ring

91

Steel ring

Figure 2.28: Details of a permanent magnet roll. Table 2.3: Typical values of magnetic induction on the roll surface, as determined from modelling and by measuring using a conventional HallEect probe. Magnet Nd-Fe-B Sm-Co Ferrite

B [T] - modelled 1.9 1.5 0.5

B [T] -measured 1.0 8.0 0.3

manent rings are arranged with the same polarity facing one another. Very high magnetic ﬁelds and ﬁeld gradients are generated on the surface of the roll. As discussed in Section 1.6.1, it is di!cult to measure the real magnitude of the ﬁeld using conventional measuring equipment because the ﬁeld varies over a scale of several hundreds of micrometers. Electromagnetic modelling software, however, allows determination the pattern of the ﬁeld around a roll as shown in Fig. 2.29. Typical values of the magnetic ﬁeld are shown in Table 2.3. The values of the magnetic ﬁeld strength measured using a conventional Hall-Eect probe are also shown. The values of the magnetic ﬁeld strength and its gradient on the roll surface and around the roll are strongly dependent on the conﬁguration of the magnet and steel rings. Thin magnet and steel rings generally produce a very high ﬁeld, the ﬁeld gradient and the magnetic force at the surface of the roll, while a long reach of the magnetic force can be achieved using thicker steel rings. The relative thicknesses of the magnet and steel rings generate a widely diering pattern of the magnetic ﬁelds around the roll. While the most common ratio of the widths of the magnet to the steel is 4:1, the correct choice of the roll

92

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.29: Pattern of the magnetic ﬂux lines around a magnetic roll.

Figure 2.30: Operation of a permanent magnetic roll separator.

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

93

c Figure 2.31: Permanent magnetic roll separator Permroll° (courtesy of E.L. Bateman Ltd.).

conﬁguration is determined mainly by the magnetic properties and particle size distribution of the material to be treated. Operation of permanent magnetic roll separators is schematically shown in Fig. 2.30. For easy removal of magnetic particles, the roll is covered by a belt, which can be as thin as 0.12 mm, to allow the feed material to be as close to the magnet as possible. The belt is supported by an idler roll. Below the conveyor is a hopper which collects the discharging material, while adjustable splitters divert the dierent fractions into collection bins placed beneath the hopper. The most common diameter of the roll used to be 72 mm or 76 mm, while rolls 100 mm and 300 mm in diameter have now become commonly available from several manufacturers. The latter design is based on magnet segments rather than rings. With increasing roll diameter, the residence time of particles in the magnetic ﬁeld, the ﬁeld depth and the e!ciency of separation increase. Alternatively, by increasing the speed of rotation, to maintain the same residence time as with a smaller roll, a higher throughput could be achieved with the roll of a larger diameter. For production-scale applications, the width of the magnetic zone of the roll is either 1000 mm or 1500 mm, although for smaller scale applications 250 mm and 500 mm wide rolls are available. Throughput of roll separators is aected by many factors, which include particle size, particle density, proportion of the magnetic component in the feed and the desired quality of the ﬁnal product. As a guideline, a throughput of 2 to 6 t/h/m can be achieved with material smaller than 2 mm, while larger material can be processed at a throughput up to 15 t/h/m. A modular design enables a number of passes to be arranged into a compact unit.

94

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.32: Installation of multistage Inprosys roll magnetic separators (courtesy of Outokumpu Technology Inc.).

A photograph of a two-stage production-size unit is shown in Fig. 2.31, while Fig. 2.32 illustrates the installation of multistage machines. One of the most important issues that aects operational ﬂexibility, ease of maintenance and cost e!ciency is the belt tracking. Tracking, tensioning and changing the belts can be extremely time-consuming, in addition to a high cost of replacement of damaged belts. Several proprietary tracking and tensioning systems and roll support structure are available and it is claimed that it is possible to replace a belt in less 5 minutes [D8]. The magnetic force generated by the permanent magnetic roll is of the same order of magnitude as that in induced magnetic rolls. A spectrum of minerals that can be successfully treated by either magnetic separator is practically identical. Permanent roll separators, however, possess numerous advantages such as low energy consumption, and smaller mass and ﬂoor space. The absence of an air gap allows treatment of particles as large as 25 mm. A few drawbacks include belt wear and inability to control the magnetic ﬁeld strength. While permanent roll separators are predominantly dry machines, wet units are being used, for instance, for the concentration of diamonds [R2].

2.3.4

High-intensity drum separators

Recent progress in the availability and aordability of rare-earth permanent magnets has resulted in design and construction of powerful high-intensity drum magnetic separators (REDS). Eriez Magnetics were probably the ﬁrst to replace

2.3. DRY HIGH-INTENSITY MAGNETIC SEPARATORS

95

Figure 2.33: Operation of a dry NdFeB drum magnetic separator (courtesy of Outokumpu Technology Inc.). standard ferrite magnets with NdFeB permanent magnets and nearly all current suppliers of REDS adhere to this conventional design philosophy [A13]. Figure 2.33 illustrates the operation of a rare-earth dry drum magnetic separator. A somewhat dierent approach [M13, W6, U1] to the design of the highintensity drum separator was based on a plurality of small magnet blocks whose direction of magnetization changed in small increments, as can be seen in Fig. 2.34. This system which was claimed to require less magnetic material in comparison to a conventional system [W6] to achieve the magnetic induction of 0.7 T on the drum surface, was incorporated into the Permos separator of KHD Humboldt Wedag AG. The density of the magnetic force (or the force index) EuE of a rare-earth drum magnetic separator is much smaller than the force index generated by most roll separators, usually not exceeding 20% of EuE for an NdFeB roll (see Table 1.1). The main reason is that the magnetic ﬁeld gradient in REDS is much lower than that in a roll separator, as a result of the geometry of the magnetic system. On the other hand, the reach of the magnetic force can be extended to greater depths, allowing eective treatment of coarse particles. The current consensus is that roll magnetic separators are not only more powerful than drum magnetic separators, but they also seem to oer greater selectivity and ﬂexibility [A13]. Generation of eddy currents in the rotating shell of the drum separator can be a serious problem because of limited temperature tolerance of NdFeB permanent magnets. The level of these currents depends on the magnetic induction, the number of magnetic poles, the speed of rotation, the shell thickness and the

96

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.34: The magnet structure of the Permos separator [U1].

conductivity of the shell material. Heat will develop in proportion to the drive power that is required for the shell to overcome the braking eect of the eddy currents [A13]. The heat generation, sometimes aggravated by high temperature of the feed material represents, therefore, a problem for standard NdFeB materials, for which a maximum operating temperature of 800 is recommended. In such situations, more advanced magnet materials with a higher temperature tolerance must be used.

2.4 2.4.1

Wet high-intensity magnetic separators Dry separation versus wet separation

Although dry high-intensity magnetic separators have been successfully applied to the beneﬁciation of a large spectrum of minerals, several basic disadvantages exist, which prohibit a wider use of a dry process. For dry magnetic separation to be successful, the ore must be completely dry and it almost invariably requires the ore to be sized into several fractions, each of which must be spread in a monolayer over the separators. With dry methods, care must also be taken to ensure control of a possible dust hazard, an expensive precaution both in capital and operating costs. Furthermore, dry separators have considerably lower throughputs than wet machines. While dry separators frequently yield an excellent separation on material coarser than 75 m, on unsized material containing a large portion of ﬁnes, the wet process is the only acceptable one. Considerable advantages must, therefore, be oered by dry separation to justify its use in preference to wet separation. In order to extend the process of magnetic separation to ﬁne weakly magnetic minerals, wet magnetic separators generating su!ciently high magnetic

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

97

Figure 2.35: The principle of operation of a continuous wet high-intensity magnetic separator. force in the working space must be used. A major development was achieved in this direction in 1955 by Jones [J1], who combined a high magnetic ﬁeld strength with Frantz’s idea of a magnetized matrix [F1]. By this approach, the magnetic force acting on magnetizable particles was increased by several orders of magnitude compared to dry magnetic separators. As shown in Table 1.1, a typical value of the product EuE for an Nd-Fe-B roll separator is 300 T2 /m, while with the magnetized steel wool matrix, this value is as high as 5×104 . Jones’s wet high-intensity magnetic separator (WHIMS) became the starting point of a remarkable progress in this ﬁeld and resulted in the development of a wide array of high-intensity high-gradient magnetic separators. This new type of separators extended the application of magnetic separation to classes of materials otherwise considered untreatable by magnetic means. A schematic diagram of operation of a continuous wet high-intensity magnetic separator is shown in Fig. 2.35.

2.4.2

Iron core-based wet high-intensity separators

Jones high-intensity magnetic separator The production-size Jones wet high-intensity separator is shown in Fig. 2.36 The magnetic ﬁeld in the working gap is generated by a conventional ironcore electromagnet and the ﬁeld gradient is enhanced by a matrix consisting of grooved plates of salient pole or of triangular groove plates, placed in the air gap. The plates, shown in Fig. 2.37, are vertically arranged in plate boxes that are placed around the periphery of the rotors.

98

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.36: Perspective view of a Jones continuous wet high-intensity magnetic separator (courtesy of Humboldt Wedag AG).

Figure 2.37: Grooved plates of Jones WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

99

Figure 2.38: Flush device for the magnetic fraction in the Jones WHIMS.

The slurry is gravity-fed onto the matrix where the magnetic particles are captured onto the plates, while the non-magnetic fraction passes through and is collected in a trough below the magnet. The feed points are at the leading edges of the magnetic ﬁeld. Feeding is continuous due to the rotation of the plate boxes in the rotors. Each rotor has two symmetrically disposed feed points. Before a plate box with captured particles leaves the magnetic ﬁeld, any entrained nonmagnetic particles are washed out by low-pressure water and these middlings are collected in a separate launder under the rotor. When the plate boxes reach the demagnetized zone half-way between the two magnetic poles, where the magnetic induction changes its polarity, and the magnetic ﬁeld is essentially zero, the adhering magnetic particles are washed out with high-pressure water sprays. A ﬂush device is shown in Fig. 2.38. The particles in the slurry feed should be smaller than 1 mm and this determines the gap between the grooved plates. As a rule of thumb, the gap width, measured between two grooved plate tips, should be 1.5 to 2 times the maximum particle size [B8]. Particle size distribution also aects selection of the pitch of the grooves. Salient pole plates are used when a high grade of the magnetic concentrate is required, while triangular groove plates are used when high recovery into the magnetic fraction is important. The height of the plates is 190 mm and the ﬁlling factor of the plate box can range from 50% to 80 %, depending on the type of plates and the gap between them. The maximum magnetic induction in the empty separation space does not exceed 1 T, although values up to 2 T are often stated. Such values can be

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

100

Table 2.4: Various models of Jones WHIMS. Type DP 335 DP 317 DP 250 DP 140 DP 90

Capacity [t/h] 180 120 75 25 10

Mass [t] 114 98 70 30 16

Rotor diameter [m] 3.35 3.17 2.50 1.4 0.9

Figure 2.39: Jones WHIMS DP 317 (courtesy of Humboldt Wedag AG).

achieved with the matrix installed in the plate box. The Jones separators are available in several sizes, some of them are summarized in Table 2.4. A photograph of a DP 317 separator is shown in Fig. 2.39. The Jones magnetic separators have been widely used in the mining industry to beneﬁciate a wide spectrum of minerals. Although these separators have been used to upgrade industrial minerals such as glass sand, feldspar and bauxite, the main area of application has been the concentration of weakly magnetic iron ores. The success of Jones separators has been based on sound mechanical design and reasonably e!cient performance. However, the grooved plates have proved to be an obstacle to long-term trouble free operation. As a result of the high ﬁlling factor of the matrix, several problems have been experienced. The frequently blocked matrix has to be removed from the plate boxes and the hard sediment must be laboriously removed. Also the eort to ﬂush the matrix,

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

101

Figure 2.40: Schematic diagram of the three-stage 6-ERM-35/135 magnetic separator [U2]. which represents up to 80 % of the volume of the plate boxes, with high-pressure water, sometimes results in uncontrolled spillage. 6-ERM-35/135 high-intensity magnetic separator The 6-ERM-35/135 WHIMS was developed in the former USSR in order to meet the increasingly demanding requirements for beneﬁciation of complex oxidized iron ores. It was observed [U2] that Jones separators could not ensure the e!cient separation of ores with complicated mineral composition and ﬁne dissemination, such as the deposits of Krivoy Rog and Kursk Magnetic Anomaly. While the design of the ERM separator is based on the Jones concepts, improved design of the matrix and of the feed mode, and incorporation of several stages of separation in one unit resulted in a greater resistance to matrix blockage, higher recovery and better selectivity of separation [U2, U3, T2]. A schematic diagram of the 6-ERM-35/135 separator is shown in Fig. 2.40. The three-rotor separator has two electromagnetic systems 1, each consisting of a magnetic circuit 2, two blocks of coils 3 and an additional upper pole 4. The rotor blocks 5, shown in Fig. 2.41, are positioned between the poles of the magnetic system. The upper rotor operates as a scalping stage to remove magnetite at a magnetic induction of 0.3 T. The lower rotors recover feebly magnetic particles at increasing magnetic induction, the lowest stage operating at a magnetic induction of 1.3 T. The throughput is speciﬁed as 100 t/h [U2]. The ERM separators are manufactured in the Ukraine by Magnis Co., Lugansk.

102

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.41: A rotor of the 6-ERM-35 magnetic separator. Eriez high-intensity magnetic separator Various designs of the magnetic circuits, diering from that of the Jones separators, were employed by other manufacturers of magnetic separators. For example, in the Eriez WHIMS, the carousel containing the matrix rotates between two poles of the electromagnet, as shown in Fig. 2.42. The background magnetic induction of up to 1.2 T in the air gap is generated by oil-cooled coils. Matrix types commonly used include expanded metal and steel balls. Commercial models range in capacity from 1 t/h to 120 t/h while the required input power ranges from 3 kW to 360 kW. A similar design was used by Boxmag-Rapid in their HIW separators. The matrix in these separators was trapezoidal wire bars placed at an angle in the carousel. For treatment of particles smaller than 30 m, the wedge wire was placed horizontally to increase the residence time. Figure 2.43 illustrates a single-head unit, while a photograph of two single rotor Boxmag-Rapid WHIMS operating in an ilmenite recovery plant is shown in Fig. 2.44.. Reading wet high-intensity separators The Reading wet high-intensity magnetic separators are based on yet another concept of the magnetic circuit design. The magnetic poles of the electromagnetic system, shown in Fig. 2.45 are arranged along the circumference of the carousel with polarity illustrated in Fig. 2.46. The iron cores are magnetized by oil-cooled coils. Each two poles with opposite polarity form a unit in which a high magnetic ﬁeld is generated and in which separation is taking place. The

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

103

Figure 2.42: Two-head Eriez CF-600 WHIMS, with capacity up to 60 t/h (courtesy of Eriez Magnetics, Inc.).

Figure 2.43: A single-head Boxmag-Rapid WHIMS (courtesy of Boxmag-Rapid, Ltd.).

104

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.44: Two Boxmag-Rapid WHIMS machines installed in an ilmenite recovery plant.

Figure 2.45: A detailed view of the magnet poles in the separation zones of the Reading WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

105

Figure 2.46: Schematic diagram of operation of the Reading wet high-intensity magnetic separator (courtesy of Roche Mining).

feed points are located close to the regions of the high magnetic ﬁeld. While the non-magnetic fraction passes through the matrix unaected, the magnetic fraction is ﬂushed from the matrix at the zero ﬁeld points that occur between the poles of like polarity. Grooved plates of the salient type are used as the matrix, with an air gap of 2.5 mm. The radial length of the matrix is 68 mm although a wider version with 120 mm radial length is also available. The throughput of these two versions is 2 t/h to 3 t/h per feed point for the narrower version and 4 t/h to 5 t/h per feed point for the wider model. The Reading WHIMS, shown in Fig. 2.47, are manufactured in several models, namely 4 pole (2 feed points), 8 pole (4 feed points) and 16 pole (8 feed points). The Reading wet high-intensity magnetic separators were developed by Reading of Lismore (Pty.) Ltd., Australia. They are well established in beach sand operations. Concentration of ilmenite, chromite and monazite are typical applications. The units are also applied to the beneﬁciation of ﬁne weakly magnetic iron ores and to puriﬁcation of various industrial minerals such as glass sand. Figure 2.48 illustrates the assembly of Reading WHIMS for application in the beach sand industry. The Reading product range was acquired by Roche Mining MT (formerly MD Mineral Technologies) in 2000.

106

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.47: The Reading 16-pole WHIMS (courtesy of Roche Mining).

Figure 2.48: Assembly of banks of Reading WHIMS.

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

107

Figure 2.49: Schematic diagram of the Ferrous Wheel magnetic separator, operating in rougher/cleaner mode (courtesy of Eriez Magnetics, Inc.).

Ferrous Wheel magnetic separator A Ferrous Wheel separator combines the basic concept of a high-gradient magnetic separator with the low-cost permanent magnet circuit. The principles of design and operation can be seen in Fig. 2.49. The vertical separating ring consists of two discs with the matrix situated in pockets between them, as shown in Fig. 2.50. The rings are assembled into a horizontal drum, the length of which is 5.5 m and outer diameter 2.4 m. Rotational speed of the drum is approximately 2 rpm. The length of the matrix, fabricated from screen cloth, is 150 mm. The choice of the mesh size of the screen cloth is determined by the size distribution of the feed ore. The separating ring is open in the middle to allow the removal of the separated products. Barium ferrite permanent magnets are mounted on each side of the separating rings, as is shown in Fig. 2.51. Each of the two magnetic heads covers an arc of 600 and the magnetic induction generated in

108

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.50: The Ferrous Wheel separating ring with 125 mm wide matrix (courtesy of Eriez Magnetics, Inc.). the gap is 0.1 T. The Ferrous Wheel separator allows a two-stage separation. The separator can be conﬁgured as either rougher/scavenger or rougher/cleaner, the latter mode being illustrated in Fig. 2.49. The feed enters the matrix in the magnetic zone located at the top of the ring. The non-magnetic particles pass through the matrix and are channeled out of the separator. This fraction represents the rougher tailings. The magnetic particles, collected onto the matrix, are ﬂushed from the matrix outside the magnetic ﬁeld and then introduced, from inside the separating ring, into the second magnetic head, to remove the entrained gangue material. An assembly of Ferrous Wheel separators is shown in Fig. 2.52. Roll-type wet high-intensity magnetic separator A useful wet alternative to dry induced roll high-intensity magnetic separators was developed in the nineteen sixties in the former USSR [D4, K2]. These separators, suitable for treatment of weakly magnetic, relatively coarse materials (up to 10 mm), consist of proﬁled rolls that rotate against proﬁled stationary poles. The poles and the rolls are magnetized by electromagnetic coils wound around the iron yoke. Various proﬁles of the rolls and of the pole pieces, as shown in Fig. 1.46, have been employed, their selection depending upon the required magnetic force and the application. Triangular teeth facing grooved poles with cuts were found to be the most e!cient proﬁle [D4]. Magnetic induction as high as 1.6 T can be achieved in the working zone of the separator. A schematic

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

109

Figure 2.51: Magnetic system of the Ferrous Wheel magnetic separator. Permanent magnets are located on each side of the vertical separating ring (courtesy of Eriez Magnetics, Inc.).

Figure 2.52: Ferrous Wheel separators under construction at Eriez Magnetics (USA) (courtesy of Eriez Magnetics, Inc.).

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

110

Feed

Magnetics Roll

Non-magnetics

Pole-tip

Coil

Iron yoke

Figure 2.53: Schematic diagram of a four-roll wet high-intensity magnetic separator. Table 2.5: Speciﬁcation of wet high-intensity roll magnetic separators. Parameter Throughput [t/h] Roll diameter [mm] Roll length [mm] Number of rolls Magnetic ﬁeld [T] Mass of separator [t] Water consumption [m3 /h] Input power [kW]

5SVK 2 to 6 300 2000 2 1.2 4.7 8 to 10 6

ERM3 5 300 2000 4 1.6 10.9 8 to 10

2MSM5 3 to 6 270 2000 2 1.2 4.9 10 4

diagram of the four-roll separator is shown in Fig. 2.53 while an isometric view of the four-roll separator ERM-3 is shown in Fig. 2.54. A detailed view of the proﬁled roll can be seen in Fig. 2.55. The lower pole tip contains slots through which the non-magnetic fraction leaves the separator. Magnetic particles from the feed are attracted to the teeth of the roll and are discharged when the roll leaves the sphere of inﬂuence of the magnetic ﬁeld. Typical speciﬁcations of various models of wet high-intensity roll magnetic separators are summarized in Table 2.5. A photograph of a 2-MSM-5 separator is shown in Fig. 2.56. These separators were successfully applied to the beneﬁciation of coarse (- 5 mm) manganese ore, iron ores such as siderite and limonite, and to the removal of serpentine from magnezite. While these separators cannot treat e!ciently

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

111

Figure 2.54: A four-roll wet high-intensity roll magnetic separator ERM-3.

Figure 2.55: A detailed view of the proﬁled roll of a wet high-intensity roll magnetic separator.

112

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.56: 2-MSM-5 wet high-intensity roll magnetic separator (courtesy of ˇ B, Czechoslovakia). Z very feebly magnetic and very ﬁne particles, their main advantage, compared to WHIMS, is the ability to treat coarse particles and the absence of the matrix blockage. The range of applicability is similar to that of the rare-earth drum magnetic separators, although the ﬁeld generated by these separators is somewhat higher than that by the drum separators, with similar magnitude of the ﬁeld gradient. Further advantage of wet induced roll separators is that it is possible to control the magnetic ﬁeld strength. They can be e!ciently applied to materials that fall between low-intensity magnetic separation and high-intensity high-gradient separation.

2.4.3

Solenoid-based magnetic separators

All wet high-intensity magnetic separators already discussed have produced the magnetic ﬁeld by means of an electromagnet with iron yoke. For small working volumes and for moderately large magnetic induction, this constitutes an e!cient and relatively cheap design, although the machines tend to be massive. The input power needed to saturate the iron poles is modest and reasonably high magnetic induction, of the order of 1 T, can be generated in the air gaps, which guarantees su!ciently high throughputs (tens of tonnes per hour) of ﬁne weakly magnetic material. However, it follows from the discussion in Section 1.7.3 that this design suers two serious drawbacks: a. The maximum magnetic induction that is obtainable in the working volume is limited by the saturation polarization of iron (approximately 2 T). Since such an induction can be generated only in a narrow gap, much lower inductions

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

113

Figure 2.57: Frantz Ferroﬁlter magnetic separator. are usually created in units designed for practical large-scale applications. b. Scale-up is very di!cult. In order to increase the throughput, the gap between the poles must be increased. This results either in a dramatic drop in the magnetic induction in the working volume, or in a substantial increase in the number of ampere-turns in order to maintain the same magnetic induction. The machine becomes extremely massive in relation to its capacity, magnetic induction becomes increasingly limited by the width of the gap, and the cooling of coils also becomes a problem. To generate su!ciently large magnetic induction at large volumes, it is necessary to use an iron-clad solenoid, as has been analyzed in Section 1.7.3. Frantz Ferroﬁlter The ﬁrst magnetic separator that used the iron-clad solenoid was the so-called Frantz Ferroﬁlter, introduced by S.G. Frantz in 1937 [F1]. This separator, shown in Fig. 2.57, became the conceptual basis of cyclic high-gradient magnetic separators. It consists of an iron-bound solenoid magnet generating a magnetic ﬁeld of about 0.15 T, while the matrix is formed by screens fashioned from thin sharp ribbons of magnetic stainless steel, as shown in Fig. 2.58. The device operates intermittently; the ﬂow is interrupted, the magnetic ﬁeld is reduced to zero and the magnetic particles are backwashed. Then the ﬁeld is switched on again and the entire cycle is repeated. Because of the low demagnetizing factor of the ribbon elements that are

114

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.58: A ribbon matrix used in a Frantz Ferroﬁlter. oriented parallel with the direction of the magnetic ﬁeld, the magnitude of the background magnetic induction was su!cient for the recovery of ﬁne ferromagnetic particles. However, in order to magnetize the randomly oriented ﬁlamentary matrix with very high aspect ratio, a much higher magnetic ﬁeld is needed. As a means of achieving a high degree of retention of quasicolloidal, feebly magnetic impurities from kaolin, Frantz’s concept was extended so that more powerful iron-clad solenoids were used in conjunction with randomly oriented steel wool. The early developments of cyclic high-gradient magnetic separators are described in detail in references [O3, K5, K7, I2, I3]. Modern cyclic high-gradient magnetic separators The ﬁrst industrial high-gradient magnetic separator, which grew from Frantz’s concept and from investigations into the removal of weakly magnetic discolouring agents from clays was built in 1969 [O4]. Figure 2.59 shows schematically the essential elements of operation of such a separator. The system comprises a canister ﬁlled with a matrix formed of compressed mats of magnetic stainless steel wool, although other types of matrices can be used. The canister is placed in an iron-clad solenoid which generates a magnetic induction up to 2 T. The matrix creates a high degree of non-homogeneity of the magnetic ﬁeld and produces a large magnetic force acting on the magnetizable particles. The slurry is fed to the canister either vertically downwards or upwards through the matrix with the magnetic ﬁeld switched on. The magnetic particles from the slurry are trapped into the surface of the magnetized matrix, while the non-magnetic particles pass through the canister. When the matrix has been loaded with the magnetic particles, the ﬂow is halted, the magnetic ﬁeld

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

Figure 2.59: Schematic diagram of operation of a cyclic HGMS.

Figure 2.60: An automated small capacity cyclic Sala-HGMSW P

115

116

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.61: High-gradient magnetic ﬁlter for e"uent control in the steel industry (courtesy of Metso Minerals, Ltd.). is reduced to zero and the magnetic fraction is ﬂushed from the matrix. Such cyclic devices are useful in applications where a slurry to be processed contains a small fraction of magnetic particles. These machines have found a widespread application in the kaolin industry and in waste water treatment. A range of cyclic high-gradient magnetic separators is manufactured by several companies. The solenoid diameter ranges from 1 m to 3 m, input power from 100 to 500 kVA and throughput as high as 200 t/h is claimed. Figure 2.60 shows a small-scale cyclic HGMS while Fig. 2.61 presents a Metso Minerals cyclic HGMS for waste water ﬁltration. A production-scale Eriez Magnetics HGMS for puriﬁcation of kaolin is shown in Fig. 2.62. Dry Allis-Sala HGMS Dry matrix high-gradient magnetic separation was developed by Allis Sala [J7] in order to extend applicability of dry separation to such a ﬁne particle range that cannot be easily beneﬁciated by roll or drum dry separators. Schematic diagram of the separator is shown in Fig. 2.63. The magnetic ﬁeld is generated by an iron-clad water-cooled solenoid and the matrix is placed in the bore of the coil. Particle transport through the matrix is accomplished by a compressed air-driven vacuum pump. The pump sucks the air through the heater into the separation circuit. The air inlet is positioned at the feed point, where the pre-heated air and particles are mixed before entering the matrix. The economic expansion of high-gradient magnetic separation to numerous mineral processing applications requires the utilization of fully continuous mag-

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

117

Figure 2.62: Eriez Magnetics cyclic HGMS for kaolin beneﬁciation (courtesy of Eriez Magnetic, Inc.).

Air heater

Feed

Air

Filter bed with matrix

Solenoid

Vacuum pump

Figure 2.63: Schematic diagram of dry Sala HGMS.

118

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.64: Continuous Sala high-gradient magnetic separator. netic separation. Cyclic devices are limited in their use to separations in which the magnetic fraction is a small portion of the feed and to the feeds that must be passed through the device at controlled slow feedrates. Continuous solenoid high-gradient magnetic separators have eliminated the limitations of the cyclic machines and several advanced devices have been built. Sala-HGMS carousel separator The Sala-HGMS carousel separator was developed from the cyclic separator to meet the need for a continuous industrial machine capable of processing ores containing a high proportion of magnetics [O5, M9, A5]. As can be seen in Fig. 2.64, a double-saddle iron-clad coil surrounds the carousel ring. Seals mounted on the ring allow independent control of feed and ﬂush velocity to enhance the separation and to increase the ﬂushing e!ciency of the magnetics. The operational sequence is similar to that used in conventional continuous iron-core-type high-intensity separators as is evident in Fig. 2.65. Further advantage of such a magnetic separator is that it can be scaled up to treat high volumes of material. Magnetic ﬁeld is parallel to the slurry ﬂow. When increased throughput is required, the width of the magnet is increased, while its height remains constant. The surface area of the matrix can, therefore, be enlarged without increasing the width of the air gap and thus the number of ampere-turns to generate the required magnetic ﬁeld. The iron return frame reduces the magnetic ﬂux leakage to places outside the magnetic head. In high-intensity magnetic separators with iron yokes, the stray

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

119

Figure 2.65: The operational sequence in a continuous Sala HGMS [A5]. magnetic ﬁeld is so high despite a reversal of polarity of two adjacent magnetic heads that the magnetic induction in the ﬂush station area usually amounts to about 20 mT. This is su!ciently high to hamper the e!cient ﬂushing of the matrix. With iron-clad solenoids, the magnetic induction outside the magnet is as low as 2 mT, depending on the matrix used. Sala HGMS are manufactured under the Metso Minerals label in various models. The number of magnetic heads ranges from one to four and magnetic induction varies from 0.5 T to 2 T. Throughput of 200 t/h per magnet head is speciﬁed for the largest model 480 ABCD. The matrix is, typically, a compartmented stack of expanded metal screens. A photograph of a single-head Sala-HGMS unit, with nominal throughput of 15 t/h is shown in Fig. 2.66. The largest model that is presently being oered by Metso Minerals is the HGMS 350 shown in Fig. 2.67. This unit can be ﬁtted with up to three magnetic heads and can reach a throughput up to 300 t/h. VMS magnetic separator A novel concept for replacement of a horizontal rotor or carousel by a vertical wheel was incorporated in the VMS magnetic separator. The VMS magnetic separator, the isometric view of which is shown in Fig. 2.68, was developed in the Ore Research Institute in Prague, in former Czechoslovakia [H9, H10, C7]. A magnetic ﬁeld is generated by the horizontally oriented solenoid wound with a water-cooled hollow conductor. The coil is enclosed in steel cladding, the upper and lower pole-pieces of which are perforated to allow passage of the slurry. The slurry is fed into the separator via a feed box and it then enters

120

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.66: MK III Sala-HGMS carousel unit.

Figure 2.67: A three-head HGMS 350 carousel machine (courtesy of Metso Minerals, Ltd.).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

121

Figure 2.68: An isometric view of VMS. a rotating drum, which carries separation chambers ﬁlled with matrix. The non-magnetic and the middling fractions are collected in launders underneath the magnet. Magnetizable particles are attracted to the matrix, placed in compartments along the periphery of the vertical wheel. When the matrix leaves the region of the magnetic ﬁeld during the rotation of the wheel, the captured particles are ﬂushed from the matrix. The magnetic product is thus washed o from the matrix at the ﬂush station in a direction opposite to that of the feed and is collected in the trough at the bottom of the separator. The maximum background magnetic induction generated by the magnet is 1.7 T, while stray magnetic induction outside the magnet is less than 5 mT. Mild steel rods of 3 mm and 5 mm in diameter, with spacing of between 1.5 mm and 2.5 mm, are used as a matrix. Woven wire mesh has also been used in some applications. In order to increase the capacity of a magnetic separator, the width of the working space must be increased. The VMS concept allows this very simply by increasing the width of the wheel. Taking into account that the magnetic ﬁeld in the VMS separator is oriented vertically, perpendicularly to the increase of the wheel width, the basic characteristics of the magnetic circuit remain unchanged, i.e. the vertical length of the air gap, which determines the magnetomotive force, or the number of ampere-turns needed to achieve the required magnetic induction, is the same for any width of the wheel. Because of the increase in the length of the conductor, energy consumption increases only linearly with the wheel width. A throughput of up to 150 t/h was speciﬁed for the largest separators VMS 100.

122

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.69: A vertical ring of the VMS HGMS, with matrix compartments ˇ B Spišská Nová Ves, Slovakia). (courtesy of Z

Figure 2.70: VMS high-gradient magnetic separator (courtesy of Ore Research Institute, Czech Republic).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

123

Figure 2.71: VMS-100 separators in a manganese ore beneﬁciation plant in the Ukraine (courtesy of Ore Research Institute, Czech Republic).

By replacing the conventional horizontal rotor by a vertically rotating wheel, Fig. 2.69, the VMS separator also addressed the problem of matrix clogging, an onerous problem for most carousel WHIMS or HGMS machines. The reverse ﬂush and very low stray magnetic ﬁeld in the ﬂush section are additional features of this separator. The VMS magnetic separator, shown in Fig. 2.70, was manufactured in sevˇ B Co. in the former Czechoslovakia. These separaeral models and sizes by Z tors were earmarked for incorporation into the Krivoy Rog and Kursk Magnetic Anomaly iron ore beneﬁciation plants in the Ukraine. The proposed capacity of the plants was 30 Mt/a and it was envisaged that at least forty VMS separators, each with capacity of 100 t/h, would be required. At the same time, several units, Fig. 2.71, were installed in manganese ore beneﬁciation plants in the Ukraine. In many demanding applications, particularly when feebly magnetic admixtures from industrial minerals are to be removed, it is necessary to control the residence time of the slurry in the separating zone and thus the ﬂow velocity through the matrix. To cater for such applications, the VMS separator was modiﬁed in such a way that the magnetic system was situated below the rotation axis of the rotor. This VMKS separator, shown in Figure 2.72 and schematically in Figure 2.73, generates a magnetic induction of 2 T and has a rotor diameter of 3 m, width of 1.4 m and throughput of 10 t/h. It was successfully applied to puriﬁcation of kaolin [Z3].

124

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.72: Continuous magnetic separator VMSK for puriﬁcation of kaolin (courtesy of Ore Research Institute, Czech Republic).

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

125

Figure 2.73: Sectional view of the VMKS separator for kaolin puriﬁcation (Ore Research Institute, Czech Republic).

SLON magnetic separator It became obvious in the late eighties, that the use of an iron-clad solenoid and application of the reverse ﬂush of the matrix enhances the e!ciency, scalability and availability of continuous high-gradient magnetic separators. The technical success of VMS separators prompted further innovative eort. The SLON HGMS, developed in 1988 by Ganzhou Non-ferrous Metallurgy Research Institute, Ganzhou, China [X1], and shown in Figure 2.74, is based on the VMKS concept. However, in order to improve the e!ciency of separation even further, the pulsation of the slurry within the matrix was incorporated into the SLON separator. The pulse generator induces vertical pulses in the slurry within the matrix. The particles are thus exposed to the pulsation force, which is much greater than the force of gravity and acts in both directions [Y2]. By the pulsation action, the mechanically entrained non-magnetic particles are removed from the matrix, which results in improvement of the quality of the magnetic concentrate. At the same time, the pulsation allows the magnetic particles in the slurry to be exposed to the entire depth of the matrix, which increases the recovery of the magnetic component. The SLON separators are manufactured in several models, speciﬁcations of three of which are listed in Table 2.6. The separator is used, on a large scale, to beneﬁciate feebly magnetic iron and ilmenite ores and appears to enjoy considerable commercial success in China.

126

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.74: SLON-2000 pulsating high-gradient magnetic separator (courtesy Ganzhou Non-Ferrous Metallurgy Research Institute, China).

Table 2.6: Parameters of SLON magnetic separators. Parameter Ring diameter [mm] Maximum magnetic induction [T] Input power [kW] Pulsating stroke [mm] Feed size [mm] Feed solid density (%) Throughput [t/h] Mass of the machine [t]

SLON-1000 1000 1

SLON-1500 1500 1

SLON-2000 2000 1

26 0 to 30 -1 10 to 45 4 to 7 6

38 0 to 30 -1 10 to 45 20 to 35 20

82 0 to 30 -2 10 to 45 50 to 80 50

2.4. WET HIGH-INTENSITY MAGNETIC SEPARATORS

127

Figure 2.75: SLON-1500 magnetic separators operating in Pang Zhi Hua ilmenite processing plant in China (courtesy of Ganzhou Non-ferrous Metallurgy Research Institute, China). It is set to make inroads into international markets. Figure 2.75 illustrates the operation of a bank of SLON-1500 separators in the Pang Zhi Hua ilmenite processing plant (China). Other innovative designs of solenoid-based magnetic separators Matrix blockage and insu!cient throughput was the main limitation to recovery of uranium and gold from Witwatersrand ores and cyanidation residues by wet high-intensity magnetic separation [C8]. In order to satisfy all the requirements for a cost-eective and reliable machine that would be able to operate for a su!ciently long period in industrial conditions, the Council for Mineral Technology (Mintek), Randburg, South Africa, designed and constructed a prototype separator [S14] shown in Figure 2.76. The design of the Mintek linear magnetic separator was based on a split-coil magnet that consisted of two parallel short race-track coils, internally watercooled, separated by a gap through which the matrix could pass. This pair of coils was enclosed in a steel cladding. The matrix consisted of woven mesh screens held vertically on a ﬂexible belt. The belt moved linearly in a horizontal direction and inverted back on itself by means of pulleys. As the belt moved round the pulleys, the matrix elements ﬂared out, thus facilitating the removal of ferromagnetic material and wood chips. The residual mechanically entrained particles were then removed by a reverse ﬂush on the lower side of the separator.

128

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.76: The Mintek linear high-gradient magnetic separator. Scale-up of the machine could be accomplished by increasing the width of the belt and by the installation of two to four magnetic heads in a single machine along the belt. Although the separator performed well on pilot-plant scale, non-technical issues prevented the industrial application of the machine. An innovative approach to the concept of the VMS separator was employed by Magnetic Technology Consultants (MTC) (South Africa) who designed and built a high-gradient separator (Figure 2.77) designed to treat weakly magnetic materials [A6]. Figure 2.78 illustrates the MTC separator operating in a glass sand plant. The feed material containing 0.08 % Fe2 O3 was upgraded to 0.022% Fe2 O3 in the ﬁrst pass and to 0.011% Fe2 O3 in the second pass. Although the separator was designed primarily for wet applications, it was successfully tested in a dry mode. A vacuum system with vacuum seals was used to propel the pyroxenite ore through the matrix and high velocity of the ore and thus high throughput were achieved.

2.5

Superconducting magnetic separators

Although high-intensity and high-gradient magnetic separators that use resistive magnets meet, in most instances, the technological requirements of the mining and materials industries, their cost-eectiveness is impaired by high energy consumption, the need to cool the windings, limited working volume and considerable mass owing to the massive iron yokes or cladding. These disadvantages can, however, be overcome by using superconducting magnets, which

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

129

Figure 2.77: The MTC continuous HGMS separator (South Africa).

Figure 2.78: MTC HGMS separator at the glass sand plant. The feed into the separator is on the right-hand side while the non-magnetic product in the ﬁrst pass is shown on the left.

130

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

oer a number of advantages: a) Superconducting magnets can produce high magnetic induction in large volumes at low energy consumption. The power is required mainly for cooling rather than to compensate for ohmic losses in the coil of the magnet. Moreover, the cost of cooling is independent of the magnetic ﬁeld generated, unlike resistive magnets where the cost of cooling is proportional to the square of the ﬁeld intensity. The economic e!ciency of the superconducting magnets thus increases with increasing ﬁeld strength. In some applications the increased magnetic ﬁeld allows the ﬂow rate of the slurry to increase and thus the throughput of the separator increases. b) Since iron cladding is generally not needed, the machine can be made physically smaller. c) The superconducting coils can be arranged in such a way that a su!ciently large ﬁeld gradient can be generated without using a matrix, while still maintaining high magnetic force. Two types of magnetic separators that use superconducting coils have been introduced into industrial practice, namely the matrix separators and opengradient magnetic separators (OGMS). The matrix separators fall into two distinct design categories, namely cyclic vertical ﬂow units operating with liquid nitrogen and helium liqueﬁer, and reciprocating HGMS. As a simple extension of the matrix-based high-gradient magnetic separators, the conventional resistive solenoid magnet was replaced by a superconducting coil. These separators operating in the cyclic mode in the switch on/o regime are based on short, large diameter, coils, processing at slow slurry velocities with fairly infrequent ﬂushing. In order to minimize the energy consumption and the running costs of superconducting magnet systems, the magnet should be as passive as possible. The persistent mode option allows the magnet to remain energized with no additional power input. Elimination of the switch on/o regime would also result in a longer duty cycle and thus in higher throughput of the separator. These issues of a passive magnet were addressed by the reciprocating concept [S15, W4, R3]. In this operation, one canister with the matrix processes the slurry while the second canister is cleaned in a region of zero magnetic ﬁeld. This technology, ﬁrst proposed by English China Clays, was not viable until the magnet technology caught up with the operational requirements in the early nineties [R4]. The second type of superconducting magnetic separators, namely OGMS, is based upon deﬂection of magnetizable particles in a non-homogeneous magnetic ﬁeld, according to their magnetic susceptibility and size. Instead of employing a matrix to generate a magnetic ﬁeld gradient, the geometry of the magnet winding is used to create the ﬁeld gradients and magnetic force that deﬂects the magnetizable particles. These open-gradient magnetic separators include a linear multipole separator and a drum magnetic separator.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

131

LHe standpipe Slurry out

Liquifier

LHe Dewar LHe GHe

LHe GHe Slurry in

Superconducting magnet

Figure 2.79: Schematic diagram of a cyclic superconducting HGMS.

2.5.1

Cyclic superconducting HGMS

The cyclic resistive high-gradient magnetic separators were exclusively designed for puriﬁcation of kaolin. A resistive magnet of diameter of 2100 mm (84”) generated the ﬁeld of 1.8 T at a power input of up to 400 kW. Bigger units with a solenoid diameter of 3000 mm and weighing up to 625 tonnes consumed 600 kW. In order to reduce the energy consumption, the Huber Corporation (USA) decided to replace the resistive solenoid by the superconducting coil. A schematic diagram of a cyclic superconducting HGMS is shown in Fig. 2.79. The ﬁrst such unit, designed and built by Eriez Magnetics and shown in Fig. 2.80, was installed at Huber Corp. in May 1986 [S16]. The ﬁlling factor of the steel wool matrix is about 6% and the matrix is 500 mm deep. The clay slurry is pumped from holding tanks into the distributor header; it ﬂows upward through the matrix to the return header. A typical ﬂowrate is between 1 and 2 m3 /min, and typical retention time ranges from 50 to 90 seconds [W5]. After a period of time, the matrix accumulates enough magnetic material so that the e!ciency of separation drops o. At this point the slurry feed is stopped, the magnet is de-energized, and the steel wool is washed in both directions with clean water. The magnet is then re-energized and the feed slurry is re-started. A typical duty cycle is 26 minutes separation, 1 minute of de-energizing, 2 minutes of ﬂushing and rinsing, and 1 minute of re-energizing [W5]. This process means that two dead time periods occur during the ramp up and down of the magnetic ﬁeld, along with a dead time while the ﬂush of the magnetics is carried out. In order to reduce this dead time, fast ramp

132

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.80: A cyclic superconducting Eriez Magnetics HGMS for kaolin beneﬁciation (courtesy of Eriez Magnetics, Inc.). superconducting magnets are used. The coil and power supply are subjected to rapid current cycles in order to apply and remove the magnetic ﬁeld. This results in increased heating of the coil by eddy currents and larger and more expensive cooling power is required. A more robust power supply to drive the current quickly is also required. This results in signiﬁcant cyclic stresses within the magnet itself [R4].

2.5.2

Reciprocating superconducting HGMS

Superconducting magnets can take advantage of a higher magnetic ﬁeld compared to resistive magnets, and can increase the processing velocity. However, as the slurry velocity increases, the duty cycle decreases and the economics of separation is aected. Also, for the optimum operation of a superconducting magnet, taking into account coil stresses, ﬁeld uniformity and power requirements, it is preferable to operate the superconducting HGMS in persistent mode. The issues of long duty cycles of separation and of optimum magnet operation are addressed by a reciprocating technology. In order to achieve economic operation, the captured particles must be ﬂushed from the matrix, with the ﬁeld on, and the capture zone must, therefore, be removed from the magnetic ﬁeld. The train of canisters, as shown in Figure 2.81, is moved by means of a ram that operates on a magnetically balanced canister, which houses a multi-section separation region. As one matrix canister is engaged in separation, the second is undergoing ﬂushing and rinsing. Reciprocation can be accomplished in 10

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

133

REFRIGERATOR

Reciprocating matrix train

Product DUMMY

ACTIVE

DUMMY

ACTIVE

DUMMY Feed

LINEAR ACTUATOR

Iron yoke

Superconducting coil

Figure 2.81: Schematic diagram of a reciprocating canister HGMS.

seconds [S17]. While economic design of resistive solenoids is based on short, large diameter coils, for superconducting coils it is far simpler to provide a coil whose length is greater than the diameter. Such a geometrical arrangement, used in Outokumpu/Carpco separators, allows the use of a radial slurry ﬂow rather than an axial ﬂow. As can be seen in Figure 2.82, the radial ﬂow allows the feed area, and thus the throughput, to be increased. The ﬁrst industrial superconducting magnetic separator was designed by the Institute for Refrigeration Engineering in Prague, Czech Republic [F6, K8]. This 5 T unit, shown in Figure 2.83 was a reciprocating canister machine for the beneﬁciation of kaolin. Although, initially, the performance of the separator was encouraging, subsequent deterioration in e!ciency and drop in throughput as a result of matrix blockage were given as the main reasons for closure of the separator [A7]. It was suspected that insu!cient velocity of ﬂush water and a strong stray magnetic ﬁeld in the ﬂush station were the main sources of the problems. In order for a superconducting magnet to operate, it has to be cooled below its critical temperature. The most common way of cooling such a magnet is to immerse it in a bath of liquid helium at 4.2 K within a vacuum-insulated cryostat. The period between liquid helium additions can be further extended by using thermal insulation and liquid nitrogen. Mechanical coolers, based on the Giord-McMahon refrigeration cycle, can extend the period between helium reﬁlls ever further. In this technique, a small volume of high-purity helium gas recirculates through a closed loop, generating a cooling eect at the point of

134

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.82: Diagram of an active matrix canister in reciprocating superconducting HGMS (Outokumpu Technology, Carpco Division).

Figure 2.83: The Czechoslovak reciprocating-canister superconducting magnetic separation for beneﬁciation of kaolin.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

135

Table 2.7: Cryoﬁlter HGMS models [S18]. Cryoﬁlter Model 5T/200 5T/360 5T/460 5T/1000

Application Pilot Industrial Industrial Industrial

Throughput 400 kg/h up to 15 t/h up to 50 t/h up to 150 t/h

Figure 2.84: Superconducting Cryoﬁlter HGMS (courtesy of Outokumpu Technology, Carpco Division). forced gas expansion. Carpco Cryoﬁlter systems are using this concept of a combination of a liquid helium bath and mechanical cooling, which ensures a reﬁll period of 1 year in normal processing operations [K9]. R ° Further developments in the Oxford Instruments Cryofree technology now allow superconducting magnet systems to be totally cooled by mechanical means, removing the requirement for helium completely [K9, A8]. Outokumpu Technology, Carpco Division, produce a range of the Cryoﬁlter HGMS employed mainly in kaolin puriﬁcation. Figure 2.84 illustrates the Outokumpu/Carpco Cryoﬁlter HGMS, while Table 2.7 lists Cryoﬁlter models. While the Cryoﬁlter supply package depends on the application, the primary items and options include [S18]: • Basic Cryoﬁlter with integral iron sheet, reciprocating canister and standard control package.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

136

Table 2.8: Comparison of resistive and superconducting cyclic magnetic systems for HGMS, with reciprocating superconducting separators [K9]. Magnet type 2100 mm resistive electromagnet 3000 mm resistive electromagnet 2100 mm superconducting magnet 3000 mm superconducting magnet 5T360 Cryoﬁlter 5T/460 Cryoﬁlter 5T/1000 Cryoﬁlter

Magnetic ﬁeld [T] 1.8

Mass [t] 270

Power [kW] 270 to 400

Capacity

1.8

625

300 to 400

2C

2.5

270

25

1.25C

2.5

625

25

2.5C

5 5 5

12 24 120

? 10 ? 10 ?12

0.4C 1.3C 4C

C

• Slurry handling system. • Advanced process control panel and SCADA monitoring system. • Detergent matrix wash system. Table 2.8 compares various types of matrix-based superconducting magnetic separators used for kaolin beneﬁciation [K9].

2.5.3

Open-gradient superconducting magnetic separators

The presence of a ferromagnetic matrix in high-gradient magnetic separators brings about a problem associated with keeping the matrix clean and passable under industrial conditions. One possible approach to eliminate the problems inherent in matrix machines is to employ a system in which magnetic particles are continuously deﬂected in a non-uniform magnetic ﬁeld, according to their magnetic properties and size. These open-gradient magnetic separators, designed for the treatment of ﬁne feebly magnetic materials, must be equipped with superconducting coils in order to provide su!ciently strong magnetic force. The ﬁeld gradients generated by a suitable combination of the conductor ﬁlaments or by coils of varying polarity are much weaker compared to the gradients created by a matrix. Magnetic induction exceeding 2 T is thus required to achieve adequate magnetic force. Figure 2.85 illustrates two dierent modes of operation of an open-gradient magnetic separator.

2.5. SUPERCONDUCTING MAGNETIC SEPARATORS

137

Figure 2.85: Dierent systems of open-gradient magnetic separators: linear multipole system [(a) and (b)] and drum separator (c). Linear multipole OGMS The design of the linear multipole system, as shown in Figure 2.85 (a) and (b), is based on the concept of the ancient Edison’s deﬂection separator [T3]. It consists of an array of vertically positioned coaxial superconducting coils that are energized in opposite directions [S19]. In its simplest form, Figure 2.85(a), the dry ore is permitted to fall vertically as a curtain around the circumference of the magnet. The magnetic force directed radially inwards diverts the magnetic particles inwards while the non-magnetic particles fall vertically, unaected by the magnetic force. The method failed to meet expectations mainly because the separation was taking place away from the region of the highest magnetic force. As a result of low depth of the magnetic ﬁeld, its gradient and interparticle collisions, the metallurgical results were unsatisfactory even at low feedrates. An improvement was achieved by bringing the feed point close to the magnet and introducing a ramp, as is shown in Figure 2.85(b). The performance of the system was su!ciently encouraging for Cryogenic Consultants Ltd. (CCL) to design and build a production-scale Cryofos OGMS unit for beneﬁciation of the pyroxenite ore in South Africa [G3]. In order to circumvent scale-up problems of magnets of cylindrical geometry used up to that time for OGMS, Good [G3] abandoned the cylindrical geometry in favour of a linear geometry. The split pair was replaced by a linear dipole of rectangular cross section, each side having a separation length of 3 m. The separator could be utilized along almost its entire length on both sides of its axis. Unfortunately, the magnet and the cryogenic system proved to be di!cult to manufacture and the separator never reached operational status [S1].

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

138

Figure 2.86: Superconducting drum magnetic separator Descos (Humboldt Wedag AG). Further development at CCL and at Carpco Inc. addressed the issues of the optimized feeding close to the region of the strongest magnetic force and of the removal of the magnetic particles from the walls of the separator. The concept of a ﬂat-faced magnet inclined at an angle with respect to the feeder R ° evolved into the Cryostream series of OGMS units marketed by Outokumpu Technology, Carpco Division [K9, S17]. In spite of considerable design progress, the concept of Cryostream has not yet enjoyed commercial success. Descos OGMS The drum magnetic separator developed by KHD Humboldt Wedag AG employed a multipole magnet and combined the advantages of a superconducting magnet with those of a conventional drum separator. As can be seen in Fig. 2.86, eight poles of the magnet system were arranged along one third of the circumference of the drum. Four race-track coils were placed in a liquid helium tank and generated 3.2 T on the surface. The drum of the separator was made of carbon-ﬁbre reinforced plastic. The diameter of the drum was 1200 mm and its length 1500 mm. Commercialization of the product proved to be di!cult as a result of its high cost, in spite of its reportedly satisfactory metallurgical performance.

2.6

Laboratory magnetic separators

A rule that applies to magnetic separation as much as to most physical separation techniques, is that the quickest and surest way of ﬁnding out how a material

2.6. LABORATORY MAGNETIC SEPARATORS

139

will behave in a separator is to run it through the machine. Theoretical models of the process, which would help to predict the e!ciency of low-intensity magnetic separation are scarce and mostly too simpliﬁed to be of practical value. A wealth of theoretical descriptions of high-intensity and high-gradient magnetic separation applies mainly to idealized situations, with limited signiﬁcance for practical problems. The information obtained from these models can sometimes even be misleading and this, combined with the fact that magnetic and some physical and chemical properties of the ores and other materials are di!cult to ascertain, indicates that laboratory tests should be carried out before conclusions can be drawn about the e!ciency of material treatment by magnetic means. A wide spectrum of laboratory devices and bench-scale magnetic separators have been built to simulate a particular process in a particular production-scale machine. Generally, the usefulness of these small-scale machines is limited. For instance, in magnetic separators based on permanent magnets, such as magnetic pulleys, overband magnets and drum magnetic separators, the magnetic ﬁeld generated is a function of the volume of the permanent magnets used in the manufacture of the separator. A small-scale separator will thus generate a lower magnetic ﬁeld, often of dierent pattern, compared to a production-scale machine. Moreover, physical dimensions of the separators, such as the diameter of a pulley or a drum, determine the residence time of material in the magnetic ﬁeld and thus the e!ciency of separation. Also, a small width of a magnetic roll or a drum introduces signiﬁcant end eects into the results. In laboratory-scale tests of high-gradient magnetic separation, it is essential to keep the matrix depth and ﬂow velocity of the slurry through the matrix the same as in the industrial conditions. Quite often it is not possible. Overall, tests on laboratory-scale units can thus be misleading and practical experience in evaluating the results of small-scale tests, on small, not necessarily representative samples, is essential. Commercially available laboratory-scale magnetic separators, such as Davis Tube and Frantz isodynamic separator can, however, be used for a reliable analysis of the separability of materials.

2.6.1

Davis Tube

A Davis Tube (DT), shown in Figure 2.87, is a laboratory instrument designed to separate small samples of strongly magnetic ores into strongly magnetic and weakly magnetic fractions. It has become a standard laboratory equipment used for the assessment of the separability of magnetic ores by low-intensity magnetic separators [S20, S1]. It was developed in 1921 and no signiﬁcant changes have been made in its design since then. The separator consists of an inclined tube 25 mm in diameter, placed between pole-tips of an electromagnet. Material to be separated is passed through the tube; the strongly magnetic fraction is held by the magnetic ﬁeld while the weakly magnetic material is washed down the tube.

140

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.87: Davis Tube magnetic separator.

Figure 2.88: The 3D model of the Davis Tube electromagnet [M24, M10].

2.6. LABORATORY MAGNETIC SEPARATORS

141

Figure 2.89: Frantz isodynamic separator.

Schultz [S20] suggested that a magnetic induction of 0.4 T or greater between the magnet poles should be used. However, Steinert and Boehm [S21] claimed that the current practice was to conduct the Davis Tube tests at a magnetic induction equal to that on the surface of the drum of the magnetic separator. Since it is the magnetic force or the force index, and not the magnetic ﬁeld strength, that are decisive in the operation, it is unlikely that this practice would yield correct information. Computer modelling of the pattern of the magnetic force generated by drum magnetic separators and a Davis Tube (shown in Fig. 2.88) was carried out by Murariu and Svoboda [M10]. It was found that in the case of conventional ferrite drum separators, with a standard gap of 25 mm between the drum and the tank, Davis Tube tests should be conducted at the magnetic induction of 0.1 T. On the other hand, correct assessment of performance of a rare-earth drum can be obtained by operating a Davis Tube at about 0.3 T or higher, depending on the design of the magnetic systems of the drum.

2.6.2

Frantz isodynamic separator

The Frantz isodynamic separator is a magnetic device that allows fractionation of materials based on their magnetic properties. This separator, shown in Fig. 2.89 consists of an electromagnet having two long pole pieces with a long narrow air gap between them. The pole design is such that the magnetic ﬁeld proﬁle is isodynamic, so that the magnetic force density across the width of the air gap

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

142 A

Fm Fg

ș

Magnetic fraction

mg

B

Non-magnetic fraction

Splitter

Figure 2.90: Forces acting on a particle in a Frantz isodynamic separator. is constant, i.e. EuE = frqvw=

(2.1)

Material to be separated enters the magnetic ﬁeld at point A, as is illustrated in Fig. 2.90. If the force of gravity Ij and the magnetic force Ip on a particle are balanced in such a way that the particle moves along the central line of the air gap, this particle has a 50 % chance of reporting to a magnetic or non-magnetic fraction. The balance of forces can be expressed as: ps j sin =

Ys EuE 0

(2.2)

where ps and Ys are the mass and the volume of the particle, respectively, j is the gravitational constant and is the transverse slope of the air gap. By re-arrangement we obtain: j " = 0 sin (2.3) EuE It can be seen that, because of the isodynamic pattern of the ﬁeld, the action of the separator on a particle is determined solely by its mass magnetic susceptibility, and is independent of the size and the mass of the particle. The magnitude of the term EuE is determined by the electric current L in the electromagnet so that sin (2.4) "= nL q where q and n are constants [M11]. With an electric current of 1.8 A, the magnetic induction at the narrowest part of the gap is approximately 2 T. In order

2.6. LABORATORY MAGNETIC SEPARATORS

143

Table 2.9: Chemical compounds used for calibration of magnetic susceptibility instruments. Compound Mohr’s salt Nickel sulphate Copper sulphate Cobalt sulphate Ferrous sulphate Manganese chloride Manganese pyrophosphate

Formula Fe(NH4 )2 (SO4 )2 ·6H2 O NiSO4 ·7H2 O CuSO4 ·5H2 O CoSO4 ·7H2 O FeSO4 ·7H2 O MnCl2 Mn2 P2 O7

" [107 ·m3 /kg] 4.1 2.0 0.74 4.6 5.2 15.4 12.9

to determine the exact values of these constants, each Frantz separator must be calibrated with compounds having well deﬁned values of magnetic susceptibilities. Chemical compounds usually used for calibration are listed in Table 2.9, together with their mass magnetic susceptibilities. Mass magnetic susceptibility " can thus be obtained from eqs. (2.3) or (2.4) by plotting the cumulative per cent recovery of the material into the magnetic fraction, versus the current. Typical magnetic proﬁles, or partition curves, are shown in Fig. 2.91. The mean magnetic susceptibility of a sample can be deﬁned as the value of " for which 50 % of the sample reports into the magnetic fraction. While the sample represented by curve 1 in Fig. 2.91 has a narrow distribution of magnetic susceptibility, the sample described by curve 2 contains a wider spectrum of the values of magnetic susceptibility. The Frantz magnetic barrier separator While the Frantz isodynamic magnetic separator employs the isodynamic pattern of the magnetic force density, expressed by eq. (2.1), the operation of the barrier separator is based on the presence of the anadynamic and katadynamic force patterns [F7]. In the katadynamic region, the magnetic force increases with the increasing ﬁeld strength, while in the anadynamic region the force decreases with the increasing magnetic ﬁeld: g g EuE A 0 (katadynamic), EuE ? 0 (anadynamic) gE gE

(2.5)

As can be seen in Fig. 2.92, the magnetic force density between the pole tips of the separator is bell-shaped and creates a barrier in the isodynamic plane, between the katadynamic and anadynamic regions [J2]. Depending upon whether paramagnetic or diamagnetic susceptibility is to be exploited, a mixture of particles is fed into the anadynamic or katadynamic region. As the mixture moves under gravity towards the isodynamic plane, the magnetic force slows the particles of the susceptibility to be exploited and accelerates the particles having susceptibility of the opposite sign. In the vicinity of the barrier, where

144

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.91: Magnetic proﬁles, or magnetic partition curves, of two types of materials, as obtained by Frantz isodynamic separator.

Figure 2.92: Superimposed graphs of the magnetic induction and magnetic force density in the barrier separator, showing katadynamic (k) and anadynamic (a) regions.

2.6. LABORATORY MAGNETIC SEPARATORS

145

Figure 2.93: Rotating disk isodynamic magnetic separator. the magnetic force has the maximum value, particles having susceptibility such that the magnetic force equals or exceeds the opposing force of gravity, are deﬂected in the direction parallel to the isodynamic plane. Particles having susceptibilities lower, or of the opposite sign, pass through the barrier. The barrier separator thus allows selective separation and fractionation of materials based on small dierences in magnetic susceptibility [R5]. Disk isodynamic magnetic separator Frantz isodynamic separator is a selective device that allows separation of mixtures based on dierences in magnetic properties. This is in contrast to most other magnetic separators (such as roll, drum and matrix separators) which use the katadynamic ﬁeld pattern and are thus non-selective from ﬁrst principles. In these machines the separation is based on dierences in magnetic properties as well as on particle size. Frantz separator is a laboratory unit that does not lend itself to scale-up. In order to overcome limitations of the Frantz separator and, at the same time to retain its high selectivity, Gerhold et al. [G29, G30, G31] designed and built a rotating disk isodynamic magnetic separator shown in Fig. 2.93. The separator consists of a horizontally rotating disk and magnetic system with pole-pieces that generate an isodynamic magnetic ﬁeld in the separation gap. The magnetic force created by the magnetic system acts radially inwards while the competing force is the centrifugal force. This force can be adjusted to the values ranging from ﬁve to ten times the force of gravity.

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

146

Pole

Pole

Tails

Tails

Pole

Feed

Pole Feed

Mags

Mags

Tails

Tails Rotating disc

Tails collector

Rotating disc

Tails collector

Figure 2.94: Schematic diagrams of operation of a dry rotating disk isodynamic separator, with two dierent proﬁles of the magnetic ﬁeld (adapted from Gerhold [G30]). Particles fed onto the disk assume the rotational velocity of the disk. The weakly magnetic particles are deﬂected outwards and are collected in a nonmagnetic bin. More strongly magnetic particles are deﬂected inwards in a form of a rotating ring and are removed before they each the feed region. The operation of the separator, with two dierent proﬁles of the magnetic ﬁeld, is shown schematically in Fig. 2.94. A pilot-scale separator with a throughput of 2 t/h, maximum magnetic induction of 2 T and ﬁeld gradient of 10 T/m, was built [G29] and selective separation of ferrimagnetic and strongly paramagnetic materials in the size ranging from 3 mm to 50 m was obtained [G30].

2.6.3

Separators with a rotating magnetic ﬁeld

Particle separation in rotating or alternating magnetic ﬁelds was proposed in the early years of development of magnetic separation technology [T3, D1]. It appears that this idea has not made its mark on the mineral processing industry. However, in many magnetic separators, the particle rotation is present as a sideeect rather then a deliberate attempt to rotate the particles. For instance, magnetic clusters in low-intensity magnetic separators are rotated slowly as they are carried past successive magnetic poles of opposing polarity. In doing so, the ﬂocs release mechanically or magnetically entrained ”non-magnetic” particles, improving thus the grade of the magnetic concentrate. In some applications it is possible to use particle rotation alone to achieve separations not possible using conventional attraction-based magnetic separation, as has been shown by Allen [A9, A10, A11]. For instance, particles

2.7. EDDY-CURRENT SEPARATORS

147

Particle rotation

S

N

S Magnet travel

Figure 2.95: Generation of particle rotation. having similar magnetic susceptibilities, but considerably dierent magnetic anisotropies, can be separated from each other by their selective rotation. As a result of magnetic anisotropy the external magnetic ﬁeld exerts a torque on the particle in order to align its axis of easy magnetization with the direction of the external ﬁeld. If the magnetic ﬁeld generated, for example, by permanent magnets with alternating polarity, is moving, then the particles will rotate as is shown in Fig. 2.95. The concept of a rotating magnetic ﬁeld has been employed in rotating magnetic ﬁeld (RMF) laboratory separators developed and manufactured by Ka (Pty.) Ltd., Australia. Figure 2.96 shows an RMF lift separator that can be employed for separation by rotating weakly ferromagnetic or even paramagnetic particles with magnetic anisotropy. Figure 2.97 illustrates an RMF separator for separation of paramagnetic minerals. In these separators, the rotating magnetic ﬁeld is generated by a rotating magnet rotor ﬁtted with magnetic poles of alternating polarity around its circumference. The rotor in Fig. 2.96, rotating in a clockwise direction, produces a ﬁeld that appears (to a particle on the outer drum surface) to be rotating in an anticlockwise direction. Therefore, a magnetically anisotropic particle dropped onto the drum will respond by rotating in an anticlockwise direction. Non-rotating particles will be carried by the drum and its belt in a clockwise direction. RMF rotation separation is basically a separation of ferromagnetic (s.l.) particles from paramagnetic particles because of a large dierence in magnetic anisotropies and thus rotabilities of these two classes of materials.

2.7

Eddy-current separators

Although the ﬁrst patent for an eddy-current separator (ECS) was granted to T.A. Edison as early as 1889, a large-scale application of eddy-current separation started only recently, particularly in connection with the recycling of wastes

148

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.96: RMF lift separator (courtesy of Ka (Pty.), Ltd.).

Figure 2.97: RMF separator for separation of paramagnetic particles (courtesy of Ka (Pty.), Ltd.).

2.7. EDDY-CURRENT SEPARATORS

149

Figure 2.98: Eddy-current separator (courtesy of Steinert GmbH).

containing non-ferrous metals. The ﬁrst industrial ECSs were based on an electromagnetic ﬁeld induced either by single coils or by linear motor technique. As a result of the dramatic development of rare-earth magnets, the currently manufactured ECSs employ exclusively permanent magnets. Figure 2.98 illustrates such an eddy-current separator. The eddy-current technique is based on the fact that if conductive particles are exposed to an alternating magnetic ﬁeld, or move through a steady magnetic ﬁeld, eddy currents are generated within the particles. These eddy currents are generated in such a way that the magnetic ﬁeld they produce opposes the external magnetic ﬁeld, according to Lenz’s law. The opposite ﬁeld then produces a repulsive force (Lorentz force) on the particle. Particles are thus deﬂected from the stream of material, as is shown in Fig. 2.99, depending on their conductivity, size, shape, and the ﬁeld strength and the rate of change of the ﬁeld. The industrial eddy-current separators consist of two drums carrying a belt, the belt usually being driven by the rear steel drum. The front non-metallic drum contains a rapidly rotating magnetic system. The permanent magnets are arranged, with alternating polarity, along the circumference of the magnetic system. The separators usually have 6 to 18 poles which rotate at frequencies up to 3000 rpm. Depending on pole arrangement and the system speed, the frequencies of magnetic ﬁeld change up to 1 kHz are achieved [N3, H11]. Two main designs of eddy-current separators, each with two dierent magnet conﬁgurations, are illustrated in Fig. 2.100, while Table 2.10 reviews the designs used by various manufacturers. Type 2 design, which employs an eccentric magnetic system, is reported to have several advantages [N3, H11]. In concentric systems, strongly magnetic particles tend to accumulate between the belt and the magnetic drum and ulti-

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

150

Figure 2.99: Material separation in eddy-current separator (courtesy of Steinert GmbH).

Type 1

Type 2

Configuration A

N

S

Configuration B

N

S N S

S

N

N S

Figure 2.100: Two designs of drum eddy-current separators (after [N3]).

2.7. EDDY-CURRENT SEPARATORS

151

Table 2.10: Manufacturers of eddy-current separators [N3]. Manufacturer Steinert (D) Lindemann (D) Eriez Magnetics (USA) Huron Valley (USA) Andrin (F) Bakker Magnetics (NL) Raoul Lenoir (F) Newell Industries (USA) Rutherford Light Metals

Type 2 1+2 1 1 1 1 1 1 1

Conﬁguration A A A A or B A A A A B

mately to damage the drum. In eccentric design, the ferromagnetic material is removed automatically from the region of the magnetic ﬁeld generated by the rotating drum. The repulsive force acting by eddy currents on a small particle [S22, Z4] is proportional to: s g 2 (2.6) Iuhs ps E s i where ps and g are the mass and diameter of the particle, respectively, E is the magnetic induction and i the frequency of its change, and s and s are the electrical conductivity and density, respectively, of the particle. It can be seen that the e!ciency of separation is determined, amongst other factors, by the ratio of material conductivity and density. The larger the dierence in the values of this ratio for the materials to be separated, the more selective the separation will be. Table 2.11 lists this ratio for materials of interest in eddycurrent separation. It is evident that aluminium and magnesium can be rather e!ciently separated from semi- and non-conductors, while lead and stainless steel will not respond to eddy currents. Selection of dierent models of eddy-current separators is usually dictated by particle size distribution of the feed material and the required throughput. The width of the belt ranges from 500 mm to 2000 mm and nominal throughput is of the order of 10 m3 /h/m. Magnetic induction on the surface of the shell ranges from 0.25 T to 0.38 T. Particles in the size range - 100 + 5 mm are usually treated in standard ECSs. Separation of ﬁne particles Although separation of particles smaller than 5 mm poses a problem [Z5, R6], several innovative designs have successfully reduced the minimum particle size to 0.1 mm. The Steinert model 6119 [H11] and Raoul Lenoir model Eddybox, are claimed to be able to separate e!ciently particles as small as 1 mm. The Eddybox separator is based on free-fall of metallic particles through a magnetic structure, has no moving parts and is claimed to achieve a throughput as high as 1 t/h.

152

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Table 2.11: The material parameter for eddy-current separation [N3, S22]. Material Aluminium Magnesium Copper Silver Zinc and Zamac Gold Brass Tin Lead Stainless steel Glass Plastics

@ [103 ×s×kg1 ×m2 ] 13.0 12.2 6.3 6.0 2.4 2.1 1.3 to 1.8 1.2 0.45 0.18 0 0

Figure 2.101: Eddy-current separator Fourmi for separation of ﬁne particles (Raoul Lenoir).

2.8. SEPARATORS WITH MAGNETIC FLUIDS

153

Figure 2.102: Schematic diagram of an eddy-current separator based on rotation of ﬁne particles (courtesy of N. Allen). R ° The design of Fourmi eddy-current separator (Raoul Lenoir), shown in Fig. 2.101, is based on a horizontally rotating polar disc with radially mounted NdFeB permanent magnets. An alternating magnetic ﬁeld generates eddy currents in metallic particles that are fed on a stationary separation disc placed above the polar disk. The conductive particles, being acted upon by repulsive forces, become ﬂuidized and are removed by air jets. Particles as small as 0.1 mm are claimed to be e!ciently separated. It will be shown in Section 3.9.3 that with decreasing particle size the torque on a particle becomes an important force. Particles in ECS then respond to the ﬁeld changes by rotation rather than by repulsion. Allen [A21, A22] proposed the use of particle rotation as the separating mechanism of ﬁne metal particles. A schematic diagram of such an ECS based on particle rotation is shown in Fig. 2.102.

2.8 2.8.1

Separators with magnetic ﬂuids Basic concept

Separation in magnetic ﬂuids is a sink-and-ﬂoat technique, which exploits dierences in the densities of materials to be separated. In this technique, a magnetic ﬂuid, placed in a non-homogeneous magnetic ﬁeld, exhibits an apparent density dierent from its natural density [R7, R8]. This density can be controlled through a wide range of values, exceeding densities of all known elements and materials. While the scope of the conventional sink-and-ﬂoat technique is re-

154

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

stricted by a limited range of densities of the separation medium, the upper limit of ferrosilicon medium being approximately 3500 kg/m3 , and that of Clerici solution about 4200 kg/m3 at room temperature, magnetic ﬂuids allow densities as high as 20 000 kg/m3 or even higher to be achieved. The apparent density d of a magnetic ﬂuid placed in a non-homogeneous magnetic ﬁeld can be written (in SI units) as: d = 0 +

i EuE 0 j

(2.7)

where 0 is the physical (true) density and i is the volume magnetic susceptibility of the ﬂuid. The apparent density of a magnetic ﬂuid is thus dependent on the magnetic properties of the ﬂuid, and the magnetic ﬁeld strength and its gradient. A magnetic ﬂuid, placed in a non-homogeneous magnetic ﬁeld, is attracted to the regions of the highest magnetic ﬁeld. This magnetic force produces an opposite force within the ﬂuid that tends to expel an immersed non-magnetic body. This results in additional, magnetically generated, levitation, which causes particles to ﬂoat. In the early days, solutions of paramagnetic salts (such as MnCl2 ) were used as a magnetic ﬂuid [A12, A1]. As a result of their low magnetic susceptibility (of the order of 6×107 m3 /kg) very high magnetic ﬁelds and high gradient were required to achieve densities greater than those obtained using heavy liquids. For instance, in order to achieve an apparent density of the paramagnetic liquid equal to 3500 kg/m3 , the second term on the right-hand side of eq. (2.7) must be equal to 5×104 T2 /m. For a magnetic induction of 2 T, a gradient as high as 2.5×104 T/m is required. These are unrealistically high values, particularly for meaningful production-scale applications of this technique. In the late sixties of the last century methods of preparation of stable suspensions of nano-sized magnetite particles in hydrocarbon carrier ﬂuids were developed [P5, R10]. These ferromagnetic ﬂuids (ferroﬂuids) are considerably more magnetic than the paramagnetic liquid and become magnetically saturated at moderate magnetic ﬁelds. Equation (2.7) can then be re-written as: d = 0 +

Pi uE j

(2.8)

where Pi is the magnetization of the ﬂuid (in [A/m]). If magnetic polarization Mi , (in [T]) is used, then eq. (2.8) is expressed in the form d = 0 +

Mi uE 0 j

(2.9)

In fjv units eq. (2.8) can be re-written as d = 0 + where Pi and E are given in [G].

Pi uE 4j

(2.10)

2.8. SEPARATORS WITH MAGNETIC FLUIDS

155

FEED

MAGNET

PRODUCTS:

N

S

FLOAT SINK

MAGNETIC FLUID

Figure 2.103: Schematic diagram of a separator with magnetic ﬂuids.

Figure 2.104: Laboratory ferrohydrostatic separator FGS-40 (courtesy of GMUO, the Ukraine).

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

156

Table 2.12: FHS separators manufactured by GMUO [G4]. Model FGS-1A FGS-70 FGS-40 FGS-40/3 FGS-200

Feed size [mm] - 50 + 0.2 - 25 + 2.5 - 10 + 0.2 - 5 + 0.2 - 100 + 10

Throughput [kg/h] 60 200 5 2 4000

Density range [kg/m3 ] 1200 - 11 000 6500 - 10 000 4000 - 9000 2500 - 3500 3000 - 6000

It can be seen from eqs. (2.8) to (2.10) that in order to achieve a constant apparent density of separation, in a magnetically saturated ferroﬂuid, the gradient of the magnetic ﬁeld must be constant. This is achieved by suitably shaping the pole tips of the magnetic system. A ferrohydrostatic separator (FHS), which uses a ferroﬂuid as a working medium, thus produces two fractions, namely a ﬂoat and a sinks products. Figure 2.103 illustrates the concept of a separator with magnetic ﬂuids. The e!ciency of ferrohydrostatic separation decreases with decreasing size of particles. In order to overcome this ine!cient separation of ﬁne particles in gravity-based FHS, a rotation-based separation Magstream process was developed [W7].

2.8.2

Ferrohydrostatic separators

AVCO Corporation and NASA (USA) pioneered the FHS technique in 1973 by employing a kerosene-based ferroﬂuid to separate automobile scrap [M12]. Considerable eort to develop this technology was subsequently expended in Japan and the USA. Hitachi [N4], Nittetsu Mining Co. [S51], Tohoku University [S50] and US Bureau of Mines [R9] further conﬁrmed the unique features of the FHS technology. Numerous pilot-plant-scale separators were designed and built, with throughputs up to 500 kg/h. Although extensive tests conﬁrmed viability of this technique, particularly when applied to the recovery of non-ferrous metals from automobile scrap, production-scale application did not take place in the Western World at that time [F8]. Comprehensive review of the history of FHS in Japan and the USA was given by Fujita [F8]. Ferrohydrostatic separation was also researched and used, in approximately the same time period, on a production scale in the former Soviet Union. The Gipromashugleobogashcheniye Institute (GMUO) in Lugansk, the Ukraine, developed a comprehensive range of models of ferrohydrostatic separators for different applications and throughputs. These separators were used in such diverse applications as densimetric analysis of coal, recovery of gold from gravity concentrates, diamond concentration and separation of non-ferrous scrap. Table 2.12 summarizes various models of FHS units manufactured by GMUO [G4]. Figure 2.104 illustrates the versatile FGS-40 separator suitable for laboratoryscale separation of various minerals in the density range from 4000 kg/m3 to

2.8. SEPARATORS WITH MAGNETIC FLUIDS

157

Figure 2.105: Production-scale ferrohydrostatic separator FGS-70 for separation of non-ferrous metals (courtesy of GMUO, the Ukraine).

158

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.106: Ferrohydrostatic separator Shlikh-1 with permanent magnets for recovery of alluvial gold (Too Geos Co.). 9000 kg/m3 . The FHS unit designed to separate non-ferrous metals in the density range between 6500 kg/m3 and 10 000 kg/m3 , with particle size up to 25 mm, is shown in Figure 2.105. As a result of geopolitical changes in the nineties of the last century, most markets for GMUO ferrohydrostatic separators in the former Soviet Union disappeared and the separators have not been innovated to meet the current standard of technology. Ferrohydrostatic separators based on permanent magnets are produced by Too Geos Co. (Russia). These small-scale low-throughput machines have been designed for the recovery of alluvial gold from gravity concentrates. Throughput of the Shlikh-2 model is approximately 50 kg/h, while a laboratory model Shlikh1, shown in Fig. 2.106 can treat about 10 kg/h. All models of the Shlikh FHS separator are supplied together with a vibrating screen and disk and roll magnetic separators, as shown in Fig. 2.107. These units allow the classiﬁcation of the material and the removal of strongly and medium magnetic materials from the feed into the FHS unit. Since FHS is a unique technique for material manipulation in areas such as diamond-processing industry, De Beers Consolidated Mines (Pty.) Ltd. (South Africa) developed a range of selective FHS separators. These fully automated computer-controlled, hands-o units are capable of treating particles in the size

2.8. SEPARATORS WITH MAGNETIC FLUIDS

159

Figure 2.107: Shlikh-1 system comprising a vibrating screen, disk and roll magnetic separators and a ferrohydrostatic separator (Too Geos Co.). range - 25 + 0.3 mm and can distinguish a density dierence of at least 20 kg/m3 (0.02 g/cm3 ). Units with a throughput exceeding 1 t/h, depending on the feed density and size, have been built [S23]. Figure 2.108 shows a twostage automated and secure ferrohydrostatic separator built by De Beers for R ° the recovery of diamonds. The ferrohydrostatic separator Rhomag , shown in Figure 2.109, is used for separating ﬁne fractions of exploration samples.

2.8.3

Magstream separator

The main limitation of ferrohydrostatic separation, in which the important competing force is the force of gravity, is ine!cient separation of ﬁne particles. Efforts were made by Revnetsev [R11] and Andres et al. [A14] to replace the force of gravity by the centrifugal force. This proposal resulted in a rotation-based separation process Magstream [W7] developed by Intermagnetics General Corp. The essential features of the Magstream separation process are shown in Fig. 2.110. Particles to be separated are combined with a ferroﬂuid and passed downward through a long, vertically oriented annular duct where they rotate with the ﬂow guide and duct about the duct axis. The duct is surrounded by a multipole magnet that produces a non-homogeneous magnetic ﬁeld. A radially inward displacement force, which results from the radially outward attraction of the magnetic ﬂuid, is felt by all particles. This force is opposed (or aided) by a radially outward (or inward) magnetic force acting on paramagnetic (or diamagnetic) particles, and by the centrifugal force. At a given speed of rotation, the inward displacement forces are greater on light particles, which then move radially inwards. Heavier particles experiencing

160

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

Figure 2.108: An automated hands-o two-stage ferrohydrostatic separator (courtesy of De Beers Consolidated Mines (Pty.) Ltd.).

R ° Figure 2.109: Ferrohydrostatic separator Rhomag for separation of ﬁne particles (courtesy of De Beers Consolidated Mines (Pty.) Ltd.).

2.8. SEPARATORS WITH MAGNETIC FLUIDS

Flowguide

Feed

Magnetic fluid

Magnet

Splitter

Light fraction

Heavy fraction

Figure 2.110: Schematic diagram of the Magstream separator.

Figure 2.111: Magstream 200 separator.

161

162

CHAPTER 2. REVIEW OF MAGNETIC SEPARATORS

higher centrifugal and magnetic forces, at the same speed of rotation, overcome displacement forces to move radially outwards. The separation density is then given by: Pi E d = 0 + frqvw 2 (2.11) $ where $ is the angular velocity. It can be seen that the additional degree of freedom, namely the speed of rotation, can be used to control the separating force acting on the particles. The Magstream separators were available in several models, ranging from laboratory-scale portable units for batch separation of samples up to 300 g, to large continuous separators with a throughput up to 250 kg/h. Figure 2.111 shows the 200 Magstream model. Magstream separators can separate particles over a range of densities from 1300 kg/m3 to beyond 21 000 kg/m3 . The accuracy of separation is claimed to be 100 kg/m3 (0.1 g/cm3 ). For the most e!cient separation, the sample should be sized between 60 m and 1 mm. Separation of samples up to 4 mm is possible with special accessories.

Chapter 3

Theory of Processes of Magnetic Separation of Materials In view of the diversity of magnetic separation techniques the theoretical descriptions of the magnetic separation process are of limited general applicability. So many factors may aect the behaviour of a system of particles that many problems appear at ﬁrst sight to be of bewildering complexity. In general, the particle motion in a non-homogeneous magnetic ﬁeld is so involved as to prevent reasonable theoretical approach. On the other hand, however, a particular problem can often be simpliﬁed considerably and a realistic appraisal of the equations describing the motion of the particles is possible. As has been mentioned in Chapter 1, a particle in a magnetic separator is acted upon by a wide array of forces of various magnitudes and ranges. The necessary (but not su!cient) condition for successful separation of more strongly magnetic particles from less strongly magnetic particles is expressed by eq. (1.1). In real situations, however, such a condition is di!cult to evaluate. The general expression for the magnetic force (eq. (1.8)) acquires speciﬁc forms in dierent types of magnetic separators, depending on the pattern of the magnetic ﬁeld and its gradient. Also, the importance of various competing forces acting on particles in a magnetic separator depends on the type of magnetic separator, on the properties of the particles, such as size, shape, magnetic properties, density, and on the type of ﬂuid in which the particles to be separated are suspended. Workable models of material separation must, therefore, be developed separately for individual types of magnetic separators. The situation is complicated by the fact that many branches of magnetic separation, such as separation by suspended magnets, magnetic pulleys or wet low-intensity drum magnetic separators still constitute highly empirical technology. Hesitant steps have been taken to develop theoretical models of dry separation in roll and drum magnetic separators. On the other hand, open-gradient magnetic separation, magnetic 163

164

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

ﬂocculation of weakly magnetic particles and wet high-gradient magnetic separation have received considerable theoretical attention. A notable number of papers dealing with the problem of particle capture in HGMS led to an understanding of the interaction between a particle and a matrix element. However, completely general treatment of the magnetostatic and hydrodynamic behaviour of an assembly of the ore particles in a system of matrix elements, in the presence of a strong magnetic ﬁeld, is a theoretical problem of considerable complexity. A brief survey of the current theoretical descriptions of separation of materials in various types of magnetic separation equipment will be given in the following sections.

3.1

The forces and the equations of particle motion

The equations of particle motion are relations between accelerations, velocities and coordinates of the particles. They are second-order dierential equations for the function u(w)> where u is the radius vector and w is the time. Their integration makes possible, in principle, the determination of this function and so of the path of the particles. The equation of particle motion in a magnetic separator can be written in a vector form as psds = l Il (3.1) where psds is the inertial force, ps is the mass of the particle and ds its acceleration. Il are all the forces that may be present in a magnetic separator, such as the magnetic force, force of gravity, hydrodynamic drag, centrifugal force, the friction force, surface forces, magnetic dipolar forces and electrostatic forces among the particles and others. In order to be able to solve eq. (3.1), it is necessary to evaluate the components of all its terms in suitable coordinates. To obtain the components of the inertial force in polar coordinates that are convenient for most types of magnetic separators, let us consider two mutually perpendicular unit vectors uˆ and ˆ= We shall assume that these vectors have directions of increasing u and and their directions change with time. Since the derivative of a unit vector is perpendicular to the vector, the time rates of uˆ and ˆ can be expressed as [G1] gˆ u g ˆ = gw gw

(3.2)

g gˆ = uˆ gw gw

(3.3)

Now, the position of the particle, in polar coordinates, is given by u = uˆ u. Dierentiating this equation and using eqs. (3.2) and (3.3), the components of

3.1. THE FORCES AND THE EQUATIONS OF PARTICLE MOTION 165 the particle velocity y are found to be yu =

gu gw

(3.4)

g (3.5) gw The subscripts u and indicate the radial and azimuthal components, respectively. By further dierentiation, the components of the particle acceleration ds are obtained and hence the components of the inertial force are [G1] " µ ¶2 # g g2 u (3.6) u ps dsu = s Ys gw2 gw · 2 ¸ gu g g ps ds = s Ys u 2 + 2 (3.7) gw gw gw In Cartesian coordinates these equations can be written as y = u

ps ds{ = s Ys

g2 { gw2

(3.8)

ps ds| = s Ys

g2 | gw2

(3.9)

Complete equations of motion are obtained by combining eq. (3.1) with eqs. (3.6) and (3.7) or (3.8) and (3.9). While it is fairly straightforward to express components of most of the competing forces, such as the force of gravity and the hydrodynamic drag, the magnetic force is more complicated. The general form of the components of the magnetic force, in polar coordinates are given by: Iu =

s CEu CEu Ys (Eu + E ) 0 Cu Cu

(3.10)

s 1 CEu CE Ys (Eu + E ) (3.11) 0 u C C In the Cartesian system the components of the magnetic force can be expressed as: s CE{ CE| Ys (E{ I{ = + E| ) (3.12) 0 C{ C{ s CE{ CE| Ys (E{ + E| ) (3.13) I| = 0 C| C| where s is the volume magnetic susceptibility. It can be seen that in order to use the above equations, we must be able to specify the components of the magnetic induction and its gradient. Each type of a magnetic separator generates its speciﬁc pattern of the magnetic ﬁeld and the problem of particle motion has to be solved separately for each type of a magnetic separator. I =

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

166

Permanent magnets

ș

R

r

ș0

Rotating drum

Figure 3.1: Arrangement of magnetic poles in a drum magnetic separator.

3.2

Particle motion in drum and roll separators

Drum and roll magnetic separators are characterized by periodic arrays of magnetic poles. Laurila [L2] made a fundamental investigation of the periodic magnetic ﬁeld of the cylindrical array of magnets with radial and axial poles used in drum and roll separators. The general expressions for the components of the magnetic force derived in [L2] can then be simpliﬁed in speciﬁc geometrical arrangements of the magnetic poles. Hopstock [H12] derived, based on mathematical and empirical analysis, approximate expressions for the radial and azimuthal components of the magnetic ﬁeld around a magnetic drum with axial arrangement of the magnetic poles, as shown in Fig. 3.1. Magnetic force in a drum separator The approximate expressions for the radial and azimuthal components of the magnetic induction, derived by Hopstock [H12] are : · ¸ (u U) Eu = E0 cos( ) exp (3.14) 0 0 U · ¸ (u U) E = E0 sin( ) exp (3.15) 0 0 U These equations were found to give a good ﬁt to experimental data in a number of dierent magnet conﬁgurations [H12]. The magnetic induction around a drum, shown in Fig. 3.1, is then given by: · ¸ (u U) (3.16) E = E0 exp 0 U

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

167

y

Ff

Fc Fgt

Fgr

ș

Fm

Fg

Figure 3.2: Forces acting on a particle placed on a magnetic drum or roll. where E0 is the magnetic induction on the surface of the drum. It can be seen that in this approximation E is independent of angle . The approximation is most accurate when the following condition is met uU =

0 U

(3.17)

The term on the right-hand side of eq. (3.16) expresses the depth of the ﬁeld, deﬁned as a distance from the surface at which the ﬁeld is reduced to 1/h of its surface value. Equations (3.14) and (3.15) allow calculation of the magnetic ﬁeld gradient and thus the magnitude of the magnetic force. As a ﬁrst approximation, Hopstock found that the radial component of the magnetic force, acting on a magnetite particle in a drum magnetic separator is given by Ipu =

3Ys E02 0 0 U

(3.18)

Under Hopstock’s approximations, the azimuthal component of the magnetic force is equal to zero, which is incorrect. In a more rigorous treatment by Birss et al. [B9], accurate expressions for the components of the magnetic ﬁeld and force were derived in the form of a Fourier series. Whether or not a particle is held on the drum and carried to the magnetic fraction depends on the relative magnitudes of the magnetic force and the gravitational and centrifugal forces. The forces acting on a particle situated on the surface of a drum or a roll are shown in Fig. 3.2. For a given angle of rotation

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

168

r Ȝ

z

R Magnets

Figure 3.3: Arrangement of magnetic poles in a roll magnetic separator. , the radial force acting of a particle can be expressed as: Iu =

s gEu Ys Eu + Ys s j cos Ys s $ 2s U 0 gu

(3.19)

where $ s is the angular velocity of the particle on a roll or drum of radius U. For a speciﬁc case of a high-speed drum, when the force of gravity can be neglected, the centrifugal force equals the magnetic force acting on a magnetite particle when the drum is rotating at the critical angular velocity (in rad/s) given by [H12]: · ¸[email protected] 3E02 (3.20) $f = 0 s 0 U2 Expressions for the components of the magnetic induction for a roll magnetic separator, shown in Fig 3.3, can be written, in cylindrical coordinates, in a more rigorous form [M14]: · ¸ 2 2 Eu = E0 sin( }) exp (u U) (3.21) · ¸ 2 2 E} = E0 cos( }) exp (u U) (3.22) where E0 is the magnetic induction on the surface of the roll, U is the radius of the roll and is the periodicity of the magnetic system. The above equations can be re-written in a more general form as [M14]: Eu = E0 sin(n1 }) exp [n2 (u U)]

(3.23)

E} = E0 cos(n1 }) exp [n2 (u U)]

(3.24)

where n1 and n2 are constants that describe the pattern of the magnetic ﬁeld as a function of u and }. These constants can be determined, for instance, from the electromagnetic modelling of a speciﬁc roll separator.

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

169

Figure 3.4: The forces acting on a particle in a drum magnetic separator (adapted from [C9] and [S24]). Magnetic force acting on a spherical particle of radius e and volume magnetic susceptibility s , on the magnetic roll or drum, can then be written as: Ip = 0 s E02

3.2.1

e2 {exp [2n2 (u e U)] exp [2n2 (u + e U)]} 3

(3.25)

Motion of a particle on the drum or roll surface

The motion of a particle of radius e> situated on the surface of a drum separator of radius U, can be divided into three phases [C9], as shown in Fig. 3.4. In the ﬁrst phase, the particle is accelerating under the inﬂuence of the force of friction Ii and the tangential component of the force of gravity Ijw , given by the following equation: Ii = g (Ip + Iju If )

(3.26)

Ijw = jYs s sin

(3.27)

where g is the coe!cient of dynamic friction and the angle is deﬁned in Fig. 3.2. The end condition of phase 1 was deﬁned by Cakir et al. [C9] as the point when the particle reaches rotor speed $ u , i.e. $ s = $ u . Once the particle acquires the speed of the drum, a static friction coe!cient v , replaces the dynamic friction coe!cient in eq. (3.26). The particle then moves with the constant angular velocity equal to the speed of the drum. When the tangential component Ijw of the force of gravity (Fig. 3.2) becomes greater than the force of friction Ii , or when the particle leaves the drum, the motion of the particle enters the third phase. At the end of the second phase Ii = v (Ip + Iju If ) = Ijw

(3.28)

170

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

In the third phase the particle begins to accelerate as it slips on the drum surface. The radial component of the force of gravity decreases in this region until the centrifugal force exceeds the radial force and the particle leaves the drum: If = Ys s $ 2u (U + e) = Ip + Iju (3.29) Equations of motion of a particle on a magnetic drum in these three phases were developed by Murariu [M14]. The equation of particle motion in the ﬁrst phase can be written · ¸ j Ip j g2 g 2 = + sin + cos ( ) (3.30) g gw2 U+e U+e gw s Ys (U + e) In the second phase the equation of motion is: g g2 = 0 and thus = $u gw2 gw In phase three the equation of motion becomes: · ¸ j Ip j g2 g 2 = sin v cos ( ) + gw2 U+e U+e gw s Ys (U + e)

(3.31)

(3.32)

with initial conditions: = 01

(3.33)

g (3.34) = $u gw where 01 is the angle of the slip point at the end of phase 2. At a certain value of the angle , denoted by 02 , the particle leaves the drum. At that moment [M14]: g s Ys (U + e)( )2 = s Ys j cos + Ip (3.35) gw It should be mentioned that in the case of the roll, the ﬁrst phase is absent since a particle is deposited on the roll at the speed of the roll.

3.2.2

Motion of the particle after it leaves the roll

When the particle leaves the roll or the drum, it is being acted upon by the force of gravity and by the magnetic force. Schematic diagram of this situation is shown in Fig. 3.5. The equations of motion, in Cartesian coordinates, are [M14]: g2 { { Ip (3.36) = 2 2 g w s Ys ({ + | 2 )[email protected] Ip | g2 | = j gw2 s Ys ({2 + | 2 )[email protected]

(3.37)

3.2. PARTICLE MOTION IN DRUM AND ROLL SEPARATORS

171

y v0 =Ȧ0 (R+b)

Fmx ș

ș02

Fmy Fm

Fg x

Figure 3.5: Forces acting on a particle when it has left the drum. where the magnetic force is given by: ¤ ¾ £ ½ 2 2 [email protected] e2 exp 2n £ 2 (({ 2+ | )2 [email protected]) e U ¤ Ip = 0 s E02 exp 2n2 (({ + | ) ) + e U 3

(3.38)

Dierential equations (3.36) and (3.37) obey the following initial conditions {(w = 0) = (U + e) sin 02

(3.39)

|(w = 0) = (U + e) cos 02 g{ (w = 0) = $ 0 (U + e) cos 02 gw g| (w = 0) = $ 0 (U + e) sin 02 gw In equations (3.39) the term $ 0 (U + e) represents the initial velocity of the particle at the moment when it leaves the drum, while $ 0 is the angular velocity of the particle at that moment. By solving the equations of motion (3.36) and (3.37), trajectories of particles can be obtained as a function of their magnetic susceptibility, size, density and of the coe!cient of friction, magnetic ﬁeld strength on the surface of the roll, the spatial distribution of the magnetic ﬁeld and the angular velocity of the roll. An example of a family of particle trajectories is shown in Fig. 3.6.

172

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.6: Particle trajectories in a roll magnetic separator. Roll diameter: 76 mm, speed of rotation: 200 rpm, particle size: 2 mm and particle mass magnetic susceptibilities (from right to left): 2.5×107 > 2.5×106 and 5×106 m3 /kg.

3.3

Separation of particles by a suspended magnet

Suspended (or overband) magnetic separators have been used over many decades to improve material purity and to protect processing machinery by removing unwanted iron and steel objects from conveyed bulk material. Although the design procedures of such magnetic systems, that use either electromagnets or permanent magnets are well established, the understanding of fundamental principles for extraction of metal is inadequate and standards for selecting suitable separators are inconsistent and often incorrect. The common practice [A15, H13] is to base the evaluation of a magnetic separator on the so-called ”force index”, which is essentially the magnetic force density acting on a ferromagnetic body to be removed from a stream of material. Such an approach requires that, for the extraction to occur, the product of the magnetic induction and its gradient assumes a certain minimum value Although such a concept is valid for certain special shapes of bodies, it does not, in general, describe correctly the behaviour of ferromagnetic particles in a magnetic ﬁeld and can lead to erroneous design of a magnetic circuit.

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

3.3.1

173

Magnetic force in a suspended magnet

A starting point in the evaluation of the e!ciency of a suspended magnet is the requirement that the magnetic force Ip acting on a particle must be greater than the sum of the competing forces, e.g. the force of gravity Ij , the drag of the environment Ig , the force of friction Ii and others. The magnetic force on a ferromagnetic particle can be conveniently written as I

p

0 = (P · u)E

(3.40)

where P is the eective magnetic dipole moment of the particle and E0 is the external magnetic induction. When both the particle and the external medium are homogeneous and isotropic, and the body has an ellipsoidal shape, the eective dipole moment is [L3] s p 0 P = Ys K (3.41) p + Q (s p ) where K0 is the external magnetic ﬁeld strength, s and p are the relative magnetic permeabilities of the particle and the external medium, respectively, Q is the demagnetization factor appropriate for the axis of the ellipsoid along which K0 is directed. Using eqs. (3.40) and (3.41) we get for the magnetic force [S25]: Ip = Ys

s p 0 0 · u)E (K p + Q (s p )

(3.42)

For a ferromagnetic body in a non-magnetic or weakly magnetic medium we = have s AA 1 and p = 1, so that eq. (3.42) becomes: Ip = Ys

s 1 0 0 · u)E ¤ (E £ 0 1 + Q (s 1)

(3.43)

The relative magnetic permeability s of the particle is the function of the magnetic ﬁeld inside the particle, s = s (K), where [L3] = K

0 0 p K E ¤ £ = p + Q (s p ) 0 1 + Q (s 1)

(3.44)

for p = 1= Q is the demagnetization factor appropriate for the axis of the easiest magnetization (i.e. the axis of the smallest Q ), as the particle is assumed to be oriented so that its axis is parallel to the external ﬁeld K0 = The expression (3.43) for the magnetic force is a product of two factors: the ﬁrst factor reﬂects the physical properties of particles to be removed, while the second factor, the magnetic force density 02 ) ip = u(E

(3.45)

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

174

Table 3.1: Static force indices (FI) and their ratios for selected shapes [S25] (l length, d-diameter). Object Rod

Sphere Plate 13×50×50 13×200×200 25×200×200

[email protected] 1.0 4.0 10.0

Force index [106 T2 m1 ] 29 889 9 515 4 037 31 811

Ratio FI/FIurg 7.4 2.4 1.0 7.9

20 300 11 130 15 300

5.0 2.8 3.8

describes the properties of the magnetic system. It is this magnetic force density that many designers call ”force index” and use to evaluate magnetic separators. Let us assume that a particle to be extracted by a suspended magnet rests on a stationary conveyor and that no burden of bulk material is present. In equilibrium Ip = Ij , where Ij = Ys (s p )j

(3.46)

and p is the density of the medium. Assuming that s AA p , and combining eqs. (3.43), (3.45) and (3.46) Svoboda obtained [S25]: ¤ £ 1 + Q (s 1) ip = s (3.47) 0j s 1 Equation (3.47) determines the minimum force density (or force index) required to lift a stationary ferromagnetic body of relative magnetic permeability s , density s and demagnetization factor Q , from its position on a belt, in the absence of a burden of bulk material. It can be seen that this minimum magnetic force density is independent of particle size and depends solely on its shape (through the demagnetization factor), its magnetic properties (through the relative magnetic permeability) and its density. Equation (3.47) also shows that the ratio of force indices for various shapes is in the ratio of their demagnetization factors (provided that Q (s 1) AA 1, which is satisﬁed for all shapes but very long rods or thin plates, for which Q ?? 1). Table 3.1 gives several examples of ratios of force index The minimum static force index (or magnetic force density) as a function of the demagnetization factor, for a given material characterized by s and s , in the absence of the burden has, therefore, general validity for any size of the object to be lifted. Figure 3.7 shows such a dependence for steel (s = 7800 kg/m3 , s = 1000). It can be seen that, for instance, for a steel sphere (Q = 0.33) I L = 0.03 T2 /m (80.8×103 G2 @inch).

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

175

Figure 3.7: Magnetic force density (or force index), for steel, as a function of demagnetization factor (adapted from [S25]). For majority of objects that are encountered in practice, the assumption that the external magnetic ﬁeld is directed along the axis of easy magnetization of the body is invalid. Objects such as plates, rods or bolts usually rest on a conveyor belt with their axes of easy magnetization perpendicular to the direction of the external magnetic ﬁeld. Demagnetization factors appropriate for such orientations are high and large force densities (or force indices) are required to lift the body towards the magnet.

3.3.2

Torque on a magnetizable body

Under the above mentioned circumstances, the role of the magnet should be ﬁrst to re-orient the ferromagnetic body in such way that its long axis (the axis of easy magnetization) is parallel with the direction of the external magnetic ﬁeld. This is accomplished by exerting a torque on the body by the externally applied magnetic ﬁeld. The magnetic torque is given [L3, L4] by: 0 W = P × E

(3.48)

s > where Ps is the magnetization of the particle, eq. (3.48) Since P = Ys P can be rewritten: 0 s ×E (3.49) W = Ys P Assuming a body of spheroidal shape, the torque is perpendicular to the plane passing through the axis of symmetry of the body and the direction of

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

176

Axis of symmetry

Į B

b t

a

Figure 3.8: A ferromagnetic bar in a transverse external magnetic ﬁeld. E0 . The magnitude of the torque is given [L5] (by analogy with the torque on a dielectric spheroid in an electric ﬁeld)[S25]: W =

(s p )2 | 1 3Q | K0 E0 Ys sin 2 ¤£ ¤ 2 (p + Q (s p ) s + p Q (s p ) £

(3.50)

and for p =1 W =

( 1)2 | 1 3Q | E02 Ys sin 2 ¤£ ¤ £ s 20 1 + Q (s 1) 1 + s Q (s 1)

(3.51)

Here is the angle between the direction of E0 and the axis of symmetry of the spheroid. It can be seen that the maximum torque occurs at = 450 . The torque is directed in such a way that it tends to turn the axis of symmetry of a prolate (i.e. Q ? 0.33) or oblate (Q A 0.33) spheroid parallel or perpendicular to E0 , respectively. Therefore, the torque tends to align the axis of easy magnetization of the body along E0 . In equilibrium, the magnetic torque is balanced by the torque exerted by the weight of the particle Js and by the weight of the burden Je . We can thus write for a particle having a shape of a bar: 1 k (3.52) jd(s + e )Ys 2 w where d and w and dimensions of the bar, as shown in Fig. 3.8, k is the height of the burden of the material and e is its bulk density. Combining eqs. (3.51) and (3.52) we obtain, in equilibrium, [S25]: W =

E02 sin 2 = dj(s +

k ) w e 0

(

s + 1 1 + Q )( Q) s 1 s 1 | 1 3Q |

(3.53)

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

177

Figure 3.9: Minimum values of the magnetic induction, required to orient steel rods of selected sizes, as a function of the depth of the burden (adapted from Svoboda [S25]). For s AA 1 we then have: k Q (1 Q ) E02 sin 2 = dj0 (s + e ) w | 1 3Q |

(3.54)

It can be seen that if the magnetic system generates the ﬁeld that is perpendicular to the plane of the rod, the rod will not orient itself since = 900 and thus W = 0. It also transpires from eq. (3.48) that the gradient of the magnetic ﬁeld does not contribute, in the ﬁrst approximation, to the torque. Therefore, only the magnitude of the ﬁeld determines whether the reorientation of the body takes place or not. It is clear that in contrast to the conventional description of separation by a suspended magnet, which requires that the magnetic system is designed in such a way that the force index EuE achieves a certain minimum value, the physical picture based on the magnetic torque approach requires a minimum value of the magnetic ﬁeld only. The physical content of such a description can have important implications for the design of the magnetic system. It follows from the previous analysis that in a suspended magnet the important parameter is the magnetic ﬁeld strength. If the ﬁeld strength is high enough so that it can orientate the body along the axis of easy magnetization, the magnitude of the force index is required to be high enough to lift the particle in the direction of its axis of easy magnetization, only. Therefore, the force index is not the only parameter needed to evaluate a suspended magnet. For instance, the force index EuE may be just large enough to lift an

178

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.10: Minimum values of the magnetic induction needed to orient steel plates of selected sizes, as a function of the depth of the burden (adapted from Svoboda [S25]). object in the direction of its axis of easy magnetization, but the magnitude of the magnetic ﬁeld itself may still be too low for the condition of eq. (3.53) to be met. The object then will not re-orientate itself appropriately and will not be lifted. When designing the magnetic system of a suspended magnet two conditions thus must be met: the magnitude and the direction of the magnetic ﬁeld must satisfy eq. (3.54) and, at the same time, the force index must fulﬁll condition given by eq. (3.47). Typical dependence of the minimum magnetic ﬁeld on the depth of the burden, for selected sizes of steel rods and plates, is shown in Figs. 3.9 and 3.10. Similar diagrams can be constructed for other shapes and sizes using eq. (3.53), provided the demagnetization factors are known. A comparison between theoretical values of the minimum magnetic induction Emin required to orient a body along its axis of easy magnetization, calculated using eq. (3.53), and experimental values is given in Table 3.2. It can be seen that the agreement is satisfactory.

3.3.3

Demagnetization factors

Calculation of the demagnetization factor for objects of shapes dierent from that of an ellipsoid is complex and the values found in literature, e.g. for ellipsoids and inﬁnite cylinders, are often of limited practical use. Brown [B3] gives tables for circular cylinders of ﬁnite length, magnetized longitudinally, and for

3.3. SEPARATION OF PARTICLES BY A SUSPENDED MAGNET

179

Table 3.2: Comparison of theoretical and experimental values of the minimum magnetic induction required to orient steel objects, as a function of the depth of the burden [S25]. Object Rod 3×30 mm Plate 0.1×22×43 mm

Bmin [T] Burden depth [mm] Exp. 0 0.0124 10 0.016 0 0.0033 10 0.0131

Theor. 0.0113 0.0132 0.0034 0.0114

Table 3.3: Demagnetization factors of ferromagnetic objects [S25]. Cylinders and plates are magnetized longitudinally(l - length, d - diameter). Object Sphere Finite cylinder

Plate

Size ([email protected]) 0 0.4 1.0 4.0 10.0 40.0 100.0 1000.0 13×50×50 mm 13×200×200 25×200×200

N 0.33 1.0 0.528 0.3116 0.098 0.041 0.011 0.004 0.0004 0.19 0.06 0.11

rectangular rods magnetized transversely. These geometries, together with an ellipsoid, should be su!cient for analysis since other shapes usually encountered in the separation practice (plates, hexagons) can be, in the ﬁrst approximation, converted into geometries for which the demagnetization factors are available. Values of demagnetization factors for selected shapes and sizes are given in Table 3.3.

3.3.4

The eect of the burden

It transpires from the above analysis that a ferromagnetic object to be lifted by the suspended magnet must be ﬁrst re-orientated by the action of the magnetic ﬁeld, in such a way that its long axis (i.e. the axis of easy magnetization) is parallel with the direction of the magnetic ﬁeld. Once this is achieved, the magnetic force is needed to overcome the weight of the object. The object will then be lifted provided the force index acting on a particle is greater than the minimum force index given by eq. (3.47).

180

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.11: The static force index as a function of the depth of the burden, for various sizes of a ferromagnetic sphere (s = 1000> s = 7800 kg/m3 , e = 800 kg/m3 ) (adapted from [S25]). In practice, however, a ferromagnetic particle is usually buried in a layer of loosely packed material, e.g. coal. With the body at rest, the minimum magnetic force required to move the object is determined by its weight and by the force of pressure on the upper hemisphere of the body: Is = e Yej

(3.55)

where Ye is the volume of the burden above the body. In equilibrium Ip = Ij + Is

(3.56)

From eq. (3.56), taking into account that s AA e > a modiﬁed version of eq. (3.47) can be written [S25]: ¤ £ 1 + Q (s 1) Ye ip = 0 (3.57) (s + e )j s 1 Ys It can be seen from eq. (3.57) that the static magnetic force density (or force index in the presence of the burden depends not only on the shape of the object, but also, in contrast to the situation when the burden is absent (eq. (3.47)), on the size of the object. A typical dependence of the static force index on the depth of the burden, for various sizes of a ferromagnetic sphere, is shown in Fig. 3.11.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

181

Similar diagrams can be constructed, using eq. (3.57), for other shapes. It can be seen that the static force index increases steeply with increasing depth of the burden for small particles, while for larger objects the dependence is mild.

3.4

High-gradient magnetic separation

During the last three decades, high-gradient magnetic separation (HGMS) has attracted considerable attention, both experimentally and theoretically. It has established itself as a powerful technique for the manipulation of ﬁne weakly magnetic particles. HGMS has also become a beloved subject of theoretical modelling and a notable number of publications dealing with the problem of particle capture led to an understanding of the interaction between a magnetizable particle and a matrix element. The problem of particle capture in a matrix of a high-gradient magnetic separator can be looked upon from both the macroscopic and microscopic points of view. The macroscopic studies are aimed at the phenomenological description of the separation process and the prediction of its dynamic behaviour. The microscopic theories are intended to provide insight into the mechanisms of particle capture by the matrix. The complex problems facing the microscopic theories were considerably simpliﬁed by considering, in the ﬁrst instance, the interaction between a single particle and a single matrix element. The theory of multi-particle and multi-collector magnetic separation was then developed as a direct extension of the single element model. Validity of such an approach has been questioned and theoretical analysis and experimental data conﬁrm only limited applicability of such an extension to real-life multi-element scenario. A detailed description of the theoretical models of high-gradient magnetic separation is given in a book by Gerber and Birss [G1] and other publications [B10, S1]. A brief survey of the theory of HGMS is given in the following section.

3.4.1

Theory of particle capture by a single-collector

The main emphasis in the early models of high-gradient magnetic separation was on the analysis of particle trajectories in the vicinity of a single magnetized matrix collector, usually a wire [W8, W9, L6, C10]. These studies were inspired by the early analysis by Zabel [Z6] who studied the mechanisms of dielectrophoretic capture on ﬁber matrix. Watson [W8] considered a ferromagnetic wire of radius d placed along the } -axis in a diamagnetic ﬂuid, as shown in Fig. 3.12. A uniform magnetic ﬁeld K0 , strong enough to saturate the wire, is applied in the { direction. Spherical paramagnetic particles of radius e are carried by a ﬂuid of viscosity that ﬂows with uniform velocity y0 in the negative {-direction. This orientation is one of the three possible arrangements between the directions of the magnetic ﬁeld and particle ﬂow velocity with respect to the ferromagnetic wire. It is always assumed that the wire is orthogonal to the external magnetic ﬁeld; the ﬂuid ﬂow can be either parallel (longitudinal - L-

182

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Y H0

v0 b

a

X

Z

Figure 3.12: A ferromagnetic wire and a paramagnetic particle in a magnetic ﬁeld.

Figure 3.13: Graphic representation of three geometrical conﬁgurations in HGMS and of the proﬁles of the particle build-up on the ferromagnetic wire.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

183

b y

H0

g

r

v0

ș ȕ Ȗ x

a

Figure 3.14: The conﬁguration of particle capture in a single-wire approximation. orientation) or perpendicular (transverse - T - orientation) to the direction of magnetic ﬁeld. The third conﬁguration, when the initial ﬂuid ﬂow is parallel to the wire, is known as the axial (A) conﬁguration. These three geometrical conﬁgurations are illustrated in Fig. 3.13. In order to describe the motion of a small paramagnetic particle travelling in a ﬂuid stream in the presence of a magnetized wire, one assumes that the particle experiences magnetic, hydrodynamic and gravitational forces. The balance of forces which describes the particle motion is given by eq. (3.1), or in a more explicit form by eq. (3.58): Il = Ip + Ig + Ij

(3.58)

where Il is the inertial force. The general conﬁguration of the particle motion problem in a single-wire approximation is shown in Fig. 3.14. In order to obtain the magnetic force acting on a small paramagnetic particle in the vicinity of a magnetized wire, the magnetic ﬁeld, external to and generated by the magnetized wire must be expressed as a function of the wire radius. The components of the magnetic ﬁeld outside the wire, in polar coordinates, as deﬁned in Figure 3.14, can be written [G1, S1] as: Ku = K0 (1 + N

d2 ) cos u2

K = K0 (1 N

d2 ) sin u2

(3.59) (3.60)

184

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where N=

P 2K0

(3.61)

For K0 ? Kv N = 1 while for K0 A Kv N = Pv @2K0 . Kv and Pv are the saturation magnetic ﬁeld strength and saturation magnetization of the wire material, respectively. The magnetic force By inserting eqs. (3.59) and (3.60) into eq. (1.8), components of the magnetic traction force on a magnetizable particle are obtained: Ipu =

0 Ys Pv d2 Pv d2 ( 2 + K0 cos 2) u3 u

(3.62)

0 d2 Ys Pv K0 sin 2 u3

(3.63)

Ip =

Ip} = 0

(3.64)

If the net volume magnetic susceptibility = s i is positive, then the radial component of the magnetic traction force between the particle and the wire is attractive provided that Pv d2 + K0 cos 2 A 0 u2

(3.65)

The component Ipu becomes repulsive for s A i in two symmetrical regions, the boundaries of which are determined by a critical angle f [B10] d2 u2 ) f = arctan( d2 1N 2 u 1+N

(3.66)

As shown in Fig. 3.15, the angle f determines sections of the wire surface that are attractive or repulsive to paramagnetic or diamagnetic particles. It is apparent from eq. (3.65) that paramagnetic particles will be collected at angles smaller than f and repelled at angles greater than f = On the other hand, diamagnetic particles, with negative susceptibilities, will be attracted to the wire collector at angles A f and repelled in regions where ? f = The situation is summarized in Fig. 3.16, which shows the contours of the magnetic force around a magnetized cylindrical wire. The hyperbolae indicate the lines of zero radial force. It can be seen from eq. (3.66) that the angle f decreases with increasing magnetic ﬁeld strength. Therefore, the area on the matrix collector, available for the capture of paramagnetic particles decreases with increasing ﬁeld strength.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

185

Figure 3.15: Attractive and repulsive regions around a wire collector (rd = [email protected])=

Figure 3.16: Pattern of the magnetic force around a magnetized cylindrical wire.

186

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The ﬂuid ﬂow distribution and the viscous drag The hydrodynamic drag acting on a particle travelling in a ﬂuid stream is evaluated by calculating the ﬂow ﬁeld around a circular cylinder. The simplest approach to this di!cult problem is to assume that the ﬂuid is inviscid and incompressible. Then the ﬂuid velocity can be written as the gradient of the velocity potential and by solving Laplace’s equation it is possible to obtain the ﬂuid velocity in polar coordinates [G1]: d2 ) cos( ) (3.67) u2 d2 (3.68) y = y0 (1 + 2 ) sin( ) u The potential ﬂow gives good description of the ﬂow conditions on the front side of wire for high Reynolds number, i.e. for Re A 1, where Re is given by 2y0 i d Re = (3.69) yu = y0 (1

For high Reynolds numbers the inertial forces exceed the viscous forces everywhere in the ﬂow ﬁeld except within a thin boundary layer at the wire surface and at the rear side of the wire. For low Reynolds numbers, Re?1, the inertial forces are smaller than the viscous forces and the ﬂow has a viscous (or creeping or laminar) character. The velocity distribution can then be obtained by Lamb’s method [B11, G1]: h u d i ln( ) 0=5 1 ( )2 d u yu = y0 cos( ) (3.70) 2=002 ln Re i h u d ln( ) + 0=5 1 ( )2 u sin( ) (3.71) y = y0 d 2=002 ln Re As has been mentioned above, ﬂow velocity at the wire surface becomes zero in the viscous ﬂow model, while in the potential ﬂow model it can reach values up to 2y0 . These dierences between the two models are particularly noticeable in the collection process. It was shown by Cummings et al. [C11] that particles in viscous (laminar) ﬂow begin to move away from the wire much further upstream than those in potential ﬂow. Because the viscous ﬂow ﬁeld ”sees” the wire much further upstream, particle transport to the region of the highest magnetic force is greatly diminished. Viscous drag force is obtained from Stokes’s equation (eq. (1.16)) and the components of this drag force can be written: gu ) (3.72) gw g Ig = 6e(y u ) (3.73) gw The components of the ﬂuid velocity yu and y are given by eqs. (3.67) and (3.68) or eqs. (3.70) and (3.71), depending on the value of the Reynolds number. Igu = 6e(yu

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

187

The gravitational force The gravitational force is given by eq. (1.14) and its components, in polar coordinates, can be written [G1, G5]: Iju = (s i )jYs cos( )

(3.74)

Ij = (s i )jYs sin( )

(3.75)

Equations of particle motion The dynamic behaviour of the particle in a single-wire approximation of highgradient magnetic separation is described by eq. (3.58). The complete equations of motion in polar coordinates were obtained by a number of authors, for instance [W8, G1, G5, C11, L6, L7]. If the analysis is limited to the motion of small particles (e.g. 2e ? 75 m), for which the gravitational force is much smaller than the hydrodynamic force, and the condition 2s e2 ?? 1 9

(3.76)

is satisﬁed, the inertial and gravitational terms in eq. (3.58) can be neglected. The radial and azimuthal components of the equation of motion can be written [B10] as : yp N cos 2 gud y0 1 ) (3.77) = (1 2 ) cos( ) ( 5+ gw d ud d ud ud3 ud

yp sin 2 yd 1 g = (1 + 2 ) sin( ) gw d ud dud3

where ud = [email protected] and yp =

20 (s i )P K0 e2 9d

(3.78)

(3.79)

is the parameter introduced by Watson [W8]. It has the dimension of [m/s] and is termed magnetic velocity. When = 0, eqs. (3.77) and (3.78) describe the motion of a particle in the longitudinal conﬁguration, while when = @2 they describe the motion in transverse conﬁguration. By combining eqs. (3.77) and (3.78) the timeindependent equation is obtained [W8]: 1 gud = ud g

yp N cos 2 1 ) cos( ) ( + ) ud2 y0 ud5 ud3 1 yp sin 2 (1 + 2 ) sin( ) + ud y0 ud3

(1

(3.80)

Particle trajectories can thus be described by an equation of a general form yp P 1 gud > ud > ) = i( > ud g y0 2K0

(3.81)

188

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The path taken by the particle depends, therefore, only on yp @y0 > [email protected] , and the initial position and the initial velocity of the particle. The complete equations of motion (eqs. (3.77) and (3.78)) can be solved only numerically. The solutions (i.e. the particle trajectories) are of two types, depending on whether the particle is captured by the wire or not. The critical trajectory, for which the particle is just captured, is characterized by the capture radius Uf . Approximate analytical solutions of the equations of motions s in the case of the potential ﬂow, under the condition that | ypd @y0d | 2> yield the following expression for the capture radius in the longitudinal and transverse conﬁgurations [G1, G5]: s · ¸ 3 3 ypd [email protected] 2 ypd [email protected] 1 ( (3.82) |) ) (| Ufd ' 4 y0d 3 y0d where the normalized quantities are deﬁned as Ufd = Uf @d> ypd = yp @d and y0d = y0 @d= Thus, for a given | ypd @y0d | ratio, both conﬁgurations have the same capture radius. s When | ypd @y0d |? 2> the critical capture radius in the longitudinal conﬁguration ( = 0) is given by Ufd =

i 1 ypd h (1 N 2 )[email protected] + N( arccos N) 2 y0d

(3.83)

and in the transverse conﬁguration ( = @2) [G1]: Ufd =

i 1 ypd h (1 N 2 )[email protected] + N(2 arccos N 2 y0d

(3.84)

It is apparent from eqs. (3.82), (3.83) and (3.84) that the dependence of Ufd upon the ratio yp @y0 can be divided into two categories: at low values of yp @y0 , the capture radius increases linearly with this ratio Ufd

yp y0

(3.85)

while at large values it increases approximately as Ufd (

yp [email protected] ) y0

(3.86)

Axial conﬁguration The analysis of a particle motion in the axial (A) conﬁguration, where the wire axis and the ﬂuid ﬂow are mutually parallel, and the magnetic ﬁeld is perpendicular to them (Figs. 3.13 and 3.17), does not require, in contrast to other cases, numerical computations. Since the results can be derived in an analytical form, this conﬁguration became a favourite object of the modelling of particle capture. The dynamics of the particles and their build-up on the wire

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

189

y H0

v0

ș

x

z

Figure 3.17: The axial conﬁguration.

in A-conﬁguration have been described in numerous papers, for example [G9, B12, U4, B13]. The equations of particle motion (eqs. (3.77) and (3.78)) are reduced in this conﬁguration to the simpliﬁed forms cos 2 gud yp N ) = ( 5 + gw d ud ud3

(3.87)

g yp sin 2 = gw d ud4

(3.88)

g}d y0 = gw d

(3.89)

The elimination of time from eqs. (3.87), (3.88) and (3.89) produces a set of dierential equations N gud = + ud cot 2 g ud sin 2

(3.90)

g}d y0 ud4 = g yp sin 2

(3.91)

From these equations the particle trajectories can be determined analytically [G1,G9, B12].

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

190

Upstream build-up

y

H0

v0 θc

x

Downstream build-up Figure 3.18: Build-up of paramagnetic particles on a magnetized wire in the longitudinal conﬁguration. Particle build-up Previous analyses of particle trajectories in the vicinity of a magnetized wire considered the capture process in the initial stage, i.e. with no loading of the wire with the captured particles. The determination of the exact process of the particle build-up is a complicated problem. As the suspension ﬂows through the matrix, some of the particles, under the inﬂuence of several forces, are deposited onto the matrix elements or onto already deposited particles. Consequently the geometry, the structure and the surface characteristics of the matrix may be signiﬁcantly modiﬁed. These changes, in turn, aect the ﬂow of the suspension through the matrix and the subsequent capture. Further complications may also arise as a result of dislodgment of the captured particles and their possible re-capture. As a result, the dynamic behaviour of the separation process varies with the time as well as with other variables. The force that is principally responsible for the particle capture is the magnetic force. Particles are attracted towards the wire if the radial component of the magnetic force Ipu ? 0= Thus the condition Ipu = 0 deﬁnes the critical angle f given by eq. (3.66). The stability of a particle on the wire surface is determined by the balance of the tangential components mainly of the magnetic and hydrodynamic forces. Gerber found that the angle s , for which a paramagnetic particle will be retained on the wire, is given as [G1]: · ¸[email protected] y0 2 | s |6 arcsin 1 ( ) yp

(3.92)

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

y

191

v0 θc

H0 x

Figure 3.19: Build-up of paramagnetic particles on a magnetized wire in the transverse conﬁguration. It transpires from eq. (3.92) that retention will occur only if yp @y0 A 1 [W8, W9]. However, the experimental results show that a much less stringent condition can still lead to a reasonably high degree of capture. Examples of the build-up of paramagnetic particles on a magnetized wire in three principal conﬁgurations are shown in Figs. 3.18, 3.19 and 3.20. Diamagnetic particles are retained in the complementary regions as follows from Fig. 3.16. The experimentally determined build-up of paramagnetic kimberlite particles in the transverse conﬁguration is shown in Fig. 3.21. Essentially all theoretical descriptions of particle capture by a magnetized wire assumed the idealized situation in which the collection wire axis was oriented orthogonally to the magnetic ﬁeld direction. This assumption resulted from the belief that only these conﬁgurations would create sizable deposits. Birss et al. [B14, S26] considered the collection process on a cylinder with its axis oriented at an angle with the magnetic ﬁeld direction. They found that the eect of the non-orthogonal wire orientation can be taken into account by replacing the coe!cients yp @y0 and N by more general terms. These terms are the functions of the oset angle , deﬁned in Fig. 3.22. Experimental observation by Svoboda et al. [S27], of particle collection at various oset angles , demonstrated that even at the oset angle as large as 800 there is considerable collection of particles, as shown in Fig. 3.23. The length of the section of the wire where the diamagnetic capture takes place is a function of the oset angle. For the oset angle equal to @2 (the magnetic ﬁeld parallel with the wire axis) the paramagnetic capture takes place only at the end of the wire while the entire length of the wire is repulsive for paramagnetic particles, as shown in Fig. 3.24.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

192

y v0

H0 x

Figure 3.20: Build-up of paramagnetic particles on a magnetized wire in the axial conﬁguration.

Figure 3.21: Build-up of paramagnetic particles of kimberlite (mean size 4.7 m, magnetic susceptibility 1.7×106 m3 /kg) on a magnetized nickel wire in transverse conﬁguration (E0 = 1.7 T, y0 = 0.25 cm/s) [S27].

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

193

Į H0

x

vo z

Figure 3.22: The plane view of the generalized transverse orientation with the magnetic ﬁeld making an angle (@2 ) with the wire axis.

Figure 3.23: Collection of kimberlite particles on a nickel wire (diameter 125 m) in the transverse conﬁguration, with the magnetic ﬁeld making an angle of 100 with the wire axis (oset angle = 800 ), (B0 = 1.7 T, v0 = 0.25 cm/s) [S27].

194

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.24: Collection of paramagnetic kimberlite particles on a nickel wire magnetized along its axis (oset angle = 900 ) [S27]. Nesset and Finch [N2, N5] developed a static model of particle capture in HGMS, in which the ﬂuid drag force included the changing boundary layer thickness over the front portion of the wire. They assumed that for a particle to remain attached to the wire, two conditions would have to be met. First, the net radial force acting on a particle must be attractive, that is Ipu + Iju 6 0

(3.93)

where Ipu and Iju are given by eq. (3.62) and (3.74), respectively. The second condition is that the net tangential force must push particles towards the region of a greater attractive radial force. In the case of the longitudinal paramagnetic build-up, this condition can be expressed as: Ip + Ij + Ig 6 0

(3.94)

where Ig is the ﬂuid drag force, which is proportional to the shear stress 0 in the boundary layer. Thus [N2] Ig =

2 2 e 0 2

(3.95)

By solving equations (3.93) and (3.94), the outline of the build-up proﬁle can be found computationally as intersecting loci of points {u> } satisfying these equations. The two retention criteria are satisﬁed only in the cross-hatched region shown in Fig. 3.25.

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

195

Figure 3.25: Loci of zero radial and azimuthal forces around the wire in the longitudinal orientation (adapted from [N5]).

Capture of diamagnetic particles It transpires from eq. (1.8) that if the susceptibility dierence s i is positive, then the magnetic force between the wire and the particle is attractive, provided that the radial component Iu is negative. This is the case of capture of paramagnetic particles, under the condition that eq. (3.65) is satisﬁed. On the other hand, there are two symmetrical curved volumes, the boundaries of which are determined by the critical angle f , given by eq. (3.66), in which the radial force acting on paramagnetic particles is repulsive, while the radial force acting on diamagnetic particles is attractive. These regions, in which collection of diamagnetic particles takes place, are complementary to the regions of collection of paramagnetic particles, as illustrated in Figs. 3.18, 3.19 and 3.20. The value of f depends on both Pv (or Mv ) and K0 (or E0 ) as shown in Fig. 3.26. It can be seen that as the strength of the external magnetic ﬁeld increases, the area of the wire collector available for the capture of diamagnetic particle also increases. The eective area for the capture of paramagnetic particles is, therefore, correspondingly reduced. This phenomenon indicates that an increase in the operating magnetic ﬁeld can negatively aect the loading capacity of the matrix, the selectivity of separation and the overall performance of a magnetic separator. The ﬁrst experimental conﬁrmation of the diamagnetic capture was reported by Friedlaender et al. [F9]. They showed that by dissolving a paramagnetic salt in water, i can be made positive and su!ciently large, so that =| s i | is large and the attractive magnetic force is su!ciently strong to recover particles of aluminium oxide. A theory of diamagnetic capture was developed and published by Birss and Parker [B15], simultaneously with

196

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.26: The critical angle f as a function of the magnetic induction (for Mv = 1.7 T) [S1]. Friedlaender’s experimental paper [F9]. Although the recovery of diamagnetic particles by magnetic separation is feasible in principle, simultaneous capture of paramagnetic particles prevents a magnetic separator from being a selective device for separation of diamagnetic materials. This limitation can be, however, overcome by magnetizing the wire collectors along their long axes (the oset angle = @2). At this orientation, the paramagnetic particles are captured only at the end tip of the wire, as is shown in Fig. 3.24. The entire length of the wire is then attractive for diamagnetic particles. Collection of diamagnetic bismuth particles in this conﬁguration was observed by Svoboda et al. [S27] and is shown in Fig. 3.27. Magnetic separation at moderate Reynolds numbers Experimental investigation by Friedlaender et al. into the particle capture on a single wire in the longitudinal conﬁguration indicated [F10] that for moderate values of Reynolds number for the wire (Re 6 to 40), the material can be captured at the rear of the wire. Theoretical treatment by Watson [W10] showed that at higher velocities of the suspension a pair of stable standing vortices, which appear on the downstream side of a wire, can induce capture of particles on the trailing side of a matrix collector. This situation is illustrated in Fig. 3.28. The shaded areas on the upstream and downstream sides of the wire are attractive for paramagnetic particles. The unshaded portions around the | axis are repulsive, and particles arriving from the front part of the wire towards the wake must, therefore, pass through the repulsive regions. It was shown in subsequent studies that the magnitude of the Reynolds num-

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

197

Figure 3.27: Collection of diamagnetic particles of bismuth (" = - 16.3×109 m3 /kg) on the upstream and downstream sides of the nickel wire magnetized parallel to its axis ( E0 = 1.9 T, v0 = 0.13 cm/s) [S27].

y O VO

x

Figure 3.28: The downstream capture into a stationary wake formed by twin vortices.

198

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

ber is not the only condition for the vortex capture [W11]. The thickness of the boundary layer, the particle size and the ﬁeld strength were found to be the main factors aecting the vortex capture. In particular it was determined that, for vortex capture to occur, it is necessary that yp @yr ? 1. The separation process, taking place under such conditions, for which the downstream particle capture takes place, was termed vortex magnetic separation by Watson [W11]. The applicability of this phenomenon, investigated mainly in single-wire experiments, to real operational situations, has been a subject of controversy [S28, W12]. It was argued by Watson et al. [L8] that if the conditions for the downstream capture are met, the recovery, the grade of the magnetic concentrate and the throughput would be very high. However, it was shown by Svoboda [S28] that such conditions can be possibly met only when very ﬁne (e.g. 125 m) steel wool matrix is used and when the ﬂow rate of the slurry through the matrix is close to the upper limit possible in such a matrix [S29]. Such conditions are usually used to remove ﬁne weakly magnetic impurities from industrial minerals, such as kaolin. In those applications, however, the magnetic fraction is a waste and its grade is of no relevance to the e!ciency of the process. On the other hand, in those applications where the magnetic fraction is the useful product, such as beneﬁciation of ferrous and non-ferrous ores, much coarser matrix (e.g. expanded metal or woven mesh) and much higher slurry velocities must be used in order to maintain meaningful economically viable throughput. Under these circumstances the conditions for the vortex formation are not met since the Reynolds number is at least an order of magnitude greater than the upper value required for downstream capture to take place.

3.4.2

Capture of particles in multi-collector matrices

The matrix of a real magnetic separator consists of a large number of individual collectors. There are essentially two possible ways of developing a theory of multi-collector magnetic ﬁlters: one way is to build the theory from ﬁrst principles and the other is to incorporate the single-collector model into a multicollector phenomenological description. In the ﬁrst approach, the particle trajectories and the capture e!ciencies were investigated for the case of wire collectors arranged in regular arrays. Conﬁgurations of single and double layers of wires were analyzed and reported in numerous publications [H14, T4, E1, S30, G7, R12, R13]. As a result of considerable mathematical complexity of the problem the applicability of the theory to real matrix is limited. Particle capture by ferromagnetic spheres. In spite of high e!ciency of a ball matrix in some industrial applications of magnetic separation [S1], only a limited attention has been paid to the theoretical analysis of particle capture by spherical collectors. The character of the particle capture and of the buildup is inevitably dierent for spheres compared to the wires. The dierence follows from the fact that the cross-sectional capture area of a sphere increases

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

199

Figure 3.29: The e!ciency of magnetic ﬁltration of Fe2 O3 particles (diameter 0.08 m) in a bed of steel spheres, as a function of the applied magnetic ﬁeld (adapted from [A16]). quadratically with the capture radius Ufd , whereas that of a wire increases only linearly. Friedlaender et al. [F11, F12] solved numerically the equation of motion (eq. 3.58) in transverse conﬁguration and found that the capture of paramagnetic particles occurred in conically shaped surfaces deﬁned by the critical angle ; h d i< ? 2 1 + 2Nv ( )3 @ u i h (3.96) | f |= arcsin = 3 1 + N ( d )3 > v u which is equivalent to eq. (3.66) derived for a cylindrical wire. The parameter Nv given by P Nv = (3.97) 3K0 is equivalent to eq. (3.61) for the wire. Capture of diamagnetic particles then takes place on conical surfaces complementary to those for paramagnetic capture. It transpired from theoretical analysis of particle capture in a bed of spheres by Watson and Watson [W13] that the probability of particle capture increased with increasing background magnetic ﬁeld until the ﬁeld was high enough to saturate magnetically the ferromagnetic spheres. However, Moyer et al. [M15, M16] argued that the observed saturation of the capture probability occurred at the magnetic ﬁeld strengths far below those required to saturate magnetically the spheres comprising the matrix bed.

200

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.30: Schematic view of the normalized build-up [email protected] in a ﬁlter, as a function of the ﬁlter length. This theoretical prediction was conﬁrmed experimentally by Arajs et al. [A16]. As Fig. 3.29 illustrates, the ﬁltration e!ciency of submicrometer particles of Fe2 O3 in a bed of steel spheres levelled o at the magnetic induction of about 0.1 T, far below the saturation polarization of 1 T of the sphere material. Such a behaviour was not observed for an isolated collecting sphere [F12]. This is a very signiﬁcant observation, since it indicates that the mechanisms of particle capture on a single collector and on an assembly of collectors in a packed bed are governed by dierent laws. It becomes clear again that it is not permissible to extend single-collector theoretical models (eqs. (3.83) and (3.84)) to multicollector assemblies of matrix collectors. Phenomenological model of HGMS The alternative approach to multi-collector magnetic separation is a phenomenological model [W14, G1], which is less rigorous but at the same time less complicated and closer to practical needs of high-gradient magnetic ﬁltration. It cannot, however, be easily applied to the process of separation of multicomponent mixtures of materials. The fundamental equations describing the particle retention in a ﬁlter and the time-dependent performance of a ﬁlter are the macroscopic conservation equations and the rate equation. Let us consider particles travelling through an absorption ﬁlter of length O, as illustrated in Fig. 3.30. By equating the dierence between the numbers of particles entering and leaving the volume { per unit time, to the time rate of increase of the number of particles, the conservation equation is obtained as CQ ({> ) Cf({> ) = y0 C C{

(3.98)

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

201

1

cout/cin

T

t

Figure 3.31: A breakthrough curve of a ﬁlter with a constant absorption coe!cient . At time W the ﬁlter becomes fully saturated. where Q ({> ) is the number of captured particles in the ﬁlter between { and { + {, at time = f({> ) is the number of suspended particles in a volume of the ﬂuid {, is the porosity of the ﬁlter matrix, y0 the superﬁcial velocity and the displacement time deﬁned as = w {@y0 = The rate equation can be expressed in the form of the Iwasaki relation [R14] (

Cf )w = f C{

(3.99)

where is the ﬁlter coe!cient having the dimension of the reciprocal length. Equation 3.99 shows that the proﬁle of the particulate concentrate in the liquid phase throughout a ﬁlter is logarithmic. The solution of the rate equation can thus be written as f({) = exp({) flq

(3.100)

frxw = exp(O) flq

(3.101)

where flq and frxw are the inﬂuent and e"uent concentrations. Since nothing is known, in the phenomenological approach, about the physical processes taking place inside the ﬁlter, all information about the ﬁlter performance must be derived from its breakthrough curve, i.e. from the output concentration as a function of time, as shown in Fig. 3.31. By incorporating the single-wire magnetic separation model into the above eqs. (3.100) and (3.101) Watson found [W8], the e!ciency of the magnetic ﬁlter to be frxw i OUfd = exp( ) (3.102) flq d

202

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where = 2 for ordered ﬁlters and = 4/3 for random ﬁlters. Ufd is the normalized capture radius given, for example, by eqs. (3.82) to (3.84), while i is the ﬁlling factor of the ﬁlter matrix (i = 1 ). Equation (3.102) clearly illustrates that it is not possible to extend the singlewire capture approach to multi-collector situation, as already demonstrated by Fig. 3.29. According to eq. (3.102), the e!ciency of the ﬁlter depends on the capture radius calculated for the single-collector scenario. In the single-collector situation the particle capture is indeed determined by the capture radius and, therefore, by the magnetic velocity or by the strength of the applied magnetic ﬁeld. In a multi-collector situation, there are several additional mechanisms that lead to particle collisions with the collectors and ultimately to capture. As will be shown in the next section, under suitable conditions, usually present in real operational situations, these mechanisms can be signiﬁcantly more important than the magnetic traction mechanism, the only mechanism of particle capture considered in the single-collector approach. By inclusion of the single-collector capture radius Ufd , eq. (3.102), therefore, underestimates, by a wide margin, the e!ciency of the ﬁlter and, at the same time, overestimates the role of the magnetic ﬁeld in particle capture. Particle capture in a real matrix It transpires from the above discussion that it is not permissible to incorporate the single-collector model into a multiple-collector situation. In a single-collector situation the probability of a particle colliding with the matrix element is very small and the particle thus must be attracted to the collector by the magnetic traction force. On the other hand, in a real situation, where the matrix is essentially a bed of matrix elements, the e!ciency of particle collision with the matrix elements is determined, to a great extent, by mechanical, i.e. ”nonmagnetic” mechanisms of collision, as has been argued by Svoboda [S31, S32]. It can, therefore, be assumed that HGMS is essentially a deep bed ﬁlter with an externally applied magnetic ﬁeld. High-gradient magnetic separation can thus be viewed as a stochastic process in which the chance of a particle reporting into the magnetic fraction is the product of two probability terms: Suhfryhu| = Sfroolvlrq × Suhwhqwlrq

(3.103)

where Suhfryhu| is the probability of recovery of a particle into the magnetic fraction, Sfroolvlrq is the probability of collision between a particle and the matrix and Suhwhqwlrq is the probability of retention of a particle on the matrix. While the ﬁrst term on the right-hand side of eq. (3.103) is controlled by the hydrodynamic and geometrical conditions in the matrix, the second term depends on the magnetic and surface forces between the particle and the matrix element, and on the hydrodynamic regime. Collision of particles with the matrix. Figure 3.32 illustrates typical collision mechanisms in a deep bed ﬁlter. These mechanisms also play a decisive role

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

203

A C

D

B a

Figure 3.32: Collision mechanisms in deep-bed ﬁltration. in multi-collector HGMS. A particle following a streamline may come in contact with the matrix element by virtue of its ﬁnite size (interception or straining, case A), and as a result of inertia (case B), sedimentation (case C) or diusion (case D). The velocity of the liquid can be also greater on one side of the particle than on the other, causing the particle to rotate. As a result, a force that develops laterally to the direction of ﬂow will drive particles across the ﬂow ﬁeld. This hydrodynamic eect also contributes to the collision of particles with collectors. The collision probability can then be written, according to eq. (3.101): ffro = 1 exp(O) flq

(3.104)

where ffro is the concentration of particles which collided with the matrix collectors. The ﬁlter coe!cient can be written in terms of the collision e!ciency of a single collector as [M17] = (

3 [email protected] s ) ln(1 ) 4 d

(3.105)

where s = (1 )[email protected] . The total ﬁlter coe!cient can be obtained from eq. (3.105) by calculating the collision e!ciencies l of individual processes (e.g. [W15, I4, C12, H15]) that lead to collision. It was found [S33] that, for example, for steel wool and ball matrices, with element diameter of 200 m and 6 mm, respectively, the dominant mechanism of collision is sedimentation. The hydrodynamic eect also contributes, particularly for small particles. On the other hand, wedging in the crevices of the matrix becomes signiﬁcant for larger particles. Equation (3.104) then can be used to calculate the ratio ffro @flq , i.e. the ratio of the concentration of particles that collided with the matrix, to the concentration of particles that entered the matrix bed. Figure 3.33 documents that all particles as small as 4 m, moving with superﬁcial velocity of 0.07 m/s

204

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.33: The proportion of particles colliding with steel wool matrix as a function of of the matrix length. y = 0.07 m/s, 2d = 400 m, = 0.95 (adapted from Svoboda [S33]).

Figure 3.34: The proportion of particles colliding with a steel ball matrix, as a function of the matrix depth. y = 0.07 m/s, 2d = 6 mm, = 0.4 (adapted from Svoboda [S33]).

3.4. HIGH-GRADIENT MAGNETIC SEPARATION

205

Figure 3.35: The proportion of particles colliding with steel wool matrix, as a function of superﬁcial velocity. O = 200 mm, 2d = 400 m, = 0.95 (adapted from [S33]). or smaller, will have collided with the steel wool matrix, with the matrix bed depth of 200 mm. A similar trend can be observed for the steel ball matrix, as illustrated in Fig. 3.34. With decreasing velocity the probability of collision rapidly increases, as shown in Fig. 3.35. The retention of particles For a particle to be retained on the matrix after a collision, the total interaction between the particles and the matrix and the ﬂuid medium must be attractive. For su!ciently large particles the surface forces can be neglected and the magnetic dipolar and the hydrodynamic interactions are decisive. The mean free magnetic energy for the interaction of a spherical paramagnetic particle of susceptibility with a ferromagnetic sphere of saturation magnetization Pv > placed in an external magnetic ﬁeld E can be written [S1] as 4E 2 e2 32 2 e3 d3 EPv Yp = (3.106) 30 9u3 where u is the distance between the interacting bodies. Since d AA e and u = d + e, eq. (3.106) gives [S31] Yp =

32 2 3 e EPv 9

(3.107)

The hydrodynamic potential energy of a particle captured on the surface of a

206

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

collector is assumed to be Stokesian: Yg = 6yde

(3.108)

A particle will remain attached to the matrix if Yp + Yg ? 0. Therefore, for a particle to be retained by the matrix, the magnetic induction must be greater than the threshold magnetic induction that can be determined from the steadystate condition Yp + Yg = 0. Therefore, [S33]: EA

27yd 16e2 Pv

(3.109)

It is evident from eq. (3.109) that, for given conditions of separation, i.e. particle size and susceptibility, ﬂow velocity and size of matrix elements, an increase in strength of the applied magnetic ﬁeld beyond the threshold value will not increase the retention of particles on the matrix. It might appear from eq. (3.109) that by increasing the magnetic ﬁeld strength it is possible to increase the ﬂow velocity and thus the throughput of a separator, and still maintain the required rate of particle retention. However, if the particle velocity is too high, the particles will never collide with the matrix bed and will thus not be available for retention. This scenario is illustrated in Fig. 3.35. Furthermore, the selectivity of the separation process is be determined by the e!ciency with which the "non-magnetic" particles are being swept away from the matrix by the erosive force of the ﬂuid. Consequently, for particles that are supposed to report into the non-magnetic fraction, the inequality inverse to that given by eq. (3.109) should apply. This is in contrast to the trajectory models, in which the non-magnetic particles never reach the matrix surface.

3.5

Linear open-gradient magnetic separation

The concept of separation in a magnetic ﬁeld with open gradient of the ﬁeld is widely practised in drum and roll magnetic separators. Paradoxically, it is the linear multipole open-gradient magnetic separation (OGMS) that received considerable attention from the theoretical point of view, in spite of its failure to prove its advantages on the production scale. It has been explained in Section 2.5.3, that the linear multipole OGMS consists of an array of vertically positioned coaxial coils energized in opposite directions. The concept is schematically shown in Figs. 2.85(a) and (b) and in Fig. 3.36. The magnetic force directed radially inwards diverts the free-falling magnetic particles inwards while the feebly magnetic particles fall vertically, unaected by the magnetic force. The main advantage of open-gradient separators, in comparison with HGMS, is the absence of matrix which allows the elimination of the blockage problem. Another advantage of OGMS is the use of superconducting magnets which lend themselves easily to scale-up. This is because in resistive magnetic systems the

3.5. LINEAR OPEN-GRADIENT MAGNETIC SEPARATION

207

Feeder

Splitter Cryostat with superconducting coils

Figure 3.36: Schematic diagram of a linear multipole open-gradient magnetic separator. magnetic ﬁeld in the separation space is limited by the non-linear saturation eects in steel [G5]. On the other hand, systems consisting of superconducting magnets are linear as far as the magnetic ﬁeld generation is concerned, and the electric power consumption, which is spent mostly for cryogenic purposes, increases only moderately with their size. It was also found by Gerber et al. [G8] that the metallurgical e!ciency of the superconducting OGMS is superior to the conventional OGMS as a result of considerably larger particle deﬂections achievable in various designs of coil conﬁgurations. A detailed analysis of particle trajectories in dry OGMS was made by Collan et al. [C13], while Kopp [K10, K11] developed a simple kinetic model of the separation process. These models were subsequently reﬁned by numerous authors [B16 , G9, J3, B17, P6, G5]. Particle trajectories and particle deﬂections as a function of particle properties, particle collisions, electric current densities in the coils and the separator geometry were determined. Diamagnetic mode of OGMS was also described theoretically and conﬁrmed experimentally by Krist et al. [K12]. Considerable eort was also devoted to the optimization of the design parameters of the superconducting coils for OGMS [G10, G11, K13, J4, P7]. Although theoretical analyses of particle motion in OGMS are of considerable mathematical elegance, their applicability to practical problems of material separation is limited. In view of a somewhat esoteric character of the subject and as a result of the failure of several eorts to industrialize the concept of

208

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

OGMS [G3, K9, A8, S17] and to achieve commercial success, detailed description is beyond the scope of this monograph. The interested reader is referred to the literature listed above.

3.6

Magnetic ﬂocculation

The demand for mineral products is subject to two factors aecting the e!ciency of beneﬁciation: a decrease in the quality of economically accessible ores and an increase in the degree of ﬁneness of their valuable components. Since the recovery of ﬁne particles is still very ine!cient, vast quantities of valuable minerals are often lost in the form of slimes. Unless new technologies are developed, the increasing amount of ﬁnely-dispersed minerals that being mined and processed, will lead to increased volumes of waste. This will result in a substantial loss of valuable components and in environmental problems. Methods for the treatment of ﬁne particles are still in the early stages of development, and conventional methods are usually ine!cient for particles smaller than 20 m. Particles smaller than 5 m can be manipulated only by HGMS, a rather specialized technique applicable to a limited range of materials. A more general solution to the problem may lie in the formation of aggregates comprising ﬁne particles. In the past, ﬂocs were successfully formed by the addition of inorganic electrolytes or polymers, for instance for the removal of colloidal particles from e"uents. Flocculation can also be induced by the application of external forces to a system of particles, e.g. by stirring, or by the application of magnetic or electrical ﬁelds. Magnetic ﬂocculation has been used for some time to create ﬂocs of ferromagnetic particles. To induce this process, a magnetic induction of the order of 0.01 T is required. Experimental observations of magnetic ﬂocculation of strongly magnetic minerals and its application to the mining industry have been described in numerous publications [B18, B19, B20, B21, L9, K14, K2]. The theoretical description of mutual coagulation of ferromagnetic particles is also well established [D9, J5, L10, L9]. Although investigations into the magnetic ﬂocculation of paramagnetic and diamagnetic particles started much later [H16, W16, S34], systematic studies of the theoretical and experimental aspects [S35, P8, S36, P9, S37, S38, W17, W18, W19, P10, T5, S39, S40, S41] show that ﬂocculation of ﬁne, feebly magnetic, particles can be induced in magnetic systems that are presently available. In the following sections the present status of the theory of magnetic ﬂocculation of strongly and weakly magnetic materials will be brieﬂy outlined.

3.6.1

Magnetic ﬂocculation of strongly magnetic materials

The tendency of an assembly of ferromagnetic particles in the magnetic ﬁeld of a magnetic separator to reduce its magnetostatic energy often results in the formation of aggregates of the particles. The eect of magnetic ﬂocculation

3.6. MAGNETIC FLOCCULATION

209

is the inherent part of any process of manipulation of ﬁnely ground strongly magnetic materials and directly aects the e!ciency of material separation. In magnetic separation the process of magnetic ﬂocculation can often play a positive role by increasing the recovery and/or throughput. In other processes, such as recovery of dense medium, magnetic ﬂocculation is detrimental to the e!ciency of dense medium separation. Theory of magnetic ﬂocculation We shall consider a suspension of identical spherical ferromagnetic particles in a non-magnetic ﬂuid. Under the inﬂuence of a su!ciently strong external magnetic ﬁeld such particles tend to associate in long chains. Each particle s. of volume Ys and magnetization Ps carries a magnetic moment P = Ys P The energy of magnetic interaction between particles (1) and (2) separated by a distance u is YP =

1 P (1)P (2) 3[P (1)u][P (2)u] { } 0 u3 u5

(3.110)

If magnetization of the particles is su!ciently large, the electrical double layer interaction and the van der Waals interaction can be neglected. Total interaction energy, therefore, consists of the magnetic dipolar term only (eq. (3.110)). Eective magnetic interaction in the suspension can be obtained by averaging YP over all orientations of the colloidal particles. Thus [C14, C15] YP Y¯P = nW ln ? exp( )A nW

(3.111)

where n is the Boltzmann constant and W is the absolute temperature and Z YP 1 YP (3.112) exp( ) A= )g 1 g 2 g 3 ? exp( 3 nW 64 nW where g l (l =1,2,3) represents an element of a solid angle describing the orientation of each of the dipoles (1, 2) and that of the external magnetic ﬁeld (3). It was shown by Chan et al. [C14, C15] and by Scholten et al. [S42] that in the weak interaction limit, i.e. when 2P @0 u3 ? nW , the average interaction energy can be written as 4 Y¯P = 2 P6 (3.113) 30 u nW while in the strong interaction limit (2P @0 u3 A nW ) 2

2 Y¯P = P3 0 u

(3.114)

It can thus be seen that although the magnetic dipole-dipole interaction (eq. (3.110)) can be either attractive or repulsive, depending on the relative orientation of the dipoles, the orientational averaging process gives the energetically favourable (attractive orientation) heavy weighing.

210

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.37: The eect of the magnetic ﬁeld strength on the degree of ﬂocculation of strongly magnetic particles (adapted from [K14, K2]). A condition for magnetic ﬂocculation to take place can be expressed as Ip A Ig + Ih

(3.115)

where Ih is the electric force as a result of electrical double layer. Since Ip AA Ih for ferromagnetic particles at reasonably strong magnetic ﬁeld, the probability of ﬂocculation is determined by the interplay between the magnetic and hydrodynamic forces. As a function of the magnetic ﬁeld strength, the process of magnetic ﬂocculation proceeds through several stages, as is shown in Fig. 3.37. In stage 1, which corresponds to the steady-state phase of the process, in which Ip 6 Ig , the degree of ﬂocculation # i is proportional to Ip and, therefore, # i = nK 2 = At this phase the grade of the ﬂocs is high and ﬂocculation is selective. With further increase in the magnetic ﬁeld strength the magnetic interaction becomes dominant and the ﬂocculation enters phase 2. The process proceeds non-selectively at a very high rate and the grade of the ﬂocs is reduced. When the concentration of solids in a suspension is reduced below a certain threshold value, the mean distance between the particles and their characteristic ﬂocculation time increase and the process enters an equilibrium phase 3.

3.6.2

Magnetic ﬂocculation of weakly magnetic minerals

In contrast to strongly magnetic materials, the magnetic ﬂocculation of paramagnetic and diamagnetic materials is a considerably more complex process. In spite of its signiﬁcant potential, the process has not found any application on industrial scale as yet. Although several theoretical models that predict the behaviour of weakly magnetic particles of quasi-colloidal dimensions, in the

3.6. MAGNETIC FLOCCULATION

211

presence of the external magnetic ﬁeld, have been developed over the last twenty years, their experimental veriﬁcation is still limited and is mainly of qualitative character. Stability of colloidal suspensions The criteria of the stability of colloidal suspensions are governed largely by the interplay of repulsive and attractive forces between the particles. A detailed description of this interplay is the basis of the theory of stability of hydrophobic colloids as proposed by Derjaguin and Landau [D14] and Verwey and Overbeek [V1] (DLVO theory). The DLVO theory views the stability of colloids as arising from electrical charges on identical particles and a consequent electrical repulsion between them. Opposing this repulsion are the attractive forces of the universal London-van der Waals type. If the repulsion force can be su!ciently reduced so that the attractive interaction becomes dominant then the particles colliding with one another will stick together to form quasi-stable aggregates. The charge on a particle, together with the equal and opposite charge in a suspension, comprise the electrical double layer (EDL). Hogg et al. [H17] showed that the interaction of EDL between two dissimilar particles, under the condition of low surface potential and small thickness of EDL compared to the particle size, is given, under the assumption of a constant surface potential, by ¸ · u e1 e2 (# 21 + # 22 ) 2# 1 # 2 1 + exp([k) 2[k YU = ) (3.116) ln + ln(1 h 4(e1 + e2 ) (# 21 + # 22 ) 1 exp([k) where e1 > e2 and # 1 > # 2 are the radii and surface potentials of particles, respectively, u the dielectric constant of the medium, [ the Debye-Hückel reciprocal length parameter, and k their distance between the surfaces of the interacting particles. [ is related to the ionic strength Lp of the medium by the expression [=

[email protected]

8h2 Lp u nW

(3.117)

In the case of identical spherical particles eq. (3.116) reduces to u e# 2 (3.118) ln(1 + h[k ) 2 When the thickness of EDL is not small (i.e. when e[ ? 1), YU can be expressed in a simple approximate form: YU =

YU = u e2 # 2

exp([k) (2e + k)

(3.119)

Similarly, the London - van der Waals interaction for dissimilar spheres can be written as 6 5 2e1 e2 2e1 e2 + + D 9 k2 + 2(e1 + e2 )k k2 + 2(e1 + e2 )k + 4e1 e2 : : (3.120) YD = 9 8 k2 + 2(e1 + e2 )k 6 7 ln 2 k + 2(e1 + e2 )k + 4e1 e2

212

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

where D is the Hamaker constant. For identical particles, eq. (3.120) simpliﬁes to ¸ · D k2 + 4ek 2e2 2e2 YD = (3.121) + ln 2 + 6 k2 + 4ek k2 + 4ek + 4e2 k + 4ek + 4e2 When the London forces operate over distances comparable to or larger than 0.1> where is the wavelength of the intrinsic electronic oscillations of the atoms, the interaction is reduced by the retardation eect [S43, R15]. Flocculation in a magnetic ﬁeld When a suspension of colloidal particles is placed in an external magnetic ﬁeld there is, in addition to the interactions considered so far, a magnetic dipolar interaction, described by eq. (3.110). In the strong interaction limit [C14, S34], the mean magnetic interaction energy can be written as YP =

80 1 2 e31 e32 K 2 9(k + e1 + e2 )3

(3.122)

where l are volume magnetic susceptibilities of particles and K is the magnetic ﬁeld strength. In agreement with the assumption of the DVLO theory that double layer and van der Waals forces are independent and additive, Svoboda [S34] supposed that the total energy of interaction of colloidal particles in the external magnetic ﬁeld is, therefore, given by the sum of electrical double-layer energy, van der Waals interaction energy and magnetic dipolar interaction energy YW = YU + YD + YP

(3.123)

Generally, the total interaction energy YW can be either attractive or repulsive depending on the sign of the individual terms on the right-hand side of eq. (3.123). Electrical double layer energy is repulsive for interaction of particles of the same material, while it can be attractive or repulsive for interaction of unlike materials (e.g. between a valuable mineral and gangue). The van de Waals interaction is usually attractive, but under certain conditions [V2], determined by relative values of the Hamaker constant of the interacting particle and the medium, the interaction becomes repulsive. Magnetic interaction can be either attractive or repulsive, depending on the signs of the magnetic susceptibilities of the interacting particles. It is clear that interaction between diamagnetic and paramagnetic particles is repulsive. On the other hand, magnetic interaction of identical materials, whether paramagnetic or diamagnetic, is always attractive. Magnetic ﬂocculation of diamagnetic particles is, therefore, possible, in principle. A curve of the total interaction energy YW as a function of the interparticle distance is shown in Fig. 3.38. A potential barrier Ymax separates two minima: a closer and deeper primary minimum and a more distant and shallow secondary

3.6. MAGNETIC FLOCCULATION

213

VT

Vmax Vmin 0

r

2b

r

Figure 3.38: The general form of the total potential energy for a pair of interacting colloidal particles of radius e= minimum of depth Ymin . The individual potential energy contributions are aected by the properties of a suspension in dierent ways. The magnitude and range of the electric double layer interaction YU are sensitive to # and [, which are controlled by the solution conditions (i.e. ionic strength and pH), whereas the van der Waals and magnetic contributions YD and YP are independent of these parameters. The magnitudes of the individual potential energy components have a dierent dependence on the particle size: YP is proportional to the cube of the radius while YU and YD are much less sensitive to particle size as they are proportional to the ﬁrst power of particle size. The height of the barrier determines the stability of a suspension. If the barrier is very low, there is nothing to prevent contact between the particles, and ﬂocculation will take place at a rate governed by the frequency with which the particles collide. If there is a secondary minimum in the curve of a potential energy, particles can ﬂocculate into this potential well. In this instance, the potential barrier need not be suppressed. Flocs thus formed will have a rather loose structure as a result of large interparticle distance at which the secondary minimum is created. The existence and position of the primary and secondary minima can be aected by changes in the magnetic ﬁeld, the magnetic susceptibility of the particles and the pH value of the suspension. The total interaction energy YW is shown in Fig. 3.39 as a function of magnetic induction and particle size. In region I the potential barrier is present and the secondary minimum is su!ciently close, while in region II the secondary minimum is too distant. In regions III and IV, in which, owing to high magnetic induction, the potential

214

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.39: Regions in which primary and secondary minima are found in the (a,B) plane, for hematite (# = 30 mV, [ = 105 m1 ), d - particle radius, E - magnetic induction (after [S36, S37]).

barrier is suppressed and the total interaction becomes attractive, and particles can ﬂocculate into the primary minimum. It follows from Fig. 3.39 that, for any particle size, a value of the magnetic induction can be found at which the potential barrier disappears. Wang et al. [W17] calculated the potential energy of interaction of particles of hematite and chromite in a magnetic ﬁeld. Typical curves shown in Fig. 3.40 illustrate that at moderate magnetic ﬁeld strength the potential barrier is eliminated and ﬂocculation into the primary minimum could take place. A deep secondary minimum is created at even lower magnetic ﬁeld. A threshold magnetic ﬁeld, at which the ﬂocculation into the primary minimum starts, can be determined provided that the total potential energy of interaction YW is negative [S34], or that the stability ratio Zs , which is given by eq. (3.124), is smaller than, or equal to, unity [S35]. The stability ratio is the ratio of the initial rate of ﬂocculation to that which would occur if the process was only diusion controlled (in the absence of an energy barrier) [P11]. µ

Z Zs = 2

exp

YW nW

¶

gv v2

(3.124)

3.6. MAGNETIC FLOCCULATION

215

Figure 3.40: The potential energy as a function of interparticle distance for 4 m hematite particles, [ = 108 m1 (adapted from Wang et al. [W17]).

Figure 3.41: Threshold magnetic ﬁeld, at which ﬂocculation into a primary minimum begins, as a function of particle size (adapted from Svoboda [S35]).

216

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

The values of the threshold magnetic ﬁeld Es , at which magnetic ﬂocculation into the primary minimum begins, are shown in Fig. 3.41, as a function of particle size, for various minerals. It can be seen that as the particle size and magnetic susceptibility increase, the threshold magnetic ﬁeld decreases. For ﬁne particles with a volume magnetic susceptibility smaller than 103 (SI), the threshold magnetic ﬁeld is too high for magnetic ﬂocculation to be practicable. This is particularly true for the magnetic ﬂocculation of diamagnetic materials, which require a magnetic induction of the order of tens of hundreds of Tesla. Flocculation in the secondary minimum As shown in Fig. 3.39, there is a secondary minimum (SM) in addition to the primary minimum in regions I, II and III. Although in regions I and II the potential barrier prevents particles from ﬂocculating into the primary minimum, particles can ﬂocculate into the secondary minimum. The secondary minimum in region II is too distant from the origin, and consequently, the aggregates will be packed too loosely. Furthermore, the secondary minimum is too shallow and the stability of the ﬂocs will be low. However, in region I, the secondary minimum can be deep enough and close enough to the origin to render it suitable for practical ﬂocculation. The mere existence of a secondary minimum does not imply an observable destabilization of a suspension. The other condition to be satisﬁed is su!cient depth of SM; the analysis indicates [S36] that, for Ymin A 1 kT (where kT is the unit of thermal energy), the value of the stability ratio Zv for ﬂocculation in a secondary minimum, as given by eq. (3.125), will be close to unity, and the ﬂocculation into SM will be rapid.

Zv =

R4

YW gv ) nW v2 Ymin 1 exp( ) nW

vp

vp

exp(

(3.125)

where vp is the position of the secondary minimum. The threshold magnetic ﬁeld Ev required to commence the ﬂocculation into SM can be determined from the condition Zv = 1. The dependence on a particle radius of threshold magnetic ﬁeld Ev in SM, which was determined from the condition of rapid ﬂocculation (Zv = 1), is shown in Fig. 3.42. A comparison of these values with those of the threshold magnetic ﬁeld Es for ﬂocculation into the primary minimum (Fig. 3.41) indicates that the magnetic ﬁeld needed to induce rapid ﬂocculation in SM is substantially lower. This conclusion has been conﬁrmed by detailed calculations by Wang et al. [W17], an example of which is presented in Fig. 3.40. Experimental conﬁrmation of the magnetic ﬁeld-induced ﬂocculation is depicted in Fig. 3.43. Figure 3.44 illustrates the experimentally determined onset of rapid ﬂocculation of hematite and chromite at threshold magnetic ﬁeld of about 0.5 T [W17].

3.6. MAGNETIC FLOCCULATION

217

Figure 3.42: Threshold magnetic ﬁeld for ﬂocculation into a secondary minimum, as a function of particle diameter (adapted from Svoboda [S35]).

Figure 3.43: The magnetic ﬁeld-induced ﬂocculation of hematite particles at various values of magnetic induction. pH = 7.8, # 45 mV, g50 = 3.9 m (adapted from Wang et al. [W17]).

218

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.44: The onset of the magnetic ﬁeld-induced ﬂocculation of hematite (g50 = 3.9 m) and chromite (g50 = 3.6 m) particles (adapted from Wang et al. [W17]). We have seen that under suitably chosen conditions, the interaction potential between a pair of colloidal particles can develop a signiﬁcant (> 1 kT) secondary minimum, while maintaining a large (AA 1 kT) primary maximum. Although the primary maximum will prevent irreversible coagulation into the primary minimum, the particles can undergo reversible ﬂocculation into the secondary minimum. The above treatment of the ﬂocculation process is applicable only to colloidal particles. For particles greater than the colloidal range, the thermal motion and the surface forces play only a limited role, and the process of ﬂocculation will be governed mainly by the gravitational and hydrodynamic forces. The kinetics of ﬂocculation It has been shown that the stability of suspensions depends on the magnitude of the potential barrier and on the existence and depth of the secondary minimum. In addition, however, determination of how quickly ﬂocculation will take place is necessary. Fuchs [F13] showed that the time taken for the number of particles to be halved is given by the relation [email protected] =

3Z 4nW Q0

(3.126)

where is the viscosity of the medium and Q0 is the initial concentration of the particles.

3.6. MAGNETIC FLOCCULATION

219

Figure 3.45: Dependence of the stability ratio Zs (as log Zs ) on magnetic induction for assorted sizes of hematite particles (adapted from Svoboda [S35]). It can be seen that the half-time of ﬂocculation is directly proportional to the stability ratio and indirectly proportional to the initial concentration of the particles. To achieve a reasonably short ﬂocculation time, low values of Z and high values of Q0 must be used. In chemical ﬂocculation, the values of Z smaller than 101 are reached with di!culty [V1]. This signiﬁcantly restricts the possibility of accelerated ﬂocculation. On the other hand, it was shown by Svoboda [S35], that in magnetic ﬂocculation, the values of the threshold magnetic ﬁeld determined from the condition Z = 1 for rapid ﬂocculation, allow reasonably short ﬂocculation time to be achieved. As is shown in Fig. 3.45, the values of Zs , of the order of 103 > can be achieved at reasonably low magnetic ﬁelds so that the ﬂocculation time into the primary minimum can be realistically short. Magnetic-hydrophobic ﬂocculation In order to explain situations in which the original DLVO theory failed, numerous ”non-DLVO” forces have been invented. A variety of forms of long-range forces such as hydrophobic/hydrophilic interaction have been introduced. For example, surface-active agents can adsorb at the mineral-water interface and render the solid hydrophobic. Particle-particle adhesion is favoured by the attraction between the hydrophobic coatings on dierent particles and the resultant reduction in the area of hydrophobic mineral-water surface. A critical review of such extensions of DLVO theory to include ”non-DLVO” interactions was published by Ninham [N6] who argued that confusion created

220

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.46: The potential energy curves for hydrophobic and magnetic ﬂocculation of rhodochrosite (2e50 = 2.25 m) hydrophobized by sodium oleate, at a magnetic induction of 0.9 T (adapted from [L11]).

by introduction of plethora of hydrophobic phenomena observed in the stability studies can, in principle, be explained by capillary condensation, i.e. thermodynamics. Several authors have shown that the stability of a colloidal suspension can be controlled, in addition to the electrostatic surface potential and the magnetic interaction, by such a hydrophobic interaction. Lu et al. [L11] included the energy of hydrophobic interaction YK as an additive term in the expression of the total interaction energy (eq. (3.123): YW = YU + YD + YP + YK

(3.127)

The hydrophobic interaction energy was expressed by two terms, each representing dierent mechanism of the hydrophobic interaction. The potential energy curves of three possible ﬂocculation mechanisms for paramagnetic rhodochrosite were calculated and are shown in Fig. 3.46. It can been seen that the potential energy of magnetic interaction exhibits a deep secondary minimum and a primary minimum barrier. In hydrophobic aggregation, a relatively low potential barrier partially prevents particles from rapid ﬂocculation into the primary minimum. On the other hand, the potential energy curve for combined magnetic and hydrophobic ﬂocculation shows deep primary and secondary minima, with no potential barrier. The experimentally determined rates of ﬂocculation in these three regimes are illustrated in Fig. 3.47. It is clear that the combined ﬂocculation by a

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION

221

Figure 3.47: Flocculation of rhodochrosite by magnetic (B = 0.85 T), hydropohobic (sodium oleate + kerosene) and combined mechanisms (adapted from [L11]). combination of magnetic and hydrophobic processes was more eective than aggregation induced by sodium oleate or magnetic ﬁeld alone. Škvarla and Zeleˇ nák [S41] developed a simple model of magnetic-hydrophobic ﬂocculation, as a variation of Lu’s model [L11]. They assumed that the potential of the hydrophobic interaction was of the short range and it was approximated by a single exponential YK = 2e VO exp(

kf k )

(3.128)

where VO is the solid/water interfacial energy of the spherical particles, kf is the contact separation distance of the spheres ( = 0.2 nm), and is the empirical constant ( = 1 nm). The model was veriﬁed by experimental observation of magnetic-hydrophobic ﬂocculation of siderite. A satisfactory correlation between the measured and calculated potential energy maxima was observed for the hydrophobic process. The prediction of the model of magnetic ﬂocculation alone was not satisfactory.

3.7

Magnetic separation by particle rotation

Motion of magnetizable particles in alternating or rotating magnetic ﬁelds is a well established research ﬁeld. In 1925 Koizumi [K15] designed a magnetic separator with a rotating magnetic ﬁeld, to eliminate entrapment of non-magnetic

222

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.48: Schematic diagram of a separator with rotating magnetic ﬁeld (courtesy of N. Allen [A17]).

particles in the magnetic concentrate. Similar approach was taken more recently by other researchers to improve the quality of magnetic concentration [T3, D1, F1, G12, G13, L9]. Although the results of these investigations had been positive, the technique did not appear to be accepted and developed further. Recently, Allen [A9] employed the concept of the eect of a rotating magnetic ﬁeld on magnetizable particles and developed rotating magnetic ﬁeld (RMF) separators, described in Section 2.6.3. The rotation separation is based on magnetic anisotropy of particles, which is present in ferromagnetic as well as paramagnetic materials. However, in paramagnetic minerals the magnetic anisotropy is generally too weak to be of practical use for particle separation. In general, ferromagnetic particles will rotate if they are placed in a rotating external magnetic ﬁeld, while paramagnetic particles will not. An RMF is generated by a rotating magnetic drum ﬁtted, around its circumference, with magnets, with alternate polarity. As is schematically illustrated in Fig. 2.95, the external magnetic ﬁeld exerts a torque on a magnetically anisotropic particle and makes it rotate and move it in the direction opposite to that of the rotating ﬁeld. A schematic diagram of such an RMF separator is shown in Fig. 3.48.

3.7.1

RMF rotation separation

In the RMF separator a particle is placed on a non-magnetic surface in a rotating magnetic ﬁeld, as shown in Fig. 3.49. If the particle is capable of rotation in the

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION x

223

Direction of particle rotation

Particle Direction of drum rotation

Magnet N S

S

N

N

Drum Fg,FgFm

Figure 3.49: Schematic diagram of a particle placed on a rotating magnetic drum. ﬁeld, it will experience a torque in order to align its axis of easy magnetization with the direction of the external magnetic ﬁeld. The torque, which thus arises when the direction of the magnetization of a particle and the external magnetic ﬁeld do not coincide, will force the particle to roll. The rolling is opposed by the force of gravity and magnetic traction force acting on the particle. The particles to be separated by rotation will, in general, contain ferromagnetic and paramagnetic regions. While the paramagnetic regions will make limited contribution to the particle rotation, they will contribute to the magnetic traction (holding) force. This traction force can, therefore, be written [A17] as: 1 Ip = s Yss EuE + Psi Ysi uE (3.129) 0 where Yss and Ysi are the volumes of the paramagnetic and ferromagnetic regions of the particle, respectively. Psi is the magnetization of the ferromagnetic components while s is the volume magnetic susceptibility of the paramagnetic contribution. The magnitude of the torque of the force I , required to rotate a particle, is the product of the magnitude of the force and the moment arm g; that is W = Ig (3.130) The particle will not start rotating unless the initial magnetic rotational torque exceeds the initial gravitational and magnetic traction force torques (case (a) in Fig. 3.50). The cubic shape of the particle is usually used to demonstrate the

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

224

(b)

(a)

( c)

B L

ș

M L

d

Fg Fm

Fg , Fm

Figure 3.50: Forces acting on a cubic particle in traction and rotating magnetic ﬁelds. case [A17, A18] and we have Wlqlw =

O (Ij + Ip ) 2

(3.131)

where O is the length of the cube edge and the force of gravity Ij is given by eq. (1.14). For a cubic ferromagnetic particle, under the assumption that the ﬁrst term on the right-hand side of eq. (3.129) can be neglected, the initial gravitational + magnetic holding torques (that is, when the particle is resting ﬂat on the surface) can be written Wlqlw = O3 s j

3.7.2

O O + Ps O3 uE 2 2

(3.132)

Magnetic torque on a particle and condition for separation by rotation

The application of an external magnetic ﬁeld to a ferromagnetic crystal, at a certain angle + to a direction of easy magnetization, causes a deviation of the magnetization, as indicated in Fig. 3.51. The external magnetic induction E applies a torque to the particle magnetization Ps and causes it to deviate from the direction of easy magnetization {. As a result, the magnetocrystalline forces apply a torque on the magnetization to return it to the direction of easy

3.7. MAGNETIC SEPARATION BY PARTICLE ROTATION

B

225

M ș

į

x

y

Figure 3.51: The torque experienced by an anisotropic magnetizable particle placed in an external magnetic ﬁeld. magnetization. This situation can be described by a relationship Ps E sin = Ps D sin

(3.133)

where D represents the anisotropy ﬁeld. If the external ﬁeld is very low, then the angle is small. If the external ﬁeld is very high, then is small [A17]. For a cubic particle, the magnetic torque given by eq. (3.48), can be rewritten as: Wpdj = Ys Ps E sin = O3 Ps E sin (3.134) where is the angle between the directions of the magnetic ﬁeld and particle magnetization, as can be seen in Figs. 3.50(b) and 3.51. Therefore, a particle will start rotating when Wpdj A Wlqlw (3.135) or, explicitly, E sin A

O s j + uE) ( 2 Ps

(3.136)

Coercive forces are very low for many ferromagnetics (s.l.), such as magnetite and steel, while anisotropy forces are high. If the external ﬁeld is smaller than the coercive force (E ? 0 Kf ), angular deviations from directions of easy magnetization are also small. Maximum torque is then applied when the external ﬁeld is very close to 900 to the particle magnetization. [A17]. Although the angle between the magnetization and the external ﬁeld has been maximized, the external ﬁeld is very low for most materials and, therefore, the torque is small. However, for materials of very high coercive force, such as roasted ilmenite, this is an advantageous situation for magnetic separation by rotation.

226

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

In a magnetic ﬁeld that exceeds the coercive force Kf of the material, the movement of domain walls within the solid substitutes for the movement of particles. The overall magnetization of a ferromagnetic particle is able to change direction in response to the direction of the external ﬁeld. However, while the changes of the direction of the domain magnetization may occur freely between directions of easy magnetization within a crystal, they are restrained for intermediate angles by magnetocrystalline anisotropy. In this case the maximum torque angle is approximately one quarter of the angle between directions of the external ﬁeld and the particle magnetization [A20, A17].

3.7.3

Rotation of particles in a liquid

It has been assumed, so far, that the particles to be rotated are suspended in air. If the particles are suspended in water, they are exposed, in addition to the force of gravity and the magnetic traction force, to hydrodynamic forces. These hydrodynamic forces are associated with a torque acting in the opposite direction [L9]. It was shown by Lantto [L9] that the hydrodynamic torque at a high Reynolds number is approximately given by Wk|gur =

1 $ 2 f4 e5 2 i

(3.137)

where $ is the frequency of the rotating magnetic ﬁeld, e the radius of the cylindrical particle, the length of which is fe (where f AA1). The magnetic torque is Wpdj = 2fe3 Ps E sin

(3.138)

Therefore, a cylindrical rod-like body will be brought into rotation when Wpdj A Wk|gur . This condition is met when EA

i $ 2 f3 e2 4Ps sin

(3.139)

It can be seen that rotation is more easily accomplished for small particles with large values of magnetization and large anisotropy angle . On the other hand, an increase in frequency of the rotating ﬁeld hampers the ability of particles to rotate. It has to be stressed, however, that if the value of the magnetic induction given by eq. (3.139) exceeds that corresponding to the coercive force (E A 0 Kf ) for the particle material, the particles will either cease to rotate and may become demagnetized. If the particles are still rotating, the angle will be reduced. In laminar ﬂow, with small Reynolds numbers, the viscosity of the liquid will play an important role; otherwise the general character of the phenomenon is the same as that at high Reynolds numbers [L9].

3.8. SEPARATION IN MAGNETIC FLUIDS

3.8

227

Separation in magnetic ﬂuids

The sink-and-ﬂoat technique of gravity separation relies on selective levitation and sinking of materials based on their relative densities and that of the separating medium. The scope of the sink-and-ﬂoat technique is restricted by a limited range of densities of the separating medium, the upper limit of ferrosilicon medium being approximately 3500 kg/m3 and that of Clerici solution about 4200 kg/m3 at room temperature. In the mid sixties of the last century the application of magnetic ﬂuids as a heavy medium, had been investigated, and it was established that by exposing a magnetic ﬂuid to a non-homogeneous external magnetic ﬁeld the ﬂuid exhibited an apparent density exceeding densities obtainable with conventional heavy liquids. Two broad classes of magnetic ﬂuids were investigated at that time, namely paramagnetic liquids [A1, A12, A19] and ferroﬂuids [R1, R7, R8, R16, G4, K16, F8]. Paramagnetic liquids are solutions of paramagnetic salts, such as MnCl2 and Mn(NO3 )2 . These liquids are paramagnetic in their behaviour: their magnetization increases linearly with an increasing magnetic ﬁeld and their susceptibility is low, of the order of 6×107 m3 /kg. On the other hand, a ferroﬂuid is a stable colloidal suspension of sub-domain ferromagnetic (s.l.) particles, for example magnetite, in a liquid carrier. The behaviour of ferroﬂuids is superparamagnetic, characterized by the absence of hysteresis and coercivity. Ferroﬂuids dier from paramagnets in having quite large magnetic susceptibilities and being able to become saturated in moderate magnetic ﬁelds. Saturation polarization of a ferroﬂuid can be as high as 0.1 T (1000 G) The concept of separation of non-magnetic particles suspended in a magnetic ﬂuid is based on the generalized Archimedes law whereby, in addition to the conventional force of gravity acting on the ﬂuid, also a magnetically induced force acts on the ﬂuid. This additional magnetic pull creates a magnetically induced buoyancy force on a particles immersed in the ﬂuid. This buoyancy force can be controlled in a wide range of values and materials as dense as 20 000 kg/m3 or higher can ﬂoat in such a ﬂuid. A schematic diagram of the process of separation in magnetic ﬂuids is shown in Fig. 3.52, while a general diagram of a magnetic circuit used in separation in magnetic ﬂuids in shown in Fig. 3.53. Permanent magnets or electromagnets are used to generate a non-homogeneous magnetic ﬁeld in the separation gap. The desired pattern of the magnetic ﬁeld and its gradient is achieved by shaping the pole tips. A separation chamber placed between the pole-pieces of the magnetic circuit is ﬁlled with a magnetic ﬂuid.

3.8.1

Apparent density of a magnetic ﬂuid

There are two dominant forces acting on a volume of the magnetic ﬂuid, placed in an external non-homogeneous magnetic ﬁeld, namely the force of gravity and the magnetic traction force. The situation is schematically depicted in Fig. 3.52.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

228

Ferrofluid Floating particles

Element of ferrofluid

Magnet

Fg

S Fm

N

Sinking particles

Figure 3.52: Schematic diagram of the process of separation in magnetic ﬂuids.

Figure 3.53: Schematic diagram of a magnetic circuit used in separators with magnetic ﬂuids.

3.8. SEPARATION IN MAGNETIC FLUIDS

229

The total force on the magnetic ﬂuid of volume Yi can be written as: 1 Ii = Ij + Ip = i Yi j + i Yi EuE 0

(3.140)

where i and i are the physical density and volume magnetic susceptibility, respectively, of the magnetic ﬂuid. For a ferromagnetic (s.l.) ferroﬂuid, the magnetic force can be expressed as 1 Ip = Mi Yi uE 0

(3.141)

where Mi is the magnetic polarization of the ferroﬂuid. When the ﬁeld gradient is parallel with the gravitational force and of the same sense, eqs. (3.140) and (3.141) can be rearranged, as

and

i Ii = Yi j (i + EuE) 0 j

(3.142)

Mi Ii = Yi j (i + uE) 0 j

(3.143)

The expressions in parentheses can be viewed as an apparent density d of a magnetic medium exposed to an external non-homogeneous magnetic ﬁeld: d = i +

i EuE 0 j

(3.144)

Mi uE 0 j

(3.145)

and d = i +

In a more general case, when the ﬁeld gradient makes an angle with gravity, eq. (3.145) becomes Mi d = i + uE cos (3.146) 0 j Equations (3.143) and (3.145) form the basis of ferrohydrostatic separation (FHS). In a typical case, a water-based ferroﬂuid with polarization of 0.02 T (200 G), placed in a magnetic ﬁeld of gradient of 2 T/m (200 G/cm) will exhibit an apparent density of approximately 4200 kg/m3 . Figure 3.54 illustrates the apparent density as a function of the ﬁeld gradient for two types of kerosenebased ferroﬂuid.

3.8.2

A particle suspended in a magnetic ﬂuid

A particle suspended in a magnetic ﬂuid is acted upon by several forces illustrated in Fig. 3.55. The force of gravity is given by Isj = s Ysj

(3.147)

230

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.54: The apparent density as a function of the gradient of the magnetic ﬁeld for two types of kerosene-based ferroﬂuid, of dierent densities and magnetic polarizations. while the magnetic traction force is 1 s Ys EuE Isp = 0

(3.148)

where s is the volume magnetic susceptibility of the particle. Such a particle experiences a loss of its weight as a result of two buoyancy forces acting on the particle. The ﬁrst buoyancy force is the classical Archimedes gravity-related force: Isje = i Ysj (3.149) The other force is the magnetically induced buoyancy force due to the magnetic traction force acting on the ferroﬂuid: 1 Ispe = Ys Mi uE 0

(3.150)

The net vertical force on a particle suspended in a ferroﬂuid and acted upon by a non-homogeneous magnetic ﬁeld with vertical gradient can thus be written: Is = Isj + Isp + Isje + Ispe

(3.151)

uE Ys (s E Mi ) Is = Ys (s i )j + 0

(3.152)

or, in an explicit form:

3.8. SEPARATION IN MAGNETIC FLUIDS

231

Fpd (1)

Fpmb

Fpgb Solid particle

Pool of ferrofluid Gradient of the magnetic field

Fpg Magnetic field Fpd (2) Fpm

Figure 3.55: Forces acting on a particle in a stationary ferroﬂuid, placed in a non-homogeneous magnetic ﬁeld. Deﬁning the eective cut-point density fs for separation as that particle density s for which Is = 0 (i.e. equilibrium of the forces acting on the particle), eq. (3.152) yields: uE fs = i + (3.153) (Mi s E) cos j For non-magnetic particles s = 0 and eq. (3.153) reduces to fs = i +

Mi uE cos 0 j

(3.154)

where is the angle between the vectors of the gravitational force and the ﬁeld gradient. When the force of gravity and the gradient of the magnetic ﬁeld are parallel, eq. (3.154) becomes fs = i +

Mi uE 0 j

(3.155)

which is equivalent to eq. (3.145). It can be seen that for non-magnetic particles, the density cut-point is equal to the apparent density of the ferroﬂuid. Particles whose densities s are smaller than the apparent density of the ferroﬂuid (s ? d ) will ﬂoat in ferroﬂuid, while particles with density greater than the apparent density of the ferroﬂuid (s A d ) will sink. Trajectories of sink and ﬂoat particles in a stationary ferroﬂuid placed in a non-homogeneous magnetic ﬁeld are shown in Fig. 3.56.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

232

Particles enter a pool of ferrofluid

Float particles Field gradient

Sink particles

Į Pool of ferrofluid

Figure 3.56: Trajectories of ﬂoat and sink particles in a stationary ferroﬂuid placed in a non-homogeneous magnetic ﬁeld.

Figure 3.57: The eect of hydrodynamic drag on cut-point density, for two particle velocities. The nominal "large-particle" (eq. 3.155) cut-point density fs = 3500 kg/m3 .

3.8. SEPARATION IN MAGNETIC FLUIDS

233

Figure 3.58: The inaccuracy in cut-point density introduced by ignoring hydrodynamic drag, for two dierent particle velocities. The nominal cut-point density fs = 3500 kg/m3 .

3.8.3

The eect of the hydrodynamic drag

In many applications of ferrohydrostatic separation it is legitimate to ignore the eect of the hydrodynamic drag. For small particles, however, the inﬂuence of the drag on the cut-point density can be signiﬁcant. If we assume that the Stokes law applies, the hydrodynamic drag is given by eq. (1.16). By including this drag in the expression of the total force (eq. (3.151)), the equilibrium of forces on a non-magnetic particle yields fs = i +

Mi 9y uE + 0 j 2je2

(3.156)

Equation (3.156) applies to a particle that is moving vertically downwards, i.e. the hydrodynamic drag Isg (1) acts on the particle. Such a particle is either a sink particle, i.e. a particle whose density is greater than d , or a ﬂoat particle that is temporarily moving downwards because of the non-zero initial velocity with which it entered the ﬂuid, as shown in Fig. 3.56. Once a ﬂoat particle reaches its terminal velocity (equal to zero), it will reverse the direction of its motion and will start moving upwards. At that point the opposite hydrodynamic drag Isg (2) will be acting on the particle and the particle will experience an apparent density given by d = i +

Mi 9y uE 0 j 2je2

(3.157)

234

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.59: Density increment, for paramagnetic particles, as a function of magnetic susceptibility, at three dierent values of the applied magnetic ﬁeld. uE = 2 T/m. Therefore, it becomes clear that, in general terms, the presence of the hydrodynamic drag increases the cut-point density for sinking particles, i.e. sink particles or ﬂoat particles in their initial phase of motion within the ferroﬂuid. For particles reporting to the ﬂoat fraction, however, the hydrodynamic drag decreases the cut-point density. It can be found from eq. (3.156) that for particles greater than, for example, 1 mm the hydrodynamic drag can be neglected and the cut-point density is independent of particle size, and is given by eq. (3.155). However, by inclusion of the hydrodynamic drag, the cut-point density begins to deviate, for particles smaller than 1 mm, from its "large particle value", as is illustrated in Fig. 3.57. Figure 3.58 shows the inaccuracy in the cut-point density introduced by ignoring the hydrodynamic drag.

3.8.4

The eect of particle magnetic susceptibility

A magnetic particle (s 6= 0) will exhibit an eective density hi i dierent from its natural (true) density s , as a result of its attraction (or repulsion) in the direction of the ﬁeld gradient. This eective density can be written: hi i = s +

s E uE cos 0 j

(3.158)

It can be seen that the dierence between the eective and true densities s = hi i s increases, for paramagnetic particles, with increasing magnetic

3.8. SEPARATION IN MAGNETIC FLUIDS

235

susceptibility, magnetic ﬁeld strength and the ﬁeld gradient. A relative density increment as a result of non-zero magnetic susceptibility of a particle, follows from eq. (3.158) hi i s "s E = uE (3.159) s 0 j where "s is the mass magnetic susceptibility of the particle. A typical dependence of the density increment as a function of magnetic susceptibility of paramagnetic particles is shown in Fig. 3.59. It is evident that the density increment increases with increasing magnetic susceptibility of the particle and the ﬁeld strength. This is a very important implication that aects the accuracy of separation of materials of non-zero magnetic susceptibility. On the other hand, the eective density of diamagnetic particles decreases, as a result of their negative magnetic susceptibility. In view of the low values of diamagnetic susceptibility, the density decrease is very small; at the magnetic induction of 2 T, the decrease is approximately 0.2%. For example, the eective density of quartz (" = - 6.0×109 m3 /kg) is reduced, at 2 T, from its physical density of = 2700 kg/m3 to approximately 2695 kg/m3 . The validity of eq. (3.159) has been tested using magnetic tracers, particles of constant density and of dierent values of magnetic susceptibility [R31]. Magnetic tracers, 5 mm in size, and of density 3550 kg/m3 , with mass magnetic susceptibility ranging from 2.5×107 m3 /kg (20×106 cm3 /g) to 1.25×105 m3 /kg (1000×106 cm3 /g), were separated in a ferroﬂuid the apparent density of which was varied from 3600 kg/m3 to 4200 kg/m3 . The magnetic induction to which the ferroﬂuid was exposed in the separation region was 0.2 T and the ﬁeld gradient was 1.5 T/m. Partition curves thus obtained are shown in Fig. 3.60. It can be seen that 50% of tracers with density of 3550 kg/m3 sank in a ferroﬂuid of apparent density of 3700 kg/m3 only when their susceptibility was greater than 1.25×106 m3 /kg. When the density of the ferroﬂuid was set to 4200 kg/m3 , 50% of magnetic tracers of density 3550 kg/m3 sank when their magnetic susceptibility was greater than 8.2×106 m3 /kg. This experimental observation can be compared with the theoretical prediction expressed by eq. (3.159). Using the above values of particle susceptibility, and taking into account that E = 0.2 T and uE = 1.5 T/m, the right-hand side of eq. (3.159) is equal to 0.19. This value agrees well with the relative density increment (4200 - 3550)/3550, obtained from the left-hand side of eq. (3.159).

3.8.5

Motion of particles in a ferroﬂuid

The equation of motion of non-magnetic particles The equations of motion of a non-magnetic particle suspended in a stationary ferroﬂuid, as depicted in Fig. 3.61, can be expressed [M18] as: gy{ 1 g2 { { { = (I { + Isp + Isg ) = gw2 gw s Ys se

(3.160)

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

236

Figure 3.60: The partition curves for magnetic tracers of density 3550 kg/m3 , as a function of their mass magnetic susceptibility, separated in a ferroﬂuid of dierent apparent densities [R31]. z h

Fzpmb, Fpgb

v0

Fpmb

grad B x

F

pmb

į

Fpg,

Į

x

Figure 3.61: Section through a pool of ferroﬂuid of depth , inclined at an angle =

3.8. SEPARATION IN MAGNETIC FLUIDS gy} g2 } 1 } } = (I } + Isg + Isp Ij ) = 2 gw gw s Ys se

237 (3.161)

These equations can be re-written gy{ + Ny{ = Z gw

(3.162)

gy} + Ny} = Z 0 gw

(3.163)

where parameters N> Z and Z 0 have the following forms: N=

d i d cos s + 2i sin2 (@2) 6e >Z = j sin > Z 0 = j (3.164) s Ys s s

The initial conditions for eqs. (3.162) and (3.163) are: for w = 0 y{ = 0 and y} = y0

(3.165)

The initial velocitys of a particle that is being dropped into the ferroﬂuid from height k is y0 = 2jk. Dierential equations (3.162) and (3.163) can be solved analytically and the solutions are [M18]: g{ Z (3.166) = y{ = (1 hNw ) gw N Z” g} = y} = y0 hNw + (1 hNw ) gw N

(3.167)

The initial conditions for eqs. (3.166) and (3.167) are for w = 0 { = 0 and } =

(3.168)

Equations (3.166) and (3.167), with these initial conditions, yield the following solutions: Z Z (3.169) w 2 (1 hNw ) {= N N } =+(

Z0 y0 Z ” 2 )(1 hNw ) + w N N N

(3.170)

Particle trajectories can be obtained from these parametric equations by calculating pairs of coordinates ({> }). Typical trajectories of non-magnetic particles of dierent densities are shown in Fig. 3.62. It can be seen that when k = 0 then y0 = 0 and the trajectory of a particle is a straight line.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

238

z (cm)

10 3300 3400

5

3500 3600

x (cm)

0 0

5

10

15

20

-5

Figure 3.62: Trajectories of non-magnetic particles of various densities: d = 3500 kg/m3 , k = 3 mm, i = 990 kg/m3 , = 1.65×103 Pa×s, = 20 . The straight dashed lines are trajectories of particles of densities of 3500 kg/m3 and 3550 kg/m3 for k = 0 (adapted from [M18]).

z (cm)

10

0

5

40 60 70

0 0

5

10

15

x (cm) -5

Figure 3.63: Trajectories of magnetic particles of various mass magnetic susceptibilities (×108 m3 /kg): d = 3500 kg/m3 , s = 3300 kg/m3 (adapted from [M18]).

3.8. SEPARATION IN MAGNETIC FLUIDS Repulsion

Attraction

N

N

239

S

S

N

S

N

Particle

Magnetic fluid

S

Magnet

Figure 3.64: Interaction between non-magnetic particles in a magnetized magnetic ﬂuid (adapted from Fujita et al. [F14]). The equation of motion of a magnetic particle As has been discussed in Section 3.8.4, a magnetic particle suspended in a ferroﬂuid placed in a non-homogeneous magnetic ﬁeld will exhibit an eective density hi i (given by eq. (3.158)) dierent from its natural density. Trajectories of magnetic particles can be obtained by replacing the natural density s of the particles by eective density. As a result of the non-uniformity of the magnetic ﬁeld, the eective density is dierent at dierent positions of the particle along the vertical axis, being the greatest where the pole tips of the magnet are closest to one another, as shown in Fig. 3.52. The mean eective density can be calculated, for example, by replacing E in eq. (3.158) with the mean magnetic induction Emean = Emin + Emax . In this situation the equations of motion remain the same as parametric equations (3.169) and (3.170). Typical trajectories of magnetic particles are shown in Fig. 3.63. Interaction of particles during separation The analysis of the particle motion in a ferroﬂuid assumed that particles were non-interacting. This simpliﬁcation ignores, however, the fact that non-magnetic particles suspended in a magnetic ﬂuid possess surface magnetic charges as a result of magnetization of the surrounding ﬂuid. Fujita and Mamiya [F14] determined, theoretically and experimentally, that non-magnetic particles, placed in a magnetized ferroﬂuid, attracted one another in the direction parallel to the direction of magnetic ﬁeld and repelled one another in the perpendicular direction. The situation is depicted in Fig. 3.64. The attractive force increases with increasing density of the ferroﬂuid and magnetic ﬁeld strength. The attractive interaction was found to reduce the selectivity of separation of non-magnetic particles in a magnetic ﬂuid.

240

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Magnet

Fpm

Fpmb

N Fpc

Fg

Fpd

Rotating ferrofluid

Figure 3.65: Forces acting on a particle in a rotating ferroﬂuid in a nonhomogeneous external magnetic ﬁeld.

3.8.6

Separation in a rotating ferroﬂuid

In order to overcome certain practical limitations of gravity-based ferrohydrostatic separation, particularly treatment of ﬁne particles, several proposals were made [R11, A14, W7] to replace the force of gravity by the centrifugal force. Work carried out at Intermagnetic Corp.(USA) in early nineteen eighties resulted in a new rotation-based separation process called Magstream. The theory and the practice of separation in a rotating ferroﬂuid have been described in several publications [W20, W21, W22, B22, B23, S44]. Forces acting on a particle suspended in a rotating ferroﬂuid exposed to a non-homogeneous magnetic ﬁeld are illustrated in Fig. 3.65. Walker and Devernoe [W22] assumed that the axis of the separator was vertical and ignored the force of gravity and the hydrodynamic drag acting on the particle. In this scenario only the radially outward centrifugal force Isf , magnetic traction force Isp and the inward buoyancy force Ispe resulting from the outward attraction of the magnetic ﬂuid by the magnetic ﬁeld were included. The centrifugal force can be written Isf = Ys (s i )$ 2 u

(3.171)

where u is the radial position of the particle and $ is the rotational velocity of the ferroﬂuid. The magnetic buoyancy force is given by eq. (3.150) while the magnetic traction force is given by eq. (3.148). The total force Isu acting on a particle in the horizontal direction, along the

3.8. SEPARATION IN MAGNETIC FLUIDS

241

radius of the rotating device, can be expressed as: Isu = Ys (s i )$ 2 u +

1 1 s Ys EuE Ys Mi uE 0 0

(3.172)

In equilibrium Isu = 0 and the cut-point density for non-magnetic particles (s = 0) can be determined from the above equation as: µ fs = i +

N Q

¶2 Mi uE

(3.173)

where Q is the number of revolutions of the rotating device per minute (Q = 60$/2), and N is a parameter determined by the design of the magnetic system of the rotating separator: µ N = 15

1 107 3 u

¶[email protected] (3.174)

Equation (3.173) is used to calculate the operating conditions in the Magstream separator [W22]. It is apparent from eqs. (3.173) and (3.174) that if the pattern of the magnetic ﬁeld is designed in such a way that the ﬁeld gradient is a linear function of the radial position u, then N = const. and the cut-point density is determined solely by the polarization and the rotational velocity of the ferroﬂuid. This condition is satisﬁed, for instance, for the magnetic ﬁeld generated by a sextupole magnet, such that the ﬁeld magnitude is given by E = E0 ([email protected] )q1 , where 2q = 6, and E0 is the magnetic induction at u0 , the outside wall of the separation annulus [W20]. Equation (3.173) is equivalent to eq. (3.154) derived for ferrohydrostatic separation. It can, therefore, be seen that the cut-point density in a rotating ferroﬂuid can be controlled, in a wide range, by varying the rotational velocity and the ﬁeld gradient. The operating density range of the ﬂuid in a ferrohydrostatic separator is, in contrast, controlled by adjusting the ﬁeld gradient only. However, in most Magstream models the magnetic ﬁeld is generated by permanent magnets and the ﬁeld gradient is given by the design of the magnetic system. For instance, in Magstream Model 200 the ﬁeld gradient is equal to uE = 13.2u T/m (1320u G/cm). Simplifying assumptions introduced by Walker and Devernoe [W22], when deriving eq. (3.173), reﬂect themselves in limited accuracy of determination of the cut-point density and thus in reduced e!ciency of separation. Bunge and Fuerstenau [B22], in order to account for the dispersion component of particle behaviour, developed a diusion model of separation. They concluded that the primary cause of non-ideal separation in a rotating ferroﬂuid is the dispersion of the settling particles. This fuzzy behaviour was ascribed to the eect of turbulence, particle shape and interparticle interactions. The model of Bunge and Fuerstenau, however, was not able to explain the dependence of the separation e!ciency on particle size and ﬂuid viscosity [B22, B23].

242

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.66: The cut-point density of non-magnetic particles in Magstream, as a function of density. u = 2.1 cm, = 5×103 Pa×s, fs (no drag) = 3130 kg/m3 (adapted from [S44]).

Svoboda [S44] included the horizontal hydrodynamic drag (eq. (1.16)) into the balance of forces and obtained, for the cut-point density,

fs = i +

1 Mi s 9ys E)uE + 2 2 ( 2 $ u 0 0 2$ e u

(3.175)

This more general expression shows that the hydrodynamic interaction of particles with the ferroﬂuid contributes to the determination of the cut-point density. The most signiﬁcant consequence of the hydrodynamic contribution is that the cut-point density depends on particle size, in contrast to eq. (3.173). It transpires from eq. (3.175) that the correction hydrodynamic term gains importance for weakly magnetic and/or highly viscous ferroﬂuids (low Mi and high ), and for small particles. In addition, the hydrodynamic term depends on the position of a particle within the separation space. The eect of particle size on the cut-point density of non-magnetic particles is illustrated in Fig. 3.66. It can be seen, for example, that a cut-point density of 3130 kg/m3 , determined by ignoring the hydrodynamic drag, is accurate down to particle size of 2 mm. For particle diameters smaller than 2 mm the relative importance of the hydrodynamic interaction steeply increases and separation becomes inaccurate.

3.9. EDDY-CURRENT SEPARATION

3.9

243

Eddy-current separation

It has been stated in Section 2.7 that when conducting particles move through a region of spatially varying magnetic ﬁeld, then an electromagnetic force, and hence eddy currents, are induced in such particles. The eddy currents are caused by time-dependent changes of the magnetic induction acting on a particle and are given by the Faraday induction law: × m = s C E u Cw

(3.176)

where m is the current density and s is the speciﬁc electrical conductivity of the particle. These eddy currents generate a magnetic ﬁeld opposed to the external magnetic ﬁeld. This opposite ﬁeld then produces a repulsive Lorentz force on a linear element gv of the conductor [S47] IO = Lgv × E

(3.177)

where L is the current carried by the conductor. This force can be made lateral to the motion of the particles and so to deﬂect them. Negligible eddy currents develop in non-conducting elements, which, therefore, experience no deﬂection. In this way it is possible to separate conducting particles from non-conducting and this method has been developed into an e!cient technique for the recovery of non-ferrous metals from streams of industrial or municipal waste. The varying magnetic ﬁelds can be generated in several ways. In linear motors, the magnetic ﬁelds are generated by electromagnets with alternating currents. The repulsive force can also be generated by moving particles through a non-homogeneous static or rotating magnetic ﬁelds. These ﬁelds can be conveniently generated by permanent magnets.

3.9.1

Static ramp eddy-current separator.

The simplest design of an eddy-current separator (ECS) proposed by Schloemann [S45] comprises a long ramp, as shown in Fig. 3.67. The ramp consists of permanent magnet strips of alternating polarity, mounted on a mild steel base plate inclined at an angle of about 450 to the ramp axis. A stream of particles is allowed to slide down the ramp. The non-conducting particles are not aected by the magnetic ﬁeld and travel straight down the ramp. The conducting particles, under the inﬂuence of the eddy-current-induced repulsive Lorentz force perpendicular to the magnet strips, are deﬂected from the stream of non-conducting particles, as shown in Fig. 3.67. The magnitude of the lateral deﬂection depends, among other things, on the electrical conductivity, density, size and shape of the particles and the strength and the periodicity of the magnetic ﬁeld.

244

CHAPTER 3. THEORY OF MAGNETIC SEPARATION Feed

Y

+ -

Magnet strips of alternating polarity

+ + -

Z

Mild steel base

ș

X Conducting particles

Non-conducting particles

Figure 3.67: Schematic diagram of a ramp eddy-current separator (adapted from Schloemann [S45]). Schloemann [S45] found that the component of the repulsive force in |direction acting on a conducting particle is given by: | IOs = ps y{

(3.178)

where ps and y{ are the mass and velocity in the { - direction of the particle, respectively. The coe!cient is a function of particle shape, and for a thin disc of diameter gs , it is given by [S45]: =

1 2 s CE} 2 ( g ) 32 s s C{

(3.179)

and approximate expression for the repulsive force (eq. (2.6)) is quoted by Schubert [S22]: s gs 2 | IOs ' ps (3.180) E y{ s 2i where i is the period of the magnetic ﬁeld. This equation, supported by additional calculations of the repulsive force on particles of various shapes [S46, V3, V4] shows that the repulsion force is a function of the material parameter s @s , given in Table 2.1, and of the square of the magnetic induction. Schloemann [S45] calculated trajectories of disc-shaped particles in a ramp eddy-current separator from the following equations of motion: gy{ gy| = j sin and = y{ gw gw

(3.181)

3.9. EDDY-CURRENT SEPARATION

245

It follows from eqs. (3.181) that {(w) =

1 2 w j sin + y0 w 2

1 1 |(w) = ( w3 j sin + y0 w2 ) 6 2 where y{ (0) = y0 . The particle trajectory, in a frictionless situation, is then: s ·³ ³ { ´[email protected] ¸ 2 {0 ´ ³ {[email protected] {0 ´[email protected] 0 |({) = + 2 1 2 1 + 3 (j sin )[email protected] { { {

(3.182) (3.183)

(3.184)

where {0 is the distance along the ramp after which a particle starting at rest has attained the velocity y0 = Therefore, {0 = y02 @2j sin . A more detailed analysis of the eect of friction on particle motion can be found in [S45]. Although ramp eddy-current separators were used in several industrial installations [S46], their commercial success was limited. Poor selectivity, particularly for small particles, and low throughput were responsible for the failure of ramp separators to ﬁnd a long-term production application. Further development of the ramp concept resulted in the design of a vertical eddy-current separator [V4, V3], in which the deﬂection occurred in a vertical channel between two arrays of magnet strips mounted on the inside of two vertical parallel mild steel plates. The strips of alternating polarity were also oriented at an angle to the base plate and, in addition, the magnets on the opposite plate were also arranged with opposite polarity. These static gravitybased separators also failed to gain industrial acceptance and were replaced by dynamic rotating drum eddy-current separators. A detailed study of the separating Lorentz force, by eliminating the competing forces such as gravity and frictional forces, was conducted theoretically by Fletcher et al. [F15, F16, F17]. These idealized physical models of separation of conducting and non-conducting elements moving in a horizontal plane and incident on a single boundary of a semi-inﬁnite magnetic ﬁeld were compared with the experimental results. Theoretical trends of the metal recovery with particle size, splitter position and boundary ﬁeld proﬁle were in good agreement with experimental observations. Although the ﬁeld geometry and the separation arrangement in these studies diered from those used in practical applications, the methodology used can serve as a starting point for more fundamental research into the mechanisms of eddy-current separation.

3.9.2

Rotating drum eddy-current separators

Presently, the eddy-current separators most frequently used in industrial practice are based on a rotating drum concept. The active part of such a separator is a drum containing rapidly rotating magnetic system. Permanent magnets are arranged, with alternating polarity, along the circumference of the magnetic system. This concept is schematically described in Figs. 2.100 and 3.68.

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

246

Drum rotation Eddy current S

Belt

N

Particle S

N

S

Lorentz force N S

N Particle

Figure 3.68: A top view of an eddy-current separator based on a rotating drum. The particles are expelled by the Lorentz force in the direction of the direction of drum rotation (adapted from [R17]). In order to calculate the forces acting on particles due to eddy current, a dipole model was developed by Rem et al. [R17, R18]. It was assumed that the magnetic ﬁeld induces eddy currents within a particle, which in turn generate a magnetic moment in that particle. The interaction between the magnetic moment P and the external magnetic ﬁeld E results in eddy current forces. The force can then be expressed as: IOs = P uE

(3.185)

where P = Ps Ys . The torque on the particle is given by eq. (3.48). In order to determine the force acting on a particle, given by eq. (3.185), a magnetic ﬁeld generated by the magnetic system must be calculated. Rem et al. [R17] have shown that the components of the magnetic induction in the cylindrical coordinate system (u> !> }) relative to the drum axis can be written: Eu =

4 X

eq ([email protected] )(2q+1)n1 sin[(2q + 1)n(! $ guxp w)]

(3.186)

eq ([email protected] )(2q+1)n1 cos[(2q + 1)n(! $ guxp w)]

(3.187)

q=0

E! =

4 X q=0

where eq are the Fourier coe!cients, Uguxp the radius of the drum, n the number of pairs of the magnets used in the drum and $ guxp the angular velocity of the drum. The Fourier coe!cients can be determined by measuring the magnetic ﬁeld strength as a function of distance from the magnetic pole surface. Based on eqs. (3.186) and (3.187), Zhang et al. [Z4] obtained the following expressions for the tangential Isw and radial Isu eddy-current forces acting on the particle: (n$ guxp + ) 2vYs E2 (3.188) IOsw = 0 z 1 + (n$ guxp + )2 2

3.9. EDDY-CURRENT SEPARATION IOsu =

2vYs (n$ guxp + )2 2 E2 0 z 1 + (n$ guxp + )2 2

247 (3.189)

where z is the width of one pair of magnets, v is the shape factor of the particle and is the angular velocity of particle rotation. is a characteristic time with which the induced magnetic ﬁeld decays in the particle given by [Z4]: = 0 s ve2

(3.190)

where e is the particle radius. The torque on the particle was found to be [Z4]: W =

vYs (n$ guxp + ) E2 0 1 + (n$ guxp + )2 2

(3.191)

It can be seen that the eddy-current forces and the torque depend on the square of the magnetic ﬁeld strength. By replacing ceramic ferrite permanent magnets by rare-earth magnets, a considerable increase in the separating force can be, therefore, achieved. Competing forces Gravitational, centrifugal, frictional and aerodynamic forces compete with eddycurrent forces and their relationship determines the particle trajectories in an eddy-current separator. Eddy current forces and a wide spectrum of competing forces and their various dependencies on particle size and shape, electrical conductivity, magnetic ﬁeld strength and its frequency (or the angular velocity of the rotating drum) make the determination of particle trajectories and thus the e!ciency of separation a problem of considerable complexity. Only rudimentary eorts have been made the develop the balance of forces in a rotating drum eddy-current separator [Z4, R17, R18]. Rem et al. [R18] developed a model for simulation of such a rotating drum ECS. The eddy-current forces and some of the competing forces were included in the model and particle trajectories were calculated. Typical trajectories, shown in Figs. 3.69 and 3.70, comprise the rolling, sliding and ﬁnally ﬂying stages. It can be seen that at low belt velocities (Fig. 3.70) light particles tend to lose contact with the belt at an early stage and they collide with the belt at a later stage. As a result of the dependence of the eddy-current forces and other forces on the cube of the particle size, the particle size is the most signiﬁcant variable aecting the performance of a separator. It transpires from the above equations that also the particle shape plays an important role in the separation process. For instance, it was observed that ﬂat particles exhibit much greater displacement by eddy-current forces than spherical particles. In spite of considerable complexity of the process, some general rules that govern the e!ciency of separation in a drum ECS can be formulated. In order to achieve a high recovery of conducting particles, the eddy-current separating force must be greater than

248

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Figure 3.69: Particle trajectories in a rotating drum ECS. Three stages of particle motion, namely rolling, sliding and ﬂying are apparent. Operating conditions: belt speed: 1.5 m/s, drum angular velocity: 35 s1 , material: aluminium particles 15 mm in diameter, 45 mm long (courtesy of P.C. Rem).

Figure 3.70: Particle trajectories in a rotating drum ECS, at low belt velocity. Belt speed: 0.5 m/s, drum angular velocity: 35 s1 , material: aluminium particles of diameter of 10 mm, 2 mm thick (courtesy of P.C. Rem).

3.9. EDDY-CURRENT SEPARATION

249

Figure 3.71: Frequencies required to rotate metal particles of various diameters (adapted from Allen [A21]). the sum of the competing forces: Ivhsdu A Ifrps

(3.192)

If, however, Ivhsdu AA Ifrp , selectivity of separation will be low, as no distinction will be made between various classes of conducting particles. Selective separation of one metal from another is determined by the interplay between corresponding eddy-current and competing forces. Selective separation of metal (1) from metal (2) will be achieved when the following relationship is met: (1) (2) Ivhsdu A Ifrps A Ivhsdu

(3.193)

However, when Ivhsdu ? Ifrps , no separation based on the characteristic property, such as electrical conductivity in ECS, will take place.

3.9.3

Eddy-current separation by particle rotation

With decreasing particle size, the torque on the particle become an important separating force. Also, when the particle size becomes much smaller than the width of the magnet strips used in the rotating drum eddy-current separators, the particles increasingly respond to the ﬁeld changes by rotation rather than by repulsion [A21]. As a result of decrease in the particle throw and increase of particle rotation as particle size decreases, Allen [A21, A22] proposed to use particle rotation as the separating mechanism of conducting particles.

250

CHAPTER 3. THEORY OF MAGNETIC SEPARATION

Allen found that the magnitude of the torque acting on a cubic conducting particle by a rotating ﬁeld is Wf =

E 2 O5 z 8(s

(3.194)

where O is the length of the cube edge, z is the magnetic ﬁeld rotation frequency and (s is the resistivity of the material. For a sphere of diameter gs , the torque is given by E 2 g5s z (3.195) Wf = 60(s If such a torque is exerted on a particle by a rotating magnetic ﬁeld, and the particle is resting on a surface, the particle will be rolled when the torque becomes greater than the gravitational force holding the particle against the surface. The gravitational torque preventing a cubic-shaped particle from rolling can be written: O4 Wj = (3.196) j 2 s Combining eqs. (3.195) and (3.196) an estimate of the minimum size of a cubic particle that could be rolled at a given magnetic ﬁeld strength is obtained [A21]: Omin =

4s (s j E 2 z

(3.197)

Equation (3.197) gives a reasonable estimate of the minimum size of a ”rollable” cubic particle when the rotating magnetic ﬁeld has its rotation axis at the centre of the particle. In a more practical situation of a rotating drum eddy-current separator, the magnetic ﬁeld not only rotates the particle, but it is also moving through the particle. This moving ﬁeld produces a ﬁeld which rotates in the opposite direction, at half the ﬁeld rotation frequency [A21]. The minimum ”rollable” cubic particle size, ignoring inter-particle interactions, can, therefore, be estimated as 8s (s j Omin = (3.198) E 2 z The rotating frequencies of the magnetic ﬁeld, required to rotate and thus to separate particles of various metals and various sizes in a magnetic ﬁeld of 0.45 T, are shown in Fig. 3.71 [A21]. It can be seen, for example, that particles of gold, as small as 60 m, could be separated by rotating them at the frequency of 1000 s1 = The concept has been demonstrated by separating aluminium particles from their mixture with sand, with the recovery of 86% and the concentrate grade of 95 % Al, at the feed rate of 5 t/h/m [A17].

Chapter 4

Elements of Design of Magnetic Separation Equipment 4.1

Introduction

The design of a magnetic circuit for a magnetic separator is based on the need to optimize the magnetic force required to separate e!ciently, and selectively, particles of dierent magnetic susceptibilities. As transpires from eq. (1.8), the magnetic force is the product of the magnetic ﬁeld strength and of the ﬁeld gradient. The desired magnetic ﬁeld strength, the ﬁeld gradient and their combination are a function of the type of material to be separated, mode of separation, required metallurgical performance and economic criteria. In this chapter the basic design criteria and techniques of the generation of the magnetic ﬁeld and its gradient, as used in magnetic separation, will be reviewed. Magnetic circuit design has been traditionally di!cult because of the usual non-analytic nature of the solutions for ﬁelds emanating from arbitrary sources. Further, unlike currents in electric circuits, magnetic ﬂux is not conﬁned to the wires but passes through various components of the circuit, including the air. Over the years, several analytical techniques have been used to give approximate solutions to magnetic design problems. In the simplest cases, the analytical solution can be exact, but in general for any practical problem, analytical solutions lead to large errors. Most designs are optimized by measurement and extrapolation, and experience of working with a particular type of a magnetic circuit is important. The advent of powerful computational techniques, such as ﬁnite element analysis, allows us to ﬁnd accurate solutions for two- or three-dimensional ﬁeld distributions in complex geometries, which in turn may be used to predict device performance with similar precision. However, these modelling techniques 251

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

252

require a detailed deﬁnition of the geometry and boundary conditions to be solved, which assumes that an initial design already exists. While providing an accurate ﬁeld solution for a given geometry, these techniques will not optimize it. Suggestions for changes in dimensions, materials etc. must come from the designer. Consequently, while computer-based ﬁeld analysis is an eective tool for simulating a known device, it is too cumbersome for design optimization [C16]. Field equations Calculation of the ﬂux in a magnetic circuit is based on two Maxwell’s equations. The ﬁrst, in its dierential form is: ×K = m u

(4.1)

where m is the current density. After integrating over an arbitrary surface V we obtain the above equation in the integral form: Z Z × K) · gd = m · gd (4.2) (u V

V

Then, using Stokes’s theorem, the left-hand side of this equation can be transformed into a line integral around a closed path F, which bounds the surface V, and I Z (4.3) K · go = m · gd = L F

V

where L is the total current. This is Ampere’s circuital law: the line integral of K around a closed path is equal to the total current crossing any surface bounded by the line integral path. The left-hand side of eq. (4.3) is known as magnetomotive force or ppi . The second fundamental relationship required for a magnetic circuit design expresses the fact that ﬂux must be conserved through any closed volume, or, that the total ﬂux ﬂowing out of any volume must be zero. Therefore Z · gd = 0 or u ·E =0 E (4.4) V

Equations (4.3) and (4.4) are two basic equations used for magnetic circuit design.

4.2 4.2.1

Design of circuits with permanent magnets Basic concepts and ﬁgures of merit

The general relationship between magnetic induction and intrinsic material magnetization or polarization is given by = 0 (K +P ) = 0 K + M E

(4.5)

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS B

253

B

Jr,Br

(BH)max

BH

Hc

H Hci i

(BH) max

(BH)max

Figure 4.1: The maximum energy products of permanent magnets. The relationship between E and K is illustrated by the hysteresis curve shown in Fig. 1.7. The second (demagnetization) quadrant of such a hysteresis curve is important for description of the quality of a permanent magnet material. Relative contributions of M and K greatly inﬂuence the magnetizing, demagnetizing and stability properties of permanent magnets. For instance, the coercive force Kf can never exceed the remanent magnetic induction Eu : 0 Kf Eu

(4.6)

while the intrinsic coercive force Kfl is not under such a restraint. There is clearly one point between Eu and Kf for which the product of E and K has a maximum value. The optimum operation of a magnet corresponds to conditions under which this EK product is maximum. This maximum value of the energy product is given by (EK)lim max =

Mv2 P2 = 0 v 4r 4

(4.7)

where Mv (or Pv ) is the saturation polarization (or magnetization) of the magnet material. It transpires from this equation that, in order to establish the maximum capability of a permanent magnet, one has to know only the value of the saturation polarization. The maximum value of the energy product corresponds to the largest rectangle which can be drawn under the demagnetization curve corresponding to the magnetic induction, as shown in Fig. 4.1. Another important ﬁgure of merit is the intrinsic energy product (EK)lmax . This quantity is of importance when the magnet is subjected to large demagnetizing inﬂuences in its operating environment. The maximum intrinsic energy product corresponds to the largest rectangle that can be drawn under the demagnetization curve

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

254

Table 4.1: Relative permeabilities of permanent magnet materials. Material Alnico 6 Ferrimag 5 NdFeB

Permeability 4.2 1.06 1.08 - 1.1

µ1

N Alnico

µ2

S

µ2>>µ1

S

N Ferrite or NdFeB

µ2 ≅ µ1

Figure 4.2: Flux leakage in two dierent types of permanent magnets.

corresponding to the material polarization. The situation is depicted again in Fig. 4.1. Dierent types of permanent magnets can dier considerably in their magnetic behaviour. For instance, the two energy products of an Alnico magnet are very similar, namely (EK)lmax = (EK)max , while for ferrite and rare-earth magnets (EK)lmax AA (EK)max = The permeability of Alnico magnets diers considerably from that of the air, namely pdwhuldo A dlu , while for ferrite and rare earth magnets these permeabilities are similar, so that pdwhuldo = dlu . Typical values of magnetic permeabilities are shown in Table 4.1. As a result of the above dierences, the patterns of the magnetic ﬂux around a magnet also dier. As is shown in Fig. 4.2, the ﬂux lines in Alnico magnets leave the magnet limb perpendicularly, since the poles of the magnet are not at the terminals, but appear to be spaced at about 0.7 of the length of the bar [P4]. On the other hand, in ferrite and rare-earth magnets the ﬂux lines tend to reach the terminal and the pole spacing is, therefore, the full length of the bar. In a long bar of Alnico 5, only 45% of the lines in the neutral section of the magnet reach the end of the bar. Therefore, a high percentage of the total energy is

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

Ag

255

Iron pole-pieces

Lg

Lm

Am

Permanent magnet

Figure 4.3: Magnetic circuit with a permanent magnet. stored in leakage ﬁelds. On the other hand, in a ferrite bar approximately 95% of the ﬂux at the neutral section reaches the end of the magnet. These magnets, therefore, store most of their energy within their volume and their useful energy approaches (EK)max [P4].

4.2.2

The static gap design

In a circuit with permanent magnets there are no currents, L = 0, and eq. (4.3) reduces to I · go = 0 K (4.8) In a simple magnetic circuit of Fig. 4.3, with a permanent magnet and an air gap, under static conditions, in which the dimensions of the air gap are constant, eq. (4.8) can be re—written Z Z · go + · go = 0 K K (4.9) jds

pdjqhw

Therefore, the sum of the magnetomotive force (mmf) in the magnet and the magnetomotive force in the air gap equals zero: Kj Oj + Kp Op = 0 or Kj Oj = Kp Op

(4.10)

assuming that the soft-iron parts have inﬁnite magnetic permeability. Also, because the ﬂux is continuous Ej Dj = Ep Dp

(4.11)

256

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

In the above equations Oj , Dj and Ej are the length, cross-sectional area and the magnetic induction of the air gap, respectively, while Op , Dp and Ep are the length, cross-sectional area and magnetic induction of the magnet. It can be seen from eq. (4.9) that the magnetomotive force inside the magnet is in the opposite direction to the magnetomotive force in the air gap. Permanent magnets thus operate in the top left-hand quadrant (demagnetization quadrant) of the hysteresis curve. By multiplying eq. (4.10) by eq. (4.11) we get Kj Ej Yj = Kp Ep Yp

(4.12)

where Yj and Yp are the volumes of the gap and magnet, respectively. This equation can be re-written as 1 2 E Yj = Kp Ep Yp 0 j

(4.13)

These equations illustrate that the larger the product Kp Ep and/or the volume of the magnet, the greater the magnetic induction in the air gap. It is also possible to determine, from the above equation, the volume of the magnet required to generate a desired ﬂux density in a given air gap: Yp =

Ej2 Yj 0 Kp Ep

(4.14)

By combining eqs. (4.12) and (4.13) we can also write Ep Dj Op Op = 0 = Sj Kp Dp Oj Dp

(4.15)

where Sj = 0 Dj @Oj is the so-called permeance of the air gap, while the permeance of the magnet can be deﬁned as Sp = 0 Dp @Op . Permeance is a measure of magnetic conductance which, if known, enables an accurate prediction to be made concerning how much of the total ﬂux of a magnet will reach the air gap. The reciprocal of permeance is called reluctance, = [email protected] . It can be seen from eq. (4.15) that by increasing the air-gap area and/or reducing the air gap length the ease with which ﬂux travels across this gap will increase. Equation (4.15) can be plotted as a straight line with a negative slope on a demagnetization curve. The intersection of this so-called load line with the demagnetization curve represents the operating point of the magnet, as shown in Fig. 4.4. The slope of the load line is equal to 0 Dj Op @Dp Oj = For a very small air gap, in the limit Oj $ 0> the magnet is short-circuited and Ep @0 Kp $ 4> as shown in Fig. 4.4. In the opposite case, if the soft iron pole pieces are removed and the magnet stands alone, the air gap becomes large and the magnet operates in the open circuit regime. The optimum operation of the magnet is obtained when the working point on the demagnetization curve corresponds to the maximum value of the product (EK), as illustrated in Fig. 4.1.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

Load line

257

Bm

Operating point

Open circuit

Hm Figure 4.4: The load lines of permanent magnets operating in dierent regimes.

4.2.3

Leakage factors

In all practical situations the pole pieces will have ﬁnite magnetic permeability and even more importantly, there will be a considerable leakage of the magnetic ﬂux. Allowance for these imperfections can be made by introducing correction factors N1 (leakage coe!cient) and N2 (loss factor) [P4]: N1 =

Total ﬂux in circuit Useful ﬂux + Leakage ﬂux = Useful ﬂux Useful ﬂux N2 =

magnet mmf useful mmf

(4.16)

(4.17)

The equation for the load line then becomes N1 Dj Op Ep = 0 Kp N2 Dp Oj

(4.18)

It is of interest to note that the Ep @Kp ratio is entirely determined by the physical relationships between the permanent magnet and the entire magnetic circuit within which it functions. This ratio is independent of the material from which the magnet is made. Although the correction factor N1 is rarely smaller than 2 and has no upper limit, for reasonably e!cient permanent magnets it is in the range from 2 to 3. The loss factor N2 is generally much smaller than N1 , usually within the range 1.05 to 1.45 [H18].

258

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Dynamic operation If the magnetic circuit geometry does not remain unaltered, then the load line slope in eq. (4.18) will change through any of the parameters Oj , Dj , N1 and N2 = The operating point of the magnet may undergo an excursion within the short and open-circuit limits shown in Fig. 4.4. A portion of the ﬂux changes from the leakage paths to the useful paths and back again, as the useful permeance is changed. The operation of a lifting magnet is a typical situation in which the magnetic system undergoes dynamic changes.

4.2.4

Determination of permeance and leakage factors

The primary requirement for magnetic circuit design, and therefore the design of the basic magnet used in the circuit, is to be able to calculate the relationships between ﬂux paths. As pointed out in the previous section, the easiest approach to such calculations is by means of permeances. In general, the permeance of the ﬂux paths varies from a minimum near the neutral section of the magnet to a maximum for zones at the end of the magnet or close to the air gap. Relatively simple formulae for various circuit geometries are available in the literature [T6, P4, M19, H18, M20]. Adding the gap and leakage permeances using these relationships is one of the methods of estimating the total permeance. For instance, permeance of the air gap between rectangular surfaces of width d and thickness e (Fig. 4.5) is given by S =

0 de Oj

(4.19)

This equation is a special case of a more general expression S =

0 Dj Oj

(4.20)

which is valid for any shape of the air gap. The leakage permeance of the geometry shown in Fig. 4.5 is given by an approximate formula [H18] S =

0 d 2e + 1) ln( Oj

(4.21)

In order to demonstrate the di!culties facing a designer, Parker and Studders [P12] quote, for the same geometry, another formula that leads to values of S about 20% to 30% higher. For a bar magnet that operates in the open-circuit mode, the permeance is the permeance from one limb of the magnet to the other, since there are no pole pieces or a well-deﬁned air gap. Permeance of such magnets, of various shapes such as bars, rods and rings, is s S = 1=77 D (4.22)

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

259

a

Lg

b

Figure 4.5: Geometry of a magnetic circuit for calculation of the leakage permeance. where D is the cross-sectional area of the pole. This relationship is applicable to ferrite and rare-earth magnets, while for Alnico magnets the relation is s (4.23) S = 1=77 × 0=7 D This equation takes into account the fact that for Alnicos the eective spacing of the poles is only 0.7 of the total length, as shown in Section 4.2.1. It is clear that the calculation of individual permeances is very laborious and various empirical formulae have been developed for the determination of the total leakage. A very simple example of such a formula [H18] is an expression for the leakage factor N1 for a gap of length Oj between circular pole-pieces of diameter g : 7Oj N1 = 1 + (4.24) g Comprehensive sets of formulae, usually attributed to Tenzer [e.g. T6], are available in the literature [e.g. H18]. For instance, in a magnetic circuit shown in Fig. 4.6, in which the permanent magnet material is adjacent to the gap, leakage from the sides and base, which are at the same potential, can be ignored. The correction factor N1 is then given by [H18, M19]: N1 = 1 +

0=67d Oj Oj (1=1Xd )(1 + ) Dj 0=67d + Oj d

(4.25)

where Xd is the perimeter of a part shown as length d= Similar equations are available for other geometries [H18, M19].

4.2.5

Magnetic ﬁeld around a permanent magnet

The distribution of the magnetic induction at various points of magnets operating in the open-circuit regime is shown in Fig. 4.7 and Table 4.2. The long thin bar is magnetized along its long axis while the thin disc is magnetized along its short axis. The sphere is magnetized along its diameter. It is of interest to

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

260

Permanent magnet

Ag

Lg

a

Mild steel yoke

Figure 4.6: A permanent magnet circuit for the calculation of the leakage coefﬁcient.

note that a thin disc magnetized through its thickness produces no magnetic ﬂux density although the magnetic ﬁeld strength K at point C is equal to [email protected]0 . Calculation of the magnetic ﬁeld around a permanent magnet can be performed either using the pole concept or the surface current models. In the former approach a magnet is treated as having a uniform distribution of poles on the ends of the magnet. Using this assumption, magnetic induction on the } axis of a circular inﬁnitely long magnet, as a function of the distance from the

H

A

B

C

D

E

A B

C

D

E

A

C

E

Figure 4.7: Distribution of magnetic induction inside and outside magnets of various shapes.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

261

Table 4.2: Distribution of magnetic induction B inside and outside magnets of various shapes [H18]. Point A B C D E

Bar J/2 J/2 J J/2 J/2

Sphere 2J/3 2J/3 2J/3 2J/3 2J/3

Disc 0 0 0

R ș2 ș1

P

z

P

(a)

(b)

Figure 4.8: Calculation of magnetic induction on the axis of a cylindrical magnet.

magnet (Fig. 4.8), is given by 5 E} =

M 2

6

9 : }@U 9 : 91 µ : ¶ 2 [email protected] 8 7 } 1+ 2 U

(4.26)

where U is the radius of the magnetic cylinder. By symmetry, E has no components perpendicular to }= It can be seen that on the surface of the magnet (} = 0) the magnetic induction E = [email protected], as shown in Table 4.2. Numerical computations are required to determine the magnetic induction o the axis. Expressions similar eq. (4.26) can also be obtained for the components of magnetic induction generated by rectangular surfaces [M19]. A uniform solenoid of rectangular or circular cross-section with surface current density mv (A/m) is equivalent, for the purpose of calculating magnetic induction, to a bar with uniform magnetization P = mv = [email protected]0 . If a solenoid has a circular cross-section, magnetic induction E> at point S on its axis, is

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

262

z

2R

z

L

L

D

W

Figure 4.9: Deﬁnition of geometrical parameters of a cylindrical and a rectangular permanent magnets for calculation of the magnetic ﬁeld. given by

mv (4.27) (cos 1 cos 2 ) 2 It can be seen that on the surface of an inﬁnitely long solenoid (1 = 0, 2 = 900 ) E = 0 [email protected], as could have been expected. Selvaggi and Selvaggi [S48] developed mathematical equations that allow the external and internal magnetic ﬁelds of cylindrical and rectangular permanent magnets of ﬁnite dimensions to be determined. These magnets are shown schematically in Fig. 4.9. The authors assumed that the surface charge density at the poles is equal to Mu and that only two parallel faces contribute to the ﬁeld. The equation for the external ﬁeld at distance } from the face of a circular magnet of radius U and length O is ) ( Mu } }+O Eh{w = (4.28) 2 [U2 + (} + O)2 ][email protected] [U2 + } 2 ][email protected] E = 0

The equation of the internal ﬁeld, at the centre of the magnet is Elqw = {

Mu 2

O (U2 +

O2 ) 4

}

(4.29)

Clearly, for O $ 4, Elqw $ Mu . It can be seen that both terms in parentheses in eqs. (4.28) and (4.29) are dimensionless and thus any system of units can be used.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

263

Similar expressions were derived for a rectangular permanent magnet of ﬁnite dimension, as deﬁned in Fig. 4.9. The equation for the external ﬁeld is

Eh{w

; ZG A A arcsin · A ¸[email protected] A 2 A Z G2 A 2 2 A 4 ( + } )( +} ) Mu ? 4 4 = ZG A A arcsin · A ¸[email protected] A 2 A Z G2 A A 2 2 = 4 ( + (} + O) )( + (} + O) ) 4 4

while the expression for the internal ﬁeld is given by ; 5 6< A A ? @ ZG Mu 9 : Elqw = 2 arccos 7 8 2 2 2 2 A Z O G O [email protected] A = > 4[( + )( + )] 4 4 4 4

< A A A A A A A @ A A A A A A A >

(4.30)

(4.31)

Considerably more complicated expressions for the o-centre magnetic ﬁeld can also be found in [S48]. Good agreement between the measured values and those determined from eqs. (4.28) to (4.31) was found.

4.2.6

Magnetic forces

Permanent magnet circuits can be designed either for holding magnetic bodies or for attracting them. The distinction is that the holding magnet has to exert a magnetic force on a material with which it makes a good contact, while the attracting magnet has to exert a force on a magnetic body at a considerable distance. The distinction is important, because the optimum design for the two purposes diers considerably. While the attraction force is essential in many forms of magnetic separators, such as suspended magnets or wet low-intensity drum magnetic separators, in other types of separators it is the holding force that plays a decisive role. The correct compromise between holding and attracting particles from a distance must be achieved. A force between two magnetic charges T1 and T2 separated by a distance u is given by Coulomb’s magnetostatic law: T1 T2 I = u0 40 u2

(4.32)

where u0 is the unit vector in the direction of u= For a thin cylindrical magnet T = MD where M is the magnetic polarization and D is the cross-sectional area of the magnet. We can then write, for semi-ﬁnite magnetic bars of the same cross-sectional area D 1 I = Md Me D2u0 (4.33) 40 u2

264

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

where Md and Me are magnetic polarizations of bars d and e, respectively. When these bars are in contact, eq. (4.33) reduces to: I =

1 Md Me D 20

(4.34)

As an example, magnetic polarization of 1 T produces a pull of 40 N/cm2 , or approximately 4 kg/cm2 , while 0.2 T creates a pull of a mere 0.16 kg/cm2 . Equation (4.34) is often simpliﬁed even further, under the assumption Md = Me = E> into the form 1 2 I = E D (4.35) 20 which is incorrect in many instances [M19]. For instance, if Me = 0, then correctly I = 0> according to eq. (4.34). The simpliﬁed formula would incorrectly yield I = Md2 [email protected]0 . Generally, eq. (4.35) is valid only when bars d and e are of the same material and when there is no source of external magnetic ﬁeld. It is obvious from eqs. (4.34) and (4.35) that the holding force is proportional to the square of ﬂux density and only to the ﬁrst power of the magnet area. By using tapered soft-iron pole-tips it is possible to concentrate the ﬂux to a higher density than the magnets themselves can provide. Although the cross-sectional area of the magnet would decrease somewhat, the holding force will increase nevertheless. Although by increasing the magnetic ﬂux it is possible to increase the holding force for zero air gap, the reach of the magnetic force would decrease once the air gap is introduced. The force of attraction would thus decrease. Therefore, in those magnetic separators in which a pull at a distance (traction force) is important, wide pole-pieces working at a low induction and allowing high force penetration into the air gap, are required. On the other hand, closely spaced poles that produce high holding force are incorporated into those magnetic separators that rely on the holding force rather than traction force. Dry drum and roll magnetic separators are an example of such machines.

4.2.7

Soft iron components of the magnetic circuits

Pole-pieces of a solid or laminated soft iron or mild steel , or occasionally cobaltiron, are an essential part of magnet design. These ﬂux-conducting members are used to complete a return path for the ﬂux and to concentrate or change the ﬂux density in a circuit. Cost is usually an important factor in the choice and majority of magnetic circuits use ordinary cold-rolled steel for these components. Cobalt-iron alloy is used in some high-performance circuits. It is a good practice to operate these materials near their maximum permeability, as shown in Fig. 1.9. This will ensure the maximum ﬂux-carrying capacity of the circuit. Magnetization curves for some high-permeability materials is shown in Fig. 4.10. Relative position of permanent magnets and mild steel components is also of signiﬁcant importance. Figure 4.11 illustrates three possible arrangements

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

265

Figure 4.10: Magnetization curves for several high-permeability materials.

Three positions of permanent magnets in a circuit

(a)

(b)

(c )

Figure 4.11: Three arrangements of a circuit with permanent magnets.

266

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Table 4.3: Reversible temperature coe!cients of permanent magnetic materials. Material Ferrite SmCo5 NdFeB

(Bu ) [%/0 C] - 0.20 - 0.04 - 0.12

(Hfl ) [%/0 C] + 0.40 - 0.30 - 0.60

of a circuit with permanent magnets. Arrangement (a) is the least e!cient as the leakage between the circuit elements is very high. On the other hand, arrangement (c) is the most e!cient as a result of low leakage. Analysis of these circuits with an Alnico 5 magnet showed that the ratio of the gap ﬂux to the total ﬂux in the arrangement (c) is three times higher than in arrangement (a) [P12]. It is clear that permanent magnets should be placed as close to the air gap as possible. A valuable advantage can be obtained by placing a magnet, magnetized through its thickness, on a ferromagnetic plate. Then the magnet behaves like one of twice its thickness.

4.2.8

Stability of permanent magnets

Permanent magnets are expected to maintain a constant ﬂux output over a long period of time, although any magnet, after being fully magnetized, is likely to lose strength slowly with time. In nearly all applications the magnet is subject to inﬂuences that tend to alter the magnet ﬂux. However, in contrast to early permanent magnets, the modern materials exhibit remarkable stability, sometimes as high as 106 . Reversible changes The magnetization changes fall into two classes, namely reversible changes and irreversible changes. The reversible changes in the magnetic properties, as a function of temperature, originate in the change in spontaneous magnetization. Reversible changes are functions of temperature and circuit loading and are time-independent. They disappear completely without need for remagnetization when the permanent magnet is returned to its initial temperature. Figure 4.12 illustrates the dependence of the remanent magnetization on temperature for three types of permanent magnet materials. The reversible changes resulting from temperature changes can be represented by temperature coe!cients, expressed as a percentage change in M or E per 0 C. A summary of the temperature coe!cients of Eu and Kfl for several permanent magnet materials is given in Table 4.3. In addition, Table 1.18 summarizes the Curie temperatures and maximum operating temperatures of various permanent magnet materials. In many instances the temperature coe!cients of magnetization and coercive force do not give enough information about how a magnet will respond to temperature changes. Changes in the shape of a demagnetization curve and the

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

267

Figure 4.12: Temperature dependence of remanent magnetization of various permanent magnetic materials (adapted from [P4]). position of the load line and the working point can only be seen from a complete set of demagnetization curves, measured at dierent temperatures. Figures 4.13 and 4.14 illustrate families of demagnetization curves at various temperatures for ferrite and NdFeB permanent magnets. Such curves are useful for graphical design of magnets operating under various temperature conditions. Complete sets of such demagnetization curves are available either in the literature (e.g. [P4]) or the most recent data can be obtained directly from magnet manufacturers. Irreversible changes In the case of irreversible changes, after the removal of the disturbing inﬂuence, the magnetization does not return to its original value. In certain types of changes however, the magnetization can be fully restored by re-magnetization. Such changes are, for instance, ambient temperature changes and exposure to an external magnetic ﬁeld. Upon exposure to an external ﬁeld, the operating point moves down the demagnetization curve and the intrinsic magnetization of the magnet shows a corresponding change. When the external ﬁeld is removed, the magnetization recovers only partially. This loss is recoverable by re-magnetization. The loss will be greater when a magnet is operating in the steepest part of the demagnetization curve. Although mechanical shock and vibration contribute energy to a permanent magnet, changing its magnetization, modern materials with high coercive forces seem to be resistant to changes by mechanical eects. At the same time, however, ﬁeld exposure is not able to completely eliminate changes that might have occurred.

268

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.13: Demagnetization curves of a ferrite magnet at dierent temperatures.

Figure 4.14: Demagnetization curves of an NdFeB magnet at various temperatures.

4.2. DESIGN OF CIRCUITS WITH PERMANENT MAGNETS

269

Table 4.4: Magnetic induction required to magnetize permanent magnet materials. Material Alnico 5 Alnico 8 Ferrite RECo5 NdFeB

Bvdw [T] 0.3 0.8 1.0 2.0 to 3.0 2.5 to 3.0

While Alnico and ferrite magnets are stable and not subject to corrosion, rare-earth magnets have oxidation problems that limit their maximum operating temperature. If no coating is provided for protection, oxygen diuses into such a magnet, causing a metallurgical change in a surface layer. The surface layer will have a lower Kfl , which will allows this region of the magnet to be demagnetized more easily. Surface oxidation thus leads irreversibly to a reduction in the magnetic properties. Irreversible changes, resulting from permanent changes in the structural or metallurgical state, are usually time-dependent and re-magnetization does not restore the original state of magnetization. The temperature at which changes in properties ﬁrst become noticeable corresponds to the maximum operating temperature. Temperature-induced irreversible losses in permanent magnets are shown in Table 1.17.

4.2.9

Magnetization of permanent magnets

It is generally accepted that to magnetize a permanent magnet to saturation, an external magnetic ﬁeld three to ﬁve times its intrinsic coercivity Kfl must be applied. Typical values of the magnetic induction required to magnetize various permanent magnet materials are summarized in Table 4.4. Simple bar or ring-shaped magnets may be magnetized by a larger permanent magnet, a solenoid or an electromagnet. To magnetize rare-earth magnets, very high ﬁelds are required and magnetization is often performed with small coils or solenoids energized by large current pulses of short duration. Large magnets cannot be magnetized by a pulse of short duration, because eddy currents prevent the ﬂux reaching the centre of the magnet. In general, the frequency i of the pulse must be chosen so that the magnetizing pulse lasts longer than the eddy current. The depth of penetration, or the skin depth , is given by µ ¶[email protected] ( = (4.36) 0 i where ( is the resistivity of the material. Resistivity plays a very important role since most permanent magnets have very low permeabilities . Ceramic ferrite magnets have high resistivity ( A 104 m and full penetration of a pulse is easy. On the other hand, Alnico and

270

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Pole

Coil

B

A

Lg Pole-piece

C Path of integration

Yoke

Figure 4.15: Schematic diagram of an electromagnet with iron yoke. rare-earth magnets, with ( 100×108 m, pose a problem and a pulse width of at least 10 ms must be used [P4].

4.3

Design of iron-core electromagnets

In section 1.7.2 the position of electromagnets with an iron yoke as a source of magnetic ﬁeld in magnetic separation was outlined. Although the iron-core electromagnets have been recently replaced by rare-earth permanent magnets in several types of magnetic separators, they still play an important role in various designs of magnetic separators. In those applications where variable magnetic ﬁeld of moderate strength in a relatively large volume is required, electromagnets with an iron yoke are the ﬁeld source of choice. In spite of availability of powerful modelling techniques for optimization of electromagnet design, the initial design ought to be created based on experience and, to some degree, on guesswork. In this section general principles of design of electromagnetic circuits with an iron core will be described. The design of such a circuit, schematically shown in Fig. 4.15, is governed by Ampere’s law given by eq. (4.3). If we suppose that coils with a total number of turns Q are wound onto the circuit, then Ampere’s law can be re-written as I · go = Q L K (4.37) F

The path of integration extends around the magnetic circuit as shown in Fig. 4.15. The magnetic induction Ej in the air gap of length Oj is, therefore, given by Z Ej = 0 (Q L Kgo) (4.38) Oj EFD

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

271

By calculating the actual ﬁeld E inside the iron part of the circuit, we can then determine the magnetic induction in the air gap from the value of the magnetomotive force (or number of ampere-turns) Q L= We can deﬁne reluctances of the air gap j and of the iron part of the circuit p as Oj (4.39) j = 0 Dj Z 1 go (4.40) p = EFD Dp where Dj and Dp are cross-sectional areas of the air gap and iron and is the permeability of iron. If the magnetization of the iron is much less than saturation, then AA 0 and j AA p = Then we have E0 = 0

QL Oj

(4.41)

This equation expresses a linear relationship between E0 and L, which is observed for any type of electromagnet at low magnetic ﬁelds. If, however, the magnetization of the iron approaches saturation, the permeability of the iron is greatly reduced. Under these conditions eq. (4.41) is not valid and we must use the following, more general equation to calculate Ej Ej =

QL (j + p )Dj

(4.42)

For this purpose we must calculate p from eq. (4.40), which is a di!cult task as we have no straightforward way of determining the value of as a function of position o= Furthermore, the leakage of the ﬂux will increase as becomes small [I1].

4.3.1

Calculation of the magnetic ﬁeld

The magnetic ﬁeld produced in an air gap of an electromagnet can be calculated by integrating contributions of the magnetic charges on the pole surface. For cylindrical ﬂat poles, as shown in Fig. 4.16, the magnetic induction in the gap is given by [M21] · ¸ { Ej = Mv f (1 cos ) = Mv f 1 2 (4.43) (u2 + {2 )[email protected] where f is a correction factor. For tapered poles with coinciding apexes (Fig. 4.16) the magnetic induction becomes u2 Ej = Mv f (1 cos + cos sin2 ln ) = (4.44) u1 · ¸ {u12 u2 { + ln (4.45) Mv f 1 2 2 2 [email protected] 2 [email protected] u1 (u1 + { ) (u1 + { )

272

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Lp

ș r2

x

ș r1

r2

Figure 4.16: Cylindrical ﬂat poles and tapered poles with coinciding apexes. It can be seen that in this case the magnetic induction consists of two terms, the ﬁrst term being the magnetic induction for cylindrical ﬂat poles. The second term is greater than zero (provided that ? 900 and u2 A u1 ), and magnetic induction generated by tapered poles, therefore, generates a greater magnetic ﬁeld than ﬂat poles. This second term achieves its maximum for = 54.70 . It was shown by Montgomery [M21] that eq. (4.43) gives good results if f = 0=7 for 1, while for = 0=5 the correction factor f = 1 gives a good agreement between calculated and measured values of magnetic induction. is a geometrical factor deﬁned as = Os @2u2 and Os is deﬁned in Fig. 4.16. In magnets with tapered pole-pieces eq. (4.45) has very good predictive capability for f = 1.

4.3.2

Shape of iron parts of the circuit

The yoke, as shown in Fig. 4.15, serves to transport the magnetic ﬂux from the end of one pole to the end of the other pole. The presence of iron permits useful values of the magnetic induction (for example, up to 2 T) to be reached with modest investments in ampere-turns. The iron yoke also conﬁnes the stray ﬂux to the immediate vicinity of the magnet gap. The yoke should, therefore, have reasonably high permeability, even when the poles and pole pieces are saturated. Since the magnetization curve of soft iron has a knee at [email protected] = 70% to 80%, it is recommended to make the cross section of the yoke about 1.2 to 1.4 times that of the poles [I1]. In modern magnets the yokes and the poles are made of laminations. In order to attain the strongest possible magnetic ﬁeld, the shape of the poles and pole pieces must be determined to satisfy the following two requirements:

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

r3

r2

x1

273

r1

x2 x3

ș1 ș2

Figure 4.17: Shape of a pole with two conical pole-pieces.

(a) The magnetization of the poles and pole pieces must produce the maximum possible ﬁeld when they are saturated. (b) Saturation should be achieved simultaneously throughout the volume of the poles and the pole pieces. In view of increasing leakage from the poles, as their magnetization approaches saturation, the cross-section of the poles must be reduced as the tip of the pole is approached. The ﬂux density will thus be maintained constant and the requirement (b) will be met. In order to satisfy the requirement (a), Ewing [E2] showed, as early as the end of the nineteenth century, that the shapes of the pole pieces must be conical, preferably with the vortex angle of 54.70 . In an actual electromagnet, however, this conical shape must be modiﬁed, in order to secure homogeneity of the ﬁeld in the air gap and to ensure that permeability is constant throughout the pole and the pole piece [I2]. Analyzing eqs. (4.43) and (4.45), Ishikawa and Chikazumi [I2] showed that the pole shape that satisﬁes the above requirements can be approximated by the shape shown in Fig. 4.17. This shape is composed of a pole-tip of radius u1 , a conical part of radius u2 and another conical part of radius u3 . Analysis of this shape indicates that that the maximum ﬁeld in the air gap depends on the value of u2 @{1 and not on u1 @{1 > while the homogeneity of the ﬁeld is determined by the value of u1 @{1 . The issue of the ﬁeld homogeneity is not critically important in magnetic separation and the parameter u1 @{1 is, therefore, of limited relevance for the design of a circuit of a magnetic separator.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

274

B0

B C A (NI)A

(NI)B

(NI)c

NI

Figure 4.18: The excitation curve of an electromagnet showing the unsaturated zone (A), transition zone (B) and saturated zone (C).

4.3.3

Practical procedure for design of the poles

The design of an electromagnet for a magnetic separator is based on two fundamental speciﬁcations, namely the required magnetic ﬁeld strength Ej and the length (2{1 ) and the depth (2u1 ) of the air gap. The former parameter is determined by the required separation e!ciency while the latter mainly by the desired throughput of the separator. In wet high intensity magnetic separators the depth of the air gap determines the depth of the matrix bed, which in turn also aects the eectiveness of separation. From an economic point of view, the size and thus the price of the magnet depends strongly on the length of the air gap Oj = 2{1 = The volume of the magnet is approximately proportional to (2{1 )3 . Contribution of iron to the magnetic ﬁeld The contribution of the iron circuit to the magnetic induction in the air gap can be divided into three regions, as illustrated by the excitation curve shown in Fig. 4.18. In the unsaturated zone D the reluctance of the air gap is much greater than the reluctance of the rest of the circuit so that almost the entire magnetomotive force appears across the gap. Once the transition zone sets in, the ﬂux that reaches the air gap is reduced. In order to achieved the desired magnetic induction, the number of ampere-turns must be increased, as shown in Fig. 4.18. It was reported by Montgomery [M21] that usually (Q L)E @(Q L)D 1.1 at 60% of the maximum magnetic ﬁeld, while a typical value of this ratio at 85% of the maximum ﬁeld is about 2. A plot of this ratio against the percentage

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

275

Figure 4.19: Ampere-turns needed to achieve a required magnetic ﬁeld.

of the maximum induction, for a typical magnet, is shown in Fig. 4.19. With the number of ampere-turns known at 60% and 85% of the maximum ﬁeld, a satisfactory curve can be drawn representing the magnetization of iron from 0 to 100% [M21]. Figure 4.20 shows the number of ampere-turns required to obtain 85% of the maximum ﬁeld, as a function of the geometry of the magnet. Design of coils Coils in an iron-core electromagnet serve two functions: they provide the electromagnetic force to magnetize the iron, and they contribute a certain magnetic ﬁeld in the air gap. The magnetic induction generated by a coil, the geometry of which is shown in Fig. 4.21, at the centre of the coil, is given by [M22]: Ej =

QL I (> ) 20 d1 ( 1)

(4.46)

where = d2 @d1 , = [email protected] and I (> ) is the ﬁeld factor deﬁned (in SI units) as + (2 + 2 )[email protected] I (> ) = ln (4.47) 1 + (1 + 2 )[email protected] The ﬁeld along the axis } of a coil of axially uniform excitation can be written [M22]: · ¸ } I (> + }@d1 ) + I (> }@d1 ) E} ( ) = E} (0) (4.48) d1 2I (> )

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

276

Figure 4.20: Ampere-turns required to reach 85% of the maximum magnetic ﬁeld in the air gap, as a function of the ratio of the pole face diameter and the gap length, u1 /{1 , for several u3 @u1 ratios (adapted from [M21]).

2b

a2 a1

z

Figure 4.21: Deﬁnition of geometrical parameters of a solenoid coil.

4.3. DESIGN OF IRON-CORE ELECTROMAGNETS

277

Figure 4.22: Empirically obtained curve expressing the maximum magnetic ﬁeld as a function of ratio of the pole diameter to air gap length (adapted from [I1]). If the point at which this ﬁeld is measured lies outside the coil (e.g. in the air gap of an electromagnet) the following relationship should be used in eq. (4.48): I (> }@d1 ) = I (> }@d1 )

(4.49)

Practical rules for the design Taking into account the above analysis, the following rules should be followed in the design of an electromagnet: (1) Although the ﬁeld homogeneity is not critical in magnetic separation, a suitable choice of the pole radius u1 , in such a way that u1 = 2{1 , usually ensures the ﬁeld homogeneity within 103 = (2) The maximum magnetic ﬁeld is a function of the maximum pole diameter 2u3 , irrespective of dierences in pole shapes [I1]. Using Figs. 4.20 and 4.22, approximate value of the maximum diameter of the pole from the selected values of Ej and {1 can be determined. (3) The optimum value of angle 1 depends on the value of u1 @{1 which again is not of major importance in magnetic separators. 1 usually ranges from 500 to 600 . (4) A generally accepted rule is that u3 = 1.2u2 to 1.4u2 = (5) The number of ampere-turns should be selected in such a way that (Q L)E = 1=1(Q L)D or 2(Q L)D , if 60% or 85% of the maximum ﬁeld is to be achieved, respectively. Figure 4.23 illustrates modelling of the magnetic ﬂux in a iron-core electromagnet.

278

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.23: Modelling of an iron-core electromagnet.

4.4

Design of solenoid magnets

As has already been discussed in Section 1.7.3, generation of magnetic induction by iron-core electromagnets is limited by the saturation of the iron. In order to overcome this limitation, Bitter [B24] proposed the use of a magnetizing solenoid surrounded by steel cladding. The magnetic induction in the working volume of such a magnet is given by the sum of the contribution from the coil and from the magnetized iron, as expressed by eq. (1.50). Figure 1.40 illustrates the relative contributions from these two components of the magnet. The idealized circuit of the iron-clad solenoid is shown in Fig. 4.24. The magnetic induction in the air gap is given by Ampere’s law (eq. (4.41)). If the magnetic reluctance of the iron frame cannot be neglected, eq. (4.42) must be used. In a more practical form, a leakage factor N can be included in eq. (4.42), and we can write: QL Ej = 0 (4.50) Oj (1 + N) The leakage factor N is often taken equal to 0.2 [T6, M23]. It transpires from eq. (4.50) that the number of ampere-turns required to generate a given magnetic induction is determined solely by the length of the ﬁeld (or the length of the air gap) Oj and is independent of the radius d1 of the working volume. Solenoids shown in Fig. 4.25 have the same length of the air gap, while their radii dier, and the number of ampere-turns required to generate a required magnetic induction is the same for both solenoids. This feature is extremely useful in the scale-up of magnetic separators. In iron-core electromagnets a higher throughput of separators is achieved by increasing the

4.4. DESIGN OF SOLENOID MAGNETS

279 t

Lg

a1 a2

Figure 4.24: Schematic diagram of an iron-clad solenoid.

length of the air gap. This requires an increased number of ampere-turns, as follows from eq. (4.41). This, in turn, results in an increase in the mass, size and cost the magnet. On the other hand, the scale-up of a magnetic separator based on an ironclad solenoid is achieved by increasing the diameter of the solenoid, keeping the length of the air gap constant. The number of ampere-turns will be constant, only the length of the conductor, and thus its resistance will increase.

Lg

2a1

Figure 4.25: Two iron-clad solenoids having the same length of the air gap and dierent radii.

280

4.4.1

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

The power requirements

The magnetic induction generated directly by the coil itself can be calculated using eqs. (4.46) and (4.48). The power Z (in watts), required to generate a given magnetic induction, is then given by: Z =

(d21 (2 1)(Q L)2 2e(d2 d1 )2

(4.51)

where ( is resistivity of the conductor and is the ﬁlling factor of the winding deﬁned as active section of the winding (4.52) = total section of the winding Combining eqs. (4.41) and (4.51) it can be seen that the power is proportional to the square of the number of ampere-turns and thus of magnetic induction, Z Ej2 . While the electric current L and the number of turns Q are related by eq. (4.41), the necessary voltage can be found from Y = LU> where the resistance of the winding can be calculated from: U=

2(Q (( + 1) Q2 Gphdq = D 2( 1)d1

(4.53)

where D is the cross-section of the winding and Gphdq is the mean diameter of the winding.

4.4.2

The choice of the conductor

The choice of the conductor, between copper and aluminium, determines the maximum current density, the mass and the volume of the coil and the cost of the magnet. Copper is 3.3 times denser than aluminium (8960 kg/m3 vs 2699 kg/m3 ) and for equal coil sizes aluminium will make a much lighter coil. On the other hand, resistivity of aluminium is about 1.58 times greater than resistivity of copper (2.45×108 m vs 1.555×108 m at 0 0 C), 1.58 time more power is required by the aluminium coil to generate the same ﬁeld. Detailed analysis of the relative merits of aluminium and copper coils, as a function of coil geometry, mass and cost can be found in [M22].

4.4.3

The cooling of coils

The removal of the Joule heat generated inside the winding can be accomplished in several ways. Indirect air cooling can be applied to magnets operating at low current densities, generally not exceeding 3 A/mm2 for a copper conductor. Direct immersion of the coil into the circulating oil or water greatly improves heat conduction and transfer and higher current densities can be used. The operating current density can be increased considerably by using hollow conductors through which the cooling liquid circulates. Water is a very e!cient

4.4. DESIGN OF SOLENOID MAGNETS

281

coolant in removing heat at conventional temperatures. The oils, for example, have heat-transfer characteristics about one-ﬁfth that of water [D11]. Coils with low resistance, operating at low voltage, are almost always cooled with deionized or demineralized water, mains water causing electrolysis even at low voltage. The cooling water is circulated through the coil, a heat-exchanger, a ﬁlter and a deionizer. In the heat-exchanger the heat is carried o by tap water. The ﬂowrate of water T (in cm3 /s or m3 /h) required to restrict the temperature rise to W (in 0 C) in a magnet with power input of Z (in watts) is given [M22] by: Z Z (fjv) = (VL) (4.54) T= 4=186W 1163=7W For instance, for a 250 kW magnet, with temperature rise of W = 30 0 C, the required ﬂowrate is approximately 2000 cm3 /s, or 7.2 m3 /h. The operating temperature of a magnet aects the resistance of the winding and thus the power needed to achieve the required magnetic ﬁeld. The hotter the coil, the higher the resistance will be and the more power will be needed. The temperature dependence of resistivity of conductors can be written (W = (20 [1 + (W 200 F)]

(4.55)

where (W and (20 are resistivities at temperature W and 20 0 C, respectively and is the temperature coe!cient. For copper (20 = 1.72×108 m and = 0.0041/0 C, while for aluminium (20 = 2.7×108 m and = 0.0045/0 C. Therefore, a copper conductor operating at 60 0 C has resistivity of 2×108 m, while an aluminium conductor has resistivity of 3.2×108 m. Whether or not the amount and ﬂow velocity of the coolant, as determined by eq. (4.54), can be forced through the winding of the magnet depends on the pumping power available and on the detailed structure of magnet. The pressure drop across a tube is the sum of the entrance and exit losses and frictional drop in the tube. The total pressure drop S (in Pa) becomes O S = (0=74 + 0=015 )103 y 2 g

(4.56)

where O and g are the length and diameter of the cooling path (in m), and y is the coolant velocity (in m/s). A typical pressure drop for copper hollow conductors is 0.5 to 0.8 MPa.

4.4.4

Thickness of the iron cladding

The basic requirement for the iron cladding is that it must not be saturated. The magnetic ﬂux in the cladding is Mv Df where Df is the cross-sectional area of the cladding. In order to avoid oversaturation of the cladding, the following inequality must be satisﬁed: Ej Dj 5 Mv Df (4.57) where Ej is the magnetic induction in the air gap of cross-sectional area of Dj . The thickness of the cladding can thus be found from this equation.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

282

Table 4.5: Properties of decarburized steel for high-ﬁeld magnets [B1]. Chemical composition Coercivity Hmax f Permeability

0.05 - 0.02% C, 0.2% Mn, 0.02% S 0.05% Cu, 0.01% P, 0.02% Ni 60 to 80 Am1 B A 0.04 T at H = 40 Am1 B A 1.5 T at H = 1200 Am1 B A 2.0 T at H = 2400 Am1

The choice of the value of Mv is important for correct dimensions of the iron cladding. The values of saturation polarization for commercial steels are usually not available and the value of 1.5 T or less should be used. Low-carbon decarburized steel is frequently used in high-ﬁeld magnets and typical speciﬁcations are shown in Table 4.5 [B1]. Several important rules relating to the usage of iron cladding can be outlined: • Magnets for which the length of the air gap is greater than the inner diameter of the solenoid, i.e. Oj A 2d1 , do not require the iron pole above and below the working volume. On the other hand, when Oj ? 2d1 , the presence of iron cladding in the vicinity of the working space is necessary. • By replacing the external air path with a magnetic circuit of low reluctance, the most signiﬁcant increase in the magnetic induction, for a given magnetomotive force, can be obtained for solenoids of small axial length. Therefore, the contribution of the iron is largest if the coil has a considerable stray magnetic ﬁeld. In the case of a long thin solenoid, in which the stray ﬁeld is small, the eect of an external iron circuit is negligible.

4.5 4.5.1

Design of drum magnetic separators The basic magnet arrangements

The basic design of the magnetic circuit of drum magnetic separators is common to most commercially available models. Permanent magnet blocks are stacked on top of each other in a speciﬁc geometrical arrangement. The simplest arrangement is shown in Fig. 4.26. Strontium or barium ferrite blocks, usually magnetized through their thickness are frequently arranged radially in low-intensity drums. The frequently used size of the blocks is 150 mm long, 100 mm wide and 25 mm thick. The number of blocks per stack is determined by the diameter of the drum. These radially magnetized stacks are most often arranged in rows parallel with the axis of the drum, separated by an air gap. A radial arrangement is also used, as discussed in Section 2.1.5. and as shown in Fig. 2.12. Figure 4.27 illustrates the axial arrangement of magnet blocks in a magnetic drum.

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

a

283

b S

N

N S

L

Figure 4.26: Schematic diagram of radially magnetized magnets in a magnetic drum with axial arrangement of the poles.

Figure 4.27: Axial arrangement of magnet blocks in a magnetic drum.

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

284 N

N

S

S

S

N

Figure 4.28: Position of a backing magnet (cross pole) in a drum magnetic separator. High-intensity drum separators employ rare-earth magnets, usually NdFeB, and it is a common practice to simply replace ferrite magnets with rare-earth blocks, with the intent to achieve a higher magnetic ﬁeld [A13]. The rare-earth blocks are smaller than the ferrite blocks, for example 50×50×15 mm. Another arrangement of permanent magnets which is frequently employed is shown in Fig. 4.28. A ferrite magnet, magnetized in a transverse direction is inserted between the radially magnetized stacks of permanent magnets. Explanations of the function of this "backing" of "blocking" magnet (or "cross pole") are as numerous as its names. Reduction of the leakage ﬂux between the adjacent main stacks and addition of extra ﬂux [M19] are the most likely explanations of the beneﬁt that this arrangement oers.

4.5.2

Geometry of the magnet assembly

Although drum magnetic separators are one of the oldest types of magnetic separators, and certainly the most widely used, design of the magnetic circuit is still to a great extent empirical. A simple rule for geometrical arrangement of the magnet blocks that was used for many decades states that the ratio of the magnet block width e and the width of the air gap d should be [email protected] = 3 to 5 for ferrite and rare-earth magnets and [email protected] = 1.2 for Alnico magnets and electromagnets [D4]. The design dierence is the result of dierent demagnetization behaviour of the permanent magnet materials, as shown in Fig. 4.2. Using computer modelling, this design rule has been revised, as will be discussed later. A typical distribution of the ﬁeld pattern along the circumference of a drum with axial pole arrangement is shown in Fig. 4.29. The maxima in the magnetic induction occur at the centres of the air gaps while the minima occur at the centre of the magnet block. Comparison of the magnetic induction generated by dierent magnet arrangements in a drum is given in Fig. 4.30. The relative values of the magnet and air gap widths aect the magnetic ﬁeld and force distribution around the drum. For instance, by reducing the distance between the magnet blocks, or the so-called pole pitch (deﬁned either

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

285

Figure 4.29: Distribution of the magnetic induction along the circumference of an NdFeB drum with axially arranged poles. The width of the radially magnetized magnets e = 100 mm and the air gap width d = 10 mm [M24].

Figure 4.30: The maximum magnetic induction generated by dierent magnet arrangements in an axial drum with radial magnetization of the magnet blocks (adapted from [M10]).

286

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.31: Magnetic ﬁeld and force index (in arbitrary units) as a function of distance from the drum surface, for dierent distances between the poles (adapted from [S13]).

Shell

Steel pole

Magnet block

Figure 4.32: Steel poles sandwiched between azimuthally arranged magnet blocks.

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

287

Figure 4.33: Magnetic induction generated by magnetic drums, with three different magnet arrangements, as a function of distance from the drum surface (adapted from [F19]).

Figure 4.34: Dependence of the magnetic induction on the surface of the drum, on the width e of the NdFeB magnet, for d = 10 mm. Three dierent conﬁgurations are shown [M24].

288

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.35: Dependence of the force index at 15 mm from the drum surface, on the width e of the NdFeB magnet, for d =10 mm. Three dierent conﬁgurations are shown [M24].

Figure 4.36: Magnetic induction as a function of the width d of the air gap, for an NdFeB magnetic drum, for e = 100 mm [M24].

4.5. DESIGN OF DRUM MAGNETIC SEPARATORS

289

Figure 4.37: Force index for an NdFeB drum, as a function of the width d of the air gap, for e = 100 mm [M24]. as d or d + e in Fig. 4.26), it is possible to increase the ﬁeld gradient. Although the ﬁeld strength is reduced, the increase in the ﬁeld gradient is su!cient to result in the increase of the force index. The situation is depicted in Fig. 4.31. It can be seen that the increase in the force index by reducing the pole pitch takes place only in the proximity of the drum surface and that the force index decreases rapidly away from the drum. In other words, the smaller the pitch, the higher the force index on the drum surface and the shorter the reach of the magnetic force. In the nineteen eighties the Fives-Lille group developed drum magnetic separators with steel poles sandwiched between ferrite magnet blocks with azimuthally arranged direction of magnetization, as shown in Fig. 4.32. As a result of their superior performance, compared to the conventional design, in terms of magnetic force and metallurgical performance, the azimuthal concept was commercially accepted for some applications. Comparison of the magnetic ﬁeld strength achievable by the conventional and azimuthal designs is shown in Fig. 4.33.

4.5.3

Electromagnetic modelling of the design

Electromagnetic modelling software that has become available in recent years allows for the optimization of the design of conventional magnetic circuits. The modelling allows the investigation of the eect of various geometrical parameters of the drum on the magnetic ﬁeld and magnetic force. For instance, Fig. 4.34

290

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.38: The dependence of the magnetic induction generated by a strontium ferrite block 100×150 mm, on its depth O, on the surface of the block and at 15 mm from the surface. illustrates the variation of the magnetic induction on the surface of a drum with the width e of the magnet block. It can be seen that for a constant width d = 10 mm of the gap, the maximum magnetic induction is achieved for the magnet width of 100 mm. The ratio [email protected] = 10 is thus in disagreement with the empirical rule-of-thumb mentioned earlier. Figure 4.34 also shows that replacement of the air gap with a steel block results in the reduction of the magnetic ﬁeld. Similar conclusions can be drawn from Fig. 4.35, which displays the eect of the magnet width on the force index. The eect of the width d of the air gap on the ﬁeld at various distances from the drum surface is illustrated in Fig. 4.36. It can be seen that by increasing d, for a constant value of the width of the magnetic block (i.e. with the ratio [email protected] decreasing), the magnetic induction decreases, at least in the proximity of the drum surface. At larger distances from the drum surface, e.g. at 50 mm, the eect of the value of d (and thus of [email protected]) is diminishing. Similar trends can be observed for the force index as shown in Fig. 4.37. The results illustrated in Fig. 4.30 and Figs. 4.34 to 4.37 were obtained for a drum with axial pole arrangement and with magnets magnetized radially. The diameter of the drum was 600 mm and the depth O of the magnet stack was 100 mm. The eect of the depth of the magnet stack can be determined by using eq. (4.30), which allows for the variation of the depth O , as shown in Fig. 4.9, and for the calculation of the magnetic ﬁeld generated by such a magnet block, at dierent distances }. Figure 4.38 illustrates such a dependence for a strontium

4.6. DESIGN OF A MAGNETIC ROLL

291

Figure 4.39: Magnetic induction on the roll surface, as a function of the magnet ring thickness. The values of magnetic induction were obtained by computer modelling [F18]. ferrite block, of dimensions 150 mm (Z ) × 100 mm (G). It can be seen that the beneﬁt of increasing the depth of the magnet stack above 140 mm is limited. The computer modelling also allowed for the development of new geometries of the magnet arrangement, capable of producing a higher magnetic strength and magnetic force [A13, S8]. Some of these new designs are proprietary and the patents are still pending. Comparison of one such a design, with conventional designs, is shown in Figs. 4.34 and 4.35.

4.6 4.6.1

Design of a magnetic roll Basic concepts of design

The overall view of a magnetic roll separator is shown in Figs. 2.30 and 2.31. The magnetic roll itself forms a part of a short conveyor fed by a vibratory feeder. The conveyor belt is made of a thin high-tensile material, often with antistatic coating. The belt is supported by second roll (idler). Roll separators are usually of modular design allowing them to be stacked in any number of passes of material. Typical speciﬁcations of such a roll separator are shown in Table 4.6. The e!ciency of separation is aected by the roll design and by several operating variables: the number of separation stages, belt speed, splitter position and belt loading. Most of these variables are determined by particle size

292

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.40: Force index as a function of the magnet ring thickness, for thickness of steel rings equal to 1 mm and 1.75 mm, on the roll surface and at 15 mm from the surface.

Figure 4.41: Magnetic induction on the surface of a roll, as a function of thickness of steel rings, for several thicknesses of permanent magnet rings.

4.6. DESIGN OF A MAGNETIC ROLL

293

Table 4.6: Typical speciﬁcations of a permanent roll magnetic separator. Parameter Belt thickness Roll diameter Roll length Max. magnetic induction

Speciﬁcation minimum 0.12 mm 72, 76, 100, 220 & 300 mm 250, 500, 1000 and 1500 mm NdFeB: 1.9 T, SmCo: 1.5 T, SrFe: 0.5 T

distribution and magnetic properties of the feed and by the recovery vs grade requirement.

4.6.2

Design parameters

Thicknesses of magnet and steel rings As has been discussed in Section 2.3.3 and shown in Fig. 2.28, the roll consists of discs or rings of permanent magnets, interleaved with mild steel rings. The adjacent permanent magnet rings are arranged with the same polarity facing one another, i.e. rings are arranged in a repulsive mode. The relative thicknesses of the magnets and the steel rings aect the magnetic ﬁeld strength and its pattern around the roll. This situation is depicted in Figs. 4.39, 4.40 and 4.41. It can be seen that the magnetic induction on the surface of a roll increases with increasing thickness of the magnet ring. At the same time it achieves the maximum value for a certain, rather small, thickness of the steel rings. With further increase in the thickness of the steel rings the magnetic induction decreases. This is a consequence of the fact that the saturation magnetization of steel is much greater than that of the permanent magnet material. If the thickness of the steel exceeds a certain optimum value, the magnet ring does not succeed in saturating the steel, as transpires from eq. (4.12). As can be seen in Figs. 4.42 and 4.43, for thin steel and magnet rings, which generate a high force index close to the roll surface, the reach of the magnetic force drops dramatically away from the surface. The rate of decrease is much smaller for thicker magnet rings and even more so for an NdFeB drum. Optimization of the design of the magnetic roll consists not only of maximizing the magnetic induction and force index on the roll surface and at a suitable distance from the roll, but also of matching the dimensions of the magnet and steel rings thicknesses to the particle size distribution of the material to be separated. Distributions of the magnetic induction along the axes of NdFeB and SrFe rolls are shown in Figs. 4.44 and 4.45. The magnetic ﬁeld (and magnetic force) on the roll surface are the greatest in a relatively narrow region at the interface between the magnet and steel rings. It can also be seen that the ﬁeld and the force along the circumference of the magnet rings are very feeble, and it is imperative, therefore, that no particles are continuously exposed to this region of the roll. The thickness of the magnet rings should thus be of magnitude similar to the

294

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.42: Force index as a function of distance from the roll surface, for various thicknesses of magnet rings. Steel ring thickness equals 1 mm.

Figure 4.43: Force index (in arbitrary units), for two conﬁgurations of NdFeB rolls and an NdFeB drum, as a function of the distance from the surface of the roll [F18].

4.6. DESIGN OF A MAGNETIC ROLL

295

Figure 4.44: Distribution of the magnetic induction on the surface on an NdFeB roll with 3/1 conﬁguration (magnet thickness: 3 mm, steel thickness: 1 mm).

Figure 4.45: Distribution of the magnetic induction on the surface of a SrFe roll with 6/2 conﬁguration (magnet thickness: 6 mm, steel thickness: 2 mm).

296

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.46: The partition curves for the recovery of 4 mm magnetic tracers by NdFeB rolls of dierent conﬁgurations [F20]. mean particle size of the material to be separated. Thin magnet rings should be used to separate ﬁne particles, while for larger particles a thicker magnetic ring oers a larger contact area with the roll, and a longer reach of the magnetic force, of the order of the radius of the particles. It transpires from the above discussion that the design of the roll, and specifically the thicknesses of the magnetic and steel rings, is dictated by the magnetic properties and size distribution of the feed. The roll design must be optimized in order to maximize the magnetic force and its reach and to match the dimensions of the particles with the magnet thickness. A speciﬁc conﬁguration expressed as magnet thickness/steel ring thickness is suitable only for a narrow size fraction and typical conﬁgurations are summarized in Table 4.7. The optimum conﬁguration obtained by electromagnetic modelling can be validated experimentally using magnetic tracers of suitable sizes and accurate values of magnetic susceptibility. Magnetic partition curves can then be constructed, the probable error Hs can be calculated and a conﬁguration with the lowest Hs can be determined. Hs for a magnetic separator can be deﬁned as Hs =

"75 "25 2

(4.58)

where "75 and "25 are the mass magnetic susceptibilities of particles 75% and 25% of which, respectively, report to the magnetic fraction. Typical partition curves, for 4 mm particles, are shown in Fig. 4.46. It can be seen that the partition curve for the roll conﬁguration 4/2.5 is steeper than that for 4/1

4.6. DESIGN OF A MAGNETIC ROLL

297

Table 4.7: Various conﬁgurations of NdFeB magnetic rolls. Conﬁgurations are expressed as the ratio magnet thickness/steel thickness. Conﬁguration 3/1, 4/1 or 4.1.5 6/1.5, 6/2, 6/3 8/2, 8/3

Size fraction - 5 + 0.1 mm - 10 + 5 mm + 10 mm

Comment Short reach, high ﬁeld Longer reach, lower ﬁeld For large particles

Figure 4.47: Force index for NdFeB rolls of dierent diameters, as a function of distance from the roll surface. Roll conﬁguration: 12/7.5. The data were obtained by computer modelling (adapted from [F18]). conﬁguration and Hs is correspondingly lower. Conﬁguration 4/2.5 is, therefore, more selective in separating 4 mm particles of dierent magnetic susceptibilities.

Diameter of magnet rings In the past, the diameter of a rare-earth magnetic roll was dictated by availability of the largest magnetic rings. While the ﬁrst commercial rolls had diameters of 72 and 76 mm, recent progress in manufacture of rare-earth permanent magnet rings and segments allows for the manufacture of rolls with diameter of 100, 220 and 300 mm. The choice is determined by a combination of throughput, performance and cost considerations. The present advantageous cost situation favours larger diameter rolls, particularly when large throughputs are required [A13]. In a simpliﬁed assumption of a constant magnetic force and constant resi-

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

298

2a1

h H

2a3

2a2

z

P

Figure 4.48: Schematic diagram of a suspended magnet. dence time, a throughput increase by increasing the roll diameter, follows the ratio G1 /G2 , where G1 and G2 are the roll diameters, as follows from eq. (5.4). It is sometimes argued that by increasing the magnet diameter the magnetic force also increases and an even higher throughput can be expected. It appears, however, that the increase in the magnet ring diameter above 100 mm brings only negligible increase in the force index, as is illustrated in Fig. 4.47. On the other hand, a longer retention time of particles in a larger-diameter roll, as a result of a longer arc of the magnet ring, to which the particles are exposed, allows for the increase of speed of rotation of the roll and thus for the increase of the throughput, while maintaining constant residence time. Experience indicates that a throughput increase by factor of two to ﬁve, maintaining the same performance, can be obtained with larger diameter rolls [A23, A13].

4.7

Design of a suspended magnet

Suspended magnets are usually installed over conveyor belts, discharge ends of feeders or screens and above chutes or launders. Their design is dictated by the burden depth, the belt speed, the clearance required over the burden and the size, shape and mass of the tramp iron that is being removed. Strength and reach of the magnetic ﬁeld and of the magnetic force must, therefore, be maximized for high e!ciency of the material removal. A schematic diagram of an electromagnet-based rectangular suspended magnet is shown in Fig. 4.48. The magnet consists of an iron yoke and a coil, which magnetizes the yoke. The magnetic ﬁeld generated at point S , at distance } from the magnet, is the sum of contributions from the magnetized steel and

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

299

Figure 4.49: Pattern of magnetic ﬂux around a suspended magnet. the coil. Dimensions of individual parts of the yoke determine the distribution of the magnetic ﬁeld and magnetic force, their value and reach. Using computer modelling, it is possible to investigate the inﬂuence of these dimensions and to determine the optimum design for a given application. The distribution of magnetic ﬂux around a suspended magnet is shown in Fig. 4.49, while a three-dimensional image is presented in Fig. 4.50. In commercially available suspended magnets, the width 2d1 of the magnet typically ranges from 900 mm to 1400 mm, the depth ranges from 700 mm to 1250 mm and the height K is around 500 mm. Aluminium is the preferred conductor materials, mainly because of its lower density. For the same electric power, the mass of the aluminium coil can be approximately halved, compared with the copper coil [K36]. In addition, the use of the aluminium foil, rather than of the wire, allows for the increase in the ﬁlling factor of the winding, by about 40% [K36]. As a result, the number of ampere-turns can be reduced, or, alternatively, at the constant number of ampere-turns, a more powerful magnet can be constructed.

4.8

Design of a ferrohydrostatic separator

Commercial and laboratory ferrohydrostatic separators use either an electromagnet or permanent magnets to generate the magnetic ﬁeld in the working space. Of fundamental importance in the operation of separators with magnetic ﬂuids are the characteristics of the magnetic levitation force, expressed by the second term on the right-hand side of equation (2.9), namely by Mi EuE. These characteristics are determined by the pattern of the gradient of the magnetic

300

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.50: A three-dimensional image of the magnetic ﬁeld around a suspended magnet. ﬁeld and, therefore, by the shape of the pole tips. The shape of the pole tips is determined by several factors, namely by the choice of the magnetic ﬂuid and the number of density fractions that are to be produced. If paramagnetic liquids are to be used, the constant apparent density of separation in the entire volume of the ﬂuid will be obtained if the force acting on a particle is constant, I = const., which corresponds to EuE = const., as transpires from eq. (3.144). This condition can be re-written as CE 2 = frqvw= C|

(4.59)

where | is the vertical axis, as shown in Fig. 4.51. This requirement is the result of the linear dependence of the ﬂuid polarization, namely i E, on the external magnetic ﬁeld. The ﬁeld that satisﬁes condition (4.59) is the isodynamic ﬁeld. As can be seen from eq. (3.145), the situation is somewhat dierent with ferroﬂuids: if the ferroﬂuid is magnetically saturated, a constant density of separation will be obtained by maintaining the constancy of the force acting on the particles by satisfying the condition uE = const. In other words, the condition CE = frqvw= (4.60) C| should be satisﬁed in a su!ciently large region of the magnetic ﬁeld. Two basic shapes of pole tips have been used in ferrohydrostatic separators, namely a simple wedge geometry of the working space, and pole tips with hyperbolic shape.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

301

y S

N

Permanent magnet

lg ș Iron yoke

Figure 4.51: Schematic diagram of an FHS magnetic circuit with a wedgeshaped working gap.

4.8.1

FHS separators with a wedge-shaped working gap

Wedge-shaped working space was used in separators with permanent magnets, such as those built by Tohoku University [S50], Nittetsu Mining Co. (Japan) [S51] and the Too Geos (Russia) [S52] machines. A schematic diagram of such a magnetic circuit is shown in Fig. 4.51. Since the gradient of the magnetic ﬁeld, in this design, is not constant along the vertical ([email protected]| 6= frqvw=), the apparent density of the ferroﬂuid along the vertical will also vary. A typical distribution of apparent density of the ferroﬂuid in a separator with wedge-shaped working space, used for recovery of non-ferrous metals, is shown in Fig. 4.52. It can be seen that essentially a continuous spectrum of densities is present in the pool of the ferroﬂuid. The usefulness of this density distribution is very limited as inter-particle collisions and interactions do not allow accurate and selective separation of individual metals into individual density fractions. Distributions of the magnetic induction and the apparent density of the ferroﬂuid along the vertical axis for the Too Geos separators with ferrite permanent magnet-based wedge-shaped pole tips were reported by Solodenko [S52]. The results are summarized in Fig. 4.53. Shimoiizaka et al. [S50] obtained a similar pattern in a separator that used SmCo permanent magnets (see Fig. 4.54). It can be seen again that a magnetic system with wedge-shaped poles creates a plurality of values of the ﬁeld gradient, and, therefore, of the apparent density of the ferroﬂuid along the vertical axis of the magnet gap. It is clear that such patterns of the apparent density can be used only for density separation of mixtures of materials with large density dierential. Speciﬁcations of the Tohoku University FHS separator, as reported by Shi-

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

302

Feed point

Surface of ferrofluid 5 g/cm3 Al

Pool of ferrofluid

6

V

8

Zn

9

Cu

10

Bi

8 6

Bottom of the magnetic pole Pb

Figure 4.52: Distribution of the apparent density of ferroﬂuid in an FHS with a wedge-shaped working space. Recovery of various non-ferrous metals at dierent positions along the vertical axis is indicated.

Figure 4.53: The apparent density and magnetic induction in a permanent magnet-based ferrohydrostatic separator with wedge-shaped pole tips, as a function of distance from the base of the pole tips (adapted from [S52]).

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

303

Figure 4.54: Magnetic induction and its gradient in the gap of a SmCo magnet-based ferrohydrostatic separator with wedge-shaped pole tips (adapted from [S50]). Table 4.8: Speciﬁcations of the Tohoku University FHS separator for the recovery of non-ferrous metals, for three dierent values of the width of the magnet gap [F21]. Parameter Magnetic ﬁeld [T] Field gradient [T/m] Apparent density [kg/m3 ]

lj = 60 mm 0.362 3.5 9600

lj = 80 mm 0.314 3.0 8200

lj = 100 mm 0.265 2.5 6900

moiizaka et al. [S50] and Fujita [F21], are summarized in Table 4.8. SmCo permanent magnets were used to generate the magnetic ﬁeld in the working space. The height of the ferroﬂuid pool was 120 mm and the angle between the pole tips amounted to 300 . Water-based ferroﬂuid of density approximately 1400 kg/m3 and magnetic polarization of 0.028 T was used. Another disadvantage of the permanent magnet-based FHS is that the value of the magnetic induction and of the ﬁeld gradient cannot be easily varied. The magnetic induction can be varied only by changing the distance between the pole tips using a mechanical device that can slide one of the poles against the other. The ﬁeld gradient can be varied by adjusting the angle = As a result of the absence of constancy of the apparent density of the ferroﬂuid and of any meaningful control of the operating magnetic ﬁeld and its gradient, the permanent magnet-based wedge-shaped ferrohydrostatic separators are suitable only for separation of materials that dier in density by at

304

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.55: Hyperbolic pole proﬁle with a mirror plate. least 2000 kg/m3 . Recovery of platinum-group metals [S53, S54, G4] and possibly separation of non-ferrous metals [S50] are applications where the limited accuracy of such separators can be tolerated. For more accurate separation of materials with small density dierences, hyperbolic pole tips must be used.

4.8.2

Separators with hyperbolic pole tips

A common objective of sink-and-ﬂoat separation is usually a production of two density fractions selectively and accurately. In order to achieve such a goal in ferrohydrostatic separation, it is necessary for the apparent density of the ferroﬂuid to be constant throughout the volume of the ferroﬂuid. As follows from eq. (3.145), this can be achieved by ensuring that the ferroﬂuid is magnetically saturated and by designing the shape of the pole tips in such a way that the ﬁeld gradient along the vertical axis is constant, namely [email protected]| = const. An additional constraint on the desired ﬁeld pattern is that the horizontal gradients, i.e. [email protected]{ and [email protected]}, are as small as possible. Therefore, for ideal density separation in ferrohydrostatic separators, the following conditions should be met: CE CE CE = frqvw 6= 0> = =0 (4.61) C| C{ C} Such a pattern of the magnetic ﬁeld can be achieved by a hyperbolic shape of the pole tips [K18], as shown in Fig. 4.55. In deriving the above conditions (eq. (4.61)), it was assumed that the branches of hyperbola forming the pole proﬁle extend to inﬁnity and that their asymptotes ({-axis) are at equal potential [G14]. The latter condition is satisﬁed in magnetic systems, in which the upper

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

305

Figure 4.56: GMUO ferrohydrostatic separator with hyperbolic pole tips. half of the hyperbolic surface is replaced by a ferromagnetic plate, coincident with the { axis, and perpendicular to the | axis, as shown in Fig. 4.55 [K18]. It was shown [K18, G15] that conditions given by eqs. (4.61) cannot be satisﬁed at all points in the working zone of the magnetic system. These conditions can be met only in the plane of symmetry passing through the centre of the interpolar gap deﬁned by the | axis in Fig. 4.55. The situation is further complicated by the fact that, in practice, the poles have ﬁnite dimensions. The hyperbolic surfaces are, therefore, terminated at some ﬁnite values of {> | and }. Such a truncation of the ideal hyperbolic shape necessitates corrections to the shape of the pole tips, in order to meet the conditions expressed by eqs. (4.61). The surfaces of the poles are shaped in such a way that they coincide with one of the elementary solutions of the Laplace equation. A powerful method for the analytical solution of Laplacian ﬁelds, namely conformal transformation, was used to calculate the magnetic ﬁeld generated by poles of ﬁnite size and of hyperbolic proﬁle [G14, G15, G16, S55]. This approach is the basis of the design of the GMUO ferrohydrostatic separators, as described in Section 2.8 and

306

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.57: The gradient of the magnetic ﬁeld along the vertical axis of the GMUO FHS-40M separator, as a function of distance from the base of the magnet pole tips.

shown schematically in Fig. 4.56. Similar design of the pole tips was used by the US Bureau of Mines [R9, K17] in their equipment for separation of non-ferrous metals. The distribution of the magnetic ﬁeld gradient along the vertical | axis in the GMUO FHS-40M separator is shown in Fig. 4.57. It can be seen that in a 40 mm long region along the vertical the gradient is constant. The apparent density of the ferroﬂuid is, therefore, also constant and selective and accurate density separation is possible in that region. It is found, using eq. (3.145), that a ﬁeld gradient of 2.5 T/m generates an apparent density of approximately 4200 kg/m3 , using, for example, a kerosenebased ferroﬂuid with magnetic polarization of 0.02 T. The apparent density can be varied by varying the electrical current in the coils and thus varying the magnetic ﬁeld in the working gap. The availability of computer electromagnetic modelling software has changed the speed and accuracy of the design of suitable proﬁles of the pole tips considerably. Although the initial proposal and design of the proﬁles still has to be worked out from ﬁrst principles of the magnet design, computer-based ﬁeld analysis can be used to verify and ﬁne-tune the design. Computer modelling, therefore, allows the pole proﬁles to be optimized so that the required density range and its accuracy are obtained. An example of the optimized hyperbolic proﬁle of pole tips of FHS is shown in Fig. 4.58 and a general view of a ferrohydrostatic separator with hyperbolic pole tips is shown in Fig. 4.59.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

307

Figure 4.58: Hyperbolic pole tips in FHS, as obtained by computer modelling.

Figure 4.59: Ferrohydrostatic separator with hyperbolic pole tips.

308

4.8.3

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Calculation of proﬁles of pole tips in FHS

Although computer modelling facilitates optimization and ﬁne-tuning of the pole proﬁles, the ﬁrst step in the design of a magnetic system of a ferrohydrostatic separator is, as a rule, the calculation of the ﬁeld and of the pole proﬁle from ﬁrst principles. The magnetic ﬁeld between the poles of the magnet can be represented by a scalar magnetic potential X : K = uX

(4.62)

Since the electrical currents are absent in this system, the magnetic potential satisﬁes the Laplace equation u2 X = X = 0

(4.63)

which can be written in polar coordinates u2

CX C2X C2X + u =0 + Cu2 Cu C2

(4.64)

A possible solution of the Laplace equation is the potential function X (u> ) = U(u)V()

(4.65)

where U is a function of u only and V is a function of only. It can be shown that these functions have the following form [B25]: U = fup + gup

(4.66)

V = j cos p + k sin p

(4.67)

and where f> g> j and k are constants. A particular solution to the Laplace equation can, therefore, be written in the form of a circular harmonic of order p as X (u> ) = (fup + gup )(j cos p + k sin p)

(4.68)

Of practical interest are, for example, solutions of the form [G17, Z7]: X0 = D0

(4.69)

Xp = Dp up sin p

(4.70)

and If the surfaces of the poles of the magnet are made to coincide with a given pair of equipotential surfaces (the proﬁle of which is independent of the third dimension), the ﬁeld between them and the proﬁle of the pole tips are described by eqs. (4.69) and (4.70).

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

309

Table 4.9: Properties of pole proﬁles. Value of m 2 3/2

Up /A u2 sin 2 = frqvw= [email protected] sin 32 = frqvw= = frqvw=

Comment constant gradient isodynamic ﬁeld, I = frqvw= wedge conﬁguration

Taking into account that K = uX , the modulus of the magnetic ﬁeld intensity is |K| = pDup1 (4.71) The gradient of the magnetic ﬁeld along the vertical (| axis) then has the form CK (4.72) = (p 1)pDup2 sin p C| while the product of the magnetic ﬁeld and its gradient (force index) are expressed as CK (4.73) = (p 1)p2 D2 u2p3 sin p K C| These equations can be used to evaluate and design various shapes of the pole proﬁles. For p = 1, [email protected]|, or the magnetic force, is zero. The simplest practical case of a wedge pattern is expressed by eq. (4.69). The wedge conﬁguration is represented by a straight line described by the equation = const= The isodynamic proﬁle, in which [email protected]| = const=> can be obtained from eq. (4.73) when p = 3/2. The isodynamic proﬁle of the pole tips is then given by 3 Xp = [email protected] sin = frqvw= (4.74) 2 and 3 CK = D2 sin (4.75) K C| 2 Pole proﬁles that generate a magnetic ﬁeld whose gradient in constant along the vertical axis can be obtained from eq. (4.72) when p = 2 and the equations of the proﬁle are as follows:

and

Xp = Du2 sin 2 = frqvw=

(4.76)

CK = 2D sin 2 C|

(4.77)

Equations (4.74) to (4.77), in which p determines the geometrical features of the ﬁeld and D describes the magnetic characteristics of the system, provide the full description of the proﬁle of the pole tips. Properties of these conﬁgurations are summarized in Table. 4.9.

310

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Design procedure We will assume that we want to design the pole proﬁles for a ferrohydrostatic separator operating with a ferroﬂuid. In order to obtain selective and accurate separation of the feed material into two density fractions, the apparent density of the ferroﬂuid in the working volume of the separator must be constant. This condition will be met if the ﬁeld gradient along the vertical axis is constant, i.e. if conditions (4.61) are met. Therefore, the proﬁle pattern must satisfy eq. (4.77). The practical procedure of designing the pole proﬁle and the magnetic ﬁeld characteristics is as follows: 1. Determine, from eq. (3.145), what ﬁeld gradient [email protected]| is needed to obtain the required density of separation, i.e. the apparent density of the ferroﬂuid. 2. Using [email protected]| = 2D (eq. (4.76)) calculate D= 3. From K = 2Du (eq. (4.71)) calculate K, for a given value of u= The length of the pole tips and the width of the gap between the pole tips are determined by u. The simplest approach would thus be to take u to represent the radius vector of the point of the closest distance O between the pole tips. 4. Based on the condition X = Du2 sin 2 = frqvw., it is possible to calculate the constant from frqvw u0 = (4.78) (sin 20 )[email protected] where u0 is the starting radius vector and 0 is the starting azimuthal angle, as shown in Fig. 4.55. Using this constant, the pole proﬁle is then given by u=

frqvw (sin 2)[email protected]

(4.79)

A similar procedure can be used to construct other pole proﬁles, for instance the isodynamic shape. The role of the mirror plate It follows from the pioneering work of Kaiser and Mir [K18] that a ferromagnetic mirror plate simulates the role of the upper half of the hyperbolic surfaces. Computer modelling of the hyperbolic pole proﬁles has shown [F20] that the presence of the mirror plate negatively aects the constancy of the vertical ﬁeld gradient for the isodynamic ﬁeld pattern. On the other hand, the constancy of the ﬁeld gradient in a magnetic system with constant vertical gradient improved by including the mirror plate. The position of the plate was found to have an inﬂuence on the magnetic characteristics of the circuit, particularly the constancy of the vertical ﬁeld gradient. For the GMUO FHS-40M separator, shown in Fig. 4.60, the optimum distance of the plate from the top of the pole pieces was about 28 mm. On the other hand, the thickness the plate did not aect the magnetic parameters.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

311

Figure 4.60: GMUO FHS-40M ferrohydrostatic separator with a mirror plate.

4.8.4

Scale-up of ferrohydrostatic separators

The application of ferrohydrostatic separation on production scale, particularly for the recovery of non-ferrous metals from automobile or electronic scrap, requires that separators with throughputs of at least 1 t/h, but preferably more, are available. In existing models of FHS, that are based on the iron-yoke concept with the air gap between the pole pieces, the increase in throughput can be accomplished by increasing the gap between the pole pieces. As has been discussed in Section 4.3, the increase in the length of the air gap results in an increase in the ampere-turns and thus of the mass, size and cost of the magnet. With ferrohydrostatic separators, the situation is aggravated even further by the fact that in order to maintain the required ﬁeld gradient, the necessary magnetic ﬁeld increases linearly with dimensions of the air gap. In other words, CK since = 2D for p = 2 (the constant gradient ﬁeld pattern), the magnetic C| ﬁeld strength, given by K = 2Du (eq. (4.71)), required to maintain this gradient, increases with u= The scale-up of a ferrohydrostatic separator by increasing the width of the air gap thus results not only in an increase in the magnetic ﬁeld, with attendant uneconomical increase in the volumes of iron and copper, but also in the increase of the height of the pole pieces well beyond the height of the pool of the ferroﬂuid required for e!cient separation.

312

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS y Separation chamber with ferrofluid

Feed x

z

Solenoid winding

Float

Sink

Figure 4.61: Schematic diagram of a ferrohydrostatic separator with a solenoid magnet [S56].

Solenoid-based FHS It is clear that the design of a large-throughput ferrohydrostatic separator must not be based on a simple increase of the air gap between the pole pieces. A natural approach to the scale-up of FHS would thus be to replace an iron-core magnet by a solenoid magnet as was proposed by Svoboda [S56]. Figure 4.61 illustrates such a solenoid-based FHS separator. A solenoid, and particularly an iron-clad solenoid, has numerous advantages compared to an iron yoke magnet. While it is necessary to increase the air gap in an iron yoke magnet in order to achieve an increase in throughput of material to be separated, with the attendant drawbacks mentioned above, the throughput of a solenoid-based separator can be increased by merely increasing the relevant transverse dimension (diameter) of the solenoid. The axial length (along the | - axis, as shown in Fig. 4.61) of the air gap and thus the number of ampere-turns required to generate a given magnetic ﬁeld remain constant. A solenoid allows the design of the magnetic ﬁeld pattern to be achieved in a simple and accurate manner. Such an approach facilitates the provision of a magnetic ﬁeld gradient which is constant, thereby enabling close control to be maintained over the apparent density of the ferroﬂuid and accordingly over the cut point density. This can be achieved, for example, by precisely designing the winding of the solenoid, or by varying the current density at dierent positions in the winding, or by using a multiple winding arrangement. This is in contrast

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

313

Feed Float 1

FHS 1

Sink 1

Float 2

FHS 2 Sink 2

Figure 4.62: A two-stage ferrohydrostatic separator with solenoid windings [S56]. to iron-core magnets, where approximate solutions of the Laplace equation are used to design approximate shape of pole tips, a task that is further complicated by non-linear magnetization characteristics of iron. The magnetic ﬁeld across the transverse dimension of a solenoid (along the { - axis) is homogeneous in a large region within the solenoid, which means that the same constant apparent density of ferroﬂuid can be achieved across the essentially full transverse dimension. Therefore, almost the entire diameter of the solenoid can be used for separation. This is in contrast to iron-core magnets where the constant gradient exists only at the plane deﬁned by the | - axis and considerable deviations from a constant gradient exist in the proximity of the pole tips. Because of the relatively small mass and size of a solenoid compared to an iron-yoke magnet, it is possible to arrange for two or more FHS units to provide for multi-stage separation, as shown in Fig. 4.62. In this arrangement the top unit, operating, for example, at the apparent density of 8000 kg/m3 > can ﬂoat zinc and sink copper and lead, while copper could be separated from lead into the ﬂoating fraction in the bottom separator operating at the apparent density of 9500 kg/m3 . Computer modelling of the solenoid-based FHS [S8] showed that it is fairly simple to achieve ﬁeld gradients of the order of 3 T/m in su!ciently large volumes of ferroﬂuid. It was also shown that the use of steel cladding considerably

314

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS Grad B B B Grad B

Conventional U-dipole FHS

C-dipole FHS

Figure 4.63: U-dipole magnetic circuit versus C-dipole circuit.

increased this volume in both axial and radial directions. The modelling also conﬁrmed the technical and economic advantages of this design by the use of a superconducting solenoid.

C-dipole-based FHS The scale-up of a conventional iron-yoke-based ferrohydrostatic separator can also be accomplished by re-orienting the U-shaped magnet (Fig. 3.53), to form a C-dipole circuit, as shown in Fig. 4.63. Svoboda [S57] proposed the use of Cdipole magnet to generate a vertical magnetic ﬁeld, the pattern of which can be controlled by appropriate design of the magnetizing coils on upper and/or lower legs of the C-dipole, and/or by controlling the relative polarity of the electrical current ﬂowing through these coils. Appropriate shaping of the pole-tips of the upper and lower pole pieces can also be employed to create a required ﬁeld pattern. The scale-up of such a C-dipole-based separator can be accomplished by merely increasing the length of the magnet Op , and maintaining a constant length of the air gap Oj between the pole-pieces, as shown in Fig. 4.64. The magnetic ﬁeld along the length of the C-dipole is homogeneous, and the same magnetic ﬁeld pattern and apparent density of the ferroﬂuid, along the vertical axis, can be maintained along the full length of the magnet. One possible embodiment of such a concept of the C-dipole FHS is shown in Fig. 4.65.

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

315

Figure 4.64: Schematic diagram of a ferrohydrostatic separator based on a Cdipole magnet [S57].

Figure 4.65: Schematic diagram of a ferrohydrostatic separator based on a Cdipole magnet [S57].

316

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

Figure 4.66: Magnetic circuit of an FHS separator with across-the-pole feeding system.

Figure 4.67: Separation process in the across-the-pole FHS concept [K19].

4.8. DESIGN OF A FERROHYDROSTATIC SEPARATOR

317

Figure 4.68: Layout of the ATP ferrohydrostatic separator [K19].

Figure 4.69: A pilot-plant ATP ferrohydrostatic separator (De Beers Consolidated Mines (Pty.) Ltd.)[K19].

318

CHAPTER 4. DESIGN OF MAGNETIC SEPARATORS

"Across-the-pole" FHS An even simpler concept for overcoming the throughput limitation of the conventional U-pole design of FHS was developed at De Beers Consolidated Mines (Pty.) Ltd. [S8, K19]. By rotating the feed direction through 900 , the throughput increase could be achieved by lengthening the pole pieces rather than increasing the width of the air gap. Figure 4.66 gives a three-dimensional impression of this across-the pole (ATP) concept, while Fig. 4.67 gives a schematic description of the separation process. As can be seen, instead of feeding the material across the width of the air gap of the magnet, the particles are introduced into the ferroﬂuid across the poles. The ﬂoat fraction passes over one of the pole pieces, while the sink fraction is collected underneath in the bottomless separation chamber. An illustration of the layout of the separator is shown in Fig. 4.68. The width of the air gap is determined by the required residence time of material in the ferroﬂuid and remains the same for any length of the pole-pieces, and, therefore, for any throughput of the separator. The magnetic pattern and the apparent density of the ferroﬂuid are determined by the proﬁle of the pole tips, in the same way as in conventional FHS units. A view of the pilot-scale ATP separators is shown in Fig. 4.69.

Chapter 5

Practical Aspects of Magnetic Methods for Materials Treatment Magnetic separation is used in a wide spectrum of areas of material handling whose requirements dier considerably. In general terms, magnetic methods of separation are used in several distinct processes: • Magnetic ﬁltration - recovery of liquid (the magnetizable solids are discarded) - recovery of magnetizable solids (liquid is discarded). • Concentration of a valuable "non-magnetic" component of a mixture by discarding the magnetizable component recovered into the magnetic fraction. • Concentration of magnetizable component into the magnetic fraction and rejection of the "non-magnetic" waste. • Concentration of non-ferrous metals by discarding the non-metallic component of a mixture, and separation of individual non-ferrous metals into individual fractions. • Separation of materials into individual density fractions. The selection of the most appropriate magnetic technique to be used in a given application is a formidable task, and clear deﬁnition of the objective of the process is an important prerequisite for successful choice of the separation technique. 319

320

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

5.1

Selection of magnetic separation technique

There are numerous types of magnetic separators, each one being suitable for only a limited range of applications. The choice is inﬂuenced by a wide variety of factors and the successful operation of a magnetic separator depends, to a great degree, on practical experience. The results of separation cannot generally be accurately predicted. As with most other physical techniques of material treatment, magnetic separation cannot be successfully performed simply on the basis of theoretical models and experience is still the foundation. At present, there is no branch of magnetic separation where theoretical treatment of the subject could be considered entirely adequate. Each magnetic separation technique has its merits as well as limitations; no single technique is applicable to all applications of magnetic separation. The evaluation of magnetic separation as a means of beneﬁciation, or generally of recovering solids, liquids or gases, is often based solely on the data collected from a few brief tests, not always carried out in a suitable magnetic separator. The likelihood of disappointing results and even of rejection of the technique is high, in spite of adaptability and large scope of the magnetic methods of materials manipulation. The choice of magnetic equipment, and the selection of appropriate operating conditions dier widely between these processes. The mode of operation, namely wet or dry, and the throughput requirements impose additional complicating restrictions on the selection of the most suitable magnetic technique. Since particle size of the material to be treated is the most important variable that determines the selection of the magnetic separation technique, the general guidelines of the process selection are based on particle size distribution, as shown in Fig. 5.1. If the size of particles to be manipulated by magnetic separation is greater than, for example, 75 m, we have an option of a dry or wet process. If, however, the particles are ﬁner than 75 m, the wet technique is more appropriate, although this threshold particle size can be smaller or greater than 75 m, depending upon the amounts of the ﬁnes present in the feed and on the physical properties of the feed. The subsequent choice of the magnetic separation technique depends on the magnetic properties of the material. If a strongly magnetic component is present in the feed, low-intensity drum magnetic separators can be used, either in wet or dry modes of operation. Coarse, weakly magnetic materials can be treated by wet roll magnetic separators, rare-earth drum separators and possibly by wet high-intensity highgradient magnetic separators. In the latter technique, there is an upper limit imposed on the particle size by the type of the matrix and particles greater than 1 mm usually cause clogging, even of a coarse matrix. In a dry mode, coarse weakly magnetic particles can be recovered by a variety of high-intensity magnetic separators, including induced magnetic roll, cross-

5.2. DRY MAGNETIC SEPARATION

321

Strongly magnetic

LIMS, Chute

Weakly magnetic

Wet roll MS, WHIMS, HGMS, REDs

Strongly magnetic

LIMS, Suspended, Pulley, Grate, Roll MS

Weakly magnetic

Roll, REDS, Cross-belt, IMR, OGMS, HGMS

Strongly magnetic

LIMS

Weakly magnetic

REDS, WHIMS, HGMS

Wet

> 75 µm

Dry Particle size

< 75 µm

Wet

Figure 5.1: Classiﬁcation of magnetic separation processes (adapted from Svoboda [S1]). belt separator, permanent magnet roll separator, rare-earth drum separator and open-gradient magnetic separator. If the particles are ﬁner than 75 m, the best approach is to use wet magnetic separation. Fine, strongly magnetic particles are usually recovered by wet lowintensity drum separators, while for weakly magnetic materials the wet highintensity or high-gradient magnetic separation is appropriate. The decision making process for selection of the magnetic separation technique is schematically shown in Fig. 5.2.

5.2

Dry magnetic separation

Dry magnetic separation is a technique dating back to the beginning of the last century. It has been practiced successfully in the removal of tramp iron from process streams, in beneﬁciation of strongly magnetic minerals, as well as feebly magnetic minerals such wolframite, cassiterite or ilmenite. Puriﬁcation of numerous industrial minerals, such as andalusite, glass sand, ﬂuorspar, feldspar, diamonds and others, by removing ﬁne strongly magnetic impurities, is very often carried out in a dry mode. More recently developed eddy-current separators also operate in a dry mode. For dry magnetic separation to be successful, the material must be com-

322

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Magnetic separation

Yes Wet MS

Particle < 75 um No

No

Strongly magnetic?

Is dry process required?

Yes

Yes Dry MS

No LIMS

Yes Wet MS

WHIMS HGMS

Strongly magnetic? No

Yes

Strongly magnetic? No

LIMS Plate Chute

WHIMS HGMS REDS Wet roll

IMR Roll REDS Cross-belt Disc OGMS HGMS

LIMS Pulley Suspended Grate Plate Roll

Figure 5.2: Selection of magnetic separation techniques (adapted from Svoboda [S1]).

5.2. DRY MAGNETIC SEPARATION

323

pletely dry, which sometimes involves an expensive heating stage. For particles smaller than a certain threshold size (for instance 75 m), the attractive electrostatic and van der Waals forces will cause sticking and the formation of aggregates. Selectivity of separation can thus be severely aected. Dry processes often require the material to be sized into several rather narrow size fractions, each of which must be spread in a monolayer over the separating surface. It is a well-established fact that when magnetic separation is performed on materials sized into, for example, three or more fractions, the e!ciency of separation is usually much improved in comparison with unsized samples. The loading of the separating surface, such as belt or drum, inﬂuences the throughput and the e!ciency of the separation, and a compromise must be found between these contradictory requirements. As a rule of thumb, when the particles are introduced onto a belt in a monolayer, a safe belt loading (portion of the belt covered with feed particles) should be approximately 25%, even when the feed contains a high percentage of the magnetic material. As a rule, a larger proportion of dry ﬁnes necessitates higher rotating speeds of a roll or drum. Although increase in speed will improve the grade of the magnetic product and the throughput of the separator, it will also increase the losses of the magnetic component. The recovery can be improved by re-treating the non-magnetic fraction in a second stage. On the other hand, when the valuable product is the non-magnetic fraction, high speed of rotation will result in high recovery and poor selectivity of separation. The grade of the concentrate can be improved by cleaning the non-magnetic fraction in the second pass.

5.2.1

Electrostatic phenomena in dry separation

During dry material handling operations, the dielectric particles invariably become electrostatically charged. The dominant charging mechanisms are triboelectriﬁcation (or frictional charging) and contact charging. These mechanisms can happen during any dynamic contact of surfaces, such as sliding, rolling and vibration of surfaces at contact. When two dissimilar dielectric materials make and then break contact, charge transfer from one of the materials to the other takes place. This is not to say that conductors will not charge by contact electriﬁcation - they usually charge - but since they are conductors, they often lose their charge quickly. While physical mechanisms of contact charging are well understood, triboelectriﬁcation, the oldest form of charging, is poorly understood and explanations are of phenomenological nature. One of the controversial rules of thumb often used for predicting the sign of the surface charge resulting from contact electriﬁcation is Coehn’s rule, which states that "when two dielectric materials are contacted and separated, the material with the higher dielectric constant becomes positively charged" [L12]. Coehn’s rule was quantitatively formulated as v = 15 × 106 (u1 u2 ) (5.1) where v is the surface charge density (in [F/m2 ]) and u1 and u2 are dielectric

324

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.1: Dielectric constants of selected materials. Material Water TiO2 Barium titanate Carbon Ilmenite Chromite Rutile Zircon Glass Quartz Hematite Limestone Fluorspar Bakelite Perspex

Dielectric constant u 80.4 90 1200 5.7 33.7 to 81 11 89 to 173 12.6 4 to 6 4.3 25 6.1 7.4 4.9 3.4

constants (relative permittivities). Although Coehn’s rule is reported to have been veriﬁed for more then 400 substances [L12], it is of limited value to the metallurgist because of the difﬁculty in determining the relative permittivities of the surface layers of two materials that are to make contact. Typical values of dielectric constant of selected materials are shown in Table 5.1. Sometimes several materials can be arranged into the so-called triboelectrical series such that each material is charged positively when it is rubbed against the previous one. Examples of such series are: • zinc-glass-cotton-ﬁlter-paper-silk-zinc [B26] and • teﬂon-metals-resins-wood-mica-quartz-glass [H19]. The triboelectric charging behaviour of materials is generally sensitive to an atmospheric environment. At high values of relative humidity, considerable negative charging takes place. At low values of relative humidity, although ﬁne particles still charge negatively, the coarse particles show a change of charging polarity such that the net charge conveyed by the powder material is positive [B27]. When a particle undergoes charging during handling, the charge transferred at the particle contact point will re-distribute itself over the particle surface by electrostatic forces. The rate at which re-distribution proceeds depends on the relaxation time h (in [s]) given by h = u 0 (

(5.2)

5.2. DRY MAGNETIC SEPARATION

325

Figure 5.3: The eect of moisture on the grade of the magnetic concentrate obtained from - 2 mm magnetite and martite ores treated by crossbelt and induced magnetic roll separators (adapted from [D4]). where ( is the resistivity of the material (in [ m]) and u its relative permittivity (dielectric constant) and 0 = 8.85×1012 F/m is permittivity of vacuum. The time dependence of the surface charge density, after completion of the charge transfer, is given by: v = 0 exp([email protected] h )

(5.3)

where 0 is the surface charge density at w = 0. As a general rule, if electrostatic phenomena arise in a material handling situation, they are likely to become increasingly signiﬁcant as particle size decreases. Particles charged triboelectrically, either positively or negatively, may adhere strongly to surfaces. Moisture contributes to the strength of adhesion and Fig. 5.3 illustrates the eect of moisture on selectivity of dry magnetic separation. It can be seen that the grade of the magnetic concentrate is seriously impaired by the presence of moisture and the permissible moisture content decreases with decreasing particle size. For instance, if an ore with size distribution - 20 mm can tolerate 4% of moisture, then the maximum moisture content in a ﬁne ore - 2 mm should not exceed 1% [D4]. The eect of air humidity The moisture concentration in an ore is also inﬂuenced by the relative humidity of the air. This is a consequence of the capillary attraction between particles, which results in adsorption and subsequent capillary condensation of the water vapours in the particle contact area. If the force of capillary attraction Ik

326

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.4: The eect of air humidity on dry magnetic separation of magnetitequartz mixtures, for dierent values of particle radii (adapted from [V10]). between a non-magnetic particle and a magnetic particle is greater than its weight J, the non-magnetic particle will report in the magnetic fraction. The force Ik is the sum of of the surface tension and the Laplace pressure force: Ik = 8u1 + 4u22 (

1 1 ) u2 u1

where ul (l = 1 and 2) are the radii of the curvatures of the meniscus between the contacting particles 1 and 2, and is the surface tension (in N/m) of the ﬂuid. Experimental investigation [V10] of the eect of the air humidity on dry magnetic separation of magnetite-quartz mixtures, as a function of particle size, conﬁrmed that the e!ciency of separation varies linearly with the ratio J/Ik = It can be seen from the results illustrated in Fig. 5.4 that with increasing humidity, the separation e!ciency decreases steeply. The eect of the air humidity becomes particularly pronounced with decreasing particle size.

5.2.2

Density and magnetic tracers

The use of the Tromp curve, or partition curve, is a well established practice for the evaluation and representation of gravity concentration processes. The partition curve can be conveniently constructed with the aid of density tracers [N15]. The density tracers are manufactured as cubes in sizes ranging from 0.8

5.2. DRY MAGNETIC SEPARATION

327

to 20 mm. They are colour-coded according to the magnitude of their density and are commercially available, for example from Bateman Engineering (Pty.) Ltd. (South Africa), in the density range from 1300 kg/m3 to 4000 kg/m3 , with density interval of 50 kg/m3 . Partition Enterprises (Pty.) Ltd. (Australia) supply density tracers that are strongly magnetic for easy recovery, by magnetic means, from density separation products. The partition number, or the percentage recovery U into the concentrate, for each size and density fraction, is usually determined as U = 100

qf qf + qw

where qf and qw are the numbers of tracers in the concentrate and in the tailings, respectively. Magnetic tracers, which have become commercially available only recently, can be used, in a fashion similar to the way density tracers are used in gravity concentration, to determine and optimize the separation e!ciency of magnetic separators. A magnetic tracer is a simulant designed to have the same size and magnetic susceptibility as the material which is being recovered or removed in a magnetic separator. Magnetic tracers of mass magnetic susceptibility ranging from 2.5×107 m3 /kg to 125.5×107 m3 /kg (20×106 cm3 /g to 1000×106 cm3 /g), in steps of 2.5×107 m3 /kg, for low-susceptibility tracers, and 12.5×107 m3 /kg for high susceptibility tracers, are available from Bateman Engineering (Pty.) Ltd., South Africa [D12]. These tracers, whose size ranges from 1 mm to 20 mm, are colour- and shape-coded, according to the magnitude of their magnetic susceptibility for easy evaluation of the separation process. Tracers smaller than 1 mm are impractical as they cannot be easily identiﬁed among the mineral particles. The magnetic partition curve can be constructed using the partition numbers, or percentage recovery into magnetic or non-magnetic fractions. In terms of the recovery of the tracers into the magnetic fraction, for example, the partition number, for a given size and magnetic susceptibility, is expressed as: U = 100

qpdj qpdj + qqrqpdj

where qpdj and qqrqpdj are the numbers of tracers in the magnetic and nonmagnetic fractions, respectively. The probable error of separation is given by eq. (4.58). While magnetic tracers are ideally suited for quantiﬁcation of the e!ciency of a magnetic separation process, their practical use is restricted to the separation of materials coarser than 1 mm. Although they can be used to evaluate the e!ciency of separation of even ﬁner materials in dry separators such as roll and drum, the particle-size dependence of the magnetic susceptibility cut point can result in considerable inaccuracy of the audit. In wet separators, such as low-intensity drum separators or WHIMS or HGMS, even the smallest 1 mm magnetic tracers would interfere with the separation process

328

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.5: Comparative metallurgical e!ciencies of various dry magnetic separators as applied to apatite recovery (adapted from Roux et al. [R19]).

5.2.3

Comparison of dry magnetic separation techniques

The minerals industry has always had a great need to beneﬁciate coarse, weakly magnetic minerals and a wide spectrum of dry magnetic separators has been developed over the years. The range of various types of separators, based on dierent principles of the generation of the magnetic ﬁeld, makes a correct choice of the most suitable technique a di!cult task. Comparisons of the separation e!ciencies of dierent techniques are usually not published and if they are, caution should be exercised when taking these comparisons at face value. Every comparison is only conditional since the relative merit of each technique is a function of the mineral to be treated and its physical properties. Sometimes comparisons are oered by manufacturers of magnetic separators who might be biased towards their own product. Comparison of dry separators for beneﬁciation of the pyroxenite ore One of the rare comprehensive comparative production-scale exercises was conducted by Roux et al. [R19]. In order to beneﬁciate pyroxenite ore to yield apatite concentrate, several dry magnetic separators were tested at Foskor (South Africa). Figure 5.5 summarizes the metallurgical e!ciencies of dierent types of separators, while Fig. 5.6 shows the relationship between phosphate recovery and particle size for IMR, HGMS and OGMS machines. A thorough practical experience with these magnetic separators was gained at Foskor and their

5.2. DRY MAGNETIC SEPARATION

329

Figure 5.6: Phosphate recovery as a function of particle size for various magnetic separators (adapted from Roux et al. [R19]). comparison is summarized in Table 5.2. A gradual deterioration in the results was observed with IMR, caused by abrasive wear on the epoxy ﬁller between the steel discs of the rolls. Furthermore, because the separation distance between the magnetics and non-magnetics is very small, a precision setting of a splitter was required. As the mineralogy of the ore varies, constant attention to the optimization of roll speed and splitter settings was required, which made it di!cult to maintain good metallurgy [R19]. A Sala HGMS 120-15 operated reliably and well for 1000 hours and it was found that single-stage separation yielded metallurgical results equivalent to that of two stages of IMR separation. The expanded metal matrix showed no measurable wear, while the metallurgy was shown to be adversely aected by oversize material, which gradually accumulated in the matrix. In order to keep coarse particles out of the feed, and to avoid the onerous task of cleaning the matrix chambers, it became necessary to ﬁt a second screen which could be kept under continuous visual observation. An extensive series of experiments with SmCo permanent roll separators showed that the feed rate, roll speed and thickness of the magnet and steel rings must be optimized for each separation stage. The open-gradient, split-coil superconducting magnet separator was tested in two modes, shown in Chapter 2 in Fig. 2.85(a) and (b). The free-fall system gave acceptable metallurgical results only at very low feed rates. A much more satisfactory ore presentation system was found to be the one in which the ore slid down a ramp, as shown in Fig. 2.85(b). The ramp imparts an outward

330

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.2: Comparison of dierent types of dry magnetic separators, as applied to phosphate recovery (after Roux et al. [R19]). Parameter Capacity Power input Ore distribution Mass [kg] per t/h of feed Sensitivity to ore variation Recovery of the ﬁnes

IMR Low, 4 t/h/m 2 kW/t Complex 2200

RE Roll Low, 8 t/h/m 0.6 kWh/t Complex 440

HGMS High, 400 t/h 5.6 kWh/t Simple 4100

OGMS High, 60 t/h

High

Low

Low

Very high

Poor

Very poor

Good

Very poor

0.5 kWh/t Simple 41

Table 5.3: Comparison of IMR and RE roll in ilmenite-rutile separation (after Arvidson [A26]). Product Magnetics (mass %) Non-mags in mags (%) Middlings (%) Non-magnetics (%) Mags in non-mags (%)

IMR @ 2.5 t/m/h 25 2.5 10 65 0.5

RE roll @ 4 t/h/m 30.5 0.46 0.8 68.7 0.28

velocity to the particles, thereby counteracting, to a considerable extent, the sweeping across of non-magnetic particles by the magnetic ones. This approach made it possible to obtain metallurgical results comparable with those of IMR separators, at feed rates of up to 6 t/h per meter width, or 3.5 times the optimum feed rate of an IMR. Comparison of dry separators for beneﬁciation of beach sands and other industrial minerals. High-intensity magnetic separation has been a standard beneﬁciation method for heavy mineral sands and various industrial minerals, and a variety of dry magnetic separators has been used. With the advent of aordable rare-earth permanent magnets, and as a result of design improvements, the conventional dry separators, such as induced magnetic roll and cross-belt separators are being replaced by reliable and economical rare-earth roll and drum separators [A24, A25, A26]. Although the plant data are usually conﬁdential, comparative studies indicate superior performance of the rare-earth-based separators. An example is shown in Table 5.3, which compares the separation e!ciency of IMR and RE roll separators as applied to ilmenite and rutile separation. A similar improvement in the e!ciency of separation after replacing the induced magnetic roll with a permanent magnetic roll, was obtained with feldspar.

5.2. DRY MAGNETIC SEPARATION

331

Table 5.4: Comparison of IMR and RE roll magnetic separation as applied to beneﬁciation of feldspar [A24]. Product Magnetic fraction Non-magnetic fraction

IMR 12% - 14% 86% - 88%

RE Roll 4% - 4.5% 95.5% - 96%

Table 5.5: Reduction of the iron content in various size fractions of feldspar, by IMR and roll permanent magnetic separators. IMR was operated at 1.8 T [A27]. Separator

Fraction [m]

Fe oxides in feed [%]

IMR

- 500 + 212 - 212 + 106 - 106 + 74 - 500 + 212 - 212 + 106 - 106 + 74

0.20 0.43 0.45 0.20 0.43 0.45

Roll

Yield into non-mags [%] 95.5 93.0 82.3 86.6 85.8 79.5

Fe oxides in non-mags [%] 0.04 0.06 0.07 0.08 0.10 0.11

This is shown in Table 5.4. On the other hand, results of another comparative study [A27], summarized in Table 5.5, indicate a superior performance of an induced magnetic roll, in the entire range of particle sizes. Dry magnetic separators can also be e!ciently used to recover metal from slags. Comparison of several dry separation techniques to recover ferrochrome from coarse slag is shown in Table 5.6 [S58]. A dry ferrite roll separator was also successfully applied to the recovery of the ferrochrome metallics from a ﬁne fraction (- 0.8 mm) of slag. Comparison of its performance with a wet rare-earth drum separator is shown in Table 5.7. Replacement of conventional electromagnet-based separators by rare-earth permanent magnet units also often results in economic advantages. Improved quality of the ilmenite concentrate and reduced operating costs contribute to improved plant e!ciency, as shown in Table 5.8. Additional cost savings result

Table 5.6: Recovery of ferrochrome metal from slag (- 15 + 2 mm) by magnetic separation [S58]. Separator Dry LIMS Lifting IMR Ferrite roll

Head grade [ FeCr %] 22.7 20.1 27.1

Mags grade [ FeCr %] 60.6 77.6 45.7

Recovery [%] 85.0 85.8 97.5

332

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.7: Recovery of ferrochrome metal from ﬁne slag (- 0.8 mm) by magnetic separation [S58]. Separator Ferrite roll Wet RE drum

Head grade [ FeCr %] 4.4 4.7

Mags grade [ FeCr %] 16.9 17.3

Recovery [%] 65.6 70.2

Table 5.8: Comparison of the operating costs of various dry magnetic separators applied to ilmenite beneﬁciation, in relation to a cross-belt separator [A24]. Magnetic separator Cross-belt IMR RE drum separator RE roll (short belt life) RE roll (long belt life)

Cost 100 42 to 53 17 21 to 42 11 to 15

from a smaller size of the plant for a given throughput. Since a plant with rare-earth magnetic separators would use between 6% and 20% of a cross-belt plant space [A24], the cost saving can be considerable. Compared to IMR for non-magnetic cleaning applications, the space saving can be 50% to 70% [A24]. Improved performance can be also obtained by implementing multiple-stage separation, as is demonstrated in Fig. 5.7. Combined with higher roll speeds, the selectivity of separation increases in addition to a higher throughput. In some applications, it was found advantageous to combine rare-earth roll separators with rare-earth drum separators. While roll separators tend to be more e!cient, more selective and can be more readily adjusted to feed variations, drum separators have a higher throughput and are less demanding from the maintenance point of view. Comparison of the roll and roll+drum options is shown in Table 5.9.

Table 5.9: Comparison of roll and roll+drum alternatives for treatment of ilmenite gravity concentrate (- 0.9 + 0.1 mm), at 30 t/h, in 1999 prices [A25]. Parameter Stages required Capacity Quantity Price per unit [US$] Total price [US$]

Drum + Roll 1 drum + 2 rolls 7 t/h/m 3 $114 000.00 $342 000.00

Roll separator only 3 stages 4 t/h/m 5 $65 000.00 $325 000.00

5.2. DRY MAGNETIC SEPARATION

333

Figure 5.7: Comparison of single and multiple-pass separation of ilmenite, by a roll separator, at dierent feed rates (adapted from Arvidson [A26]). Comparison of roll and matrix separators Jirestig and Forssberg [J7] carried out a detailed comparative study of four dry high-intensity magnetic separators. Three of these separators were roll units: R R ° ° Permroll (E.L. Bateman) with Kevlar belt, High Force (Inprosys) with polyurethane belt, induced magnetic roll (Humboldt Wedag) and dry HGMS (Sala). An expanded metal matrix, with and without spacers, was used in the Sala HGMS and particles were propelled through the matrix by a compressed air-driven vacuum pump. Various size fractions of calcite and dolomite samples were used as test materials. Permroll, High force and dry HGMS, operating at 2 T yielded products of similar brightness for ﬁne to medium-size (- 450 + 38 m) particles, as can be seen in Fig. 5.8. For particles larger than 450 m, the Sala HGMS machine experienced problems with matrix clogging, while the e!ciency of the induced magnetic roll was slightly inferior. The signiﬁcant advantage of the matrix separator, compared to belt-type separators, is its high selectivity of separation of ﬁne particles, smaller than 100 m. The high brightness of products from belt separators was achieved at great cost to the recovery. Only about 5% of 38 m material reported to the magnetic fraction in the matrix separator, while Permroll and High Force machines experienced signiﬁcant losses (35% to 80 %) of the valuable material into the magnetic tailings. The dierent performances of the two belt separators are probably due to dierent types of belts used and the results indicate the importance of controlling electrostatic properties of the belt material, as discussed in Section 5.2.1.

334

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.8: Brightness of various size fractions of the calcite non-magnetic product, as obtained in several dry magnetic separators (adapted from Jirestig and Forssberg [J7]). Comparison of rolls of dierent diameters Magnetic rolls of diameter ranging from 72 mm to 300 mm are commercially available and judicious selection of the most suitable unit is essential for optimum metallurgical results and operating costs. Figures 5.9 and 5.10 illustrate that magnetic rolls of larger diameter (300 mm) can operate at higher feed rates than standard 76 and 100 mm diameter rolls. By increasing the speed of rotation the same performance can be maintained. As has been discussed in Section 4.6.2, the magnetic force is practically independent of the magnetic ring diameter. The increase in the rotational speed of the roll, maintaining the same residence time of particles in the magnetic ﬁeld as in a smaller diameter roll, results in the increase of the centrifugal force on a particle. In turn, this results in a closer balance of the magnetic and competing forces and better selectivity of separation can thus be obtained. This additional beneﬁt of larger ring diameters is depicted in Fig. 5.10. Comparison of RE roll and RE drum separators Rare-earth roll separators and rare-earth drum separators are designed to address similar beneﬁciation applications. The choice between these two types of separators is rarely made on the basis of comprehensive comparative tests. Since the pattern of the magnetic force around the roll and drum dier considerably, correct systematic evaluation of the operation is essential. As has been discussed in Section 4.6.2, magnetic roll separators generate a much higher mag-

5.2. DRY MAGNETIC SEPARATION

335

Figure 5.9: Comparison of separation e!ciencies of magnetic rolls of diameters 100 and 300 mm, at dierent throughputs, as applied to beneﬁciation of - 3 mm iron ore (adapted from Arvidson and Dillé [A23]).

Figure 5.10: Comparison of performances of 76 mm and 300 mm rolls at dierent speeds of rotation, applied to puriﬁcation of - 600 + 800 mm silica sand (adapted from Dobney [D8]).

336

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.11: Magnetic partition curves. The ideal curve corresponds to a magnetic susceptibility cut-point of "50 = 80×106 cm3 /g (10×107 m3 /kg) [M24].

netic force, which, however, is of short reach. On the other hand, the magnetic force on the surface of a drum separator is much lower, as a result of a considerably lower magnetic ﬁeld gradient. The reach of the force is, however, much longer than that in a roll separator. The behaviour of particles in these two types of separator is dierent and the settings of the optimum operating conditions dier widely. Detailed comparative tests on rare earth roll and drum separators were conducted by Murariu and Svoboda [M24]. Magnetic tracers of various sizes and mass magnetic susceptibilities were used to set the optimum operating conditions, and magnetic partition curves were generated. The values of Hs, given by eq. (4.58), of these curves were compared. Figure 5.11 illustrates such a partition curve for the cut-point magnetic susceptibility of 80×106 cm3 /g (10×107 m3 /kg). The cut-point is deﬁned as the value of magnetic susceptibility ("50 ), for which the particles having this susceptibility split equally into the magnetic and non-magnetic fractions. It was observed that the same cut point could be obtained using dierent combinations of the speed of rotation of the drum or roll and of the position of the splitter. However, not all combinations of these parameters give the same optimum e!ciency of separation, as is demonstrated by Fig. 5.12. It can be seen that, for a drum separator, a lower speed and a closer position of the splitter between the magnetic and non-magnetic fractions, result in lower Hs and thus

5.2. DRY MAGNETIC SEPARATION

337

Figure 5.12: Experimental partition curves for an NdFeB drum magnetic separator. The curves were obtained for the same value of the cut point, but for dierent positions of the splitter and the rotational speed of the drum. Drum diameter: 600 mm, magnetic induction on the drum surface: 0.9 T [M24]. a more e!cient separation. However, with a roll separator (diameter 100 mm), a more selective separation was achieved at a high roll speed and with a splitter far from the roll. This dierence in the optimum operations of drum and roll magnetic separators results from the fact that the magnitude of the magnetic force acting on a particle in a drum is much smaller than that in a roll separator. As discussed in Section 1.2, the separation is selective when the magnitudes of the magnetic force and the competing forces are of comparable magnitudes. The magnetic roll, which generates a higher magnetic force than the drum, requires a higher centrifugal force (i.e. a higher roll speed) and a more distant position of the splitter. Tracer tests showed that the setting of the cut point, that is of the rotation speed of the roll or drum and position of the splitter, is dependent on particle size. The size dependence was found to be approximately linear for both separators, as is illustrated in Fig. 5.13. The slope of the plots indicates sensitivity of a separator to the size of the tracers. It can be seen that roll magnetic separators are considerably more sensitive to particle size and the sensitivity increases with decreasing thicknesses of the magnet and steel rings. A roll separator of a given conﬁguration is, therefore, suitable for accurate separation of only a narrow size range of the feed particles. For example, if the cut point is set to 10×107 m3 /kg (80×106 cm3 /g) and the required accuracy is ± 10% (two horizontal lines in Fig. 5.13), a roll separator with conﬁguration 12/7.5 will satisfy the accuracy

338

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.13: Variation of the cut-point magnetic susceptibility with the size of magnetic tracers, for roll and drum magnetic separators of dierent conﬁgurations [M24].

requirement for a size fraction - 6 + 4 mm. A roll separator with conﬁguration 4/2.5 will meet this requirement only for particle size of 2 mm. On the other hand, the drum separator will be able to treat selectively a size fraction of - 16 + 8 mm.

The loading of the belt or the drum The loading of the drum and of the belt of the roll separator, inﬂuences the throughput and the e!ciency of separation, and a compromise must be found between these two contradictory requirements. As a result of a short residence time of particles on the roll surface, the feed material must be distributed evenly over the belt in a monolayer and a safe belt loading is approximately 25%. Lower belt loadings lead to a low throughput and generally cannot be justiﬁed in view of a limited beneﬁt and high cost of the separator. In drum separators, the residence time is much longer and if the feeding system is optimized and the feeder tray is su!ciently close to the drum, to avoid particle bouncing, the particles usually spread evenly on the drum surface even when particles ﬂow in a thicker layer on the feeder tray. Typical ﬂow of material onto a drum surface is shown in Figs. 5.14 and 5.15. However, adherence of strongly magnetic particles on the drum surface can be a problem, as shown in Fig. 5.16.

5.2. DRY MAGNETIC SEPARATION

339

Figure 5.14: Flow of the - 2 + 1 mm material on the surface of an NdFeB drum magnetic separator.

Figure 5.15: Flow of the - 16 + 8 mm material on the surface of an NdFeB drum magnetic separator.

340

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.16: Attachment of strongly magnetic particles to the surface of a drum magnetic separator. Throughput of a roll separator The throughput of a roll separator is determined by a variety of factors and only experimental determination can give reliable information on this important speciﬁcation. The general formula for throughput calculation is Ys s zyi F= (5.4) Ds where F is the throughput (in [kg/s]), Ys is the particle volume (in [m3 ]), s is the particle density (in [kg/m3 ]), z is the belt width (in [m]), y is the belt speed (in [m/s]), Ds is the cross-sectional area of a particle (in [m2 ]) and i is the ﬁlling factor of the belt. It is evident from this equation that the shape of the particles must be known before the throughput can be calculated. Belt tracking As the belts used in roll magnetic separators are frequently very thin, usually between 0.13 mm and 0.25 mm, they are prone to wear and their life time is often short. Accumulation of dust and magnetic particles underneath the belt and misalignment of the belt, result not only in impaired separation performance but also cause damage to the belt. Various manufacturers of roll separators use dierent mechanisms for the belt tracking, with dierent levels of resistance to misalignment. Considerable eort has been expended to extend the wear life by developing and applying correct tracking system. Crown idler rolls have been used successfully for many years, particularly for small diameter rolls and for separators with a large distance between the

5.2. DRY MAGNETIC SEPARATION

341

Figure 5.17: The temperature of the shell of an NdFeB drum magnetic separator, as a function of time. Drum diameter: 600 mm, magnetic induction on the shell: 0.9 T, speed of rotation: 50 rpm [M24]. roll and the idler. With the advent of large diameter rolls (e.g. 300 mm), the conventional crowned idler system has been replaced, for rolls longer than 0.5 mm, by a self-adjusting roller system [A23, A13]. Depending on the application, the average lifetime of a thin belt (0.13 mm) ranges from one month to six months, while a thicker belt (0.25 mm) can last as long as 12 months [A24]. The changing of a damaged belt can also be an onerous and time-consuming exercise. It is claimed, however, that the belt changing time for a one meter long roll can be shorter than 5 minutes [D8]. Eddy currents and temperature increase in the drum shell It has frequently been observed that the temperature of the shell of drum magnetic separators increases during operation. This phenomenon is based on the fact that as the metallic shell of a drum separator rotates around a stationary magnetic system, eddy currents are developed in the shell. These eddy currents are generated in such a way that the magnetic ﬁeld they produce opposes the external magnetic ﬁeld, as discussed in Section 2.7. This interaction energy is converted into heat which might be detrimental to operation of a drum magnetic separator and it could reduce the lifetime of the permanent magnet material. This is of particular importance for high-ﬁeld rare-earth drum separators which are often operated at higher rotational speeds than low-intensity magnetic drum separators. Figure 5.17 illustrates the temperature development on the surface of the shell of an NdFeB drum separator [M24]. The temperature was measured by

342

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

a thermocouple as a function of time over a period of eight hours. The temperature increased rapidly within the ﬁrst 30 minutes of operation from the room temperature of 24 0 C to 36 0 C. Afterwards, the temperature kept increasing asymptotically to the temperature of 45 0 C, which remained constant after eight hours. While the temperature within the permanent magnet material inside the drum will be higher than on the shell surface, it is probably still well below the critical operational temperature of the permanent magnet material. Nevertheless, caution should be exercised in this aspect. The eect of the increased temperature of the magnetic system on the separation e!ciency was investigated using 8 mm magnetic tracers and - 4 + 2 mm kimberlite gravel [M24]. It was found that the experimental partition curves determined at room temperature and after six hours of the drum operation, exhibited the same cut-point magnetic susceptibility. Also, the mass recoveries of the gravel into the magnetic fraction were identical, indicating that the separation e!ciency was not aected by the increased temperature of the drum.

5.3

Wet magnetic separation

As shown in Fig. 5.1, wet magnetic separation can be applied to coarse as well as ﬁne particles, that are either strongly or weakly magnetic. Strongly magnetic materials can be recovered by wet low-intensity machines, which are by far the most common in use. Weakly magnetic particles, coarse or ﬁne, can be treated by rare-earth drum magnetic separators, while wet high-intensity magnetic separators (WHIMS) and high-gradient magnetic separators (HGMS) are applied, as a rule, to ﬁne weakly magnetic materials only.

5.3.1

Wet low-intensity drum magnetic separation

Wet low-intensity drum magnetic separators (LIMS) are used to recover strongly magnetic solids from a slurry feed. The major areas of application are media recovery in dense media separation plants (DMS) and in magnetite ore beneﬁciation. Physical construction of wet drum separators is slightly dierent for the two applications, with the ore concentrator being more rugged in construction and subject to more detailed speciﬁcations than the media recovery units. This is particularly true with reference to feed and collection tank design, bearing construction, wear covers on the drums, magnet assembly design and magnetic ﬁeld strength rating. On the other hand, modern LIMS machines for DMS plant operation have a longer pick-up zone [D13], compared to the conventional separators. Wet magnetic drum separators for media recovery In media recovery application the particle size of the feed, particularly the magnetic portion, is quite ﬁne and drum wear is not a serious problem. Maximum magnetic recovery is important, and the highest magnetic purity and solids content in the magnetic concentrate is desired.

5.3. WET MAGNETIC SEPARATION

343

Table 5.10: Maximum concentration of solids in the feed into LIMS for dense media recovery [S59]. Separator Con-current Counter-rotation Double drum

Max. solids concentration [% by weight] 20 25 50

Factors that are considered in selecting a wet drum separator for media recovery are: • Percentage of solids in the feed slurry • Percentage of magnetics in the feed solids • Grade of the media used • Feed volume (m3 @h) to the separator • Magnetic discharge rate (t/h) from the separator • Desired magnetic recovery. Media recovery magnetic drums are available in diameters of 762 mm (30"), 914 mm (36") and 1219 mm (48"), and in drum widths up to 3050 mm (120"). A 1200 mm diameter magnetic separator has approximately twice the capacity of a 900 mm unit. This allows circuits to be designed with fewer magnetic separators and therefore with reduced vulnerability to mechanical failure, uneven feed distribution and poor control [D13]. Both con- and counter-current feed arrangements have been used. The concurrent drum arrangement usually gives the highest magnetic content in the magnetic discharge and provides the highest percentage of solids in the discharge. The overwhelming majority of the magnetic separators installed in DMS plants has been of the con-current design. The counter-rotation units have been used successfully as secondary separators [D13]. Solids content in the feed For e!cient operation of the DMS plant it is desirable to keep the media as free of ﬁnes as possible. The reduced concentration of ﬁnes limits the viscosity problem and results in sharper separation. It also improves the magnetic recovery by the magnetic drum and gives a cleaner magnetic concentrate. Typically, a single LIMS will be used in plants where the feed solids are in the 10% to 15% range. It is signiﬁcant to note that an extremely dilute feed makes the magnetic recovery more di!cult and the feed volume should be reduced by a factor of 0.5 to 0.75 for such a dilute feed [B28, M26]. For solids in the 20% to 25% range, either 900 mm diameter single drum or 760 mm diameter double drum units are recommended. Above 25% solids, 900

344

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Table 5.11: Recovery of ferrosilicon in a magnetic separator at low concentration of the magnetics in the feed [D13]. Mags in the feed [g/c] 55 38 5 2 0.5

Recovery [%] 98.8 98.0 92.0 67.0 56.0

Mags in e"uent [%] 0.83 0.76 0.40 0.67 0.22

Table 5.12: Suggested feed volumes into LIMS for dense media recovery [B28, M26]. Separator 762 mm single drum 914 mm single drum 762 mm double drum 914 mm double drum

Feed rate [m3 /h/m] 50 - 55 55 - 70 55 - 70 70 - 95

mm diameter double drum are advised. The suggested maximum concentrations of solids in the feed are shown in Table 5.10. Magnetic content of the feed solids Typically, the magnetic content of solids will be 60% or higher. When the magnetic content of the solids falls below 60%, the feed volume should be reduced and multi-drum arrangement considered, in order to maintain a high magnetic recovery. Table 5.11 illustrates the detrimental eect of low concentrations of the magnetics on their recovery. It is well established that the magnetics-to-ore ratio and the solids content are two parameters that control concentrate purity most eectively [S59]. Recommended feed volume and discharge rate of the magnetics In selecting drum size for media recovery, the feed volume and magnetic solids discharge should be balanced. In Table 5.12. typical feed rates are suggested for various single and double wet low-intensity magnetic separators. Magnetic discharge rates should not exceed the rates given in Table 5.13, in order to maintain high magnetic media recovery. The eect of the magnet position Plant experience conﬁrms that the initial settings of a drum magnetic separator, recommended by manufacturers, are only a rough guide. Settings of such parameters as the magnet position and drum-to-tank clearance should be optimized based upon the plant experience. For instance, it was found by Dardis [D13] that the magnet position signiﬁcantly inﬂuenced tailings losses and the return density of the concentrate. Two minima in the loss curve were observed [D13], corresponding to the minima in the proﬁle

5.3. WET MAGNETIC SEPARATION

345

Table 5.13: Recommended maximum discharge rates of the magnetics [M26, S59]. Separator 762 mm drum 914 mm drum 1200 mm drum Double 762 mm Double 914 mm Double 1200 mm

Max. discharge rate [t/h/m] 10 15 24 18 30 48

of the magnetic force (or force index) shown in Fig. 4.29. Similarly, the critical role of the magnetic position on the recovery of magnetite was reported by Howell et al. [H21]. On the other hand, Rayner and Napier-Munn reported [R20] that the magnet position had no signiﬁcant eect on the performance of the drum separator. The distance between the drum and the tank has a two-fold eect on the separation e!ciency. With increasing clearance between the drum and the tank, the magnetic ﬁeld strength and the magnetic force are reduced in the areas furthest from the drum. This negatively aects the e!ciency of separation, particularly of ﬁne particles. On the other hand, by increasing the clearance, the velocity of ﬂow through the separation zone decreases and so does the hydrodynamic drag on particles. This results in a more e!cient attraction of magnetic particles to the drum and in reduced shear stress acting on particles already captured on the drum. The combined eect of these two contradictory phenomena can lead to improved recoveries when the clearance is increased [D13]. Media types and size The most common medium for separation is a suspension in water of ﬁne magnetite, ferrosilicon (FeSi), or a mixture of the two, depending on the separation density required. Magnetite alone is used when a density is required in the range 1250 to 2200 kg/m3 , a mixture for 2200 to 2900 kg/m3 and ferrosilicon alone for 2900 to 3700 kg/m3 . Magnetite, the density of which ranges from 4800 to 5200 kg/m3 > is the most popular choice for medium solids used in coal preparation, while ferrosilicon is invariably used, for instance, for the concentration of diamonds, for the recovery of aluminium in recycling plants, and for beneﬁciation of iron and manganese ores. Ferrosilicon containing between 14% to 16% silicon has a density ranging from 6700 to 7100 kg/m3 . It is non-rusting and strongly magnetic. With concentrations of silicon greater than 22% the material is feebly magnetic, while with concentrations of silicon lower than 15%, it is prone to rusting. Magnetite and ferrosilicon are thus selected as media because they meet a number of essential criteria: they are physically stable and chemically inert, easily removable from the products and are readily recovered for re-use by magnetic

346

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.14: Particle size distribution of magnetite for DMS [M26]. Size fraction [m] - 300 + 212 - 212 + 150 - 150 + 106 - 106 + 75 - 75 + 45 - 45

Fine grade [%] 3.8 4.4 6.2 7.6 13.5 64.5

Coarse grade [%] 8.2 4.3 14.1 12.0 19.9 32.7

Table 5.15: Particle size distributions of selected grades of milled and atomized ferrosilicon (Samancor, South Africa). Size fraction [m] + 212 + 150 + 106 + 75 + 45 - 45

48D 0-2 4-8 12 - 18 19 - 27 27 - 35 27 - 35

100D 0-1 0-1 1-4 5 - 10 28 61 - 69

270D 0 0 0-1 0-3 7 - 11 85 - 93

Cyclone 60 0 0-2 0-4 2-6 18 - 26 65 - 78

separation. Media is supplied in several size grades and the grade used will vary with each individual plant. While ﬁner grades improve stability, ﬁne particles, in addition to possible viscosity problems, are more di!cult to recover and the feed into LIMS should then be reduced by a factor of 1.5 to 2, to maintain the magnetic recovery. A typical particle size distribution of ground magnetite is shown in Table 5.14, while size distributions of several grades of ferrosilicon are listed in Table 5.15. There are two basic types of ferrosilicon available to the operators of dense medium plants, namely milled (e.g. 270D) and atomized spherical grades (e.g. Cyclone 60). There is a marked dierence in both the shape and nature of ferrosilicon particles produced by grinding and atomizing. Particles produced by grinding are rough and angular in shape, whereas particles produced by atomizing are smooth and largely spherical or rounded. This dierence in the particle shape has marked eects on the rheological properties of aqueous suspensions of the two types of ferrosilicon [C7]. The critical value of slurry density for atomized grades is much higher than for the milled grades. At densities above 3000 kg/m3 , the viscosities of suspensions of atomized ferrosilicon are signiﬁcantly lower than those of the milled grades, owing to the greater friction among the colliding irregularly shaped milled particles [C17]. This superior property of atomized ferrosilicon allows very high suspension densities to be obtained (up to 3800 kg/m3 ) and this has made possible the heavy-medium separation of certain ores that were not

5.3. WET MAGNETIC SEPARATION

347

previously amenable to the treatment. On the other hand, grades of milled ferrosilicon show greater stability than grades of atomized ferrosilicon of equivalent size distribution. Since the desired conditions of separation are those of minimum viscosity with maximum stability, selection of the grade of ferrosilicon is based on a trade-o between these contradictory requirements and on cost considerations. Viscosity of dense medium suspensions Magnetite media are characterized by high apparent viscosities, extremely sensitive to rate of shear. Viscosities of the magnetite medium ranging from 700 cP (0.7 Pa×s) at the shear rate of 1000 s1 to 2740 cP (2.74 Pa×s) at 1000 s1 were reported at the operating density of 2800 kg/m3 [G18]. Viscosities of ferrosilicon under similar conditions ranged from 84 cP (0.084 Pa×s) to 200 cP (0.2 Pa×s). Similar results were obtained for various grades of ferrosilicon [D14]. The modelling data and their veriﬁcation by experimental measurements show that the apparent viscosity of atomized ferrosilicon (e.g. Cyclone 60), at the operating density of 3800 kg/m3 ranged from 0.025 Pa×s at the shear rate of 150 s1 to 0.3 Pa×s at 10 s1 . Media losses Historically, media losses have frequently been the largest single component of the operating costs of dense medium separation plants. Losses of magnetite in coal washing plants range from 0.4 kg to 2 kg per tonne of raw coal. In modern large cyclone plants treating - 45 + 0.5 mm material, the average losses amount to 0.45 kg/t [E3]. In DMS plants that use ferrosilicon, the losses amount to 20% to 40% of the DMS plant operating costs [D13] and may range widely, from 0.1 to 2.8 kg/t [H20], although in modern plants they do not exceed 0.25 kg/t [D13]. In an iron ore cyclone plant, the ferrosilicon losses are reported to be 0.12 kg/t and 0.15 kg/t, for intermediate and ﬁne ore fractions, respectively [K20]. It is generally claimed that the losses in the magnetic circuit usually represent the major component of the total loss. For instance, Hunt et al. [H20] report that, excluding plant housekeeping, the average losses attributable to magnetic separation, adhesion and corrosion occur in the ratio 6:3:1. In another investigation, however, magnetic losses not exceeding 30% of the total loss were observed [N7]. Magnetic properties of ferrosilicon and magnetite The magnetic properties of magnetite and ferrosilicon are important for easy recovery and cleaning of the medium in the circuit. The running costs of a DMS plant are also aected by the magnetic properties. Baran and Svoboda [B29] conducted an extensive study of magnetic properties of both magnetite and ferrosilicon of various grades. A typical hysteresis curve of 270D milled ferrosilicon is shown in Fig. 5.18. Table 5.16 summarizes the magnetic characteristics of ferrosilicon and magnetite, as determined from measurements by a vibrating sample magnetometer. It can be seen that atomized grades of FeSi exhibit slightly higher values of the saturation polarization (by 5% to 7%) compared to the milled grades. The saturation polarization of magnetite (0.45 T) is lower than that of FeSi by factor

348

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Magnetisation of 270D FeSi 8000 6000 4000 2000 0 -2000 Magnetisation (G)

-4000 -6000 -8000 -15000

-10000

-5000

0

5000

10000

15000

Magnetic Field (Oe)

Figure 5.18: A hysteresis curve of 270D ferrosilicon as measured by a vibrating sample magnetometer [B29].

Table 5.16: Saturation polarization Js, remanent polarization Jr and coercive force Hc of various grades of ferrosilicon (Samancor) and magnetite (Amcoal), as measured by a vibrating sample magnetometer [B29]. Material Cyclone 60 48D 65D 100D 150D 270D Magnetite

Jv [T] 0.93 0.83 0.87 0.87 0.86 0.83 0.45

Ju [T] 0.047 0.052 0.055 0.048 0.048 0.051 0.063

Hf [kA/m] 9.96 10.2 10.6 9.33 9.89 9.89 14.3

5.3. WET MAGNETIC SEPARATION

349

Figure 5.19: Relationship between the Si concentration and the saturation polarization of FeSi (after [B29]). of two, and it was found to be by about 25% lower than the literature value of 0.6 T, as a result of the presence of weakly magnetic impurities. The coercive force of magnetite is 50% higher than that of ferrosilicon. This might indicate a need for a higher demagnetization ﬁeld for magnetite. Although the milled grades of FeSi were found to be much more susceptible to corrosion than the atomized grades, no substantial eect of corrosion on the magnetic properties was observed. Also, no signiﬁcant dierences in the magnetic behaviour of various size fractions of FeSi were observed. Only a slight reduction (less than 5%) in the saturation polarization values for fractions smaller than 106 m was observed. Losses of ﬁne FeSi in DMS plants can thus be ascribed to the reduced e!ciency of magnetic separators to recover ﬁne particles rather than to reduced magnetization. The initial magnetic susceptibility of all grades of FeSi was approximately 2.8×104 m3 /kg, while that of magnetite was found to be equal to 3.5×104 m3 /kg. It was also observed that a substantial increase in the saturation polarization of FeSi could be achieved by decreasing the concentration of Si as is illustrated in Fig. 5.19. It was found that the saturation polarization changed by 0.16 T for every 1% in the Si content, in the range 14% to 16%. Demagnetization The passage of heavy medium through magnetic separators in the medium recovery circuit induces remanent magnetization of the medium. This may result in the formation of magnetic ﬂocs with subsequent deterioration of the medium properties, such as stability and viscosity.

350

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.20: The eect of the demagnetizing magnetic induction on FeSi viscosity in a cone circuit at Premier Diamond Mine, South Africa (adapted from [C17]).

It is common practice at DMS plants to install demagnetization coils on the magnetic separator return lines. Although the need to demagnetize media has been recognized in the static-bath processes, the usefulness of demagnetization coils in cyclone plants has been a subject of dispute. The views range from outright rejection to unconditional acceptance. These polarized views are part of the DMS plant folklore, although there is an overwhelming scientiﬁc and engineering evidence of the beneﬁcial eect of media demagnetization. In general, the installation of demagnetization coils in DMS cyclone plants is recommended (e.g. [N8]). The inverse relationship between the magnetic ﬁeld strength in a demagnetization coil and the viscosity of the circulating medium FeSi medium in the cone circuits is illustrated in Fig. 5.20. A similar beneﬁcial eect of FeSi demagnetization, in a cyclone plant, was reported by Napier-Munn and Scott [N7]. They observed that the coil had a rapid and substantial eect on the viscosity and the results are summarized in Fig. 5.21. The viscosity had started to drop shortly after the coil was activated and to rise again after the coil was de-activated. Measurements of the magnetic susceptibility of magnetized samples of ferrosilicon showed that the values of magnetic susceptibility were higher than those of unmagnetized samples [B29]. After demagnetization by a coil generating the a.c. magnetic induction of 0.06 T, the magnetic susceptibility returned to its original value. Practical aspects of demagnetization are discussed in Section 5.5.

5.3. WET MAGNETIC SEPARATION

351

Figure 5.21: The eect of demagnetization on the viscosity of 150D FeSi medium at the cyclone plant of the Mount Isa Mines lead-zinc concentrator, Australia, (adapted from [N8]). Wet magnetic drum separators for ore concentration Wet low-intensity drum magnetic separators are also used for the concentration of magnetite ore or other strongly magnetic minerals. Most of the low-intensity magnetic separation technology used today was developed during the 1960s with no signiﬁcant changes taking place. The most noticeable changes over the years have occurred with the increased diameter and length of the drum. With each increase of the drum diameter, the process capacity of units increased and throughputs as high as 160 t/h per meter length of the drum were recorded. However, tests with 1500 mm diameter drum separators could not reproduce this trend for the capacity increase, and currently not many concentrators of this size have been installed [S13]. The improved design and more e!cient permanent magnetic materials allowed the magnetic ﬁeld rating of the drum magnetic separators, traditionally expressed as the magnetic induction at 50 mm (or 2 inches), to be increased, from 0.05 T to about 0.12 T available today. In the ore concentration applications, the separators are designed for three basic operations, namely as cobbers, roughers (cleaners) and ﬁnishers. Cobbers Drum separators used in cobbing operations are designed to obtain maximum rejection of a non-magnetic fraction and maximum recovery of the magnetic material. Most iron-ore concentrating drum separators are applied in multi-drum, usually con-current, conﬁgurations so that the high-grade magnetic concentrate is obtained. In cobbing operations, two drums are typical, but as

352

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

many as four drums have been used. The diameter of the drums is either 900 or 1200 mm and the magnetic ﬁeld rating, at 50 mm, of 0.1 T is standard for cobbers. Roughers Drum magnetic separators used in roughing or cleaning are applied after the size of the cobber concentrate has been further reduced. Because the cobbing has signiﬁcantly upgraded the ore, magnetic loading of the drum is usually increased considerably. The objective of roughing is to obtain a highgrade magnetic concentrate, while maintaining high recovery. Double-drum separators, in con- or counter-current modes of operation are typically used in roughers and the required magnetic ﬁeld at 50 mm is, as a rule, 0.07 T to 0.09 T. Finishers Finishing drum magnetic separators are designed to produce the highest possible iron content in the concentrate. The feed tank and feed arrangements are usually of semi-counter-current design, with the objective of dispersing the feed particles in order to obtain maximum rejection of non-magnetic particles. Both 760 and 900 mm-diameter drums are used in the ﬁnisher applications, with the magnetic ﬁeld strength at 50 mm lower (e.g. 0.05 T) than in a rougher, to improve selectivity of separation. The feed size is usually reduced to less than 75 m or 45 m. Variables in low-intensity magnetic separation of ores Factors associated with the properties of the feed, to be considered in the selection of a wet drum magnetic separation applied to the ore beneﬁciation, are [M26]: • Feed rate (t/h/m) • Feed particle size (max. 10 mm) and size distribution • Feed volume (m3 /h) • Concentration of magnetic particles • Degree of liberation • Desired recovery into the magnetic fraction. As shown in Table 5.17, the maximum feed rate varies with the type of separator considered; maximum and recommended feed volumes are also given. Typical sizes of feed particles for the three modes of operation are: Cobbers: - 6 mm + 850 m Roughers: - 500 m + 300 m Finishers: - 75 m + 45 m.

5.3. WET MAGNETIC SEPARATION

353

Table 5.17: Feed rates and feed volumes in LIMS, as applied to ore beneﬁciation [M26]. Application Cobber Rougher Finisher

Feed rate [t/h/m] Max. Recommended 75 45 60 45 15 15

Feed volume [m3 /h/m] Max. Recommended 100 70 100 70 35 20

Table 5.18: Number of drums and magnetic poles used in LIMS for ore beneﬁciation [M26]. Separator Cobbers Roughers Finishers

Number of drums 2 to 4 1 or 2 2 or 3

Number of poles 5 or 6 5 or 6 4 to 10

Magnetic content and degree of liberation The magnetic content of iron ores to be concentrated by LIMS varies over a fairly wide range. Ores with iron concentrations from 10% to 50% or more have been successfully treated. Since liberation is not complete at the cobber stage, a substantial amount of gangue is carried into the cobber concentrate. Typically, the cobber concentrate contains 50% Fe or more and, accordingly, the magnetics content of the rougher feed is quite high. The ﬁnisher feed contains 2% to 5% of non-magnetics and thus has a very high concentration of the magnetic material. Complete liberation of most iron ores that are being treated by LIMS is usually at sizes ﬁner than 150 m, although some ores have to be reduced to 45 m. Magnetic ﬁeld strength and number of poles Increased magnetic ﬁeld strength achievable in modern low-intensity drum magnetic separators allows not only more e!cient recovery of ﬁne particles, but also the throughput of a separator can be increased without losing recovery. Such an eect of magnetic ﬁeld strength on throughput and recovery is illustrated in Fig. 5.22. The number of drums used in various applications varies with the individual ores and the choice is determined by the results of pilot-plant or laboratory tests. In addition, various types of magnetic assemblies and pole combinations have been successfully used. Typical magnetic pole speciﬁcations and number of drums are shown in Table 5.18. Throughput The feed rate in a low-intensity magnetic separator aects its metallurgical performance, as can be seen in Figs. 5.22 and 5.23. With increasing feed rate, the recovery of magnetic particles into the magnetic fraction decreases, the rate of decrease being strongly dependent on the magnetic ﬁeld

354

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS

Figure 5.22: Recovery of iron by LIMS, as a function of throughput, for dierent values of magnetic induction at 50 mm (adapted from Sundberg [S13]). strength generated by the magnetic drum.

5.3.2

Wet high-intensity magnetic separation

Wet high-intensity magnetic separation is used in three dierent technological processes, as shown in Fig. 5.24. These separators can thus be used either as a magnetic ﬁlter to remove a single solid component from a suspension, or as a magnetic separator to remove an unwanted magnetic component from a mixture of materials, or for a concentration of valuable weakly magnetic materials from a mixture. The high intensity of the magnetic ﬁeld in these separators is generated either by rare earth or ferrite permanent magnets (for example in RE drum separators or in a Ferrous Wheel separator), or by resistive electromagnets or superconducting magnets. Magnetic ﬁeld gradient, an equally important parameter in magnetic separation, is generated by three dierent methods. Close-gradient, open-gradient and matrix (polygradient) techniques produce magnetic ﬁeld gradients of widely dierent magnitudes, as can be seen in Table 1.20. As a result of these dierent attributes of high-intensity magnetic separators, a plethora of names and terms is being used to classify them, although the operating principle of many of them are the same or, at worst, they can address similar separation objectives. The resulting chaos is further magniﬁed by the advent of new magnetic materials and advanced magnet designs that allow new approaches to high ﬁeld and high

5.3. WET MAGNETIC SEPARATION

355

Figure 5.23: The eect of feed rate on the recovery of magnetite, in a lowintensity magnetic drum separator. Drum length: 1.2 m, drum diameter: 900 mm (adapted from [K14]).

< 1% solids

Cyclic

> 1% solids

Continuous

< 1% solids

Cyclic

> 1% solids

Continuous

Filtration

Wet highintensity magnetic separation

Removal from mixture

High recovery Concentration from mixture

Continuous separation

High grade High grade and recovery

Figure 5.24: The range of applications of wet high-intensity magnetic separation (adapted from Svoboda [S1]).

356

CHAPTER 5. PRACTICAL ASPECTS OF MAGNETIC METHODS Table 5.19: Nomenclature for wet high-intensity magnetic separators. Separator Rare-earth drum separator Linear multipole open-gradient separator Matrix continuous separator Matrix cyclic separator Matrix cyclic magnetic ﬁlter

Acronyms REDS, REDMS, MIMS OGMS WHIMS, HGMS, HIMS HGMS HGMF, HIMF

gradient generation. A summary of the terms most frequently used to describe wet high-intensity magnetic separators is given in Table 5.19. A schematic diagram of dierent technological processes, in which wet highintensity magnetic separators are used, is shown in Fig. 5.24. It is clear that conditions for successful separation in these three categories can dier widely. Their correct selection must be based upon proper identiﬁcation of the target of the process and the deﬁnition of criteria that would distinguish successful separation from unsuccessful. The decision-making process in such a selection is outlined in Fig. 5.25 and its detailed discussion will be presented in subsequent sections. Wet rare-earth drum magnetic separators Although dry rare-earth drum magnetic separators have been readily accepted by the mining industry, it has taken somewhat longer to develop and implement wet RE drum separators. One of the reasons for reluctant acceptance of wet RE drums by the industry is the onerous problem with the removal of strongly magnetic material from the drum, even when these particles are present in trace concentrations. Conventional high-pressure spraying or scraping methods are not su!ciently eective in overcoming the strong magnetic force holding the particles on the drum, and new approaches to this problem are being investigated [A23]. Magnetic ﬁltration Magnetic ﬁltration is used primarily for the removal of ﬁne and quasi-colloidal particulates from dilute ﬂuid suspensions. Removal is carried out by passing suspensions through a magnetized matrix, which leads to the retention of particles throughout the matrix. The ﬂuid stream may be either liquid or gas. The process of magnetic ﬁltration is analogous to that of deep bed ﬁltration, the dierence being that an additional external force, namely the magnetic force, contributes to the ﬁltration e!ciency in magnetic ﬁltration. Although the magnetic force does not signiﬁcantly increase the probability of particle collision with the matrix [S31, S33], the enhanced e!ciency of particle attachment caused by the presence of strong, static dipolar magnetic interaction between the matrix and a colliding particle increases signiﬁcantly the e!ciency of the

5.3. WET MAGNETIC SEPARATION

357

HGMS

Yes Single solid component?

Magnetic filtration

No

Continuous MS

Magnetic component valuable?

No

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close